This textbook presents a detailed description of basic semiconductor physics, covering a wide range of important phenome

*310*
*66*
*20MB*

*English*
*Pages 800
[790]*
*Year 2023*

- Author / Uploaded
- Chihiro Hamaguchi

*Table of contents : PrefaceContents1 Energy Band Structures of Semiconductors 1.1 Free-Electron Model 1.2 Bloch Theorem 1.3 Nearly Free Electron Approximation 1.4 Reduced Zone Scheme 1.5 Free–Electron Bands (Empty–Lattice Bands) 1.5.1 First Brillouin Zone 1.5.2 Reciprocal Lattice Vectors of fcc Crystal 1.5.3 Free Electron Bands 1.6 Pseudopotential Method 1.6.1 Local Pseudopotential Theory 1.6.2 Pseudopotential Form Factors 1.6.3 Nonlocal Pseudopotential Theory 1.6.4 Spin–Orbit Interaction 1.6.5 Energy Band Calculation by Local Pseudopotential Method 1.6.6 Energy Band Calculations by Nonlocal Pseudopotential Method with Spin–orbit Interaction 1.7 kcdotp Perturbation 1.7.1 kcdotp Hamiltonian 1.7.2 Derivation of the k cdotp Parameters 1.7.3 15–band k cdotp Method 1.7.4 Antisymmetric Potentials for Zinc Blende Crystals 1.7.5 Spin–Orbit Interaction Hamiltonian 1.7.6 30–band kcdotp Method with the Spin–Orbit Interaction 1.8 Density of States 1.9 Problems References2 Cyclotron Resonance and Energy Band Structures 2.1 Cyclotron Resonance 2.2 Analysis of Valence Bands 2.3 Spin–Orbit Interaction 2.4 Non-parabolicity of the Conduction Band 2.5 Electron Motion in a Magnetic Field and Landau Levels 2.5.1 Landau Levels 2.5.2 Density of States and Inter Landau Level Transition 2.5.3 Landau Levels of a Non-parabolic Band 2.5.4 Effective g Factor 2.5.5 Landau Levels of the Valence Bands 2.5.6 Magneto–Optical Absorption 2.6 Luttinger Hamiltonian 2.7 Luttinger Parameters 2.8 Problems References3 Wannier Function and Effective Mass Approximation 3.1 Wannier Function 3.2 Effective-Mass Approximation 3.3 Shallow Impurity Levels 3.4 Impurity Levels in Ge and Si 3.4.1 Valley–Orbit Interaction 3.4.2 Central Cell Correction 3.5 Electron Motion Under an External Field 3.5.1 Group Velocity 3.5.2 Electron Motion Under an External Force 3.5.3 Electron Motion and Effective Mass 3.6 Problems References4 Optical Properties 1 4.1 Reflection and Absorption 4.2 Direct Transition and Absorption Coefficient 4.3 Joint Density of States 4.4 Indirect Transition 4.5 Exciton 4.5.1 Direct Exciton 4.5.2 Indirect Exciton 4.6 Dielectric Function 4.6.1 E0, E0+ Δ0 Edge 4.6.2 E1 and E1+Δ1 Edge 4.6.3 E2 Edge 4.6.4 Exciton 4.7 Piezobirefringence 4.7.1 Phenomenological Theory of Piezobirefringence 4.7.2 Deformation Potential Theory 4.7.3 Stress-Induced Change in Energy Band Structure 4.8 Problems References5 Optical Properties 2 5.1 Modulation Spectroscopy 5.1.1 Electro-optic Effect 5.1.2 Franz–Keldysh Effect 5.1.3 Modulation Spectroscopy 5.1.4 Theory of Electroreflectance and Third-Derivative Form of Aspnes 5.2 Raman Scattering 5.2.1 Selection Rule of Raman Scattering 5.2.2 Quantum Mechanical Theory of Raman Scattering 5.2.3 Resonant Raman Scattering 5.3 Brillouin Scattering 5.3.1 Scattering Angle 5.3.2 Brillouin Scattering Experiments 5.3.3 Resonant Brillouin Scattering 5.4 Polaritons 5.4.1 Phonon Polaritons 5.4.2 Exciton Polaritons 5.5 Free–Carrier Absorption and Plasmon 5.6 Problems References6 Electron–Phonon Interaction and Electron Transport 6.1 Lattice Vibrations 6.1.1 Acoustic Mode and Optical Mode 6.1.2 Harmonic Approximation 6.2 Boltzmann Transport Equation 6.2.1 Collision Term and Relaxation Time 6.2.2 Mobility and Electrical Conductivity 6.3 Scattering Probability and Transition Matrix Element 6.3.1 Transition Matrix Element 6.3.2 Deformation Potential Scattering (Acoustic Phonon Scattering) 6.3.3 Ionized Impurity Scattering 6.3.4 Piezoelectric Potential Scattering 6.3.5 Non–polar Optical Phonon Scattering 6.3.6 Polar Optical Phonon Scattering 6.3.7 Inter–Valley Phonon Scattering 6.3.8 Deformation Potential in Degenerate Bands 6.3.9 Theoretical Calculation of Deformation Potentials 6.3.10 Electron–Electron Interaction and Plasmon Scattering 6.3.11 Alloy Scattering 6.4 Scattering Rate and Relaxation Time 6.4.1 Acoustic Phonon Scattering 6.4.2 Non–polar Optical Phonon Scattering 6.4.3 Polar Optical Phonon Scattering 6.4.4 Piezoelectric Potential Scattering 6.4.5 Inter–Valley Phonon Scattering 6.4.6 Ionized Impurity Scattering 6.4.7 Neutral Impurity Scattering 6.4.8 Plasmon Scattering 6.4.9 Alloy Scattering 6.5 Mobility 6.5.1 Acoustic Phonon Scattering 6.5.2 Non–polar Optical Phonon Scattering 6.5.3 Polar Optical Phonon Scattering 6.5.4 Piezoelectric Potential Scattering 6.5.5 Inter–Valley Phonon Scattering 6.5.6 Ionized Impurity Scattering 6.5.7 Neutral Impurity Scattering 6.5.8 Plasmon Scattering 6.5.9 Alloy Scattering 6.6 Problems References7 Magnetotransport Phenomena 7.1 Phenomenological Theory of the Hall Effect 7.2 Magnetoresistance Effects 7.2.1 Theory of Magnetoresistance 7.2.2 General Solutions for a Weak Magnetic Field 7.2.3 Case of Scalar Effective Mass 7.2.4 Magnetoresistance 7.3 Shubnikov–de Haas Effect 7.3.1 Theory of Shubnikov–de Haas Effect 7.3.2 Longitudinal Magnetoresistance Configuration 7.3.3 Transverse Magnetoresistance Configuration 7.4 Magnetophonon Resonance 7.4.1 Experiments and Theory of Magnetophonon Resonance 7.4.2 Various Types of Magnetophonon Resonance 7.4.3 Magnetophonon Resonance Under High Electric and High Magnetic Fields 7.4.4 Polaron Effect 7.5 Problems References8 Quantum Structures 1 8.1 Historical Background 8.2 Two-Dimensional Electron Gas Systems 8.2.1 Two-Dimensional Electron Gas in MOS Inversion Layer 8.2.2 Quantum Wells and HEMT 8.3 Transport Phenomena of Two-Dimensional Electron Gas 8.3.1 Fundamental Equations 8.3.2 Acoustic Phonon Scattering and Non-Polar Optical Phonon Scattering 8.3.3 Inter-Valley Phonon Scattering 8.3.4 Polar Optical Phonon Scattering 8.3.5 Piezoelectric Potential Scattering 8.3.6 Ionized Impurity Scattering 8.3.7 Surface Roughness Scattering 8.3.8 Screening Effect 8.3.9 Remote Ionized Impurity Scattering 8.3.10 Mobility of a Two-Dimensional Electron Gas 8.4 Mesoscopic Phenomena 8.4.1 Mesoscopic Region 8.4.2 Definition of Mesoscopic Region 8.4.3 Landauer Formula and Büttiker–Landauer Formula 8.4.4 Research in the Mesoscopic Region 8.4.5 Aharonov–Bohm Effect (AB Effect) 8.4.6 Ballistic Electron Transport 8.5 Quantum Hall Effect 8.6 Problems References9 Quantum Structures 2 9.1 Superlattices 9.1.1 Kronig–Penney Model 9.1.2 Effect of Brillouin Zone Folding 9.1.3 Tight Binding Approximation 9.1.4 sp3sast Tight Binding Approximation 9.1.5 Energy Band Calculations for Superlattices 9.1.6 Second Nearest-Neighbor sp3 Tight Binding Approximation 9.2 Quantum Dots 9.2.1 Addition Energy 9.2.2 Exact Diagonalization Method 9.2.3 Hamiltonian for Electrons in a Quantum Dot 9.2.4 Diagonalization of N Electrons Hamiltonian Matrix 9.2.5 Electronic States in Quantum Dots 9.2.6 Quantum Dot States in Magnetic Field 9.2.7 Electronic States in Elliptic and Triangular Quantum Dots 9.3 Coulomb Blockade and Single Electron Transistor 9.4 Surface modulation of Two-dimensional Electron Gas and Weiss Oscillation 9.5 Wannier–Stark Effect in Superlattices 9.6 Bloch Oscillation 9.7 Problems References10 Light Emission and Laser 10.1 Einstein Coefficients A and B 10.2 Spontaneous Emission and Stimulated Emission 10.3 Band Tail Effect 10.4 Luminescence 10.4.1 Luminescence Due to Band to Band Transition 10.4.2 Luminescence Due to Excitons 10.4.3 Luminescence via Impurities 10.4.4 Luminescence in GaP and GaAsP via N Traps 10.4.5 Luminescence from GaInNAs 10.4.6 Light Emitting Diodes (LEDs) in Visible Region 10.5 Heterostructure Optical Waveguide 10.5.1 Wave Equations for Planar Waveguide 10.5.2 Transverse Electric Modes 10.5.3 Transverse Magnetic Modes 10.5.4 Effective Refractive Index 10.5.5 Confinement Factor 10.5.6 Laser Oscillations 10.6 Stimulated Emission in Quantum Well Structures 10.6.1 Confinement in Quantum Well 10.6.2 Optical Transition in Quantum Well Structures 10.6.3 Reduced Density of States and Gain 10.6.4 Strain Effect 10.6.5 Wurtzite Semiconductor Lasers 10.6.6 Optical Gain of Nitride Quantum Well Structures 10.7 Problems References11 Wade Bandgap Semiconductor and Photonic Crystals 11.1 Energy Band Structures of Nitrides 11.1.1 Energy Band Calculations of GaN, AlN, and InN 11.1.2 Energy Band Structures of Ternary Alloys 11.1.3 Spin–Orbit–Interaction and Valence Band Structures 11.2 Electron and Hole Mobilities of GaN 11.2.1 Acoustic Deformation Potential Scattering 11.2.2 Piezoelectric Potential Scattering 11.2.3 Ionized Impurity Scattering 11.2.4 Polar Optical Phonon Scattering 11.2.5 Remote Impurity Scattering 11.2.6 Other Scatterings 11.2.7 Evaluation of Electron and Hole Mobility 11.3 SiC and Other Semiconductors 11.3.1 SiC 11.3.2 Electron Mobility in 4H-SiC 11.4 Photonic Crystals 11.4.1 One-Dimensional Photonic Crystal 11.4.2 Two-Dimensional Photonic Crystal 11.4.3 Defects in Photonic Crystal 11.4.4 FDTD Method 11.5 Problems References12 Answers for ProblemsAppendix A Delta Function and Fourier TransformA.1 Dirac Delta FunctionA.2 Cyclic Boundary Condition and Delta FunctionA.3 Fourier TransformAppendix B Gamma FunctionAppendix C Uniaxial Stress and Strain Components in Cubic CrystalsAppendix D Boson OperatorsAppendix E Random Phase Approximation and Lindhard Dielectric FunctionAppendix F Density MatrixAppendix G Spontaneous and Stimulated Emission RatesAppendix H Spin–Orbit Interaction ReferencesIndex*

Graduate Texts in Physics

Chihiro Hamaguchi

Basic Semiconductor Physics Fourth Edition

Graduate Texts in Physics Series Editors Kurt H. Becker, NYU Polytechnic School of Engineering, Brooklyn, NY, USA Jean-Marc Di Meglio, Matière et Systèmes Complexes, Bâtiment Condorcet, Université Paris Diderot, Paris, France Sadri Hassani, Department of Physics, Illinois State University, Normal, IL, USA Morten Hjorth-Jensen, Department of Physics, Blindern, University of Oslo, Oslo, Norway Bill Munro, NTT Basic Research Laboratories, Atsugi, Japan Richard Needs, Cavendish Laboratory, University of Cambridge, Cambridge, UK William T. Rhodes, Department of Computer and Electrical Engineering and Computer Science, Florida Atlantic University, Boca Raton, FL, USA Susan Scott, Australian National University, Acton, Australia H. Eugene Stanley, Department of Physics, Center for Polymer Studies, Boston University, Boston, MA, USA Martin Stutzmann, Walter Schottky Institute, Technical University of Munich, Garching, Germany Andreas Wipf, Institute of Theoretical Physics, Friedrich-Schiller-University Jena, Jena, Germany

Graduate Texts in Physics publishes core learning/teaching material for graduateand advanced-level undergraduate courses on topics of current and emerging fields within physics, both pure and applied. These textbooks serve students at the MS- or PhD-level and their instructors as comprehensive sources of principles, definitions, derivations, experiments and applications (as relevant) for their mastery and teaching, respectively. International in scope and relevance, the textbooks correspond to course syllabi sufficiently to serve as required reading. Their didactic style, comprehensiveness and coverage of fundamental material also make them suitable as introductions or references for scientists entering, or requiring timely knowledge of, a research field.

Chihiro Hamaguchi

Basic Semiconductor Physics Fourth Edition

Chihiro Hamaguchi Osaka University Suita, Osaka, Japan

ISSN 1868-4513 ISSN 1868-4521 (electronic) Graduate Texts in Physics ISBN 978-3-031-25510-6 ISBN 978-3-031-25511-3 (eBook) https://doi.org/10.1007/978-3-031-25511-3 1st & 2nd editions: © Springer-Verlag Berlin Heidelberg 2001, 2010 3rd edition: © Springer International Publishing AG 2017 4th edition: © The Editor(s) (if applicable) and The Author(s), under exclusive license to Springer Nature Switzerland AG 2023 This work is subject to copyright. All rights are solely and exclusively licensed by the Publisher, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. The publisher, the authors, and the editors are safe to assume that the advice and information in this book are believed to be true and accurate at the date of publication. Neither the publisher nor the authors or the editors give a warranty, expressed or implied, with respect to the material contained herein or for any errors or omissions that may have been made. The publisher remains neutral with regard to jurisdictional claims in published maps and institutional affiliations. This Springer imprint is published by the registered company Springer Nature Switzerland AG The registered company address is: Gewerbestrasse 11, 6330 Cham, Switzerland

Preface

The purpose of this book was to provide a detailed understanding of the basic semiconductor physics such as properties of electronic, optical, transport, and quantum structures of semiconductors. We may find many well-established books on semiconductor physics including theoretical and device oriented books. For an understanding of semiconductor physics, an introduction to elementary quantum mechanics, solid physics, and mathematics are required. However, these subjects are given independently for the courses in physics and electrical engineering. Therefore this book omits some of the elementary topics. Instead, more important subjects such as energy band structure, transport, light emission, laser, LED, and new wide band gap materials of nitrides are properly included. The first edition of Basic Semiconductor Physics was published in 2001 and the second edition in 2010, which have been widely used by various readers. Some of the readers point out that many important equations used in the textbook are derived reasonably and the results give a good guide to study the physics of semiconductors. Especially the energy band calculations, optical properties, transport properties, and quantum structures are well described and help the readers to start research on the physics of semiconductors. The second edition was planned to include the physics of light emission, LED, and lasers, according to the suggestions of the readers. They also asked the author to revise the textbook with the energy band calculations with spin-orbit interaction, and optical and transport properties, showing calculated results and keeping the subject at the appropriate level for the third edition. The third edition was planned to present some important subjects in more detail, such as the energy band calculations, optical properties, transport of carriers, and semiconductor lasers. The new edition (fourth edition) is planned to correct errors in the third edition and to rewrite the energy band calculations with properly determined parameters throughout the textbook. Most of the figures are calculated with the new parameters and drawn in colors by computer programs, which will provide a very good guide to an understanding of basic semiconductor physics. The aim of this fourth edition follows the style of the third edition and most of the figures are recalculated and drawn in colors. New subjects are added such as surface modulated superlattice, Wannier-Stark effect, Bloch oscillation, wide band gap semiconductors, and photonic crystals. v

vi

1.

2.

3.

4.

5.

6.

7.

8.

Preface

In Chap. 1, we explain cyclic boundary condition and Bloch theorem, and then energy band calculations are discussed in detail. Starting from nearly free electron model, pseudopotential method and κ · p perturbation method are discussed, and energy band structures of various semiconductors are calculated in the full Brillouin zone. In order to understand the valence band structure, energy band calculations with spin-orbit interaction are discussed in the full Brillouin zone using the local pseudopotential, non-local pseudopotential method, and κ · p perturbation method. Once the readers understand the methods, numerical calculations are straight forward because all the matrix elements are given in this textbook. The energy band structures of various semiconductors recalculated and figures are drawn in colors. In Chap. 2, the cyclotron resonance is described in detail, where effective masses in many valley structure are discussed. The valence band structure analysis based on κ · p perturbation is described for the application to various calculations. Landau levels in high magnetic field are discussed and magneto-optical absorption experiments are analyzed. The valence band parameters known as Luttinger parameters are explained in detail. In Chap. 3, we discuss the effective mass approximation which is widely adopted in the analysis of optical transition and transport properties. Its explanation and validity are discussed with its application to shallow impurity states. Also, we show that the expectation value of velocity operator with Bloch function is related to the electron energy expressed by the wave vector. Then, we prove that the motion of an electron with effective mass in an external force is expressed by the classical mechanics, in other words, by Newton’s law. In Chap. 4 (Optical Properties 1), theoretical analysis of optical properties of semiconductors is given, where we explain the optical transition and the dielectric functions with respect to various optical processes. Derived formulas are very important to understand energy band structure and to develop optical devices that have been accepted as the most important tool to learn the energy band structures. In Chap. 5 (Optical Properties 2), we will concern with the optical spectroscopy placing special emphasis on modulation spectroscopy, and Raman and Brillouin scatterings in semiconductors. In Chap. 6, we present theoretical treatment of transport with the help of Boltzmann transport equation. Scattering processes of electrons are described by taking account of various kinds of phonons (lattice vibrations), impurity density, plasmon, and so on. The results help our understanding of electron transport and semiconductor device physics. In Chap. 7, we discuss the subject of magnetotransport effects. Hall effect is one of the most important experimental methods. Classical Hall effect is given in detail and data of Hall effect experiment are analyzed as a good example. In Chap. 8 (Quantum Structure 1), we deal with transport properties of twodimensional electron gas (2DEG) in MOS inversion layer and heterostructure such as HEMT (High Electron Mobility Transistor) and quantum wells. Mesoscopic phenomena such as Landauer formula and Aharonov-Bohm (AB)

Preface

9. 10.

11.

12.

13.

vii

effect are introduced. The discovery of “Quantum Hall Effect” by Klaus von Klitzing has opened the door to basic physics and to newly developed quantum physics. This chapter will provide a guide to new and important region of basic semiconductor physics. In Chap. 9 (Quantum Structure 2), we discuss superlattice, quantum dot, Weiss oscillation, Wannier–Stark effect, and Bloch oscillation in semiconductors. In Chap. 10, we start with Einstein coefficients for optical transition, absorption, spontaneous and stimulated emission, and then we discuss luminescence in various semiconductors. Light emission diodes (LED’s) and laser diodes (LD’s) are now very useful devices. We discuss heterostructure wave guide and quantum well structure for the light emission devices. In Chap. 11, we discuss wide band gap materials and photonic crystals, which are very popular subjects in recent years. Nitrides such as GaN, GaInN are playing the most important role in the optical and high frequency devices. We calculate energy band structures of such materials as GaN, InN, AlN, and their ternary alloys by using pseudopotential method. SiC materials are also very well known wide band gap semiconductors. In this chapter we will concern with 4H-SiC which is most widely investigated. Finally, we present basic physics of photonic crystals. More than 70 problems are provided through the textbook and the solutions (Answers) will provide more detailed understanding of semiconductor physics. Many of the numerical calculations are straight forward because SI units are used throughout. The colored illustrations (figures) throughout the book are very informative for readers to understand the semiconductor physics. Appendix was planned to provide a supplement to mathematical treatments. The Dirac delta function and Fourier transform are very useful to handle mathematical equations for the cyclic boundary conditions. The physics of spin-orbit interaction is very important for the analysis of the valence bands and the brief introduction is helpful for readers to learn how to manage it.

The author would like to express his special thanks to Prof. Dr. Nobuya Mori, Osaka University, for his contribution to the energy band calculations of nitrides and for many stimulated discussions on the basic physics. I want to thank Prof. Dr. Masato Morifuji for the contribution to the subject on photonic crystals. Also, I want to note my special thanks to the late Professors, Dr. Yoshiro Sasaki for the modulation spectroscopy, Dr. Tatsuya Ezaki for the exact calculation of electronic states in quantum dots, and Dr. Masufumi Yamaguchi for the tight-binding analysis of Wannier-Stark effect in superlattices. I want to express my thanks to many graduate students of Osaka University for the discussion on the theoretical calculations of the subjects included in this textbook. The author expresses his grateful thanks to Prof. Dr. Klaus von Klitzing for inviting me to Max Planck Institute, Stuttgart, to finish the full band κ · p perturbation theory, providing him a chance to discuss this subject with the late Prof. Dr. Manuel Cardona. The author is thankful to his wife Wakiko for her patience during the work of this textbook.

viii

Preface

Finally I want to thank the staff of the Springer Verlag for their help and for the valuable suggestions for clarification of this book. Chihiro Hamaguchi Professor Emeritus Fellow of APS (USA), IOP (UK), IEEE (USA), and JSAP Osaka University Suita, Osaka, Japan [email protected]

Contents

1

Energy Band Structures of Semiconductors . . . . . . . . . . . . . . . . . . . . . 1.1 Free-Electron Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Bloch Theorem . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3 Nearly Free Electron Approximation . . . . . . . . . . . . . . . . . . . . . . . . 1.4 Reduced Zone Scheme . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5 Free–Electron Bands (Empty–Lattice Bands) . . . . . . . . . . . . . . . . . 1.5.1 First Brillouin Zone . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.2 Reciprocal Lattice Vectors of fcc Crystal . . . . . . . . . . . . . 1.5.3 Free Electron Bands . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6 Pseudopotential Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6.1 Local Pseudopotential Theory . . . . . . . . . . . . . . . . . . . . . . 1.6.2 Pseudopotential Form Factors . . . . . . . . . . . . . . . . . . . . . . 1.6.3 Nonlocal Pseudopotential Theory . . . . . . . . . . . . . . . . . . . 1.6.4 Spin–Orbit Interaction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6.5 Energy Band Calculation by Local Pseudopotential Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6.6 Energy Band Calculations by Nonlocal Pseudopotential Method with Spin–orbit Interaction . . . 1.7 k · p Perturbation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.7.1 k · p Hamiltonian . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.7.2 Derivation of the k · p Parameters . . . . . . . . . . . . . . . . . . . 1.7.3 15–band k · p Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.7.4 Antisymmetric Potentials for Zinc Blende Crystals . . . . 1.7.5 Spin–Orbit Interaction Hamiltonian . . . . . . . . . . . . . . . . . 1.7.6 30–band k · p Method with the Spin–Orbit Interaction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.8 Density of States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.9 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

1 1 3 5 9 10 10 12 13 16 16 21 23 25 27 32 34 34 41 46 50 51 54 59 62 62

ix

x

Contents

2

Cyclotron Resonance and Energy Band Structures . . . . . . . . . . . . . . . 2.1 Cyclotron Resonance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Analysis of Valence Bands . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Spin–Orbit Interaction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Non-parabolicity of the Conduction Band . . . . . . . . . . . . . . . . . . . . 2.5 Electron Motion in a Magnetic Field and Landau Levels . . . . . . . 2.5.1 Landau Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5.2 Density of States and Inter Landau Level Transition . . . 2.5.3 Landau Levels of a Non-parabolic Band . . . . . . . . . . . . . . 2.5.4 Effective g Factor . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5.5 Landau Levels of the Valence Bands . . . . . . . . . . . . . . . . . 2.5.6 Magneto–Optical Absorption . . . . . . . . . . . . . . . . . . . . . . . 2.6 Luttinger Hamiltonian . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.7 Luttinger Parameters . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.8 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

65 65 74 80 88 92 92 97 99 103 106 112 116 120 127 128

3

Wannier Function and Effective Mass Approximation . . . . . . . . . . . . 3.1 Wannier Function . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Effective-Mass Approximation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Shallow Impurity Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4 Impurity Levels in Ge and Si . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 Valley–Orbit Interaction . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 Central Cell Correction . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.5 Electron Motion Under an External Field . . . . . . . . . . . . . . . . . . . . 3.5.1 Group Velocity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.5.2 Electron Motion Under an External Force . . . . . . . . . . . . 3.5.3 Electron Motion and Effective Mass . . . . . . . . . . . . . . . . . 3.6 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

129 129 131 136 139 142 144 146 146 150 153 155 155

4

Optical Properties 1 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Reflection and Absorption . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Direct Transition and Absorption Coefficient . . . . . . . . . . . . . . . . . 4.3 Joint Density of States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4 Indirect Transition . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5 Exciton . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5.1 Direct Exciton . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5.2 Indirect Exciton . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.6 Dielectric Function . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.6.1 E 0 , E 0 + Δ0 Edge . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.6.2 E 1 and E 1 + Δ1 Edge . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.6.3 E 2 Edge . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.6.4 Exciton . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.7 Piezobirefringence . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.7.1 Phenomenological Theory of Piezobirefringence . . . . . .

157 157 162 164 169 175 175 185 187 190 193 194 194 196 196

Contents

5

6

xi

4.7.2 Deformation Potential Theory . . . . . . . . . . . . . . . . . . . . . . 4.7.3 Stress-Induced Change in Energy Band Structure . . . . . . 4.8 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

198 201 207 209

Optical Properties 2 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1 Modulation Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1.1 Electro-optic Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1.2 Franz–Keldysh Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1.3 Modulation Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1.4 Theory of Electroreflectance and Third-Derivative Form of Aspnes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2 Raman Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.1 Selection Rule of Raman Scattering . . . . . . . . . . . . . . . . . 5.2.2 Quantum Mechanical Theory of Raman Scattering . . . . 5.2.3 Resonant Raman Scattering . . . . . . . . . . . . . . . . . . . . . . . . 5.3 Brillouin Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.1 Scattering Angle . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.2 Brillouin Scattering Experiments . . . . . . . . . . . . . . . . . . . . 5.3.3 Resonant Brillouin Scattering . . . . . . . . . . . . . . . . . . . . . . . 5.4 Polaritons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.1 Phonon Polaritons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.2 Exciton Polaritons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5 Free–Carrier Absorption and Plasmon . . . . . . . . . . . . . . . . . . . . . . . 5.6 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

211 211 211 213 217

Electron–Phonon Interaction and Electron Transport . . . . . . . . . . . . 6.1 Lattice Vibrations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1.1 Acoustic Mode and Optical Mode . . . . . . . . . . . . . . . . . . . 6.1.2 Harmonic Approximation . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2 Boltzmann Transport Equation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 Collision Term and Relaxation Time . . . . . . . . . . . . . . . . . 6.2.2 Mobility and Electrical Conductivity . . . . . . . . . . . . . . . . 6.3 Scattering Probability and Transition Matrix Element . . . . . . . . . . 6.3.1 Transition Matrix Element . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.2 Deformation Potential Scattering (Acoustic Phonon Scattering) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.3 Ionized Impurity Scattering . . . . . . . . . . . . . . . . . . . . . . . . 6.3.4 Piezoelectric Potential Scattering . . . . . . . . . . . . . . . . . . . . 6.3.5 Non–polar Optical Phonon Scattering . . . . . . . . . . . . . . . . 6.3.6 Polar Optical Phonon Scattering . . . . . . . . . . . . . . . . . . . . 6.3.7 Inter–Valley Phonon Scattering . . . . . . . . . . . . . . . . . . . . . 6.3.8 Deformation Potential in Degenerate Bands . . . . . . . . . . 6.3.9 Theoretical Calculation of Deformation Potentials . . . . .

220 225 231 236 242 245 247 251 254 257 257 262 265 270 271 273 274 274 279 288 290 293 298 298 302 304 308 312 313 318 319 321

xii

Contents

6.3.10 Electron–Electron Interaction and Plasmon Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.11 Alloy Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Scattering Rate and Relaxation Time . . . . . . . . . . . . . . . . . . . . . . . . 6.4.1 Acoustic Phonon Scattering . . . . . . . . . . . . . . . . . . . . . . . . 6.4.2 Non–polar Optical Phonon Scattering . . . . . . . . . . . . . . . . 6.4.3 Polar Optical Phonon Scattering . . . . . . . . . . . . . . . . . . . . 6.4.4 Piezoelectric Potential Scattering . . . . . . . . . . . . . . . . . . . 6.4.5 Inter–Valley Phonon Scattering . . . . . . . . . . . . . . . . . . . . . 6.4.6 Ionized Impurity Scattering . . . . . . . . . . . . . . . . . . . . . . . . 6.4.7 Neutral Impurity Scattering . . . . . . . . . . . . . . . . . . . . . . . . 6.4.8 Plasmon Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4.9 Alloy Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.5 Mobility . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.5.1 Acoustic Phonon Scattering . . . . . . . . . . . . . . . . . . . . . . . . 6.5.2 Non–polar Optical Phonon Scattering . . . . . . . . . . . . . . . . 6.5.3 Polar Optical Phonon Scattering . . . . . . . . . . . . . . . . . . . . 6.5.4 Piezoelectric Potential Scattering . . . . . . . . . . . . . . . . . . . . 6.5.5 Inter–Valley Phonon Scattering . . . . . . . . . . . . . . . . . . . . . 6.5.6 Ionized Impurity Scattering . . . . . . . . . . . . . . . . . . . . . . . . 6.5.7 Neutral Impurity Scattering . . . . . . . . . . . . . . . . . . . . . . . . 6.5.8 Plasmon Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.5.9 Alloy Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7

Magnetotransport Phenomena . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.1 Phenomenological Theory of the Hall Effect . . . . . . . . . . . . . . . . . 7.2 Magnetoresistance Effects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2.1 Theory of Magnetoresistance . . . . . . . . . . . . . . . . . . . . . . . 7.2.2 General Solutions for a Weak Magnetic Field . . . . . . . . . 7.2.3 Case of Scalar Effective Mass . . . . . . . . . . . . . . . . . . . . . . 7.2.4 Magnetoresistance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3 Shubnikov–de Haas Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3.1 Theory of Shubnikov–de Haas Effect . . . . . . . . . . . . . . . . 7.3.2 Longitudinal Magnetoresistance Configuration . . . . . . . . 7.3.3 Transverse Magnetoresistance Configuration . . . . . . . . . . 7.4 Magnetophonon Resonance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4.1 Experiments and Theory of Magnetophonon Resonance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4.2 Various Types of Magnetophonon Resonance . . . . . . . . . 7.4.3 Magnetophonon Resonance Under High Electric and High Magnetic Fields . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4.4 Polaron Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

326 334 336 339 343 346 349 350 353 354 355 356 357 358 359 363 364 365 367 368 369 371 372 373 375 375 382 382 383 384 388 391 391 396 398 402 402 409 414 419 423 424

Contents

8

9

Quantum Structures 1 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1 Historical Background . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2 Two-Dimensional Electron Gas Systems . . . . . . . . . . . . . . . . . . . . . 8.2.1 Two-Dimensional Electron Gas in MOS Inversion Layer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2.2 Quantum Wells and HEMT . . . . . . . . . . . . . . . . . . . . . . . . 8.3 Transport Phenomena of Two-Dimensional Electron Gas . . . . . . . 8.3.1 Fundamental Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3.2 Acoustic Phonon Scattering and Non-Polar Optical Phonon Scattering . . . . . . . . . . . . . . . . . . . . . . . . . 8.3.3 Inter-Valley Phonon Scattering . . . . . . . . . . . . . . . . . . . . . . 8.3.4 Polar Optical Phonon Scattering . . . . . . . . . . . . . . . . . . . . 8.3.5 Piezoelectric Potential Scattering . . . . . . . . . . . . . . . . . . . . 8.3.6 Ionized Impurity Scattering . . . . . . . . . . . . . . . . . . . . . . . . 8.3.7 Surface Roughness Scattering . . . . . . . . . . . . . . . . . . . . . . 8.3.8 Screening Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3.9 Remote Ionized Impurity Scattering . . . . . . . . . . . . . . . . . 8.3.10 Mobility of a Two-Dimensional Electron Gas . . . . . . . . . 8.4 Mesoscopic Phenomena . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.4.1 Mesoscopic Region . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.4.2 Definition of Mesoscopic Region . . . . . . . . . . . . . . . . . . . . 8.4.3 Landauer Formula and Büttiker–Landauer Formula . . . . 8.4.4 Research in the Mesoscopic Region . . . . . . . . . . . . . . . . . 8.4.5 Aharonov–Bohm Effect (AB Effect) . . . . . . . . . . . . . . . . . 8.4.6 Ballistic Electron Transport . . . . . . . . . . . . . . . . . . . . . . . . 8.5 Quantum Hall Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.6 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quantum Structures 2 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1 Superlattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1.1 Kronig–Penney Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1.2 Effect of Brillouin Zone Folding . . . . . . . . . . . . . . . . . . . . 9.1.3 Tight Binding Approximation . . . . . . . . . . . . . . . . . . . . . . 9.1.4 sp 3 s ∗ Tight Binding Approximation . . . . . . . . . . . . . . . . . 9.1.5 Energy Band Calculations for Superlattices . . . . . . . . . . . 9.1.6 Second Nearest-Neighbor sp 3 Tight Binding Approximation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Quantum Dots . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.1 Addition Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.2 Exact Diagonalization Method . . . . . . . . . . . . . . . . . . . . . . 9.2.3 Hamiltonian for Electrons in a Quantum Dot . . . . . . . . . . 9.2.4 Diagonalization of N Electrons Hamiltonian Matrix . . . 9.2.5 Electronic States in Quantum Dots . . . . . . . . . . . . . . . . . . 9.2.6 Quantum Dot States in Magnetic Field . . . . . . . . . . . . . . .

xiii

427 427 428 428 437 445 445 447 450 452 456 458 460 463 466 476 483 483 486 488 493 494 495 497 510 511 515 515 515 517 520 523 523 530 538 538 543 545 547 549 550

xiv

Contents

9.2.7

Electronic States in Elliptic and Triangular Quantum Dots . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.3 Coulomb Blockade and Single Electron Transistor . . . . . . . . . . . . 9.4 Surface modulation of Two-dimensional Electron Gas and Weiss Oscillation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.5 Wannier–Stark Effect in Superlattices . . . . . . . . . . . . . . . . . . . . . . . 9.6 Bloch Oscillation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

559 563 567 570 570

10 Light Emission and Laser . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.1 Einstein Coefficients A and B . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.2 Spontaneous Emission and Stimulated Emission . . . . . . . . . . . . . . 10.3 Band Tail Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.4 Luminescence . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.4.1 Luminescence Due to Band to Band Transition . . . . . . . . 10.4.2 Luminescence Due to Excitons . . . . . . . . . . . . . . . . . . . . . 10.4.3 Luminescence via Impurities . . . . . . . . . . . . . . . . . . . . . . . 10.4.4 Luminescence in GaP and GaAsP via N Traps . . . . . . . . 10.4.5 Luminescence from GaInNAs . . . . . . . . . . . . . . . . . . . . . . 10.4.6 Light Emitting Diodes (LEDs) in Visible Region . . . . . . 10.5 Heterostructure Optical Waveguide . . . . . . . . . . . . . . . . . . . . . . . . . 10.5.1 Wave Equations for Planar Waveguide . . . . . . . . . . . . . . . 10.5.2 Transverse Electric Modes . . . . . . . . . . . . . . . . . . . . . . . . . 10.5.3 Transverse Magnetic Modes . . . . . . . . . . . . . . . . . . . . . . . . 10.5.4 Effective Refractive Index . . . . . . . . . . . . . . . . . . . . . . . . . . 10.5.5 Confinement Factor . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.5.6 Laser Oscillations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.6 Stimulated Emission in Quantum Well Structures . . . . . . . . . . . . . 10.6.1 Confinement in Quantum Well . . . . . . . . . . . . . . . . . . . . . 10.6.2 Optical Transition in Quantum Well Structures . . . . . . . . 10.6.3 Reduced Density of States and Gain . . . . . . . . . . . . . . . . . 10.6.4 Strain Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.6.5 Wurtzite Semiconductor Lasers . . . . . . . . . . . . . . . . . . . . . 10.6.6 Optical Gain of Nitride Quantum Well Structures . . . . . . 10.7 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

575 576 578 584 589 589 590 593 597 601 603 604 604 609 611 612 614 616 619 621 625 630 633 638 645 647 647

11 Wade Bandgap Semiconductor and Photonic Crystals . . . . . . . . . . . . 11.1 Energy Band Structures of Nitrides . . . . . . . . . . . . . . . . . . . . . . . . . 11.1.1 Energy Band Calculations of GaN, AlN, and InN . . . . . . 11.1.2 Energy Band Structures of Ternary Alloys . . . . . . . . . . . . 11.1.3 Spin–Orbit–Interaction and Valence Band Structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.2 Electron and Hole Mobilities of GaN . . . . . . . . . . . . . . . . . . . . . . . . 11.2.1 Acoustic Deformation Potential Scattering . . . . . . . . . . .

651 651 652 659

551 554

662 665 668

Contents

11.2.2 Piezoelectric Potential Scattering . . . . . . . . . . . . . . . . . . . . 11.2.3 Ionized Impurity Scattering . . . . . . . . . . . . . . . . . . . . . . . . 11.2.4 Polar Optical Phonon Scattering . . . . . . . . . . . . . . . . . . . . 11.2.5 Remote Impurity Scattering . . . . . . . . . . . . . . . . . . . . . . . . 11.2.6 Other Scatterings . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.2.7 Evaluation of Electron and Hole Mobility . . . . . . . . . . . . 11.3 SiC and Other Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.3.1 SiC . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.3.2 Electron Mobility in 4H-SiC . . . . . . . . . . . . . . . . . . . . . . . 11.4 Photonic Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.4.1 One-Dimensional Photonic Crystal . . . . . . . . . . . . . . . . . . 11.4.2 Two-Dimensional Photonic Crystal . . . . . . . . . . . . . . . . . . 11.4.3 Defects in Photonic Crystal . . . . . . . . . . . . . . . . . . . . . . . . 11.4.4 FDTD Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.5 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

xv

670 672 673 675 676 676 680 680 684 685 685 687 688 690 691 692

12 Answers for Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 695 Appendix A: Delta Function and Fourier Transform . . . . . . . . . . . . . . . . . . 733 Appendix B: Gamma Function . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 741 Appendix C: Uniaxial Stress and Strain Components in Cubic Crystals

745

Appendix D: Boson Operators . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 749 Appendix E: Random Phase Approximation and Lindhard Dielectric Function . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 755 Appendix F: Density Matrix . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 759 Appendix G: Spontaneous and Stimulated Emission Rates . . . . . . . . . . . . 763 Appendix H: Spin–Orbit Interaction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 769 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 777

Chapter 1

Energy Band Structures of Semiconductors

Abstract The physical properties of semiconductors can be understood with the help of the energy band structures. This chapter is devoted to energy band calculations and interpretation of the band structures. Bloch theorem is the starting point for the energy band calculations. Bloch functions in periodic potentials is derived here and a periodic function is shown to be expressed in terms of Fourier expansion by means of reciprocal wave vectors. Brillouin zones are then introduced to understand energy band structures of semiconductors. The basic results obtained here are used throughout the text. The energy band calculation is carried out first by obtaining freeelectron bands (empty lattice bands) which are based on the assumption of vanishing magnitude of crystal potentials and of keeping the crystal periodicity. Then we show that the energy band structures are calculated with a good approximation by the pseudopotential method with several Fourier components of crystal potential with the spin–orbit interaction. Also k · p perturbation method for energy band calculation is described in detail. The method is extended to obtain the full band structures of the elementary and compound semiconductors. In order to understand semiconductor physics the articles [1–10] are very useful not only for energy band structure but also throughout the textbook.

1.1 Free-Electron Model It is well known that the physical properties of semiconductors are understood with the help of energy band structures. The energy states or energy band structures of electrons in crystals reflect the periodic potential of the crystals and they can be calculated when we know the exact shape and the magnitude of the crystal potentials. The shape and the magnitude of the potential are not determined directly from any experimental methods, and thus we have to calculate or estimate the energy bands by using the assumed potentials. Many different approaches to calculations of energy bands have been reported, but in this textbook we will deal with several methods, © The Author(s), under exclusive license to Springer Nature Switzerland AG 2023 C. Hamaguchi, Basic Semiconductor Physics, Graduate Texts in Physics, https://doi.org/10.1007/978-3-031-25511-3_1

1

2

1 Energy Band Structures of Semiconductors

Fig. 1.1 One-dimensional crystal with periodic potential, where only several lattice points are included

which are not so difficult to understand. It is possible to carry out energy band calculations by using a PC commercially available. We begin with the most simplified method to calculate electronic states in a model crystal. For simplicity we consider a one-dimensional crystal with a periodic potential as shown in Fig. 1.1, and assume that each atom provides one free electron and that the atom has a charge of +e, forming an ion. The ion provides potential energy V (r ) = −e2 /4π0 r , where r is the distance from the central position of the ion. Therefore, the one-dimensional crystal has a potential energy consisting of the superposition of that of each atom, as shown in Fig. 1.1. From the figure we find the potential energy of the walls is higher than the inside potential and thus the electrons are confined between the walls. However, we have to note that the above results are derived from a very simplified assumption and the potential distribution is obtained without electrons. In a crystal there are many electrons and thus electron–electron interactions play a very important role in the potential energy distribution. Electron–electron interaction will be discussed in the case of plasmon scattering in Chap. 6 and in calculating the electronic states in quantum dots in Sect. 9. In the discussion of the energy band structure we will not deal with the electron–electron interactions and consider a simplified case where we calculate the electronic states for a single electron and then put many electrons in the energy states by taking the Pauli exclusion principle into account. The large conductivity in metals is understood to arise from the fact that many free electrons exist in the conduction band. Therefore such electrons have an energy higher than the potential maxima and lower than the confining wall potentials. In the extreme case we can make an approximation that the electrons are confined in a square potential well, as shown in Fig. 1.2, where we assume the potential is infinite at x = 0 and x = L. In such a case the electron energy may be obtained by solving the one-dimensional Schrödinger equation −

2 d 2 + V (x) Ψ (x) = EΨ (x), 2m dx 2

(1.1)

3

⁄

1.2 Bloch Theorem

Fig. 1.2 Simplified quantum well model and electronic states

and the solutions are given by the following relations: Ψ (x) = A sin(kn x) = A sin

πn

L 2 πn 2 2 2 k = · , E= 2m n 2m L πn (n = 1, 2, 3, . . .) kn = L

·x , (1.2)

Eigenfunctions and their energy level for n = 1, 2, 3, . . . are shown in Fig. 1.2. It is very easy to extend this one-dimensional model to the three-dimensional model, which will not be given here. We have to note that energy band structures are well understood by introducing periodic boundary conditions and the Bloch theorem shown in the following section.

1.2 Bloch Theorem When we introduce a translational vector T , the crystal potential has the periodicity V (r) = V (r + T ), and thus the squared wave function of the electron |Ψ (r)|2 has the same periodicity. The amplitude of the wave function Ψ (r) has an ambiguity of a phase factor exp(ik · r). The cyclic boundary condition in the case of a onedimensional crystal requires the condition that the wave function including the phase factor is the same at x and at x + L, and thus Ψ (x) = Ψ (x + L), where L is the length of the crystal. The results are summarized as follows [1]:

4

1 Energy Band Structures of Semiconductors

Ψ (r) = exp(ik · r)u k (r),

(1.3)

u k (r + T ) = u k (r),

(1.4)

2π (n x a∗ + n y b∗ + n z c∗ ), N

(1.5)

k=

where k is called the electron wave vector and T = n 1 a + n 2 b + n 3 c is the translational vector defined by using the fundamental vectors a, b, c with n 1 , n 2 , n 3 = 0, ±1, ±2, . . . . The function Ψ (r) is called the Bloch function and the function u(r) is the periodic function of the translational vector, u(r + T ) = u(r).

(1.6)

The wave vector k is expressed in terms of the reciprocal lattice [1], b×c , a · (b × c) c×a , b∗ = a · (b × c) a×b c∗ = , a · (b × c)

a∗ =

(1.7) (1.8) (1.9)

which satisfy the following relations [1]: a∗ · a = b∗ · b = c∗ · c = 1, ∗

∗

∗

(1.10) ∗

a · b = a · c = · · · = c · a = c · b = 0.

(1.11)

The reciprocal lattice vector is defined by G n = 2π(n 1 a∗ + n 2 b∗ + n 3 c∗ ), where n 1 , n 2 , n 3 are integers.

(1.12)

Periodic functions with the lattice vectors a, b, c are Fourier expanded with the reciprocal lattice vectors, u k (r) =

A(G m ) exp(−iG m · r),

(1.13)

V (G n ) exp(−iG n · r),

(1.14)

m

V (r) =

n

where A(G m ) and V (G n ) are Fourier coefficients. The coefficients are obtained by the inverse Fourier transformation,

1.3 Nearly Free Electron Approximation

A(G i ) =

1 Ω

V (G j ) =

1 Ω

5

Ω

exp(+iG i · r)u k (r)d3 r,

(1.15)

exp(+iG j · r)V (r)d3 r,

(1.16)

Ω

where Ω is the volume of the unit cell of the crystal. From the definition of the reciprocal lattice vector (1.12), we can easily prove the following important relation (see Appendix A.2), 1 Ω

Ω

exp [i (G m − G n ) · r] d3 r = δmn .

(1.17)

Here we have used the Kronecker delta defined by δmn =

1 for m = n . 0 for m = n

(1.18)

1.3 Nearly Free Electron Approximation For simplicity we begin with the one-dimensional case. From (1.16) we obtain V (G n ) =

1 a

a

V (x) exp(iG n x)dx,

(1.19)

0

which gives the following zeroth-order Fourier coefficient, V (0), when we put G n = 0 in the above equation 1 V (0) = a

a

V (x)dx.

(1.20)

0

The coefficient V (0) gives the average of the potential energy. In the case of threedimensional crystals, the coefficient V (0) =

1 Ω

Ω

V (r)d3 r

(1.21)

also gives the average value of the potential energy V (r) in the unit cell Ω. In the following we measure the energy from V (0) and thus we put V (0) = 0. The electronic states of an electron in the periodic potential V (r) are given by solving the Schrödinger equation, 2 2 ∇ + V (r) Ψ (r) = E(k)Ψ (r). − 2m

(1.22)

6

1 Energy Band Structures of Semiconductors

Putting (1.13) into (1.3), we obtain 1 A(G n ) exp(−iG n · r), Ψ (r) = √ exp(ik · r) Ω n 1 = √ A(G n ) exp [i (k − G n ) · r] , Ω n

(1.23)

√ where the factor 1/ Ω is introduced to normalize the wave function Ψ (r) in the unit cell. Putting (1.14) and (1.23) into (1.22), the following result is obtained:

1 2 2 (k − G n ) − E(k) + V (G m ) exp(−iG m · r) √ Ω n 2m m × A(G n ) exp [i(k − G n ) · r] = 0.

(1.24)

√ Multiplying (1/ Ω) exp[−i(k − G l ) · r] to the both sides of the above equation and integrating in the unit cell with the help of (1.17), we find that the first and the second terms are not 0 for n = l, and that the third term is not 0 for −(G m + G n ) = −G l (or G l − G n = G m ). Therefore, the integral is not 0 only in the case of m = l − n, and we obtain the following result:

2 V (G l − G n )A(G n ) = 0. (k − G l )2 − E(k) A(G l ) + 2m n

(1.25)

In the free-electron approximation of Sect. 1.1, we assumed the potential is given by the square well shown in Fig. 1.2, and thus the Fourier coefficients are V (G m ) = 0 (m = 0). As stated above, we take the energy basis at V (0) and put V (r) = 0. Then (1.22) gives the following solution: E(k) =

2 k 2 , 2m

1 Ψ (r) = √ A(0) exp(ik · r). Ω

(1.26) (1.27)

In the nearly free electron approximation, the potential energy is assumed to be very close to the square well shown in Fig. 1.2 and the Fourier coefficients V (G l ) are assumed to be negligible except for V (0). Therefore, we replace the energy E(k) by (1.26) in (1.25) and only the term including A(0) is kept in the second term. This assumption results in

2 2 k 2 2 A(G l ) + V (G l )A(0) = 0. (k − G l ) − 2m 2m

(1.28)

1.3 Nearly Free Electron Approximation

7

From this equation we obtain A(G l ) =

V (G l )A(0) . (2 /2m) k 2 − (k − G l )2

(1.29)

In the nearly free electron approximation, the electron wave function may be approximated by (1.27). In other words, the terms A(G l ) are very small except G l = 0. From the result given by (1.29), however, we find that the term A(G l ) is very large when (k − G l )2 ≈ k 2 . The condition is shown by the following equation: (k − G l )2 = k 2 ,

(1.30)

which gives rise to Bragg’s law (law of Bragg reflection) and determines the Brillouin zones of crystals. When the electron wave vector ranges close to the value given by (1.30), we keep the term A(G l ) in addition to the term A(0), and neglect the other terms. Then we obtain the following relations from (1.25):

2 2 k − E(k) A(0) + V (−G l )A(G l ) = 0, 2m 2 2 (k − G l ) − E(k) A(G l ) + V (G l )A(0) = 0. 2m

(1.31a) (1.31b)

The solutions of the above equations are obtained under the condition that the coefficients A(0) and A(G l ) are both not equal to 0 at the same time. The condition is satisfied when the determinant of (1.31a) and (1.31b) is 0, which is given by

V (−G l ) (2 /2m)k 2 − E(k) = 0. (2 /2m)(k − G l )2 − E(k) V (G l )

(1.32)

From this we obtain 1 2 2 k + (k − G l )2 E(k) = 2 2m 2 2

2 ± k 2 − (k − G l )2 + 4|V (G l )|2 , 2m

(1.33)

where the relation V (−G l ) = V ∗ (G l ) is used. When k 2 = (k − G l )2 and thus 2k · G l = G l2 , we find 2 k 2 ± |V (G l )|, (1.34) E(k) = 2m which means that there exists an energy gap of 2|V (G l )|.

8

1 Energy Band Structures of Semiconductors

Here we will apply the results to a one-dimensional crystal. Replacing G l by G n in (1.33) and using the relation G n = 2πn/a(n = 0, ±1, ±2, ±3, . . .), we have the following equation: 2πn 2 1 2 2 E(k) = k + k− 2 2m a 2 2 2πn 2 2 k2 − k − ± + 4|V (G n )|2 . 2m a

(1.35)

Therefore, E(k) ∼ = 2 k 2 /2m is satisfied, except in the region close to the condition 2 2 k = G n = (k − 2πn/a)2 or k = nπ/a. This result gives the choice of ± in (1.35). Taking account of the sign of the square root, in the region k < (k − G n )2 we should choose the minus sign and in the region k > (k − G n )2 we have to choose the plus sign in (1.35). Therefore, in the region k ≈ nπ/a > 0, we obtain the following relations: nπ : a nπ : k≥ a k≤

2 k 2 − |V (G n )|, 2m 2 k 2 E(k) = + |V (G n )|. 2m E(k) =

(1.36) (1.37)

Using the above relations and plotting E(k) as a function of k, we obtain the results shown in Fig. 1.3a. Such a plot of energy in the whole region of the k vector shown in Fig. 1.3a is called the “extended zone representation”. In such a one-dimensional crystal model with N atoms, however, the electron system has N degrees of freedom

2

3

2

2

2

2

2

3

Fig. 1.3 Energy band structure of one-dimensional crystal obtained from the nearly free electron approximation. a Extended zone representation, b reduced zone representation, and c energy bands in real space. Energy in units of (2 /2m)(π/a)2

1.4 Reduced Zone Scheme

9

and thus the wave vector of the electron may take N values in the range −π/a < k ≤ π/a, corresponding to the first Brillouin zone. When we take this fact into account, the energy can be shown in the first Brillouin zone −π/a < k ≤ π/a. This may be understood from the fact that the wave vectors k and k + G m are equivalent because of the equivalence of the wave functions with these two wave vectors from the result shown by (1.23) (see Sect. 1.4). Using this result we easily find that the region −2π/a < k ≤ −π/a in Fig. 1.3a is moved in the region 0 ≤ k ≤ π/a of the first Brillouin zone by adding G = 2π/a and that π/a ≤ k ≤ 2π/a is moved into −π/a ≤ k ≤ 0 by adding G = −2π/a. The region −2π/a < k ≤ −π/a and π/a ≤ k ≤ 2π/a is called the second Brillouin zone. The 3rd Brillouin zone, 4th Brillouin zone, . . . are defined in the same manner and they can be reduced to the first Brillouin zone. The energy plotted in the first Brillouin zone is shown in Fig. 1.3b and this is called the “reduced zone representation”. Usually the energy band structure is shown in the reduced zone scheme. Figure 1.3c shows the allowed energy region with the shaded portion and the region is called the “allowed band”, while electrons cannot occupy the region in between the allowed bands, which is called the “forbidden band” or “energy band gap”, where the horizontal axis corresponds to the coordinate of real space.

1.4 Reduced Zone Scheme The Bloch function in a crystal is given by 1 A(G l )ei(k−Gl )·r . ψ(r) = √ Ω l

(1.38)

Let us examine the phase between two Bloch functions with k-vectors k − G l and k. The phase difference at r between exp[ik · r] and exp[i(k − G l ) · r] is G l · r. The phase difference of the Bloch functions at a point displaced by the translational vector T , r + T , is easily obtained in the following way. Since we have the relations T = n 1 a + n 2 b + n 3 c,

(1.39)

G l = 2π(m 1 a∗ + m 2 b∗ + m 3 c∗ ),

(1.40)

G l · T = 2π(m 1 n 1 + m 2 n 2 + m 3 n 3 ) = 2πn,

(1.41)

and we obtain k · (r + T ) − (k − G l ) · (r + T ) = G l · r + G l · T = G l · r + 2πn,

(1.42)

10

1 Energy Band Structures of Semiconductors

where n is an integer and the relation a∗ · a = 1 is used. From the above considerations we find the following results. The phase differences between the two functions exp[ik · r] and exp[i(k − G l ) · r] at two different positions r and r + T differs by the amount 2πn and thus the Bloch function ψ(r) behaves in the same way at the position displaced by the translational vector T . In other words, we can conclude that electrons with k and k − G l are equivalent. Therefore, we can reduce the electronic state of an electron with wave vector k into the state k − G l , and represent the electronic states in the first Brillouin zone. This procedure is called the reduced zone scheme and hereafter the energy band is represented in the reduced zone scheme. On the other hand, the energy band representation over the whole k region is called the extended zone scheme.

1.5 Free–Electron Bands (Empty–Lattice Bands) 1.5.1 First Brillouin Zone In order to calculate energy band structures of a semiconductor the following procedures are required to carry out the calculations. These are 1. Calculate the first Brillouin zone. 2. Calculate the energy band structures in the limit of zero potential energy. This procedure is to obtain the free-electron bands or empty-lattice bands and plot the energy as a function of wave vector k in the reduced zone scheme. 3. Then calculate the energy bands using an appropriate method. In the energy band calculation the most important procedure is to obtain the emptylattice bands, which are calculated by assuming zero lattice potential V (r) = 0 and keeping the lattice periodicity. In other words we assume the wave functions are given by the free-electron model with the wave vectors of the electrons in the periodic potential. Such an energy band structure is called empty-lattice bands or free-electron bands and thus the band structure exhibits the characteristics of the lattice periodicity. Here we will show an example of empty-lattice bands in the case of the facecentered cubic (fcc) lattice. First, we calculate the Brillouin zone of the fcc lattice. Figure 1.4a shows the fcc structure. The diamond structure is obtained by displacing the lattice atoms by the amount (a/4, a/4, a/4), which is shown in Fig. 1.4b. Therefore, the diamond structure belongs to the fcc structure. Diamond (C), Si and Ge have this diamond structure. On the other hand, the displaced lattice atoms are different from the original atoms, and the structure is called the zinc-blende structure, which is shown in Fig. 1.4c. Crystals such as GaAs, GaP, AlAs, InAs, InSb belong to the zincblende structure. The fundamental vectors and volume v of a fcc lattice are defined by

1.5 Free–Electron Bands (Empty–Lattice Bands)

11

Fig. 1.4 a Face-centered cubic lattice, b the diamond crystal lattice is obtained by displacing the lattice atoms of (a) by (a/4, a/4, a/4), c when the displaced lattice atoms are different from the original lattice atoms, the crystal structure is called the zinc-blende crystal structure

a a a (ex + e y ), b = (e y + ez ), c = (ez + ex ), 2 2 2 v = a · (b × c) a 3 a 3 1 (ex + e y ) · [(e y + ez ) × (ez + ex )] = 2 = a3, = 2 2 4

a=

(1.43)

where e is the unit vector. The reciprocal vectors of the fcc structure are obtained as follows: b × c a 2 (e y + ez ) × (ez + ex ) a 2 (ex − ez + e y ) = = v 2 v 2 a 3 /4 1 = (ex + e y − ez ), (1.44) a

a∗ =

b∗ = c∗ =

1 (−ex + e y + ez ), a

(1.45)

1 (ex − e y + ez ). a

(1.46)

From these results we find that the reciprocal lattices of the fcc lattice form bodycentered cubic lattices. Therefore, the reciprocal lattice vectors G of the fcc lattice are given by G = 2π(n 1 a∗ + n 2 b∗ + n 3 c∗ ). (1.47) The Brillouin zone of the fcc lattice is defined by k 2 = (k − G l )2

(1.48)

2k · G l = G l2 .

(1.49)

or

12

1 Energy Band Structures of Semiconductors

Fig. 1.5 The first Brillouin zone of a face-centered cubic lattice and b body-centered cubic lattice

Using the above equation the first Brillouin zone is easily calculated, as shown in Fig. 1.5a. For comparison the first Brillouin zone of body-centered cubic lattices, which form face-centered cubic lattices, is shown in Fig. 1.5b. Since the lattice potential is 0 in the empty-lattice model, the energy of an electron is given by the free-electron model: E(k) =

2 2 k . 2m

(1.50)

We plot the energy E(k) versus wave vector k curves in the reduced zone scheme, using the relation (1.51) k = k − G, and choose k in the first Brillouin zone. Then the empty lattice bands are given by E(k ) =

2 2 k +G . 2m

(1.52)

1.5.2 Reciprocal Lattice Vectors of fcc Crystal In the next Sect. 1.6, we discuss detailed treatment of pseudopotential method for energy band calculations and show how to program the energy band calculation. For this purpose we evaluate the matrix elements of the pseudopotential Hamiltonian of a face centered cubic (fcc) crystal. First, we calculate the reciprocal lattice vectors. Inserting (1.44)–(1.46) into (1.47), we obtain the following relations for the reciprocal vectors

1.5 Free–Electron Bands (Empty–Lattice Bands)

G=

2π (n 1 − n 2 + n 3 )ex + (n 1 + n 2 − n 3 )e y a +(−n 1 + n 2 + n 3 )ez

13

(1.53)

and thus the x, y, z components of G, and G 2 are 2π (n 1 − n 2 + n 3 ) , a 2π Gy = (n 1 + n 2 − n 3 ) , a 2π Gz = (−n 1 + n 2 + n 3 ) , a G 2 = G 2x + G 2y + G 2z 2 2π (n 1 − n 2 + n 3 )2 + (n 1 + n 2 − n 3 )2 ≡ a +(−n 1 + n 2 + n 3 )2 . Gx =

(1.54) (1.55) (1.56) (1.57)

(1.58)

Using these relations the reciprocal wave vectors of a face–centered cubic lattice are easily evaluated, by putting n 1 , n 2 , n 3 = ±0, ±1, ±2, ±4, ±5, . . .. It is very convenient to introduce dimensionless lattice vectors K defined by, K=

a G. 2π

(1.59)

The calculated reciprocal lattice vectors K are listed in Table 1.1, where G x , G y , G z are obtained by multiplying K by (2π/a) and they are tabulated for K 2 = K x2 + K y2 + K z2 = 0 ∼ 27.

1.5.3 Free Electron Bands Free electron bands (empty lattice bands) are easily calculated using the results of Table 1.1, which are shown in Fig. 1.6 for a crystal with lattice constant a = 5.43 Å. This kind of energy band plotting is called as full band representation or full band structure. For better understanding we list several reciprocal lattice vectors from the lowest orders, which are given by (see (1.53) and Table 1.1)

14

1 Energy Band Structures of Semiconductors

Table 1.1 Reciprocal lattice vectors of a face-centered cubic lattice calculated from (1.53), where K x = (a/2π)G x , K y = (a/2π)G y , K z = (a/2π)G z . Here the vectors are obtained for K 2 = K x2 + K y2 + K z2 from 0 to 27 [K ]

Permutations

[000] [111] [200] [220]

[000] ¯ [1¯ 1¯ 1] ¯ [020] ¯ [2¯ 20] ¯ [022] ¯ ¯ ¯ [131] ¯ [311] ¯ [311] ¯ ¯ [22¯ 2] ¯ [040] ¯ [3¯ 3¯ 1] ¯ [133] ¯ [313] ¯ [2¯ 40] ¯ [240]

[311]

[222] [400] [331]

[420]

[422]

[511]

[333]

[204] ¯ [2¯ 4¯ 2] ¯ ¯ [422] ¯ 2] ¯ [24 ¯ [511] ¯ 1] ¯ [51 ¯ [115] [333]

K2

¯ [1¯ 11] ¯ [200] ¯ [02¯ 2]

¯ [11¯ 1] ¯ [002] ¯ 2] ¯ [20

¯ 1] ¯ [11 [002] ¯ [022]

[202] ¯ [3¯ 1¯ 1] ¯ ¯ [113] ¯ 1] ¯ [13 ¯ ¯ [222] ¯ [400] ¯ [3¯ 31] ¯ [313] ¯ [133] ¯ [4¯ 20] ¯ [420]

[022] ¯ [1¯ 31] ¯ [11¯ 3] ¯ [131] ¯ [22¯ 2] ¯ [004] ¯ [1¯ 3¯ 3] ¯ [33¯ 1] ¯ [313] ¯ [04¯ 2] ¯ [024] ¯ [402] ¯ ¯ [242] ¯ [22¯ 4] ¯ [224] ¯ [1¯ 51] ¯ [1¯ 1¯ 5] ¯ [115]

[220] ¯ [3¯ 11] ¯ ¯ [113] [113] ¯ 2] ¯ [22 [004] ¯ [3¯ 1¯ 3] ¯ [331] ¯ [133] ¯ 2] ¯ [40 ¯ [204] ¯ [042] ¯ ¯ [422] ¯ 4] ¯ [22

[024] [422] ¯ [422] ¯ [242] ¯ [1¯ 5¯ 1] ¯ [511] ¯ [115] ¯ [3¯ 33]

¯ [33¯ 3]

[224] ¯ [5¯ 1¯ 1] ¯ [1¯ 15] ¯ 1] ¯ [15 ¯ 3] ¯ [33

G0 = G3 = G4 = G8 = G 11 =

¯ [111] [200] ¯ [202]

¯ [111] [020] ¯ [220]

¯ [111]

[111]

¯ [220]

¯ [202]

¯ [1¯ 1¯ 3] ¯ [113] ¯ [311] ¯ [222] [400] ¯ [1¯ 33] ¯ 1] ¯ [33

¯ [13¯ 1] ¯ [113] ¯ [131] ¯ [222] [040] ¯ [3¯ 13] ¯ [331] ¯ [331] ¯ [402] ¯ [024]

¯ [131] ¯ [113] [311] ¯ [222]

¯ 1] ¯ [31 ¯ ¯ [311] [131] [222]

¯ [13¯ 3] ¯ [31¯ 3]

¯ 3] ¯ [31 ¯ 3] ¯ [13

[331] ¯ [02¯ 4] ¯ [420]

[313] ¯ 4] ¯ [20 ¯ [240]

[042] ¯ [2¯ 24] ¯ [224] ¯ [242] [115] ¯ [51¯ 1]

[420] ¯ [24¯ 2] ¯ ¯ [422] [422] ¯ [15¯ 1] ¯ ¯ 5] [11 ¯ [151] ¯ [333]

[240] ¯ [242] ¯ [422] [242] ¯ [151] ¯ [511]

[133] ¯ [042] ¯ [204] [402] ¯ [2¯ 2¯ 4] ¯ [224] ¯ [422] ¯ ¯ [511] ¯ [11¯ 5] ¯ [151] ¯ [333]

[511] ¯ [333]

2π [0, 0, 0], a 2π [±1, ±1, ±1], a 2π [±2, 0, 0], a 2π [±2, ±2, 0], a 2π (±3, ±1, ±1). a

[151] ¯ [3¯ 3¯ 3]

0 3 4 8 11

12 16 19

20

24

27

27

(1.60a) (1.60b) (1.60c) (1.60d) (1.60e)

Putting these values in (1.52), the empty-lattice bands (free-electron bands) are easily calculated. In the following we use k instead of k and take account of k in the first Brillouin zone. The free electron band is shown in Fig. 1.6. As an example we

1.5 Free–Electron Bands (Empty–Lattice Bands)

15

Fig. 1.6 Free electron bands (empty lattice bands) of a face-centered lattice with lattice constant a = 5.43 Å are plotted as a function of electron wave vector k along the direction shown in Fig. 1.5a, where the energy range is 0 ∼ 30 eV. This kind of plotting is called full band representation

calculate the energy bands along the direction 100 in the k-space shown in Fig. 1.5. In other words, we calculate the energy band structures E versus k from the Γ point to the X point. Since k y = k z = 0 in this direction, putting the reciprocal lattice vectors into (1.50), the energy is given by the following equations: G 0 : E = k x2 ,

(1.61a)

G 3 : E = (k x ± 1)2 + (±1)2 + (±1)2 , (k x − 1)2 + 2 (4-fold degeneracy) , = (k x + 1)2 + 2 (4-fold degeneracy) ⎧ 2 ⎨ k x + 4 (4-fold degeneracy) G 4 : E = (k x − 2)2 (single state) , ⎩ (k x + 2)2 (single state)

(1.61b) (1.61c)

where the energy is measured in the units 2 (2π/a)2 /2m and the wave vector k in the units 2π/a. When we plot these relations, we obtain the curves shown in Fig. 1.7. Next we calculate the E versus k curves in the 111 direction of k-space, or along the direction from the Γ point to the L point. The results are 2 , G 0 : E = k x2 + k 2y + k z2 ≡ k111

(1.62a)

G 3 : E = (k x ± 1) + (k y ± 1) + (k z ± 1) , ⎧ 2 2 2 ⎪ ⎨ (k x ± 2) + k y + k z (2-fold degeneracy) G 4 : E = k x2 + (k y ± 2)2 + k z2 (2-fold degeneracy) , ⎪ ⎩ 2 k x + k 2y + (k z ± 2)2 (2-fold degeneracy) 2

2

2

(1.62b) (1.62c)

16

1 Energy Band Structures of Semiconductors

Fig. 1.7 Empty–lattice bands (free-electron bands) of a face-centered cubic lattice in the Brillouin zone including Γ , X and L points. 000 , 111 , 200 , and 220 represent the reciprocal lattice vectors G 0 , G 3 , G 4 , and G 8 , respectively, and the numbers in ( ) show the degeneracy of the wave functions. See the text for detail

√ 2 where k x2 + k 2y + k z2 = k111 and k x = k y = k z = k111 / 3. Using these results we obtain the energy bands, E versus k curves in the direction 111 , which are shown in the left half of Fig. 1.7. In Fig. 1.7, the notation of the point group for Oh is used to represent the symmetry properties of the Brillouin zone edge. Note here that the energy E is expressed in units of 2 (2π/a)2 /2m.

1.6 Pseudopotential Method In this section we will concern with the energy band calculations based on the pseudopotential method. First we introduce local pseudopotential theory in which the locality of the core states are ignored, and we will show how to calculate the energy band structures of the diamond and zinc blende semiconductors by using small number of the pseudopotentials. In the later section we will discuss the nonlocal pseudopotential theory in which the core potential of the occupied states is taken into account.

1.6.1 Local Pseudopotential Theory The electronic states in a crystal are obtained by solving the following non-relativistic Schrödinger equation in the one-electron approximation: 2 2 − ∇ + V (r) Ψn (r) = En (k)Ψn (r). 2m

(1.63)

1.6 Pseudopotential Method

17

However, it is possible only when we know the crystal potential V (r). In the following we will express the wave function Ψn (r) by the ket vector as |Ψn (r) and show how the Schrödinger equation is solved to a good approximation by using empirical parameters, known as pseudopotentials, and the orthogonality of the wave functions [6–8, 11–13]. The idea of the pseudopotential method is based on the assumption that the real crystal potential V (r) is given by the sum of the attractive core potential and the weak repulsive potential (to keep the valence electrons out of the core). The addition of the repulsive potential to the core potential cancels the real potential, resulting in a weak net potential (pseudopotential). The introduction of the pseudopotential enables us to treat valence electrons as nearly free electron approximation or to solve Schödinger equation with a small number of Fourier components of the pseudopotential. First, we assume the electron wave functions of the core states and their energies are given by |φ j and E j , respectively. We then have H |φ j = [H0 + Vc (r)] |φ j = E j |φ j ,

(1.64)

where Vc (r) is the attractive core potential, and H0 = −

2 2 ∇ . 2m

(1.65)

The true wave function |Ψ of an electron is then expressed as the sum of a smooth wave function |χn (r) of a valence electron (subscript n is the band index) and a sum over occupied core states |φ j ; |Ψ = |χn +

b j |φ j .

(1.66)

j

Since the true wave function is orthogonal to the core states, the expansion coefficient b j is determined by the orthogonality φ j |Ψ = 0 as follows. φ j |Ψ = φ j |χn +

φ j |b j φ j j

= φ j |χn + b j = 0,

(1.67)

which gives b j = −φ j |χn and thus we obtain |Ψ (k, r) = |χn (k, r) −

φ j |χn |φ j .

(1.68)

j

We have to note here that |χn is defined as a smooth wave function for a valence electron and called as the pseudo-wave-function. As in the case of nearly free electron approximation, we calculate energy band structures by using plane waves for

18

1 Energy Band Structures of Semiconductors

|χn (k, r) and in this scheme (1.68) is called the OPW (orthogonalized plane wave). Substituting (1.68) into (1.63) we find φ j |χn H |φ j = En (k) |χn − φ j |χn |φ j , H |χn − j

(1.69)

j

and then we obtain the following relation: H |χn +

[En (k) − E j ]|φ j φ j |χn = En (k)|χn .

(1.70)

j

We introduce a new parameter according to the definition of Cohen and Chelikowsky [6] Vr (r) = [En (k) − E j ]|φ j φ j |, (1.71) j

or Vr (r)|χn =

[En (k) − E j ]|φ j φ j |χn .

(1.72)

j

This term acts like a short-ranged non-Hermitian repulsive potential. Using this definition we obtain the following equation. [H + Vr (r)]|χn = En (k)|χn .

(1.73)

If H is separated into a kinetic energy H0 = −(2 /2m)∇ 2 and attractive core potential Vc (r), then (1.73) becomes 2 2 ∇ + Vc (r) + Vr (r) |χn = En (k)|χn , − 2m

(1.74)

where En (k) is the energy of the band we are interested in. There exists the following inequality between the energies of the core states, E j , and the energies of the valence and conduction bands, En (k): (1.75) En (k) > E j , and thus we find from (1.72) that Vr (r) > 0.

(1.76)

[H0 + Vps (r)]|χn = En (k)|χn , Vps (r) = Vc (r) + Vr (r),

(1.77) (1.78)

We may rewrite (1.74) as

1.6 Pseudopotential Method

19

Fig. 1.8 Schematic plot of pseudopotential in real space (after Cohen and Chelikowsky [6])

and it may be possible to make Vps small enough, since the attractive core potential Vc (r) < 0 and the repulsive potential Vr (r) > 0 cancel each other. The new potential Vps (r) is called the pseudopotential. Since the pseudopotential Vps is the sum of the attractive long–range potential Vc and a short–range repulsive potential Vr , Vps becomes weak long–range attractive regions away from the core and weakly repulsive or attractive regions near the core (see Fig. 1.8 [6]). The pseudopotential Vps (r) is also periodic, and we can expand it as the Fourier series Vps (G j )e−iG j ·r , (1.79) Vps (r) = j

where the Fourier coefficients Vps (G j ) are given by 1 Vps (G j ) = √ Ω

Ω

Vps (r)eiG j ·r d3 r.

(1.80)

For the reason stated above the potential Vps (r) may be chosen as small as possible, and thus we choose Vps (G j ) so that the potential Vps (G j ) is expressed with a small number of the Fourier coefficients Vps (G j ); in other words, we may keep several values of Vps (G j ) and neglect the other values because of their smallness. We should note that |Vps (r)| is smaller than |V (r)|, but it does not mean that V (r) converges with only a small number of its Fourier coefficients. The empirical pseudopotential method is based on the approximation that the Fourier coefficients of Vps (r) are empirically chosen so that the shape of the critical points and their energies show good agreement with experimental observation. Energy band calculations based on the empirical pseudopotential method take into account as few the pseudopotentials Vps (G j ) as possible and use the Bloch functions of the free-electron bands for the wave functions |χn . The energy bands are obtained by solving

20

1 Energy Band Structures of Semiconductors

2 2 − ∇ + Vps (r) |χn (r) = En |χn (r), 2m

(1.81)

1 i(k+G j )·r |χn (r) = √ e , Ω j

(1.82)

Vps (r) =

Vps (G j )eiG j ·r .

(1.83)

j

Then the energy band structures are calculated by solving the equation, √ following where the jth component is given by dropping the factor (1/ Ω) j : 2 2 − Vps (G j )eiG j ·r ei(k+G j )·r = En (k)ei(k+G j )·r . ∇ + 2m j

(1.84)

The eigenvalues and eigen functions of the above equation are easily obtained by solving the following matrix equation. First, we introduce pseudopotential Hamiltonian by 2 2 ∇ + Vps (r), Hps = − (1.85) 2m and rewrite (1.84) as Hps |k + G j = En (k)|k + G j ,

(1.86)

1 |k + G j = √ ei(k+G j )·r . Ω

(1.87)

Then the solutions are equivalently obtained by solving the determinant |||k + G i |Hps |k + G j − E(k)δi, j || = 0,

(1.88)

where the matrix elements of the Hamiltonian Hps are written as k + G i |Hps |k + G j =

2 (k + G i )2 δ G i ,G j + Vps (G j − G i ). 2m

(1.89)

When we know the pseudopotential form factors Vps (G j − G i ), the energy band calculations are straightforward by solving the eigen equation (1.88). In the next subsection we will deal with the evaluation of non–vanishing pseudopotential form factors.

1.6 Pseudopotential Method

21

1.6.2 Pseudopotential Form Factors Once we know the Fourier coefficients Vps (G j ), the solutions of (1.88) are easily calculated with a personal computer. It is very interesting to point out that the calculated energy bands using the reciprocal wave vectors given by (1.60a)–(1.60e) and the free-electron Bloch functions show very reasonable results, where only several pseudopotential parameters are used. The most important contribution to the energy band calculation was done by Cohen and Bergstresser [11], where they carried out very detailed calculations of energy band structures for several semiconductors with diamond and zinc blende crystal structures as discussed later. First we explain the pseudopotential parameters. In general a unit cell of a crystal contains a single atom or multi–atoms and thus the pseudopotential is expressed as [12] Vps (r) =

V (G j )e−iG j ·r ,

(1.90a)

Sα (G j )Vα (G j ),

(1.90b)

j

V (G j ) =

α

1 −iG j ·Rαm e , Nα cell m 1 Vα (G j ) = eiG j ·r Vpsα (r)d3 r. Ωα Sα (G j ) =

(1.90c) (1.90d)

Derivation of the above relations is understood by taking account of multi–atoms in the unit cell α V (G j )e−iG j ·r → Vα (G j )e−iG j ·(r+Rm ) , j

j

α cell m

where Sα (G) is called a structure factor, Nα is the number of atomic species α present, Rαm is the position of the mth atom of the αth species, and Ωα is the atomic volume. Here the crystalline potential is assumed to be a sum of local atomic pseudopotential Vpsα (r). The diamond-type crystal structure such as Ge and Si contains two atoms A and B (A = B) in the unit cell (Nα = 2), and the zinc-blende-type crystal structure has two different atoms A and B (A = B) (Nα = 2). When a new vector τ = (a/8)(111) is defined, the atomic positions of A and B are given by R A = −τ and R B = +τ , respectively. Taking the origin of coordinates to be the center of those two atoms, the structure factors are written as SA (G j ) =

1 iG j ·τ 1 e , SB (G j ) = e−iG j ·τ 2 2

(1.91)

22

1 Energy Band Structures of Semiconductors

and thus the pseudopotential form factor V (G) is given by 1 VA (G j )eiG j ·τ + VB (G j )e−iG j ·τ 2 = V S (G j ) cos(G j · τ ) + iV A (G j ) sin(G j · τ ).

V (G j ) =

(1.92)

Here we introduce following new parameters V S (G j ) = [VA (G j ) + VB (G j )]/2,

(1.93a)

V (G j ) = [VA (G j ) − VB (G j )]/2,

(1.93b)

A

where V S and V A are called the symmetric and antisymmetric form factors, respectively. The structure factor plays an important role in electronic properties such as energy band structure, diffraction effect and so on. S S (G j ) = cos(G j · τ ) and S A (G j ) = sin(G j · τ ) are the real part and imaginary part of the structure factor. From the definition of diamond-type crystal we have V A (G j ) = 0 and the structure factor reduces to cos(G j · τ ). In Table 1.2 the pseudopotentials are defined by using the relations V S (G j ) = V jA and V A (G j ) = V jA , where G j is defined by (1.60a)–(1.60e). As shown in Table 1.2 some of the pseudopotentials V S (G j ) and V A (G j ) vanish. This may be understood from the following considerations. The symmetric component of the pseudopotential is written as a G jx + G jy + G jz . V S (G j ) cos G j · τ = V S (G j ) cos 8

(1.94)

Let’s examine the pseudopotentials for the reciprocal vectors Eq.(1.60a)–(1.60e). The pseudopotentials for smaller values of G j are evaluated as V S (G 0 ) cos (G 0 · τ ) = V S (G 0 ),

π

[±1 ± 1 ± 1] = 0, 4 π V S (G 4 ) cos (G 4 · τ ) = V S (G 4 ) cos [±2] = 0, 4 π S S V (G 8 ) cos (G 8 · τ ) = V (G 8 ) cos [±2 ± 2] = 0, 4 π S S V (G 11 ) cos (G 11 · τ ) = V (G 11 ) cos [±3 ± 1 ± 1] = 0. 4 V S (G 3 ) cos (G 3 · τ ) = V S (G 3 ) cos

Therefore the symmetric components of the pseudopotentials V S (G 0 ) = V0S , S remain and V S (G 4 ) = V4S will not V S (G 3 ) = V3S , V S (G 8 ) = V8S , V S (G 11 ) = V11 contribute. In a similar fashion, there is no contribution from the antisymmetric components of the pseudopotential V A (G 0 ) = V0A and V A (G 8 ) = V8A . These results give the pseudopotentials for smaller values of |G j | in Table 1.2, where we find that pseudopotentials of large |G j | are diminished. Since the energy bands calculated with

1.6 Pseudopotential Method

23

Table 1.2 Pseudopotentials for several semiconductors in units of Rydberg [Ry] and lattice constants a in [Å] (from Cohen and Bergstresser [11]) S A a[Å] V3S V8S V11 V3A V4A V11 Si Ge Sn GaP GaAs AlAs AlSb InP GaSb InAs InSb ZnS ZnSe ZnTe CdTe

5.43 5.66 6.49 5.44 5.64 5.66 6.13 5.86 6.12 6.04 6.48 5.41 5.65 6.07 6.41

−0.21 −0.23 −0.20 −0.22 −0.23 −0.221 −0.21 −0.23 −0.22 −0.22 −0.20 −0.22 −0.23 −0.22 −0.20

+0.04 +0.01 0.00 +0.03 +0.01 0.025 +0.02 +0.01 0.00 0.00 0.00 +0.03 +0.03 0.00 0.00

+0.08 +0.06 +0.04 +0.07 +0.06 0.07 +0.06 +0.06 +0.05 +0.05 +0.04 +0.07 +0.06 +0.05 +0.04

0 0 0 +0.12 +0.07 0.08 +0.06 +0.07 +0.06 +0.08 +0.06 +0.24 +0.18 +0.13 +0.15

0 0 0 +0.07 +0.05 0.05 +0.04 +0.05 +0.05 +0.05 +0.05 +0.14 +0.12 +0.10 +0.09

0 0 0 +0.02 +0.01 −0.004 +0.02 +0.01 +0.01 +0.03 +0.01 +0.04 +0.03 +0.01 +0.04

these pseudopotentials given in Table 1.2 show good agreement with experimental observation, higher order components of the pseudopotentials are usually neglected. The term V S (G 0 ) = V0S results in a shift of the energy reference and thus we put V0S = 0.

1.6.3 Nonlocal Pseudopotential Theory Here we will be concerned with the energy band calculations by the pseudopotential method where the non locality of the core potential is considered. The method described above is called local pseudopotential method, where the core potential is assumed to be uniform neglecting the angular orbitals of the core electrons. The nonlocal pseudopotential method takes account of nonlocal properties of the core electrons. The core potential Vc (r) consists of a sum over the occupied core states φ j , and it consists of the various states with the respective angular momentum symmetry as discussed by Cohen and Chelikowsky [6, 12, 13] (see also the references listed there). Therefore the core potential is given by the sum of s–, p–, and d– components of the respective angular momentum quantum number l = 0, 1, 2, . . . Vc (r) = Vs + V p + Vd + . . . .

(1.95)

24

1 Energy Band Structures of Semiconductors

As an example we consider carbon atom C. Its core states are (1s)2 and thus carbon has no p–repulsive potential. The (2 p) electrons of the valence states (2s)2 )(2 p)2 are affected by the core potential. This repulsive core potential is expected to be stronger because of its closer distance to the core than in Si and Ge. In general, the core potential is energy dependent and the nonlocal (NL) correction term to the local atomic potential term is expressed as the following [6, 8, 13] α VNL (r, E) =

∞

Alα (E) fl (r )Pl ,

(1.96)

l=0

and flα (r ) =

1, r ≤ Rm , 0, r ≥ Rm

(1.97)

where Alα (E) is an energy-dependent well depth of the α species, Rm is the model radius, which is taken to be the same for all l, and Pl is projects out the lth angular momentum component of the wave function. When we assume a square well for the model potential defined by (1.97), the matrix element of the nonlocal potential is given by VNL (K , K ) =

4π α A (E)(2l + 1) Ωα l,α l ×Pl cos θ K ,K S α (K − K )Flα (K , K ),

(1.98)

where S α (K ) is the structure factor defined by (1.90c) with K = k + G and K = k + G , θ K ,K is the angle between K and K , and the sum of α is carried out over the atomic species present. Fl (K , K ) = ⎧ 3 R ⎪ ⎨ m [ jl (K Rm )]2 − jl−1 (K Rm ) jl+1 (K Rm ) , K = K , 2 2 Rm ⎪ ⎩ K jl+1 (K Rm ) jl (K Rm ) − K jl+1 (K Rm ) jl (K Rm ) , K = K . 2 2 K −K Pl (x) is a Legendre polynomial and jl (x) is a spherical Bessel function, which are given for smaller values of the subscript l: P0 (x) = 1, P1 (x) = x, P2 (x) = (1/2)(3x 2 − 1), j0 (x) = x −1 sin x, J1 (x) = x −2 sin x − x −1 cos x, j2 (x) = (3x −3 − x −1 ) sin x − 3x −2 cos x, j3 (x) = 5x −1 j2 (x) − j1 (x). Energy band calculations require the estimation of energy dependent term Alα (E) and radii Rm = R0 , which are reported by Cohen and Chelikowsky [13]. They make

1.6 Pseudopotential Method

25

the approximation for A0 (E) for the s state as

A0 (E) = α0 + β0 [E 0 (K )E 0 (K )]1/2 − E 0 (K F ) ,

(1.99)

where E 0 (K ) = 2 K 2 /2m, K F = (6π 2 Z /Ω)1/3 and Z is the valence of the atomic species of interest [12, 13]. Now the energy band calculations with local and nonlocal pseudopotentials are straight forward. The eigenvalues and eigenvectors are obtained by solving the secular equation (1.100) det HG,G (k) − E(k)δ G,G = 0. For the local pseudopotential approximation, we have L HG,G =

2 (k + G)2 + Vps (|G − G |). 2m

(1.101)

When we include the nonlocal pseudopotential term we obtain L HG,G = HG,G + VNL (K , K ) 4π α L Al (E)(2l + 1)Pl cos θ K ,K = HG,G + Ωα l,α

×S α (G − G )Flα (K , K ),

(1.102)

where the sum is carried out over the atomic species α. Nonlocal pseudopotential parameters reported by Chelikowsky and Cohen [13] are listed in Table 1.5. In their calculations, the model radius of the Rl for the pseudopotential is taken to be the same for all l and α0 = 0 for the cations. Energy band calculations based on the nonlocal pseudopotentials require many parameters, but the calculated results differ only a little compared to the simple local pseudopotential method. We will present only the energy band structure of GaAs calculated by the nonlocal pseudopotential method in Sect. 1.6.6. Before dealing with the energy band calculations by nonlocal pseudopotential, we present energy band structures calculated by the local pseudopotential method for diamond and zinc blende semiconductors without spin–orbit interaction in Sect. 1.6.5. Later in Sect. 1.6.6 we will show calculated results for Ge and GaAs with the spin–orbit interaction for comparison, and finally we present the energy band calculation of GaAs by the nonlocal pseudopotential method.

1.6.4 Spin–Orbit Interaction Once the reciprocal vectors are calculated, the free-electron wave functions (1.87) (called as plane waves in this textbook) are easily formulated. Then putting the wave

26

1 Energy Band Structures of Semiconductors

functions into (1.84) we obtain (1.88) which is called eigen-value equation and easily diagonalized to give eigenvalues and eigen functions. The matrix element in (1.84) is written as (k + G i )|Hps |(k + G j ) = T (k) G i ,G j + VG i ,G j + Δ(k) G i ,G j ,

(1.103)

where we included spin–orbit interaction by introducing the term Δ(k) G i ,G j . The derivation of spin–orbit interaction term is shown in Appendix H. The three terms of (1.103) are given by 2 (k + G i )2 δ G i ,G j , T (k) G i ,G j = 2m VG i ,G j = V S ( Q) cos( Q · τ ) + iV A ( Q) sin( Q · τ ) Q=G i −G j , Δ(k) G i ,G j = iσ · G i × G j − k × (G i − G j ) × λS cos( Q · τ ) + iλA sin( Q · τ ) , where Q = Gi − G j ≡

2π K. a

(1.104) (1.105)

(1.106)

(1.107)

The term T (k) G i ,G j has diagonal elements only and is easily formulated by using the reciprocal wave vectors listed in Table 1.1. The pseudopotential term VG i ,G j is separated in symmetric parts and antisymmetric parts (for zinc blende crystal) and their matrix elements are evaluated as follows. Using K = (a/2π) Q = (a/2π)(G j − G i ), and τ = (a/8)[111], the symmetric parts of the pseudopotentials are π V S ( Q) cos( Q · τ ) = V3S cos (K x + K y + K z ) if |K |2 = 3 (1.108a) 4 π S = V8 cos (K x + K y + K z ) if |K |2 = 8 (1.108b) 4π S = V11 cos (K x + K y + K z ) if |K |2 = 11 (1.108c) 4 = 0 if |K |2 > 11, (1.108d) and in a similar fashion we obtain the antisymmetric parts of the pseudopotentials for a zinc blende crystal V A ( Q) sin( Q · τ ) = V3A sin

π

(K x + K y + K z )

if |K |2 = 3 4 π = V4A sin (K x + K y + K z ) if |K |2 = 4 4 π A = V11 sin (K x + K y + K z ) if |K |2 = 11 4 = 0 if |K |2 > 11.

(1.109a) (1.109b) (1.109c) (1.109d)

1.6 Pseudopotential Method

27

The matrix elements of the spin–orbit Hamiltonian are easily evaluated by using the results shown in Appendix H (see also Sect. 1.7.5 for the evaluation of the matrix elements of the spin–orbit Hamiltonian), and the manipulation similar to the pseudopotential term leads to the following relations (K x + K y + K z ) , π4 λA sin( Q · τ ) = λA sin (K x + K y + K z ) . 4

λS cos( Q · τ ) = λS cos

π

(1.110) (1.111)

The expression of spin–orbit interaction shown here is based on the derivation by Melz [15] and known to be mathematically equivalent to the long-wavelength limit of the OPW formulation due to Weisz [16], but the formalism is based on the empirical pseudopotential (local pseudopotential) method. See the paper by Chelikowsky and Cohen [13] for more detailed treatment. Since we are interested in the valence bands and lower lying conduction bands, we may restrict the number of plane waves to calculate the spin–orbit interaction term. It is well known that the atomic spin–orbit splittings are larger for the heavier elements. Therefore we expect that the spin–orbit splitting at the valence band maximum increases with the heavier elements. For example the spin–orbit splitting of Ge is larger than Si, and it increases in order of the mass for GaP, GaAs, GaSb, InP, InAs, and InSb.

1.6.5 Energy Band Calculation by Local Pseudopotential Method In this section we show the calculated results of the energy band structures with the local pseudopotential method by taking the spin–orbit interaction into account. As discussed by Chelikowsky and Cohen [12, 13], the overall feature of the calculated results by the local pseudopotential method shows a good agreement with the results by the nonlocal pseudopotential method, except a small change in the region near some critical points. Instead, the spin–orbit interaction plays a more important role in the energy regions near the critical points. In order to understand the energy band calculation by the pseudopotential, first we will concern with the energy band calculation by the local pseudopotential method. Since we have only few numbers of the pseudopotential form factors, the energy band calculations are straight forward. However, the accuracy of the calculated energy band structures depends on the number of plane waves used for the pseudopotential Hamiltonian matrix. When the number of plane waves are increased, a large computation time is required to diagonalize the matrix. Therefore we have to limit the number of the plane waves. One of the most popular method is to limit the number of plane waves to form the matrix elements in a reasonable size and the higher energy states are taken into account by using the perturbation method proposed by Löwdin [25]

28

1 Energy Band Structures of Semiconductors

as reported by Brust [14] and Cohen and Bergstresser [11]. Now high performance PC’s such as Windows 10 with Intel CORE i7 are available and 300 × 300 matrix is solved to give the eigen energies and eigenstates in a reasonable time. In the next section we will deal with k · p perturbation method to calculate energy bands, where 15 eigenstates are used. In this textbook the energy band structures are calculated by the empirical pseudopotential method with 113 plane waves and thus 226 plane waves with spin–up and –down states. The energy band structures of typical semiconductors with diamond and zinc blende crystal structures are obtained by the following method. First, we use the pseudopotentials determined by Cohen and Bergstresser [11] and Chelikowsky and Cohen [12] and appropriate values of spin–orbit interaction parameters, and compare with the reported experimental data. The present calculations are based on direct diagonalization of 113 × 113 matrix without spin–orbit interaction and 226 × 226 matrix with spin–orbit interaction. The calculated energy levels at Γ , X and L points are compared with the data listed by Chelikowsky and Cohen [12] and newer data reported so far. Although more recent experimental data on direct gaps and spin–orbit splitting are available, these data are vary in some energy range. When the calculated results fall in the reported rage, the calculations are assumed to be converged. Table 1.3 is the summary of the the used parameters obtained by the present work. We present two different results of Si for 15 plane waves and for 113 plane waves, because these results provide an information of the convergence of the energy band calculation by the pseudopotential method. A beginner for the energy band calculations is recommended to calculate the energy bands of Si for example using 15 plane waves [000], [111] and [200] (K 2 ≤ 4 in Table 1.1 and disregarding the spin–orbit interaction in Si (very small spin–orbit splitting in Si). The overall features of the calculated energy band structure of Si are quite similar between the two with 15 and 113 plane waves,as shown in Fig. 1.9, where energy band structures calculated by 15

Table 1.3 Local pseudopotentials for several semiconductors in units of Rydberg [Ry], spin-orbit parameters [Ry] and lattice constants a in [Å] (from [11]) a[Å]

V3S

V8S

Si

5.43

−0.2241 +0.551

Ge

5.65

−0.234

+0.019

GaAs

5.64

−0.254

GaP

5.45

GaSb

6.12

InAs InP

S V11

V3A

λS

λA

V4A

A V11

+0.0724 0

0

0

+0.050

0

0

0

0.00065

0.00

+0.014

+0.067

+0.055

+0.038

+0.017

0.00080

0.00021

−0.245

+0.031

+0.067

+0.16

+0.055

+0.024

0.00

0.00

−0.238

+0.216

+0.045

+0.04

+0.030

+0.015

0.00150

0.00036

6.05

−0.230

+0.0055 +0.045

+0.080

+0.060

+0.030

0.00064

0.00015

5.86

−0.248

+0.024

+0.053

+0.080

+0.060

+0.030

0.00021

0.00005

InSb

6.47

−0.20

+0.0033 +0.044

+0.044

+0.030

+0.015

0.00150

0.00035

ZnSe

5.65

−0.215

+0.025

+0.064

+0.19

+0.10

+0.027

0.00060

0.00011

ZnTe

6.07

−0.221

0.001

+0.050

+0.150

+0.100

+0.010

0.00100

0.00022

CdTe

6.48

−0.220

0.0009

+0.061

+0.10

+0.05

+0.025

0.00123

0.00022

1.6 Pseudopotential Method

29

Fig. 1.9 Energy bands of Si calculated by the local empirical pseudopotential method with 15 plane waves (a) and 113 plane waves (b). The curves of b are obtained by diagonalizing 113 plane waves 0 ≤ E (K ) ≤ E (K ) = 20 (where E (K ) = (2 /2m)(2π/a)2 )K 2 ) exactly. Note the curves of a exhibit discontinuity at U, K points, degeneracy of the lower conduction bands at Γ point, and a curve of higher conduction band in the region K 1 to Γ is missing

plane waves are shown by the curves in (a) and the curves in (b) are calculated by 113 plane waves. We find here that overall features are in good agreement but some disagreement exists as described below. It should be pointed out that a reasonable agreement exists in the energy bands calculated with 113 plane waves and higher number of plane waves, for example 169. The curves obtained by 113 plane waves show smooth continuity at the points U and K (at K 2 ). The lowest conduction bands of Γ2 and Γ15 are degenerate for 15 plane waves, while the degeneracy is removed with 113 plane waves. The points U and K in the Brillouin zone are equivalent because of the symmetry of the representation as seen in Figs. 1.5 and 1.21 and thus obtained bands are expected to be continuous through the points U and K . In addition to the discontinuity, a higher conduction band obtained by 113 plane waves is missing in the bands of 15 plane waves calculation in the region K 1 to Γ as seen in Fig. 1.9a. This will be discussed in Sect. 1.7, where energy band calculations by k · p perturbation method of 15 states will be discussed. Present energy band calculations based on the local pseudopotentials with spinorbit interaction are carried out by comparing the results with experimental data. The experimental data reported by many papers vary in some range and thus we focus on the energy band gap and spin–orbit splitting, and the order of conduction bands minima at the critical points of Γ , X and L. The most important thing of the empirical pseudopotential method is to choose reasonable number of plane waves, and we fixed to 113 plane waves without spin and 226 plane waves with spin–up and –down. Then we diagonalize 113 × 113 Hamiltonian matrix without spin or 226 × 226 matrix with

30

1 Energy Band Structures of Semiconductors

spin up and spin down. The electron wave vector k is divided into 50 points in each Brillouin zone, and typical calculation time of full band structure was one minute for 113 plane waves and several minutes for 226 plane waves. Figure 1.10 shows energy band structure of Ge by local pseudopotential (a) without and (b) with spin–orbit interaction. Calculated energy bands of GaAs, GaP, and GaSb are shown in Fig. 1.11, where the spin orbit splitting in GaP is very small and thus its interaction is neglected. Also calculated energy bands of InAs, InP and InSb are shown in Fig. 1.12 and the results on ZnSe, ZnTe and CdTe are presented in

Fig. 1.10 Energy band structures calculated by the empirical pseudopotential method for Ge a without spin–orbit interaction and b with spin–orbit interaction. Note the critical points shown in a without spin–orbit interaction are single group representation and b with spin–orbit interaction are double group representation

Fig. 1.11 Energy band structures calculated by the empirical pseudopotential method for GaAs, GaP, GaSb. The spin–orbit interaction is included

1.6 Pseudopotential Method

31

Fig. 1.12 Energy band structures calculated by the empirical pseudopotential method for a InAs, b InP, c InSb. The spin–orbit interaction is included

Fig. 1.13 Energy band structures calculated by the empirical pseudopotential method for a ZnSe, b ZnTe, c CdTe. The spin–orbit interaction is included

Fig. 1.13. Note here that the parameters are for low temperature values, T = 4.2 or T = 10 K which are estimated by the formula of Varshni [18]. Energy eigen values at critical points Γ , X , and L for several valence bands and conduction bands are given in Table 1.4.

32

1 Energy Band Structures of Semiconductors

Table 1.4 Energy levels at Γ , X and L points calculated by local pseudopotential method with spin–orbit interaction for semiconductors Si, Ge, GaAs, GaP, and GaSb. Energies in [eV], Note the critical point notation is for double group, while single group is used for Si and GaP. The notation of the lowest two conduction bands Γ6c1 and Γ7c2 for Ge should be reversed. Notation of the superscript of the first column represents the order of the conduction bands from the lowest and the order of the valence bands from the top. These results correspond to experimental data at T = 4.2 or at T = 0 K (estimated by Varshni formula) Si

Ge

GaAs

GaP

GaSb

InAs

InP

InSb

ZnSe

ZnTe

CdTe

Γ8c3

4.14

3.24

4.48

5.61

3.68

4.66

4.79

3.42

6.67

6.54

Γ7c2

3.37

3.01

4.20

5.61

3.04

4.46

4.73

2.76

6.63

6.34

4.56

Γ6c1

3.37

1.01

1.52

2.85

0.815

0.415

1.42

0.256

2.88

2.39

1.57

Γ8v1

0.0

0.0

0.0

0.0

0.0

0.0

0.0

0.0

Γ7v2

0.0

−0.282

−0.342

0.0

−0.0766

−0.395

−0.105

−0.836

−0.972

−0.880

Γ6v3

−12.6

X 8c3

12.6

−12.20 11.5

−12.0

−13.2

12.1

13.3

−10.45

−11.46

10.0

10.4

0.0

0.0

−0.429

4.97

0.0

−11.5

−9.61

−13.1

−12.1

−9.86

11.7

8.67

12.7

11.4

9.65

X 6c2

1.19

0.95

2.42

3.43

2.10

2.81

3.18

1.66

4.10

4.36

X 7c1

1.19

0.95

2.10

2.72

1.74

2.12

2.43

1.40

3.94

4.08

3.18

X 8v1

−3.02

−2.78

−2.28

−2.16

−2.11

−1.73

−1.87

−1.86

−1.61

−1.21

−1.25

−2.35

− 2.16

−2.22

−1.86

−1.91

X 7v2

−3.02

−2.78

−6.51

−5.34

−5.89

−4.78

−5.10

X 6v3

−8.31

−8.40

−9.75

L c3 8

8.74

3.91

5.16

10.96

4.26

5.07

5.25

3.92

L c2 6

3.93

3.82

5.04

6.08

3.99

4.98

5.23

L c1 7

2.10

0.73

1.85

2.79

1.31

1.68

L v1 8

−1.27

−0.114

−0.91

−0.852

0.804

L v2 7

−1.27

−0.133

−1.13

−0.852

−7.30

−7.15

−6.16

−5.43

−10.48

12.01

−9.12

L v3 6

−10.2

−10.2

−11.6

−2.00

−1.81

−1.61 −3.70

−1 1.6

−9.03

6.82

6.75

5.49

3.63

6.79

6.66

5.29

2.25

0.907

3.73

3.64

2.48

−0.66

−0.74

−0.689

−0.593

−0.441

−0.474

−1.32

−0.90

−0.805

−1.24

−0.852

−1.02

−1.02

−5.49

−4.74

−5.02

−4.91

−4.18

−3.40

−10.3

−10.6

−10.0

−10.5

−8.04

−8.52

−3.97

−1.64 −3.28

−8.47

−5.18

3.35

−12.1

−12.4

−11.7

−3.62 −9.25

1.6.6 Energy Band Calculations by Nonlocal Pseudopotential Method with Spin–orbit Interaction Here, we show the calculated results by the nonlocal pseudopotential method with spin–orbit interaction for Ge in Fig. 1.14a with 226 plane waves of spin–up and spin– down with the spin–orbit interaction with λS = 0.00065 [Ry] for Ge, gives the spin– orbit splitting energy about 0.285 [eV]. The results for GaAs shown in Fig. 1.14b are obtained by the nonlocal pseudopotential methods of Chelikowsky and Cohen [13]. The nonlocal pseudopotential values used for GaAs are listed in Table 1.5. There exists only a slight difference in the energies at X , L and other critical points between the present calculations and the results calculated by Chelikowsky and Cohen [13]. In the calculation the plane waves for 0 ≤ K 2 ≤ E1 = 20 (113 plane waves and thus 226 plane waves with spin–up and –down states) are exactly diagonalized. The spin–orbit parameters are λS = 0.00080 and λA = 0.00023. The results are shown in Fig. 1.14 which give the energy gap EG = 1.505 [eV] and the spin–orbit splitting at the Γ point 0.34065 [eV]. The present results for E1 = 20 exhibit no recognizable

1.6 Pseudopotential Method

33

Fig. 1.14 Energy bands of Ge and GaAs calculated by the nonlocal pseudopotential method, where the spin–orbit interaction is taken into account. The states for 0 ≤ K 2 ≤ E1 = 20 (113 plane waves and thus 226 plane waves with spin–up and –down states) are exactly diagonalized Table 1.5 Pseudopotential parameters for the diamond and zinc blende semiconductors and the nonlocal parameters (after Chelikowsky and Cohen [13]) Pseudopotential form factors [Ry] Lattice S A Materials V3S V8S V11 V3A V4A V11 constant [Å] Si Ge GaP GaAs GaSb InP InAs InSb

−0.257 −0.221 −0.230 −0.254∗ −0.220 −0.235 −0.230 −0.200

−0.040 0.019 0.020 0.014 0.005 0.000 0.000 −0.010

0.033 0.056 0.057 0.067 0.045 0.053 0.045 0.044

0.100 0.055 0.040 0.080 0.055 0.044

0.070 0.038 0.030 0.060 0.045 0.030

0.025 0.010∗ 0.000 0.030 0.010 0.015

5.43 5.65 5.45 5.65 6.10 5.86 6.05 6.47

The pseudopotential values of GaAs with asterisk differ from the values A = 0.001 of Chelikowsky and Cohen[13] V3S = −0.214 and V11

difference between the results with and without the perturbation terms of the plane waves for E1 < K 2 ≤ 27.

34

1 Energy Band Structures of Semiconductors

Material Si Ge

Nonlocal parameters for Si and Ge α0 [Ry] β0 A2 [Ry] R0 [Å] 0.55 0.32 0 1.06 0 0 0.275 0

R2 [Å] 0 1.22

Nonlocal parameters for zinc blende semiconductors (R0 = 1.27 for the cation and 1.06 Å for the anion) (α0 = 0 for the cation) Cation Anion Material α0 [Ry] β0 A2 [Ry] α0 [Ry] β0 A2 [Ry] GaP 0 0.30 0.40 0.32 0.05 0.45 GaAs 0 0 0.125 0 0 0.625 GaSb 0 0.20 0.20 0 0.30 0.60 InP 0 0.25 0.55 0.30 0.05 0.35 InAs 0 0.35 0.50 0 0.25 1.00 InSb 0 0.45 0.55 0 0.48 0.70

As reported by Chelikowsky and Cohen [13] the over all features of the energy bands are almost the same as the results calculated by the local pseudopotential method except some critical points. Therefore the results shown in the text are calculated by the local pseudopotential method, unless otherwise mentioned, because we have to adjust more parameters for the nonlocal pseudopotential methods. The local pseudopotential method requires fewer number of the pseudopotential parameters to get results in agreement with the experimental observation, and provides the energy bands and optical properties of various semiconductors which help us to understand the optical characteristics and transport properties based on the full band Monte Carlo simulation.

1.7 k · p Perturbation 1.7.1 k · p Hamiltonian The k · p perturbation was introduced by Kane [17] in 1956 to analyze the energy band structures of III–V compound semiconductors and led to a successful result. The method was originally used in 1936 to discuss the character table of the symmetry points in the Brillouin zone by Bouckaert, Smoluchowski and Wigner [19]. Later Dresselhaus, Kip and Kittel [20] used the k · p perturbation method to analyze the detailed structure of the valence bands of Ge and Si. This method is described in detail in Sect. 2.1, where the k · p perturbation method is applied to analyze the experimental results of cyclotron resonance in Ge. In this section we will consider the method used by Cardona and Pollak [21] to calculate energy band structures.

1.7 k · p Perturbation

35

We consider the non-relativistic Schrödinger equation for a one-electron system: 2 2 − ∇ + V (r) Ψ (r) = EΨ (r), 2m

(1.112)

where V (r) is the crystal potential energy with the lattice periodicity. The solution of (1.112) is given by the Bloch function Ψ (r) = eik·r u n,k (r),

(1.113)

where u n,k is a function of the lattice periodicity for band index n. Putting this Bloch function into (1.112) and using the following relations ∇Ψ (r) = ikΨ (r) + eik·r ∇u n,k (r),

(1.114a)

∇ Ψ (r) = −k Ψ (r) + 2ike ∇u n,k (r) + e ∇ u n,k (r), = eik·r (−k 2 + 2ik · ∇ + ∇ 2 )u n,k (r), 2

2

ik·r

ik·r

2

we obtain 2 2 2 2 2 − ∇ + V (r) + k − i (k · ∇) u n,k (r) = En (k)u n,k (r). 2m 2m m

(1.114b)

(1.115)

Using the relation −i∇ = p for the momentum operator, the above equation may be rewritten as 2 k 2 H0 + + k · p u n,k (r) = En (k)u n,k (r), (1.116) 2m m where H0 = −(2 /2m)∇ 2 + V (r) is Hamiltonian. The terms 2 k 2 /2m in [ ] on the left-hand side is a constant (c-number) without any operator and thus the term gives rise to an energy shift of 2 k 2 /2m from En (k). First solving (1.116) for k = 0 and then treating (/m)k · p as a perturbing term, we obtain eigenstates as a function of k which gives the energy band structure. Therefore, this method is called k · p perturbation. The eigenstates for the Hamiltonian H0 are obtained by using the pseudopotentials, but here we show a simplified method to obtain the eigenstates by solving 2 × 2 matrices following the method reported by Cardona [5]. Although such a calculation is very simple, obtained eigen energies and eigenvectors are very useful to understand the band structures. The above k · p Hamiltonian is rewritten by using atomic units as follows:

36

1 Energy Band Structures of Semiconductors

2 2 2 ∇ = − 2m 2m 2 k 2 2 = 2m 2m 2 k· p= m 2m

1 aB 1 aB 1 aB

2 (−iaB ∇)2 = Ry · (−iaB ∇)2

(1.117a)

(aB k)2 = Ry · (aB k)2

(1.117b)

2 2

aB2

(2k · p) = Ry ·

aB2

(2k · p), (1.117c)

where aB = 4π0 2 /(me2 ) 0.529 [Å] is Bohr radius and Ry = me4 /(82 h 3 c) 13.6 [eV] is Rydberg constant. Using the dimensionless notation or the atomic units k (in [a.u]) = aB k,

p (in [a.u]) =

aB p = −iaB ∇,

(1.118)

and then the (/m)k · p operator of (1.117c) is rewritten as k · p = Ry · (2k · p). m

(1.119)

Finally, the length is expressed in atomic units or normalized by aB and then the k · p Hamiltonian is rewritten as H0 +

2 k 2 k· p+ = −∇ 2 + 2k · p + k 2 . m 2m

(1.120)

When we put k = 0 in (1.116), we obtain 2 2 ∇ + V (r) u n,0 (r) = En (0)u n,0 (r), H0 u n,0 (r) = − 2m

(1.121)

which is rewritten in atomic units as −∇ 2 + V (r) u n,0 (r) = En (0)u n,0 (r).

(1.122)

Since the crystal potential V (r) and Bloch function u n,0 (r) are periodic with the lattice constant, and thus these two functions are expanded by Fourier series. Therefore we may use the pseudopotential theory stated before, and the diagonalization of the Hamiltonian matrix gives the eigenstates and the corresponding eigenvalues. In the k · p perturbation theory we need eigenstates at k = 0 (at the Γ point) only. For this purpose we rewrite (1.86) and (1.87) as −∇ 2 + V ps (|G|2 ) |G j = En |G j , 1 |G j = √ eiG j r , Ω

(1.123) (1.124)

1.7 k · p Perturbation

37

Table 1.6 Character table of small representations of Oh group BSW E 3C42 6C4 6C2 8C3 J 3J C42 Γ1 Γ2 Γ12 Γ15 Γ25 Γ1 Γ2 Γ12 Γ15 Γ25

1 1 2 3 3 1 1 2 3 3

1 1 2 −1 −1 1 1 2 −1 −1

1 −1 0 1 −1 1 −1 0 1 −1

1 −1 0 −1 1 1 −1 0 −1 1

1 1 −1 0 0 1 1 −1 0 0

1 1 2 3 3 −1 −1 −2 −3 −3

1 1 2 −1 −1 −1 −1 −2 1 1

6J C4

6J C2

8J C3

1 −1 0 1 −1 −1 1 0 −1 1

1 −1 0 −1 1 −1 1 0 1 −1

1 1 −1 0 0 −1 −1 1 0 0

where Vps (r) is expanded with Fourier coefficients Vps (|G|2 ) (pseudopotential form factors). Simplified solutions of the above equations are very helpful to obtain the eigenstates and to explain the group theoretical representations used in Fig. 1.7. The k · p Hamiltonian for semiconductors with inversion symmetry has off-diagonal terms only. In addition, we classify the matrix elements with the help of group theory, and so the number of the matrix elements are extremely decreased. Cardona and Pollak [21] proposed to calculate the energy band structures using 15 electronic states (wave functions) at the Γ point (at k = 0) and obtained very accurate energy band structures of germanium and silicon. Here we will show the energy band calculations of germanium and silicon based on the k · p perturbation method of Cardona and Pollak, where the spin–orbit interaction is not included. First we classify the free electron energy bands shown in Fig. 1.7 with the help of group theory. Here we summarize important and useful results of group theory without showing the derivation. The most important factors are to use the character table of the crystal. The character table for a face centered cubic lattice which includes diamond and zinc blende crystals is shown in Table 1.6 (see Koster et al. [24]). Although detailed description of group theory is not shown here, the character table is very useful to calculate non-vanishing matrix elements and thus selection rule of optical transition. Another important information about the symmetry properties of quantum states is the basis functions for the representations, which is summarized in Table 1.9. In a crystalline solid the notation of atomic orbitals is classified by using the spherical harmonics Ylm (θ, φ)(m = −l, . . . , +l) which constitute a basis for the irreducible representation and thus the electronic states are related to the states of an atom as shown below [9],

38

1 Energy Band Structures of Semiconductors

State s (l = 0) = Γ1 , State p (l = 1) = Γ15 , State d (l = 2) = Γ25 + Γ12 , State f (l = 3) = Γ15 + Γ25 + Γ2 , State g (l = 4) = Γ25 + Γ15 + Γ12 + Γ1 , State h (l = 5) = Γ25 + 2Γ15 + Γ12 . In a crystalline solid the wave functions of an atom and the next nearest neighbor are hybridized, resulting in bonding and anti-bonding states and thus in energy shift, as discussed below. A concept of atomic orbitals, LCAO (Linear Combination of Atomic Orbitals), is very helpful to understand the energy bands at k = 0. Here we follow the method of Cardona [5]. First, we consider electronic states in the outer shell of an atomic Ge, where two s–states and two p–states are filled with electrons. Therefore the other two p–states and ten d–states are empty. Since two atoms are included in a unit cell of diamond structure, the states are doubled when the two atoms are put together. In such a case, the electronic states are modified by linear combinations of the atomic orbitals, the bonding and anti-bonding states, and thus the states split as shown in Fig. 1.15. No mixing by the crystal field occurs between s– and p–orbitals at k = 0. The s–orbitals contain a negligible admixture of f–orbitals while the p–orbitals may contain a significant admixture of d–orbitals of the same shell. The ordering of the states are illustrated so as to fit the observed conduction and valence bands. The ordering between the sates is changed by the bonding–antibonding splitting. If the splitting is small, as in the case of α–Sn with large lattice constant, the Γ1 and Γ2 are filled and Γ25 only partially filled. As the bonding–antibonding splitting becomes larger, the Γ2 –state becomes higher than Γ25 , resulting in an energy gap. This is the case for Ge and Si as shown in Fig. 1.15. In order to calculate the energy bands of Ge and Si by the k · p method, we have to choose the eigenstates at k = 0 properly, not so many states but enough to lead reasonable results. First we show the free electron bands for lower energy states in Table 1.7, where the free electron energies are estimated for Ge (a = 5.66Å), G 3 band is 1.038 a.u. (14.1eV), and G 4 is 1.38 a.u. (18.8eV). The fourth band G 8 is 2.77

Fig. 1.15 Splitting of the atomic states of Ge, Si and α–Sn under the presence of the crystalline field of the diamond structure at Γ point of the Brillouin zone, where a bar corresponds to a degenerate energy state with spin up and down (after Cardona [5])

1.7 k · p Perturbation

39

Table 1.7 Reciprocal of smaller free electron energies, where dgn means the degeneracy of the states and the free electron energy in [a.u.] is estimated for a = 5.66[Å] G Vector components dgn Representations Energy in [a.u.] G0 G3 G4 G8 G 11

= (2π/a)[0, 0, 0] = (2π/a)[±1, ±1, ±1] = (2π/a)[±2, 0, 0] = (2π/a)[±2, ±2, 0] = (2π/a)[±3, ±1, ±1]

1 8 6 12 24

Γ1l l +Γ +Γl +Γu Γ25 15 1 2 u +Γ +Γu Γ25 12 2 Γ1 + Γ12 + 2Γ15 + Γ25 Γ1 + Γ12 + Γ2 + Γ12 Γ15 + Γ25 + 2Γ25 + 2Γ15

0 1.038 1.38 2.77 3.81

a.u. (37.7eV), which is well higher than the G 4 bands and we may limit the plane waves up to G 4 . This enables us to choose 15 eigenstates with the representations; l l u u u Γ1l , Γ25 , Γ15 , Γ2 , Γ1 , Γ25 , Γ12 , and Γ2 . This approximation was used by Cardona and Pollak [21]. Next, we discuss relation between the LCAO and plane waves of free electron bands expressed by a combination of the reciprocal lattice vectors [G x , G y , G z ] of the empty lattice bands at Γ point (at k = 0 of the Brillouin zone). The plane waves of [000], [111] and [200] are related to the LCAO states as shown by Cardona [5]. Γ l; ⎧ l1 ⎪ ⎪ Γ25 ; ⎨ Γ15 ; [111] l ⎪ ⎪ Γ2u ; ⎩ Γ ; ⎧ 1u ⎨ Γ25 ; [200] Γ12 ; ⎩ u Γ2 ;

[000]

s–bonding; p–bonding p–anti-bonding s–anti-bonding s–bonding (next shell); d–bonding d –bonding s–anti-bonding (next shell),

where the superscript l and u denote the lower and the upper of the two states of the same symmetry. For simplicity we use the relation (1.59) to express dimensionless reciprocal lattice vector K . The group of reciprocal wave vectors K [±1, ±1, ±1](8) have 8 components (dimension is 8), and a combinations of the 8 plane waves gives the following representations by using the character table of Table 1.6 l K [±1, ±1, ±1](8) = Γ1u (1) + Γ2u (1) + Γ15 (3) + Γ25 (3).

(1.125)

The representation Γ1u has the same character of the lowest valence band Γ1l arising from the reciprocal wave vector K [0, 0, 0]. Representation Γ1u in (1.125) is understood as follows. A summarized combination of orthogonalized plane waves for Γ1u is composed from [±1, ±1, ±1]

40

1 Energy Band Structures of Semiconductors

1 ¯ 1, 1] − [1, 1, ¯ 1] − [1, 1, 1] ¯ Γ1u [±1, ±1, ±1] = √ [1, 1, 1] − [1, 8 ¯ 1, ¯ 1] − [1, ¯ 1, 1] ¯ − [1, 1, ¯ 1] ¯ + [1, ¯ 1, ¯ 1] ¯ −[1, (1.126) and the character is the same of Γ1l [0, 0, 0], where we used the notation 2π Kx x + K y y + Kz z . [K x , K y , K z ] = exp i a

(1.127)

In a similar fashion other symmetrized combinations of the orthogonalized plane l waves are composed for Γ2u , Γ15 , and Γ25 . The representations of the plane waves are summarized in Table 1.7. In the following several symmetrized combinations of the orthogonalized plane waves [K x , K y , K z ] belonging to the Γ –representation are given: Γ2l [111] 1 ¯ − [11 ¯ 1] ¯ − [1¯ 11] ¯ − [1¯ 1¯ 1] ¯ + [111] ¯ ¯ + [111]}, ¯ = √ {[111] − [11¯ 1] + [111] 8 1 ¯ ¯ − [002] ¯ , − [020] Γ2u [200] = √ [200] + [020] + [002] − [200] 6 l Γ25 (X ) [111] 1 ¯ + [11 ¯ 1] ¯ + [1¯ 11] ¯ + [1¯ 1¯ 1] ¯ − [111] ¯ ¯ + [111]}, ¯ = √ {[111] − [11¯ 1] + [111] 8 1 u ¯ Γ25 (X ) [200] = √ {[200] + [200]}, 2 Γ15 (x) [111] 1 ¯ + [11 ¯ 1] ¯ + [1¯ 11] ¯ − [1¯ 1¯ 1] ¯ + [111] ¯ ¯ − [111] ¯ , − [111] = √ [111] − [11¯ 1] 8 1 ¯ + [002]}, ¯ Γ12 (1) [200] = {[020] − [002] − [020] 2 1 ¯ ¯ + [002]}. ¯ Γ12 (2) [200] = √ {2[200] − [020] − [002] − 2[200] + [020] 12 l The Y and Z components of Γ25 , and y and z components of Γ15 are obtained by means of cyclic permutation.

1.7 k · p Perturbation

41

1.7.2 Derivation of the k · p Parameters Energy band calculation by means of k · p perturbation requires estimation of l l momentum matrix elements such as Γ25 | p|Γ2 and energy eigenstates at the Γ point of the Brillouin zone (k = 0). For this purpose we use pseudopotential method stated in the previous Sect. 1.6. These values are used for the initial data and then adjusted to the values so that the calculated critical points agree with the experiment. Cardona [5] applied the pseudopotential method for the purpose as described below. First we solve (1.123) with (1.124). For simplicity, irreducible representations of linear combinations of orthogonalized plane waves [000], [111] and [200] are considered, and then we find in Table 1.7 that representations Γ1 , Γ2 and Γ25 appear twice, and designated as upper “u” and lower “l” states. In the case of a diamond crystal such as Ge and Si there exist symmetric pseudopotential terms only, and we obtain eigenvalues and eigenfunctions by diagonalizing 2 × 2 matrices of Hamiltonian H0 = −∇ 2 + V ps (|G|2 ) for the Γ1 , Γ2 and Γ25 states: Γ1 [000] Γ1 [111] 0 2V3S , S 2V3 3(2π/a)2 + 3V8S

(1.128a)

Γ2 [111] √ Γ2 [200] S S S 2 3(2π/a) + 3V 6(V 3 3 + V11 ) , √ S 6(V3S + V11 ) 4(2π/a)2 + 4V8S

(1.128b)

Γ25 [111] √ Γ25 S[200] S S 2 3(2π/a) − V3 2(V3 − V11 ) . √ S 2(V3S − V11 ) 4(2π/a)2

(1.128c)

In the following we estimate the eigen energies and eigenfunctions using the pseudopotentials listed in Table 1.2 and thus the obtained results differ a little from those reported by Cardona [5] and Cardona and Pollak [21]. The energies of Γ1 states are −0.171 [Ry] (−2.326 [eV]) and 1.237[Ry] (16.8 [eV] for germanium, and 0.735 [Ry] (10.0 [eV] and −0.2399 [Ry] (−3.263 [eV]) for silicon. The energies of the Γ2 states are given by 1.69 [Ry] (22.9 [eV]) and 0.77 [Ry] (10.5 [eV]) for germanium, and 1.81 [Ry] (24.6 [eV]) and 0.977 [Ry] (13.3 [eV]) for silicon. The eigenstates of the lower energies are Γ2l for Ge : Γ2l for Si, :

0.843Γ2 [111] + 0.539Γ2 [200], 0.906Γ2 [111] + 0.422Γ2 [200].

(1.129a) (1.129b)

In a similar fashion the eigenstates of Γ25 are obtained by solving 2 × 2 Hamiltonian matrix. The eigen energies are 1.74 [Ry] (23.6 [eV]) and 0.909 [Ry] (12.37 [eV]) for Ge, and 1.84 [Ry] (25.0 [eV]) and 1.00 [Ry] (13.6 [eV]) for Si.

42

1 Energy Band Structures of Semiconductors

Table 1.8 Energy eigenvalues at k = 0 (Γ point) calculations by simplified matrices of the pseudopotentials. Values are given in atomic unit Rydberg [Ry], and relative values (rel.[Ry]) are with l . For comparison eigenvalues obtained by solving respect to the energy of the top valence band Γ25 15 × 15 pseudopotential matrix is shown by full [Ry] At k = 0 Waves Germanium Silicon [Ry] rel.[Ry] full [Ry] [Ry] rel.[Ry] full [Ry] l Γ25 Γ2l Γ15 Γ1u Γ1l Γ12 u Γ25 Γ2u

[111] [111] [111] [111] [000] [200] [200] [200]

0.909 0.769 1.026 1.237 −0.171 1.36 1.74 1.687

l Γ25 for Ge : l Γ25 for Si, :

0.00 −0.139 0.117 0.331 −1.08 0.452 0.828 0.778

0.00 0.0342 0.2694 0.4805 −0.9270 0.6044 0.8938 0.9396

1.00 0.977 1.085 1.374 −0.128 1.42 1.836 1.809

0.00 −0.023 0.086 0.246 −1.28 0.421 0.836 0.809

0.755Γ25 [111] + 0.656Γ25 [200], 0.774Γ25 [111] + 0.634Γ25 [200].

0.00 0.2396 0.2521 0.5406 −0.9611 0.5870 0.9192 0.9996

(1.130a) (1.130b)

The energies of the single state Γ15 is given by 3(2π/a)2 − V8S , and the doubly– degenerate states Γ12 (1)[200]) and Γ12 (2)[200] are given by 4(2π/a)2 − 2V8S , where matrix elements are 0 between the states Γ12 (1) and Γ12 (2). The calculated energies at k = 0 (at Γ point) are listed in Table 1.8, where energies of the first row of the material in the table in units of [Ry] are obtained by solving a single band and 2 × 2 pseudopotential matrices, and the second row of rel.[Ry] is the relative values l with respect to the valence band top of Γ25 . The third row of the material shows the eigenvalues calculated by diagonalizing 15 × 15 pseudopotential matrices. In the 15 × 15 pseudopotential calculation, 15 reciprocal wave vectors of [000](1), [±1, ±1, ±1](8), and [±2, 0, 0](6) (numbers in ( ) are degeneracy of the states) are l u used, and the result reveals that Γ25 , Γ25 and Γ15 states are triply–degenerate, and Γ12 states are doubly–degenerate. We find in Table 1.8 that the values deduced from a simplified method give a very good guide to locate the eigenstates of the valence and conduction bands. The results obtained by the simple method are very close to the values of “pseudo” in Table 1.10, although the energy levels of Γ2 estimated by the simple method are negative and thus lie below the valence band top for both Ge and Si. In the k · p perturbation calculations, however, the parameters are adjusted to fit the data of experimental critical points and thus these estimations will be used for the initial parameters. Estimation of the momentum matrix element reported by Cardona [5] is very helpful to understand the energy band structure and thus it is described below in l l detail. The momentum matrix elements of p between Γ25 and Γ2 which is expressed as P are given by using (1.129a)–(1.130b) l l l l l l Γ25 (X )| p x |Γ2 = Γ25 (Y )| p y |Γ2 = Γ25 (Z )| pz |Γ2

1.7 k · p Perturbation

43

Table 1.9 Basis function of irreducible representation of Oh group at Γ point Representation Degeneracy Basis functions Γ1 Γ2 Γ12 Γ15 Γ25 Γ1 Γ2 Γ12 Γ15 Γ25

1 1 2 3 3 1 1 2 3 3

1 x 4 (y 2 − z 2 ) + y 4 (z 2 − x 2 ) + z 4 (x 2 − y 2 ) z 2 − 21 (x 2 + y 2 ), (x 2 − y 2 ) x y(x 2 − y 2 ), yz(y 2 − z 2 ), zx(z 2 − x 2 ) x y, yz, zx x yz[x 4 (y 2 − z 2 ) + y 4 (z 2 − x 2 ) + z 4 (x 2 − y 2 )] x yz x yz[z 2 − 21 (x 2 + y 2 )], x yz(x 2 − y 2 ) x, y, z z(x 2 − y 2 ), x(y 2 − z 2 ), y(z 2 − x 2 )

Table 1.10 Energy eigenvalues used for energy band calculations by the k · p perturbation method in units of Rydberg (from Ref. [21]) At k = 0 Waves Germanium Silicon k· p OPWa Pseudo k· p OPWa Pseudo l Γ25 Γ2l Γ15 Γ1u Γ1l Γ12 u Γ25 Γ2u

[111] [111] [111] [111] [000] [200] [200] [200]

0.00 0.00 0.0728b −0.081 0.232b 0.231 0.571 0.571 −0.966 −0.929 0.770 0.770 1.25c 1.35

0.00 −0.007 0.272 0.444 −0.950 0.620 0.890 0.897

0.00 0.265b 0.252b 0.520 −0.950 0.710 0.940 0.990

0.00 0.164 0.238 0.692 −0.863 0.696

0.00 0.23 0.28 0.52 −0.97 0.71 0.94 0.99

a F.

Herman, in Proceedings of the International Conference on the Physics of Semiconductors, Paris, 1964 (Dunod Cie, Paris, 1964), p.3 b M. Cardona, J. Phys. Chem. Solids 24, 1543 (1963) c G. Dresselhaus, A.F. Kip, and C. Kittel, Phys. Rev. 98, 368 (1955); E.O. Kane, J. Phys. Chem. Solids 1, 82 (1956)

2π [0.843 × 0.755 + 0.539 × 0.656] a = 0.58 = P (: for Ge), l l l l l l Γ25 (X )| px |Γ2 = Γ25 (Y )| p y |Γ2 = Γ25 (Z )| pz |Γ2 2π = [0.906 × 0.774 + 0.422 × 0.634] a = 0.59 = P (: for Si). =

l The momentum matrix elements of p between Γ25 and Γ15 states are

(1.131)

(1.132)

44

1 Energy Band Structures of Semiconductors l l l Γ25 (Z )| p x |Γ15 (y) = Γ25 (X )| p y |Γ15 (z) = Γ25 (Y )| pz |Γ15 (x) 2π = × 0.755 = 0.44 = Q (: for Ge), (1.133) a l l l Γ25 (Z )| p x |Γ15 (y) = Γ25 (X )| p y |Γ15 (z) = Γ25 (Y )| pz |Γ15 (x) 2π × 0.774 = 0.47 = Q (: for Si). (1.134) = a

The momentum matrix elements for the k · p perturbation should be multiplied by a factor 2, and thus P = 1.16 for Ge (P = 1.18 for Si) and Q = 0.88 for Ge (Q = 0.94 for Si), which are very close to the parameters used by Cardona and Pollak [21] in Table 1.11. The matrix elements P play a very important role in the determination of the valence band structure to be dealt with in Chap. 2 and the optical absorption due to the direct transition discussed in Chap. 4. The 15 states at the Γ point are classified into Γ1l (1), Γ1u (1), Γ2l (1), Γ2u (1), l u Γ25 (3), Γ15 (3), Γ25 (3), Γ12 (2), where the superscripts l and u correspond to the lower and upper states of the bands, respectively, and number in the parentheses ( ) is the dimension of the representation. It is evident from the character table of the group theory that Γ25 is 3-dimensional with three eigenstates. The energy eigenstates are estimated roughly by the pseudopotential method or other approximations [21] as stated above, and shown in Table 1.10. The momentum operator p has the same symmetry as Γ15 and thus the matrix elements of k · p for the 15 eigenstates have non-zero components, as shown in the following equations and in Table 1.11.

Table 1.11 The values of momentum matrix elements used for the energy band calculations of germanium and silicon by the k · p perturbation (atomic units) Momentum

Germanium

Matrix elements

k· p

l | p|Γ l P = 2iΓ25 2 l | p|Γ Q = 2iΓ25 15 l | p|Γ R = 2iΓ25 12 l | p|Γ u P = 2iΓ25 2 u | p|Γ l P = 2iΓ25 2 u | p|Γ Q = 2iΓ25 15 u | p|Γ R = 2iΓ25 12 u | p|Γ u P = 2iΓ25 2 u T = 2iΓ1 | p|Γ15 T = 2iΓ1l | p|Γ15

† Values

Silicon Pseudo

c.r.†

1.24

1.36a

0.99

1.07a

0.8049

0.75

0.92c

0.1000

0.09

0.1715

0.0092

1.360 1.070

k· p

Pseudo

c.r.†

1.200

1.27

1.20b

1.050

1.05

1.05b

0.830

0.74

0.68d

0.100

0.10

−0.090

−0.10

−0.65

−0.807

−0.64

1.4357

1.13

1.210

1.21

1.6231

1.30

1.32

1.37

1.2003

1.11

1.080

1.18

0.5323

0.41

0.206

0.34

−0.752

used to analyze the cyclotron resonance experiments a B.W. Levinger and D.R. Frankl, J. Phys. Chem. Solids 20, 281 (1961) b J.C. Hensel and G. Feher, Phys. Rev. 129, 1041 (1963) c Calculated from cyclotron resonance data d Calculated from cyclotron resonance data of reference b

1.7 k · p Perturbation

45 l l P = 2iΓ25 | p|Γ2 ,

Q= R= P = P = Q = R = P = T = T =

l 2iΓ25 | p|Γ15 , l 2iΓ25 | p|Γ12 , l u 2iΓ25 | p|Γ2 , u l 2iΓ25 | p|Γ2 , u 2iΓ25 | p|Γ15 , u 2iΓ25 | p|Γ12 , u u 2iΓ25 | p|Γ2 , 2iΓ1u | p|Γ15 , 2iΓ1l | p|Γ15 .

(1.135a) (1.135b) (1.135c) (1.135d) (1.135e) (1.135f) (1.135g) (1.135h) (1.135i) (1.135j)

The factor 2 of the momentum matrix elements in Table 1.11 and (1.135a)–(1.135j) is understood from k · p perturbation Hamiltonian given by (1.119) and (1.120), where energy is in Rydberg [Ry] and the length in unit aB ( Bohr radius) as discussed above. We note here the matrix elements of Γ25 |k · p|Γ12 used in the present calculations. Using the character table and the basis function we may deduce the non-vanishing matrix elements for the k · p theory. In the present analysis the matrix elements between Γ25 and Γ12 are evaluated by using the property of the character table in Table 1.6, (1.136) Γ25 × Γ12 = Γ15 + Γ25 , Γ15 × Γ12 = Γ25 + Γ15 . The wave vectors p = [ px , p y , pz ] have the same property as [x, y, z], and thus the representation is Γ15 . Therefore we find non-zero matrix elements Γ25 | p|Γ12 and Γ15 | p|Γ12 . However, Γ15 states belong to the plane waves [±3, ±1, ±1] and the free electron energy is 11(2π/a)2 which is much higher than the upper states of Γ25 [200] with the free electron energy 4(2π/a)2 , and thus Γ15 states may be disregarded. Therefore the following matrix elements for the states Γ12 are included in the 15 × 15 k · p perturbation (see (1.143a)–(1.143f) for a detailed treatment). l 2iΓ25 (X )| p|Γ12 = R,

(1.137a)

u 2iΓ25 (Y )| p|Γ12 = R .

(1.137b)

Using the parameters listed in Table 1.11 and following the procedures below, the energy band structures of Ge and Si are easily calculated. First, we calculate the 15 × 15 matrix elements of the k · p Hamiltonian, and second diagonalize the matrix to obtain the energy eigenvalues and their eigenstates at k of the Brillouin zone. The matrix of the k · p Hamiltonian has 15 × 15 complex elements. When we include the spin–orbit interaction, the matrix of k · p Hamiltonian is given by 30 × 30 complex elements.

46

1 Energy Band Structures of Semiconductors

1.7.3 15–band k · p Method It is very important to point out here that the 15 × 15 matrices for Ge and Si are factorized into smaller matrices when we use group theoretical consideration, as shown by Cardona and Pollak [21]. For simplicity we consider the energy bands along the 100 , 110 and 111 directions of the k-vector. The direction 100 starts from the Γ point and ends at the X point along the Δ axis, and the 110 direction is from the Γ point to the K point along the Σ axis, while the 111 direction is from the Γ point to the L point along the Λ axis. With the help of the compatibility relation given in Table 1.12 (see [19]) the matrix elements of the k · p Hamiltonian are factorized in several groups of smaller matrices. In the following we use atomic units as stated above, and thus 2 k 2 /2m and p 2 /2m are expressed as k 2 and p 2 , respectively. In the following we show the factorized matrices of the k · p Hamiltonian in the [100], [110] and [111] directions. 1. [100] direction (a) Δ5 bands From Table 1.12 we find that three Γ bands exist, but the bands in the parentheses ( ) are neglected because of their high energy states. u l Δ5 bands: (Γ15 ), Γ25 , Γ25 , Γ15 The matrix elements for these 3 bands are l u |Γ25 |Γ15 |Γ25 2 kx Qk x 0 . Qk x E(Γ15 ) + k x2 Q kx u 2 0 Q kx E(Γ25 ) + kx

(1.138)

(b) Δ1 bands Δ1 bands: Γ1l , Γ1u , (Γ12 ), Γ15 The matrix elements for these three bands are

Table 1.12 Compatibility relations Γ1

Γ2

Γ12

Γ15

Γ25

Γ1

Γ2

Γ12

Γ15

Γ25

Δ1

Δ2

Δ1 Δ2

Δ1 Δ5

Δ2 Δ5

Δ1

Δ2

Δ1 Δ2

Δ1 Δ5

Δ2 Δ5

Λ1

Λ2

Λ3

Λ2 Λ3

Λ1 Λ3

Λ2

Λ1

Λ3

Λ1 Λ3

Λ2 Λ3

Σ1

Σ4

Σ1 Σ4

Σ2 Σ3 Σ4

Σ1 Σ2 Σ3 Σ2

Σ3

Σ2 Σ3

Σ1 Σ3 Σ4

Σ1 Σ2 Σ4

X1

X2

X3

X4

X5

X1

X2

X3

X4

X5

Δ1

Δ2

Δ2

Δ1

Δ5

Δ1

Δ2

Δ2

Δ1

Δ5

Z1

Z1

Z4

Z4

Z2 Z3

Z2

Z2

Z3

Z3

Z1 Z4

S1

S4

S1

S4

S2 S3

S2

S3

S2

S3

S1 S4

M1

M2

M3

M4

M5

M1

M2

M3

M4

M5

Σ1

Σ1

Σ4

Σ4

Σ2 Σ3

Σ2

Σ2

Σ3

Σ3

Σ1 Σ4

Z1

Z1

Z3

Z3

Z2 Z4

Z2

Z2

Z4

Z4

Z1 Z3

T1

T2

T2

T1

T5

T1

T2

T2

T1

T5

1.7 k · p Perturbation

47

|Γ15 |Γ1u |Γ1l 2 E(Γ15 ) + k x T kx T kx . u 2 T kx E(Γ1 ) + k x 0 T kx 0 E(Γ1l ) + k x2

(1.139)

(c) Δ2 bands l u l u Δ2 bands: Γ25 , Γ25 , Γ2 , Γ2 , Γ12 The matrix elements for these five bands are l u |Γ2l |Γ25 |Γ12 |Γ25 |Γ2u l 2 E(Γ2 ) + k x Pk x P kx 0 √ 0 2 Pk x k 2Rk 0 P kx x √ √ x , 2 2Rk x E(Γ 2R 0 ) + k k 0 12 x x √ u 2 P kx 0 2R k x E(Γ25 P k x ) + kx 0 P kx 0 P kx E(Γ2u ) + k x2

(1.140)

√ √ √ where the factor 2 of 2Rk x and 2R k x arises from the definition of Γ12 states (Γ12 (1) and Γ12 (2)) as given by Cardona and Pollak [21] and the Γ12 (2) state does not interact with any other state in the [100] direction and behaves like a free electron band (see (1.143a), (1.143b), (1.144)). 2. [110] direction From Table 1.12, Σ1 , Σ4 , Σ3 , Σ2 are included in this direction. l u (a) Σ1 bands: Γ1l , Γ1u , (Γ12 ), Γ25 , Γ25 , Γ15 (: 5 bands) (b) Σ4 bands: (Γ2 ), (Γ12 ), (Γ15 ), Γ15 , (Γ25 ) (: 1 band) l u l u (c) Σ3 bands: (Γ15 ), Γ25 , Γ25 , Γ2 , Γ2 , Γ12 , Γ15 (: 6 bands) u (d) Σ2 bands: (Γ15 ), Γ25 l, Γ25 , (Γ1 ), Γ12 , (Γ25 ) (: 3 bands) Therefore, for the bands in the [110] direction, Σ bands, 15 × 15 matrix elements results in irreducible matrix of 6 × 6, 5 × 5, 3 × 3, 1 × 1. 3. [111] direction From Table 1.12, Λ1 , Λ3 are included in this direction. l u l u (a) 7 bands of Λ1 bands: Γ1l , Γ1u , Γ25 , Γ25 , Γ2 , Γ2 , Γ15 l u (b) 4 bands of Λ3 bands: (Γ12 ), (Γ15 ), Γ25 , Γ25 , Γ12 , Γ15 , (Γ25 ) and the Λ bands in the [111] direction are classified in 7 × 7 and 4 × 4 irreducible matrix. It should be noted here that above 15 × 15 k · p matrix is easily extended to include k y and k z components. However we have to take account of correct symmetry of the Γ12 (1) and Γ12 (2) states, which is done by extending the method

48

1 Energy Band Structures of Semiconductors

of Dresselhaus [20] and convert them into the representations of Cardona and Pollak [21] as follows. Using the definition of Dresselhaus et al. and following their procedures, we obtain Γ25 (X )| px |γ1− = R, Γ25 (X )| px |γ2− = −R, Γ25 (Y )| p y |γ1− = ω R,

Γ25 (Y )| p y |γ2− = −ω 2 R, Γ25 (Z )| pz |γ1− = ω 2 R,

Γ25 (Z )| pz |γ2− = −ω R,

(1.141a) (1.141b) (1.141c) (1.141d) (1.141e) (1.141f)

where we have to note that the matrix elements R defined by Dresselhaus, Kip and Kittel [20] (RDKK ) and R defined by Cardona and Pollak [21] (RCP ) are related by RCP = 2RDKK . When we choose the eigenstates Γ12 defined by Cardona and Pollak [21]; 1 Γ12 (1) = √ (γ1− − γ2− ), 2

1 Γ12 (2) = √ (γ1− + γ2− ), 2

(1.142)

we obtain the following results Γ25 | px |Γ12 (1) =

√

2R,

(1.143a)

Γ25 | px |Γ12 (2) = 0, (1.143b) √ √ 2 Γ25 | p y |Γ12 (1) = (ω + ω )R/ 2 = −R/ 2, (1.143c) √ √ 2 Γ25 | p y |Γ12 (2) = (ω − ω )R/ 2 = ω(1 − ω)R/ 2 = iR 3/2, (1.143d) √ √ (1.143e) Γ25 | pz |Γ12 (1) = (ω 2 + ω)R/ 2 = −R/ 2, √ √ 2 Γ25 | pz |Γ12 (2) = (ω − ω)R/ 2 = ω(ω − 1)R/ 2 = −iR 3/2, (1.143f) where ω is the solutions of ω 3 = 1 (exclude the solution ω = 1) or the solutions of ω√2 + ω + 1 = 0. The above results are obtained by√using the solution ω = (−1 + i 3)/2. When we choose the solution ω = (−1 − i 3)/2, the sign of the imaginary part is changed, but the energy band calculations give the same result. In addition we have to note that ω = 1, one of the solutions of ω 3 = 1, does not give a correct energy bands. This is because the solution ω = 1 does not represent the correct symmetry of γ1− and γ2− . Here we show the 15 × 15 k · p Hamiltonian matrix without the spin–orbit interaction (antisymmetric potential terms for zinc blende crystals are included);

1.7 k · p Perturbation

49

l (X ) l (Y ) l (Z ) |Γ25 |Γ25 |Γ25 |Γ15 (x) |Γ15 (y) |Γ15 (z) l ) + k2 E(Γ25 0 0 −iV1− Qk z Qk y l ) + k2 0 E(Γ25 0 Qk z −iV1− Qk x l ) + k2 0 0 E(Γ25 Qk y Qk x −iV1− iV1− Qk z Qk y E(Γ15 ) + k 2 0 0 − Qk z iV1 Qk x 0 E(Γ15 ) + k 2 0 Qk y Qk x iV1− 0 0 E(Γ15 ) + k 2 0 0 0 −iV4− Q kz Q ky − 0 0 0 Q kz −iV4 Q kx − k k 0 0 0 Q Q −iV y x 4 √ √ √ 2Rk x −(R/ 0 0 0 √ 2)k y −(R/ √ 2)k z 0 −iR 3/2k y iR 3/2k z 0 0 0 Pk x Pk y Pk z 0 0 0 P k x P k y P k z 0 0 0 0 0 0 T kx T ky T kz 0 0 0 T kx T ky T kz u (X ) u (Y ) u (Z ) |Γ25 |Γ25 |Γ25 0 0 0 0 0 0 0 0 0 iV4− Q kz Q ky iV4− Q kx Q kz Q ky Q kx iV4− u 2 0 0 E(Γ25 ) + k u ) + k2 0 E(Γ25 0 u ) + k2 0 0 E(Γ 25 √ √ √ 2R k x −(R / 2k y −(R / 2)k z √ √ 0 −iR 3/2k y iR 3/2k z P kx P ky P kz P kx P ky P k z 0 0 0 0 0 0

|Γ √12 (1) 2Rk √x −(R/ √2)k y −(R/ 2)k z 0 0 √ 0 2R√k x −(R / √2)k y −(R / 2)k z E(Γ12 ) + k 2 0 0 0 0 0

|Γ1u |Γ1l |Γ2l (x yz) |Γ2u (x yz) Pk x P k x 0 0 Pk y P k y 0 0 Pk z P k z 0 0 0 0 T kx T kx 0 0 T ky T ky 0 0 T kz T kz P kx P k x 0 0 P ky P k y 0 0 P kz P k z 0 0 0 0 0 0 0 0 0 0 E(Γ2l ) + k 2 0 iV2− iV3− 0 E(Γ2u ) + k 2 iV5− iV6− −iV2− −iV5− E(Γ1u ) + k 2 0 −iV3− −iV6− 0 E(Γ1l ) + k 2

|Γ12 (2) 0 √ iR 3/2k y √ −iR 3/2k z 0 0 0 0 √ iR 3/2k y √ −iR 3/2k z 0 E(Γ12 ) + k 2 0 0 0 0

(1.144)

50

1 Energy Band Structures of Semiconductors

Fig. 1.16 Energy band structure of Si and GaAs calculated by 15 band k · p perturbation without spin–orbit interaction. The results are obtained by solving secular equation (1.144) with the parameters given in Table 1.13

It should be noted here that Γ12 (2)| p y |Γ25 (Y ) is given by the complex conjugate of Γ25 (Y )| p y |Γ12 (2) . Energy bands without the spin–orbit interaction are easily calculated by solving (1.144) in any directions of the Brillouin zone. As an example calculated energy band structure of Si along the L, Γ , X , W , K to Γ points is shown in Fig. 1.16. Also in the figure the energy band structure of GaAs is shown, where the antisymmetric potential is taken account (see Sect. 1.7.4).

1.7.4 Antisymmetric Potentials for Zinc Blende Crystals We have to note here the definition of the matrix elements of the anti-antisymmetric potentials. As discussed in Sect. 1.6, a diamond type crystal has inversion symmetry and thus V A (G) = 0, while a zinc blende type crystal has no inversion symmetry and thus V A (G) = 0. In order to extend the k · p Hamiltonian for a zinc blende crystal we have to evaluate the matrix elements of the anti-symmetric potential as shown in (1.144). Here we present how to evaluate approximate values of the matrix elements of the anti-symmetric potential. First, we obtain non-vanishing matrix elements of the 15 plane waves of [0, 0, 0], [±1, ±1, ±1], and [±2, 0, 0] which are classified as l l u u u Γ1l , Γ25 , Γ15 , Γ12 , Γ2 , Γ1 , Γ25 , Γ12 , and Γ2 as shown in Table 1.7. In Table 1.6, an inversion operation is expressed by J and representation Γi has the inversion symmetry when J > 0 but no inversion symmetry when J < 0. The product of Γi × Γ j has the same symmetry property. Noting the anti-symmetric potential V − has negative sign for the inversion operation, non-vanishing matrix elements Γi |V − |Γ j are Γ15 |V − |Γ25 and Γ2 |V − |Γ1 . When we use the notations of Pollak, Higginbotham,

1.7 k · p Perturbation

51

and Cardona [26], these are given by the following relations, l A V1− = Γ15 |V − |Γ25 = V4 , V2− = Γ2l |V − |Γ1u = −3V4A ,

V3− = Γ2l |V − |Γ1l = 2V3A , √ A u A V4− = Γ15 |V − |Γ25 2 V3 − V11 , = √ − u − u A A , V5 = Γ2 |V |Γ1 = −( 6/3) (4V3 + 2V11 √ − u − l A V6 = Γ2 |V |Γ1 = (2 6/3)V4 ,

(1.145a) (1.145b) (1.145c) (1.145d) (1.145e) (1.145f)

where the last terms of the above equations are evaluated from the pseudopotentials in Table 1.2 and the relations defined by (1.109a)–(1.109d) with linear combinations of the plane waves (1.126) and (1.128)–(1.128). As an example we evaluate these terms for GaAs using the pseudopotentials given in Table 1.2. We obtain V1− = 0.05 (0.12652), V2− = −0.15 (−0.24791), V3− = 0.14 (0.38210), V4− = 0.0849 (0.12297), V5− = −0.245 (−0.34820), and V6− = 0.0816 (0.0), where the values in the parentheses are determined form the energy band calculations and summarized in Table 1.13 for several zinc blende type semiconductors. Since the term V6− corresponds to interactions between very distant atomic orbitals Γ2u and Γ1l (difference in the free electron energy is 4(2π/a)2 = 1.38 [a.u.] for GaAs), we may safely assume that V6− = 0.0 [26]. When we include the spin–orbit interaction, the above equation leads to 30 × 30 k · p complex matrix because each state is doubled with spin–up ↑ and spin–down ↓ . In Chap. 2, we will discuss the second order perturbation of the k · p Hamiltonian and the parameters defined by Dresselhaus et al. [20] and by Luttinger [22, 23], where the above results are used to evaluate the contributions from γ1− and γ2− (Γ12 (1) and Γ12 (2)).

1.7.5 Spin–Orbit Interaction Hamiltonian When we take account of the spin–orbit interaction, the eigenstates are doubled with spin–up and spin–down as discussed above, and then we have to solve 30 × 30 complex matrix. In the following we choose the wave functions |X ↑ , l |X ↓ , |Y ↑ , |Y ↓ , |Z ↑ , |Z ↓ for Γ25 , and |x ↑ , |x ↓ , |y ↑ , |y ↓ , |z ↑ , |z ↓ for Γ15 . This approximation leads to 30 × 30 complex matrix with the spin–orbit interaction. In this subsection we formulate the spin–orbit matrix elements using these eigenstates. Spin–orbit interaction is also discussed in Sect. 2.3 to analyze the valence band structure, in addition to describe the effective mass and effective g factor (Landé g factor) of the conduction band. Evaluation of the matrix elements of spin–orbit Hamiltonian is given in detail in Sect. 2.3.

52

1 Energy Band Structures of Semiconductors

We put the spin–orbit interaction term (H.18) of Appendix H into (1.112), and obtain 2 [∇ × p] · σ + [∇ × k] · σ, (1.146) Hso = 2 2 4m c 4m 2 c2 which should be added to the terms in the brackets of the left hand side of (1.116). The second k–dependent term is very small compared to the first k–independent term (see Kane [17]) and thus only the first term is considered in this text. Thus the k–independent term of the spin–orbit Hamiltonian is rewritten as Hso ∝ L · σ = (r × p) · σ = −i(r × ∇) · σ

(1.147)

and therefore we find that ∂ ∂ ∂ ∂ σx + z −x σy y −z dz dy dx dz ∂ ∂ σz , (1.148) + x −y dy dx

− i(r × ∇) · σ = −i

where σ is Pauli spin operator1 and the matrix elements are evaluated by using the basis functions given in Table 1.9. l l l X (Γ25 ) ↑ |Hso |Y (Γ25 ) ↑ = iΔ25 /3, l l l X (Γ25 ) ↑ |Hso |Z (Γ25 ) ↓ = Δ25 /3,

(1.149a) (1.149b)

l l l Y (Γ25 ) ↑ |Hso |Z (Γ25 ) ↓ = iΔ25 /3.

(1.149c)

In the same manner the spin–orbit interaction for Γ15 is written as x(Γ15 ) ↑ |Hso |y(Γ15 ) ↑ = iΔ15 /3,

(1.150a)

x(Γ15 ) ↑ |Hso |z(Γ15 ) ↓ = Δ15 /3, y(Γ15 ) ↑ |Hso |z(Γ15 ) ↓ = iΔ15 /3,

(1.150b) (1.150c)

and the antisymmetric term of the spin–orbit interaction is treated as l − X (Γ25 ) ↑ |Hso |y(Γ15 ) ↑ = iΔ /3, l − X (Γ25 ) ↑ |Hso |z(Γ15 ) ↓ = +Δ /3, l − Y (Γ25 ) ↑ |Hso |z(Γ15 ) ↓ = iΔ /3.

(1.151a) (1.151b) (1.151c)

The spin–orbit interaction in the valence bands is discussed in Chap. 2. Here we l will show the present treatment leads to the same results. The Γ25 valence bands l (|X , |Y , |X ) are triply–degenerate at the Γ point (k = 0). The degenerate Γ25 bands split into doubly–degenerate heavy hole and light hole bands, and the spin– 1

See (2.50) of Chap. 2 for the definition and (H.33c) of Appendix H for the matrix elements.

1.7 k · p Perturbation

53

orbit–split–off band as discussed in Chap. 2. Here it is shown that the above matrix l elements of the spin–orbit Hamiltonian for the valence bands Γ25 give the same results of the spin–orbit splitting dealt in Chap. 2. The matrix of the spin–orbit Hamill tonian for the valence band Γ25 is written as |X ↑ |Y ↑ |Z ↓ l l 0 iΔ25 /3 Δ25 /3 |X ↑ −iΔl /3 0 iΔl25 /3 |Y ↑ , l 25 l Δ /3 −iΔ /3 0 |Z ↓ 25 25

(1.152)

and diagonalization results in (1/3)Δl u v1 0 0 25 u v2 . 0 (1/3)Δl25 0 0 0 −(2/3)Δl25 u v3

(1.153)

l l Therefore the spin–orbit splitting of Γ25 bands is Δ0 = Δ25 and the corresponding eigenfunctions are

i u v1 = √ (X − iY ) ↑, 2 1 u v2 = √ (X ↑ +Z ↓), 2 −1 u v3 = √ [(X + iY ) ↑ −Z ↓] . 3

(1.154a) (1.154b) (1.154c)

Using these results we may obtain the matrix elements of the spin–orbit Hamiltonian Hso for the Γ25 states: |X ↑ |Y ↑ |Z ↓ |X ↓ |Y ↓ |Z ↑ 0 i 1 0 0 0 −i 0 i 0 0 0 Δ 1 −i 0 0 0 0 , Γ25 |Hso |Γ25 = 3 0 0 0 0 i 1 0 0 0 −i 0 i 0 0 0 1 −i 0

(1.155)

and the matrix is separated by two 3 × 3 matrices and diagonalization of the matrix gives the following eigenvalues and eigen functions,

54

1 Energy Band Structures of Semiconductors

|vv1 |vv2 |vv3 |vv4 |vv5 |vv6 1 0 0 0 0 0 0 1 0 0 0 0 Δ 0 0 1 0 0 0 , Γ25 |Hso |Γ25 = 3 0 0 0 1 0 0 0 0 0 0 −2 0 0 0 0 0 0 −2

(1.156)

The eigenstates of the fourfold degenerate valence bands are 1 u v1 = √ [|X ↑ + |Z ↓ ] , 2 1 u v2 = √ [|X ↓ + |Z ↑ ] , 2 i u v3 = √ [|(X − iY ) ↓ ] , 2 i u v4 = √ [|(X − iY ) ↑ ] , 2 and for twofold degenerate spin–orbit split off bands are 1 u v5 = − √ [|(X + iY ) ↑ − |Z ↓ ] , 3 i u v6 = − √ [|(X + iY ) ↓ − |Z ↑ ] , 3 where we find that the spin–orbit interaction results in the split valence band Δ/3, Δ/3, and −2Δ/3. Note here that the obtained eigen functions differ from those defined by (2.63a)–(2.63f) in Chap. 2 because of the different definition of the original (unperturbed) basis functions. Similar relations for the Γ15 states and antisymmetric parts are easily evaluated.

1.7.6 30–band k · p Method with the Spin–Orbit Interaction We have to note here that the full band calculation (energy states at any points of the Brillouin zone) is easily carried out by extending 15 × 15 k · p matrix of (1.144) to 30 × 30 k · p matrix with spin–up and spin–down states. The matrices of the spin– u orbit interaction Hamiltonian for Γ25 states, Γ15 states, and the antisymmetric parts u between Γ25 and Γ15 states are obtained by (1.155). The 30–band k · p Hamiltonian with complex elements are solved to obtain 30 eigenstates. The full band calculations based on the 30–band k · p methods have been reported in the literatures [30–37], where the treatment of the matrix elements R and R1 are deduced by Voon and

1.7 k · p Perturbation

55

Fig. 1.17 Energy band structure of Ge and GaAs calculated by the 30–band k · p method with spin–orbit interaction in k space along L, Γ , X , W , K , and Γ of the Brillouin zone

Willatzen [30].2 All the k · p parameters for semiconductors such as Ge and Si with diamond crystal structure and several III–V compound semiconductors such as GaAs and GaP are summarized in Table 1.13. It should be noted again that III-V compound semiconductors with a zinc blende structure have no inversion symmetry and thus we have to include the anti-symmetric terms of the potentials and spin–orbit interaction as discussed by Pollak et al. [26]. A lack of the inversion symmetry results in the antisymmetric potential V − , and the antisymmetric parts of Δ− in the spin–orbit Hamiltonian of which matrix elements are defined by (1.151a)–(1.151c). The calculated energy band structures of in the energy range −15 ∼ 10 [eV] are shown for Ge and GaAs in Fig. 1.17 and for GaP and InP in Fig. 1.18, where we find that the 30–band k · p perturbation method gives a reasonable result although the matrix elements are very few compared to the pseudopotential method. Since the energy bands near the lowest conduction band and the top valence bands are very important to understand the electrical and optical properties of semiconductors, the energy band structures in the vicinity of the conduction minima and the valence band maxima calculated by the 30–band k · p perturbation method are shown in Fig. 1.19 for Ge and GaAs, where the parameters are from the Refs. [21, 26–29]. The k · p perturbation method is very simple, as shown above, and gives an information about the matrix elements of the optical transition in addition to detailed and accurate energy band structures [21]. We have to note here some difference of the calculated band structures between the empirical pseudopotential method and 30–band k · p perturbation method. As 2

The author is thankful for M. Cardona to remind the work by Voon and Willatzen after his visit to Max Planck Institute at Stuttgart in June, 2013.

56

1 Energy Band Structures of Semiconductors

Fig. 1.18 Energy band structures calculated by the 30–band k · p perturbation method for GaP and InP, where the spin–orbit interaction is included

Fig. 1.19 Energy band structures near the conduction and valence bands calculated by the 30–band k · p perturbation method for Ge and GaAs, where the spin–orbit interaction is included

seen in the first Brillouin zone of a face centered cubic crystal given in Fig. 1.5a and Fig. 1.21 the U point and K point are equivalent and we may expect the same energy eigenvalues at the two points. This feature is understood from the symmetry properties of the free electron band in the region U and K of Fig. 1.6. However, when we plot energy bands obtained by the 30–band k · p method along X to U point and K to Γ point, we find a small discontinuity at the points U and K , although the pseudopotential method gives smooth curve in this region. This may be ascribed to the

1.7 k · p Perturbation

57

Fig. 1.20 Energy band structures of GaAs along L–Γ , Γ –X , X –U, K , and U, K –Γ points a calculated by the 30–band k · p perturbation method and b calculated by the empirical pseudopotential method with 113 plane waves (226 plane waves with spin–up and spin–down), where the spin–orbit interaction is included. See the textbook for the used parameters

assumption of limited number of eigen sates at the Γ point for the k · p perturbation method as follows. The free electron bands of a face centered cubic lattice are shown in Figs. 1.6 and 1.7, where we find that one of the 12 free electron bands of [220] is merged into one of the 6 free electron bands of [200]. This is clearly seen in Fig. 1.20, where the energy band structures of GaAs calculated by 30–band k · p are shown in Fig. 1.20a and the results obtained from the empirical pseudopotential method with 113 plane waves (226 plane waves with spin–up and spin–down) are shown in Fig. 1.20b. In the calculations we used the parameters listed in Table 1.3.These parameters lead to EG = 1.52 eV and spin–orbit splitting Δ = 0.342 eV as shown in Table 1.4. The 30–band k · p method with the parameters listed in Table 1.13 gives the same values. In Fig. 1.20a we find the bands obtained from 30–band k · p method are discontinuous at U and K points, while the bands calculated by the empirical pseudopotential method with 226 plane waves are continuous. In addition the second lowest conduction band in the region Γ –X calculated by 30–band k · p method does not appear in the region of between U, K and Γ points. These features are observed in the band structures calculated by the pseudopotential method with 15 plane waves shown in Fig. 1.9, while the energy bands with 113 plane waves show much more smooth (continuous) curves near U and K points. Although such a small difference exists in the energy band structure calculated by the 30–bands k · p perturbation method, the obtained overall features of the full band structures are very in good agreement with the empirical pseudopotential method and the bands along L, Γ , X , W , K to Γ are very smooth. As discussed in Sect. 1.8, the

58

1 Energy Band Structures of Semiconductors

Fig. 1.21 The first Brillouin zone of face centered cubic lattice and the symmetry points. The box defined by the lines is 1/48th part of the volume of the first Brillouin zone

density of states are calculated by dividing the polyhedron, the 1/48 volume of the first Brillouin zone, starting the basal plane of L, Γ , X , W , K . Then the calculations of the density of states are straight forward. From the results of the pseudopotential and k · p perturbation methods we find the important features of the energy band structures of the semiconductors which we deal with in this text. All these semiconductors have valence band maxima at k = 0 (Γ point) and most III–V semiconductors (except several compounds such as GaP, AlAs and so on) have the conduction band minimum at k = 0 (Γ point), and so are classified as direct gap semiconductors. On the other hand, other semiconductors such as Ge, Si, GaP, AlAs and so on have the conduction band minima at k = 0, and so are called indirect gap semiconductors. Ge has the conduction band minima at k = (π/a)[111] (L point), which are degenerate and consist of equivalent four conduction bands, and thus the conduction bands have a “many–valley structure.” On the other hand, Si has the conduction band minima at the Δ point close to the X point and six equivalent conduction band minima. Later we will discuss the optical properties of semiconductors, where we find that the direct and indirect semiconductors are quite different in their optical properties such as absorption and light scattering. The electrical properties also exhibit the features of many-valley structures in Ge and Si, and also the Gunn effect of GaAs, which arises from the inter-valley transfer of electrons in a high electric field from the high electron mobility Γ valley to the low mobility L and/or X valleys. From these results we understand that the energy band structures play a very important role in the understanding of the electrical and optical properties of semiconductors. In addition, once we know the procedures for calculating energy band structures it is very easy to extend the method to calculate the energy band structures of superlattices (periodic layers of different semiconductors such as GaAs/AlAs) as treated in Chap. 9. It is also possible to predict the basic features of semiconductors from the results of energy band calculations. In this text the basic physics of semiconductors is treated on the basis of their energy band structures.

1.7 k · p Perturbation

59

Table 1.13 Energy eigenvalues (in Rydberg) and momentum matrix elements (in atomic units) used in the k · p Hamiltonians for Si, Ge, GaAs, GaP, InP and InSb. Matrix elements of the antisymmetric potentials V − and anti-symmetric spin–orbit splitting parameter Δ− (in Rydberg) for GaAs, GaP, InP and InSb are also listed. Values are from Refs. [21, 26–29] Si Ge GaAs GaP InP InSb l Γ25 Γ2l Γ15 Γ1u Γ12 u Γ25 Γ2u Γ1l P Q R P P Q R P T T Δl25 Δ15 V1 V2 V3 V4 V5 V6 Δ−

0.00 0.00 0.265 0.0728 0.252 0.232 0.520 0.571 0.710 0.771 0.940 1.25 0.990 1.35 −0.950 −0.966 1.200 1.360 1.050 1.070 0.830 0.8049 0.100 0.100 −0.090 0.1715 −0.807 −0.752 1.210 1.436 1.320 1.623 1.080 1.200 0.206 0.5323 0.0032 0.0213 0.0036 0.0265 l = Γ15 |V − |Γ25 = Γ2l |V − |Γ1u = Γ2l |V − |Γ1l u = Γ15 |V − |Γ25 u u − = Γ2 |V |Γ1 = Γ2u |V − |Γ1l

0.00 0.0845 0.2596 0.4940 0.6063 0.9002 0.9849 −0.844 1.3225 1.1599 0.7635 0.2465 0.0438 −0.5511 0.9697 1.5530 1.1387 0.5323 0.0251 0.0135 0.12652 −0.24791 0.38210 0.12297 −0.34820 0.0 0.0051

0.00 0.2566 0.2511 0.5222 0.7126 0.9535 1.0056 −0.9827 1.207 1.051 0.8289 0.100 −0.07863 −0.8046 1.220 1.333 1.0852 0.2202 0.00399 0.00459 0.14924 −0.26885 0.45687 0.21044 −0.33021 0.0 0.00485

0.00 0.0929 0.2622 0.5057 0.5803 0.8745 0.9792 −0.8107 1.0876 1.1346 0.8045 0.1267 0.1031 −0.6585 1.1038 1.4281 1.0806 0.3906 0.00823 0.00573 0.1347 −0.2003 0.2252 0.1131 −0.2601 0.0 0.00682

0.00 0.022 0.232 0.400 0.494 0.726 0.765 −0.846 1.3460 1.0990 0.5914 0.5324 0.0666 −0.2120 1.0760 1.2340 0.9070 0.0210 0.0590 0.0287 0.0869 −0.1558 0.2391 0.0581 −0.1252 0.0 0.0160

1.8 Density of States As shown in Sect. 4.3, density of states (DOS) is defined as the number of states per unit energy. When the number of states in a small volume of k-space in a small range of energy, [E, E + ΔE] is given by (1/2π)3 Δv(k), the density of states JDOS (E) is defined by (spin factor 2 is omitted) JDOS (E) =

k

1 Δv(k) . (2π)3 ΔE

(1.157)

60

1 Energy Band Structures of Semiconductors

Fig. 1.22 1/48th part of the first Brillouin zone of face centered cubic lattice is discretized into polyhedrons using unit length kf = (X − Γ )/8 = π/4a, where a is the lattice constant

Here v(k) is a small volume of the wave vector k in the first Brillouin zone. The density of states is required to calculate dielectric function (joint density of states) and also to calculate scattering rate of electrons. It is well known that Monte Carlo simulation [38] gives a good description of transport properties at high electric fields. Full band Monte Carlo simulation is used very often, where the calculated energy band structure is used to simulated electron motion in k-space, and thus the density of states is required to obtain the scattering rate. In this textbook we will not deal with high field transport (see [39] for a review on high field transport) and thus we will not concern with Monte Carlo simulation. However, it is very important to know how to calculate the density of states defined by (1.157) from the calculated energy band structure. Various methods have been reported to calculate DOS from the energy bands. Brust [14] reported a rigorous analysis of the joint density of states in Ge and Si, but the method is very complicated. Here we will show a simple but accurate method to calculate the density of states. First, let’s take a look of the Brillouin zone shown in Fig. 1.21 which is the same as shown in Fig. 1.5a. It is clear from the 48-fold symmetry of the Brillouin zone that 1/48th part of the zone shown in Fig. 1.21 is sufficient to calculate the density of states. In other words, all the other k-points in the first Brillouin zone may be obtained by rotation of the 1/48th of the Brillouin zone. Using a unit length kf = (X − Γ )/8 = π/4a with the lattice constant a, 1/48th part of the first Brillouin zone can be divided into polyhedrons shown in Fig. 1.22. The bottom plane consists of the critical points Γ, X, W, K . The second plane is displaced by kf in the k z direction with respect to the first pane, and intersects Λ, S, Q. The third plane with the same displacement intersects Λ, U, Q, and the fourth intersects Λ, Q, L. The two neighboring planes form polyhedrons of which volume gives the number of states. The discretization shown in Fig. 1.22 is not sufficient to calculate the density of states. Here we have to note the most important idea to use this type of discretization. In order to get smaller volumes of the polyhedrons, use the unit length kf /N → kf , where N is 2, 4, 8, . . . . Then the volumes of new polyhedrons becomes 1/8, 1/64, 1/512, . . . of the original polyhedrons and the number of polyhedrons are 8, 64, 512, . . . times of the original number. The density of states are easily calculated using this discretization. We calculate the energy eigenstates at the corners of a polygon and tabulate them. Then pick up the minimum Emin and the maximum Emax from the lowest pairs of the tabulated eigenstates. Calculate ΔE = Emax − Emin and E = (Emax + Emin )/2. This gives us

1.8 Density of States

61 5

Fig. 1.23 Energy band structures of Si calculated by empirical pseudopotential method with the pseudopotentials listed in Table 1.2 and the calculated density of states (DOS) (grateful to Prof. N. Mori for providing the results)

Energy (eV)

0

−5

−10

L

X WK

0

Wave Vector

2

4

6

2

4

6

DOS (1022 / eV cm3)

5

Fig. 1.24 Energy band structures of GaAs calculated by empirical pseudopotential method with the pseudopotentials listed in Table 1.2 and the calculated density of states (DOS) (grateful to Prof. N. Mori for providing the results)

JDOS (E)

Energy (eV)

0

−5

−10

L

X WK

Wave Vector

1 Δvf (k) , (2π)3 ΔE

0

DOS (1022 / eV cm3)

(1.158)

where Δvf (k) is the volume of the polyhedron. In a similar fashion we calculate the density of states for the second lowest pairs, third lowest pairs and so on up to a required E value. The obtained DOS JDOS (E) is not uniform but scattered in the energy E and thus we have to rearrange the data in the histogram, 0.1–eV histogram for example. Then smoothing procedure will give a smooth curve of JDOS (E) as a function of E. Typical examples of the energy bands and the DOS are shown in Fig. 1.23 for Si and in Fig. 1.24 for GaAs.

62

1 Energy Band Structures of Semiconductors

1.9 Problems (1.1)

Calculate the reciprocal lattice vectors of a zinc blende type crystal structure and compare with the result of Table 1.1.

(1.2)

Energy band calculations are carried out by using atomic units [a.u]. Give wave vector k = 2π/aB , and energy (2 /2m)/aB2 ) in atomic units, where aB = (0 h 2 /πme2 ) = 0.529177 [Å] is Bohr radius.

(1.3)

Rewrite Eq. (1.35), using the atomic units.

(1.4)

Evaluate energy bands of two band model based on the nearly free electron approximation, taking free electron bands of G n = 0 and G n = 1, where G n = 2nπ/a, a = 0.543 [Å], and V (G 1 ) = V3s = −0.21 [a.u.]. Calculate the energy band E(k x ) and plot the energy bands together with the free electron bands.

(1.5)

Derive fundamental vectors [a, b, c] of (i) simple cubic, (ii) body centered cubic, (iii) face centered cubic and hexagonal closed pack crystals, and calculate their unit cell volume v.

(1.6)

Derive the reciprocal lattice vectors [a∗ , b∗ , c∗ ] of (i) simple cubic, (ii) body centered cubic, (iii) face centered cubic and hexagonal closed pack crystals, and calculate their unit cell volume v.

(1.7)

Derive spin–orbit interaction given by (1.149a) l l l X (Γ25 ) ↑ |Hso |Y (Γ25 ) ↑ = iΔ25 /3

(1.8)

In order to calculate full band structure in the first Brillouin zone, we have to determine the wave vectors at the critical points (symmetry points) and their lengths. Referring Figs. 1.21 and 1.22, evaluate the symmetry points and the lengths between the symmetry points of a face centered cubic crystal.

References 1. 2. 3. 4.

C. Kittel, Introduction to Solid State Physics, 7th edn. (Wiley, New York, 1996) C. Kittel, Quantum Theory of Solids (Wiley, New York, 1963) J. Callaway, Quantum Theory of the Solid State, vol. 2 (Academic, New York, 1974) W.A. Harrison, Electronic Structure and the Properties of Solids; The Physics of the Chemical Bond (W.H. Freeman, San Francisco, 1980)

References

63

5. M. Cardona, Optical properties and band structure of germanium and zincblende-type semiconductors, in Proceedings of International School of Physics Enrico Fermi (Academic, New York, 1972) pp. 514–580 6. M.L. Cohen, J.R. Chelikowsky, Electronic Structure and Optical Properties of Semiconductors (Springer, Heidelberg, 1989) 7. V. Heine, The pseudopotential concept. Solid State Phys. 24, 1–36 (1970) 8. M.L. Cohen, V. Heine, The fitting pseudopotentials to experimental data and their subsequent application. Solid State Phys. 24, 37–248 (1970) 9. F. Bassani, G. Pastori Parravicini, Electronic States and Optical Transitions in Solids (Pergamon Press, New York, 1975) 10. P. Yu, M. Cardona, Fundamentals of Semiconductors (Springer, Heidelberg, 1996) 11. M.L. Cohen, T.K. Bergstresser, Phys. Rev. 141, 789 (1966) 12. J.R. Chelikowsky, M.L. Cohen, Phys. Rev. B 10, 5095 (1974) 13. J.R. Chelikowsky, M.L. Cohen, Phys. Rev. B 14, 556 (1976) 14. D. Brust, Phys. Rev. A 134, 1337 (1964) 15. P.J. Melz, J. Phys. Chem. Solids 32, 209 (1971) 16. G. Weisz, Phys. Rev. 149, 504 (1966) 17. E.O. Kane, J. Phys. Chem. Solids, 1, 82 (1956) and 249 (1957) 18. Y.P. Varshni, Physica 34, 149 (1967) 19. L.P. Bouckaert, R. Smoluchowski, E. Wigner, Phys. Rev. 50, 58 (1936) 20. G. Dresselhaus, A.F. Kip, C. Kittel, Phys. Rev. 98, 368 (1955) 21. M. Cardona, F.H. Pollak, Phys. Rev. 142, 530 (1966) 22. J.M. Luttinger, W. Kohn, Phys. Rev. B 97, 869 (1955) 23. J.M. Luttinger, Phys. Rev. 102, 1030 (1956) 24. G.F. Koster, J.O. Dimmock, R.G. Wheeler, H. Statz, Properties of The Thirty-Two Point Groups (M.I.T. Press, Cambridge, MA, 1963) 25. P.O. Löwdin, J. Chem. Phys. 19, 1396 (1951) 26. F.H. Pollak, C.W. Higginbotham, M. Cardona, J. Phys. Soc. Jpn. 21(Supplement), 20 (1966) 27. H. Hazama, Y. Itoh, C. Hamaguchi, J. Phys. Soc. Jpn. 54, 269 (1985) 28. T. Nakashima, C. Hamaguchi, J. Komeno, M. Ozeki, J. Phys. Soc. Jpn. 54, 725 (1985) 29. H. Hazama, T. Sugimasa, T. Imachi, C. Hamaguchi, J. Phys. Soc. Jpn. 55, 1282 (1986) 30. L.C.L.Y. Voon, M. Willatzen, The k · p Method: Electronic Properties of Semiconductors (Springer, 2009) 31. D. Rideau, M. Feraille, L. Ciampolini, M. Minondo, C. Tavernier, H. Jaouen, Phys. Rev. B 74, 195208 (2006) 32. M.E. Kurdi, G. Fishman, S. Sauvage, P. Boucaud, J. Appl. Phys. 107, 013710 (2010) 33. F.H. Pollak, M. Cardona, C.W. Higginbotham, F. Herman, J.P. Van Dyke, Phys. Rev. B 2, 352 (1970) 34. M. Willatzen, M. Cardona, N.E. Christensen, Phys. Rev. B 50, 18054 (1994) 35. M. Cardona, N.E. Christensen, G. Fasol, Phys. Rev. B 38, 1806 (1988) 36. S. Richard, F. Aniel, G. Fishman, Phys. Rev. B 70, 235204–1 (2004) 37. D.W. Bailey, C.J. Stanton, K. Hess, Phys. Rev. B 42, 3423 (1990) 38. C. Jacoboni, L. Reggiani, Rev. Mod. Phys. 55, 645 (1983) 39. E.M. Conwell, High field transport in semiconductors, in Solid State Physics, Suppl. 9 (Academic, New York, 1967)

Chapter 2

Cyclotron Resonance and Energy Band Structures

Abstract Cyclotron resonance experiments were successfully used to determine the effective masses of electrons in the conduction band and holes in the valence bands. Electrons are subject to rotational motion in a magnetic field (cyclotron motion) and resonantly absorb the radiation fields (microwaves or infrared radiation) when the cyclotron frequency is equal to the radiation frequency. The resonant condition gives the effective mass of the electron. Analyzing the cyclotron resonance data of Ge and Si, detailed information of the electrons in the conduction band valleys. In addition, the analysis of the hole masses based on the k · p perturbation reveals the detailed valence band structures such as the heavy hole, light hole, and spin– orbit split–off bands. The non-parabolicity of the conduction band is also discussed. Quantum mechanical treatment of the electrons in the conduction band and holes in the valence bands leads us to draw the picture of Landau levels which is used to understand magnetotransport in Chap. 7 and quantum Hall effect in Chap. 8.

2.1 Cyclotron Resonance Cyclotron resonance has been successfully used to determine the effective masses of electrons in semiconductors. In addition, the cyclotron resonance has played a very important role in understanding the valence band structures of Ge and Si and later led to an accurate determination of the energy band structures. In this chapter first we will describe the cyclotron resonance experiment and its analysis in order to discuss the anisotropy of the electron effective mass and the many valley structures. Second, we will discuss the analysis of the valence band structures by using the k · p perturbation method, which will reveal the importance of the cyclotron resonance experiments. When a particle with electronic charge q is placed in a magnetic field, the particle make a circular motion in the plane perpendicular to the magnetic field. This motion is caused by the Lorentz force perpendicular to the magnetic field B and the velocity v of the particle, and is given by the relation F L = qv × B . © The Author(s), under exclusive license to Springer Nature Switzerland AG 2023 C. Hamaguchi, Basic Semiconductor Physics, Graduate Texts in Physics, https://doi.org/10.1007/978-3-031-25511-3_2

(2.1) 65

66

2 Cyclotron Resonance and Energy Band Structures

When the particle is not scattered, the equation of motion for a particle with mass m is given by m

dv = qv × B . dt

(2.2)

Assuming that the magnetic field is applied in the z direction and putting B = (0, 0, Bz ), the equation results in dvx = qv y Bz , dt dv y = −qvx Bz , m dt

m

which give rise to

d2 vx qvx Bz =− 2 dt m

(2.3)

for vx and a similar equation for v y . Therefore, the solutions for vx and v y are vx = A cos(ωc t), where ωc =

v y = A sin(ωc t), q Bz m

(2.4)

is the cyclotron (angular) frequency of the particle. From the results we find that the particle in a magnetic field Bz orbits with angular frequency ωc in the plane perpendicular to B (x, y plane) and the motion is referred to as “cyclotron motion.” When an electromagnetic field of frequency ω = ωc is applied, the particle absorbs the energy of the electromagnetic field resonantly. This is called cyclotron resonance. In semiconductors there exist various scattering processes and thus the particle (electron and hole) resonance is modified by the scattering. If we define the scattering time (or relaxation time) by τ , the condition for well-defined resonance is ωc τ 1 .

(2.5)

In other words, the cyclotron resonance is smeared out and no clear resonance is observed when condition (2.5) is not fulfilled. In order to observe clear cyclotron resonance, therefore, we have to apply a high magnetic field (higher B results in higher ωc and higher ω) or achieve a condition where less scattering occurs (longer τ is achieved at lower temperature T ). Let us consider the condition for a typical semiconductor with effective mass m ∗ = 0.1m (m = 9.1 × 10−31 kg is the free electron mass). When a magnetic field B = 1 T is applied, the cyclotron frequency is

2.1 Cyclotron Resonance

67

ωc =

1.6 × 10−19 × 1 2 × 1012 rad/s , 0.1 × 9.1 × 10−31

which corresponds to a microwave field of frequency f = ω/2π 3 × 1011 Hz. In addition, in order to realize the condition given by (2.5), ωc τ =

q Bz τ = μBz 1 , m∗

(2.6)

which requires a semiconductor sample with electron mobility greater than μ = 1m2 /Vs = 104 cm2 /Vs is required. A high magnetic field is achieved by using a superconducting solenoid and a high angular frequency electromagnetic field (ω = ωc ) by using microwave or infrared light. When we use an electromagnet, a field of 1 T is achieved and thus cyclotron resonance is observed in a sample with electron mobility larger than 104 cm2 /Vs. The electron mobility becomes higher at lower temperatures, where less phonon scattering occurs and the first observation of the cyclotron resonance was made at 4.2 K. At low temperatures electrons and holes are captured by donors and acceptors, and no free carriers exist for absorbing the microwave field. In the first cyclotron resonance measurements on Ge, light illumination was used to excite the carriers from the valence band to the conduction band, and resonance due to holes in addition to electrons was observed. Here we will discuss the cyclotron resonance curves. First we consider the case of an electron with isotropic effective mass m ∗ for simplicity. The equation of motion for the electron is m∗v dv + = q(E + v × B) . (2.7) m∗ dt τ The microwave field is linearly polarized with E = (E x , 0, 0), and the magnetic field is applied in the z direction as B = (0, 0, Bz ). When we write the microwave field with angular frequency ω as E = E x cos(ωt) = {E x exp(−iωt)}, we may use the relation d/dt = −iω and the motion of equation is written as 1 vx = q(E x + v y Bz ) , m ∗ −iω + τ 1 m ∗ −iω + v y = q(0 − vx Bz ) . τ

(2.8) (2.9)

From these equations we obtain qτ (1 − iωτ ) · Ex , ∗ m (1 − iωτ )2 + ωc2 τ 2 qτ ωc τ Ex , vy = − ∗ · m (1 − iωτ )2 + ωc2 τ 2

vx =

(2.10) (2.11)

and the current density in the x direction is deduced from the relation Jx = nqvx . This gives the power absorption P per unit volume given below.

68

2 Cyclotron Resonance and Energy Band Structures

1 1 nq 2 τ 2 1 − iωτ P = (Jx E x ) = E · 2 2 m∗ x (1 − iωτ )2 + ωc2 τ 2 1 1 1 2 + ≡ σ0 E x · 4 (1 − iωτ ) − iωc τ (1 − iωτ ) + iωc τ 1 1 1 2 + = σ0 E x , 4 (ω − ωc )2 τ 2 + 1 (ω + ωc )2 τ 2 + 1

(2.12)

where σ0 = nq 2 τ /m ∗ is the d.c. the conductivity of the semiconductor with carrier density n, and ωc = q B/m ∗ is the cyclotron angular frequency. The two terms on the right-hand side of (2.12) are plotted in Fig. 2.1 as the dotted curves, which are symmetric with respect to the peaked at ω = ±ωc and are called the Lorentz function FL (ω) =

Γ /2π . (ω − ωc )2 + (Γ /2)2

(2.13)

The Lorentz function given by the above equation has a full-width half-maximum of Γ and the integral of the Lorentz function with respect to ω is unity. Therefore, the Lorentz function behaves like a delta function when Γ becomes very small. The two peaks in Fig. 2.1a arise from different signs of the charge q and thus the curves for ωc < 0 and ωc > 0 correspond to the resonance for electrons and holes, respectively. When the microwave field is right-circularly polarized and left-circularly polarized, resonance is observed due to holes and electrons, respectively. The resonance curves of (2.12) for a linearly polarized microwave field are plotted by solid curves in Fig. 2.1b for ωτ = 0.5, 1.0, 2.0, 3.0, 4.0 and 5.0, where a clear resonance is seen for ωτ 1. In cyclotron resonance experiments a microwave field with fixed frequency is applied and the resonance due to the microwave absorption is detected as a function of the magnetic field. Therefore, the horizontal axis of Fig. 2.1 is the magnetic field (ωc /ω). From (2.12) and the curves in Fig. 2.1 it is evident that the full-width halfmaximum is 2/τ . Next, we consider the case of semiconductors with anisotropic effective masses such as in Ge and Si. Defining the effective mass tensor by m , the equation of motion for a carrier with electronic charge q is expressed as m · v˙ +

m ·v = q(E + v × B) . τ

(2.14)

Assuming the electric field and the carrier velocity are given by E = E exp(−iωt) and v = v exp(−iωt), respectively, and using the relation d/dt = −iω, the equation 1 −iω + m · v = q(E + v × B) τ

(2.15)

2.1 Cyclotron Resonance

69

Fig. 2.1 a The cyclotron resonance curves for a particle of mass m and charge q as a function of cyclotron frequency ωc = q B/m. The dotted green curve peaked in the right half (ωc > 0) is the resonance for holes with q > 0, and the dotted green curve peaked in the left half (ωc < 0) is the resonance for electrons with q < 0. These dotted curves correspond to the resonance due to a microwave field which is right-circularly polarized and left-circularly polarized, respectively. The solid curve is the absorption for a particle charge |q| in the case of a linearly polarized microwave. The curves are obtained for ωτ = 5. b Microwave absorption line shapes of the cyclotron resonance for ωτ = 0.5, 1.0, 2.0, 3.0, 4.0, and 5.0. The cyclotron resonance is clearly observed in the case of ωτ 1

is derived. In order to solve this equation we introduce the following variables: 1 ω = ω + i . τ

(2.16)

For simplicity (valid for Ge and Si) we assume that the effective mass m has diagonal parts only, i.e. ⎡ ⎤ 1/m 1 0 0 1 ⎢ ⎥ = ⎣ 0 1/m 2 0 ⎦ , (2.17) m 0 0 1/m 3 and that the magnetic field is applied in an arbitrary direction: B = (Bx , B y , Bz ) ≡ B(α, β, γ) . Then (2.15) can be rewritten as ⎧ ⎨ iω m 1 vx + q(v y Bz − vz B y ) = 0, iω m 2 vx + q(vz Bx − vx Bz ) = 0, ⎩ iω m 3 vx + q(vx B y − v y Bx ) = 0, where we put E = 0. This assumption of E = 0 is based on the fact that the resonance condition is derived in a vanishing electric field. Writing the magnetic field B = B(α, β, γ), (2.15) becomes

70

2 Cyclotron Resonance and Energy Band Structures

iω m 1 q Bγ −q Bβ −q Bγ iω m 2 q Bα = 0 , q Bβ −q Bα iω m 3

(2.18)

where ω = (ω + i/τ ) is used. From this equation a solution for ω is easily obtained. Under the condition of clear resonance (ωτ 1) we obtain ω ∼ = ω and thus we may put ω = ω = ωc . From these considerations the resonance condition is given by qB ωc = ∗ = q B m

m 1 α2 + m 2 β 2 + m 3 γ 2 , m1m2m3

(2.19)

where m ∗ is the cyclotron mass. Figure 2.2 shows a typical experimental setup for the cyclotron resonance experiment. A microwave field generated by a klystron (with a circuit to control the frequency constant) is guided by a waveguide and fed into a cavity with a semiconductor sample. The cavity is installed in a cryostat and the sample temperature is controlled down to 4.2 K. In order to achieve the condition ωc τ 1, the sample is cooled down to 4.2 K. At low temperatures the carriers in the semiconductor are frozen out and pulsed light is used to excite photo-carriers (electrons and holes). When the magnetic field is swept, the microwave absorption increases at resonance, which is detected by a microwave diode installed in the waveguide and amplified by a lock-in amplifier. Thus the measured microwave absorption versus magnetic field curve reveals cyclotron resonance. Typical experimental results are shown in Fig. 2.3 for Ge and

Fig. 2.2 Experimental setup for cyclotron resonance measurements. Microwave field generated by a klystron is guided to a cavity where a sample is inserted. The cavity is installed in a cryostat to be cooled down to 4.2 K. The carriers of the semiconductor sample are frozen out at low temperatures, and electrons and holes are excited by light illumination guided into the cavity by an optical pipe and the light is pulsed by a chopper to provide the reference signal for a lock-in amplifier. The magnetic field is swept slowly and the microwave absorption is recorded as a function of the magnetic field

2.1 Cyclotron Resonance

71

Fig. 2.3 Cyclotron resonance in Ge. ω/2π = 24 GHz, T = 4.2 K. The magnetic field is applied in the direction 60◦ with respect to the 001 axis in the (110) plane. (From Ref. [1])

Fig. 2.4 Cyclotron resonance in Si. ω/2π = 24 GHz, T = 4.2 K. The magnetic field is applied in the direction 30◦ with respect to the 001 axis in the (110) plane. (From Ref. [1])

in Fig. 2.4 for Si [1]. As seen in Figs. 2.3 and 2.4 signals due to several kinds of electrons and two holes (heavy holes and light holes) are observed. These complicated resonance peaks are discussed here but the detailed interpretation is described later. We now discuss the cyclotron mass. When we change the direction θ of the magnetic field with respect to the 001 axis in the plane (110) and calculate the cyclotron mass defined below from the magnetic field Bc for resonance, m∗ =

q Bc , ω

we obtain the cyclotron masses as a function of the direction θ, which are shown in Fig. 2.5 for Ge and in Fig. 2.6 for Si. The angular dependence of the cyclotron masses shown in Figs. 2.5 and 2.6 is analyzed as follows. From the results of the energy band calculations in Chap. 1, we learned that the conduction band minima of Ge are located at the L point along the

111 axis and that the conduction band minima of Si are located at the Δ point, 15% from the X point, along the 100 axis. When we take these axes as the principal axes of a newly defined k-vector and put k = 0 at the bottom of the conduction band, then the symmetry of the conduction band valleys leads to E=

2 2 2 2 (k x + k 2y ) + k . 2m t 2m l z

(2.20)

72

2 Cyclotron Resonance and Energy Band Structures

Fig. 2.5 Cyclotron masses of electrons in the conduction bands of Ge as a function of the magnetic field direction θ. The angle θ is the angle between the magnetic field and the

001 axis in the (110) plane. See the text for the valley indices 1, 2, …, 8

Fig. 2.6 Cyclotron masses of electrons in the conduction bands of Si as a function of the magnetic field direction θ. The angle θ is the angle between the magnetic field and the

001 axis in the (110) plane. See the text for the valley indices 1, 2, …, 6

The constant energy surfaces of the conduction bands are shown in Fig. 2.7 for Ge and in Fig. 2.8 for Si. Since the conduction bands consist of multiple energy surfaces, the conduction bands are called many valleys or many-valley structure. In Si there are 6 valleys, while in Ge there exist 4 valleys (the pairs of valleys along the principal axis are apart from the reciprocal lattice vector G and they are equivalent). The cyclotron mass in the conduction band with the ellipsoidal energy surface is given by (2.19) with m 1 = m 2 = m t , m 3 = m l as 1 = m ∗c

m t (1 − γ 2 ) + m l γ 2 , m 2t m l

(2.21)

where γ is the direction cosine between the magnetic field and the principal axis of the ellipsoid (k z direction), i.e. Bz = Bγ. Let us assume that the magnetic field is applied in the direction of the angle θ with respect to the 001 axis in the (110) plane. In this case we have

2.1 Cyclotron Resonance

73

Fig. 2.7 Many-valley structure of the conduction bands in Ge

Fig. 2.8 Many-valley structure of the conduction bands in Si

sin θ sin θ B = B √ , √ , cos θ ≡ Be B . 2 2 First we consider the case of Ge. As stated above, 4 valleys should be taken into account, but here we have 8 valleys (we find pairs along the principal axis are degenerate in the following). The unit vectors of the principal axes are 1 em : ± √ (1, 1, 1) 3 1 ± √ (−1, 1, 1) 3 1 ± √ (−1, −1, 1) 3 1 ± √ (1, −1, 1) 3

(valleys: 1, 2), (valleys: 3, 4), (2.22) (valleys: 5, 6), (valleys: 7, 8),

74

2 Cyclotron Resonance and Energy Band Structures

and therefore the direction cosine γ is given by γ = em · e B 1 √ = ± √ ( 2 sin θ + cos θ); (valleys: 1, 2) , 3 1 = ± √ (cos θ) (valleys: 3, 4, 7, 8) , 3 √ 1 = ± √ (− 2 sin θ + cos θ) (valleys: 5, 6) . 3

(2.23)

Inserting these relations into (2.21) we obtain three solid curves as shown in Fig. 2.5, where we used the following parameters for the masses: m t = 0.082 m ,

m l = 1.58 m .

(2.24)

In Fig. 2.5 good agreement is found between the experimental data and the calculated curves. Next, we consider the case of Si, where the constant energy surfaces of the conduction band consists of 6 valleys along the 100 directions as shown in Fig. 2.8. We have already shown from the energy band calculations in Chap. 1 that the conduction band minima are located at k x = 0.85(2π/a) near the X point in the Brillouin zone. When we choose the angle θ between the magnetic field and the 001 axis in the (110) plane, the direction cosine γ is given by 1 γ = ± √ sin θ (valleys: 1, 2, 3, 4) , 2 γ = ± cos θ (valleys: 5, 6) .

(2.25)

Substituting the above relations in (2.21) and assuming m t = 0.19 m ,

m l = 0.98 m ,

(2.26)

we obtain the solid curves in Fig. 2.6, which show good agreement with the experimental observations.

2.2 Analysis of Valence Bands We see in Figs. 2.3 and 2.4 that there exist two resonance peaks for holes in Ge and Si and that the curves are quite simple compared to the resonance curves for electrons. However, the analysis of the cyclotron resonance for holes is very complicated and requires more detailed analysis based on the k · p perturbation method as stated later.

2.2 Analysis of Valence Bands

75

Fig. 2.9 Cyclotron masses of holes in Ge. θ is the angle between the magnetic field and

001 axis in the (110) plane

Fig. 2.10 Cyclotron masses of holes in Si. θ is the angle between the magnetic field and

001 axis in the (110) plane

First, we plot the cyclotron masses of holes as a function of the angle between the magnetic field and the 001 axis in the (110) plane, which are shown in Fig. 2.9 for Ge and in Fig. 2.10 for Si. In the figures we find the angular dependence of the hole cyclotron masses exhibits quite different features compared with the electron cyclotron masses. The two hole masses do not cross each other and thus we can conclude that there exist two different holes. We define the heavy holes for the heavy effective-mass carriers and light holes for the light effective-mass carriers. As seen in Figs. 2.9 and 2.10 the heavy hole mass is anisotropic but the light hole mass is isotropic with narrower full-width half maximum. These features are well explained with the help of valence band analysis based on the k · p perturbation method. In the following we will consider valence band analysis by the k · p perturbation method [1]. As described in the energy band calculations of Chap. 1, the valence band top is located at the Γ point (k = 0) and the valence bands are triply degenerate when the spin–angular orbit interaction is disregarded. The three valence bands are expressed by the symmetry of Γ25 , whose basis functions are given by |X , |Y , and |Z . Also, we know that the lowest conduction band at the Γ point has the symmetry Γ2 and the basis function is |x yz. For simplicity, first we consider only these four bands in the k · p perturbation method. When the perturbation term is disregarded, the eigenstates and the eigenvalues of these four bands are given by H0 | j = E j | j ,

(| j = |Γ2 , |X , |Y , |Z ) ,

(2.27)

76

2 Cyclotron Resonance and Energy Band Structures

or the matrix elements of H0 for the four bands are |Γ2 |X |Y |Z ⎤ Ec 0 0 0 ⎢ 0 0 0 ⎥ Ev ⎢ ⎥. ⎣ 0 0 Ev 0 ⎦ 0 0 0 Ev ⎡

(2.28)

Next, we consider how the energy bands are modified by applying the k · p perturbation. This perturbation yields 2 k 2 | j ≡ λ j | j , (H0 + H1 )| j = E j − 2m where λj = Ej −

2 k 2 . 2m

(2.29)

(2.30)

The above equation gives the following relation:

Γ2 |H1 |X = Γ2 | − i

2 ∂ 2 k · ∇|X = x yz| − i k x |yz m m ∂x

≡ Pk x .

(2.31)

Thus we obtain the following matrix: |X |Y |Z |Γ2 ⎤ Ec − λ j Pk x Pk y Pk z ⎥ ⎢ Pk x Ev − λ j 0 0 ⎥ = 0. ⎢ ⎦ ⎣ Pk y 0 Ev − λ j 0 0 0 Ev − λ j Pk z ⎡

(2.32)

From the above equation we obtain E1,2

Ec + Ev ± = 2

Ec − Ev 2

E3,4 = Ev +

2 + P 2k2 +

2 k 2 . 2m

2 k 2 , 2m

(2.33)

(2.34)

The results mean that the perturbation term H1 gives rise to a splitting of the three valence bands: one valence band, E2 , and doubly degenerate valence bands, E3 and E4 . However, the degenerate valence bands exhibit minima at the Γ point (k = 0), which is unreasonable for the valence band characteristic because a light hole and

2.2 Analysis of Valence Bands

77

a heavy hole are observed in the cyclotron resonance measurements. The features of the valence bands are well explained when we take into account the spin–orbit interaction, which will be discussed in detail later. Next, we consider more accurate k · p perturbation. As described in Sect. 1.7, the energy band calculations take into account many bands in addition to Γ25 and Γ2 . Therefore, the unreasonable results obtained above are due to the fact that we disregarded other conduction bands than the conduction band Γ2 . We will discuss a general treatment of the k · p perturbation method in the following. The more accurate treatment of the valence bands has been reported by Dresselhaus, Kip, and Kittel [1] and Luttinger and Kohn [7]. Here we will follow the method of Luttinger and Kohn. In the perturbing Hamiltonian, 2 k 2 | j , (H0 + H1 )| j = E j − 2m

(2.35)

we consider all eigenstates in addition to the degenerate valence bands |Γ25 . We learned from the above treatment that the closest conduction band Γ2 affects the perturbation only slightly. Therefore, we consider the second-order perturbation in order to calculate (2.35) and neglect the first-order perturbation. The eigenstates of the valence bands Γ25 at k = 0 are defined as | j = |X , |Y , |Z , and the eigenvalues are given by E j = Ev ≡ E0 . The second-order perturbation of (2.35) for the valence bands Γ25 leads to the following result: 2 k 2 j|H1 |i i|H1 | j + + E0 , (2.36) E= 2m E0 − Ei i, j where the eigenstates | j, | j are the triply-degenerate valence bands Γ25 (|X , |Y , and |Z ) with eigenvalue E0 and the eigenstates |i correspond to any bands with eigenvalue Ei other than the valence bands Γ25 . Since the perturbation term is given by 2 2 ∂ ∂ ∂ kx + ky + kx H1 = k · p = −i k · ∇ = −i m m m ∂x ∂y ∂z kl pl , = (k x px + k y p y + k z pz ) = m m l=x,y,z

(2.37)

78

2 Cyclotron Resonance and Energy Band Structures

Equation (2.36) is written as E(k) = E0 + ≡ E0 +

l m 2 k 2 2 π ji πi j kl k m + 2 2m m l,m i, j E0 − Ei

Dlm j j kl k m ,

(2.38)

j

l,m

where we define the following relations:

i| pl | j = πil j , Dlm j j =

(2.39)

l m 2 2 π ji πi j δ j j δlm + 2 . 2m m i E0 − Ei

(2.40)

The eigenstates of the valence bands | j and | j of Γ25 have the symmetry |X = |yz, |Y = |zx, |Z = |x y as stated before and therefore we find that there are three combinations of the subscripts j, j , l, m: xx 1

yy 2

XX 1

YY 2

and

zz 3

yz, zy 4

x z, zx 5

x y, yx , 6

Z Z Y Z , Z Y X Z , Z X X Y, Y X . 3 4 5 6

Using the tensor notation α, β = 1, 2, 3, 4, 5, 6,

(2.41)

the matrix elements are rewritten as Dilmj ≡ Dαβ ,

(2.42)

where Dlm j j are fourth-rank tensors. In the case of cubic crystals we have the following components D11 D12 D12 0 0 0 D12 D11 D12 0 0 0 D12 D12 D11 0 0 0 (2.43) 0 0 0 D44 0 0 , 0 0 0 0 D44 0 0 0 0 0 0 D44

2.2 Analysis of Valence Bands

79

and the non-zero components are yy

D11 = D Xx xX = DY Y = D ZzzZ = L , yy

yy

D12 = D X X = D XZ ZX = DYx xY = DYzzY = D Zx xZ = D Z Z = M, D44 =

xy DXY

+

yx DXY

=

yz DY Z

+

zy DY Z

(2.44)

= D ZzxX + D Zx zX = N .

From these results, the matrix elements of the k · p Hamiltonian are given by |X |Y |Z 2 2 2 Ck x k y Ck x k z

X | Ak x + B(k y + k z )

Y | Ck x k y Ak 2y + B(k x2 + k z2 ) Ck y k z .

Z | Ck x k z Ck y k z Ak 2 + B(k 2 + k 2 ) z

x

(2.45)

y

The three parameters A, B, and C of Luttinger are written as [2] A=

x πixX 2 2 π Xi + 2 , 2m m i E0 − Ei

(2.46a)

B=

y y 2 π Xi πi X 2 + 2 , 2m m i E0 − Ei

(2.46b)

C=

y y x x πiY + π Xi πiY 2 π Xi . m2 i E0 − Ei

(2.46c)

The secular equation of (2.45) gives the eigen energy E(k), while the k · p Hamiltonian of Dresselhaus, Kip, and Kittel [1] is given by replacing A, B, and C with the following parameters, L, M, and N defined by (2.44), respectively L=

x πixX 2 π Xi , m 2 i E0 − Ei

(2.47a)

M=

y y 2 π Xi πi X , m 2 i E0 − Ei

(2.47b)

N =

y y x x πiY + π Xi πiY 2 π Xi , m2 i E0 − Ei

(2.47c)

and the corresponding secular equation gives the eigen energy λ = E(k) − 2 k 2 /2m. The k · p perturbation gives rise to a splitting of the triply degenerate valence bands at k = 0 and the E(k) curves are given by (2.45), which are shown on the left of Fig. 2.11. Here we have to note that the cyclotron resonance tells us the existence

80

2 Cyclotron Resonance and Energy Band Structures

Fig. 2.11 Valence band structure. The left figure shows the splitting of the valence bands at k = 0 due to the interaction between the bands, and the right figure shows the valence band structures obtained by taking the spin–orbit interaction into account, where the heavy hole and light hole bands are doubly-degenerate at k = 0 and the lowest band is the spin–orbit split-off band due to the spin–orbit interaction (see Sect. 2.3)

of two hole bands, not triply degenerate bands at k = 0. This is explained when we take the spin–orbit interaction into account as shown in the next section and the results are shown on the right of Fig. 2.11.

2.3 Spin–Orbit Interaction The interaction between spin angular momentum and orbital angular momentum is due to the relativistic effect of the electrons [1–3]. In Appendix H the derivation of the spin–orbit interaction Hamiltonian is described in detail.1 Here we use the interaction Hamiltonian Hso given by Hso = ξ(r )L · S, 1 1 dV ξ(r ) = , 2m 2 c2 r dr

1

See also Sect. 1.7 of Chap. 1 and (1.146).

(2.48) (2.49)

2.3 Spin–Orbit Interaction

81

where L and S are the orbital and spin angular momentum, respectively. When we define S = σ, 2 the Pauli spin matrix is given by

01 0 −i 1 0 σx = , σy = , σz = . 10 i 0 0 −1

(2.50)

Here the spin states Sz = +/2 and Sz = −/2 are sometimes referred to as ↑ spin and ↓ spin and their eigenstates are 1 0 | ↑ = |α = , | ↓ = |β = . 0 1

(2.51)

Next, we define the angular momentum operators for the Γ25 valence bands. As stated in Sect. 2.2 the eigenstates of the valence bands at k = 0 are expressed by |X , |Y , |Z . Their angular momentum L = r × p has a quantum number of unity and the matrix representation of the operator is ⎡ ⎤ ⎡ ⎡ ⎤ ⎤ 10 0 010 0 −i 0 ⎣ 1 0 1 ⎦ , L y = √ ⎣ i 0 −i ⎦ , L z = ⎣ 0 0 0 ⎦ . Lx = √ 2 010 2 0 i 0 0 0 −1

(2.52)

When we choose the basis of the eigenstates defined by ⎡ ⎤ 1 1 u + = √ (|X + i|Y ) = ⎣ 0 ⎦ , 2 0 ⎡ ⎤ 0 1 u − = √ (|X − i|Y ) = ⎣ 0 ⎦ , 2 1 ⎡ ⎤ 0 u z = |Z = ⎣ 1 ⎦ , 0

(2.53a)

(2.53b)

(2.53c)

the angular momentum operators are given by L ± = L x ± iL y , where L+ =

√

⎡

⎤ 010 2 ⎣ 0 0 1 ⎦ , 000

L− =

√

(2.54) ⎡

⎤ 000 2 ⎣ 1 0 0 ⎦ . 010

(2.55)

82

2 Cyclotron Resonance and Energy Band Structures

Similarly, the spin momentum operators are expressed as σ± = σx ± iσ y ,

(2.56)

and their matrix representations are given by

01 00 σ+ = 2 , σ− = 2 . 00 10

(2.57)

Using these results, the Hamiltonian of the spin–orbit interaction becomes Δ L·σ Δ = L x σ x + L y σ y + L z σz Δ 1 = (L + σ− + L − σ+ ) + L z σz , 2

Hso =

(2.58)

where 3Δ = Δ0 is called spin–orbit splitting energy and gives the value of the energy splitting of the valence bands at k = 0. The six states of the valence bands |u + α, |u + β, |u z α, |u − β, |u − α, |u z β give rise to the matrix elements of the spin–orbit interaction Hamiltonian: u α u+β u z α u−β u−α u z β + Δ 0 0 √0 0 0 0 −Δ 2Δ 0 0 0 √ 0 2Δ 0 0 0 0 . 0 0 0 Δ 0 √0 0 0 0 0 √ −Δ 2Δ 0 0 0 0 2Δ 0

(2.59)

Expression (2.59) is derived as follows: L + σ− |u + α = L + |u + σ− |α ⎡ ⎤⎡ ⎤ 010 1 √ 0 = 2 ⎣ 0 0 1 ⎦ ⎣ 0 ⎦ × 2 1 000 0 L − σ+ |u + α = L − |u + σ+ |α ⎡ ⎤⎡ ⎤ 000 1 √ 0 = 2 ⎣ 1 0 0 ⎦ ⎣ 0 ⎦ × 2 0 010 0

0 0

1 =0 0

1 0

1 =0 0

(2.60a)

(2.60b)

2.3 Spin–Orbit Interaction

83

⎡

⎤⎡ ⎤ 10 0 1 1 0 1 ⎣ ⎦ ⎣ ⎦ 0 L z σz |u + α = 0 0 0 0 −1 0 0 0 −1 0 ⎡ ⎤ 1 1 = |u + |α = |u + α . = ⎣0⎦ 0 0

(2.60c)

Using the above results we find

u + α|L z σz |u + α = ,

(2.61)

and a similar treatment gives the results of (2.59). Expression (2.59) is expressed as a 6 × 6 matrix and many of the non-diagonal elements have the value 0. When we investigate the matrix of (2.59), we find that the matrix is factorized into two 3 × 3 matrices and that they are also factorized into two matrices of dimensions 1 × 1 and 2 × 2. The 2 × 2 matrix is easily diagonalized and (2.59) reduces to Δ 0 0 0 0 0 0 Δ 0 0 0 0 0 0 −2Δ 0 0 0 (2.62) 0 0 0 Δ 0 0 . 0 0 0 0 Δ 0 0 0 0 0 0 −2Δ From the result given in (2.62) we see that the 6-fold degenerate valence bands split into 4-fold valence bands with energy shifted by Δ, consisting of the heavy hole and light hole bands, and into a doubly degenerate spin–orbit split-off band shifted down by 2Δ. These features are shown in Fig. 2.11. It should be noted that the 4-fold degenerate bands at k = 0 split into the doubly degenerate heavy hole and light hole bands at k = 0. The corresponding eigenstates are given by the following equations. The fourfold valence band–edge eigenstates are u v1 u v2

3 3 1 = |u + α = √ |(X + iY ) ↑ , = , 2 2 2 3 1 1 2 |u z α = − √ |u + β − = , 2 2 3 3 1 = − √ [|(X + iY ) ↓ + 2 |Z ↑ ] , 6

(2.63a)

(2.63b)

84

2 Cyclotron Resonance and Energy Band Structures

u v3

u v4

3 1 1 2 |u z β = , − = − √ |u − α − 2 2 3 3 1 = − √ [|(X − iY ) ↑ + 2 |Z ↓ ] , 6 3 3 1 = , − = |u − β = √ |(X − iY ) ↓ , 2 2 2

(2.63c) (2.63d)

and for twofold spin–spit off bands are u v5 = = u v6 = =

1 1 2 1 , 2 2 = − 3 |u + β + 3 |u z α 1 − √ [|(X + iY ) ↓ − |Z ↑ ] , 3 1 1 , − = − 2 |u − α + √1 |u z β 2 2 3 3 1 − √ [|(X − iY ) ↑ − |Z ↓ ] . 3

(2.63e)

(2.63f)

The eigenstates with the time reversal symmetry are reported by Luttinger and Kohn [7], which are shown by (2.137b)–(2.137g). Now we discuss the cyclotron masses or the effective masses of the valence bands by deriving the k dependence of the bands. This is done by applying the method of Luttinger and Kohn [7] to the analysis of the valence bands, where we have to use the eigenstates (basis functions) derived by taking the spin–orbit interaction into account. This approach has been adopted by Dresselhaus, Kip and Kittel [1]. They used the eigenfunctions of (2.63a)–(2.63f) and calculated the matrix elements of the Hamiltonian with the spin–orbit interaction. Defining the matrix element Hi j by H11 = Lk x2 + M(k 2y + k z2 ) , H22 = Lk 2y + M(k z2 + k x2 ) , H33 = Lk z2 + M(k x2 + k 2y ) , H12 = N k x k y , H23 = N k y k z , H13 = N k x k z , the result is given by the 6 × 6 matrix of (62) in their paper [1]:

2.3 Spin–Orbit Interaction

85

H13 − iH23 H11 − H22 − 2iH12 H11 + H22 − − √ √ 2 3 2 3 H13 + iH23 4H33 + H11 + H22 − 0 √ 6 3 H − H + 2iH 4H33 + H11 + H22 11 22 12 0 √ − 6 2 3 − H + 2iH + iH23 H H 11 22 12 13 0 − √ √ 2 3 3 H13 + iH23 H11 + H22 − 2H33 H13 − iH23 − − √ √ √ 6 3 2 2 H − H + 2iH H13 + iH23 H11 + H22 − 2H33 11 22 12 √ √ √ − 6 2 3 2

0 H11 − H22 − 2iH12 √ 2 3 H13 − iH23 √ 3 H11 + H22 2 H11 − H22 − 2iH12 √ 6 H13 − iH23 − √ 6

−

H13 − iH23 H11 − H22 − 2iH12 − √ √ 6 6 H11 + H22 − 2H33 H13 − iH23 − √ √ 2 3 2 H13 + iH23 H11 + H22 − 2H33 √ √ 2 3 2 . H11 − H22 + 2iH12 H13 + iH23 − √ √ 6 6 H11 + H22 + H33 0 − Δ0 3 H11 + H22 + H33 0 − Δ0 3 −

(2.64)

The matrix of (2.64) is approximately divided into two matrices comprising the upper-left 4 × 4 matrix and the lower-right 2 × 2 matrix [1]. The other two blocks of 2 × 4 will give rise to an error of the order of k 4 /Δ0 and thus the above approximation is accurate enough to enable us to discuss the valence bands. The 4 × 4 matrix gives the solutions of (for derivation see Problem (2.7) and its answer) E(k) = Ak 2 ±

B 2 k 4 + C 2 (k x2 k 2y + k 2y k z2 + k z2 k x2 ) ,

(2.65)

where 1 (L + 2M), 3 1 B = (L − M), 3 1 C = [N 2 − (L − M)2 ] , 3 A=

(2.66)

86

2 Cyclotron Resonance and Energy Band Structures

Fig. 2.12 Energy contour lines of the valence bands in Si , a the heavy–hole band in the (k x , k y , k z ) space for E = 0.20 [eV], b the heavy–hole band in the (001) plane (k z = 0), and c the light–hole band in the (001) plane (k z = 0), where k x , k y , k z are in units of 2π/a

where the coefficients A, B, and C differ from the parameters of (2.46a)–(2.46c) defined by Luttinger. On the other hand, from the 2 × 2 matrix we obtain the solutions E(k) = Ak 2 − Δ0 .

(2.67)

Equation (2.65) gives the k dependence of the heavy and light holes in the valence bands and (2.67) leads to the spin–orbit split-off band. It is evident from the above analysis that the splitting is due to the spin–orbit interaction. The constant energy surface of the heavy-hole band is not spherical for C = 0 but warped as shown in Fig. 2.12a, where the energy contour of the heavy hole band of Si in the (k x , k y , k z ) space for E = 0.20 [eV] are shown, and the contour lines in the in the (001) plane for k z = 0 are plotted in Fig. 2.12b in the region k x ≤ 0.1, k y ≤ 0.1. Energy contour of the heavy hole band in the region of k x , k y , k z 0 are spherical but for larger values of k x , k y and k z the contour lines are warped. On the other hand, the light-hole band is almost spherical in the wide range of wave vectors as seen in Fig. 2.12c. As stated above, the valence bands, especially the heavy hole band, are complicated and thus require us to use a different approach for the analysis of the cyclotron masses in the valence bands [1]. We use the cylindrical coordinates (k H , ρ, φ) for the wave vector of the hole, where k H is the z component of the wave vector (parallel to the applied magnetic field). Using this notation the cyclotron mass is expressed as 2 m = 2π ∗

ρ dφ . ∂E/∂ρ

(2.68)

Assuming the magnetic field is applied in the (001) plane and putting k H = 0, we obtain

2.3 Spin–Orbit Interaction

87

2 m = π ∗

π/2

0

dφ A±

{B 2

+

1 2 C [1 4

+ g(φ)]}1/2

,

(2.69)

where g(φ) = −3(3 cos2 θ − 1)[(cos2 θ − 3) cos4 φ + 2 cos2 φ] ,

(2.70)

and θ is the angle with respect to the (001) axis in the (110) plane. The term g(φ) is expanded as m∗ =

1 2 2 2 A ± B + (C/2)2 C 2 (1 − 3 cos2 θ)2 + ··· . × 1± 64 B 2 + (C/2)2 A ± B 2 + (C/2)2

(2.71)

Using these results and choosing the parameters A, B and C to fit the experimental data of the cyclotron mass we find the curves shown in Figs. 2.9 and 2.10. From these analyses we derive the valence band parameters A, B and C, which are listed below. A = −(13.0 ± 0.2)(2 /2m) , |B| =

(8.9 ± 0.1)(2 /2m) ,

|C| =

(10.3 ± 0.2)(2 /2m) ,

(2.72)

for Ge and A = −(4.1 ± 0.2)(2 /2m) , |B| =

(1.6 ± 0.2)(2 /2m) ,

|C| =

(3.3 ± 0.5)( /2m) ,

(2.73)

2

for Si. It may be pointed out here that the parameters L, M and N are easily deduced from (2.66) using the values of A, B and C given above [1]. The effective masses of the heavy and light holes averaged in k space are

C2 , B2 + 5 m C2 , B2 + ∗ = −A + m lh 5

m = −A − m ∗hh

(2.74) (2.75)

88

2 Cyclotron Resonance and Energy Band Structures

where A, B, and C are given by dimensionless values in units of 2 /2m.2 The average effective masses of the heavy and light holes are estimated to be 0.336 m (0.520 m) and 0.0434 m (0.159 m) for Ge (Si), respectively.

2.4 Non-parabolicity of the Conduction Band We are concerned with the valence band structure by taking the spin–orbit interaction in the previous section. Here in this section we will deal with the effect of the spin– orbit interaction on the conduction band, where we consider the conduction band |Γ2 and the valence bands |Γ25 only for simplicity. In this approximation the matrix elements of the k · p Hamiltonian are Ec0 − λ 0 0 √ Pk 0 E − Δ /3 − λ 2Δ /3 0 v0 0 0 √ = 0, Pk 2Δ0 /3 Ev0 − λ 0 0 0 0 Ev0 + Δ0 /3 − λ

(2.76)

where P = (/m) Γ2 | px | X is defined by (2.31) and λ = E − k 2 . For simplicity we put k x = k y = 0, k z = k without any loss of generality. From the upper-left 3 × 3 matrix we obtain 2Δ0 Δ0 λ − Ev0 + λ − Ev0 − λ − Ec0 3 3 Δ0 2 2 = 0. −P k λ − Ev0 + 3

(2.77)

We may write Ec = Ec0 ,

Ev = Ev0 +

Δ0 , 3

Ec − Ev − EG ,

(2.78)

and then (2.77) reduces to 2Δ0 = 0. λ − Ev + Δ0 λ − Ev λ − Ec − P 2 k 2 λ − Ev + 3

2

In many references the average effective mass is expressed as m C2 = −A ± B 2 + , m∗ 6

which should be corrected as above.

(2.79)

2.4 Non-parabolicity of the Conduction Band

89

Since we are interested in the effective mass of the conduction band edge, the term 2 k 2 /2m is taken to be small and λ in the terms other than λ − Ec is replaced by Ec . This approximation gives rise to λ = Ec (k) − or E(k) =

P 2 k 2 (Ec − Ev + 2Δ0 /3) 2 k 2 = + Ec , 2m (Ec − Ev + Δ0 )(Ec − Ev )

P 2k2 2 k 2 + 2m 3

2 1 + Ec , + EG EG + Δ0

(2.80)

(2.81)

and therefore the band edge effective mass m ∗0 is obtained as 2P 2 1 1 + ∗ = m0 m 32

2 1 + EG EG + Δ0

.

(2.82)

We introduce energy parameter E P0 which is often used to analyze the valence band parameters, E P0 =

2 2 P , m 0

(2.83a)

P0 = Γ25 (X )| px |Γ2 ,

P=

P0 , m

(2.83b)

and then (2.82) is rewritten as 1 E P0 1 + = m ∗0 m 3m

2 1 + EG EG + Δ0

(2.84)

This relation is known to explain the observed effective masses quite well in III–V compound semiconductors, as shown below. Here we discuss the case of GaAs as an example. The parameter E P0 = (2/m)P02 is rewritten by using the definition of 2 2 /(2m)(= Pau in atomic units) Pau = 2P0 used by Cardona and Pollak [4] as E P0 = Pau 2 3 = 1.32 × 13.6 = 23.7 eV (see Table 1.13), the energy gap EG = 1.53 eV and the spin–orbit split-off energy Δ0 = 0.34 eV give the band-edge effective mass m ∗0 = 0.0643 m from (2.84), which is in good agreement with the observed value 0.067 m. When we put the relation λ = Ec (k) − k 2 (= Ec (k) − 2 k 2 /2m) into (2.79), the k dependence of the energy of the conduction band electrons Ec (k) deviates from the parabolic band 2 k 2 . (2.85) Ec (k) = 2m ∗0

Note that P used in Tables 1.11 and 1.13 is Pau = 2 Γ2 | px | X = 2P0 and thus E P0 = 2 /2m which is equivalent to P 2 in atomic units. (2/m)P02 = Pau au

3

90

2 Cyclotron Resonance and Energy Band Structures

Such a band is called a non-parabolic band. The conduction band of the order of k 4 is obtained by neglecting the term λ3 which gives the energy of the order of k 6 . The solution of the quadratic equation of λ is given by E(k) =

2 3EG + 4Δ0 + 2Δ20 /EG m ∗0 2 2 k 2 2 k 2 . − 1 − 2m ∗0 m 2m ∗0 (EG + Δ0 )(3EG + 2Δ0 )

(2.86)

Another good example of a non-parabolic conduction band is the case of InSb, where Δ0 EG is satisfied. In this case we may approximate (2.79) by (λ − Ec )(λ − Ev ) −

2 2 2 P k = 0, 3

(2.87)

and thus the conduction band is expressed by the following equation. Ec + Ev 2 k 2 + + E(k) = 2m 2

2 (Ec − Ev )2 + P 2k2 . 4 3

(2.88)

This approximation is done by considering the conduction band and the top valence band only, and thus it is called the two-band approximation. When the energy reference is taken to be the conduction band bottom (Ec = 0), the conduction band non-parabolicity is expressed as 2 8P 2m 2 k 2 +1 1+ 2m 3EG2 2 4E p 2 k 2 EG 2 k 2 + +1 , = 1+ 2 · 2m 2 2m EG

EG 2 k 2 + E(k) = 2m 2

(2.89)

where the relation (note the difference between E p and E P0 ) Ep =

4m P 2 2 ≡ E P0 2 3 3

(2.90)

is used.4 Equation (2.89) gives the solution for 2 k 2 /2m EG + E p 4E p E 2 k 2 . =E+ 1− 1+ 2m 2 (EG + E p )2

(2.91)

In Sect. 2.6 we deal with the Luttinger parameters and introduce E P0 = (2/m)P02 with the momentum matrix element P0 = Γ2 | px |X . The parameter E P0 is often cited for the analysis of the valence band states and of the Luttinger parameters [2, 22]. The values of E P0 for various semiconductors range from 19 to 27 eV. The matrix element introduced by Cardona and Pollak [4] is P = 2P0 and E P0 = P 2 /2m. Also note the difference between the subscripts of E p and of E P0 . 4

2.4 Non-parabolicity of the Conduction Band

91

When E is small, the terms of the square root of the above equation may be expanded to give the following result: ! " E p2 E 2E p3 E 2 EG 2 k 2 =E + − +····· . 2m EG + E p (EG + E p )3 (EG + E p )5

(2.92)

From the fact that the energy band approaches the parabolic band E = 2 k 2 /2m ∗0 in the limit of E → 0, the band-edge effective mass is given by m ∗0 /m =

EG . EG + E p

(2.93)

For example, in the case of InSb we have EG = 0.235 eV, m ∗0 /m = 0.0138, Δ0 = 0.9 eV, and thus the condition Δ0 > EG is satisfied. From the above result we obtain E p ≈ 17 eV, which shows a good agreement with the parameter used for the energy band calculations, E p ≈ 20 eV. From (2.92) and (2.93) the dispersion of the conduction band is rewritten as 2 k 2 = γ(E) = E[1 + αE + βE 2 + · · · · ·] , 2m ∗0

(2.94)

where α and β are defined by m ∗0 2 1 α= = 1− · , EG (EG + E p )2 m EG E p2

β=−

2E p3 EG (EG + E p )4

.

(2.95) (2.96)

Since EG E p in general, we can neglect the terms beyond the second term on the right-hand side and we obtain E 2 k 2 , ≡ γ(E) = E 1 + 2m ∗0 EG

(2.97)

which is referred to in the literature very often to express the conduction band nonparabolicity.

92

2 Cyclotron Resonance and Energy Band Structures

2.5 Electron Motion in a Magnetic Field and Landau Levels 2.5.1 Landau Levels In this section we will deal with the motion of an electron in a magnetic field using the effective-mass equation described in Sect. 3.2. The treatment is based on the method developed by Kubo et al. [5, 6]. The Hamiltonian of an electron in a magnetic field B is written as 1 (2.98) H= ( p + e A)2 , 2m where A is the vector potential defined as B = ∇ × A.

(2.99)

Since the vector potential satisfies the relation ∇ · A = 0, we find the following relation A · p − p · A = i∇ · A = 0 (2.100) and thus the momentum operator and the vector potential commute with each other. We define the following general momentum operator [5]: π = p + eA.

(2.101)

Then the effective mass Hamiltonian is given by the following equation: H = E0 (π) + U (r) ,

(2.102)

where E0 ( p) represents the Bloch state of the electron with crystal momentum p = k and U (r) is the perturbing potential. As shown in Chap. 3 the effectivemass equation allows us to express the operator as E0 (−i∇) without a magnetic field or E0 (−i∇ + e A) with a magnetic field. The momentum operator satisfies the following commutation relation: π × π = −ie B .

(2.103)

When the magnetic field B is applied in the z direction, we obtain πx = px + e A x ,

(2.104a)

πy = py + e A y , πz = pz

(2.104b) (2.104c)

and thus the commutation relations are

2.5 Electron Motion in a Magnetic Field and Landau Levels

#

$ πx , π y = −ieBz # $ [πx , x] = π y , y = −i .

93

(2.105a) (2.105b)

Here we introduce following new variables ξ=

1 1 πy , η = − πx , eBz eBz

X = x − ξ, Y = y − η .

(2.106a) (2.106b)

Using (2.105b) we obtain the following relation, [ξ, η] =

1 i eBz

≡

− i eB1 z

l2 i

(2.107a)

2 − li

(2.107b)

≡ [X, Y ] = [ξ, X ] = [η, X ] = [ξ, Y ] = [η, Y ] = 0 , where l=

/eBz

(2.107c)

(2.108)

is the cyclotron radius of the ground state (called as “magnetic length”) and is independent of the electron effective mass. From the commutation relations stated above, the combination of the following variables form a complete set of canonical variables: (ξ, η), (X, Y ), ( pz , z) . The Hamiltonian is then expressed as follows by using the relative coordinates: H=

2 k z2 2 2 2 (ξ + η ) + . 2m ∗l 4 2m ∗

(2.109)

As an example, we deal first with the case without a perturbing potential (U = 0). Since the Hamiltonian E0 (π) does not include X and Y , these variables will not change in time. This is consistent with the physical model of the cyclotron motion of the electron, where the coordinates (X, Y ) represent the cyclotron motion in the plane x–y perpendicular to the magnetic field B. For this reason the coordinates (X, Y ) are called the center coordinates of the cyclotron motion. It is evident from (2.106b) that ξ and η represent the relative coordinates of the cyclotron motion (X, Y ). We also find the following relation from (2.107b) and the uncertainty principle: ΔX ΔY = 2πl 2 =

h . eBz

(2.110)

This relation is sometimes referred to as the degeneracy in a magnetic field of the eigenstate E0 (πx , π y , pz ). Since the energy eigenvalue is independent of (X, Y ),

94

2 Cyclotron Resonance and Energy Band Structures

the energy eigenvalue is unchanged under the movement of the cyclotron center coordinates (x, y). When the size of a sample in the directions of x and y is assumed to be L x and L y , respectively, the allowed cyclotron orbits are L x L y /πl 2 . Therefore, this treatment will give the degenerate states of 1/πl 2 per unit area. The degeneracy is different by a factor of 2 from (2.110). Here we consider a conduction band with a spherical constant energy surface and with a parabolic band, E0 (k) = 2 k 2 /2m ∗ , where m ∗ is the scalar effective mass. When we choose the Landau gauge and put A = (0, Bz x, 0), the effective-mass equation in a magnetic field is given by

pz2 1 px2 2 ( p y + eBz x) + + ψ = Eψ . 2m ∗ 2m ∗ 2m ∗

(2.111)

Since E0 (π), pz and p y commute with each other, we may choose the eigenfunction as (2.112) ψ = exp(ik y ) exp(ik z )F(x) . Inserting (2.112) into (2.111), the eigenfunction F(x) is found to satisfy the following relation 2 px 1 2 2 2 + B x + e B x (2.113) F(x) = E F(x) , 2ek y z z 2m ∗ 2m ∗ where E = E +

2 k 2y 2m ∗

+

2 k z2 . 2m ∗

(2.114)

Expression (2.113) may be rewritten in a very convenient form by using the following relation k y X =− (2.115) eBz giving rise to the following result

2 k 2y e2 Bz2 px2 2 F(x) = E F(x) + (x − X ) + 2m ∗ 2m ∗ 2m ∗ 2 k z2 F(x) . = E− 2m ∗

(2.116)

The transform from x to (X, ξ) may be evident from the above equation and we find that the electron motion in a magnetic field is well described by the relative coordinate ξ = x − X . The equation is known as the equation for the one-dimensional simple harmonic oscillator with the angular frequency

2.5 Electron Motion in a Magnetic Field and Landau Levels

ωc =

eBz m∗

95

(2.117)

and Eq. (2.116) is rewritten as !

" 2 k z2 1 ∗ 2 2 F(ξ) . + m ωc ξ F(ξ) = E − 2m ∗ 2 2m ∗ pξ2

(2.118)

The energy of the cyclotron motion is then given by E=

2 k z2 1 N+ , ωc + 2 2m ∗

(2.119)

where N is the quantum number of the Landau level. The eigenstates of (2.118) are given by |N , X, pz =

1 |x − X |2 exp − √ 2l 2 (2 N N ! πl)1/2 pz z x−X Xy × exp i HN − 2 , l l

(2.120)

where HN (x) are Hermite polynomials. The above results are summarized in Fig. 2.13. The left-hand figure shows the energy bands without a magnetic field. When a magnetic field B is applied in the z direction, the electron motion is quantized in the x, y plane and forms Landau levels as shown in the right-hand figure. Next, we consider the case of a perturbing potential U . The electron motion in a perturbing potential will be solved by inserting E0 + U into the Hamiltonian (2.102).

Fig. 2.13 Electronic states in a magnetic field. The left-hand figure represents the energy bands without magnetic field. Electron in the conduction band and hole in the valence band are quantized in the plane perpendicular to the magnetic field, resulting in the Landau levels as shown in the right-hand figure

96

2 Cyclotron Resonance and Energy Band Structures

Let us consider the equation of motion for the operator Q, which is written as i Q˙ = [H, Q] .

(2.121)

Therefore, we obtain i 1 i [H, π y ] ξ˙ = [H, ξ] = eBz η˙ =

i 1 i [H, η] = − [H, πx ] . eBz

Using the commutation relations given by (2.105b), we obtain the following equations ∂E0 ξ˙ = − ∂πx ∂E0 η˙ = + ∂π y

1 eBz 1 eBz

∂U ∂y ∂U . ∂x

(2.122a) (2.122b)

In a similar fashion we find the following relations. i i 1 ∂U X˙ = [H, X ] = [U, X ] = , eBz ∂ y 1 ∂U i , Y˙ = [U, Y ] = − eBz ∂x ∂E0 ∂U p˙ z = − , z˙ = . ∂z ∂ pz

(2.123a) (2.123b) (2.123c)

These relations are summarized as follows. ∂E0 ∂U − ∂π y ∂x ∂E0 ∂U . π˙ y = +eBz − ∂πx ∂y π˙ x = −eBz

(2.124a) (2.124b)

The velocity v = (vx , v y , vz ) is written as ∂E0 vx ≡ x˙ = ξ˙ + X˙ = ∂πx ∂E 0 v y ≡ y˙ = η˙ + Y˙ = ∂π y ∂E0 vz ≡ z˙ = . ∂ pz

(2.125a) (2.125b) (2.125c)

2.5 Electron Motion in a Magnetic Field and Landau Levels

97

Fig. 2.14 Electron motion in a magnetic field applied in the z direction (perpendicular to the text page) and in a uniform electric field applied parallel to the text page. In the absence of scattering, the electron moves in the direction perpendicular to the magnetic field and the electric field, as shown by green curve in the left half of the figure. In the presence of scattering the cyclotron center is scattered and a drift component appears along the direction of the electric field, which is shown by the purple curve in the right half of the figure

When a uniform electric field is applied, the perturbing potential is expressed as ∂U ∂U = −eE x , = 0, ∂x ∂y

(2.126)

and we obtain the following relation from (2.123a) and (2.123b) Ex Y˙ = , Bz

X˙ = 0 .

(2.127)

This means that the cyclotron center moves with a constant velocity E x /Bz in the direction perpendicular to the magnetic and electric fields, which is shown in the left half of Fig. 2.14. However, in the presence of scattering centers, the electron is scattered and changes the center of the cyclotron motion, giving rise to a drift motion along the electric field direction, as shown in the right half of Fig. 2.14.

2.5.2 Density of States and Inter Landau Level Transition Now we discuss the density of states of the electrons in the presence of a magnetic field. As explained above, an electron is quantized in the x, y plane and the energy eigenstate is independent of the cyclotron center, resulting in a degeneracy of pd = 1/2πl 2 . Since the wave vector in the z direction is given by k z = (2π/L z )n (n = 0, ±1, ±2, ±3, . . .), we obtain kz

=

Lz 2π

+k0 −k0

dk z =

Lz π

+k0

dk z ,

(2.128)

0

where k0 = (2π/L z )(N /2) and k z have N degrees of freedom. Equation (2.119) may be rewritten as

98

2 Cyclotron Resonance and Energy Band Structures

2 k z2 1 ωc = E =E− n+ , 2 2m ∗

and thus we obtain

kz

Lz = π

+k0 0

(2.129)

√ L z 2m ∗ dk z = √ dE . 2π E

(2.130)

Multiplying the degeneracy factor pd to the above equation, the number of electronic states for electrons in a magnetic field is given by N (E ) =

√ L x L y L z eBz 2m ∗ 1 √ . (2π)2 E

(2.131)

Therefore, the density of states g(E, Bz ) per unit volume in the energy range between E and E + dE is defined as √ 1 eBz 2m ∗ g(E, Bz ) = . (2.132) (2π)2 n E − (n + 1 )ω 2

c

The density of states in a magnetic filed is shown in Fig. 2.15 as a function of the electron energy. Next we will discuss the quantum mechanical treatment of cyclotron resonance. In the quantum mechanical picture the cyclotron resonance arises from the electron transition between Landau levels by absorbing photon energy (energy of a radiation field). As described in Sect. 4.2, the interaction Hamiltonian between the electron and the radiation field is given by (4.30), which is written as

Fig. 2.15 Density of states in a magnetic field (blue curve). The divergence of the density reflects the one-dimensionality of an electron in a magnetic field and the divergence is removed by taking account of the broadening due to electron scattering. The red curve represents the density of states for electrons in three dimensions when B = 0

2.5 Electron Motion in a Magnetic Field and Landau Levels

Her =

e A· p. m

99

(2.133)

A circularly polarized wave may be expressed as the following by defining the vector potential A = e · A: 1 e± = √ ex ± e y , 2

1 p± = √ p x ± p y , 2

(2.134)

where p± are the momentum operators for right and left polarized waves, respectively. When we define the z components of e and P as ez and pz , the transition rate calculated for the circularly polarized and linearly polarized waves gives the same result. In order to calculate the transition rate we use the eigenstates of the electron in a magnetic field given by (2.120), and then the transition rate is given by w=

&2 2π % N , X , pz |Her | N , X, pz

= 2π

e3 A2 Bz (N + 1)δk y ,k y δkz ,kz δ N ,N ±1 δ (ω − ωc ) . m∗

(2.135)

It is evident from the above equation that the selection rule for the cyclotron resonance is expressed as δk y = k y − k y = 0, δk z = k z − k z = 0, δ N = N − N = ±1.

2.5.3 Landau Levels of a Non-parabolic Band In Sect. 2.4 the non-parabolicity of the conduction and valence bands were discussed. The non-parabolicity plays an important role in the magnetotransport and cyclotron resonance. As described above, the Landau levels in a parabolic band are equally spaced in energy. In this section we will deal with Landau levels in a non-parabolic band along with the treatment of Luttinger and Kohn [7], and Bowers and Yafet [8]. The wave functions of the conduction band and valence bands are well described by using Bloch functions at k = 0: |nk = u n,0 eik·r ,

(2.136)

where u n,0 were derived in Sect. 2.3 by diagonalizing the spin–orbit interaction Hamiltonian and are given by Luttinger and Kohn [7] u 1,0 (r) = |S ↑ , u 2,0 (r) = |iS ↓ √ u 3,0 (r) = |(1/ 2)(X + iY ) ↑ , √ u 4,0 (r) = |(i/ 2)(X − iY ) ↓ , √ u 5,0 (r) = |(1/ 6)[(X − iY ) ↑ +2Z ↓ ] ,

(2.137a) (2.137b) (2.137c) (2.137d)

100

2 Cyclotron Resonance and Energy Band Structures

√ u 6,0 (r) = |(i/ 6)[(X + iY ) ↓ −2Z ↑ ] , √ u 7,0 (r) = |(i/ 3)[−(X − iY ) ↑ +Z ↓ ] , √ u 8,0 (r) = |(1/ 3)[(X + iY ) ↓ +Z ↑ ] ,

(2.137e) (2.137f) (2.137g)

where the time reversal symmetry is taken account. In a magnetic field applied in the z direction, the vector potential is described as A x = −By,

A y = 0,

Az = 0 ,

(2.138)

and therefore the Hamiltonian becomes H = H0 +

s s2 2 ypx + y , m 2m

(2.139)

where s is defined by using the cyclotron radius l as s=

1 eB = 2. l

(2.140)

It is easy to find the following relations for the matrix elements of the term which includes the contribution of the magnetic field:

nk|ypx |n k =

ei(k −k)·r u ∗n,0 y(k x − i∇x )n n ,0 d3 r

= −i

∂ ∂k y

= −i

∂ x [(k x + πnn )δ(k − k)] ∂k y

ei(k −k)·r u ∗n,0 (k x − i∇x )u n ,0 d3 r

x = (k x δnn + πnn )

1 ∂δ(k − k) , i ∂k y

(2.141)

In a similar fashion we find

nk|y 2 |n k =

'

y 2 ei(k −k)·r u ∗n,0 u n ,0 d3 r

∂ = −i ∂k y =−

(2

ei(k −k)·r u ∗n,0 u n ,0 d3 r

∂ 2 δ(k − k) δnn , ∂k 2 y

(2.142)

2.5 Electron Motion in a Magnetic Field and Landau Levels

101

and finally we obtain the relation 2 2 ∇ + V (r)|n k 2m 2 k 2 α δ(k − k ) . δnn + kα πnn = En + 2m m

nk|H0 |n k = nk| −

(2.143)

First, we will derive approximate solutions for the Landau levels of a non-parabolic conduction band. We define the zeroth-order wave function by a linear combination of Bloch terms f j (r)u j,0 (r) , (2.144) Ψ (r) = j

and then the matrix elements of the Hamiltonian H are derived as follows: 1 ¯ EG − λ 0 P k+ 0 2 1 ¯ 0 EG − λ 0 P k− 2 1 ¯ P k+ 0 −λ 0 2 1 ¯ 0 P k− 0 −λ 2 1 ¯ P k− − 23 Pk z 0 0 6 2 1 ¯ − i 3 Pk z P k+ 0 0 6 1 i 13 P k¯− Pk z 0 0 3 1 1 ¯ Pk z i 3 P k+ 0 0 3 1 ¯ 1 P k− i 23 Pk z −i 13 P k¯− Pk z f1 6 3 1 − 23 Pk z 16 P k¯+ Pk z −i 13 P k¯+ f 2 3 0 0 −λ 0 0 0

0 0 0 −λ 0 0

0 0 0 0

0 0 0 0 0

−Δ0 − λ 0 −Δ0 − λ

f3 f 4 = 0 , (2.145) f5 f6 f7 f8

102

2 Cyclotron Resonance and Energy Band Structures

where 2 k¯ 2 2m 2 2 k¯ = k¯ x + k¯ 2y + k z2 λ=E−

k¯± = k¯ x ± k¯ y

(2.146)

∂ k¯ x = k x − is ∂k y k¯ y = k y . Now we have to note the definition of the vector potential. In the previous subsection we defined the vector potential as (0, Bz x, 0), whereas in this subsection we adopt the gauge of (−Bz y, 0, 0). It is explained in the previous subsection that the energy of the cyclotron motion is independent of the cyclotron center X = −k y /eBz . Therefore, the gauge used in this subsection gives rise to the result that the cyclotron energy is independent of k x . This results allows us to put k x = 0 in the following calculations. Another assumption is made in this subsection that we neglect the contribution of spin–orbit interaction to the k dependence in (2.145). It is found that (2.145) may be easily solved when the term 2 k¯ 2 /2m is negligible. In this subsection we are interested in the Landau levels at k z = 0 and thus the above assumptions are valid in the analysis [8]. Under these assumptions Eq. (2.145) leads to the following two equations, where terms other than f 1 and f 2 are neglected: ∂2 1 (EG − λ)λ + 23 P 2 k z2 + k 2y − s 2 ∂k 2 + 2s y 2 2 ∂ λ k z2 + k 2y − s 2 ∂k − s f1 = 0 + 3(ΔP0 +λ) 2 y ∂2 1 (EG − λ)λ + 23 P 2 k z2 + k 2y − s 2 ∂k 2 − 2s y 2 ∂2 λ k z2 + k 2y − s 2 ∂k f2 = 0 . + 3(ΔP0 +λ) 2 + s y

(2.147)

(2.148)

When we investigate the above equations, we find that the equations √ represent simple harmonic oscillator equations with dimensionless variable k y / s. Therefore we obtain the following solutions: D(λn± ) ≡ λn± (λn± − EG )(λn± + Δ0 ) # $ 1 2 = −P 2 k z2 + s(2n + 1) λn± + Δ0 ± P 2 Δ0 s = 0 , (2.149) 3 3 where λn,± stands for λkz , n (spin quantum number), ±, and s = eB/. It is evident from (2.149) that the latter coincides with the solution for a parabolic band in the absence of a magnetic field, i.e. for B = 0 (and thus s = 0). Using the relation

2.5 Electron Motion in a Magnetic Field and Landau Levels

103

λ = E − 2 k 2 /2m in (2.149) and neglecting the small spin-splitting term, the Landau levels at k x = 0 are approximated as below [9]. [They are easily derived from (2.86).] 1 m ∗ 2 3EG + 4Δ0 + 2Δ20 /EG ωc − 1 − 0 En = n + 2 m (EG + Δ0 )(3EG + 2Δ0 ) 2 1 × n+ (ωc )2 , 2

(2.150)

where m ∗0 is the band-edge effective mass of the conduction band and is given later (2.152) (or see (2.84)) and ωc = eB/m ∗0 as defined before.

2.5.4 Effective g Factor Landau levels of the conduction band electron is expressed as 2 k z2 1 1 ∗ + E±,n,kz (B) = ωc n + ∗ ± μB |g0 |B , 2 2m 0 2

(2.151)

where m ∗ is the band edge effective mass, ωc = eB/m ∗0 , the quantum numbers ± refer to the spin, and μB = e/2m is the Bohr magneton. The constant g0∗ is the Landé g factor, referred to as the effective g–factor. The band edge effective mass m ∗0 and the effective g factor g0∗ are deduced by Roth et al. [10] and cited many papers [11–14]. Here we use the definition of Herman and Weisbuch [14]: 1 E P0 1 + ∗ = m0 m 3m

2 1 + EG EG + Δ0

,

(2.152)

g0∗ 1 1 Γ6c | px |u u| p y |Γ6c − Γ6c | p y |u u| px |Γ6c = 1+ (2.153) 2 m i u Ec − Eu 1 1 E P0 − = 1+ 3 EG + Δ0 EG 1 E P1 1 + C , + − (2.154) 3 E(Γ8c ) − EG E(Γ7c ) − EG where the factor 2 of the denominator of g0∗ /2 is the free electron g factor (g0 = 2) and the energies are define by the magnitude (positive value). The relation of (2.153) and thus (2.154) arises from the spin–orbit interaction. For reference the energy band structure near k = 0 with respective energies are shown in Fig. 2.16. Ec is the energy of the conduction band |Γ6c (or |Γ2 in the single group representation). The energies Eu for the valence bands are E(Γ8v ) = −EG and its spin–split off band E(Γ7v ) = −EG − Δ0 . For the higher conduction band Eu are E(Γ7c ) − EG and its spin–split off band E(Γ8c ) − EG = E(Γ7c ) + Δ15 − EG , and thus

104

2 Cyclotron Resonance and Energy Band Structures

Fig. 2.16 Schematic energy band structure near k = 0 in a direct band gap semiconductor, group theoretical symbols for a diamond type (single group representation) and zinc blende type (double group representation)

the energy denominators are, respectively, Ec − E(Γ7c ) − EG and Ec − E(Γ8c ) − EG = Ec − E(Γ7c ) − Δ15 − EG . Putting Ec = 0, we obtain the result given by (2.154). The higher conduction band E(Γ7c ) and E(Γ8c ) = E(Γ7c ) + Δ15 are measured from the valence band top. These higher conduction band energies are obtained as E1 and E1 + Δ15 , where E1 is the optical transition energy between the valence band top Γ8v (Γ25 band) and Γ7c (Γ15 ) band (called as E 1 –edge). Derivation of (2.154) from (2.153) is straight forward by evaluating the matrix elements using the eigenstates of Γ7v and Γ8v valence bands (Γ25 bands in single group representation) given by (2.63a)–(2.63f) and similar eigenstates for Γ7c and Γ8c conduction bands (Γ15 bands in single group representation). The diagonalization of spin–orbit Hamiltonian gives the corresponding eigenvalues and eigen sates, where different forms of the eigen functions are reported by Luttinger and Kohn [7] (see (2.137b)–(2.137g)), where the time reversal symmetry is taken account. Roth et al. [10] defined the eigenstates as given below, which are the same as (2.63a)–(2.63f) of this textbook. Here we list the eigenstates derived by Roth et al. [10]: for fourfold valence bands are 3 3 1 = √ |(X + iY ) ↑ , (2.155a) u v1 = , 2 2 2 3 1 1 u v2 = , = − √ [|(X + iY ) ↓ + 2 |Z ↑ ] , (2.155b) 2 2 6 3 1 1 u v3 = , − = − √ [|(X − iY ) ↑ + 2 |Z ↓ ] , (2.155c) 2 2 6 3 3 1 (2.155d) u v4 = , − = √ |(X − iY ) ↓ , 2 2 2

2.5 Electron Motion in a Magnetic Field and Landau Levels

105

and for twofold spin–split off bands are u v5 u v6

1 1 1 = √ [|(X + iY ) ↓ − |Z ↑ ] , = , 2 2 3 1 1 1 = , − = √ [|(X − iY ) ↑ − |Z ↓ ] . 2 2 3

(2.155e) (2.155f)

The term C represents the contributions from far–higher lying bands. The energies E(Γ7c ) and E(Γ8c ) are measured from the the valence band top and thus all the energy values are taken to be positive. Here we adopted the notations defined in Sect. 2.6, and E P0 and E P1 are defined as 2 | Γ2 | px |Γ25 (X )|2 , m 2 = | Γ2 | px |Γ15 (x)|2 . m

E P0 =

(2.156)

E P1

(2.157)

The above relations were first derived by Roth et al. [10]. Also similar treatment leads to the band edge effective mass for the 14 band band model and the results are shown in Sect. 2.6. Here we estimate the effective g– factor for GaAs at low temperature, where we choose EG = 1.519 [eV], Δ0 = 0.341 [eV], E P0 = 28.8 [eV], E1 = 4.488 [eV], Δ15 = 0.171 [eV], E P1 = E P0 /4 = 7.2 [eV], and C = −0.02. These parameters give g0∗ = −0.445 with good agreement of experiment g0∗ = −0.44. The parameters assumption E P1 = E P0 /4 and C are not well established and thus the above values are open for discussion. Litvinenko et al. introduce another mixing term and their parameters give g0∗ = −0.44. In this textbook we presented the magnitude of g–factor without discussion of the sign and the reported values for various III–V materials are negative values except some compounds. The effective g factor of (2.154) leads to (2.159) of 8 band model by neglecting the higher band contributions. When we take account of Γ6c conduction band, and Γ7v and Γ8v valence bands only we obtain 1 E P0 2Δ0 + 3EG 1 + , = m ∗0 m 3m EG (Δ0 + EG ) g0∗ 1 E P0 m Δ0 1 =1+ =1+ 1− ∗ − . 2 3 EG + Δ 0 EG m 0 2Δ0 + 3EG

(2.158) (2.159)

The effective g–factor of InSb is estimated by (2.159) as expected from Kane’s two band model. We choose the parameters of InSb at low temperature as, EG = 0.2353 [eV], EP0 = 23.1 [eV], and Δ0 = 0.803 [eV]. These values give g0∗ = −48.6, which shows a reasonable agreement with the measurements g0∗ −50 in InSb [11, 12]. The effective g–factor depends on the electron energy E and given by Litvinenko et al. [12]

106

2 Cyclotron Resonance and Energy Band Structures

E P0 g0∗ =1+ 2 3

1 1 − EG + Δ0 + E EG + E

,

(2.160)

and shows a good agreement with the experiments. We have to note here that the above formulations are based on the k · p perturbation theory. Narrow gap semiconductors such as InSb is well expressed by the Kane’s two band model (8 band model with spin–orbit interaction), and that more general form with higher bands contributions is useful for more accurate modeling for zinc blende semiconductors such as GaAs, where we have to use 14 band model. The results shown above are obtained by using the energy eigenstate notations of the double group (see also the treatment in Sect. 2.6) and with magnetic field applied in the z direction,

2.5.5 Landau Levels of the Valence Bands It may be expected that the calculations of Landau levels for valence bands are complicated because of the degeneracy of the bands and the spin–orbit interaction. In this subsection we deal with the Landau levels in the valence bands along with the treatment of Luttinger [2] and the method extended by Pidgeon and Brown [15]. First we investigate the valence bands using (2.44) and (2.45). The non-diagonal term N k x k y is given by xy

yx

D X Y = D X Y kx k y + D X Y k y kx .

(2.161)

We define the antisymmetric term by xy

yx

K = DXY − DXY ,

(2.162)

and then D X Y is rewritten as D X Y = N {k x k y } +

1 K (k x , k y ) , 2

(2.163)

where 1 (k x k y + k y k x ), 2 (k x , k y ) = k x k y − k y k x . {k x k y } =

(2.164a) (2.164b)

From the commutation relation of (2.105b) (k x , k y ) = −ieBz

(2.165)

2.5 Electron Motion in a Magnetic Field and Landau Levels

107

is derived and therefore we obtain D X Y = N {k x k y } +

K eBz . 2i

(2.166)

DY X = N {k x k y } −

K eBz . 2i

(2.167)

Similarly we find

The other terms are also expressed in a similar fashion. As a result (2.45) is divided into two terms (2.168) D = D (S) + D (A) , where D (S) is obtained from (2.45) by putting kα kβ → {kα kβ }, and D (A) is given by the matrix 0 −iBz iB y eK (A) iB 0 −iBx z D = (2.169) 2 −iB y iBx 0 We define the operators Jx , Jy and Jz , which have the same characteristics as the momentum operators expressed by a 4 × 4 matrix, i.e. (Jx , Jy ) = iJz , (Jy , Jz ) = iJx , (Jz , Jx ) = iJy Jx2 + Jy2 + Jz2 = 23 23 + 1 = 15 . 4

(2.170a) (2.170b)

Using these results we obtain the Luttinger Hamiltonian given by 1 D= m

5γ2 k 2 γ1 + − γ2 (k x2 Jx2 + k 2y Jy2 + k z2 + Jz2 ) 2 2 −2γ3 ({k x k y }{Jx Jy } + {k y k z }{Jy Jz } + {k z k x }{Jz Jx }) +eκ J · B + eq(Jx3 Bx + Jy3 B y + Jz3 Bz ) ,

(2.171)

where units are chosen that = 1, 1 1 γ1 = − (A + 2B) , 2m 3 1 1 γ2 = − (A − B) , 2m 6

1 (3κ + 1) = −K , m 1 1 γ3 = − C . 2m 6

(2.172a) (2.172b)

The parameter q is introduced for the correction due to the spin–orbit splitting, which is neglected because of the small contribution. The parameters defined above are called Luttinger parameters. Following the treatment of Luttinger and Kohn [7], the k · p Hamiltonian is expressed as (in atomic units)

108

2 Cyclotron Resonance and Energy Band Structures

) j

1 l Dlm j j kl km + π j j kl + 2 s(σ3 ) j j

+ 4c12 [(σ × ∇V ) · p] j j + E j δ j j f j (r) = E f j (r) , where Dlm j j ≡

(2.173)

πlji πimj 1 . δ j j δlm + 2 E0 − Ei i

(2.174)

The summations with respect to j and j in the above equation are carried out for 2 conduction bands and 6 valence bands, i is for all bands, and l, m are for 1, 2, 3 or for x, y, z. Ei and E j are the average energies for the states i and j, respectively. Equation (2.173) is evaluated by using (2.137g) and (2.144), giving rise to a 8 × 8 ¯ plane, the Luttinger matrix matrix. When the magnetic field is applied in the (110) D becomes (2.175) D = D0 + D1 , where D0 may be solved exactly and D1 may be solved by a perturbation method [15]. The detail of the analysis is not described here. In the following we put k3 = 0. Then D0 is divided into two 4 × 4 matrices: D0 =

Da 0 . 0 Db

(2.176)

In addition we neglect the perturbation term of the conduction band and thus all the terms except the first term of (2.174). This assumption is also adopted by Pidgeon and Brown, where they put F = 0. Finally we obtain √ EG − Ea + s(n + 1) i s Pa † √ −i s Pa −s[(γ1 + γ )(n + 21 ) + 23 κ] − Ea √ −i 13 s Pa † −s 3γ a †2 √ 2 s Pa † is 6γ a †2 3 2 i 31 s Pa s Pa 3 √ 2 √ 2 −s 3γ a −is 6γ a √ 1 1 −s[(γ1 − γ )(n + 2 ) − 2 κ] − Ea is 2[γ (n + 21 ) − 21 κ] √ −is 2[γ (n + 21 ) − 21 κ] −s[γ1 (n + 21 ) − κ] − Δ0 − Ea

f1 f3 f5 f7

=0

2.5 Electron Motion in a Magnetic Field and Landau Levels

EG − Eb + sn i 13 s Pa † −i 13 s Pa † −s[(γ1 − γ )(n + 21 ) + 21 κ] − Eb √ √ −i s Pa † −s 3γ a †2 √ 2 s Pa −is 2[γ (n + 21 ) + 21 κ] 3 √ 2 s Pa † i s Pa 3 √ 2 √ −s 3γ a is 2[γ (n + 21 ) + 21 κ] √ −s[(γ1 + γ )(n + 21 ) − 23 κ] − Eb is 6γ a †2 √ −is 6[γ a 2 −s[γ1 (n + 21 ) + κ] − Δ0 − Eb

109

f2 f6

= 0.

f4 f8

Here we have used the creation operator a † and the annihilation operator a defined as 1 a † = √ (k1 + ik2 ) , 2s 1 a = √ (k1 − ik2 ) , 2s n = a†a

(2.177a) (2.177b) (2.177c)

P is the matrix element of the momentum operator defined previously, P = −i S| pz |Z ), and γ and γ are given by 2 1 2 γ = γ3 + (γ2 − γ3 ) (3 cos θ − 1) , 2 2 1 1 1 1 γ = γ3 + γ2 + (γ2 − γ3 ) (3 cos2 θ − 1) , 3 3 6 2

(2.178a) (2.178b)

where θ is the angle between the z axis and the magnetic field. The valence band parameters used here, γ1 , γ2 , γ3 and κ are different from the Luttinger parameters γ1L , γ2L , γ3L and κ L , and they are given by 2P 2 , 3EG P2 γ2 = γ2L − , 3EG P2 γ3 = γ3L − , 3EG P2 κ = κL − . 3EG γ1 = γ1L −

(2.179a) (2.179b) (2.179c) (2.179d)

110

2 Cyclotron Resonance and Energy Band Structures

Here we will show the derivation of the relations (2.177a)–(2.177c). Using the generalized momentum defined by πx = px + e A x = px − yeB

(2.180a)

πy = py + e A y = py

(2.180b)

we find k1 = −i

e Ax ∂ + , ∂x

k2 = −i

e Ay ∂ + , ∂y

(2.181a) (2.181b)

and thus we obtain the relation 2 (k1 , k2 ) = ( px + e A x , p y + e A y ) = ( px , p y ) + ( px , e A y ) + (e A x , p y ) + e2 (A x A y − A y A x ) = 0 + ( px , 0) + (−eBy, p y ) + 0 = −eB(y, p y ) = −ieB, (k1 , k2 ) =

eB s ≡ . i i

(2.182)

When we define new variables by k1 =

√ √ s p, k2 = sq ,

(2.183)

p and q are canonical variables which satisfy ( p, q) =

1 . i

(2.184)

We can now define new operators for the creation and annihilation operators a † and a by 1 1 a † = √ ( p + iq) = √ (k1 + ik2 ) , 2s 2

(2.185a)

1 1 a = √ ( p − iq) = √ (k1 − ik2 ) . 2s 2

(2.185b)

The commutation relation for the new operator is (a, a † ) = 1

(2.186)

2.5 Electron Motion in a Magnetic Field and Landau Levels

111

and the relations (2.177a)–(2.177c) are derived as follows: 1 2 1 1 ( p + q 2 )u n = a † a + un = n + un , 2 2 2

(2.187a)

a † au n = nu n , √ au n = nu n−1 , √ a † u n = n + 1u n+1 ,

(2.187d)

n =a a.

(2.187e)

(2.187b) (2.187c)

†

It is evident from the two eigenvalue equations in matrix form below (2.176) that the solutions of these equations are given by the solutions of a simple harmonic oscillator equation: a 1 Φn a3 Φn−1 , fa = a5 Φn+1 a7 Φn+1

a 2 Φn a6 Φn−1 fb = . a4 Φn+1 a8 Φn−1

(2.188)

Using these relations the eigenvalues for a and b are given by √ EG − Ea + s(n + 1) i sn P √ −s[(γ1 + γ )(n − 21 ) + 23 κ] − Ea −i sn P √ −i 31 s(n + 1)P −s 3n(n + 1)γ √ 3 s(n + 1)P is 6n(n + 1)γ 2 1 2 s(n + 1)P s(n + 1)P 3 3 √ √ −s 3n(n + 1)γ −is 6n(n + 1)γ = 0 , (2.189) √ 3 1 −s[(γ1 − + 2 ) − 2 κ] − Ea is 2[γ (n + 23 ) − 21 κ] √γ )(n −is 2[γ (n + 23 ) − 21 κ] −s[γ1 (n + 23 ) − κ] − Δ0 − Ea and EG − Eb + sn i 13 sn P −i 31 sn P −s[(γ1 − γ )(n − 21 ) + 21 κ] − Eb √ √ −i s(n + 1)P −s 3n(n + 1)γ √ 3 sn P is 2[γ (n − 21 ) + 21 κ 2 √ 2 i s(n + 1)P sn P 3 √ √ 1 1 −s 3n(n + 1)γ −is 2)[γ = 0 . (2.190) √ (n − 2 ) + 2 κ] 3 3 −s[(γ1 + γ√)(n + 2 ) − 2 κ] − Eb is 6n(n + 1)γ −is 6n(n + 1)γ −s[γ1 (n − 21 ) + κ] − Δ0 − Eb

112

2 Cyclotron Resonance and Energy Band Structures

These equations are valid for n ≥ 1. In the case of n = −1 we put a1 = a3 = a2 = a6 = a8 = 0, and in the case of n = 0 we put a3 = a6 = a8 = 0. The Landau levels of the electron in the conduction band and holes in the valence bands are obtained by solving the above equations. It may also be possible to obtain the selection rule for the transition between the Landau levels from the eigenstates derived here.

2.5.6 Magneto–Optical Absorption As described above the Landau levels of the valence bands are complicated and the detailed analysis requires accurate values of Luttinger parameters. One of the methods is the analysis of the cyclotron resonance of holes as discussed in this chapter. Another method is magneto–absorption measurements [10, 15–20]. Here a simple case is described for the purpose of introduction to the magneto–absorption effects. In Fig. 2.17 a schematic diagram of a simplified model of two parabolic bands are shown and the bars are the Landau levels. The Landau levels of the conduction and valence bands are given by 2 k z2 1 + , Ec = Ec (0) + ωc n + 2 2m c 2 k z2 1 − , Ev = Ev (0) − ωv n + 2 2m v

(2.191a) (2.191b)

where ωc = eB/m c and ωv = eB/m v are the cyclotron frequencies of the conduction and valence bands, respectively. In Chap. 4 optical properties of semiconductors will be discussed and the absorption coefficient is proportional to the joint density of states. In the absence of magnetic field the absorption coefficient of 3 dimensional case is given by (see (4.56) and (4.58)) 3/2 2μ 4π ω − EG , 3 (2π) 2 πe2 |e · pcv |2 K = 0 m 2 ω 2 1/μ = 1/m c + 1/m v , EG = Ec − Ev . α0 = K

(2.192a) (2.192b) (2.192c)

In the presence of a magnetic field the density of states is one dimensional and given by (2.132). Therefore the absorption coefficient is written as

2.5 Electron Motion in a Magnetic Field and Landau Levels

113

Fig. 2.17 Schematic diagram of the Landau levels at k = 0 for a simple two bands model of conduction and valence bands. The allowed transitions are shown by the arrows between the Landau levels with quantum numbers of the conduction and valence bands

√ eB 2μ [ω − ωn ]−1/2 , (2π)2 n 1 (ωc + ωv ) ωn = EG + n + 2 αB = K

(2.193a) (2.193b)

In Fig. 2.18 absorption coefficients (in a.u. units) for B = 0 and B = 0 are plotted, where the broadening effect is taken into account by putting ω → ω + iΓ , with Γ = 0.05(ωc + ωv ). In the figure we see the maxima of magneto–absorption appear periodically with the spacing of photon energy ωc + ωv . This is not the case observed by experiments as shown below. Since the conduction and valence bands are nonparabolic, and the valence bands consist of the degenerate heavy and light hole bands at the Γ point (k = 0) and spin–orbit split–off band and thus the Landau levels are complicated as analyzed above. Here a comparison between the experimental and theoretical results in InSb reported by Pidgeon and Brown [15] is shown, as one of the best examples. The experiments are carried out by choosing two different configurations of the electric field vector E of the incident radiation (light polarization) and the applied magnetic field B, E ⊥ B [100] and E B [100], and optical absorption data (magnetoabsorption data) were obtained at a fixed photon energy by sweeping the magnetic field B. In Fig. 2.19 are shown plots of photon energy of the transmission minima as a function of magnetic-field field strength for the principal transmission in the E ⊥ B, with B parallel to the [100] crystal direction, along with the theoretical curves. In Fig. 2.20 are shown similar plots for the configuration E B [100].

114

2 Cyclotron Resonance and Energy Band Structures

Fig. 2.18 Absorption coefficient as a function of incident photon energy (normalized by (ωc + ωv )) for the bands shown Fig. 2.17, where broadening effect is taken into account for both B = 0 (dashed line) and B = 0. The density of states shown in Fig. 2.15 is obtained without broadening effect

Fig. 2.19 Plot of the photon energy of magneto-absorption maxima (transmission minima) as a function of magnetic field for E ⊥ B [100] in n-InSb at T = 4.2 K. The solid lines are calculated from Eqs. (2.189) and (2.190) in the text for a and b series and the notation of the transitions is defined in the text and the transitions are as follows: (after Pidgeon and Brown [15]) 1. a − (2)a c (0) 6. b+ (2)bc (2) 11. b+ (6)bc (4) 2. b+ (0)bc (0) 7. a + (4)a c (2) 12. b+ (5)bc (5) 3. a + (1)a c (1) 8. b+ (3)bc (3) 13. a + (7)a c (5) 4. b+ (1)bc (1) 9. a + (5)a c (3) 5. a + (3)a c (1) 10. b+ (4)bc (4)

2.5 Electron Motion in a Magnetic Field and Landau Levels

115

Fig. 2.20 Plot of the photon energy of magneto-absorption maxima (transmission minima) as a function of magnetic field for E B [100] in n-InSb at T = 4.2 K. The solid lines are calculated from Eqs. (2.189) and (2.190) in the text for a and b series and the notation of the transitions is defined in the text and the transitions are as follows: (after Pidgeon and Brown [15]) 1. b− (2)a c (0) 6. a − (2)bc (2) 11. b− (8)a c (6) 2. a + (0)bc (0) 7. b− (5)a c (3) 12. b− (9)a c (7) 3. b− (3)a c (1) 8. a − (3)bc (3) 13. b− (10)a c (8) 4. a + (1)bc (1) 9. b− (6)a c (4) 14. b− (11)a c (9) 5. b− (4)a c (2) 10. b− (7)a c (5)

We see a good agreement between the experimental and assigned theoretical curves in Figs. 2.19 and 2.20. Here the notation for the transitions are defined as follows. In the notations a ± (n)a c (n ) and b± (n)bc (n ), a and b mean the a, and b series, and +, −, and c refer to the light–hole, heavy–hole, and conduction electron, respectively. The orbital quantum number is given in brackets and the selection rules result in allowed transitions for Δn = 0, −2. For example, the notation a − (2)a c (0) means the transition between the light–hole level of a series with quantum number n = 2 and the conduction electron level of a series with quantum number n = 0. The non–linearity of the calculated and experimental data in Figs. 2.19 and 2.20 arises from the nonparabolic effects of the conduction and valence bands. Here we find the observed transitions are mostly from the light–hole levels. On the other hand for the configuration E B [100] the following transitions are observed. For the configuration E B [100], strongest transitions are from the heavy–hole levels. From the fitting procedure Pidgeon and Brown [15] obtained the following band–edge parameters for InSb:

116

2 Cyclotron Resonance and Energy Band Structures

P 2 = 0.403 au ,

(2.194a)

EG = 0.2355 eV , Δ = 0.9 eV , γ1L = 32.5 ,

(2.194b) (2.194c) (2.194d)

γ2L = 14.3 , γ3L = 15.4 ,

(2.194e) (2.194f)

κ L = 13.4 ,

(2.194g)

where they found that F is very small and put it equal to zero.

2.6 Luttinger Hamiltonian Here we derive so called “Luttinger Hamiltonian”, which will be used for the analysis of the valence band states in a quantum structure and for the analysis of semiconductor quantum well lasers in Chap. 10. First, we calculate several matrix elements of (2.64) defined by Dresselhaus, Kip, and Kittel [1] and relate them to the Luttinger parameters. From (2.64) we obtain the following matrix elements 1 L+M 2 H11 + H22 2 2 = (k x + k y ) + Mk z → P(k) , 2 2 2 H13 − iH23 N − = − √ (k x − ik y )k z (→ L(k)) , √ 3 3 (L − M)(k x2 − k 2y ) − 2iN k x k y H11 − H22 − 2iH12 − = √ √ 2 3 12 (→ M(k)) , $ 1# H33 + H11 + H22 = (L + M)(k x2 + k 2y )P + 2Mk z2 6 6 1 2 2 2 + M(k x + k 2y ) + Lk z2 → P(k) + Q(k) , 3 6 3

(2.195a) (2.195b)

(2.195c)

(2.195d)

and other elements are also easily calculated. The notations in the parentheses are the definition of Luttinger and Kohn [7], and L, M, and N of Dresselhaus et al. [1] are related to A, B, and C of Luttinger [2, 7] by A = 2 /2m + L, B = 2 /2m + M, and C = N . Using the wave functions defined by (2.63a)–(2.63f) and following the treatment of Luttinger and Kohn [7], (2.64) is rewritten as5 5

The matrix elements derived by using the expressions of Dresselhaus et al. are equivalent to the expressions of Luttinger and Kohn except the diagonal elements as discussed before, and the corresponding secular equation of Luttinger and Kohn Hamiltonian gives eigenvalue E (k), while the secular equation of Dresselhaus, Kip and Kittel gives λ = E (k) − 2 k 2 /2m.

2.6 Luttinger Hamiltonian

117

√ √ | 23 , 23 P/2 L M 0 iL/ 2 √ −i 2M √ | 23 , 21 L∗ P/6 + 2Q/3 0 M −i(P − 2Q)/3 2 i 3/2L √ √ | 23 , − 21 M∗ 0 P/6 + 2Q/3 −L −i √3/2L ∗ −i(P − 2Q)/3 2 √ | 23 , − 23 0 √ M∗ √ −L ∗ P/2 −i 2M ∗ −iL ∗ / 2 √ √ ∗ | 21 , 21 −iL i 3/2L √ i 2M 0 √ / 2 i(P −√2Q)/3∗ 2 √ (P + Q)/3 − Δ0 | 21 , − 21 i 2M ∗ −i 3/2L i(P − 2Q)/3 2 iL/ 2 0 (P + Q)/3 − Δ0

(2.196)

where P(k) =

$ 2 # (A + B)(k x2 + k 2y ) + 2Bk z2 , 2m

C 2 (k x − ik y )k z , L(k) = −i √ 3 2m Q(k) =

$ 2 # B(k x2 + k 2y ) + Ak z2 , 2m

$ 1 2 # (A − B)(k x2 − k 2y ) − 2iCk x k y . M(k) = √ 12 2m

(2.197a) (2.197b) (2.197c) (2.197d)

Here A, B, and C are dimensionless constants obtained by dividing the original values by 2 /2m and Δ0 is spin–orbit splitting at k = 0. Equation (2.196) is called Luttinger Hamiltonian and Luttinger parameters γ1 , γ2 and γ3 given by (2.172a), (2.172b), and (2.172b ) are rewritten as follows by recovering units of = 1 such as (1/2m)γ1 → (2 /2m)γ1 , and so on, 1 γ1 = − (A + 2B) , 3 1 γ2 = − (A − B) , 6 1 γ3 = − C , 6

(2.198b)

− A = γ1 + 4γ2 ,

(2.199a)

−B = γ1 − 2γ2 , −C = 6γ3 .

(2.199b) (2.199c)

(2.198a)

(2.198c)

or

It should be noted here that the above parameters are for the electronic states and that the parameters for the holes of the valence bands are obtained by replacing −A, −B and −C by A, B and C, respectively.

118

2 Cyclotron Resonance and Energy Band Structures

When the matrix elements are redefined as P =

2 2 1 (P + Q) = −γ1 (k + k 2y + k z2 ) , 3 2m x

(2.200a)

2 2 1 (P − 2Q) = −γ2 (k + k 2y − 2k z2 ) , 6 2m x √ 2 L = 2i 3γ3 (k x − ik y )k z , 2m √ 2 # $ γ2 (k x2 − k 2y ) − 2iγ3 k x k y , M=− 3 2m

Q =

(2.200b) (2.200c) (2.200d)

and then (2.196) is rewritten as √ iL/ 2 √ L∗ P − Q 0 M −i 2Q √ M∗ 0 P − Q −L −i 3/2L ∗ √ 0 M∗ −L ∗ P + Q −i 2M ∗ √ √ √ √ −iL ∗ / 2 i 2Q i 3/2L i 2M P − Δ0 √ ∗ √ √ √ i 2M −i 3/2L ∗ i 2Q iL/ 2 0 P + Q

L

M

0

√ −i 2M √ i 3/2L √ −i 2Q √ . −iL ∗ / 2

(2.201)

0

P − Δ0

In order to deal with optical properties of quantum structures such as quantum wells, quantum dots and so on, we have to solve the electronic states of the conduction and the valence bands together. In such cases we have to solve 8 × 8 k · p Hamiltonian adding two electronic states of the conduction band |Γ2 ↑ and |Γ2 ↓ to the 6 × 6 k · p Hamiltonian (2.196) or (2.201). The eight–band theory has been reported by Bahder [27], Zhang [28], and Pryor [24]. We calculate the valence band dispersions by 6 × 6 k · p Hamiltonian and by the local pseudopotential method with spin–orbit interaction, which are shown in Fig. 2.21. The results show a reasonable agreement with each other in the region k 0, but a considerable discrepancy near the zone edges. The results restrict us to use 6 × 6 Luttinger Hamiltonian (and the extended 8 × 8 k · p Hamiltonian) for analyzing the periodic quantum dots of superlattices, in which Brillouin zone folding effect plays an important role as discussed in Chap. 9. Many papers have been published to deal with the optical properties of quantum structures. Among these methods very popular one is to solve 8 × 8 k · p Hamiltonian adding two electron states of the conduction band |Γ2 ↑ and |Γ2 ↓ to the 6 × 6 k · p Hamiltonian (2.196) or (2.201), which is given in the following

2.6 Luttinger Hamiltonian T 0 V √0 ∗ 3V √ − 2U −U √ 2V

0 V∗ √ √0 T − 2U − 3V ∗ √ −√2V P + Q L − 3V L∗ P − Q 0 M∗ 0 ∗ −V 0 √ M∗ √ ∗ √ ∗ 2V −iL √ / ∗ 2 i√ 2Q ∗ U i 2M −i 3/2L

119 √

3V 0 M 0 P − Q −L ∗ √ i √3/2L i 2Q

√ − (2)U −U √ −V 2V √ 0 iL/ √ 2 M −i √ 2Q √ −L −i √ 3L ∗ / 2 P√+ Q −i 2M ∗ i 2M P − Δ0 √ iL/ 2 0

√

2V ∗ U √ −i 2M √ i √ 3/2L −i 2Q √ −iL ∗ / 2 0 P − Δ0

(2.202)

where T = Ec + (k x2 + k 2y + k z2 ) , 1 1 U = √ P0 k z = √ E P0 k z , 3 3 1 1 V = √ P0 (k x − ik y ) = √ E P0 (k x − ik y ) , 6 6 P0 = Γ2 | px |Γ25 (X ) ,

(2.203a) (2.203b) (2.203c) (2.203d)

and P0 is the momentum matrix element between the conduction and valence bands and equivalent to P0 defined by (2.83b). The energy reference is the valence band top and thus we put Ev = 0. Since we use SI units and k · p Hamiltonian is defined by (/m)k · p, the term with P0 should be evaluated as 2 1/2 2 k P0 k z → P0 k z = (m/2)E P0 k z = E P0 m m 2m z → E P0 k z (in atomic units)

(2.204)

where we used the relation E P0 = (2/m)P02 given by (2.203d). Here we show in Fig. 2.21 the calculated curves of the valence band structures of GaAs by the 6 × 6 k · p Luttinger Hamiltonian and the full band calculations obtained by 30 × 30 k · p Hamiltonian with the spin–orbit interaction. We find that the red solid curves obtained by the 6 × 6 Luttinger Hamiltonian gives a reasonable agreement with the blue dotted curves calculated by the 30 × 30 k · p Hamiltonian near k 0, but a considerable deviation in the full Brillouin zone. Used parameters for the k · p full band calculations are in Table 1.13 and for the Luttinger parameters are in Table 2.1. It should be noted here that 6 × 6 and 8 × 8 Luttinger Hamiltonians are valid only for small values of wave vectors near the band edge (k 0) and thus the results of 6 × 6 k · p Luttinger Hamiltonian are plotted. Figure 2.21 gives a good guide to understand the k · p perturbation theory and its application to the energy band structures.

120

2 Cyclotron Resonance and Energy Band Structures

Fig. 2.21 Comparison of the valence band dispersions between the 30 k · p (dotted blue curves) and 6 × 6 k · p Luttinger Hamiltonian (solid red curves), where dispersions are shown in the first Brillouin zone in Γ to X and Γ to L points. Solid green curve is parabolic dispersion of the conduction band with m∗ = 0.067m

2.7 Luttinger Parameters It should be noted here that the valence band parameters of Luttinger are subject to reinterpretation because they are determined experimentally and thus all the contributions from the bands are included. If we use the parameters to solve k · p 8 × 8 Luttinger-Hamiltonian, the contribution from the |Γ2 conduction band is included. Therefore we have to exclude the contribution form the conduction band. First, we discuss how to determine the valence band parameters of Luttinger using the analysis made by Kane [3], Dresselhaus, Kip and Kittel [1], Groves et al. [21] and Lawaetz [22], F =−

2 | Γ25 (X )| px |Γ2 , j|2 , m j E(Γ2 , j)

(2.205a)

G=−

2 | Γ25 (X )| px |Γ12 , j|2 , m j E(Γ12 , j)

(2.205b)

H1 = −

2 | Γ25 (X )| p y |Γ15 , j|2 , m j E(Γ15 , j)

(2.205c)

H2 = −

2 | Γ25 (X )| p y |Γ25 , j|2 , m j E(Γ25 , j)

(2.205d)

2.7 Luttinger Parameters

121

where the valence band edge Γ25 (Γ8 ) at k = 0 is taken to be energy zero. 6 The contributions to the parameters L, M, and N of (2.47a)–(2.47c) defined defined by Dresselhaus, Kip and Kittel [1] from the above four conduction bands are calculated as follows. 1. Contributions to L (or Lk x2 ) are from Γ2 and Γ12 . The contribution to A from |Γ2 is evaluated by taking account of the relations X | px |Γ2 = Y | p y |Γ2 =

Z | pz |Γ2 , and thus −

2 X | px |Γ2 X | px |Γ2 2 | X | px |Γ2 |2 =− = F. m E(Γ2 ) m E(Γ2 )

(2.206)

The contribution from |Γ12 (1) and |Γ12 (2) is evaluated by using (1.141a) and (1.141b) or (1.143a) and (1.143b) in Sect. 1.7. In the following we use the notations |γ1− → |Γ12 (1) and |γ2− → |Γ12 (2), −

2 | Γ25 (X )| px |Γ12 , j|2 m j E(Γ12 , j) 2 | Γ25 (X )| px |Γ12 (1)|2 2 | Γ25 (X )| px |Γ12 (2)|2 − m E(Γ12 ) m E(Γ12 ) 2 R∗R 2 (−R) ∗ (−R) =− − = 2G . (2.207) m E(Γ12 ) m E(Γ12 ) =−

Therefore the term L is given by L=

2 [F + 2G] . 2m

(2.208)

2. The parameter M (or Mk 2y ) is associated with the states Γ15 and Γ25 and we easily obtain the following results, H1 = −

2 | X | p y |Γ15 (z)|2 2 | X | p y |Γ15 , j|2 =− , m j E(Γ15 ) m E(Γ15 )

(2.209)

H2 = −

2 | X | p y |Γ25 (1)|2 2 | X | p y |Γ25 , j|2 =− , m j E(Γ25 ) m E(Γ25 )

(2.210)

6

The reason why the upper four conduction bands appear in the matrix elements is understood from the the selection rules Γ25 | p|Γl, j , where p is momentum operator and transforms as the representation Γ15 , and Γl, j are upper conduction band states. The direct product is given by using the character table of Table 1.6 Γ25 × Γ15 = Γ12 + Γ15 + Γ2 + Γ25 , and thus only the conduction band states of the four representations on the right hand perturb the valence band edge.

122

2 Cyclotron Resonance and Energy Band Structures

and then we obtain M=

2 [H1 + H2 ] . 2m

(2.211)

3. Finally N (or C) is evaluated as follows. Contribution from Γ2 to N k y k z : −

2 Y | p y |Γ2 Γ2 | pz |Z 2 | Y | p y |Γ2 |2 =− = F. m E(Γ2 ) m E(Γ2 )

(2.212)

Contribution from Γ12 to N k y k z :

Y | p y |Γ12 ( j) Γ12 ( j)| pz |Z

j

= Y | p y |Γ12 (1) Γ12 (1)| pz |Z + Y | p y |Γ12 (2) Γ12 (2)| pz |Z = (ω R)(ω †2 R) + (−ω 2 R)(−ω † R) = [ω · ω †2 + ω 2 · ω † )R 2 = [ω † + ω]R 2 = −R 2 , (2.213) and thus contribution from Γ12 to N k y k z is −

2 | Y | p y |Γ12 |2 = −G . m E(Γ12 )

(2.214)

Contribution from Γ15 to N k y k z is −

2 | Z | p y |Γ15 (x) Γ15 (x)| pz |Y | = H1 . m E(Γ15 )

(2.215)

Contribution of Γ25 to N k y k z is evaluated using the following symmetry operation. We define Γ25,1 = |z(x 2 − y 2 ) ,

(2.216a)

Γ25,2 = |x(y 2 − z 2 ) , Γ25,3 = |y(z 2 − x 2 ) ,

(2.216b) (2.216c)

X | p y |Γ25,1 = yz| p y |z(x 2 − y 2 ) = U.

(2.217)

and the matrix element by

Symmetry operations by π/2 along x, y and z give the following relations, x − axis : X | pz |Γ25,3 = −U , y − axis : Z | p y |Γ25,2 = −U ,

(2.218) (2.219)

z − axis : Y | px |Γ25,1 = −U .

(2.220)

2.7 Luttinger Parameters

123

When we define 2 2 X | p y |Γ25, j 2 U ·U − =− = H2 , m j E(Γ25, j ) m E(Γ25 )

(2.221)

the contribution of Γ25 to N k y k x is −

2 U · (−U ) 2 X | p y |Γ25, j Γ25, j | px |Y =− = −H2 . m j E(Γ25, j ) m E(Γ25 )

(2.222)

Therefore the total contribution to N (or C) is found to be N=

2 [F − G + H1 − H2 ] . 2m

(2.223)

From these considerations we obtain the following relations for the parameters L, M, N of Dresselhaus, Kip, and Kittel, 2 [F + 2G] , 2m 2 M= [H1 + H2 ] , 2m 2 [F − G + H1 − H2 ] , N = 2m L=

(2.224) (2.225) (2.226)

and thus the parameters A, B, and C of Luttinger are given by 2 [1 + F + 2G] , 2m 2 B= [1 + H1 + H2 ] , 2m 2 [F − G + H1 − H2 ] . C= 2m A=

(2.227) (2.228) (2.229)

Neglecting the spin–orbit splitting of |Γ15 conduction band states, the Luttinger valence band parameters are given by Groves et al. [21] and Lawaetz [22], which are obtained by putting (2.227), (2.228), and (2.229) into (2.198a), (2.198b), and (2.198c) as follows,

124

2 Cyclotron Resonance and Energy Band Structures

1 γ1 = − (F + 2G + 2H1 + 2H2 ) − 1 , 3 1 γ2 = − (F + 2G − H1 − H2 ) , 6 1 γ3 = − (F − G + H1 − H2 ) . 6

(2.230a) (2.230b) (2.230c)

These Luttinger parameters are modified by the parameter q when the spin–orbit splitting Δ15 of the Γ15 conduction band states is taken account [21, 23]. Including the term κ which represents the magnetic filed effect in the Luttinger Hamiltonian, the Luttinger parameters are then given by 1 γ1 = − (F 3 1 γ2 = − (F 6 1 γ3 = − (F 6 1 κ = − (F 6

1 + 2G + 2H1 + 2H2 ) − 1 + q , 2 1 + 2G − H1 − H2 ) − q , 2 1 − G + H1 − H2 ) + q . 2 1 9 − G − H1 + H2 ) − − q , 3 2

where q−

2 H1 Δ15 . 9 E(Γ15 )

(2.231a) (2.231b) (2.231c) (2.231d)

(2.232)

Usually the Luttinger parameters are determined from the experimental data and the energy values of EG = Ec (Γ25 ) − Ev ≡ E0 and Ec (Γ15 ) − Ev (Γ25 ) = E0 are known from optical spectroscopies, and contributions from higher lying bands may be neglected because of the larger energy denominators E j . Then the following two terms are taken into account (note the difference between E P0 and E p as stated in (2.90)), 2 2 | Γ25 (X )| px |Γ2 |2 = P02 , m m 2 2 = | Γ25 (X )| p y |Γ15 (z)| , m

E P0 =

(2.233a)

E P1

(2.233b)

and we obtain F =−

E P0 , EG

H1 = −

E P1 , E1

(2.234)

where the spin–orbit interaction is neglected. When the spin–orbit interaction is included, the matrix element F between the conduction band |Γ2 , j and the valence bands |Γ25 should be modified. Taking account of the lowest conduction band |Γ2 only and of the 6 valence band states | 23 , ± 23 , | 23 , ± 21 , and | 21 , ± 21 , F is evaluated, for the spin–conserved matrix elements, as follows;

2.7 Luttinger Parameters

125

2 | Γ25 (X )| px |Γ2 |2 , m j E(Γ25 ) − E(Γ2 , j) E P0 2 1 =− . + 3 EG E G + Δ0

F=

(2.235)

Since the 8 × 8 k · p Hamiltonian includes the coupling between the conduction band |Γ2 and the valence bands |Γ25 , we have to exclude the contributions from the conduction band |Γ2 , the term F. Therefore the Luttinger parameters γ1 , γ2 , and γ3 should be modified. We redefine the Luttinger parameters as γ1L , γ2L , and γ3L and the new valence band parameters γ1 , γ2 , and γ3 are given by 1 γ1 = γ1L − − F , 3 1 γ2 = γ2L − − F , 6 1 γ3 = γ3L − − F , 6

(2.236a) (2.236b) (2.236c)

and then we obtain 1 3 1 γ2 = γ2L − 6 1 γ3 = γ3L − 6 γ1 = γ1L −

1 E P0 2 , + 3 EG E G + Δ0 E P0 2 1 , · + 3 EG E G + Δ0 E P0 2 1 , · + 3 EG E G + Δ0 ·

(2.237a) (2.237b) (2.237c)

where EG = Ec − Ev is the energy gap and Δ0 is the spin–orbit splitting.7 For more detailed discussion see the Refs. [1, 15, 22, 24]. It should be noted here that the hole effective masses of the valence bands are evaluated by using the original Luttinger parameters γ1L , γ2L , and γ3L , while the eigenstates and eigenvalues of the 8 × 8 k · p Hamiltonian matrix are obtained by using new Luttinger parameters γ1 , γ2 , and γ3 . The new values of the Luttinger parameters are calculated by (2.237a)–(2.237c), but the reported values of F have not yet settled. Pigeon and Brown [15] reported that the experimental data of the inter band magneto-absorption are well explained by putting F = 0 for InSb. They used E P0 = 10.96 [eV], EG = 0.2355 [eV], Δ0 = 0.9 [eV], γ1L = 32.5, γ2L = 14.3, and γ3L = 15.4, and they found a good over–all fit of the magneto-absorption spectra in InSb by putting F = 0. From their data we obtain F = −34.5 (F/3 = −11.5) and the correction factor F/3 is not negligible. Vurgaftman, Meyer, and Ram-Mohan [25] recommend to use E P0 = 23.3 [eV], EG = 0.235 7

Equations (2.179a)–(2.179c) are obtained by neglecting the spin–orbit splitting, or by putting Δ0 = 0 in (2.237a)–(2.237c).

126

2 Cyclotron Resonance and Energy Band Structures

Table 2.1 Energy band parameters of Ge, Si, GaAs, InAs, AlAs, and GaP. The parameters γ1 , γ2 , and γ3 are the original Luttinger parameters which correspond to the redefined Luttinger parameters γ1L , γ2L , and γ3L , respectively, and the effective mass m ∗ is normalized by the free electron mass m Parameters Γ EG EGX EGL

[eV] [eV] [eV] Δ0 [eV] m ∗e (Γ ) m l∗ (L) m ∗t (L) m l∗ (X ) m ∗t (X ) γ1 γ2 γ3 E P0 [eV] F F†

Ge

Si

GaAs

InAs

AlAs

GaP

0.8872 1.3 0.82 0.297 n.a. 1.57 0.0807 n.a. n.a. 13.35 4.25 5.69 26.3 −27.2

4.185 1.17 n.a. 0.044 n.a. n. a. 0.19 0.916 0.19 4.26 0.38 1.56 21.6 −5.14

1.519 1.981 1.815 0.341 0.067 1.90 0.075 1.98 0.27 6.98 2.06 2.93 28.8 −17.8 (−1.94)

0.417 1.433 1.133 0.39 0.026 0.64 0.05 1.13 0.16 20.0 8.5 9.2 21.5 −43.3 (−2.90)

3.099 2.24 2.46 0.28 0.15 1.32 0.15 0.97 0.22 3.76 0.82 1.42 21.1 −6.62 (−0.48)

2.886 2.35 2.72 0.08 0.13 2.0 0.253 1.2 0.15 4.05 0.49 2.93 31.4 −10.78 (−2.04)

n.a. means the value is not available F: Estimated from F = −(E P0 /3)[2/EG + 1/(EG + Δ0 )] F † : F values in parentheses are recommended by Vurgaftman, Meyer, and Ram-Mohan [25]

[eV], Δ0 = 0.81 [eV], γ1L = 34.8, γ2L = 15.5, γ3L = 16.5 and F = −0.23 for InSb. Also they recommend F = −1.94 for GaAs which is about 1/10 of the calculated value from F = −(E P0 /3)[2/EG + 1/(EG + Δ0 )] = −17.8. The band parameters of several semiconductors are summarized in Table 2.1. It is well known that the effective masses in III-V semiconductors may be estimated by the relation (2.84), which is rewritten as E P0 m =1+ m ∗0 3

2 1 =1− F. + EG EG + Δ0

(2.238)

However more accurate values are evaluated by taking account of the contribution from higher lying conduction bands, Γ8c and Γ7c (which are relate to the single group c ), and expressed by the following relation [14, 22, 26] representation Γ15 m = 1 − F − H1 + F , m ∗0 2 1 2 P12 , + H1 = − m 3 E(Γ8c ) E(Γ7c ) + Δ15

(2.239a) (2.239b)

2.8 Problems

127

where E(Γ8c ) and E(Γ7c ) are the energies of the conduction bands (related to the higher lying Γ15 conduction bands in the single group expression) measured from the valence band top Γ8v and Δ15 is the spin–orbit splitting of the bands. The momentum matrix element P1 is defined by Q = 2P1 in (1.135b) of Chap. 1 and the values are given in Tables 1.11 and 1.13. Observed effective mass of the lowest conduction band is known to be well expressed by the above relation with F −2 [14, 22, 26].

2.8 Problems (2.1)

Estimate the magnetic field strength to observe cyclotron resonance for microwave frequency 24 GHz for (1) effective mass m 2 = 0.3m (for Si and Ge) and (2) m ∗ = 0.067m (for GaAs). (3) Discuss the experimental conditions of the cyclotron resonance for the case of (1) and (2).

(2.2)

Prove the commutation relation (2.100) A · p − p · A = i∇ · A = 0 ,

(2.3)

Assume a non–parabolic conduction band and show what kind of dispersion relation of the conduction band is expected when the band gap approaches zero.

(2.4)

Figures 2.3 and 2.4 show the cyclotron masses for heavy and light holes in Ge and Si as a function of applied magnetic field. Heavy holes exhibit maximum in the magnetic field direction [1, 1, 1], while the light hole cyclotron mass is minimum. Explain the behaviour by using the constant energy contour of the valence bands in Fig. 2.12.

(2.5)

Estimate electron effective mass m ∗0 and effective g0∗ factor of InAs using the following parameters. EG = 0.417 [eV], Δ0 = 0.39 [eV], E P0 = 21.5 [eV], E1 = 4.44 [eV], Δ15 = 0.16 [eV], E P1 = E P0 /4 = 5.375 [eV], and C = −0.02. Experimental values are m ∗ = 0.024m and g = −14.7 sin −17.5.

(2.6)

Calculate the matrix element of spin–orbit interaction u − α|L · σ|u − α

(2.7)

The most important relations for the valence band structure are given by Eq. (2.65) and we call here the equations as DKK-ABC after the paper by Dresselhaus, Kip and Kittel [1]. Derive Eq. (2.65) by solving Eq. (2.64) and obtain DKK-ABC coefficients, A, B, and C, given by Eq. (2.66).

(2.8)

Calculate the density of states in (1) parabolic conduction band (2.85) and (2) non–parabolic band given by (2.158).

128

2 Cyclotron Resonance and Energy Band Structures

(2.9)

When magnetic field is [0, 0, B], show the corresponding vector potential A is given by [0, Bx, 0]. This representation is called Landau gauge. List the other representations.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28.

G. Dresselhaus, A.F. Kip, C. Kittel, Phys. Rev. 98, 368 (1955) J.M. Luttinger, Phys. Rev. 102, 1030 (1956) E.O. Kane, J. Phys. Chem. Solids 1, 82 (1956), and 249 (1957) M. Cardona, F.H. Pollak, Phys. Rev. 142, 530 (1966) R. Kubo, H. Hasegawa, N. Hashitsume, J. Phys. Soc. Jpn. 14, 56 (1959) R. Kubo, S.J. Miyake, N. Hashitsume, in Solid State Physics, vol. 17, ed. by F. Seitz and D. Turnbull (Academic, New York, 1965) p. 269 J.M. Luttinger, W. Kohn, Phys. Rev. 97, 869 (1955) R. Bowers, Y. Yafet, Phys. Rev. 115, 1165 (1959) Q.H.F. Vrehen, J. Phys. Chem. Solids 29, 129 (1968) L.M. Roth, B. Lax, S. Zwerdling, Phys. Rev. 114, 90 (1959) W. Zawadzki, Phys. Lett. 4, 190 (1963) K.L. Litvunenko, L. Nikzat, C.R. Pidgeon, J. Allam, L.F. Cohen, T. Ashley, M. Emeny, W. Zawadzki, B.N. Murdin, Phys. Rev. B 77, 033204 (2008) W. Zawadzki, P. Pfeffer, R. Bratschitsch, Z. Chen, S.T. Cundiff, B.N. Murdin, C.R. Pidgeon, Phys. Rev. B 78, 245203 (2008) C. Herman, C. Weisbuch, Phys. Rev. B 15, 823 (1977) C.R. Pidgeon, R.N. Brown, Phys. Rev. 146, 575 (1966) E. Burstein, G.S. Picus, Phys. Rev. 105, 1123 (1957) S. Zwerdling, R.J. Keyes, H.H. Kolm, B. Lax, Phys. Rev. 104, 1805 (1956) S. Zwerdling, B. Lax, Phys. Rev. 106, 51 (1957) S. Zwerdling, B. Lax, L.M. Roth, Phys. Rev. 108, 1402 (1957) S. Zwerdling, B. Lax, L.M. Roth, K.J. Button, Phys. Rev. 114, 80 (1959) S.H. Groves, C.R. Pidgeon, A.W. Ewald, R.J. Wagner, J. Phys. Chem. Solids 30, 2031 (1970) P. Lawaetz, Phys. Rev. B 4, 3460 (1971) J.C. Hensel, K. Suzuki, Phys. Rev. Lett. 22, 838 (1969) C. Pryor, Phys. Rev. B 57, 7190 (1998) I. Vurgaftman, J.R. Meyer, L.R. Ram-Mohan, J. Appl. Phys. 89, 5815 (2001) H. Hazama, T. Sugimasa, T. Imachi, C. Hamaguchi, J. Phys. Soc. Jpn. 55, 1282 (1986) T.B. Bahder, Phys. Rev. B 41, 11992 (1990) Y. Zhang, Phys. Rev. B 49, 14352 (1994)

Chapter 3

Wannier Function and Effective Mass Approximation

Abstract Effective–mass equation is very useful to understand the transport and optical properties of semiconductors. In this chapter the effective–mass equation is derived with the help of Wannier function. Using Schrödinger equation based on the effective–mass approximation, we discuss the shallow impurity levels of donors in Ge and Si. Transport properties of electrons and holes are interpreted in terms of the effective mass in the classical mechanics (Newton equation). In this chapter the group velocity (the expectation value of the velocity) is shown to be given by v = (1/)∂E/∂k in a periodic crystal potential. In the presence of an external force F, an electron is accelerated in k space in the form of ∂k/∂t = F. The electron motion is then expressed in the classical picture of a particle with the effective mass m ∗ or 1/m ∗ = (1/2 )∂ 2 E/∂k2 and the momentum p = k = m ∗ v. The results are used to derive transport properties in Chap. 6.

3.1 Wannier Function There have been reported several methods to derive the effective–mass equation. In this chapter we use the Wannier function approach to derive the effective–mass equation because of its importance in semiconductor physics. However, in this chapter a simplest case will be dealt with, where only a single band is taken into account. For this purpose we begin with the introduction of the Wannier function showing that it is localized at the lattice point and that the Wannier function is obtained from the Bloch function by the Fourier transform. When the Bloch function of a energy band n is defined by bkn (r), the Wannier function wn (r − R j ) is derived from the Bloch function by the Fourier transform [1]: 1 wn (r − R j ) = √ exp(−ik · R j )bkn (r), (3.1) N k where N is the number of atoms and R j is the position of jth atom. We have shown in Chap. 1 that the Bloch function extends over the crystal. On the other hand, the

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2023 C. Hamaguchi, Basic Semiconductor Physics, Graduate Texts in Physics, https://doi.org/10.1007/978-3-031-25511-3_3

129

130

3 Wannier Function and Effective Mass Approximation

Wannier function is localized at the atom, as shown later. Here we will investigate the features of the Wannier function. First, we will show the Bloch function can be expanded in Wannier functions: 1 exp(ik · R j ) · wn (r − R j ). bkn (r) = √ N j

(3.2)

We find that this expansion is just the inverse transform of the Wannier function given by (3.1) and it is easily proved as follows. Inserting (3.1) in (3.2) we obtain 1 1 bkn (r) = √ exp(ik · R j ) √ exp(−ik · R j )bk n (r) N j N k 1 = exp i(k − k ) · R j bk n (r) ≡ bkn (r). N

(3.3)

jk

The final result of the above equation is obtained by using (A.28) of Appendix A.2:

exp i(k − k ) · R j = N δk,k .

(3.4)

j

Next, we show the orthonormal property of Wannier functions that Wannier functions associated with different atoms are orthogonal and that Wannier functions of different energy bands are diagonal.

wn∗ (r − R j )wn (r − R j )d3 r 1 = d3 r exp(ik · R j − ik · R j )b∗k n (r)bkn (r) N k,k 1 = exp(ik · R j − ik · R j ) b∗k n (r)bkn (r)d3 r N k,k

1 exp ik · (R j − R j ) δn,n = δ j, j δn,n , = N k

(3.5)

and thus it is proved that Wannier functions are orthonormal. Let us examine the localization characteristics of the Wannier function wn (r − R j ) at each lattice point R j . As shown in Chap. 1 the Bloch functions are not localized in the crystal. For simplicity we assume that the Bloch function is approximated as bkn (r) = u 0n (r) exp(ik · r)

(3.6)

and that the term u 0n (r) is independent of k. This approximation is understood to be quite reasonable because the electronic states are well described by the Bloch

3.2 Effective-Mass Approximation

131

function at the band edge as shown in the k · p perturbation method of Sect. 1.7. Under this assumption the Wannier function is approximated as 1 exp ik · (r − R j ) . wn (r − R j ) = √ u 0n (r) N k

(3.7)

As given by (A.21) and (A.22) in Appendix A.2 the following relation is easily obtained: eik·(r−R j ) = L 3 δ(r − R j ), (3.8) k

1 L3

d3 rei(k−k )·r = δk,k ,

(3.9)

where δ(r − r ) is the Dirac delta function and δk,k is the Kronecker delta function. Using this result the Wannier function is written as 1 wn (r − R j ) = √ u 0n (r)L 3 δ(r − R j ), N

(3.10)

and therefore we find that the Wannier function is localized at the lattice point R j .

3.2 Effective-Mass Approximation Here we will derive of the effective–mass approximation which may be applied to a wide variety of calculations of the electronic properties of semiconductors, for example shallow impurity states, transport, optical properties and so on. Here we assume that the perturbing potential H1 (r) varies very slowly compared with the lattice constant a. This assumption allows us to simplify the effective–mass equation based on a single band. The Schrödinger equation for the one-electron Hamiltonian is written as (3.11) [H0 + H1 (r)]Ψ (r) = E · Ψ (r), where H0 =

p2 + V (r), 2m

(3.12)

and we will show that the solution of above equation is given by the solution 2 − ∗ ∇ 2 + H1 (r) F(r) = E · F(r), 2m

(3.13)

132

3 Wannier Function and Effective Mass Approximation

where m ∗ is the effective–mass of the electron we are concerned with. In the following we assume the effective–mass is given by a scalar effective–mass for simplicity. Therefore, the energy of the electron E is assumed to be expressed by the wave vector k: 2 k 2 . (3.14) E0 (k) = 2m ∗ Equation (3.13) is called the effective–mass equation and this approximation is called the effective–mass approximation. The reason why we call this the effective– mass approximation is quite clear. The Schrödinger equation (3.11) with the Hamiltonian of (3.12) is expressed in a simple Schrödinger equation by replacing the Hamiltonian of (3.12) by −(2 /2m ∗ )∇ 2 , where the potential disappears and m is replaced by m ∗ . The derivation of the effective–mass equation will be shown later. First, we calculate the eigenfunction Ψ (r) of (3.11). Since the Wannier function is expressed by the Fourier transform of the Bloch functions and thus Wannier functions have orthonormality and completeness, any function may be expanded by Wannier functions: Fn (R j )wn (r − R j ). (3.15) Ψ (r) = n

j

In the following we consider a specific band and neglect the band index n of the subscript. In the absence of perturbation the Schrödinger equation is expressed in terms of the Bloch functions bkn (r) as H0 bk (r) = E0 (k)bk (r). Inserting Ψ (r) =

F(R j )w(r − R j )

(3.16)

(3.17)

j

into (3.11), multiplying w ∗ (r − R j ) on both sides and integrating over the crystal volume we obtain w ∗ (r − R j )H0 F(R j )w(r − R j )d3 r j

+

=

j

E

w ∗ (r − R j )H1 F(R j )w(r − R j )d3 r

w ∗ (r − R j )F(R j )w(r − R j )d3 r.

j

When we define the following relations

(3.18)

3.2 Effective-Mass Approximation

(H0 ) j j =

(H1 ) j j =

133

w ∗ (r − R j )H0 w(r − R j )d3 r,

(3.19)

w ∗ (r − R j )H1 w(r − R j )d3 r,

(3.20)

(3.18) is rewritten as (H0 ) j j · F(R j ) + (H1 ) j j · F(R j ) = E · F(R j ). j

(3.21)

j

The right-hand side of the above equation is rewritten with the help of (3.5). Since we assume that the perturbing potential varies very slowly, the following approximation is possible. From the properties of the Wannier function, w∗ (r − R j ) and w(r − R j ) are localized at R j and R j , respectively, and thus only the overlapping part of w ∗ (r − R j ) and w(r − R j ) will contribute to the integration of (3.20). The integration arising from small values of (R j − R j ) or the integration over the nearest neighbor will contribute. In a more simplified approximation only the contribution from R j = R j may be taken into account. In this approximation the summation of (3.20) over j results in

(H1 )

H1 (R j )

j j

w ∗ (r − R j )w(r − R j )d3 r = H1 (R j ).

(3.22)

j

It is evident from (3.20) that (H0 ) j j is a function of (R j − R j ), which is shown by using the Wannier function as follows. H0 is independent of the translation vector R. Therefore, replacing r − R j with r we find (H0 ) j j =

w ∗ (r)H0 w(r − R j + R j )d3 r ≡ h 0 (R j − R j ).

(3.23)

Using these results (3.21) is rewritten as the following set of equations:

h 0 (R j − R j )F(R j ) + H1 (R j )F(R j ) = E · F(R j ).

(3.24)

j

Exchanging the order of the summation of the first term on the left-hand side of the above equation, (R j − R j ) → R j , we obtain the following result:

h 0 (R j )F(R j − R j ) + H1 (R j )F(R j ) = E · F(R j ).

(3.25)

j

Equation (3.12) gives the relation E0 (k) =

b∗k (r)H0 bk (r)d3 r

(3.26)

134

3 Wannier Function and Effective Mass Approximation

and it may be rewritten as follows by using (3.2), which is an expansion of the Bloch function in Wannier functions: E0 (k) = =

1 exp[−ik · (R j − R j )](H0 ) j j N j j

1 exp[−ik · (R j − R j )]h 0 (R j − R j ). N j j

(3.27)

It is very important to point out that R j and R j give a combination of the same lattices. Therefore, the summation of R j with respect to j gives the same value for different R j . In other words, the summation is exactly the same for j = 1, 2, 3, . . . , N . This will lead us to obtain the equation: E0 (k) =

1 N exp(−ik · R j )h 0 (R j ) = exp(−ik · R j )h 0 (R j ). N j j

(3.28)

The result may be understood as follows. The energy band E0 (k) is a periodic function in k space and the period is the lattice vectors R j ; therefore, E0 (k) can be expanded by the lattice vector R j . In addition, the Fourier coefficient h 0 (R j ) of the expansion is given by 1 E0 (k) exp(ik · R j ). (3.29) h 0 (R j ) = N k

Next, let us consider a function F(r − R j ) and apply the Taylor expansion to it at the position r , which gives rise to the following result in the case of a one–dimensional crystal: F(r − R j ) = F(r ) − R j

1 d d2 F(r ) + (R j )2 2 F(r ) − · · · . dr 2! dr

(3.30)

In the case of a three-dimensional crystal the function F(r − R j ) is expanded as F(r − R j ) = F(r) − R j · ∇ F(r) + = exp(−R j · ∇)F(r),

1 (R j · ∇)[R j · ∇ F(r)] − · · · 2!

and therefore we obtain h 0 (R j )F(r − R j ) = h 0 (R j ) exp(−R j · ∇)F(r). j

(3.31)

(3.32)

j

On the other hand, when (3.28) is multiplied by F(r) on the both sides, we find

3.2 Effective-Mass Approximation

E0 (k)F(r) =

135

h 0 (R j ) exp(−ik · R j )F(r).

(3.33)

j

Now, let us compare (3.32) with (3.33), we find that a replacement of k with −i∇ in (3.33) gives exactly the same result as in the right-hand side of (3.32). Therefore, the following relation may be obtained:

h 0 (R j )F(r − R j ) = E(−i∇)F(r).

(3.34)

j

Using this result and replacing R j by r, (3.25) becomes

h 0 (R j )F(r − R j ) + H1 (r)F(r) = E · F(r)

(3.35)

j

and may be rewritten as E0 (−i∇)F(r) + H1 (r)F(r) = E · F(r).

(3.36)

Or it is possible to rewrite it in the following form: [E0 (−i∇) + H1 (r)] F(r) = E · F(r),

(3.37)

which is called the effective–mass equation. This kind of approximation is called the effective–mass approximation. We have to note here that the function F(r) given by (3.37) is an envelope function and that the Fourier coefficients F(R j ) of the wave function Ψ (r) expanded in Wannier functions are given by F(R j ), which may be obtained by replacing r of the envelope function F(r) by R j . Now we find that the envelope function F(r) should be a slowly varying function of r. In other words the coefficient F(R j ) should vary very slowly over the distance of the lattice spacing (R j+1 − R j ) as shown in Fig. 3.1. E0 (k) is the electronic energy as a function of the wave vector without the perturbing potential H1 , and thus it gives the energy band of the electron. For simplicity we assume that the energy band is given by a spherical parabolic band with isotropic effective mass m ∗ :

Fig. 3.1 Schematic illustration of the Fourier coefficient F(R j ) and its envelop function F(r), where R j is a lattice point and F(r) gives wave function of the effective mass approximation

136

3 Wannier Function and Effective Mass Approximation

E0 (k) =

2 k 2 . 2m ∗

(3.38)

The effective–mass equation is therefore given by 2 2 − ∗ ∇ + H1 (r) F(r) = E · F(r). 2m

(3.39)

When we compare (3.11) with (3.39), we find the following features. The periodic potential V (r) of (3.11) disappears and the free electron mass m is replaced by the effective–mass m ∗ . The effective–mass equation is named after these features. As stated before, various properties of semiconductors are calculated by using the effective–mass equation. This means that the determination of the effective–mass is very important. We have to note that the effective mass equation or effective–mass approximation is derived by different approaches [2] and that one of the methods is shown in the analysis of exciton given in Sect. 4.5.

3.3 Shallow Impurity Levels One of the best examples of the applications of the effective–mass approximation is the analysis of donor levels in semiconductors. First, we deal with the donor level associated with a conduction band expressed by a scalar effective–mass m ∗ . Under this assumption the effective–mass equation is given by 2 e2 − ∗ ∇2 − F(r) = E · F(r). 2m 4πκ0 r

(3.40)

Careful observation of the above equation reveals that it is equivalent to the Schrödinger equation used to derive the electronic states of a hydrogen atom. The above equation is from the Schrödinger equation of the hydrogen atom, replacing the free electron mass m by m ∗ and the dielectric constant of free space by the dielectric constant of the semiconductor κ0 = . Therefore, the ground state energy E and the effective Bohr radius aI of the donor are m ∗ e4 m ∗ /m = − ER 2(4π)2 2 (/0 )2 me4 ER = 2(4π0 )2 2 4π2 /0 aI = ∗ 2 = ∗ aB , m e m /m

E=−

(3.41) (3.42) (3.43)

3.3 Shallow Impurity Levels

137

where ER is the ionization energy of the hydrogen atom (ER = 1 Rydberg = 13.6 eV). Let us try to estimate the ionization energy of a donor by assuming the effective– mass m ∗ = 0.25 m and the relative dielectric constant /0 = 16. We obtain the ionization energy of donor as 0.013 eV, which is very close to the ionization energy observed in Ge. We have already shown in Chaps. 1 and 2 that the conduction band minima of Ge and Si are located at the L and the Δ points near the X point in the Brillouin zone, respectively, and that they consist of multiple valleys with anisotropic effective–masses. Therefore, the above simplified analysis cannot be applied to the case of donors in Ge and Si. In addition we have to note that the donor levels in manyvalley semiconductors are degenerate due to the multiple conduction band minima. First, we neglect the degeneracy to analyze the donor levels of Ge and Si, and later we deal with the degeneracy. Let us consider a conduction band with an ellipsoidal energy surface and take the z direction to be along the longitudinal axis of the ellipsoid. When we measure the energy with respect to the bottom of the conduction band at k0 and define the effective–masses along the longitudinal axis as m l and the transverse axis as m t , we may write the energy band as k z2 2 k x2 + k 2y . Ec (k) = + 2 mt ml

(3.44)

Therefore, the effective–mass equation for donor levels associated with the conduction band becomes 2 ∂ 2 ∂ 2 2 ∂2 − − + 2 2 2m t ∂x ∂y 2m l ∂z 2 e2 ψ(r) = E · ψ(r), (3.45) − 4π(x 2 + y 2 + z 2 )1/2 where is the dielectric constant of the semiconductor. Defining the effective–mass ratio mt γ= (< 1) (3.46) ml and rewriting (3.45) using cylindrical coordinates we obtain 2 1 ∂ ∂ ∂2 1 ∂2 − +γ 2 r + 2 2m t r ∂r ∂r r ∂ϕ2 ∂z e2 ψ(r) = E · ψ(r). − 4π(r 2 + z 2 )1/2 The effective–mass Hamiltonian is then written as

(3.47)

138

3 Wannier Function and Effective Mass Approximation

2 H=− 2m t

1 ∂ ∂ 1 ∂2 ∂2 r + 2 + γ r ∂r ∂r r ∂ϕ2 ∂z 2

−

e2 . 4π(r 2 + z 2 )1/2

(3.48)

It is impossible to solve (3.47) analytically. Therefore, we adopt the variational principle to obtain approximate solutions. In order to obtain the ground state level of the donor we use the following trial function for the state [3–5]: ψ = (πa b) 2

−1/2

r2 z 2 1/2 exp − 2 + 2 , a b

(3.49)

where a > b and ψ is normalized such that ψ|ψ = 1. We use the following transform of the variables to obtain ψ|H|ψ: r = au cos v, z = bu sin v, +∞ 3 d r = 2π r dr

V

0 +∞

= 2π 0

+∞

dz

−∞ +π/2

−π/2

abu 2 cos v dy du.

Then the ground state of the donor is given by E = ψ ∗ |H|ψ +∞ +π/2 2 cos v 2 sin2 v (u −1 + 1) =− +γ 2 2m t 0 a2 b −π/2

γ 2 2 −1 −1 + 2 u + u − a2 b a I (a 2 cos2 v + b2 sin2 v)1/2 ×e−2u 2u 2 cos v dv du

2 a 2 − b2 γ 2 2 −1 =− sin − 2− 2+ √ . 2m t 3a 3b a2 a I a 2 − b2

(3.50)

The variational principle is used to minimize E in (3.50) by varying the parameters a and b. To do this we introduce another transform of the variables by ρ2 =

a 2 − b2 , (0 < ρ2 < 1), a2

(3.51)

and eliminate b to obtain 2(1 − ρ2 ) + γ 2 2 sin−1 ρ − 3 . E =− + 2m t 3a (1 − ρ − 2) ρaaI

(3.52)

139

⁄

3.4 Impurity Levels in Ge and Si

Fig. 3.2 Ionization energy of a donor calculated from the effective–mass equation and by the variational principle plotted as a function of the effective–mass ratio γ = m t /m l

The value of a to minimize the above equation is easily deduced and is given by a=

ρ[2(1 − ρ2 ) + γ] aI . 3(1 − ρ2 ) sin−1 ρ

(3.53)

Inserting this value of a into (3.50) we obtain the ground state energy: E=

3(1 − ρ2 )(sin−1 ρ)2 EI . ρ2 [2(1 − ρ2 ) + γ]

(3.54)

where EI = − =−

m t e4 2 2 (4π)2

m t 0 2 ER (ER = 13.6 eV = 1 Rydberg). m

(3.55)

From this expression we find that EI is the ground state energy of the donor associated with a conduction band of a semiconductor with the transverse effective–mass m t and dielectric constant . The ionization energy of the donor may be obtained from the value of ρ to minimize (3.54) for an arbitrary value of γ = m t /m l . However, the value to minimize (3.54) may not be obtained analytically, and thus we used a numerical analysis. The results are shown in Fig. 3.2.

3.4 Impurity Levels in Ge and Si The parameters used for the calculations of the impurity levels in Ge and Si are summarized in Table 3.1 and the results obtained by the variational principle are shown in Table 3.2, where the ionization energies are 9.05 meV for Ge and 29.0 meV for Si. The experimentally observed ionization energies (summarized in Table 3.3) are about 10 meV for Ge, in good agreement with the calculation, and about 45 meV

140

3 Wannier Function and Effective Mass Approximation

Table 3.1 Parameters used to calculate the donor levels of Ge and Si. The parameters are given in dimensionless units m t /m m l /m γ /0 Ge Si

0.082 0.190

1.58 0.98

0.0519 0.1939

16.0 11.9

Table 3.2 Ground state energies of donors in Ge and Si calculated by the effective–mass approximation and the variational principle −E I −E /E I (−E ) aI a/a I (a) b/a I (b) [meV] [meV] [Å] [Å] [Å] Ge Si

4.36 18.3

2.08 1.59

(9.05) (29.0)

103.2 33.14

0.622 0.740

(64.2) (24.5)

0.221 0.415

(22.8) (13.8)

Table 3.3 The ionization energies E0 (meV) of various donors in Ge and Si determined by experiments Li P As Sb Bi Si Ge

33

45 12.0

49 12.7

39 9.6

69

for Si, not in good agreement with the calculation. The good agreement is understood from the large value of the effective Bohr radius in Ge and thus the impurity potential varies slowly compared with the lattice constant, leading to a good condition to use the effective–mass approximation. On the other hand, the effective Bohr radius for Si is smaller and the effective mass approximation seems to be invalid for the calculation of the ground states in Si. The discrepancy between the calculation and the experimental values may arise from the neglect of the degeneracy of the conduction band minima in addition to the validity of the effective–mass approximation. We will discuss these two factors in the following. We may expect that the excited states of an impurity give a good agreement between the calculation and the experiment. This is because the wave functions of the excited states extend over space more than the ground state, and thus the effective– mass approximation becomes more accurate for the excited states. In order to check the validity of the effective–mass equation for the excited states we calculate the excited states using the trial functions shown in Table 3.4. Using the parameters given in Table 3.4 and the variational method, the excited states of donors in Ge and Si are calculated and are summarized in Table 3.5. As stated above the discrepancy between theory and experiment is considerable for the ground state in Si. We compare the calculations based on the effective–mass approximation with the experimental data in Si, which is shown in Table 3.6 and in Fig. 3.3. Although the ground state level does not show a good agreement, the excited states show reasonable agreement between the experiment and calculation.

3.4 Impurity Levels in Ge and Si

141

Table 3.4 Trial functions for calculating the excited states of donors by the variational method States Variational functions 2 r z 2 1/2 1s (πa 2 b)−1/2 exp − 2 + 2 a b 2 r z 2 1/2 2s (C1 + C2 r 2 + C3 z 2 ) exp − 2 + 2 a b 2 2 z 1/2 r 2p0 C z exp − 2 + 2 a b 2 r z 2 1/2 2p±1 Cr exp − 2 + 2 exp(±iφ) a b 2 z 2 1/2 r 3p0 (C1 + C2 r 2 + C3 z 2 )z exp − 2 + 2 a b 2 r z 2 1/2 exp(±iφ) 3p±1 (C1 + C2 r 2 + C3 z 2 )r exp − 2 + 2 a b

Table 3.5 Ground state and excited states levels of the donors in Ge and Si States Si Ge 1s 2p, m 2s 2p, m 3p, m 3p, m

−29 −10.9 −8.8 −5.9 −5.7 −2.9

=0 = ±1 =0 = ±1

±1 ± 0.2 ± 0.6 ± 0.1 ± 0.6 ± 0.05

−9.2 −4.5

± 0.2 ± 0.2

−1.60 −2.35 −0.85

± 0.03 ± 0.2 ± 0.05

Table 3.6 Experimental values of the ground state and the excited state levels of various donors (P, As and Sb) in Si (meV) and the calculated values by the effective–mass approximation (shown by EMA) Impurities Ground state Excited states P As Sb EMA

45 53 43 29

10.5 10.9 11.2 10.9

5.5 5.6 6.5 5.9

2.4 2.4 3.1 2.9

0.4 0.1

This suggests us the validity of the effective–mass approximation, giving rise to a good agreement for the excited states. From these considerations we may conclude that the excited states of donors in Ge and Si are well described by the effective–mass approximation. In order to discuss the ground state we have to take into account the degeneracy of the conduction band minima (many valleys), valley–orbit interaction. and later the method for improving the calculation for the ground state (central cell correction) [6].

142

3 Wannier Function and Effective Mass Approximation

Fig. 3.3 Experimental values of the donor levels of P, As and Sb in Si compared with the calculated values by the effective–mass approximation (EMA)

3.4.1 Valley–Orbit Interaction As an example we discuss the valley–orbit interaction in Si, which has six equivalent valleys located at the Δ point in the 100 direction of Brillouin zone. The eigenfunctions of these six valleys are described by ψ (i) (r) =

6

αij F j (r)u j (r) exp(ik0 j · r),

(i = 1, . . . , 6)

(3.56)

j=1

where j = 1, 2 . . . , 6 are the indices for the conduction band minima of six valleys at (±k0 , 0, 0), (0, ±k0 , 0) and (0, 0, ±k0 ), and u j (r) exp(ik0 j · r) and F j (r) are the Bloch function of the jth conduction band and the H atom-like envelope function determined from the effective–mass approximation, respectively. The linear combination of the wave functions is factorized with the help of group theory to give an irreducible representation, and the coefficients of the irreducible representation, αij , are then given by √ α1j : 1/ 6(1, 1, 1, 1, 1, 1)

α2j : 1/2(1, 1, −1, −1, 0, 0) α3j : 1/2(1, 1, 0, 0, −1, −1) ⎫ √ α4j : 1/ 2(1, −1, 0, 0, 0, 0) ⎪ ⎬ √ α5j : 1/ 2(0, 0, 1, −1, 0, 0) √ ⎪ α6j : 1/ 2(0, 0, 0, 0, 1, −1) ⎭

(A1 ) (E)

(3.57)

(T1 )

It may be expected from the above equation that the ground state of a donor in Si splits into three groups due to the valley–orbit interaction: singlet, doublet and triplet. The matrix elements of the Hamiltonian Hvo for the valley–orbit interaction

3.4 Impurity Levels in Ge and Si

143

are then described as the following for the wave functions F j (r) ( j = 1, 2, . . . 6) by introducing a parameter Fi (r) exp[i(k0i − k0 j ) · r]|Hvo |F j (r) = −Δ [7, 8]: 0 −Δ −Δ −Δ −Δ −Δ 0 −Δ −Δ −Δ −Δ −Δ 0 −Δ −Δ i|Hvo | j = −Δ −Δ −Δ 0 −Δ −Δ −Δ −Δ −Δ 0 −Δ −Δ −Δ −Δ −Δ

−Δ −Δ −Δ . −Δ −Δ 0

(3.58)

Diagonalization of (3.58) gives rise to a single state with energy 5Δ and a 5–fold degenerate state with energy −Δ. The single state corresponds to the singlet state given by (3.58), and the 5–fold degenerate state to the doublet and triplet states of (3.58). The splitting of the doublet and triplet states is due to the difference in the valley–orbit interaction between the sets of the valleys. The valley-orbit interaction between the valleys such as (±k0 , 0, 0) (g–type) and between the sets such as (k0 , 0, 0) and (0, k0 , 0) (f–type) are expected to be different. When we take account of the difference and assume the interaction for the g–type as (1 + δ)Δ, the matrix elements are rewritten as 0 −(1 + δ)Δ −Δ −Δ −Δ −Δ −(1 + δ)Δ 0 −Δ −Δ −Δ −Δ −Δ −Δ 0 −(1 + δ)Δ −Δ −Δ −Δ −Δ −(1 + δ)Δ 0 −Δ −Δ −Δ −Δ −Δ −Δ 0 −(1 + δ)Δ −Δ −Δ −Δ −Δ −(1 + δ)Δ 0 −5Δ − δΔ 0 0 0 0 0 0 Δ − δΔ 0 0 0 0 0 0 Δ − δΔ 0 0 0 = .(3.59) 0 0 0 Δ + δΔ 0 0 0 0 0 0 Δ + δΔ 0 0 0 0 0 0 Δ + δΔ From (3.59) we obtain the following results for the ground states, where we have assumed that the singlet state A1 is the ground state: E(A1 )= 0 (singlet), E(E) = 6Δ (doublet), E(T1 ) = 6Δ + 2δΔ (triplet),

(3.60)

where we find that the valley–orbit interaction results in the splitting of the 1s ground state in three groups. From the analysis by infrared spectroscopy of the donors P, As

144

3 Wannier Function and Effective Mass Approximation

Table 3.7 Binding energies of 1s states for donors of P, As and Sb in Si (meV). The splitting is due to valley-orbit interaction (see text) States P As Sb 1s(E) 1s(T1 ) 1s(A1 )

32.21 33.58 45.31

31.01 32.42 53.51

30.23 32.65 42.51

and Sb in Si, the binding energies of the 1s states are given by the values listed in Table 3.7 [9]. From the analysis of the intensity of infrared absorption of P donors in Si, the valley–orbit interaction given by (3.60) is determined to be 6Δ = 13.10 meV and 2δΔ = −1.37 meV, and therefore we can conclude that the 1s donor state splits into 1s(A1 ) (singlet), 1s(T1 ) (triplet) and 1s(E) (doublet) in the order from the lowest to the highest level. The splitting due the valley–orbit interaction is very small and the difference between experiment and theory cannot be explained. This may require more detailed analysis of the donor states. The discrepancy may be explained by taking an exact wave functions for the donor, but it is impossible to go further. Instead we will derive an appropriate method to analyze the optical spectra of donors in Ge and Si in the next subsection.

3.4.2 Central Cell Correction In the derivation of the effective–mass equation we noted that the validity of the effective–mass approximation requires a larger effective Bohr radius aI of a donor compared with the lattice constant a (aI a). As seen in Table 3.2, the variational parameters a and b are smaller in Si than in Ge. In addition we know that the effective radius of the orbit is larger for the excited states compared to the ground state. These results will explain the better agreement of the ground state energy in Ge than in Si and a reasonable agreement of the excited states in Si between experiment and the effective–mass theory. We have to note that the difference between the donor states in different donor atoms cannot be explained by the effective–mass approximation. The disagreement of the theory may be due to the potential shape near the center of the impurities and it is expected that the potential near the impurity atom is not Coulombic. The exchange interaction of donor electrons with core electrons and their correlations will play an important role in the determination of the ground state. In addition, the screening effect is weakened in the region near the core. Taking all of these effects into account, we have to correct the potential near the core in the effective–mass approximation. Here we will present the “central cell correction” according to the treatment reported by Kohn [6]. The treatment is based on the assumption that the ground state reflects the energy observed from experiments. Then a correction is made for the wave function of the ground state to explain the infrared

3.4 Impurity Levels in Ge and Si

145

Fig. 3.4 Central cell correction of the donor ground state, where the corrected wave function and the envelope function of the effective–mass equation are shown. The corrected wave function is chosen to give the experimental donor level and extrapolated near the center

absorption spectra between the ground state and the excited states. No corrections for the excited states are required because of the good agreement between the experiment and theory. Since the experimental value of the ground state binding energy Eobs is larger than the result of the effective–mass approximation in general, the wave function is expected to increase steeply near the center of the impurity atom, as shown in Fig. 3.4. Therefore, we assume that 1 F(r) u j (r)eik j ·r , 6 j=1 2 2 e F(r) = Eobs F(r), − ∗ ∇2 − 2m 4πr F(∞) = 0, 6

r ≥ rs :

ψ=

(3.61) (3.62) (3.63)

and use the wave function F(r), which shows a good agreement with experiment. In other words, we determine the effective Bohr radius of the function F(r) ≈ e−r/a

∗

(3.64)

to give the experimental value of the donor ground state. We find that a ∗ is determined by the following relation using the values of the effective–mass equation Eeffmass and of experiment Eobs . a∗ =

Eeffmass aI . Eobs

(3.65)

In the region r < rs the potential reflects the respective type of the donor and thus the corresponding correction to the wave function. However, it may be well approximated by (3.66) r < rs ; F(r) F(r s ).

146

3 Wannier Function and Effective Mass Approximation

This procedure is shown in Fig. 3.4 and the process is called the “central cell correction”. This method is known to give a good explanation of the infrared absorption spectra and the intensity of the absorption [9].

3.5 Electron Motion Under an External Field Here we derive equations of electron motion under an external field in a periodic potential. The equations are well known but the derivation so far reported is based on an assumption that group velocity v g of an electron in a crystal is given by vg =

1 ∂E . ∂k

(3.67)

The above equation is derived by using the following relations vg =

∂ω , ∂k

E = ω.

(3.68)

Such a derivation does not deal with electrons in periodic potential correctly, but it is based on an analogy of electron particle with propagating wave as given by (3.68). First, we derive the expectation value of electron velocity in periodic potential, which is shown to coincide with the group velocity given by (3.67). Then we show quantum mechanical treatment of acceleration of an electron in the energy band. The results lead to the similarity of electron motion in classical mechanics and to the definition of effective mass.

3.5.1 Group Velocity In this subsection we will show that the expectation value of the electron velocity v is defined by the following relation; v =

1 1 gradk E(k) = ∇k E(k).

(3.69)

The velocity in classical mechanics may be related to the expectation value of the velocity in quantum mechanics. Once we obtain the group velocity, then the electron motion may be described by the equation of motion in classical mechanics. The expectation value of the electron velocity should be evaluated by using the eigenfunction of an electron. Here we calculate the expectation value by using Bloch function in periodic potential V (r). The Bloch function is given by (1.23) of Chap. 1 as

3.5 Electron Motion Under an External Field

147

1 Ψk (r) ≡ |k = √ A G (k)ei(k+G)·r , Ω G

(3.70)

where G is the reciprocal lattice vector and Ω is the volume of the unit cell. In the following we assume that the external field is weak and the electron moves in the same band, and thus we omit the index of the energy bands. Since the momentum operator is given by p = −i∇, the expectation value of the electron velocity v in the state |k is given by i i 1 k|v|k = k| p|k = − k|∇|k = − m m m

Ψk∗ (r)∇Ψk (r)d3 r.

(3.71)

The above equation is evaluated by using the following relations derived in Chap. 1 ∇|k = ∇Ψk (r) =

G

∇ 2 |k = ∇ 2 Ψk (r) = −

i(k + G)ei(k+G)·r A G (k),

(k + G)2 ei(k+G)·r A G (k).

The Bloch function Ψk (r) is normalized in the unit cell Ω as 1 Ψk∗ (r)Ψk (r)d3 r = A∗G (k)A G (k)d3 r Ω Ω Ω G |A G (k)|2 = 1. =

(3.72) (3.73)

(3.74)

G

Using (3.72) and the reciprocal lattice vectors G and G , (3.71) is written as k|v|k = =

1 mΩ

A∗G (k)e−i(k+G )·r (k + G)ei(k+G)·r A G (k)d3 r

G ,G

1 (k + G) A∗G (k)A G (k)ei(G−G )·r d3 r, m Ω

(3.75)

G ,G

where the above integral becomes 0 except the case G = G , and thus we obtain the following equation k|v|k =

k + (k + G)|A G (k)|2 = G|A G (k)|2 . m G m m G

(3.76)

When the right hand side of (3.76) is shown to be equal to (1/)∇E(k), then the relation (3.69) will be proved.

148

3 Wannier Function and Effective Mass Approximation

Using (3.73) Schrödinger equation is written as 2 (k + G)2 A G (k)ei(k+G)·r + V (r)A G (k)ei(k+G)·r 2m G G i(k+G)·r = E(k) A G (k)e .

(3.77)

G

Multiplying both sides of the above equation by e−i(k+G )·r and integrating in the unit cell we obtain 2 2 (k + G) A G (k)ei(G−G )·r d3 r 2m G V (r)A G (k)ei(G−G )·r d3 r + G

= E(k)

A G (k)ei(G−G )·r d3 r.

(3.78)

G

As described in Chap. 1, the periodic potential of a crystal V (r) can be expanded in terms of the reciprocal lattice vectors by Fourier expansion theorem, and its expansion coefficient is given by V (G) = (1/Ω) V (r)eiG·r . Therefore we obtain 2 (k + G )2 A G (k) + Ω V (G − G )A G (k) = E(k)A G (k). 2m G

(3.79)

Since G and G are the reciprocal lattice vectors, we exchange G and G in (3.79) and we obtain the following relation 2 (k + G)2 A G (k) + Ω V (G − G)A G (k) = E(k)A G (k). 2m

(3.80)

G

The complex conjugate of the above equation is written as 2 (k + G)2 A∗G (k) + Ω V (G − G)A∗G (k) = E(k)A∗G (k), 2m

(3.81)

G

First, we multiply both sides of (3.80) by ∇k A∗G (k) and sum up with respect to G . Second, we multiply both side of (3.81) by ∇k A G (k) and sum up with respect to G . Then we sum up each side of the derived two equations, and find

3.5 Electron Motion Under an External Field

149

2 (k + G)∇k (A∗G · A G ) 2m G V (G − G)(A G ∇k A∗G + A G ∇k A G ) +Ω G

G

= E(k)

(A G ∇k A∗G + A∗G ∇k A G ) ≡ 0.

(3.82)

G

The equality (≡ 0) of the above equation is proved by using (3.74) as follows,

(A G ∇k A∗G

+

A∗G ∇k A G

= ∇k

G

|A G |

2

= ∇k (1) ≡ 0.

(3.83)

G

∗ On the other hand, operating ∇k on both sides of (3.80) and multiplying A G (k) from the left, then the summing up with respect to G results in

2 2 (k + G)|A G |2 + (k + G)2 A∗G ∇k A G 2m G 2m G +Ω V (G − G)A∗G ∇k A G G

=

G

|A G |2 ∇k E(k) + E(k)

G

A∗G ∇k A G .

(3.84)

G

In a similar fashion we operate ∇k on both sides of (3.81) and multiply G A G . Then we sum up left hand sides and right hand sides of the derived two equations separately, we obtain the following equation 2 2 (k + G)|A G |2 + (k + G)2 ∇k (A∗G A G ) m G 2m G V (G − G)(A G ∇k A G + A G ∇k A∗G ) +Ω =2

G

G

G

|A G |2 ∇k E(k) + E(k)

∇k (A∗G A G ) ≡ 2∇k E(k).

(3.85)

G

The sum of the second and third terms of the left hand side results in 0 from the relation of (3.82). Therefore (3.85) reduces to 2 (k + G)|A G (k)|2 = ∇k E(k). 2m G Using above result in (3.76), we obtain the following relations

(3.86)

150

3 Wannier Function and Effective Mass Approximation

k|v|k =

1 ∇k E(k),

(3.87a)

or for the matrix element of momentum operator p = mv k| p|k =

m ∇k E(k).

(3.87b)

The result means that the expectation value of the electron velocity in periodic potential is given by the gradient of electron energy E(k) in a band. When we assume the expectation value of the electron velocity is equivalent to the group velocity, then the classical representation of (3.67) is verified.

3.5.2 Electron Motion Under an External Force Next we derive equation of electron motion in a crystal in the presence of an external force F. In classical mechanics a particle motion, or acceleration, is normally written as dp = F, (3.88) dt where p = mv is the momentum of a particle with the mass m and the velocity v. The most important case in this textbook is the electron motion in an electric field E, and thus the external force is written as F = −e E,

(3.89)

where −e is the electronic charge. We assume that a uniform electric field applied to a crystal is so week that no interband transition occurs and that the wave function of an electron is described by the following time-dependent Schrödinger equation with Hamiltonian H . ∂ (3.90) i Ψ (r, t) = (H − F · r)Ψ (r, t). ∂t Now we expand the wave function Ψ (r) by Bloch functions Ψk (r). Here we assumed the case where the electric field is so weak that no tunneling occurs, and 1 thus the electron moves in a specific energy band. Also we assume a continuous function with respect to k and the summation k is replaced by integration. Then we obtain ak (t)Ψk (r) = α(k, t)Ψk (r)d3 k. (3.91) Ψ (k, t) = k

In a general case (3.91) is defined by replacing α(k, t) with index.

1

n

αn (k, t), where n in the band

3.5 Electron Motion Under an External Field

151

Inserting (3.91) into (3.90), and using the relation H Ψ (r) = E(k)Ψ (r), we obtain i

α(k, ˙ t)Ψk (r)d3 k = α(k, t)E(k)Ψk (r)d3 k − α(k, t)(F · r)Ψk (r)d3 k.

(3.92)

Multiplying the above equation by Ψk∗ (r), integrating in the unit cell, and using orthonormality relation of the Bloch function Ψk (r), we obtain the following relation. iα(k, ˙ t) = α(k, t)E(k) −

α(k, t)F ·

Ψk∗ (r)rΨk (r)d3 rd3 k.

(3.93)

Here we perform the spatial integration of the second term on the right hand side of (3.93). Using the Bloch function Ψk (r) = eik·r u k (r), the spatial integration reduces to ∗ 3 X = Ψk (r)rΨk (r)d r = e−ik ·r u ∗k reik·r u k (r)d3 r =i ∇k e−ik ·r u ∗k (r)eik·r u k (r)d3 r =i ∇k e−ik ·r u ∗k (r) − e−ik ·r ∇k u ∗k (r) eik·r u k (r)d3 r = i∇k δk,k − iδk,k u k (r)∇k u ∗k (r)d3 r. (3.94) Inserting this into (3.93), we obtain iα(k, ˙ t) = α(k, t)E(k) −

α(k, t)F · Xd3 k

= α(k, t)E(k) − iF · ∇k α(k, t) +iα(k, t) (F · ∇k u ∗k (r))u k (r)d3 r.

(3.95)

Complex conjugate of this equation is given by − iα˙ ∗ (k, t) = α∗ (k, t)E(k) + iF · ∇k α∗ (k, t) −iα∗ (k, t) (F · ∇k u k (r))u ∗k (r)d3 r.

(3.96)

Multiplying (3.95) by α∗ (k, t) and (3.96) by −α(k, t), then summation of each sides results in

152

3 Wannier Function and Effective Mass Approximation

i

∂ |α(k, t)|2 = −iF · ∇k |α(k, t)|2 ∂t +i|α(k, t)|2 F · u k (r)∇k u ∗k (r) + u ∗k (r)∇k u k (r) d3 r.

(3.97)

Here we find that the second term of the right side gives rise to 0 as shown below. Normalization of the Bloch function is given by

Ψk∗ (r)Ψk (r)d3 r

=

u ∗k (r)u k (r)d3 r = 1.

(3.98)

Differentiating this equation with respect to k and we obtain

(u k (r)∇k u ∗k (r) + u ∗k (r)∇k u k (r)d3 r = 0.

(3.99)

This result reveals that the second term of the right side of (3.97) becomes 0. Therefore, (3.97) results in or

∂ |α(k, t)|2 = −F · ∇k |α(k, t)|2 , ∂t

∂ + ∂t

F · ∇k

(3.100)

|α(k, t)|2 = 0.

(3.101)

A general solution of the above equation is given by an arbitrary function G with k and t, 1 (3.102) |α(k, t)|2 = G(k − Ft). Here α(k, t) is the expansion coefficient of the wave function as given by (3.91) and thus |α(k, t)|2 represents the probability of electrons in the state k at time t. Therefore we choose a function G to exhibit a maximum at time t = 0 and k = k0 . If the function has a maximum at time Δt and at k and no scattering occurs, we obtain the following relation.2 G(k0 ) = G(k −

1 FΔt).

(3.103)

Therefore we obtain the relation k0 = k − FΔt/, and thus Δk = k − k0 = 2

1 FΔt,

(3.104)

This assumption is based on the fact that the function G will stay un–changed without scattering and thus the maximum value of G is not changed with time t. Scattering induces a change in the wave function and the maximum value will stay constant before the next scattering.

3.5 Electron Motion Under an External Field

153

In other word, we obtain the following relation

dk = F(= −e E), dt

(3.105)

and (3.88) is proved. In general, when there exist no scattering events, the electron wave vector k at time t changes from the initial state k0 at time 0 according to k = k0 +

1 Ft.

(3.106)

In this case the state k should be empty because of Pauli exclusionprinciple. When we include interband transition, |α(k, t)|2 should be replaced by |αn (k, t)|2 and then (3.102) is valid. In the case of interband transition, the wave vector after the transition should be equal to k given by (3.102). In the calculation of electrical conduction, we can neglect such an interband transition because the energy of an electron is smaller than the band gap energy. If the electron scattering by phonons exists, we have to take account of momentum and energy conservation, which will be discussed in Chap. 6.

3.5.3 Electron Motion and Effective Mass We have already learned that the electronic states are given by the relation of electron energy as a function of electron wave vector, E(k). In the above subsections we find that an external force induces a change in the electron wave vector k, and thus in the electron energy according the relation E(k). In order to deal with electron transport, therefore, we have to know the energy band. The electron distribution is governed by Fermi-Dirac distribution function and electrons in semiconductors in the thermal equilibrium occupy the states near the conduction band minimum. Such electrons are well described by the relation E(k) = 2 k 2 /2m ∗ , where m ∗ is called the effective mass. Here we will show that the effective mass approximation is valid for the description of electron transport. First, we summarize the results obtained in the above two subsections. The expectation value of the electron velocity or the electron group velocity is given by (3.67) v ≡ v g =

1 dE , dk

(3.107)

and an external force F produces a change in the wave vector of the electron as

dk = F(= −e E). dt

(3.108)

154

3 Wannier Function and Effective Mass Approximation

The time derivative of (3.107) is given by dv 1 d dE = dt dt dk

(3.109)

Since the acceleration of the electron in the external force is governed by (3.108), and the electron energy is given by a function of the wave vector as E(k), the right hand side of the above equation is rewritten as dv 1 d dE 1 dk d2 E . = = dt dt dk dt dk2

(3.110)

Inserting (3.108) into (3.110), we obtain 1 d2 E dv = 2 2 F. dt dk

(3.111)

This relation should be compared with Newton’s law of motion of a particle with the velocity v and the mass m, 1 dv = F. (3.112) dt m Comparing (3.111) with (3.112), we may write (3.111) as dv 1 = ∗ F, dt m 1 1 d2 E = 2 2, m∗ dk

(3.113) (3.114)

where m ∗ is equivalent to a particle mass and called as the effective mass. In general the inverse effective mass 1/m ∗ is defined as

1 m∗

= ij

1 d2 E . 2 dki dk j

(3.115)

Since we are interested in the electrons near the band edge (conduction band minimum Ec ), the energy band is well approximated by parabolic function of the electron wave vector k 2 2 E= k + Ec . (3.116) 2m ∗ This relation is easily derived from (3.114) by carrying out integration with respect to k. We have already used this relation to develop the effective mass approximation. From these considerations we conclude that the effective mass defined by (3.114) can be used to evaluate transport properties of electrons in the form of classical mechanics.

References

155

3.6 Problems (3.1)

Effective mass equation is derived in different ways. The other method not dealt with this textbook is given by Luttinger and Kohn. See the following paper for the derivation of the effective mass equation used for analysis of shallow impurity states and of the cyclotron resonance: Joaquin M. Luttinger and Walter Kohn. “Motion of electrons and holes in perturbed periodic fields.” Phys. Rev. 97 (1955) 869–883.

(3.2)

An electron with its effective mass m ∗ is put in a magnetic field B applied in z direction. (1) Solve the cyclotron motion of the electron and show its angular frequency is give by ωc = eB/m ∗ . (2) Calculate its cyclotron radius Rc . (3) Apply Bohr’s quantization condition pdl = h to the orbital motion, where p = m ∗ v with the velocity v of the orbital motion. Then show this condition leads to the cyclotron radius obtained by solving Schrödinger equation.

References 1. 2. 3. 4. 5. 6.

G. Wannier, Phys. Rev. 52, 869 (137) J.M. Luttinger, W. Kohn, Phys. Rev. 97, 869 (1955) W. Kohn, J.M. Luttinger, Phys. Rev. 97, 1721 (1955) C. Kittel, A.H. Mitchell, Phys. Rev. 96, 1488 (1954) W. Kohn, J.M. Luttinger, Phys. Rev. 98, 915 (1955) W. Kohn, in Solid State Physics, ed. by F. Seitz, D. Turnbull, vol. 5 (Academic Press, New York, 1957) pp. 257–320 7. D.K. Wilson, Feher, Phys. Rev. 124, 1068 (1961) 8. R.A. Faulkner, Phys. Rev. 184, 713 (1969) 9. R.L. Aggarwal, A.K. Ramdas, Phys. Rev. 140, A1246 (1965)

Chapter 4

Optical Properties 1

Abstract This chapter deals with fundamental theory of optical properties in semiconductors. First, reflection and absorption coefficients are derived by using Maxwell’s equations. Then quantum mechanical derivations of direct and indirect optical transition rates are given in addition to the classification of the joint density of states. Optical transitions associated with electron–hole pair, exciton, are also discussed. Dielectric functions are discussed in connection with the critical points of semiconductors. Also we will discuss stress effect on the optical transition such as piezobirefringence and stress–induced change in the energy band structure. The results are used in Chap. 9 to evaluate the strain effect in quantum well lasers. Readers are recommended to refer textbooks and review papers [1–4].

4.1 Reflection and Absorption The classical theory of electromagnetic waves is described by Maxwell’s equations. Let us define the electric field E, electric displacement D, magnetic field intensity vector H, magnetic field flux (referred to as “magnetic field” in this text) B, current density J, and charge density ρ; then the macroscopic domain is governed by the classical field equations of Maxwell: ∇×E=−

∂B , ∂t

∇ × H = J = σE +

(4.1a) ∂D , ∂t

(4.1b)

∇ · D = ρ,

(4.1c)

∇ · B = 0.

(4.1d)

In the case of a material with a complex dielectric constant κ = κ1 + iκ2

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2023 C. Hamaguchi, Basic Semiconductor Physics, Graduate Texts in Physics, https://doi.org/10.1007/978-3-031-25511-3_4

(4.2)

157

158

4 Optical Properties 1

we obtain D = κ0 E.

(4.3)

In the following we assume that there exists no excess charge in the domain we are interested in. Then we obtain the following relations from Maxwell’s equations. For simplicity we assume that there is no charge to induce the current, i.e. σ = 0. When charge carriers exist, the following results may be modified by introducing the complex conductivity as described by (4.24), (4.25a) and (4.25b), and also as discussed in Sect. 5.5. ∂ (∇ × B), ∂t ∂D ∂ = −μ0 σE + , ∂t ∂t

∇×∇× E = −

= −μ0 κ0

∂2 E, ∂t 2

(4.4)

Since there is no excess charge, we put ρ = 0 and find the following result: ∇ × ∇ × E = ∇(∇ · E) − ∇ 2 E, ∇ · E = 0, ∇ 2 E = μ0 0 κ

∂2 E , ∂t 2

(4.5)

Let us assume a plane wave for the electromagnetic field E ∼ E exp[i(k · r − ωt)].

(4.6)

Inserting this into (4.5) we obtain (ik)2 = (−iω)2 μ0 0 κ.

(4.7)

The phase velocity of the electromagnetic wave is then given by ω 1 c =√ √ = √ = c , k κ 0 μ0 κ

(4.8)

where c is the velocity of light in vacuum (κ = 1) 1 ∼ c= √ = 3.0 × 108 m/s 0 μ0 and c is the velocity of light in a material with dielectric constant κ

(4.9)

4.1 Reflection and Absorption

159

c c c = √ = . n κ

(4.10)

√ In the above equation we have used the definition of the refractive index n = κ. Since we have defined the dielectric constant by a complex number, we have to introduce a complex refractive index. Let us assume that the electromagnetic wave propagates in the z direction with electric field amplitude E ⊥ : k z−t E(z, t) = E ⊥ exp[i(kz − ωt)] = E ⊥ exp iω ω √ κ = E ⊥ exp iω z−t . c

(4.11)

We also define the incident, reflected and transmitted electric fields of the electromagnetic field at the boundary shown in Fig. 4.1 by 1 E i exp iω z − t , c 1 E r exp iω − z − t , c √ κ E t exp iω z−t . c Since we assume that there is no excess charge at the boundary, the electric field and its gradient are required to be continuous at z. The reflection coefficient r (E r = r E i ) and the transmission coefficient t (E t = t E i ) have to satisfy the following relations. 1 =r +t

√ √ 1 = −r + t κ = −r + (1 − r ) κ.

Fig. 4.1 Schematic illustration of incident, reflected, and transmitted electromagnetic waves (light) at the boundary of a material surface in the air

(4.12a) (4.12b)

160

4 Optical Properties 1

From these relations we obtain the reflection coefficient √ κ−1 r=√ . κ+1

(4.13)

When we define complex refractive index n ∗ by

or

√ κ = n ∗ ≡ n 0 + ik0 ,

(4.14)

κ1 + iκ2 = n 0 + ik0 ,

(4.15)

then we may express the real and imaginary parts of the complex dielectric constant by κ1 = n 20 − k02 , κ2 = 2n 0 k0 ,

(4.16a) (4.16b)

where n 0 and k0 are called the refractive index and the extinction coefficient, respectively. From these relations, the amplitude reflection coefficient is given by r=

2k0 n 0 − 1 + ik0 . = |r | tan θ, tan θ = 2 n 0 + 1 + ik0 n 0 + k02 − 1

(4.17)

The reflection coefficient is generally defined as the power reflection coefficient (the reflection coefficient for the incident energy), and thus we have to calculate the reflection coefficient for E 2 , H 2 or the Poynting vector E × H, which is given by R = |r |2 = =

(n 0 − 1)2 + k02 (n 0 + 1)2 + k02

(κ21 + κ22 )1/2 − [2κ1 + 2(κ21 + κ22 )1/2 ]1/2 + 1 . (κ21 + κ22 )1/2 + [2κ1 + 2(κ21 + κ22 )1/2 ]1/2 + 1

(4.18)

Inserting (4.14) into (4.11), √ κ n 0 + ik0 E(z, t) = E ⊥ exp iω z−t = E ⊥ exp iω z−t c c n0 ωk0 z exp iω z−t (4.19) = E ⊥ exp − c c is obtained and the attenuation of the electric power or the Poynting vector of the electromagnetic waves is written as

4.1 Reflection and Absorption

161

ωk0 z ≡ E ⊥2 exp(−αz), I ∝ E 2 ∝ E ⊥2 exp −2 c where α=2

ωk0 ωκ2 = c n0c

(4.20)

(4.21)

is called the absorption coefficient which gives rise to an attenuation of the incident power by 1/e 1/2.7 0.37 per unit propagation length. Next we discuss the relation of the complex conductivity and the complex dielectric constant to the power dissipation (power loss) per unit volume of a material, which is exactly the same as the dielectric loss. Using the complex dielectric coefficient in the electric displacement in (4.1b), it is rewritten as D = κ0 E = (κ1 + iκ2 )0 E.

(4.22)

Since we assume a plane wave for the electromagnetic wave, we may put ∂/∂t → −iω and then the current density is given by J = σE +

∂D = σ E − iω(κ1 + iκ2 )0 E ≡ σ ∗ E. ∂t

(4.23)

When we write the complex conductivity σ ∗ as σ ∗ = σr + iσi

(4.24)

we find the following relations between the complex conductivity and the complex dielectric constant: σr = σ + ωκ2 0 , σi = −ωκ1 0 .

(4.25a) (4.25b)

It is well known that the power loss is given by w = σr E 2 /2 and thus the power loss per unit volume of a dielectric with κ = κ1 + iκ2 is written as w=

1 ωκ2 0 E 2 , 2

(4.26)

which is known as the “dielectric loss.” This relation holds exactly for light absorption in a material and is used later to relate optical transitions and light absorption. In the case of semiconductors where free carriers exist, the real part of the complex dielectric constant κ1 is related to the imaginary part of the complex conductivity by κ1 = κl −

σi , ω0

(4.27)

162

4 Optical Properties 1

where κ1 is the real part of the dielectric constant due to the crystal lattices and we may expect κ1 to become zero at a specific frequency (plasma frequency). This relation is often used to discuss the classical theory of plasma oscillation (see Sects. 5.4.1 and 5.5).

4.2 Direct Transition and Absorption Coefficient In this Section we will consider the band-to-band direct transition of an electron from the valence band to the conduction band induced by the incident light. To do this we consider the electron motion induced by the incident light in a perfect crystal. The Hamiltonian of the electron is given by H=

1 ( p + e A)2 + V (r), 2m

(4.28)

where A is the vector potential of the electromagnetic filed and V (r) is the periodic potential of the crystal. The vector potential is expressed by the plane wave: A=

1 A0 e ei(kp ·r−ωt) + e−i(kp ·r−ωt) , 2

(4.29)

where kp and e are the wave vector of the electromagnetic field and its unit vector (polarization vector), respectively. In the above equation the vector potential is expressed as a real number by adding its complex conjugate. Using the relation A · p = p · A and neglecting the small term A2 , the Hamiltonian is rewritten as H

e p2 + V (r) + A · p ≡ H0 + H1 . 2m m

(4.30)

Assuming H1 = (e/m) A · p as the perturbation, the transition probability per unit time wcv for the electron from the initial state |vk to the final state |ck is calculated to be 2π e | ck | A · p|vk|2 δ E c (k ) − Ev (k) − ω m 2 πe2 2 = A0 ck | exp(ikp · r)e · p|vk 2 2m ×δ Ec (k ) − Ev (k) − ω .

wcv =

(4.31)

The matrix element of the term which includes the momentum operator p is called the matrix element of the transition and gives the selection rule and the strength of the transition. Let us consider the Bloch function to express the electron state:

4.2 Direct Transition and Absorption Coefficient

| j k = eik·r u j k (r),

163

(4.32)

where j = v and c represents the valence band and conduction band states, respectively. Then the matrix element of the transition is given by

1 e−ik ·r u ∗ck (r)eikp ·r e · peik·r u vk (r)d3 r V V

1 ei(kp +k−k )·r u ∗ck (r)e · ( p + k)u vk (r)d3 r. = V V

e · pcv =

(4.33)

From the property of the Bloch function, u(r) = u(r + Rl ), where Rl is the translation vector, and the matrix element is rewritten as e · pcv =

1 exp{i(kp + k − k ) · Rl } V l

× ei(kp +k−k )·r u ∗ck (r)e · ( p + k)u vk (r)d3 r,

(4.34)

Ω

where Ω is the volume of the unit cell. Summation with respect to Rl becomes 0 except for (4.35) kp + k − k = G m (= m G), where G m is the reciprocal lattice vector (G is the smallest reciprocal lattice vector and m is an integer). The wave vector of light (electromagnetic waves) with a wavelength of 1 µm is |kp | = 6.28 × 104 cm−1 and the magnitude of the reciprocal lattice vector for a crystal with a lattice constant of 5 Å is |G| = 1.06 × 108 cm−1 , and thus the inequality kp G is fulfilled in general. Therefore, the largest contribution to the integral in (4.34) is due to the term for G m = 0 (m = 0). This condition may be understood to be equivalent to the conservation of momentum. From these considerations (4.35) leads to the important relation k = k

(4.36)

for the optical transition. That is, electron transitions are allowed between states with the same wave vector k in k space. In other words, when a photon of energy greater than the band gap is incident on a semiconductor, an electron with wave vector k in the valence band is excited into a state with the same wave vector in the conduction band. From this fact the transition is referred to as a direct transition. Since the integral with respect to k in (4.34) vanishes because of the orthogonality of the Bloch functions, we obtain

1 u ∗ (r)e · pu vk (r)d3 rδk,k . (4.37) e · pcv = Ω Ω ck

164

4 Optical Properties 1

Using the above results, the photon energy absorbed in the material per unit time and unit volume is given by ωwcv , which is equivalent to the power dissipation of the electromagnetic waves per unit time and unit volume given by (4.26): ωwcv =

1 ωκ2 0 E 02 . 2

(4.38)

From the relation between the electric field and the vector potential, E = −∂ A/∂t, we may put E 0 = ω A0 ; thus the imaginary part of the dielectric constant is given by the equation 2 ωcv 0 ω 2 A20 2 πe2 e · pcv δ Ec (k ) − Ev (k) − ω δkk . = 0 m 2 ω 2

κ2 =

(4.39)

k,k

It is evident that the absorption coefficient is obtained by inserting κ2 into (4.21).

4.3 Joint Density of States In the previous section we derived the dielectric function for the direct transition, which is given by (4.39). When we assume that the matrix element e · pcv varies very slowly as k or is independent of k (this is a good approximation), the term |e · pcv |2 in (4.39) may be moved out of the summation. The imaginary part of the dielectric constant can then be rewritten as κ2 (ω) =

πe2 |e · pcv |2 δ[Ecv (k) − ω], 2 2 0 m ω

(4.40)

k

Ecv (k) = Ec (k) − Ev (k).

(4.41)

The summation with respect to k in (4.40) may be understood as the summation of the pair states of |vk and |ck due to the delta function and called the joint density of states. Replacing the summation by an integral in k space, the joint density of states Jcv (ω) is written as

2 Jcv (ω) = δ[Ecv (k) − ω] = (4.42) d3 k · δ[Ecv (k) − ω], (2π)3 k

where the spin degeneracy factor 2 is taken into account. Integration of the above equation is carried out by the following general method. Consider two constant energy surfaces in k space, E = ω and ω + d(ω). The density of states in d(ω) is then obtained as follows.

4.3 Joint Density of States

165

Fig. 4.2 Derivation of the general form of the joint density of states. Consider two constant energy surfaces E and E + δ E displaced by δ E . The small element of volume in k space is then defined by the product of the bottom area δS and the distance δk⊥ perpendicular to the constant energy surface

Jcv (ω) · d(ω) =

2 (2π)3

dS · d(ω). |∇k Ecv (k)|

ω=Ecv

(4.43)

Therefore, the joint density of states Jcv (ω) is rewritten as Jcv (ω) =

2 (2π)3

dS , |∇k Ecv (k)|

ω=Ecv

(4.44)

where we have to note that the integral is carried out over the constant energy surface, ω = Ecv (k), because of the delta function. This general form of the density of states is derived as follows. Referring to Fig. 4.2, let us consider constant energy surfaces displaced by a small amount of energy δE in k space, E and E + δE. The small element of the volume δV (k) in k space is defined by the volume contained in the bottom area δS and its height δk⊥ between the two constant energy surfaces. The states allowed in a volume element d3 k in k space per unit volume is given by 2 2 d3 k = δV (k). (4.45) (2π)3 (2π)3 The distance between the constant energy surfaces is given by (∂k⊥ /∂E)δE = (∂E/∂k⊥ )−1 δE, where ∂E/∂k⊥ is the gradient of E in the direction normal to the energy surfaces and we find ∂E = |∇k E| = ∂k⊥

∂E ∂k x

2

or δk⊥ =

+

∂E ∂k y

δE . |∇k E|

2

+

∂E ∂k z

2 ,

(4.46)

(4.47)

From the definition of the volume element δV (k) = δS · δk⊥ , the density of states in energy space between E and E + δE is given by

166

4 Optical Properties 1

ρ(E)dE =

2 (2π)3

S

dS dE. |∇k E|

(4.48)

It is evident from the above derivation that the joint density of states is obtained by replacing E(k) by Ecv (k) in the above equation and thus that the derivation of (4.44) is straightforward. The joint density of states Jcv (ω) given by (4.44) diverges when ∇k Ecv (k) = 0 is satisfied. This leads to a maximum probability for the optical transition. We may expect such behavior at various points in the Brillouin zone. Such a point in the Brillouin zone is called a critical point or singularity of the joint density of states. The behavior may be expected to occur under the following two conditions: ∇k Ec (k) = ∇k Ev (k) = 0,

(4.49)

∇k Ec (k) = ∇k Ev (k) = 0.

(4.50)

These equations reflect the conditions that the slopes of the two bands are parallel. The former condition means that the slopes are horizontal and will be satisfied at points of Brillouin zone with high symmetry. For example, this condition is satisfied at the Γ point. The second condition is satisfied at various points of Brillouin zone. The critical points behave differently depending on the type of critical point. The properties of the critical points were first investigated by van Hove [5] and thus are called van Hove singularities. In order to discuss the singularities in more detail we expand Ecv (k) at the point ∇k (k) = 0 (k = k0 , Ecv = EG ) in a Taylor series and keep terms up to the second order: 3 2 Ecv = EG + (ki − ki0 )2 , (4.51) 2μ i i=1 where the first-order term of k disappears due to the singularity condition ∇k Ecv = 0. The constant μi has the dimension of mass and is given by the following equation with the effective mass m ∗e of the conduction band and m ∗h of the valence band. 1 1 1 = ∗ + ∗ . μi m e,i m h,i

(4.52)

The mass μi is called the reduced mass of the electron and hole. Using this result, the joint density of states Jcv at the critical point is then calculated in the following way. Defining the new variable si =

(ki − ki0 ) , √ 2|μi |

(4.53)

4.3 Joint Density of States

167

Equation (4.51) is rewritten as Ecv (s) = EG +

3

αi si2 ,

(4.54)

i=1

where αi = ±1 is the sign of μi , and αi = +1 for μi > 0 and αi = −1 for μi < 0. Using the definition of the variable we may calculate the joint density of states given by (4.44) (for the M0 critical point: αi > 0 for all αi ) as 2 Jcv (ω) = (2π)3 2 = (2π)3

8|μ1 μ2 μ3 | 6 8|μ1 μ2 μ3 | 6

1/2

Ecv =ω

dS |∇s Ecv (s)|

Ecv =ω

dS , 2s

1/2

(4.55)

where s = (s12 + s22 + s32 )1/2 . It is straightforward to obtain the density of states for point. In this case we have Ecv − EG = s12 + s22 + s32 = s 2 and then the M0 critical we obtain dS = 4πs 2 for ω > EG , which leads to the following result for the joint density of states Jcv (ω): Jcv (ω) =

⎧ ⎨0 4π ⎩ (2π)3

8μ1 μ2 μ3 6

1/2

; ω ≤ EG √ ω − EG ; ω ≥ EG .

(4.56)

It is evident from (4.51) or (4.54) that the singularities or critical points are classified in four categories depending on the combination of the signs of the reduced masses, or in other words we define the critical point M j ( j = 0, 1, 2 and 3) by j, the number of negative μi . The critical point M0 has 3 positive reduced masses ( j = 0: zero negative reduced mass): μ1 > 0, μ2 > 0 and μ3 > 0. The critical points M1 , M2 and M3 are for 1, 2, and 3 negative reduced masses, any of μ1 , μ2 and μ3 . The joint density of states Jcv (ω) for the critical points M1 , M2 and M3 have been calculated and the results are summarized in Table 4.1 (see for example [6, 7]). Inserting (4.56) into (4.39) the imaginary part of the dielectric constant for the M0 critical point is given by e2 κ2 (ω) = |e · pcv |2 2π0 m 2 ω 2

8μ1 μ2 μ3 6

1/2

ω − EG ,

(4.57)

where ω > EG . The absorption coefficient is obtained by inserting this equation for κ2 (ω) into (4.21): e2 |e · pcv |2 α(ω) = 2π0 m 2 cn 0 ω

8μ1 μ2 μ3 6

1/2

ω − EG for ω > EG .

(4.58)

168

4 Optical Properties 1

Table 4.1 Joint density of states Jcv (ω) for 3–dimensional critical points Types of critical points Jcv (ω) μ1 μ2 + + − + − − − − 1/2 8μ1 μ2 μ3 4π C1 = (2π)3 6 Types M0 M1 M2 M3

μ3 + + + −

ω ≤ EG 0 C2 − C1 (EG − ω)1/2 C2 C1 (EG − ω)1/2

ω ≥ EG C1 (ω − EG )1/2 C2 C2 − C1 (ω − EG )1/2 0

Fig. 4.3 Joint density of states Jcv (ω) for a 3D, b 2D and c 1D bands

It is also evident from (4.51) that Ecv becomes a maximum at k0 for the M0 critical point (all of μi are positive) and that Ecv becomes a minimum at k0 for the M3 critical point (all of μi are negative). On the other hand, the M1 (M2 ) critical point exhibits a saddle point at k0 , where Ecv shows a maximum (minimum) at k0 in one direction and a minimum (maximum) in other directions. When we consider a pair of conduction and valence bands, the lowest energy critical point is M0 and the highest energy critical point is M3 . It should be noted that Fig. 4.3a is calculated by using the relations given in Table 4.1 for 3D case. We will present an example of the calculations of DOS (Density of states) for the 3D energy bands obtained by a simple treatment of the tight-binding approximation in the case of the simple cubic lattice. The first Brillouin zone is determined by the reciprocal lattice vectors G x = G y = G z = ±2π/a and thus the zone edge wave vectors are k x = k y = k z = ±π/a. The energy bands are then given by Ecv (k) = (EG + 3γ) − γ cos(ak x ) + cos(ak y ) + cos(ak z )

(4.59)

The energy band E(k x ) is shown in Fig. 4.4a. The density of states (DOS) of the energy band is obtained by discretizing the first Brillouin zone as described in Chap. 1, Sect. 1.8, and the results are shown in Fig. 4.4b, where we see M0 M1 M2 and M3 critical points. The joint densities of states Jcv for 2–dimensional (2D) and 1–dimensional (1D) bands are summarized in Table 4.2 and in Fig. 4.3b, c. It is very important to point

4.4 Indirect Transition

169

Fig. 4.4 Energy band and its density of states. a Energy bad structure obtained by the tight–binding approximation (4.59) for a simple cubic lattice. b Density of states (DOS) obtained by numerical calculations from (4.59), where all the four critical points M0 , M1 , M2 , and M3 are clearly seen Table 4.2 Joint density of states Jcv (ω) for 1–dimensional and 2–dimensional critical points Types of critical points

Jcv (ω)

Dimension

Types

ω ≤ EG

ω ≥ EG

1D

M0

0

A(ω − EG )−1/2 − ω)−1/2

1D

M1

A(EG

2D

M0

0

B1

2D

M1

(B1 /π)(B2 − ln |EG − ω|)

(B1 /π)(B2 − ln |EG − ω|)

2D 2 A= · 4π

2|μ| 1/2 , 2

M2 2 B1 = · 4π

B1 4|μ1 μ2 | 1/2 , 4

0

0 B2 = ln |2B3 − (EG − ω) + 2 B32 − (EG − ω)B3 |

out that in Fig. 4.3b, c the joint densities of states Jcv at the saddle point for the 2D critical point and at the 1D critical points diverge. The behavior of the 1D critical point has already been shown in Chap. 2 to describe the density of states in a high magnetic field, where an electron is quantized in the perpendicular direction to the magnetic field and the electron can move along the magnetic field, and thus the electron behaves like a 1D carrier.

4.4 Indirect Transition In Sects. 4.1 and 4.2 we considered the process where an electron in the valence band absorbs one photon and makes a transition to the conduction band vertically in k space, i.e. a direct transition. This process plays the most important role in direct gap semiconductors such as GaAs, InSb and so on. On the other hand, we have shown in Chaps. 1 and 2 that the conduction band minima in Ge and Si are located at the L point and Δ point, respectively, whereas the top of the valence band at the Γ

170

4 Optical Properties 1

point. Therefore, the fundamental absorption edge (lowest optical transition) is not direct, and thus direct transitions of electrons from the top of the valence band to the lowest conduction band minima is not allowed. Experimental results in Ge and Si reveal a weak transition for the photon energy corresponding to the indirect band gap between the top of the valence band at k = 0 and the conduction minima at k = 0. This process is interpreted as the indirect transition in which an electron in the valence band absorbs a photon and then absorbs or emits a phonon to make the transition to the conduction band minima. This process is caused by a higher-order interaction or second-order perturbation in quantum mechanics, as described below in detail. The higher-order perturbation produces a weaker transition probability compared with the direct transition, and thus the weak absorption is explained. In addition we have to note that the transition is validated through a virtual state for the transition from the initial to the final states, and for this reason the transition is called an indirect transition. Let us define the Hamiltonian He for electrons, Hl for lattice vibrations, Hel for the electron–phonon interaction and Her for the electron-radiation (photon) interaction. Then the total Hamiltonian is written as H = He + Hl + Hel + Her .

(4.60)

We will discuss the Hamiltonian of the lattice vibrations and the electron–phonon interaction in Chap. 6 and will not go into detail here. The Hamiltonian of electrons and phonons is written as H0 = He + Hl and the eigenstates are expressed as | j =

|ck, n αq (for an electron in the conduction band) |vk, n αq (for an electron in the valence band)

,

(4.61)

where k is the wave vector of the electron and n αq is the phonon quantum number of mode α and wave vector q. Expressing the perturbation Hamiltonian as H = Hel + Her

(4.62)

and keeping the perturbation up to the second order, the transition probability from an initial state |i to a final state | f through a virtual state |m is then given by f |H |m m|H |i 2 2π δ(Ei − E f ), f |H |i + wif = E − E i m m

(4.63)

where it is evident that the relation f |H |i = f |Her |i + f |Hel |i = 0 holds because of the following reasons. The matrix element f |Her |i is the same as the element for the direct transition stated in the previous section and the transition is allowed between the same k vectors in k space. In the case of an indirect transition, however, the wave vectors k are different between the initial state |i at the top of the valence band and the final state | f at the bottom of the conduction band, and thus

4.4 Indirect Transition

171

Fig. 4.5 Processes for the indirect transition. (1) An electron at the top of the valence band A interacts with radiation to absorb a photon and makes a transition to a virtual state D in the conduction band, followed by a transition by phonon absorption or emission to the final state C. (2) An electron makes a transition from the top of the valence band A to a virtual state in the valence band B by absorbing or emitting a phonon and then absorbs a photon to end up at the final state C

we find that f |Her |i = 0. On the other hand, the matrix element f |Hel |i ensures momentum conservation (wave vector conservation), δ(ki ± q − k f ), but energy is not conserved because of the small value of the phonon energy compared with the band gap. Therefore, we find that f |Hel |i = 0. From these considerations only the second term in (4.63) will contribute to the indirect transition and so finally we get wif =

2π f |H |m m|H |i 2 δ(Ei − E f ). m Ei − Em

(4.64)

When we insert (4.62) into (4.64), such terms as f |Hel |m m|Hel |i, f |Her |m m|Her |i and so on appear. However, these terms will not contribute to the indirect transition for the reason stated above. Finally, we find that the two processes shown in Fig. 4.5 will remain. The first process is: (1) an electron at the top of the valence band A interacts with radiation to absorb a photon and makes a transition to a virtual state D in the conduction band, followed by a transition by phonon absorption or emission to the final state C. The second process is: (2) an electron makes a transition from the top of the valence band A to a virtual state in the valence band B by absorbing or emitting a phonon and then absorbs a photon to end up at the final state C. The second process can be understood in a different way: an electron in the valence band B absorbs a photon, leaving a virtual state of a hole there and making a transition to the final state C, and an electron at the top of the valence band A is then transferred to this virtual state by absorbing or emitting a phonon. These processes are expressed by the following equation:

172

4 Optical Properties 1

wif =

2π Ck f , n αq ± 1|Hel |Dki , n αq Dki , n αq |Her |Aki , n αq Ei − E D +

Ck f , n αq ± 1|Her |Bk f , n αq ± 1 Bk f , n αq ± 1|Hel |Aki , n αq 2 E −E i

B

×δ(Ei − E f ), where the upper sign (+) of ± represents phonon emission and the lower sign (−) of ± corresponds to phonon absorption. When we neglect the phonon energy term ωq because of its smallness compared to the photon energy or the band gap, we find following relations: k f = ki ∓ q, Ei − E f = Ev (ki ) + ω ∓ ωqα − Ec (k f ), Ei − ED = Ev (ki ) + ω − ED (ki ) ∼ = Ec (k f ) − ED (ki ) ∼ = Ec0 − Ec1 , α ∼ Ev (ki ) − EB (k f ) = ∼ Ev0 − Ev1 . Ei − EB = Ev (ki ) ∓ ω − EB (k f ) = q

Assuming that the matrix element is independent of the wave vector k, we may approximate 2π m,α,± 2 M δ(Ei − E f ) (4.65) wif = m,α,± cv for the transition probability and κ2 (ω) =

πe2 m,α,± 2 M 0 m 2 ω 2 m,α,± cv × δ Ec (k ) − Ev (k) − ω ± ωqα k,k

(4.66)

for the imaginary part of the dielectric constant. The first summation is carried out for the virtual state (|m), the phonon mode, and its emission (+) and absorption (−). The probability of phonon emission and absorption is proportional to n αq + 1 and n αq , respectively, and the average excited phonon number is given by Bose–Einstein statistics as 1 . (4.67) n αq = exp(ωqα /kB T ) − 1 Using these results (4.65) may be written as 2π m,± 2 α 1 1 Acv nq + ± wif = m,α,± 2 2 × δ Ec (k ) − Ev (k) − ω ± ωqα . k,k

(4.68)

4.4 Indirect Transition

173

The second summation with respect to k and k represents the density of states for the indirect transition, which is calculated as follows. ind = δ Ec (k ) − Ev (k) − ω ± ωqα Jcv k,k

δ Ec0 − Ev0 +

k,k

+

k 2y k2 2 k x2 + + z 2 m hx m hy m hz

k 2y k2 k 2x + + z m ex m ey m ez

− ω ± ωqα ,

(4.69)

where the conduction band near the bottom is approximated by Ec (k ) = 2 k 2 /2m e + Ec0 with the electron effective mass m e and the valence band near the top by Ev (k) = −2 k 2 /2m h+ Ev0 with the hole effective mass m h . The summation k is replaced √ √ by 2/(2π)3 d3 k and transformations such as x = k x / 2m hx , x = k x / 2m ex etc. are used. Then the density of states is given by ind = Jcv

2K dxdydzdx dy dz (2π)6 2 2 2 ×δ x 2 + y 2 + z 2 + x + y + z + EG − ω ± ωqα ,

(4.70)

where we have assumed that the spin of the electron is not changed in the transition (no spin–flip transition) and that the spin degeneracy is used for one of the bands. In addition we have used K and EG given by K =

26 m hx m hy m hz m ex m ey m ez , 12 EG = Ec0 − Ev0 .

ind we use polar coordinates (x, y, z) = (r, θ, φ) In order to carry out the integral of Jcv with r 2 = s and r 2 = s ( sin θdθdφ = 4π), which leads to ind = Jcv

2K (2π)6

(4π)2

dsds √ ss δ(s + s + EG − ω ± ωqα ). 4

The integral of the above equation is easily carried out by using the δ function, and we obtain

ω∓ωqα −EG √ 4π 2 2K s ω ∓ ωqα − EG − s ds 6 (2π) 0 π 2K · (ω ∓ ωqα − EG )2 . = 4 (2π) 8

ind = Jcv

(4.71)

174

4 Optical Properties 1

Finally, we obtain the dielectric function for the indirect transition given by πe2 K m,α,± 2 M · (ω ∓ ωqα − EG )2 0 m 2 ω 2 (4π)3 m,α,± cv πe2 K m,α,+ 2 (ω − ωqα − EG )2 Acv = · · 0 m 2 ω 2 (4π)3 m,α 1 − exp(−ωqα /kB T ) m,α,− 2 (ω + ωqα − EG )2 + Acv · , exp(ωqα /kB T ) − 1

κ2 (ω) =

(4.72)

where the first and second terms on the right-hand side are associated with the transition followed by phonon emission and by phonon absorption, respectively. The virtual state of the indirect transition is determined by the phonon mode and its deformation potential and also by the selection rule for the electron–radiation field interaction. As the simplest case we take into account a virtual state and a phonon mode and calculate the temperature dependence of the absorption coefficient. The denominator of the second term becomes large for the case kB T ωqα and the transition followed by phonon absorption disappears at low temperatures. On the other hand, the denominator of the first term becomes 1 at low temperatures. Therefore, the indirect transition will be governed by phonon emission at low temperatures. The √ feature is shown in Fig. 4.6, where κ2 is plotted as a function of ω − EG for different temperatures, by taking into account the fact that the square root of the imaginary part of the dielectric function √ and thus of the absorption coefficient is proportional √ to ω ∓ ωq − EG ( κ2 ∝ α ∝ (ω ∓ ωq − EG ) (α: absorption coefficient). At lower temperatures the process of phonon absorption decreases and the absorption coefficient becomes very weak. We find that the phonon energy involved in the process is given by the half-width of the lower straight line and that the band gap EG lies in the middle of the line. The experimental results √ for Si are shown in Fig. 4.7, where the square root of the absorption coefficient α is plotted as a function of photon energy and find the feature of the indirect transition shown in Fig. 4.6 [8]. The turning point of the curve shifts to lower photon energy at higher temperatures, which is explained in terms of the temperature dependence of the band gap (the band gap decreases with increasing lattice temperature). The experimental results for Ge are shown in Fig. 4.8 [9], where turning points are observed in the spectrum for T = 249 K at about 0.65 and 0.71 eV. These turning points correspond to the transition due to the absorption and emission of one LO phonon, and the transition due to phonon emission disappears at low temperatures. A weak absorption is observed at T = 4.2 K below the photon energy around 0.77 eV due to LA phonon emission process, which is believed to be due to a forbidden transition followed by TA phonon emission. It is most important to point out here that the square root of the absorption coefficient is not a straight line but exhibits a hump. This is caused by exciton effects as discussed in Sect. 4.5.

4.5 Exciton

175

Fig. 4.6 Absorption coefficient at the indirect transition edge, where√the square √ root of the absorption coefficient α ∝ κ is plotted as a function of photon energy minus the band gap ω − EG for different temperatures

Fig. 4.7√ Square root of the absorption coefficient α plotted as a function of photon energy ω for Si, where the transitions due to phonon absorption and emission are well resolved (from [8])

Fig. 4.8 The √ square root of the absorption coefficient α of Ge at the indirect transition edge is plotted as a function of photon energy ω (from [9])

4.5 Exciton 4.5.1 Direct Exciton In Sect. 4.2 we discussed optical absorption spectra due to direct transitions, where an electron in the valence band (wave vector k) is excited by photon absorption into the conduction band (the wave vector at the band is k = ke ) and leaves a hole in the valence band (the wave vector of the hole is kh = −k). The two carriers are subject to the Coulomb interaction, which is disregarded in Sect. 4.2 and also in Sect. 4.4. In this section we will be concerned with the Coulomb interaction between electrons

176

4 Optical Properties 1

and holes at the critical point M0 , where we assume the bound state is very weak and thus the effective mass approximation is valid for the treatment. The bound state of the electron–hole pair is called an exciton. The exciton based on the approximation is called a Wannier exciton. When the electron–hole interaction is neglected, the wave function of the one electron and one hole system is given by Ψi j (r e , r h ) = ψi ke (r e )ψ j kh (r h ), where i and j are the band indices, and r e , r h , ke and kh are the coordinates and wave vectors of the electron and hole, respectively. In the absence of the Coulomb interaction the Hamiltonians of an electron in a conduction band, He , and an electron in a valence band, Hv , are written as1 He ψcke (r e ) = Ec (ke )ψcke (r e ), Hv ψvkv (r v ) = Ev (kv )ψvkv (r v ). In the following calculations we consider the Hamiltonian Hh for a hole in the valence band and use the Bloch function given by ψv,kh (r h ) = ψv,kv (r v ). As stated above, the crystal momentum vectors of an electron and a hole in the valence band have the same magnitude but different signs, and so we define the total wave vector of the electron–hole system by K = k + (−k) = ke + kh .

(4.73)

In the presence of the electron–hole interaction (Coulomb interaction) V (r e − r h ), the Hamiltonian for an exciton (electron-hole pair) is thus written as H = He + Hh + V (r e − r h ),

(4.74)

and the wave function of the exciton may be expanded by the Bloch functions of the electron and hole: n,K Acv (ke , kh )ψcke (r e )ψvkh (r h ). (4.75) Ψ n,K (r e , r h ) = c,ke ,v,kh

Using the wave function of (4.75) in the Hamiltonian of (4.74), multiplying the complex conjugate of the Bloch functions ψc∗ k (r e )ψv∗ k (r h ), and integrating over e h r e , r h , we obtain

1

Here we are dealing with the Hamiltonian of an electron in a valence band Hv and we express the state by the Bloch function ψv,k (r v ) and its energy eigenvalue by Ev (kv ). When a hole state is considered, we have to use the relations: kh = −kv , Eh (kh ) = −Ev (−kv ).

4.5 Exciton

177

Ec (ke ) + Eh (kh ) − E Acn,K v (k e , k h ) n,K + c ke ; v kh |V (r e − r h )|cke ; vkh Acv (ke , kh ) = 0,

(4.76)

c,ke ,v,kh

where we have used the orthonormality of the Bloch functions. Since we are interested in the Wannier exciton, which is weakly bound, the electron–hole interaction potential (Coulomb potential) V (r e − r h ) is assumed to vary very slowly over the distance of the lattice constant, and thus the interaction term may be moved outside of the integral. Taking into account the periodicity of the Bloch functions, the integral may be replaced by a summation of the integral in the unit cell. Therefore, we can derive n,K (ke , kh ) = 0, [Ec (ke ) + Eh (kh ) + V (r e − r h ) − E] Acv

(4.77)

where c , ke , . . . are written as c, ke , . . . for simplicity. Here we assume that the conduction and valence bands are parabolic with scalar masses and that at the top of the valence band Ev = 0, i.e. Ec (ke ) =

2 k 2 + EG , 2m e

Eh (kh ) =

2 kh2 , 2m h

n,K is given by where Ec − Ev = EG is the energy gap. The Fourier transform of Acv n,K (r e , r h ) = Φcv

1 ike ·r e ikh ·r h n,K e e · Acv (ke , kh ) V

(4.78)

ke ,kh

and the Fourier transform of (4.77) is derived in a similar fashion giving rise to n,K (r e , r h ) = 0. [Ec (−i∇e ) + Eh (−i∇h ) + V (r e − r h ) − E] Φcv

(4.79)

In the derivation of the above equation we used the following relation under the assumption of parabolic bands: 2 2 n,K n,K (r e , r h ) = − ∇e + EG Φcv (r e , r h ) Ec (−i∇e )Φcv 2m e 2 2 ke n,K n,K + EG Φcv (r e , r h ) = Ec (ke )Φcv (r e , r h ), = 2m e and a similar relation for the hole band. Equation (4.79) is the effective-mass equation for exciton. Equation (4.79) is also obtained from the effective-mass equation derived in Sect. 3.2. The effective-mass equation (4.79) for the exciton may be rewritten as

178

4 Optical Properties 1

−

2 2 2 2 ∇e + EG − ∇ 2m e 2m h h e2 n,K − (r e , r h ) = 0. − E Φcv 4π|r e − r h |

(4.80)

This equation is well known as the two body problem in quantum mechanics and the solution is obtained by separating the variables into center-of-mass motion and relative motion. Then we put r = re − rh,

R=

1 1 1 + , = μ me mh

me r e + mh r h , me + mh

M = me + mh,

and (4.80) is rewritten as 2 2 2 e2 − ∇ R + − ∇ r2 − Φ n,K (r, R) 2M 2μ 4πr = [E − EG ] · Φ n,K (r, R).

(4.81)

The solution of this equation is given by Φ n,K (r, R) = φ K (R)ψn (r), where φ K (R) and ψn (r) are respectively given by the separate equations 2 2 ∇ φ K (R) = E(K ) · φ K (R), H R φ K (R) ≡ − 2M R 2 2 Hr ψn (r) ≡ − ∇ r + V (r) ψn (r) = En · ψn (r). 2μ

(4.82) (4.83)

The total energy of the system (exciton state) E is then given by E = E(K ) + En + EG .

(4.84)

The energy due to the center-of-mass motion E(K ) is calculated by inserting the wave function φ K (R) ∝ exp(iK · R) into (4.82): E(K ) =

2 K 2 . 2M

(4.85)

On the other hand, the energy due to the relative motion En is obtained from (4.83), which is the same as the bound state energy for shallow donor states derived from

4.5 Exciton

179

the effective mass equation: μ 0 2 EH Eex · 2 = − 2 (n = 1, 2, 3, . . .), m n n μ 0 2 μe4 Eex = EH = , m 2(4π)2 2

En = −

(4.86) (4.87)

where EH is the ionization energy for the hydrogen atom. From these results we obtain the total energy of an exciton E =−

2 K 2 Eex + EG . + n2 2M

(4.88)

Here we have to note that the energy of an exciton is measured from the bottom of the conduction band (Ec = 0). The above calculations reveal that the exciton states consists of the center-of-mass motion of the electron–hole pair with wave vector K and of the relative motion bound by the Coulomb attraction force, and that the total energy of the exciton is the sum of the energies due to the center-of-mass motion E K = 2 K 2 /2M and to the motion of relative coordinates En . As an example, we assume parameters close to those of GaAs, such as μ/m = 0.05 and /0 = 13, and then we obtain En = −3 × 10−4 EH /n 2 which gives the bound energy of the ground state (n = 1) of about 4 meV. The exciton Bohr radius is estimated from (3.43) to be aex = (m/μ)(/0 )aB which gives aex ≈ 150 Å. Figure 4.9 illustrates the energy states of an exciton, where the energy depends on the wave vector K for the center-of-mass motion. In general, we are concerned with the optical excitation of exciton and thus we can assume K = 0. As shown in the above example, the effective Bohr radius of an exciton is much larger than the lattice constant and thus this condition validates the use of the effective mass approximation. As described above we divide the exciton motion into two motions, relative motion in the space r and center-of-mass motion in the space R, and express the wave functions of the effective mass equation by 1 Φ n,K (r, R) = √ exp(iK · R)φn (r), V

Fig. 4.9 Energy states of exciton as a function of wave vector K for the center-of-mass motion. Discrete states are shown by solid curves and the continuum state by the chequered region

(4.89)

180

4 Optical Properties 1

where φn (r) is called the envelope function of an exciton. The ground state of the exciton is given in analogy to the hydrogen atom with a shallow donor state as φ1 (r) =

1 3 πaex

exp(−r/aex ),

(4.90)

where aex = (m/μ)(/0 )aB is the effective Bohr radius of the exciton. By the inverse n,K (ke , kh ) transformation of the wave function (4.89), we obtain the coefficient Acv n,K (ke , kh ) = Acv

1 V

1 = √ V 1 = √ V k∗ =

n,K (ke , kh ) d3 r e d3 r h e−ike ·r e e−ikh ·r h Φcv

d3 rd3 Re−i R·(ke +kh −K ) φn (r)e−ik

∗

·r

∗

d3 re−ik ·r φn (r)δ K ,ke +kh ,

m h ke − m e kh . M

(4.91) (4.92)

As defined in (4.73), the wave vector K is the sum of the wave vectors of the electron and hole (ke + kh ). The coefficient A1,K cv (k e , k h ) for the exciton ground state is obtained by inserting (4.90) into the above equation for n = 1: 1 A1,K cv (k e , k h ) = √ V

64π 5 aex

1/2 (k ∗ 2

1 δ , 2 )2 K ,ke +kh + 1/aex

(4.93)

where A1,K cv (k e , k h ) is found to decrease very rapidly when |k e | and |k h | exceed 1/aex and thus the wave vectors contributing to the 1s exciton are limited to a narrow region of the Brillouin zone |k| ≤ 1/aex . In the case of the Wannier exciton, aex is very large compared to the lattice constant and thus only a narrow region of wave vectors in k space plays an important role in the formation of the exciton. A similar conclusion is drawn for the case of shallow donors. Next we will discuss light absorption by exciton. Let us assume the initial state to be given by Ψ0 = φc,ke φv,−kh = φc,ke φv,ke before excitation, with an electron in the valence band, and the transition from the initial state to the excited state of an exciton given by Ψ λ,K . According to the treatment stated in Sect. 4.2 the transition probability per unit time wif is written as

4.5 Exciton

181

wif =

2 1 λ,K 2π e2 Ψ | exp(ikp · r)e · p|Ψ0 · 2 |A0 |2 m V λ

×δ(EG + Eλ − ω) 2 1 λ,K 2π e2 Acv (ke , −ke ) φc,ke |e · p|φv,ke = · 2 |A0 |2 m V ke ,λ

×δ(EG + Eλ − ω),

(4.94)

where the wave vector of light kp is assumed to be 0 and the momentum conservation law ke = −kh is used. The total energy of the exciton Eλ includes the continuum λ,K has a large value only in a narrow region of ke ≈ 0, the state (En > 0). Since Acv term φc,ke |e · p|φv,ke is regarded as constant in the narrow region of k space we are interested in. Under these assumptions and the condition ke = −kh we obtain λ,K (ke , −kh ) = Acv

1 V

λ,K (r e , r h ). d3 r e d3 r h e−ike ·(r e −r h ) Φcv

(4.95)

The summation in (4.95) with respect to ke is non-zero only when r e − r h = 0, as shown in Appendix A.2. Therefore, we obtain wif =

2π e2 · 2 |A0 |2 |e · pcv |2 |φλ (0)|2 δ(EG + Eλ − ω), m

(4.96)

λ

where |e · pcv | is the momentum matrix element defined in Sect. 4.2. The imaginary part of the dielectric function κ2 (ω) = 2 (ω)/0 is then written as κ2 (ω) =

πe2 2 |e · p | |φλ (0)|2 δ(EG + Eλ − ω). cv 0 m 2 ω 2

(4.97)

λ

First, we consider the excitation of the discrete states of the bound exciton and their transition probability. When we assume parabolic bands with scalar effective masses for simplicity, the relation φλ (0) = 0 is fulfilled only for the s state of the bound exciton. The quantum number λ of the exciton states can then be expressed only by the principal quantum number n: |φn (0)|2 =

1

3 n3 πaex Eex Eλ = En = − 2 , n

,

(4.98) (4.99)

and therefore we find the following relation for the bound states: κ2 (ω) =

1 πe2 Eex 2 1 |e · p | δ E − − ω . G cv 3 0 m 2 ω 2 πaex n3 n2 n

(4.100)

182

4 Optical Properties 1

In the above equation the spin degeneracy is disregarded and κ2 (ω) differs by a factor of 2 from the result in Sect. 4.2. Equation (4.100) reveals that the oscillator strength of exciton absorption spectra is proportional to 1/n 3 and that the discrete lines converge to ω = EG . On the other hand, the continuum states of exciton is given by φλ (0) = 0 only for the magnetic quantum number m = 0, and its state is determined by the wave vector k. Elliott [10] has shown that πα0 exp(πα0 ) , sinh(πα0 ) 2 k 2 Eλ = Ek = , 2μ |φk (0)|2 =

(4.101) (4.102)

where α0 = (aex |k|)−1 = [Eex /(ω − EG )]1/2 . We obtain the imaginary part of the dielectric function for the continuum state: κ2 (ω) =

2π πe2 2 2 0 m ω (2π)3

8μ1 μ2 μ3 6

1/2 π exp(πα0 ) 1/2 Eex |e · pcv |2 . sinh(πα0 )

(4.103)

Now, we consider two extreme conditions. The asymptotic solutions of κ2 (ω) for α0 → 0 (ω → ∞) and for α0 → ∞ (ω → EG ) may be given by, respectively, 8μ1 μ2 μ3 1/2 2π πe2 0 m 2 ω 2 (2π)3 6 ×|e · pcv |2 ω − EG , πe2 1 8μ1 μ2 μ3 1/2 1/2 = Eex |e · pcv |2 . 0 m 2 ω 2 2π 6

κ2 (ω)α0 →0 =

κ2 (ω)α0 →∞

(4.104a) (4.104b)

In the case of α0 → 0, Eex is very small and the relation 2 k 2 /2μ Eex holds. Therefore, the energy of the exciton is much larger than the electron–hole interaction potential and thus we may neglect the Coulomb interaction, giving rise to the result obtained for the one-electron approximation. This is evident from the fact that (4.104a) agrees with (4.39) obtained for the M0 critical point in Sect. 4.3 except for the spin degeneracy factor 2. In the case of α0 → ∞, on the other hand, (4.104b) may be expected to agree with κ2 (ω) for the discrete exciton. When n is large, the exciton absorption lines will overlap each other and cannot be distinguished each other, leading to a quasi-continuum state. The density of states for this case is estimated from (dE/dn)−1 = n 3 /2Eex , and then we obtain |φn (0)|2 ·

dE dn

−1

=

1 1 = 3 E 2πaex 2π ex

8μ3 6

1/2 1/2 Eex .

(4.105)

4.5 Exciton

183

Fig. 4.10 Absorption spectra (κ2 ) due to direct exciton and due to the one-electron approximation (without electron–hole interaction) are plotted in the region near the fundamental absorption edge as a function of photon energy, where the spectrum for exciton absorption is calculated by assuming Γ = 0.2Eex and the Lorentz function for the discrete (bound) exciton

Now we find that the dielectric functions κ2 (ω) obtained from the bound (discrete) states and from the continuum state agree with each other at ω = EG . Figure 4.10 shows absorption spectra (spectra of α(ω) ∝ κ2 (ω)) calculated by taking account of the electron–hole interaction, where the dielectric function without the electron–hole interaction (one-electron approximation) is also plotted for comparison. We have to note here that the calculations are approximated by using the Lorentz function with the broadening parameter Γ = 0.2Eex and by neglecting the spin degeneracy factor 2. We see exciton absorption associated with n = 1 and n = 2 in Fig. 4.10. Here we will discuss the Lorentz function approximation of the dielectric function for the discrete (bound) exciton. We express (4.100) by Eex κ2 (ω) = C · δ EG − 2 − ω . n As shown in Appendix A, the Dirac delta function can be approximated by the Lorentz function in the limit of Γ → 0. Using the Dirac identity in the limit of Γ → 0, we may write 1 EG − Eex /n 2 − (ω + iΓ ) 1 + iπδ EG − Eex /n 2 − ω =P 2 EG − Eex /n − ω

(4.106)

and a comparison of the dielectric function κ2 (ω) with the imaginary part of above equation gives the following relation:

184

4 Optical Properties 1

C/π EG − Eex /n 2 − (ω + iΓ ) Eex = C · δ EG − 2 − ω . n

κ2 (ω) =

CΓ /π = 2 EG − Eex /n 2 − ω + Γ 2 (4.107)

The second relation of the above equation with C = 1 is called the Lorentz function. The Lorentz function is characterized by the center located at ω = (EG − Eex /n 2 ) and by its full-width half-maximum Γ . The integral of the Lorentz function with respect to ω is equal to unity. In the limit of Γ → 0, therefore, the Lorentz function is equivalent to δ(EG − Eex /n 2 − ω). From these considerations it is possible to replace the delta function by the Lorentz function. As shown in Sect. 4.6, the real part of the dielectric function is obtained from the Kramers–Kronig relation of (4.126a): 2 κ1 (ω) = P π = =

2 P π

∞

ω κ2 (ω ) dω (ω )2 − ω 2

∞

ω · C · δ(EG − Eex /n 2 − ω ) dω (ω )2 − ω 2

0

0

EG − Eex /n 2 2C . π (EG − Eex /n 2 )2 − (ω)2

(4.108)

The above result may be approximated by EG − Eex /n 2 2C π (EG − Eex /n 2 )2 − (ω)2 C/π C/π + = 2 EG − Eex /n − ω EG − Eex /n 2 + ω C/π . EG − Eex /n 2 − ω

κ1 (ω) =

(4.109)

The final relation of the above equation is obtained from the second relation by assuming that the second term is non-resonant and small compared to the first term, enabling us to neglect the second term. The complex dielectric function of the exciton is therefore approximated by κ(ω) = κ1 (ω) + iκ2 (ω) =

C/π . EG − Eex /n 2 − (ω + iΓ )

(4.110)

The above relation coincides with the result obtained by the second quantization method [11]. The experimental results for the optical absorption in GaAs is shown in Fig. 4.11 [12]. At low temperatures (T = 186, 90, 21 K) the exciton absorption peak for n = 1 is clearly seen and the overall features are in good agreement with the calculated absorption spectrum shown in Fig. 4.10.

4.5 Exciton

185

Fig. 4.11 Experimental results of the optical absorption in GaAs at different temperatures. The exciton peak is clearly observed at low temperatures from (Sturge [12]) and the overall features are in good agreement with the calculated results shown in Fig. 4.10

4.5.2 Indirect Exciton In the above calculations, we dealt with exciton associated with the fundamental absorption edge of the M0 critical point at the Γ point (direct transition), where the top of the valence band and the bottom of the conduction band are located at k = 0. We have also shown that a weak absorption will appear for the indirect transition where the top of the valence band and the bottom of the conduction band are located at different k in the Brillouin zone and is an indication of the existence of the exciton effects in such indirect gap semiconductors. In this Subsection we will be concerned with exciton effect in indirect gap semiconductors such as Ge, Si, GaP and so on. The top of the valence band and the bottom of the conduction band are assumed to be located at kv0 (= −kh0 ) and kc0 (= ke0 ) (kv0 = kc0 ), respectively, and the bands are approximated by the parabolic functions Ec = EG + Eh = −Ev =

2 (kc − kc0 )2 , 2m e 2 (kv − kv0 )2 . 2m h

Putting ke = kc − kc0 = ke − kc0 , kh = −(kv − kv0 ) ≡ kh − kh0 , then the effective mass equation for this exciton is written as 2 2 2 2 e2 − Φ λ,K (r e , r h ) ∇e − ∇h − 2m e 2m h 4πr

= Eλ Φ λ,K (r e , r h ),

(4.111)

where K = ke + kh = (ke + kh ) − (ke0 + kh0 ). Following the treatment of the direct exciton, the wave function Φ λ,K (r e , r h ) may be separated into translational (center-of-mass) motion (R) and relative motion (r):

186

4 Optical Properties 1

1 Φ λ,K = √ φλ (r) exp(iK · R) V where we find that φλ (r) satisfies (4.83) and thus the total energy of the exciton is given for the bound state by Eλ = En = −Eex /n 2 +

2 K 2 . 2M

(4.112)

Therefore, we obtain the dielectric function of the indirect exciton for the bound state as πe2 |e · pm,α,± |2 |φn (0)|2 cv 0 m 2 ω 2 m,α,± Eex 2 2 α {ke + kh − (ke0 + kh0 )} − ω ± ωq × δ EG − 2 + n 2M 2M 3/2 1 πe2 1 m,α,± 2 1 = · |e · p | · · 3 cv 3 0 m 2 ω 2 2π 2 m,α,± πaex 2 n × ω − EG ∓ ωqα + Eex /n 2 . (4.113)

κ2 (ω) =

It is evident from these results that the dielectric function κ2 (ω) for the bound state of the indirect exciton does not exhibit any discrete lines but a continuum spectrum. This feature may be understood by noting that the wave vector K of the indirect exciton is different from the direct exciton due to the exchange of momentum of the indirect exciton with the lattice vibrations, giving rise to the possibility of the wave vector taking arbitrary values. Figure 4.12 shows an illustration of (4.113). As stated in Sect. 4.5, the absorption coefficient calculated from the one-electron approximation shows an increase at the photon energies corresponding to phonon absorption and phonon emission. When the Coulomb interaction between the electron and hole is taken into account,

Fig. 4.12 Optical absorption spectra associated with an indirect exciton, where α(ω) ∝ κ2 (ω) is plotted as a function of photon energy. The absorption coefficient increases at photon energies associated with phonon emission and absorption

4.6 Dielectric Function

187

Fig. 4.13 Square root of the absorption coefficient α1/2 in GaP is plotted as a function of photon energy. The arrows indicate an increase in the absorption coefficient due to exciton effect (phonon emission) (Gershenzon et al. [13])

κ2 (ω) increases at photon energies EG − Eex /n 2 ± ωqα and the distance between the two rising points is equal to twice the phonon energy. The most significant difference between the two curves is the photon energy dependence of the absorption coefficients. The dielectric function κ2 (ω) exhibits quadratic behavior with respect to photon energy in the case without Coulomb interaction, whereas κ2 (ω) for the indirect exciton shows a square root dependence √of photon energy. These features explain the deviation from a linear relation of the α versus photon energy plot of Ge in Fig. 4.8 by means of the exciton effect. The experimental observation of indirect exciton in GaP is shown in Fig. 4.13, where the square root of the absorption coefficient is plotted as a function of photon energy. The results are in good agreement with (4.113) [13], where phonon modes involved with the transition are indicated. We note here that a general expression of κ2 (ω) as a function of ω is not obtained, but that an asymptotic form is obtained for ω − EG Eex , which agrees with the result of the one-electron approximation without the exciton effect (see [10]).

4.6 Dielectric Function The polarization vector P(ω) in a material due to an external field E(ω) of angular frequency ω is defined by (4.114) P(ω) = χ(ω)0 E(ω), where χ(ω) is the susceptibility tensor. Since the susceptibility tensor is an analytical function of frequency in real numbers, it is rewritten by using the Cauchy relation as

χ(ω) =

+∞ −∞

χ(ω ) dω , 2πi ω − ω − iε

(4.115)

where ε is an infinitely small positive number. In Appendix A we derive the Dirac identity relation given by (A.2)

188

4 Optical Properties 1

1 1 = P + iπδ(ω). ε→0 ω − iε ω lim

(4.116)

The integration of (4.115) is carried out by using the Dirac identity relation, which gives rise to

χ(ω) = P

∞ −∞

dω χ(ω ) 1 + 2πi ω − ω 2

or χ(ω) = P

∞

−∞

∞

−∞

dω χ(ω )δ(ω − ω),

dω χ(ω) . πi ω − ω

(4.117)

(4.118)

Now, we define the complex dielectric function by χ(ω) = χ1 (ω) + iχ2 (ω)

(4.119)

and then we obtain the following relation from (4.118):

∞

dω χ2 (ω ) , −∞ π ω − ω

∞ dω χ1 (ω ) χ2 (ω) = −P . −∞ π ω − ω χ1 (ω) = P

(4.120a) (4.120b)

We divide the integration for χ1 into the following two regions:

χ1 (ω) = P

0 −∞

dω χ2 (ω ) +P π ω − ω

∞

0

dω χ2 (ω ) . π ω − ω

The reality condition for the susceptibility tensor (dielectric tensor) χ(ω) = χ∗ (−ω) leads to the following relations χ1 (ω) = χ1 (−ω),

(4.121a)

χ2 (ω) = −χ2 (−ω).

(4.121b)

Using these relations we obtain for χ1 (ω)

χ1 (ω) = P

∞

0

=P

0

∞

1 dω 1 χ2 (ω ) + π ω +ω ω −ω dω 2ω χ2 (ω ) 2 . π ω − ω2

(4.122)

In a similar fashion we calculate χ2 (ω) and therefore obtain the following relations:

4.6 Dielectric Function

189

χ1 (ω) =

2 P π

χ2 (ω) = −

∞ 0

2ω P π

ω χ2 (ω ) dω , ω 2 − ω 2

0

∞

χ1 (ω ) dω . ω 2 − ω 2

(4.123a) (4.123b)

The above relations are called the Kramers–Kronig relations, and the transform between the real and imaginary part of the susceptibility tensors is called the Kramers–Kronig transform. The dielectric constant κ(ω) is related to the susceptibility by using the definition of electric displacement D through D = 0 E + P = (1 + χ)0 E ≡ κ0 E ≡ E,

(4.124)

and the following relation holds: κ(ω) = 1 + χ(ω).

(4.125)

Therefore, the Kramers–Kronig relations for the dielectric constant κ(ω) are given by

∞ ω κ2 (ω ) 2 P dω π ω 2 − ω 2 0

∞ κ1 (ω ) 2ω κ2 (ω) = − P dω , π ω 2 − ω 2 0 κ1 (ω) = 1 +

(4.126a) (4.126b)

or, using (4.40), the relations π e 2 |e · pcv |2 δ [Ecv (k) − ω] , 0 mω k

2 ∞ ω κ2 (ω )dω χ1 (ω) = κ1 (ω) − 1 = π 0 ω 2 − ω2 2 1 |e · pcv |2 2 e · 2 = 0 m Ecv (k) Ecv (k) − 2 ω 2

χ2 (ω) = κ2 (ω) =

(4.127a)

(4.127b)

k

are obtained. The energy band structure of Ge calculated by the k · p perturbation method is shown in Fig. 4.14, where the optical transitions at the critical points are indicated by arrows and the notation of the critical points is after Cardona [6, 14]. It should be noted that the representation used for the energy bands is the notation for the single group instead of the double-group representation. The reason is due to the fact that the basis functions used for the k · p perturbation calculations are those for the single-group representation. In the following we will derive the dielectric functions, real and imaginary parts, at the critical points shown in Fig. 4.14. The results are

190

4 Optical Properties 1

Fig. 4.14 Energy band structure of Ge calculated by the k · p perturbation method and the direct transitions at several important critical points (shown by arrows)

very important for understanding the optical properties of semiconductors. First, we derive the imaginary part of the dielectric function for a critical point, and the real part is calculated by using the Kramers–Kronig relation.

4.6.1 E0 , E0 + 0 Edge The critical points E 0 and E 0 + Δ0 are associated with the direct transition from the valence band and the spin–orbit split-off band to the lowest conduction band at the Γ point and thus they are M0 type. The imaginary part of the dielectric function κ2 (ω) is calculated in Sects. 4.2 and 4.3. The real part of the dielectric function is calculated from the Kramers–Kronig relations.2 The imaginary part of the dielectric function for the E 0 edge is κ2 (ω) =

A| c| p|vi |2

i=1,2

A=

e2 1/2 2π0 m 2

2μi 2

1 (ω − ω0 )1/2 , ω2

(4.128)

3/2 ,

(4.129)

where i represents the heavy and light hole valence bands and the summation is carried out for the two bands. μi is the reduced mass of the valence bands and the conduction band, and ω0 = E 0 / ≡ EG /. Similarly the absorption coefficient for the transition at the E 0 + Δ0 edge between the spin–orbit split-off and the conduction band is calculated, which is given by replacing the momentum matrix element by | c| p|vso |2 = | c| p|vi |2 ≡ P02 (P0 is defined in (2.83b) and (2.203d)), the reduced mass by μso and ω0 by ω0 s = (EG + Δ0 )/.

2

In this section we follow the custom adopted in the optical spectroscopy of semiconductors, and the critical points are expressed by symbols such as E 0 , E 1 and E 2 instead of the notation for energy E| used in this text. In later Sections we use E for the electric field, which will not introduce any complication or confusion.

4.6 Dielectric Function

191

Using (4.126a) we obtain κ1 (ω) − 1 −3/2 1 2 − (1 + x0 )1/2 − (1 − x0 )1/2 ; for x < x0 2 x0

(4.130a)

−3/2 1 2 − (1 + x0 )1/2 ; for x > x0 2 x0

(4.130b)

= A P02 ω0 = A P02 ω0

where x0 = ω/ω0 (see Problem (4.4) and its answer for derivation). According to the k · p perturbation method described in Sect. 2.4, the effective mass is defined as a function of the momentum matrix element P0 and the energy gaps. From (2.82) we have 1 2P02 1 = + m(Γ2 ) m 3m

2 1 + ω0 ω 0 + Δ0

(4.131)

for the electron in the conduction band at the Γ point. We take into account the Γ2 conduction and the Γ25 valence bands and neglect the perturbation due to higher bands. The effective mass in the 001 direction is obtained from (2.65) and (2.67) as 2 /2 = −A − |B|, m hh (001)

(4.132a)

2 /2 = −A + |B|, m lh (001)

(4.132b)

2 /2 = −A − Δ0 . m so

(4.132c)

Using the definitions of Luttinger (2.227), (2.228) and (2.229 in Sect. 2.7 and neglecting contribution from the higher lying conduction bands, we obtain

and using (2.235)

A=

2 2 [1 + F + 2G] [1 + F], 2m 2m

(4.133a)

B=

2 2 [1 + H1 + H2 ] [1], 2m 2m

(4.133b)

C=

2 2 [F − G + H1 − H2 ] [F]. 2m 2m

(4.133c)

192

4 Optical Properties 1

F =−

E P0 3

2 1 2 , E P0 = P02 . + EG E G + Δ0 m m = −2 − F m hh (001) m = −F m hh (001) m = −(1 + F) m so (001) m =1− F m(Γ2 )

(4.134) (4.135a) (4.135b) (4.135c) (4.135d)

Therefore the reduced masses are given by m m m 2E P0 + = = −1 − 2F = −1 + μhh m(Γ2 ) m hh 3

2 1 + EG E G + Δ0

2E P O (4.136a) EG m m m 2E P0 2 1 + = =1−2F =1+ + μlh m(Γ2 ) m lh 3 EG E G + Δ0 −1 +

1+

2E P O EG

(4.136b)

m m m 2E P0 + = = −2 F = μso m(Γ2 ) m so 3

2 1 + EG E G + Δ0

2E P O EG

(4.136c)

The above results reflect that the electron effective mass m(Γ2 ) is small compared with the effective masses of the heavy, light, and spin–orbit split off bands. As an example we consider the case of GaAs, where EG = 1.51 [eV]. Δ0 = 0.341 [eV], and E P = 28.8 [eV]. Assuming EG Δ0 and E P O /EG 1, we obtain the following simple relation: 1 1 1 2E P O 2E P O = = = = μhh μlh μso mEG mω0 μi ≡=

(4.137)

mEG mω0 = 2E P O 2E P O

(4.138)

Therefore, the real part of the dielectric function due to the contribution from the E 0 edge and the E 0 + Δ0 edge is given by κ1 (ω) − 1 = C0

1 f (x0 ) + 2

ω0 ωso

3/2 f (x0s )

(4.139)

4.6 Dielectric Function

193 −3/2

where C0 2 A P02 ω0 with μi = mω0 /(2E P O ) = mEG /2E P0 , x0 = ω/ω0 and x0s = ω/(ω0 + Δ0 ). The function f (x) is defined as f (x) = x −2 2 − (1 + x)1/2 − (1 − x)1/2 .

(4.140)

4.6.2 E1 and E1 + 1 Edge We have already mentioned that the joint density of states for the optical transition given by (4.44) exhibits a divergence when the condition given by (4.49) or (4.50) is satisfied. The energy band calculations show that the conduction band and the valence band are parallel over a wide range of the wave vector k in the 111 direction of k space, satisfying the condition of (4.50). As discussed in Chap. 2, the conduction band Λ1 originated from Γ2 and the valence bands Λ3 (doubly degenerate bands split into heavy and light hole bands due to the spin–orbit interaction) originated from Γ25 exhibit the parallel behavior, and these features appear in almost all semiconductors, giving rise to a critical point called E 1 and E 1 + Δ1 . Since the critical point is associated with the parallel feature over a wide range in the 111 direction, the critical point may be approximated as being two–dimensional and the density of states can be expressed by the step function : κ2 = B| c| p|v|2 ω −2 H (ω − ω1 )

E1

E 1 + Δ1 : κ2 = B | c| p|v|2 ω −2 H (ω − ω1 − Δ1 )

,

(4.141)

√ √ where B = 3πμ(E 1 )e2 /0 2 m 2 a0 , B = 3πμ(E 1 + Δ1 )e2 /0 2 m 2 a0 B, and H is the step function defined as H (x) = 0 for x < 0 and H (x) = 1 for x > 0. The detail of the derivation is found in the papers by Cardona [15] and Higginbotham et √ lattice constant a0 appears in the above equation from the integral al. [16]. The dk z = 2π 3/a0 . The real part of the dielectric function for the E 1 edge and the E 1 + Δ1 edge is calculated from the Kramers–Kronig relation as 2 ω − ω2 B κ1 (ω) − 1 = − | c| p|v|2 ω −2 ln 1 2 π ω1 B 1 ω2 2 −2 = | c| p|v| ω1 1 + + ··· π 2 ω12 for the E 1 edge, and

(4.142)

194

4 Optical Properties 1

(ω1 + Δ1 )2 − ω 2 B 2 −2 κ1 (ω) − 1 = − | c| p|v| ω ln π (ω1 + Δ1 )2 B 1 ω2 2 −2 = 1+ | c| p|v| (ω1 + Δ1 ) + ··· π 2 (ω1 + Δ1 )2

(4.143)

for the E 1 + Δ1 edge.

4.6.3 E2 Edge The reflectance R and the imaginary part of the dielectric function κ2 (ω) in semiconductors exhibit a large peak at around ω 4 eV and the peak is called the E 2 edge. The origin of the E 2 edge is not well identified, but is believed to be associated with a combination of several critical points. Here the dielectric function of the E 2 edge is treated by the method proposed by Higginbotham, Cardona and Pollak [16]. Since the E 2 edge has a large peak at ω = E 2 , the dielectric function is approximated by using a simple harmonic oscillator model, the Drude model. Then the dielectric function is given by κ1 (ω) − 1

C2 ω22 C2 (1 + x22 ), ω22 − ω 2

(4.144)

where ω2 = E 2 and x2 = ω/ω2 .

4.6.4 Exciton As we discussed in Sect. 4.5, exciton absorption will occur in semiconductors with a direct gap, where exciton consists of electron–hole pairs interacting through the Coulomb potential and the absorption energy is below the fundamental absorption edge by the exciton binding energy (a few meV). For simplicity, we will consider the ground state exciton excited at the E 0 edge, and then the absorption may be approximated by the Lorentz function. The real part of the dielectric function for the exciton is derived in Sect. 4.5 and given by (4.108): κ1 (ω)

2 Cex ωex Cex = , 2 2 2 ωex − ω 1 − xex

(4.145)

where ωex is the energy of the exciton, the binding energy is Eex = (ω0 − ωex ), and xex = ω/ωex . The above results are summarized to give the real part of the dielectric function below the E 0 edge as

4.6 Dielectric Function

κ1 (ω) − 1 =

195

3/2 Cex 1 ω0 + C ) + f (x ) , f (x 0 0 0s 2 1 − xex 2 ω0s ω1 2 +C1 h(x1 ) + h(x1s ) + C2 (1 + x22 ), ω1s

(4.146)

where x1 = ω/ω1 , x1s = ω/(ω1 + Δ1 ) and 1 h(x) = 1 + x 2 . 2

(4.147)

It is well known that the higher-energy edges exhibit only a weak dispersion in the dielectric constant and thus the contribution is approximated by replacing 1 with a constant D in κ1 (ω) − 1. This approximation is known to give good agreement with experiment in many semiconductors. Examples of the comparison between the theory and experiment are shown in Fig. 4.15 for Ge and in Fig. 4.16 for GaAs, where the solid curves are best fitted by using (4.146) by neglecting the contribution from the exciton effect and we find good agreement between the theory and experiment. The parameters used to calculated the theoretical curves in Fig. 4.15 for Ge and in Fig. 4.16 for GaAs are shown in Table 4.3. It has been shown that the dielectric function is well expressed by taking the contribution from the E 0 edge and the E 0 + Δ0 edge into account [17]. When we adopt this approximation, the real part of the dielectric function is given by the terms

Fig. 4.15 The real part of the dielectric function for Ge, where experimental results are compared with the best fitted curve calculated from (4.146) (without the exciton effect) (from [16])

Fig. 4.16 The real part of the dielectric function for GaAs, where experimental results are compared with the best fitted curve calculated from (4.146) (without the exciton effect) (from [16])

196

4 Optical Properties 1

Table 4.3 Parameters use to fit the theoretical curves of the dielectric function with the experimental results in Ge and GaAs. All the parameters are for T = 300 K and the critical point energies are shown in units of [eV] Ge GaAs Experiment Calculation Experiment Calculation C0 C1 C2 E0 E 0 + Δ0 E1 E 1 + Δ1 E2

4.85 5.60 3.10 0.797 1.087 2.22 2.42 4.49

1.90 3.22

7.60 2.05 3.50 1.43 1.77 2.895 3.17 4.94

1.53 2.50

due to the E 0 edge and the E 0 + Δ0 edge and the constant D due to the contributions from the other edges. Therefore, the dielectric function is well expressed by ω 1 ω0 3/2 ω + + D. κ1 (ω) = C0 f f ω0 2 ω0s ω0s

(4.148)

The difference in C0 between the fit and the theory is believed to be due to the exciton effect and neglect of the contribution from the higher-energy critical points.

4.7 Piezobirefringence 4.7.1 Phenomenological Theory of Piezobirefringence When a stress is applied to a semiconductor crystal, it produces a change in the refractive index in the parallel and perpendicular directions. This effect is called piezobirefringence. The plane of polarization of the light makes an angle of 45◦ with the stress direction. Experimentally, one obtains the phase difference Δ between the components of the light polarized parallel and perpendicular to the stress axis. Assuming a sample thickness t the phase difference per unit length is given by [16] 2π n − n ⊥ Δ = , t λ

(4.149)

where λ is the wavelength of the incident light, and n and n ⊥ are the refractive indices of the polarization in the directions parallel and perpendicular to the stress. Normally the piezobirefringence experiment is carried out in the transparent region

4.7 Piezobirefringence

197

of the optical spectrum, where the absorption coefficient is small, enabling us to neglect the imaginary part of dielectric function (κ2 0) and thus to use (4.149) π 2π (κ1 ) − (κ1 )⊥ Δ = (κ1 ) − (κ1 )⊥ , t λ n + n⊥ λn 0

(4.150)

where n 0 is the refractive index without stress and relations derived from (4.15) are used such as n = (κ1 ) . Piezobirefringence has a very important property for investigating the stress effect on the energy bands, especially on the valence bands. In this Subsection we will deal with a phenomenological theory of piezobirefringence and microscopic theory based on the band structure of semiconductors. It may be easily understood by replacing stress with phonons that piezobirefringence is related to Brillouin scattering and Raman scattering as discussed later. When a stress Tkl is applied to a crystal, the dielectric constant tensor κi j is changed by Δκi j . We define the change by Δκi j = Q i jkl Tkl ,

(4.151)

where Q i jkl is called the piezobirefringence tensor of fourth rank. The fourth-rank tensor is often expressed by Q αβ (α, β = 1, 2, . . . , 6) and the non-zero components are Q 11 , Q 12 , Q 44 for a crystal with cubic symmetry. We consider the case where the stress is applied in the [100] direction (Tx x = T1 = X ) as an example. The change in the dielectric constant for light polarized parallel to the stress is then given by Δκ = Δκx x = Q x x x x Tx x = Q 11 X, and for light polarized perpendicular to the stress is given by Δκ⊥ = Δκzz = Q zzx x Tx x = Q 31 T1 = Q 12 X. Therefore, piezobirefringence coefficient α(100) is given by α(100) =

κ − κ⊥ = Q 11 − Q 12 . X

(4.152)

Similarly, we can obtain the piezobirefringence coefficient for the stress applied in the other directions. The above treatment is phenomenological and the piezobirefringence coefficients reflect the stress-induced change in the energy band structure and thus depend on the critical points. In general, a stress induces a change in the lattice constant, giving rise to a change in the energy band structure. The change is estimated quantitatively by using the deformation potential, which will be discussed in more detail in Chap. 6 in connection with the electron–phonon interaction. In this section we will consider the general theory of the deformation potential and its application to piezobirefringence theory.

198

4 Optical Properties 1

4.7.2 Deformation Potential Theory Defining the coordinate vectors before and after the deformation by r and r and the displacement vector by u, we find u = r − r = e · r,

(4.153)

where e is the strain tensor defined by e = ei j =

1 2

∂u j ∂u i + ∂r j ∂ri

.

(4.154)

Equation (4.153) can be rewritten as ri = ri −

ei j r j .

(4.155)

j

Then the operator ∇ of the old coordinates r is expressed by new coordinates r as ∂ ∂ ∂ = − ei j , ∂ri ∂ri ∂r j j

(4.156)

and thus we obtain ∂2 = ∂ri2

∂ ∂ ei j − ∂ri ∂r j j

2

∂2 ∂2 −2 ei j , 2 ∂ri ∂r j ∂ri j

(4.157)

where the above equation takes account of the first order of ei j and neglects the higher-order terms. Then we obtain ∇ 2 = ∇ 2 − 2

ei j

i, j

∂2 . ∂ri ∂ j

(4.158)

Since the crystal potential is given by V (r) = V (r + e · r) V (r + e · r ),

(4.159)

it is expanded with respect to e as: V (r) = V0 (r ) +

i, j

Vi j (r )ei j ,

(4.160)

4.7 Piezobirefringence

199

where the expansion coefficient Vi j (r ) is given by3 ∂V (r + e · r ) ∂V (r ) Vi j (r ) = = − r . ∂ei j ∂ri j e=0

(4.161)

In the following we neglect the stress effect on the spin–orbit split-off-band, because experiments have shown no significant stress effect on this band. Therefore, the Hamiltonian of an electron is written as H = H0 + Hso + Hs , 2 H0 = − 2m + V0 (r),

(4.162) (4.163)

where H0 is the Hamiltonian without stress, Hso is spin–orbit interaction, and Hs is the Hamiltonian for the stress effect. Using (4.158) and (4.160), the stress Hamiltonian is written as: ∂2 2 ei j + Vi j ei j ≡ D i j ei j , (4.164) Hs = m ij ∂ri ∂r j ij where Di j =

2 ∂ 2 + Vi j m ∂ri ∂r j

(4.165)

is called the deformation potential operator. For simplicity we discuss the stress effect in a cubic crystal. It may be understood that the treatment can be applied to any crystal by taking the crystal symmetry into account. The valence bands are assumed to be 3-fold degenerate p states, which is equivalent to taking into account the Γ25 valence bands as shown in Sect. 2.2 to analyze the valence band structure. Following the treatment of Sect. 2.2, the matrix elements of Hs are shown to be k|D i j |lei j ≡ Dkli j ei j , (4.166) k|Hs |l = ij

ij

where Dkli j = k|D i j |l.

(4.167)

Dkli j is a fourth-rank tensor, called the deformation potential tensor, and has elements similar to (2.43). Using (2.53a), we obtain for example

3

From (4.155) we obtain ∂V ∂V ∂ri ∂V ∂V = = − r j − r j . ∂ei j ∂ri ∂ei j ∂ri ∂ri

.

200

4 Optical Properties 1

1 Dx x x x ex x + Dx x yy e yy + Dx x zz ezz 2 +D yyx x ex x + D yyyy e yy + D yyzz ezz 1 = (D11 + D12 )(ex x + e yy ) + D12 ezz 2 ≡ G1.

u + |Hs |u + =

(4.168)

(4.169)

In a similar fashion other elements are calculated and finally we obtain the following result: G1 G2 G4 ∗ (4.170) k|Hs |l = G 2 G 1 G ∗4 , G∗ G4 G3 4 1 (D11 + D12 )(ex x + e yy ) + D12 ezz , 2 1 G 2 = (D11 − D12 )(ex x − e yy ) − 2iD44 ex y , 2 G1 =

G 3 = D12 (ex x + e yy ) + D11 ezz , G4 =

√ 2D44 (ex z − ie yz ).

From the above analysis we find that the deformation of the valence bands due to stress or strain is described by three potential constants D11 , D12 and D44 . Another approach to the stress effect has been reported by Picus and Bir [18], who introduced the deformation potential due to the volume deformation (ex x + e yy + ezz ; hydrostatic term) and to the uniaxial term. The strain Hamiltonian for the Γ25 bands at k = 0 is then written as 1 2 (i) (i) (i) 2 L x − L ex x + c.p. Hs = −a (ex x + e yy + ezz ) − 3b 3 (i) 6d (4.171) − √ {L x L y }ex y + c.p. , 3 where the index i represents one of the three valence bands, L is a dimensionless operator given by the angular momentum operator for the quantum number l = 1 of (2.52) divided by , c.p. is the cyclic permutation of x, y, z, and {L x L y } = (1/2)(L x L y + L y L x ).4 The constant a (i) is the hydrostatic deformation 4

The reported matrix elements of the strain Hamiltonian are evaluated by using the angular momentum operators in terms of “spin” matrices corresponding to spin unity according to Picus and Bir [18], where the basis functions are taken as 1 S+ = √ |X + iY , 2

S0 = |Z ,

1 S− = √ |X − iY . 2

4.7 Piezobirefringence

201

potential for the band i, and b(i) and d(i) are the deformation potentials for the uniaxial strain (ei j , i = j) and the shear strain (ei j , i = j), respectively. Since experiments measure the change in the energy gap between the Γ2 (Γ1 ) conduction band and the Γ25 (Γ15 ) valence bands under hydrostatic pressure, the deformation potential a (i) corresponds to the relative change in the energy gap (not the valence bands only). In Chap. 10 we will discuss the strain effect on the quantum well lasers, where the deformation potential ac for the conduction band and av for the valence bands are defined. When the conduction band–edge shift is expressed by E(X ) − Ec (X = 0) = ac (ex x + e yy + ezz ) and the valence band top by −av (ex x + e yy + ezz ), then the change in the energy gaps due to the hydrostatic pressure is given by (ac + av )(ex x + e yy + ezz ). Therefore the total deformation potential is sometimes defined by a = ac + av . It should be noted here that the Hamiltonian Hs with Dαβ and the Hamiltonian with a (i) , b(i) , d(i) give rise to the same results as expected from the analysis given above and that the relations between the two types of deformation potential is easily obtained.

4.7.3 Stress-Induced Change in Energy Band Structure A typical energy band structure in the vicinity of k = 0 (Γ ) such as Ge and GaAs is shown schematically in Fig. 4.17 for the conduction band and the valence bands. The valence bands without stress consist of doubly degenerate bands | 23 , 23 , | 23 , 21 and the spin–orbit split-off band | 21 , 21 , as shown on the left of Fig. 4.17. When stress is applied, the degeneracy is removed, as shown on the right of Fig. 4.17 for the compressive uniaxial stress. Therefore, we may expect a remarkable change in the optical properties of semiconductors by the application of stress. In experiments uniaxial stress along the [001], [111] or [110] direction is applied. Using the results in Appendix C the strain components for the stress X are (X > 0 and X < 0 correspond to the tensile and compressive stresses, respectively), [001] stress ezz = s11 X, ex x = e yy = s12 X, ex y = ex z = e yz = 0, [111] stress ex x = e yy = ezz = (s11 + 2s12 )( 31 X ), ex y = e yz = ezx = ( 21 s44 )( 13 X ), The corresponding operators are then expressed by the relation (2.52). The matrix elements of the strain Hamiltonian in the text are evaluated by using the basis functions and the corresponding operators.

202

4 Optical Properties 1

Fig. 4.17 Energy band structure of semiconductors such as Ge and GaAs near k = 0 with and without stress. The degenerate valence bands without stress split into three bands under the compressive uniaxial stress (X < 0) as shown on the right. The bands V1 , V2 and V3 originate from V1 , V2 and V3 bands but they are mixed up with each other at k = 0

[110] stress ex x = e yy = (s11 + s12 )( 21 X ), ezz = s12 X, ex y = ( 21 s44 )( 21 X ), ex z = e yz = 0, where sαβ (ei j = si jkl Tkl , eα = sαβ Tβ ; i, j = x, y, x; α, β = 1, 2, . . . , 6) is the elastic compliance tensor (see Appendix C). In the following the band index i is dropped out. The matrix elements of the strain Hamiltonian are easily evaluated using (4.171) and the wave functions (2.63a)–(2.63f), which will be used to derive the 6 × 6 Hamiltonian matrix in Sects. 10.6.2 and 10.6.4. We rewrite the strain Hamiltonian Hs in the following form. Hs = −av ex x + e yy + ezz − 3b

L 2x −

= Hshydro + Hsshear , Hshydro = −av ex x + e yy + ezz , 1 Hsshear = −3b L 2x − L 2 ex x + c.p. , 3

1 2 L ex x + c.p. 3 (4.172a) (4.172b) (4.172c)

where the deformation potential av is defined for the valence bands. When we define the hydrostatic pressure dependence of the conduction band edge by ac ex x + e yy + ezz , the total band gap change due to the hydrostatic pressure is given by (ac + av ) ex x + e yy + ezz . Then the matrix elements for H hydro are given by

4.7 Piezobirefringence

203

! 3 1! 1 1! 3 3 hydro 3 3 3 1 1 1 , Hs = , Hshydro , = , Hshydro , , 2 2 2 2 2 2 2 2 2 2 2 2 (4.173) = −av ex x + e yy + ezz , and the matrix elements for Hsshear are5 ! 3 3 shear 3 3 b , Hs , = + (ex x + e yy − 2ezz ), 2 2 2 2 2 ! 3 1 shear 3 1 b , H = − (ex x + e yy − 2ezz ), , 2 2 s 2 2 2 ! 3 1 shear 1 1 1 , Hs , = −i √ b ex x + e yy − 2ezz ., 2 2 2 2 2

(4.174a) (4.174b) (4.174c)

# " where we have to note that 3/2, 3/2 Hsshear 3/2, 1/2 = 0 because of the diagonal property of the spin directions. We define these non–zero components as Δhydro = −av (ex x + e yy + ezz ) = −av (s11 + 2s12 ) X, b Δshear = + ex x + e yy − 2ezz = −b (s11 − s12 ) X. 2

(4.175a) (4.175b)

These results give the Hamiltonian matrix | 23 , 21 | 21 , 21 |3, 3 hydro2 2 shear Δ +Δ 0 0 √ hydro shear shear 0 Δ √ −Δ −i 2Δ , 0 i 2Δshear −Δ0 + Δhydro

(4.176)

where the energy is measured from the top of the doubly degenerate valence band edge. Equation (4.176) will be used to derive 6 × 6 Hamiltonian matrix (10.161) for a quantum well with strain in Sect. 10.6.4. In the case of [001] stress, the parameters defined by Pollak and Cardona [19] are given by δ E H = −Δhydro = +a(s11 + 2s12 )X,

(4.177a)

δ E 001 = −2Δshear = +2b(s11 − s12 )X,

(4.177b)

where a = ac + av and thus δ E H = a(s11 + 2s12 )X = (∂Eg /∂ P) · P is the change in the energy gap due to the hydrostatic component of the strain (P: hydrostatic linear splitting of the 23 , ± 23 and The term δ E 001 = 2b(s11 − s12 )X is the pressure). 3 , ± 1 valence bands, and the mixing between 3 , ± 1 and 1 , ± 1 valence bands. 2 2 2 2 2 2 5 The relation of (4.174a) is sometimes expressed by using negative sign (−b/2 · · · ·) as discussed in Chap. 9. The change of expressions, however, is just the change in the sign of the deformation potential b.

204

4 Optical Properties 1

Since the stress does not remove the Kramers degeneracy of each state, diagonalization of the matrix of the Hamiltonian Hso + Hs is done by diagonalizing the matrix for positive m J of the valence states |J, m J , which gives rise to the following matrix [19] | 23 , 21 | 21 , 21 | 23 , 23 1 3 Δ0 − δ E H − 21 δ E 001 0 0 √ 1 1 1 0 Δ − δ E + δ E 2δ E H 001 001 , 3 0 2 2 √ 1 0 2δ E 001 − 23 Δ0 − δ E H 2

(4.178)

where the origin of the energy is set to the top of the triply degenerate valence bands without spin-orbit interaction. Diagonalizing the matrix, the energy splitting and corresponding eigenstates are obtained. Figure 4.17 shows a schematic illustration of the stress induced change of the three valence bands for a compressive stress. Thus the energy band gap shift at k = 0 is given by the following equations, where the approximation is valid for δ E 001 Δ0 : 1 1 Δ(Ec − Ev1 ) = − Δ0 + δ E H + δ E 001 , 3 2 1 1 Δ(Ec − Ev2 ) = Δ0 + δ E H − δ E 001 6 4 1/2 1 − Δ20 + Δ0 δ E 001 + (9/4)(δ E 001 )2 2 1 1 1 ≈ − Δ0 + δ E H − δ E 001 − (δ E 001 )2 /Δ0 + · · · 3 2 2 1 1 Δ(Ec − Ev3 ) = Δ0 + δ E H − δ E 001 6 4 1/2 1 2 + Δ0 + Δ0 δ E 001 + (9/4)(δ E 001 )2 2 2 1 ≈ + Δ0 + δ E H + (δ E 001 )2 /Δ0 + · · · . 3 2

(4.179a)

(4.179b) , (4.179c)

(4.179d) (4.179e)

The wave functions under the application of stress are then given by ! 3 3 , u v1,X = , 2 2 ! 3 1 + u v2,X = , 2 2 ! 1 1 − u v3,X = , 2 2

(4.180a) ! 1 1 1 , √ α0 , 2 2 2 ! 3 1 1 , √ α0 , 2 2 2

(4.180b) (4.180c)

4.7 Piezobirefringence

205

where α0 = δ E 001 /Δ0 . Using these results the momentum matrix elements between the valence and conduction bands which determine the strength of the optical transition are calculated as | c| p |v1 |2 = 0, 1 | c| p⊥ |v1 |2 = P 2 , 2 2 2 3 2 2 | c| p |v2 | = P 1 + α0 − α0 + · · · , 3 4 1 2 3 2 2 | c| p⊥ |v2 | = P 1 − 2α0 + α0 + · · · , 6 2 1 2 3 2 2 | c| p |v3 | = P 1 − 2α0 + α0 + · · · , 3 2 1 2 3 2 2 | c| p⊥ |v3 | = P 1 + α0 − α0 + · · · . 3 4

(4.181a) (4.181b) (4.181c) (4.181d) (4.181e) (4.181f)

In the above equations P is the momentum matrix element between the |Γ25 valence band and the |Γ2 conduction band, which is written as P = c ↑ | px |X ↑ = c ↑ | p y |Y ↑ = c ↑ | pz |Z ↑ .

(4.182)

For the cases of [111] and [110] stresses the analysis is similarly straightforward and the results are given in [19]. The change in the real part of the dielectric constant due to stress is calculated from these results and (4.130a). For E 0 we find Δκ1 (ω) =

∂κ1 ∂M

v1 ,v2

+

ΔM +

∂κ1 Δω0 ∂ω0

1 ∂ 2 κ1 ∂ 2 κ1 2 Δω (Δω ) + ΔM , 0 0 2 ∂ω02 ∂ω0 ∂ M

(4.183)

where M = | c| p,⊥ |v|2 . This may be rewritten as Δ0 (κ1 ) − (κ1 )⊥ = α0 f (x0 ) − g(x0 ) 4ω0 Δ0 3 g(x0 ) − α02 f (x0 ) + 4 2ω0 Δ0 1 α0 αH Δ0 g(x0 ) + l(x0 ) . + 2 ω0 4ω0 −3/2 Aω0 P 2

For the E 0 + Δ0 gap, we obtain

(4.184)

206

4 Optical Properties 1 −3/2

(κ1 )⊥ − (κ1 ) = Aω0s

P2

3 −α0 + α02 f (x0s ) 4 α0 αH Δ0 g(x0s ) , − 2ω0s

(4.185)

where f (x) = (1/x 2 )[2 − (1 + x)1/2 − (1 − x)1/2 ], g(x) = (1/x 2 )[2 − (1 + x)−1/2 − (1 − x)−1/2 ],

(4.186a) (4.186b)

l(x) = (1/x 2 )[2 − (1 + x)−3/2 − (1 − x)−3/2 ], x0 = ω/ω0 , x0s = ω/ω0s , αH = δ E H /Δ0 .

(4.186c) (4.186d)

When we take account of the E 0 , E 0 + Δ0 , E 1 , E 1 + Δ1 and E 2 critical points, the real part of the dielectric constant in the presence of a [100] stress is given by [16] 4ω0 ω0 3/2 f (x0 ) − f (x0s ) (κ1 ) − (κ)⊥ = C0 X −g(x0 ) + Δ0 ω0s 2 1 2 1 2 ω1 1 + x1s = C1 X 1 + x1 − 2 ω1s 2 % $ (4.187) +C2 X 1 + 2x22 . The piezobirefringence experiment is carried out by using the setup shown in Fig. 4.18. The light from the source is chopped into pulses, dispersed by a monochromator. The polarizer is oriented so that the beam incident on the sample is polarized at 45◦ to the stress axis. Under these conditions, the light components polarized parallel and perpendicular to the stress are equal. The signal is obtained as a function of

Fig. 4.18 Experimental setup for piezobirefringence measurements. P and A are the polarizer and analyzer, respectively, S is the sample, D is the detector, C is the light chopper, and the load cell is a stress transducer to detect the stress magnitude

207

⁄

4.8 Problems

Fig. 4.19 Piezobirefringence coefficient [(κ1 ) − (κ1 )⊥ ]/ X of GaAs plotted as a function of photon energy [16]. The calculated result from (4.187) is shown by a solid curve fitted to the experimental data. The critical point energies are those listed in Table 4.3 and C0 = −0.51, C1 = −10.0, C2 = 3.6 [10−11 cm2 /dyne]

stress for the analyzer with its polarization plane either perpendicular or parallel to that of the polarizer. The signal intensity is given by [16] I =

1 I0 (1 ± cos Δ), 2

(4.188)

where Δ is the phase difference between the parallel and perpendicular components of the transmitted light, and is given by (4.149) or (4.150). The symbol ± corresponds to the configuration of the analyzer with respect to the polarizer, parallel or perpendicular. The transmitted light intensity oscillates as a cosine function with a frequency depending on the stress, and thus the relation between Δ/t and stress X is obtained. When we plot Δ/t as a function of X , the slope with the help of (4.150) gives [(κ1 ) − (κ1 )⊥ ]/ X . The measured data are plotted as a function of photon energy in Fig. 4.19, where the calculated result from (4.187) is shown by a solid curve fitted to the experimental data. It is evident from Fig. 4.19 that piezobirefringence in GaAs is well explained by the theory stated above. From the analysis we may deduce the deformation potentials.

4.8 Problems (4.1)

Disregarding the relation, calculate reflectivity R as a function real part of dielectric constant κ1 for κ2 = 0.1, 5.0 and 10 and show the result in figure.

(4.2)

We assume that a conduction band and a valence band are given by

208

4 Optical Properties 1

2 k 2 + EG 2m c 2 k 2 Ev = 2m v Ec =

where EG is the band gap, and Ecv =

2 2 k + EG , 2μ

1 1 1 = + μ mc mv

(1) Calculate the joint density of states by using (4.42). (2) Calculate the joint density of states by using (4.44). (4.3)

Absorption coefficient due to indirect transition is shown in Fig. 4.6. Explain the temperature dependence of the absorption coefficient with respect to the following two features: (1) Absorption coefficient increases with temperature. (2) A clear bending point is observed at a low temperature.

(4.4)

Derive the real part of the dielectric function κ1 (ω) given by equations (4.130a) and (4.130b) by applying Kramers–Kronig relation to the imaginary part of the dielectric function (4.128) for the E 0 gap.

(4.5)

Express the dielectric functions κ2 and κ1 as a function of x = ω/ω0 with parameters A, P02 , and ω0 = EG /.

(4.6)

Evaluate the coefficient A P02 ω0 for GaAs with the parameters EG = 1.51 eV, E P0 = 28.8, and the reduced mass μi = μ = 0.067 m.

(4.7)

Plot κ2 (x) and κ1 (x) as a function of x using the parameters given above for GaAs for E 0 transition. Since the E 0 critical point reflects the transition from the heavy and light hole bands to the conduction band, we may put 2C0 as stated in the text.

(4.8)

Derive real part of the dielectric constant of GaAs at the band edge from (4.130a) for E 0 transition. The material constants are EG = 1.51 eV, E P0 = 28.8. The reduced mass μi is assumed to be the conduction electron effective mass m ∗c = 0.067 m. (1) Evaluate κ1 for the case of simple bands with a conduction band and a heavy hole band. (2) Evaluate κ1 for the case with three valence bads with spin–orbit split band. (3) At higher temperature the energy pap EG becomes smaller. Evaluate above two cases for EG = 1.43 eV.

−3/2

References

209

References 1. P.Y. Yu, M. Cardona, Fundamentals of Semiconductors (Springer, Heidelberg, 1996) 2. J.O. Dimmock, in Semiconductors and Semimetals, vol. 3, ed. by R.K. Willardson, A.C. Beer (Academic Press, New York, 1967), pp. 259–319 3. F. Abelès, (ed.), Optical Properties of Solids (North-Holland, Amsterdam, 1972) 4. D.L. Greenaway, G. Harbeke: Optical Properties and Band Structure of Semiconductors (Pergamon, New York, 1968) 5. L. van Hove, Phys. Rev. 89, 1189 (1953) 6. M. Cardona, Modulation Spectroscopy, ed. by F. Seitz, D. Turnbull, H. Ehrenreich (Academic Press, New York, 1969) 7. B. Batz, Semiconductors and Semimetals, vol. 9, ed. by R.K. Willardson, A.C. Beer (Academic Press, New York, 1972) 8. G.G. MacFarlane, V. Roberts, Phys. Rev. 98, 1865 (1955) 9. G.G. MacFarlane, T.P. McLean, J.E. Quarrington, V. Roberts, Phys. Rev. 108, 1377 (1957) 10. R.J. Elliott, Phys. Rev. 108, 1384 (1954) 11. H. Haug and S.E. Koch, Quantum Theory of the Optical and Electronic Properties of Semiconductors (World Scientific, Singapore, 1993), Chaps. 10–11 12. M.D. Sturge, Phys. Rev. 127, 768 (1962) 13. M. Gershenzon, D.G. Thomas, R.E. Dietz, in Proceedings of the International Conference on the Physics of Semiconductors held at Exeter, vol. 1962 (The Institute of Physics and the Physical Society. London, 1962), p. 752 14. F.H. Pollak, C.W. Higginbotham, M. Cardona, J. Phys. Soc. Jpn. 21 (Suppl.), 20 (1966) 15. M. Cardona, Optical properties and band structure of germanium and zincblende-type semiconductors, in Proceedings of the International School of Physics “Enrico Fermi” on Atomic Structure and Properties of Solids (Academic Press, New York, 1972), pp. 514–580 16. C.W. Higginbotham, M. Cardona, F.H. Pollak, Phys. Rev. 184, 821 (1969) 17. P.Y. Yu, M. Cardona, J. Phys. Chem. Solids 34, 29 (1973) 18. G.E. Picus, G.L. Bir: Sov. Phys.-Solid State 1, 136 (1959); 1, 1502 (1960); 6, 261 (1964); Sov. Phys.-JETP 14, 1075 (1962) 19. F.H. Pollak, M. Cardona, Phys. Rev. 172, 816 (1968)

Chapter 5

Optical Properties 2

Abstract In this chapter precision optical spectroscopy is discussed. Modulation spectroscopy has been successfully used to investigate energy band structure of semiconductors [1–6]. Electroreflectance spectroscopy is described in detail, which is shown to be related to the third derivative form of the dielectric function with respect to the photon energy. Electric field–induced change in the dielectric functions is shown to reflect the type of the critical point. Other optical spectroscopy such as Raman scattering and Brillouin scattering is also described [7–10]. In addition, resonant Raman scattering and resonant Brillouin scattering are discussed. In the last part of this chapter we deal with coupled modes such as phonon polariton and exciton polariton, and finally free–carrier absorption and plasmon.

5.1 Modulation Spectroscopy 5.1.1 Electro-optic Effect Two phenomena are known as the electric field induced change in reflectivity. One is linearly proportional to the electric field and is known as the Pockels effect and the other is quadratically proportional to the electric field and is known as the Kerr effect. These two phenomena are called the electro-optic effect and are observed in the transparent region and thus well below the fundamental absorption edge. For example, the Pockels effect is expressed by (δκ−1 )i j = ri jk E k (≡ δβi j ) where E is the electric field applied to a crystal, (δκ−1 )i j is the i j component of the change in the inverse dielectric constant and ri jk is called the Pockels electro-optic constant. In this Section we will not go into detail on this kind of phenomenological treatment but we will consider the magnitude of the change in the dielectric constant near the fundamental absorption edge induced by the applied electric field in a semiconductor.

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2023 C. Hamaguchi, Basic Semiconductor Physics, Graduate Texts in Physics, https://doi.org/10.1007/978-3-031-25511-3_5

211

212

5 Optical Properties 2

The application of an electric field E results in the addition of the potential energy term −e E · r to the electron Hamiltonian and thus the translational symmetry is lost in the direction of the electric field. This gives rise to a mixing of the electronic states of the wave vectors k0 and k = k0 − e Et/ as discussed later. First, we will consider optical transition under an applied d.c. electric field. When the Coulomb interaction is neglected, the effective mass equation for the relative motion of an electron–hole pair is 2 2 − ∇ − e E · r ψ(r) = Eψ(r) , (5.1) 2μ or

2 d2 2 d2 2 d 2 − − − − e(E x x + E y y + E z z) ψ(x, y, z) 2μx dx 2 2μ y dy 2 2μz dz 2 = Eψ(x, y, z) , (5.2)

where μi is the value in the direction of the principal axis of the reduced effective mass tensor. The solutions of the above equation are given by the product of the wave functions ψ(x)ψ(y)ψ(z), where each function satisfies the equations. 2 d 2 − − eE r − E i i i ψ(ri ) = 0, 2μi dri2 E = E x + E y + Ez .

(5.3a) (5.3b)

Equation (5.3a) may be solved easily by changing the variables: 1/3 e2 E i2 2 θi = , 2μi Ei + eE i ri ξi = . θi

(5.4) (5.5)

Then (5.3a) can be rewritten as d2 ψ(ξi ) = −ξi ψ(ξi ) . dξi2

(5.6)

The solution of this equation is known to be given by the Airy function [11], and we obtain ψ(ξi ) = Ci Ai(−ξi ) , (5.7) where Ci is a normalization constant of the function ψ(ξ) and is given by √ Ci =

e|E i | . θ

(5.8)

5.1 Modulation Spectroscopy

213

Therefore, the solution of (5.3a) is written as ψ(ξx , ξ y , ξz ) = C x C y C z Ai(−ξx )Ai(−ξ y )Ai(−ξz ) .

(5.9)

5.1.2 Franz–Keldysh Effect For simplicity we consider the case where the electric field is applied in the x direction. Since we have E y = E z = 0, (5.3a) gives rise to

2 k 2y 2 k z2 2 d2 − + + − eE x ψ(x, y, z) = Eψ(x, y, x) 2μx dx 2 2μ y 2μz

(5.10)

and the solution is given by ψ(x, y, z) = C · Ai

−eE x − E + 2 k 2y /2μ y + 2 k z2 /2μz

× exp{i(k y y + k z z)} .

θx (5.11)

It is evident from this result that the wave function in the y, z directions is periodic, given by a Bloch function, but the localization of the electron–hole pair function occurs in the x direction due to the lack of translational symmetry due to the electric field. As an example, if we assume k y = k z = 0 and E = 0, then the wave function is written as (5.12) ψ(x) = C · Ai(−eE x/θx ) . Figure 5.1 shows a plot of the wave function as a function of x. Let us consider the one-dimensional motion of a particle with effective mass μx . In the classical picture the particle cannot penetrate into the region (x < 0) of positive potential (−eE x > 0), and thus the point x = 0 is the turning point for the motion. In the quantum mechanical picture, however, the particle can penetrate into the region x < 0

Fig. 5.1 Wave function of an electron–hole pair in a static electric field, with a tilted potential barrier. The wave function penetrates into the region x < 0 (E < V = −eE x)

214

5 Optical Properties 2

and the wave function has an exponential tail in that region as shown in Fig. 5.1. As a result, an electron in a valence band is allowed to be excited into a conduction band by absorbing a photon with its energy below the band gap. This effect is known as the Franz–Keldysh effect [12, 13] and the detailed treatment is given later. Next we discuss the effect of the electric field on the interband transition. The wave function ψ(x, y, z) given by (5.9) is the same as the envelope function described in Sect. 4.5 and represents the wave function of the relative motion of the electron–hole pair. Therefore, the imaginary part of the dielectric function κ2 (ω, E) = 2 (ω, E)/ 0 in the presence of a static electric field may be obtained byinserting (5.9) into (4.97). Replacing the summation with respect to λ in (4.97) by dEx dE y dEz , we obtain κ2 (ω, E) =

πe2 |e · pcv |2 e3 |E x E y E z | dEx dE y dE z 0 m 2 ω 2 (θx θ y θz )2

Ey Ex Ez

2 · Ai − · Ai − ×

Ai − θx θ y θz

×δ EG + Ex + E y + Ez − ω ,

(5.13)

and the evaluation of this equation for the van Hove critical points is straightforward. For example, we will show the calculations for the case of the M0 critical point (μx , μ y , μz > 0). When we assume that the electric field E is parallel to one of the principal axes, x, (E x = 0, E y = E z = 0), the results are the same as stated above. The integral with respect to dEx dE y is given by the joint density of states for the 2D (ω − EG − Ex ), and thus we obtain two-dimensional band Jcv κ2 (ω, E) =

e|E x | πe2 |e · pcv |2 0 m 2 ω 2 (θx )2

+∞

Ex

2 2D × Jcv (ω − EG − Ex ) ·

Ai − dEx . θx

−∞

(5.14)

The two-dimensional joint density of states is shown in Table 4.2, which is ⎧ (μ μ )1/2 ⎪ ⎨ B1 = y z , 2D π2 (ω) = Jcv ⎪ ⎩ 0, Then (5.14) is given by

ω > EG ω < EG .

(5.15)

5.1 Modulation Spectroscopy

215

1/2 ω−EG

Ex

2 πe2 2 e|E x ||μ y μz |

κ2 (ω, E) = |e · pcv |

Ai − θ dEx 0 m 2 ω 2 (θx )2 π2 x −∞ 1/2 8|μx μ y μz | e2 = |e · pcv |2 (θx )1/2 2 0 m 2 ω 2 6 (5.16) × |Ai (−η)|2 + η|Ai(−η)|2 , where η=

ω − EG . θx

(5.17)

Here we will discuss the properties of the Airy functions in the limiting case where the photon energy is well above the fundamental absorption edge. In the case of η 0 (η → ∞) and thus in the case of ω EG , (5.16) is approximated by using asymptotic forms of the Airy functions 1 −1/4 2 3/2 π z + , sin lim Ai(−z) = √ z z→∞ 3 4 π 1 2 3/2 π z + , lim Ai (−z) = √ z 1/4 cos z→∞ 3 4 π

(5.18a) (5.18b)

and then we find |Ai (−η)|2 + η|Ai(−η)|2 =

√ η (ω − EG )1/2 = . π π(θx )1/2

(5.19)

Insertion of (5.19) into (5.16) gives exactly the same dielectric function as that for the one-electron approximation derived in Chap. 4 (4.39). On the other hand, we find a very interesting result in the other limiting case where the photon energy is below the fundamental absorption edge. In this case we find η 0 (η → −∞) and thus ω EG . The asymptotic solutions for the Airy functions are 3C1 1 2 (5.20a) lim Ai(z) = √ z −1/4 exp − z 3/2 1 − 3/2 , z→∞ 3 2z 2 π 21C1 1 2 lim Ai (z) = √ z 1/4 exp − z 3/2 1 + , (5.20b) z→∞ 3 10z 3/2 2 π where C1 = 15/216 [11]. Therefore, the dielectric function for the incident photon energy below the band gap is

216

5 Optical Properties 2

e2 |e · pcv |2 1 8|μx μ y μz | 1/2 κ2 (ω, E x ) = (EG − ω)1/2 2 0 m 2 ω 2 2π 6 4 EG − ω 3/2 × exp − 3 θx 4 EG − ω 3/2 1 , = κ2 (ω) exp − 2 3 θx

(5.21)

or inserting this into (4.21) the absorption coefficient α is given by the relation e2 |e · pcv |2 1 8|μx μ y μz | 1/2 (EG − ω)1/2 2 0 m 2 cn 0 ω 2π 6 4 EG − ω 3/2 × exp − 3 θx 4 EG − ω 3/2 1 , = α(ω) exp − 2 3 θx

α(ω, E x ) =

(5.22)

where κ2 (ω) and α(ω) are the imaginary part of the dielectric constant without and with electric field, respectively. These results indicate that absorption occurs for an incident photon with an energy less than the band gap in the presence of an electric field and that the absorption coefficient has an exponential tail. This effect is predicted independently by Franz and Keldysh and is called the Franz–Keldysh effect. This effect is well explained in terms of the penetration of the wave function in the presence of a high electric field with the help of the illustration of Fig. 5.2, where the electron and hole penetrate into the band gap due to quantum mechanical effects and an optical transition becomes allowed in the region ω < EG . It may be expected that the absorption coefficient shows an exponential decay as the photon energy decreases. Using the result for the M0 point given by (5.16), κ2 (ω, E) and κ2 (ω, 0) are plotted in Fig. 5.3. In the absence of electric field, E = 0, the dielectric constant κ2 (ω, 0) is zero in the region ω < EG . In the presence of an electric field E = 0, however, the wave function penetrates into the band gap and the dielectric constant κ2 (ω, E)

Fig. 5.2 Illustration of Franz–Keldysh effect in a semiconductor. In the presence of a high electric field the wave functions of the electron and the hole penetrate into the band gap and an optical transition is allowed in the photon energy region below the band gap ω < EG

5.1 Modulation Spectroscopy

217

Fig. 5.3 κ2 (ω, 0)/A without electric field and κ2 (ω, E)/A with electric field are plotted as a function of photon energy near the M0 critical point

is not zero in the region below the fundamental absorption edge (ω < √ EG ), giving rise to an exponential tail. Although κ2 (ω, 0) exhibits an increase as ω − EG in the photon energy region above the fundamental absorption edge, κ2 (ω, E) exhibits an oscillatory behavior (with a modulation by a weak oscillatory component) and converges to κ2 (ω, 0) in the region well above the fundamental absorption edge.

5.1.3 Modulation Spectroscopy In the previous section we discussed the change in dielectric constant in the presence of an electric field. The change is pronounced near critical points such that it decreases exponentially below the fundamental absorption edge and oscillates beyond the edge, converging to the dielectric constant without electric field at higher photon energies. When we introduce new variables, (5.16) is written as ω −ω 1 Ai , dω 2 κ2 (ω , 0) κ2 (ω, E) = ω |Ω| Ω −∞

∞

ω

2

(5.23)

where Ω (Ω has the dimensions of energy) is defined by Ω=

θ 22/3

=

(θx θ y θz )1/3 = 22/3

e2 E 2 8μ E

1/3 (5.24)

and μ E is the reduced mass in the direction of the electric field. It should be noted that (5.23) behaves as κ2 (ω, 0) but modulated by the Airy function and that the behavior arises from the mixing of the different states of k induced by the electric field, as pointed out earlier. The change in the dielectric constant in an electric field is quite small and even in an available high electric field such as (≤105 V/cm) will give rise to a change of a small fraction. Therefore, it is very difficult to observe the exponential tail and oscillatory behavior of the dielectric constant shown in Fig. 5.3. However, applying

218

5 Optical Properties 2

Fig. 5.4 Experimental setup for modulation spectroscopy. Different modulation methods produce different types of modulation spectroscopy

a periodically oscillating electric field and using a phase-sensitive detector (lock-in amplifier), the change in dielectric constant Δκ Δκ(ω, E) = κ(ω, E) − κ(ω, 0)

(5.25)

can be measured with high accuracy. This method is often referred to as electroreflectance or electroabsorption and has been applied to study the optical properties of semiconductors in the region from the ultraviolet to the infrared since the 1960s and gives us very important information about the band structure of semiconductors. The method is also called modulation spectroscopy, including many other modulation methods. In general modulation spectroscopy is carried out by using the experimental setup shown in Fig. 5.4. Modulation methods have been reported so far such as electric field modulation (electroreflectance), laser excitation (photoreflectance), applying high current to a sample or to a sample holder and modulating the sample temperature (thermoreflectance) and stress modulation by using a piezoelectric element (piezoreflectance), and so on. Let us the dielectric constant of the sample is κ = κ1 + iκ2 and the modulation is uniform in the modulated sample, then the relation between the change in the reflectance ΔR/R and the change in the dielectric constants Δκ1 and Δκ2 is given by ΔR = α(κ1 , κ2 )Δκ1 + β(κ1 , κ2 )Δκ2 . (5.26) R The above relation is easily calculated to give the following result by using (4.13) R=

(κ21 + κ22 )1/2 − [2κ1 + 2(κ21 + κ22 )1/2 ]1/2 + 1 , (κ21 + κ22 )1/2 + [2κ1 + 2(κ21 + κ22 )1/2 ]1/2 + 1

and the coefficients are given as follows:

(5.27)

5.1 Modulation Spectroscopy

219

2γ , + δ2 2δ , β= 2 γ + δ2 n(n 2 − 3k 2 − n 0 ) , γ= n0 k(3n 2 − k 2 − n 0 ) δ= , n0

α=

(5.28a)

γ2

(5.28b) (5.28c) (5.28d)

where n 0 is the refractive index of the non-absorbing medium of incidence and assumed to be n 0 = 1 for the air or vacuum. Note here that n and k are the refractive index√ and the extinction coefficients of a semiconductor as defined in Sect. 4.1 (n + ik = κ1 + iκ2 ). The coefficients α and β are functions of the incident photon energy and are called the Seraphin coefficients [14]. The spectra of the electric field induced change in the dielectric constant Δκ(ω, E) have been calculated for all the critical points under the assumption of the oneelectron approximation and parabolic energy bands [15, 16]. For example, the change for the M0 critical point is obtained from (4.39) and (5.16) as Δκ2 (ω, E) = κ2 (ω, E) − κ2 (ω, 0) = A · {π[Ai2 (−η) + ηAi2 (−η)] − u(η) ·

√

η}

≡ A · F(−η) .

(5.29)

The real part of the dielectric function is easily derived through the Kramers–Kronig transform given by (4.126a), giving rise to Δκ1 (ω, E) = A · G(−η) ,

(5.30)

where the functions F(−η) and F(−η) are √ F(−η) = π[Ai2 (−η) + ηAi2 (−η)] − η · u(η) , √ G(−η) = π[Ai (−η) · Bi (−η) + ηAi(−η) · Bi(−η)] + −η · u(−η) ,

(5.31a) (5.31b)

and u(x) is the step function such that u(x) = 0 for x < 0 and u(x) = 1 for x ≥ 0. The coefficient A is defined as e2 |e · p|2 A= 2π 0 m 2 ω 2

8|μx μ y μz | 6

1/2 |θ|1/2 .

(5.32)

These functions are shown in Figs. 5.5 and 5.6. From these considerations we find that the change in the dielectric functions exhibit spectra rich in structures reflecting the critical points. The component of the modulated dielectric function is quite weak but phase-sensitive detection with the

220

5 Optical Properties 2

Fig. 5.5 Electric field-induced change in the real part of the dielectric constant for the M0 critical point Δκ1 (ω, E)

Fig. 5.6 Electric field-induced change in the imaginary part of the dielectric constant for the M0 critical point

help of a lock-in amplifier provides clear spectra with high signal-to-noise ratio. These features are well displayed in Fig. 5.7. The upper part of the figure shows the reflectivity of GaAs as a function of photon energy and several peaks are noticed such as the E 1 , E 1 + Δ1 and E 2 critical points, but the critical points E 0 and E 0 + Δ0 are not well resolved. On the other hand, the lower part of the figure shows electroreflectance spectra of GaAs, where all the critical points E 0 , E 0 + Δ0 , E 1 , E 1 + Δ1 , E 0 , and E 2 are well resolved with high signal-to-noise ratio. The electroreflectance spectra are affected by the uniformity and strength of the applied electric field, exciton effects and so on, and thus the spectra are not obtained in the same sample and in the same experiment. However, measurements in the relevant region of photon energy will provide similar spectra to those found in the literature.

5.1.4 Theory of Electroreflectance and Third-Derivative Form of Aspnes Electroreflectance experiments and their analysis have revealed that the obtained spectra do not exhibit Franz–Keldysh oscillations but very simple structures. From the detailed analysis the spectra were found to agree well with the third derivative of the

5.1 Modulation Spectroscopy

221

Fig. 5.7 Spectra of reflectance and electroreflectance of GaAs at room temperature (300 K) in the photon energy region from near infrared to ultraviolet. The critical points are not well resolved in the reflectance spectra, whereas the electroreflectance spectra exhibit sharp structures near the critical points and the critical points are easily identified with good accuracy. The reflectance data are from [17]

dielectric function with respect to the photon energy. This effect was found by Aspnes [6, 18–20] and is called the third derivative form of Aspnes, cited often as thirdderivative modulation spectroscopy. The principle of third-derivative modulation spectroscopy is illustrated in Fig. 5.8. In the case of static modulation, the periodicity of the lattice is preserved and thus no mixing of the electronic states occurs, resulting only in the displacement of the critical point, as shown in the upper part of Fig. 5.8. Therefore, static modulation gives rise to the first-derivative form of the dielectric function. This is the case for stress modulation, thermo-modulation and so on. For example, let us consider the change in the band gap ΔωG (X ), which is given by Δκ2 (ω, X ) = κ2 (ω, X ) − κ2 (ω, 0) =

dκ2 (ω, 0) ΔωG (X ) . dω

(5.33)

On the other hand, the application of an electric field gives rise to a potential energy term −eE x and to a lack of periodicity in the electric field direction (x). As a result such transitions as those shown in the lower part of Fig. 5.8 become possible. In order to understand the theory of third-derivative modulation spectroscopy, a qualitative discussion will be given first and then we will present its theoretical analysis. Equation (4.39) of Sect. 4.3 or (4.128) of Sect. 4.6 may be rewritten as κ2 = C ·

1 [E − (Ec − Ev )]1/2 , E2

(5.34)

where Ec and Ev are the bottom of the conduction band and the top of the valence band, respectively, and E = ω is the photon energy. The constant C contains the

222

5 Optical Properties 2

Fig. 5.8 Schematic illustration of the change in the imaginary part of the dielectric constant. The upper figure is the case for a static external force (such as stress modulation) which preserves the periodicity of the lattice, and the change in the dielectric constant is given by the first derivative of the dielectric function with respect to photon energy. On the other hand, electric field modulation breaks the lattice periodicity and the perturbation will give rise to a mixing of the electronic states, resulting in a complicated structure of the change in the dielectric constant. See text for details

momentum matrix element, the effective mass and so on and is assumed to be constant in the region near the critical point we are concerned with. The time required for the transition is estimated from the Heisenberg uncertainty principle as τ=

. E − (Ec − Ev )

(5.35)

Under the electric field E x an electron–hole pair with the reduced mass μ will move a distance x given by x =−

2 eE x eE x 2 τ =− . 2μ 2μ [E − (Ec − Ev )]2

(5.36)

This displacement is caused by the term −eE x of the potential energy of the Hamiltonian. The term gives rise to a perturbation to the electron in the conduction band and the hole in the valence band, and as a result produces a change in the energy given by 2 e2 E x2 . (5.37) Δ(Ec − Ev ) = 2μ [E − (Ec − Ev )]2

5.1 Modulation Spectroscopy

223

The change in the dielectric constant due to the change in energy is estimated from (5.34) as Δκ2 = =

2 dκ2 e2 E x2 · Δ(Ec − Ev ) = −C d(Ec − Ev ) 4μ E 2 [E − (Ec − Ev )]5/2 3 22 e2 E x2 ∂ 3 2 4 3 ∂ (E κ ) = (θ ) (E 2 κ2 ) . 2 x 3μ E 2 ∂E 3 3E 2 ∂E 3

(5.38)

In a similar fashion the change in the real part of dielectric constant is estimated.1 From this qualitative analysis, we find that the change in the dielectric constant due to an applied electric field is expressed by the third derivative of the dielectric constant with respect to the photon energy. Aspnes [6, 18, 20] has shown from analysis of ellipsometry measurements that the third derivative of the dielectric constant shows good agreement with the electroreflectance data. Theoretical analysis of third-derivative modulation spectroscopy has been done by Aspnes and the outline of his treatment is given below. Several methods have been reported for the derivation and the details are given in the paper by Aspnes and Rowe [19]. The dielectric constant is expressed as follows in terms of the energy E, broadening constant Γ , and electric field E [19] (the dielectric function is derived from the polarization current under the one-electron approximation and from its Fourier transform): κcv (E, Γ, E)

∞ e2 1t 3 = 1+ eE d k dt e · pcv k − 0 m 2 ω 2 B.Z. 2 0 1t e E exp[i(E + iΓ )t/] × e · pcv k − 2 t/2 × exp −i (dt /)Ecv (k − e Et /) . (5.39) −t/2

In the above equation the integral with respect to t is carried out by expanding the exponential term in the following way under the condition of weak electric field: t 1 (dt /)Ecv (k − e Et /) Ecv + t 3 Ω 3 , 3 −t/2

(5.40)

1 2 e 2 E 2 2 e (E · ∇k )2 Ecv = 3 8μ

(5.41)

exp −i

t/2

where (Ω)3 =

1

Use (5.96) and the calculations are straightforward [3].

224

5 Optical Properties 2

and the relation between θ defined by (5.4) and Ω is given by (5.24). From this result (5.39) is rewritten as κcv (E , Γ, E) =

iQ πω 2

∞

d3 k B.Z.

0

dt 1 exp − it 3 Ω 3 + it (E + iΓ − Ecv )/ , (5.42) 3

where the relative dielectric constant of 1 for air is omitted. Q is given by Q=

2 πe2 |e · pcv |2 · , 0 m 2 (2π)3

(5.43)

where we have assumed that Γ |Ω|. In addition we assume that the integration may be carried out in the region where −it 3 Ω 3 /3 is not significantly large, and thus we can expand as (5.44) exp(−it 3 Ω 3 /3) = 1 − it 3 Ω 3 /3 − · · · . Then we obtain κcv (E, Γ, E) ∼

−Q πω 2 +

2Q πω 2

d3 k B.Z.

1 E + iΓ − Ecv (k)

d3 k B.Z.

(Ω)3 [E + iΓ − Ecv (k)]4

≡ κcv (E, Γ, 0) + Δκcv (E, Γ, E).

(5.45)

In the absence of an electric field, we have E = 0 and thus Ω = 0, which leads to the result −Q 1 . (5.46) d3 k κcv (E, Γ, 0) = πω 2 B.Z. E + iΓ − Ecv (k) It is evident from the Dirac delta function shown in Appendix A that the above relation is exactly the same as (4.40), (4.42) and (4.39) of Sect. 4.3 or (4.128) of Sect. 4.6. From these results we obtain the following relation 1 Δκcv (E, Γ, E) ≡ 3E 2

∂ 3 2 Ω E κcv (E, Γ, 0) . ∂E

(5.47)

Equation (5.47) agrees with the result obtained from qualitative analysis except for the constant of the prefactor. Therefore, we may conclude that the electroreflectance spectra are given by the third derivative of the dielectric function with respect to photon energy. From this fact (5.47) is referred to as the third-derivative form of Aspnes. When we keep the higher-order term in the expansion of (5.44), the experimental data show a better agreement with the theory [21].

5.2 Raman Scattering

225

Fig. 5.9 Electroreflectance spectra of GaAs at T = 300 K. The solid curve is experimental and the dotted curve is a best fit to the experimental curve using the third-derivative theory of Aspnes. In the analysis the following data were used: Eg1 = E 1 = 2.926 eV, Γ1 = 46.4 meV, θ1 = 3.275, C1 = 0.00386, Eg2 = E 1 + Δ1 = 3.153 eV, Γ2 = 59.1 meV, θ2 = 3.061, C2 = 0.003015

The third-derivative modulation spectra valid in the low electric field region are written as ΔR iθ j −m j , (5.48) = C j e (E − E j + iΓ j ) R j where E j is the energy of the jth critical point, C j is the amplitude constant, θ j is the phase constant, Γ j is the broadening constant, and means the real part of the equation. m j = 4 − d/2 depends on the dimension d of the critical point and m j = 5/2, 3, and 7/2 for 3-, 2-, and 1-dimension, respectively. Figure 5.9 shows electroreflectance spectra of n-GaAs epitaxially grown on an n+ GaAs substrate, where a semitransparent electrode of Ni on the surface of n-GaAs and a Au electrode on the back of the GaAs substrate were formed and a weak a.c. voltage was applied to the electrodes to produce electric field modulation in the low-field limit. The dotted curve is fitted to the experimental curve by using the thirdderivative form of Aspnes. It is evident from Fig. 5.9 that the electroreflectance data are well explained by the Aspnes theory. The electroreflectance measurements and analysis based on the Aspnes theory provide detailed information about the critical points. From the above analysis we obtain E 1 = 2.926 eV, E 1 + Δ1 = 3.153 eV.

5.2 Raman Scattering When an electric field E is applied to a medium, a polarization vector P is induced which is related to the field by P = 0 χE

226

5 Optical Properties 2

and its components are given by P j = 0 χ jk E k

≡ 0 χ jk E k ,

(5.49)

k

where χ jk is the electric susceptibility and is a second-rank tensor. Let us consider an electromagnetic field with frequency ω incident on the medium and express the field by the plane wave E(r, t) = E(ki , ωi ) cos(ki · r − ωi t) .

(5.50)

Then the polarization is written as P(ki , ωi ) cos(ki · r − ωi t) .

(5.51)

Therefore, we find the following relation between the amplitudes of the electric field and the polarization: P(ki , ωi ) = 0 χ(ki , ωi )E(ki , ωi ) .

(5.52)

The light scattering in which we are interested in this section is induced by a local change of the susceptibility χ. Here we are concerned with the light scattering by lattice vibrations and we express the atomic displacement by u(r, t) = u(q, ωq ) cos(q · r − ωq t) ,

(5.53)

where q and ωq are the wave vector and angular frequency of the lattice vibrations. The modes of the lattice vibrations will be described in Chap. 6. When the amplitude of the lattice vibrations is small compared to the lattice constant, the change in the susceptibility due to the lattice vibrations is expanded in a Taylor series as

(0)

χ(ki , ωi , u) = χ (ki , ωi ) +

∂χ ∂u

u(r, t) + · · · ,

(5.54)

u=0

and thus the susceptibility tensor is expressed as χ jk = χ(0) jk + χ jk,l u l + χ jk,lm u l u m + · · · ,

where χ jk,l =

∂χ jk ∂u l

, χ jk,lm = u=0

∂ 2 χ jk ∂u l ∂u m

(5.55)

.

(5.56)

u=0

It is evident from the result that χ jk,l and χ jk,lm are the third-rank and fourth-rank tensors, respectively. The first terms on the right hand sides of (5.54) and (5.55) are the susceptibility without perturbation and the terms beyond this are the compo-

5.2 Raman Scattering

227

nents induced by the perturbation. Keeping up to the second term on the right-hand side of (5.54) and inserting them into (5.52), we obtain the following result for the polarization: (5.57) P(r, t, u) = P (0) (r, t) + P (ind) (r, t, u) , and the two components on the right-hand side are given by P (0) (r, t) = χ(0) (ki , ωi ) 0 E(ki , ωi ) cos(ki · r − ωi t), ∂χ P (ind) (r, t, u) = u(r, t) 0 E(ki , ωi ) cos(ki · r − ωi t) . ∂u u=0

(5.58) (5.59)

The term P (ind) in the above equation is the polarization induced by the lattice vibrations and is related to Raman scattering. It is rewritten as: P (ind) (r, t, u)

∂χ u(q, ωq ) cos(q · r − ωq t) 0 E(ki , ωi ) cos(ki · r − ωi t) ∂u u=0 ∂χ 1 = 0 u(q, ωq )E(ki , ωi ) 2 ∂u u=0 × cos{(ki + q) · r − (ωi + ωq )t} + cos{(ki − q) · r − (ωi − ωq )t} . (5.60)

=

The above results are understood as follows. The polarization P (ind) consists of the Stokes shifted wave with wave vector kS = (ki − q) and angular frequency ωS = (ωi − ωq ) and of the anti-Stokes wave with wave vector kAS = (ki + q) and angular frequency ωAS = (ωi + ωq ). In Raman scattering experiments, therefore, we observe two scattered beams, one is a Stokes shifted wave and the other is an antiStokes shifted wave. In other words, these two different scattered lines appear on both sides of the laser line shifted by the phonon frequency and the shift is called the Raman shift. In the scattering event the energy conservation law and momentum conservation law hold: ωi = ωs ± ωq ,

(5.61)

ki = ks ± q,

(5.62)

where the sign ± means Stokes scattering for + and anti-Stokes scattering for −. Since the difference between ωi and ωs is small, |ki | and |ks | are almost the same. In this case the scattering angle θ in Fig. 5.10a is given by q = 2ki sin(θ/2) .

(5.63)

228

5 Optical Properties 2

Fig. 5.10 Geometry of the light scattering experiment. a General case, b right-angle (90◦ ) scattering geometry, and c back scattering geometry. ki is the wave vector of the incident photon, ks is the wave vector of the scattered photon, and q is the phonon wave vector

From these discussions we may understand that the intensity of the Raman scattering is determined by P (ind) . In the following we will derive the Raman scattering intensity, where the intensity is defined by using the Raman tensor. Here we will discuss the Raman tensor first. The polarization due to the lattice vibrations χi j is defined by χi j = χi(0) χi j,k u k + χi j,kl u k u l + 0(u 3 ) , (5.64) j + k

where χi j,k =

∂χi j ∂u k

k,l

, u=0

χi j,kl =

∂ 2 χi j ∂u j ∂u l

.

(5.65)

u=0

The term proportional to u gives the first-order Raman scattering and the first derivative of χ of the above equation is called the first-order Raman tensor. In a similar fashion the second derivative of χ gives second-order Raman scattering, which will not be discussed in detail. It is evident that χi j,k is the third-rank tensor and its non-zero components are determined from the crystal symmetry. The intensity of the first-order Raman scattering has been derived by Smith [22], and the result for the intensity of unpolarized light is given by Is =

3ωs4 LdΩ |χzy,x |2 (n q + 1) , ρc4 ωq

(5.66)

where L is the sample length along the light wave vector ki , ρ is the crystal density, n q is the occupation number of phonons (given by Bose–Einstein statistics), and dΩ is the detector solid angle. The above equation is for Stokes scattering, and the intensity for anti-Stokes scattering is obtained by replacing n q + 1 by n q . The result is derived from classical mechanics and its quantum mechanical treatment will be described later.

5.2 Raman Scattering

229

In standard experiments, Raman scattering is measured by using polarized light, and the electric polarization to produce the scattering is expressed as P

(ind)

∝

∂χi j ∂χ (i) u k (q, ωq ) · e(i) u(q, ωq ) · e = ∂u ∂u k

(i) k = (χi j,k )u k · e(i) j ∼ R ji · e j ,

where e(i) is the unit polarization vector of the incident light. The scattered light intensity of the polarization direction e(s) is given by e(s) · P (ind) , and thus we obtain for the scattered intensity

2

2

(s)

(i)

(i) k (s) 2 ∂χ (i)

k (s)

u · e ∼ e · R ji · e ∼ e j R ji ei

, Is ∝ e · ∂u

(5.67)

where the subscripts i, j, k mean the x, y, z components, and the superscripts (i) and (s) are for incident and scattered light, respectively. As mentioned before, χi j,k is the third-rank tensor, and χi j,k multiplied by a displacement vector u = ξ · u (ξ is the unit vector of the displacement) results in the second-rank tensor. In other words χi j,k u k ∼ R kji ξk χi j,k · u = k

k

is the second-rank tensor and its non-zero components are determined by the crystal symmetry. For the same reason the Raman tensor R kji or χi j,k is determined by the crystal symmetry. The Raman tensor R kji depends on the incident light polarization j, scattered (Raman) light polarization i, and phonon polarization k. The unperturbed susceptibility χi(0) j is a second-rank tensor. In the case of Raman scattering the frequencies of the incident and scattered light are different, and thus the Raman tensor R kji (χi j,k ) is no longer a second-rank tensor in the strict sense. The Raman tensor determines the selection rule of Raman scattering, and Raman scattering and infrared absorption are complementary. The Raman tensor χi j,k = (∂χi j /∂u) reflects the crystal symmetry. As an example, we consider the Raman tensor of a crystal with inversion symmetry. The Raman tensor of a crystal with inversion symmetry is invariant under the operation of inversion, whereas there are two types of phonon modes: one does not change sign under the inversion operation (even parity) and the other changes sign under the inversion operation (odd parity). Since the displacement u of a phonon mode with odd parity changes sign under the inversion operation, the sign of χi j,k = (∂χi j /∂u) is changed. In other words, we may conclude that the Raman tensor for the phonon modes with odd parity vanishes. It should also be noted that phonons with odd parity are infrared-active and phonons with even parity are infra-red-inactive. It is well known that a crystal without inversion symmetry exhibits piezoelectricity. As an example we consider a zinc blende crystal such as GaAs. Piezoelectricity is a

230

5 Optical Properties 2

phenomenon in which a strain e jk induces an electric field, and the i component of the electric field E i is related to the strain according to E i = ei jk e jk , where ei jk is a piezoelectric constant and a third-rank tensor. The definition of strain is given in Appendix C. Here we adopt the contraction of the subscripts of the tensor defined in Appendix C: x x = 1, yy = 2, zz = 3, yz = zy = 4, zx = x z = 5, and x y = yx = 6 for jk. Then the piezoelectric constant tensor of a cubic crystal Td is given by ⎤ ⎡ 0 0 0 e14 0 0 ⎣ 0 0 0 0 e14 0 ⎦ , (5.68) 0 0 0 0 0 e14 and its non-zero components consist of one independent constant e14 . The non-zero components arise from the components x yz, yzx, zx y. The Raman tensor R kji is expected to have the same properties as the piezoelectric tensor. Detailed analysis has been done with the help of group theory. Here we adopt the notation used so far and express the Raman tensor by the 3 × 3 matrices. ⎡

x x R yz , Rzy

⎤ ⎡ ⎤ ⎡ ⎤ 000 00d 0d0 y z = ⎣ 0 0 d ⎦ , Rzx , Rxyz = ⎣ 0 0 0 ⎦ , Rxz y , R yx = ⎣d 0 0⎦. 0d 0 d00 000 (5.69)

As described earlier, the Raman tensor ( k R kji ) is a second-rank tensor and it may be possible to express it by an irreducible representation as is the case for the strain tensor. Referring to Appendix C, the Raman tensor shown above belongs to the Γ4 group. Using (C.15) in Appendix C we obtain the following result: ⎡

⎤ a00 R(Γ1 ) = ⎣ 0 a 0 ⎦ , 00a ⎡ ⎤ ⎡ b0 0 b 0 √ R(Γ3 ) = ⎣ 0 b 0 ⎦ , 3 ⎣ 0 −b 0 0 −2b 0 0 ⎡ ⎤ ⎡ ⎤ 000 00d ⎣0 0 0⎦, R(Γ4 ) = ⎣ 0 0 d ⎦ , 0d 0 d00

(5.70) ⎤ 0 0⎦, 0 ⎡ ⎤ 0d0 ⎣d 0 0⎦. 000

(5.71)

(5.72)

x The Raman tensor R(Γ4 ) of the above equation is equivalent to Rxz y , R yz and so on of √ from the normalization of the basis functions (5.69). The factor 3 of (5.71) arises √ √ shown in Appendix C such as (1/ 2)(ex x − e yy ) and (1/ 6)(ex x + e yy − 2ezz ).

5.2 Raman Scattering

231

Table 5.1 Raman tensors of a cubic crystal and Raman-active phonon modes ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ a 00 b00 b00 00 0 00d ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎣0 a 0⎦ ⎣0 b 0⎦ ⎣0 b 0⎦ ⎣0 0 d ⎦ ⎣0 0 0⎦ 00a 00b 00b 0d 0 d 00 T Th O Td Oh

A Ag A1 A1 A1g

E Eg E E Eg

E Eg E E Eg

F(x) Fg Fg F2 (x) F2g

F(y) Fg Fg F2 (y) F2g

⎡

⎤ 0d 0 ⎢ ⎥ ⎣d 0 0⎦ 0 00 F(z) Fg Fg F2 (z) F2g

When we use the form of the strain tensor (C.16) in Appendix C, (5.71) is rewritten as ⎡ ⎤ ⎡ ⎤ b00 b00 R(Γ3 ) = ⎣ 0 b 0 ⎦ , ⎣ 0 b 0 ⎦ . (5.73) 00b 00b In the above equation two equivalent tensors are listed because the phonons are doubly degenerate. A table of Raman tensors have been reported which are obtained with the help of group theory. In this section we show the Raman tensors in Table 5.1 derived by Loudon [8], where the modes with (x), (y), and (z) are both Raman-active and infrared-active with the polarization direction x, y, and z, respectively. It should be noted that all of the Raman-active modes are not observed as the first-order Raman scattering. As shown in the previous example of a crystal with Td symmetry, optical phonons have Γ4 symmetry and phonons with Γ1 (A1 ) and Γ3 (E) symmetry are not optical phonons. These phonon modes are normally observed as the secondorder Raman scattering. Also, it should be noted that Table 5.1 obtained under the assumption of infinite phonon wave vectors (wave vector: q = 0) and that the tensors are classified with the help of the point group of the crystals. In experiments on Raman scattering, phonons with the wave vector q = 0 are involved.

5.2.1 Selection Rule of Raman Scattering Here we will discuss the first order Raman intensity (single phonon Raman scattering) using the results obtained above. For the purpose of better understanding, we will consider Raman scattering in a crystal with inversion symmetry (Oh group) and a crystal without inversion symmetry (Td group). From Table 5.1 we find that optical phonons in a crystal with inversion symmetry Oh consist of triply degenerate F2 g (Γ25 ) phonons at the Γ point: two transverse optical phonon modes and one longitudinal phonon mode. The scattering intensity is given by

232

5 Optical Properties 2

I =A

(s) e(i) j R ji ei

2 ,

(5.74)

j,i=x,y,z

where A is a constant determined from by the material and the scattered photon (s) are the j and i components of the unit polarization frequency, and e(i) j and ei vector of the incident and scattered light. Referring to Fig. 5.10a, we calculate the scattering intensity for the two cases where the polarization of the scattered light is parallel and perpendicular to the scattering plane (x, z plane), respectively. Noting that the summation is carried out for degenerate phonon modes, the intensities for the two cases are given by 2 2 2 (i) (i) (i) I = A ex Rx z + e y R yx + e y R yz = A|d|

2

sin θ

2

2 (i) 2 2 + e y (cos θ + sin θ)

2 , sin θ + e(i) = A|d| y 2 2 (i) 2 = A|d| ex(i) . I⊥ = A e x R x y 2

ex(i) ex(i)

2

(5.75a) (5.75b)

On the other hand, in a crystal without inversion symmetry Td the doubly degenerate transverse optical (TO) phonons and longitudinal optical (LO) phonons split. In such a case the Raman tensor depends on the phonon polarization direction. Defining the unit polarization vector of the phonons by ξ, the scattering intensity is given by I =A

(s) k e(i) j R ji ξk ei

2 .

(5.76)

j,i,k=x,y,z

For the scattering geometry shown in Fig. 5.10a, the scattering intensity for LO phonons is given by x (s) (i) z (s) 2 I (LO) = ALO e(i) y R yz ξx ez + e y R yx ξz ex 2 = ALO |dLO |2 e(i) , y sin(3θ/2) (i) z 2 2 = ALO |dLO |2 ex(i) sin(θ/2) , I⊥ (LO) = ALO ex Rx y ξz e(s) y and for TO phonons

(5.77a) (5.77b)

5.2 Raman Scattering

233

2 x (s) (i) z (s) 2 ex(i) Rxyz ξ y ez(s) + e(i) y R yz ξx ez + e y R yx ξz ex 2 2 = ATO |dTO |2 ex(i) sin θ + e(i) , (5.78a) y cos(3θ/2) (i) z 2 2 I⊥ (TO) = ATO ex Rx y ξz e(s) = ATO |dTO |2 ex(i) cos(θ/2) . (5.78b) y I (TO) = ATO

When we put ALO |dLO |2 = ATO |dTO |2 = A|d|2 , we obtain I (LO) + I (TO) = I , and I⊥ (LO) + I⊥ (TO) = I⊥ , which agree with (5.75a) and (5.75b), respectively. In the cases of the right angle scattering and back scattering geometries shown in Fig. 5.10b–c, the scattered intensities are obtained by putting θ = π/2 and θ = π, respectively. Raman scattering geometry or selection rule is often defined by ki (e(i) , e(s) )ks , where four vectors are used; two wave vectors ki and ks and two polarization vectors e(i) and e(s) for incident and scattered light, respectively. When we use this notation the selection rule of Td crystal is given by Table 5.2 in the case of back and 90◦ scattering geometries. Raman scattering experiments are usually carried out by using a laser in the visible region. The photon energy is higher than the band gap of many semiconductors such as GaAs and Si and thus the light is not transmitted. In such semiconductors the incident photon is absorbed in the surface region and thus Raman measurements with a right-angle (90◦ ) scattering geometry are not possible. In such a case the back-scattering geometry is adopted. From Table 5.2, we find that only LO phonons are detected by Raman scattering. In order to detect TO phonons by Raman scattering we have to use the following configuration. When we define new axes y and z along ¯ respectively, the Raman configurations y (z , x) y¯ and the directions [011] and [011], y (z , z ) y¯ will provide a Raman intensity proportional to |dTO |2 for TO phonons and zero for LO phonons. We now discuss the experimental results on Raman scattering. There have been numerous papers published so far and it is not the purpose of this textbook to survey all of the data. Instead, only very recent experimental results will be reported, which were obtained for the purpose of this book. First, we will show the experimental results on GaAs, which belongs to the Td group. As shown in Table 5.1, Ramanactive optical phonons are F2 (Γ4 or Γ15 after the notation of BSW). In addition, we find from Table 5.2 that LO phonons are observed by using the z(x, y)¯z configuration

Table 5.2 Selection rule for Raman scattering in the Td group (includes zinc blende crystal such as GaAs) in back scattering and right-angle scattering geometries Scattering geometry Selection rule TO phonons LO phonons Back scattering 90◦ scattering

z(y, y)¯z ; z(x, x)¯z z(x, y)¯z ; z(y, x)¯z z(x, z)x z(y, z)x z(x, y)x

0 0 |dTO |2 |dTO |2 /2 |dTO |2 /2

0 |dLO |2 0 |dLO |2 /2 |dLO |2 /2

234

5 Optical Properties 2

in the (001) plane of GaAs, and that TO phonons are detected by using the x (z , y )x¯ configuration in the (110) plane of GaAs. Here, [x, y, z] are the coordinates along the crystal axes and [x , y , z ] are new coordinates obtained by rotating by 45◦ around the z axis. Therefore, the (x , z ) or (y , z ) plane corresponds to the (110) plane. This definition is the same for other cubic crystals. The selection rule and the intensity of Raman scattering in the new coordinates are summarized in Fig. 5.11. Although Fig. 5.11 is for the results on Si, Oh group, the same results may be obtained for GaAs, Td group, referring to Table 5.1. Raman scattering experiments have been carried out by utilizing a double monochromator or a triple monochromator and photon counting system or a CCD camera. The data shown here are taken by a new Raman spectrometer “Ramascope” (Raman microscope) made by Renishaw which utilizes a notch filter to remove Rayleigh scattering components and provides high accuracy and convenience. Raman scattering signals of Si observed with the equipment are shown in Fig. 5.12a, where the Raman configuration is z(x, y)¯z . Under this configuration Raman scattering due to LO phonons is expected to be observed, while the experimental result shows sig-

Fig. 5.11 Raman scattering intensity for two different configurations of Si. The results on Si, Oh group, may be applied to GaAs, Td group. The intensity is obtained from Table 5.1

Fig. 5.12 Raman scattering data of GaAs at room temperature. a In addition to LO phonon scattering, which is allowed for the z(x, y)¯z configuration, a weak signal due to TO phonon scattering, which is forbidden in this configuration, is observed due to misalignment of the configuration. b For the configuration x (z , y )x¯ , TO phonon scattering is allowed but LO phonon scattering is forbidden

5.2 Raman Scattering

235

nals due to forbidden TO phonons in addition to LO phonon scattering in the region 200–300 cm−1 . The signal may arise from imperfect polarization of light and from the fact that the incident light angle depends on the depth of focus. Raman scattering due to TO phonons may be observed under the Raman configuration x (z , y )x¯ using the (100) plane, which is determined from Fig. 5.11. The results are shown in Fig. 5.12b, where a strong peak of TO phonons and a weak peak of LO phonons are observed. Temple and Hathaway [23] have reported detailed results for multi-phonon Raman scattering in Si. Referring to this paper, we discuss how to observe the firs-t and second-order Raman scattering. Experiments are carried out by utilizing the Ramascope of Renishaw in a similar way as used for GaAs. Since Si belongs to the Oh group, the phonon modes of A1 g (Γ1 ), Eg (Γ12 ), F2g (Γ25 ) are found to contribute to Raman scattering from Table 5.1. In the following we adopt the notation of BSW (Bouckaert, Smoluchowski and Wigner) (in brackets). Since optical phonons belong to Γ25 , the first-order Raman scattering arises from the Raman tensor belonging to Γ25 . The experimental results in the (001) plane of Si are shown in Fig. 5.13.

Fig. 5.13 Raman scattering observed in the (001) plane of Si at T = 300 K. (a) z(x , x )¯z configuration: all the phonon modes of representations Γ1 + Γ12 + Γ25 are observed. The peak at 519 cm−1 is due to first-order Raman scattering by Γ25 optical phonons at the Γ point, and the other signals arise from second-order Raman scattering. (b) z(x, y)¯z configuration: only Γ25 phonons will provide allowed Raman scattering. (c) z(x, x)¯z configuration: second-order Raman scattering due to phonons of representations Γ1 + Γ12 is observed. (d) z(x , y )¯z configuration: Raman scattering due to Γ12 phonons is expected. According to the slight misalignment second-order Raman scattering is observed in the region 900–1000 cm−1 in addition to the strong peak due to first-order Raman scattering

236

5 Optical Properties 2

It is evident from Fig. 5.11 that the z(x , x )¯z configuration of Fig. 5.13a enables us to observe all the phonon modes of the representations Γ1 + Γ12 + Γ25 . The strong peak at 519 cm−1 is due to one-phonon Raman scattering due to the degenerate TO and LO phonons (Γ25 ) at the Γ point. The broad peak in the region 200–450 cm−1 is due to the second-order Raman scattering of two acoustic phonons, and the peak slightly above the peak due to the one-phonon Raman scattering arises from the second-order Raman scattering of simultaneously emitted optical and acoustic phonons. The peak near 1000 cm−1 is due to second-order Raman scattering which involves two optical phonons. It should be noted here that the energy and momentum conservation rules hold for the second-order Raman scattering and that the two phonons have wave vectors in the reverse direction to each other. The intensity of the second-order Raman scattering reflects the density of states for the phonon mode and thus will provide information about the dispersion of the phonon branches. Figure 5.13b shows Raman scattering for the z(x, y)¯z configuration, where Raman scattering due to Γ25 phonons is allowed. In the figure, however, we find first-order Raman scattering due to optical phonons at the Γ point and second-order Raman scattering due to two optical phonons. Raman scattering for the z(x, x)¯z configuration is shown in Fig. 5.13c, where phonons of the Γ1 + Γ12 representations may be observed. In other word, we observe only the second-order Raman scattering due to acoustic and optical phonons except for a weak component due to Γ25 phonons. The Raman configuration z(x , y )¯z of Fig. 5.13d enables us to observe the Γ12 phonons. The second-order Raman scattering is so weak that the first-order Raman scattering due to optical phonons of Γ25 type appears, which may be caused by a slight misalignment of the optical path. Although the intensity is very low, second-order Raman scattering is observed in the region 900–1000 cm−1 .

5.2.2 Quantum Mechanical Theory of Raman Scattering The microscopic interpretation of Raman scattering is as followings. An incident photon creates an excited state of an electron from its ground state, or an electron– hole pair, and the electron or the hole (or electron–hole pair, exciton) interacts with a phonon (phonon scattering) to create a new excited state. Then the electron and the hole recombine to emit a photon. Therefore, we may expect that the scattering intensity increases rapidly when the incident photon energy approaches the fundamental absorption edge. This rapid increase is discussed later and called resonant Raman scattering. The processes are schematically illustrated in Fig. 5.14, where the conduction band and the heavy and light hole bands are considered. Figure 5.14a corresponds to the case where an excited electron is scattered by a phonon and (b) to the case of hole scattering by a phonon. In such a quantum mechanical process, three interactions are involved: (1) interaction of an incident photon with an electron in the semiconductor, (2) interaction of an exciton or electron–hole pair with a phonon, (3) recombination (the electron-hole pair with a scattered photon), and therefore the process may be treated by third-order perturbation theory of quantum mechanics.

5.2 Raman Scattering

237

Fig. 5.14 Quantum mechanical representation of Raman scattering. Interband transition induced by an incident photon, electron or hole scattering by a phonon, and emission of a scattered photon

Fig. 5.15 Representations of Raman scattering by diagrams: a after Loudon [24] and b after Yu and Cardona [3]

Theoretical analysis has been done by Loudon [24]. Usually quantum mechanical calculations have been carried out with the help of diagrams and various methods have been adopted. Among them two methods adopted by Loudon [24] and by Yu and Cardona [3] are very convenient for us. The process in Fig. 5.14 is shown by diagrams in Fig. 5.15, where (a) is after Loudon and (b) is after Yu and Cardona. In this textbook we will follow the method of Yu and Cardona. First we define the following rules to draw a diagram: (a) Excitations such as the photon, electron–hole pair and phonon are called propagators, and are drawn by dotted, solid and dashed lines as shown in Fig. 5.16. (b) The interaction between these excitations is indicated by an intersection connecting two propagators, and the intersection is called a vertex. Vertices are expressed by various notations, but here we use • for electron–photon (radiation field) interaction and for the electron–phonon interaction. (c) Propagators are drawn with arrows. The direction of the arrows represents the creation and annihilation at the interaction. An arrow toward a vertex indicates annihilation and an arrow leaving a vertex indicates creation. (d) The sequential progress of the interactions are from the left to the right and all the interactions are lined up according to this rule.

238

5 Optical Properties 2

Fig. 5.16 Propagator and vertex used to express diagrams

Fig. 5.17 Six diagrams for Raman scattering (Stokes)

(e) Once a diagram is drawn, then draw all the diagrams by changing the order of the vertices. Using these rules, 6 diagrams for Raman scattering are easily obtained by taking account of 3 vertices, which are shown in Fig. 5.17. Next, we will consider the perturbation calculations of Raman scattering. Defining an initial state by |i and the final state by |f, the scattering rate is calculated by using Fermi Golden Rule as follows. We consider the case of Fig. 5.17a as an example. The Hamiltonian to be solved is H = H0 + Her + Hel , where H0 = He + Hl is the sum of the electron and lattice vibration Hamiltonians, Her is the interaction Hamiltonian of an electron–photon pair (radiation field), and Hel is the interaction Hamiltonian for electron–lattice vibrations. The next step is to calculate the perturbation expansion of the scattering probability using the diagrams, which is shown as follows.

5.2 Raman Scattering

239

1. From the first vertex we obtain n

n|Her (ωi )|i , [ωi − (En − Ei )]

(5.79)

where |i is the initial state with energy Ei , and |n is the intermediate state with the energy En . The term ωi of the energy denominator has + sign for absorption of the quanta (photon) and − sign for emission. The summation is carried out over all the intermediate states |n. 2. Using this rule, the contribution from the second vertex is carried out and summed as n,n

n |Hel (ωq )|nn|Her (ωi )|i , ωi − (En − Ei ) − ωq − (En − En ) [ωi − (En − Ei )]

(5.80)

where |n is another intermediate state and the minus sign of the term −ωq arises from rule (1), corresponding to the phonon emission. This equation is rewritten as n,n

n |Hel (ωq )|nn|Her (ωi )|i . ωi − ωq − (En − Ei ) [ωi − (En − Ei )]

(5.81)

In a similar fashion we may take account of other vertices and obtain higher-order perturbations. 3. Note here that the total energy is conserved when we calculate the final vertex term, which is done as follows. The energy denominator for the final (third) vertex is given by

ωi − (En − Ei ) − ωq − (En − En ) − ωs − (Ef − Ei ) = ωi − ωq − ωs − (Ei − Ef ) .

(5.82)

However, the electron returns to the ground state after Raman scattering, and thus the final state |f is the same as the initial state |i. Therefore we obtain the following relation ωi − ωq − ωs . The energy conservation rule tells us that the above term should be zero. The calculation of the scattering probability is done by replacing the above term by the Dirac delta function δ[ωi − ωq − ωs ], and the scattering probability is given by

240

5 Optical Properties 2

w(−ωi , ωs , ωq ) 2π =

0|H (ω )|n n |H (ω )|nn|H (ω )|i 2 er s el q er i

ωi − ωq − (En − Ei ) [ωi − (En − Ei )]

n,n

×δ ωi − ωq − ωs .

(5.83)

In a similar fashion the calculations for other five diagrams in Fig. 5.17 are straightforward. Summing up all the contributions we obtain the following result, where the initial and final states are assumed to be the ground state |0 and we have used the relation |i = |f = |0. w(−ωi , ωs , ωq )

2π

0|Her (ωs )|n n |Hel (ωq )|nn|Her (ωi )|0 = n,n ωi − ωq − (En − E0 ) [ωi − (En − E0 )] +

0|Her (ωs )|n n |Her (ωq )|nn|Hel (ωi )|0 [ωi − ωs − (En − E0 )] [ωi − (En − E0 )]

0|Her (ωs )|n n |Hel (ωq )|nn|Her (ωi )|0 + −ωs − ωq − (En − E0 ) [−ωs − (En − E0 )] +

0|Her (ωs )|n n |Her (ωq )|nn|Hel (ωi )|0 [−ωs + ωi − (En − E0 )] [−ωs − (En − E0 )]

0|Her (ωs )|n n |Hel (ωq )|nn|Her (ωi )|0 + −ωq + ωi − (En − E0 ) −ωq − (En − E0 )

2 0|Her (ωs )|n n |Hel (ωq )|nn|Her (ωi )|0

+ −ωq − ωs − (En − E0 ) −ωq − (En − E0 )

×δ[ωi − ωq − ωs ].

(5.84)

Loudon deduced the Raman scattering intensity using the above result [8], which is shown below, where the scattering geometry is the same as in thee classical theory used by Smith (5.66): I =

e4 ωs V (n q + 1)LdΩ x 2 y 2 |R yz | + |Rzx | + |Rxz y |2 , 3 4 2 4 4 m d Mc ωq ωi

(5.85)

where e and m are the magnitude of the electronic charge and the effective mass of electron, d the lattice constant, V the volume of the crystal, M (1/M = 1/M1 + 1/M2 ) the reduced mass of the lattice atoms, and n q the phonon occupation number. x used in (5.85) is the Raman tensor defined previously and given by the following R yz relation for diamond type (Oh ) and for zinc blende type crystals(Td ):

5.2 Raman Scattering

241

x R yz (−ωi , ωs , ωq ) y z x Ξβα pα0 p0β 1 + 5 other terms , = V (ωi − ωq − ωβ )(ωi − ωα )

(5.86)

α,β

where ωα = Eα − E0 ,

ωβ = Eβ − E0

y

and pα0 = α| p y |0 is the momentum matrix element for the light polarization y. i is given by Ξαβ ¯i i u , α|Hel |β = Ξαβ d where u is the relative displacement of the optical phonons and u¯ i is the amplitude in the x direction of its quantized representation (the quantization of the lattice vibrai is the deformation potential constant defined tions will be treated in Chap. 6). Ξαβ by Bir and Picus [25]. According to the analysis of Loudon [8], the scattering efficiency is estimated to be about 10−6 to 10−7 from (5.85). It is impossible to calculate the scattering efficiency from (5.84) because of the uncertainty of the coefficients involved. Therefore, we pick up the term of the most important contribution from (5.84) and treat the other terms as background, replacing them by a constant. This approximation has been successfully used to analyze resonant Raman scattering and resonant Brillouin scattering. From these discussions we learn the relation between the macroscopic (classical) theory of the Raman tensor and the quantum mechanical result of the Raman tensor. We have to note here that relations such as χxyz = χzy,x hold from the macroscopic x . This may theory, but there are no such relations for the quantum mechanical R yz x be understood from the fact that the subscripts y, z of R yz are for the polarization x corresponds to the directions of incident (y) and scattered (z) photons and that Rzy time reversal sequence of Fig. 5.17a, from the right to the left, which should be expressed from the quantum mechanical point of view (time reversal) as x x (−ωi , ωs , ωq ) = Rzy (−ωi + ωq , ωs + ωq , −ωq ) . R yz

(5.87)

The phonon energy is much smaller than the photon energy in Raman scattering and we may safely put ωq 0 to obtain x x (−ωi , ωi , 0) = Rzy (−ωi , ωi , 0) . R yz x has the same property as χ yz,x . Therefore, we find that R yz

(5.88)

242

5 Optical Properties 2

5.2.3 Resonant Raman Scattering As shown in Fig. 5.14, Raman scattering involves the creation of an electron–hole pair as the intermediate state. Therefore, when the incident photon energy approaches the fundamental absorption edge, the efficiency of creating electron–hole pairs increases and the Raman scattering efficiency is enhanced dramatically. The resonant enhancement is called resonant Raman scattering. This enhancement is clear from the scattering efficiency obtained in Sect. 5.2.2. The strongest contribution in (5.84) comes from the diagram shown in Fig. 5.17a, which is evident from the following result. From (5.86) we put x = R yz

y z x p0β Ξβα pα0 1 , V (ωi − ωq − ωβ )(ωi − ωα )

(5.89)

α,β

and assuming that the bands are isotropic and parabolic and that the momentum matrix element is independent of the wave vector, we find x = R yz

2 y pz Ξ x p (2π)3 0β βα α0 4πk 2 dk × , k 2 k 2 B.Z. ωgβ + ωq − ωi + ωgα − ωi + 2μ 2μ

(5.90)

where ωgα and ωgβ are the energy gaps for the incident and scattered light. In the case of the zinc blende crystals shown in Fig. 4.17, ωgα = ωgβ . μ is the reduced mass of the electron–hole pair of the intermediate state and we assume that the masses are the same for the states α and β. Integration of (5.90) is easily performed by using the result shown in the first footnote of in Appendix A.1. When we put the upper bound of the integration as the band edge energies (bandwidths of the joint state of the conduction and valence bands) Δωα and Δωβ , we obtain x R yz

3/2 y z x p0β Ξβα pα0 4 2μ = · · (2π)2 ωgβ − ωgα + ωq 1/2 1/2 Δωβ × ωgβ − ωs arctan ωgβ − ωs 1/2 1/2 Δωα . − ωgα − ωi arctan ωgα − ωi

For simplicity we put ωgα = ωgβ = ωg , and then (5.91) reduces to

(5.91)

5.2 Raman Scattering

243

Fig. 5.18 The resonant term of resonant Raman scattering (resonant Brillouin scattering) calculated from (5.92) is plotted as a function of incident photon energy; ωq /ωg = 0.025 assumed. When the incident photon energy approaches the fundamental absorption edge, the scattering efficiency increases resonantly

x R yz (−ωi , ωs , ωq ) =

2μ 3/2 z x y p0β Ξβα pα0 1/2 1/2 1 ωg − ωs . × − ω g − ωi ωq 1 2π

(5.92)

x 2 The scattering efficiency |R yz | versus photon energy curve calculated from (5.92) is plotted in Fig. 5.18, where we put ωq /ωg = 0.025. It is clear from this figure that the scattering efficiency increases resonantly as the incident phonon energy approaches the band gap. From this reason the phenomenon is called resonant Raman scattering. As discussed later, we find a similar result for resonant Brillouin scattering, where the difference is the phonon energy ωq involved. Next, we will show that Raman scattering is interpreted in terms of the modulation of the dielectric function with respect to the phonon energy. This was first pointed out by Cardona [10]. This idea was introduced from the following investigation [3]. When we take into account the finite lifetime of the intermediate state, the Raman tensor is rewritten by introducing the damping constant or the broadening constant Γα as y z x p0β Ξαα pα0 x R yz = . (5.93) V α (ωs − Eα + iΓα )(ωi − Eα + iΓα )

We rewrite this equation as x R yz =

y z x p0β Ξαα pα0 ωq

k

1 1 − Ecv (k) − ωi − iΓα Ecv (k) − ωs − iΓα

, (5.94)

244

5 Optical Properties 2

where we put ωα = Eα = Ec (k) − Ev (k) ≡ Ecv (k). Using the Dirac delta function of Appendix A.1, we find the following relation: 1 1 = + iπδ [Ecv (k) − ωi ] . Ecv (k) − ωi − iΓα Ecv (k) − ωi

(5.95)

Comparing (5.95) with (4.127b), we find that the imaginary part of (5.95) corresponds to the imaginary part of the dielectric function (or electric susceptibility). In addition, assuming that the photon energy is close to the fundamental absorption edge (Ecv (k) = Eg + 2 k 2 /2μ ∼ ω), we rewrite (4.127b) as |e · pcv |2 |e · pcv |2 1 1 · 2 · = 2 2 Ecv (k) Ecv − ω Ecv (k) (Ecv + ω)(Ecv + ω) k

k

∼

|e · pcv |2 1 , 22 ω 2 Ecv (k) − ω

(5.96)

k

and this gives the real part of (5.95). From these considerations we obtain x R yz (−ωi , ωs , ωq ) ∝

1 [κ(ωi ) − κ(ωs )] . ωq

(5.97)

If the phonon energy ωq is much smaller than ωi and ωs , then (5.97) is equivalent to the first derivative of the dielectric function with respect to the energy; in other words, we obtain ∂κ(ω) x . (5.98) (−ωi , ωs , ωq ) ∝ R yz ∂(ω) Therefore, the scattering efficiency is given by

2

∂κ

I ∝

, ∂E

(5.99)

where we put ω = E. This approximation is more accurate because the phonon energy involved is much smaller [10, 26, 46]. This approximation is called the quasi-static approximation. Experiments on resonant Raman scattering have been carried out by utilizing a laser with a wavelength very close to the band gap. One of the best examples is the experiment on GaP near the E0 edge, which is shown in Fig. 5.19. In the experiment TO phonon Raman scattering is observed by using several laser lines, which is shown by +. The solid curve is calculated from (5.99) by taking into account the two band edges, the E0 edge and the spin–orbit split-off band E0 + Δ0 , whereas the dashed curve takes into account of the E0 edge only [27]. As seen in Fig. 5.19 we find good agreement between the experiment and theory.

5.3 Brillouin Scattering

245

Fig. 5.19 The Raman scattering intensity for TO phonons in GaP is plotted as a function of incident photon energy ω L , where resonant enhancement is observed at the E0 edge and the E0 + Δ0 edge. The solid curve is calculated by taking the E0 and E0 + Δ0 edges into account, whereas the dashed curve is calculated by taking account of the E0 edge only. The theoretical curves are obtained by putting (ωg + ωq ) for the band gap in the derivative form of the dielectric function (quasi-static approximation)

5.3 Brillouin Scattering Brillouin scattering involves the interaction of acoustic phonons instead of optical phonons in Raman scattering, and thus its treatment is quite similar to that for Raman scattering. While the optical phonon energy is about several 10 meV, the acoustic phonon energy involved in Brillouin scattering is about 4 × 10−6 eV = 4 µeV for 1 GHz phonons and 4 meV for 1 THz phonons. Therefore, it is very difficult to observe Brillouin scattering with the double or triple monochromator used in Raman scattering experiments. Brillouin scattering was predicted theoretically by L. Brillouin in 1922 [28]. Brillouin scattering should be included in the Pockels effect reported by F. Pockels in 1889 [29]. The Pockels effect is often referred to as the photoelastic effect, where the optical property is changed by a change in the dielectric function induced by elastic deformation of a solid. Elastic deformation includes static stress and thermal disturbance (lattice vibrations or sound propagation); the latter is to be understood as Brillouin scattering. In general, the photoelastic effect is characterized by the photoelastic constant tensor pi jkl . When a strain ekl is applied to a crystal, a change in the inverse dielectric constant δκ−1 is expressed as (δκ−1 )i j = pi jkl ekl ,

(5.100)

where pi jkl is called the photoelastic constant tensor of Pockels. From this relation we obtain (5.101) δκi j (r, t) = −κim pmnkl ekl κn j ,

246

5 Optical Properties 2

where we have dropped the summation with respect to the subscripts on the right-hand side. For simplicity we consider the cases for cubic and wurtzite crystals, where their tensors contain diagonal elements only, and then the change in dielectric constant is given by δκi j (r, t) = δχi j (r, t) = −κii κ j j pi jkl ekl .

(5.102)

The scattering efficiency, therefore, is given by an equation similar to (5.66) for Raman scattering and obtained by replacing χi j,k u k with δκi j (= δχi j ). Theoretical calculations of the Brillouin scattering cross section in cubic crystals have been reported by Benedek and Fritsch [30], in hexagonal crystals by Hamaguchi [31], and in a general form by Nelson, Lazay and Lax [32]. Although δκi j is a second-rank tensor and the same as the Raman tensor χikj u k , the change in the dielectric constant for Brillouin scattering contains the fourth-rank tensor of the photoelastic constant pi jkl , which has three non-zero components p11 , p12 and p44 for cubic crystals and five non-zero components p11 , p12 , p13 , p44 and p66 = (1/2)( p11 − p12 ), where p66 is not independent. The Brillouin scattering cross section per unit solid angle σB (ωi ) (scattering efficiency I : I ∝ σB (ωi )) is given by [32] σB ΔΩ ∝ where

2 ωi4 kB T ΔΩ

(s)

(i) χ e b a

e

, i jkl k l i j 8π 2 c4 ρvμ2 sin(θs )n (s) n (i) 1 χi jkl = − κim pmnkl κn j 2

(5.103)

(5.104)

and ω is the angular frequency of the incident light and the angular frequency of the scattered light is given by ωs = ωi ± ωq ωi . c is the light velocity, ρ the density of the material, vμ the sound velocity, ΔΩ the solid angle of the detector to collect the scattered light, ei(s) and e(i) j are the polarization directions of the incident and scattered light, respectively, θ the scattered angle inside the material, n (s) and n (i) are the refractive indices for the incident and scattered light, respectively, and bk and al are the unit displacement vector and unit wave vector of the elastic waves [32]. It should be noted that the rotational components of the strain tensor are taken into account in [32] and that the authors define a new photoelastic constant p(i j)kl instead of the photoelastic constant pi jkl used in this book. In addition Nelson et al. [32] take into account the indirect effect due to piezoelectricity, the angle between the Poynting vector and the wave vector, and the scattering volume. Therefore, the cross-section of (5.103) is different from used in the original work of Nelson et al. [32].

5.3 Brillouin Scattering

247

5.3.1 Scattering Angle First, we consider the scattering angle in a cubic or isotropic crystal. Let us define the wave vectors of the incident and scattered light inside the crystal as ki and kd , respectively, and the respective angular frequencies as ωi and ωd . The scattering is assumed to be induced by elastic waves with wave vector q and angular frequency ωμ = 2π f . The momentum and energy conservation rules are therefore written as ki ± q = kd , ωi ± ωμ = ωd .

(5.105a) (5.105b)

Using the light velocity c (≈3 × 108 m/s) and the sound velocity vμ (≈3 × 103 m/s), we obtain following relations: ωi = cki , ωd = ckd , ωμ = vμ q. Since the sound velocity vμ is much smaller than the light velocity c (vμ c), we have vμ q cki for the elastic waves of which wave vector is comparable to the incident light wave vector, and thus ωμ ωi , giving rise to ωi ∼ = ωd ,

ki ∼ = kd .

Therefore, three vectors ki , kd and q form an isosceles triangle, and the relation is expressed by using a circle as shown in Fig. 5.20a. In this case we find a relation (θˆs /2 = θˆi = θˆd ), where θˆs is the angle (scattered angle) between the incident and scattered light, and thus we obtain ˆ θs q = 2ki sin 2

(5.106)

or the frequency of the elastic waves (phonons) f is given by f =

Fig. 5.20 Wave vectors involved in Brillouin scattering for a isotropic material and b anisotropic material

ˆ 2nvμ θs , sin λ0 2

(5.107)

248

5 Optical Properties 2

where λ0 is the wavelength of the light in the air, n is the refractive index, and the relation ki = 2πn/λ0 is used. In the case of right-angle (90◦ ) scattering or back scattering shown in Fig. 5.10b or c, the scattering angle inside the crystal is the same as the outside scattering angle, and the above relation is valid. In the case where the incident or scattered light is not perpendicular to the incident plane, however, the angles θi and θd outside the sample should be calculated by using Snell law, Snell law leads to the relations sin θi = n sin θˆi , θi = θd = θs /2 and thus we obtain f =

2vμ θs sin . λ0 2

(5.108)

The angle θs is called the scattering angle outside the crystal. In a Brillouin scattering event, the scattered light polarization rotates by 90◦ with respect to the incident light polarization under some scattering configurations. When this rotation occurs in an anisotropic crystal, the anisotropy of the refractive indices induces a pronounced effect on the scattering angles. As an example we consider the case of CdS, and choose the c plane (plane perpendicular to the c axis) as the scattering plane (plane containing the incident and scattered light). Elastic waves are assumed to be transverse and the displacement vector is parallel to the c axis. Since the strain of the transverse elastic waves is ezy , the corresponding photoelastic constant is p44 = pzyzy , and thus we find that the scattered light polarization is parallel to the c axis for the incident light polarization perpendicular to the c axis. The refractive indices are different for the two different polarizations, which is called birefringence. We often use a He–Ne laser for Brillouin scattering and here we discuss the birefringence in CdS at the light wavelength λ0 = 6328 nm. The refractive indices are n o = 2.460 and n e = 2.477 for the polarization perpendicular and parallel to the c axis, respectively. Although the difference in the refractive indices is quite small, (n e − n o )/[2(n e + n o )] = 0.7%, the birefringence leads to a big effect on the scattering angle. When we define n i and n d for the refractive indices of the incident and diffracted (scattered) light, we find the following relation. ωi 2πn i ni = , c λ0 ωd ∼ ωi 2πn d nd = nd = kd = . c c λ0 ki =

(5.109a) (5.109b)

The momentum conservation rule in the presence of birefringence is shown in Fig. 5.20b, where we find an inequality θˆi = θˆd . From this figure we obtain ni nd f sin θˆi + sin θˆd = , λ0 λ0 vμ ni nd cos θˆi = cos θˆd . λ0 λ0

(5.110a) (5.110b)

5.3 Brillouin Scattering

249

Fig. 5.21 Incident angle θˆ i and diffracted (scattered) angle θˆ d inside an anisotropic crystal (CdS) plotted as a function of elastic wave frequency. The incident and diffracted angles in an isotropic crystal are given by the straight line

This will lead to the following relations [33]. vμ2 2 n − n 2d , f + f λ20 i vμ2 2 λ 0 2 cos θˆd = n − nd . f − 2n d vμ f λ20 i λ0 sin θˆi = 2n i vμ

(5.111a) (5.111b)

Therefore, the scattering angle inside the crystal θˆs = θˆi + θˆd is given by 1/2 f 2 (n i − n d )2 f θˆs sin = √ − . 2 2 nind vμ λ20

(5.112)

The incident angle θˆi and diffracted (scattered) angle θˆd are calculated by (5.111a) and (5.111b) in CdS and plotted as a function of the elastic wave frequency in Fig. 5.21, where the refractive indices used are n i = n o = 2.460 and n d = n e = 2.477. In the figure the straight line is the curve calculated for the incident and diffracted angles θˆi = θˆd = θˆs /2 for an isotropic crystal assuming that the refractive index n i = n d = (n o + n e )/2. The angles outside the crystal are calculated with the help of Fig. 5.22 and of Snell’s law: #$ 2 v λ 0 μ sin θi = n i sin sin−1 n 2 − n 2d , f + 2n i vμ f λ20 i #$ ! " vμ2 2 λ0 −1 2 cos θd = n d sin sin n − nd . f − 2n d vμ f λ20 i !

"

(5.113) (5.114)

250

5 Optical Properties 2

Fig. 5.22 Incident angle θi , diffracted angle θd , and scattering angle θs = θi + θd outside a crystal and their relations to the angles inside the crystal θˆ i , θˆ d

Fig. 5.23 Incident angle θi and diffracted (scattered) angle θd outside an anisotropic crystal (CdS) as a function of elastic wave frequency, where the refractive indices are n i = n o = 2.460 and n d = n e = 2.477

Note that the angles outside an isotropic crystal are obtained by putting n i = n d . The incident angles θi and diffracted angle θd outside a CdS crystal are calculated and plotted as a function of elastic wave frequency, which are shown in Fig. 5.23. The following result is obtained from (5.112). When the frequency of the elastic waves is % % vμ vμ n 2i − n 2d = n 2e − n 2o , (5.115) f0 = λ0 λ0 the incident angle becomes θˆi = 0. In addition, the minimum observable frequency f min is obtained by putting θˆs = 0 in (5.112), f min =

vμ vμ |n i − n d | = (n e − n o ) . λ0 λ0

(5.116)

On the other hand, the maximum observable frequency is obtained by putting θˆs = π: f max =

vμ vμ (n i + n d ) = (n e − n o ) . λ0 λ0

(5.117)

5.3 Brillouin Scattering

251

Table 5.3 Observable frequencies and other properties of elastic waves from Brillouin scattering experiments in the anisotropic crystals CdS and ZnO CdS ZnO f min f0 f max ni = no nd = ne vμ

[GHz] [GHz] [GHz]

[m/s]

0.473 0.806 13.7 2.460 2.477 1.76×103

0.736 1.130 17.3 1.994 2.011 2.74×103

As typical examples, we present f 0 , f min , and f max for CdS and ZnO in Table 5.3. From the table we find that f 0 ≈ 1GHz, f min ≈ 0.5GHz, and f max ≈ 15GHz.

5.3.2 Brillouin Scattering Experiments The phonons (elastic waves) involved in Brillouin scattering are for the acoustic modes and their energies are very small compared with the optical phonon energy involved in Raman scattering. Therefore, the frequency shift due to Brillouin scattering is quite small and its detection using a normal monochromator is extremely difficult. Brillouin scattering induced by thermal lattice vibrations (thermal phonons) is usually investigated by using the Fabry–Perot interferometer. The parallel plane Fabry–Perot (PPFP) interferometer is sometimes called the Fabry–Perot etalon, which consists of two parallel plates coated with a high dielectric constant material. When a multiple of the light wavelength is equal to the distance between the plates, interference occurs and the light is transmitted. In order to observe a small change in the wavelength, the thickness of the PPFP is controlled by a piezoelectric element or the PPFP container is evacuated to change the refractive index of the gas (air) inside. Figure 5.24 shows an example of an experimental Fabry–Perot interferometer setup for observing Brillouin scattering. In order to improve the signal-to-noise ration another PPFP is connected in series (tandem type PPFP interferometer) or the light beam is formed into multiple paths by using a prism (multiple path Fabry– Perot interferometer) [34]. Since the scattered signal is extremely weak, the signals are detected by a photon counting system or a multi-channel analyzer (MCA). We present an example of a Brillouin scattering experiment on the Si (100) surface in Fig. 5.25, where the laser line with λ = 488 nm is used. R and L in Fig. 5.25 are the Rayleigh scattering (no frequency shift) and Brillouin scattering signals due to longitudinal acoustic phonons [34]. The study of the elastic properties of solids has a long history and measurements of the velocity of have played a very important role in this aspect. The measurements of the velocity of sound have been performed by using a transducer consisting of a

252

5 Optical Properties 2

Fig. 5.24 Experimental setup to observe Brillouin scattering. PPFP is a parallel plane Fabry–Perot interferometer. Triple path of the light in the PPFP discriminates undesired components of Rayleigh scattering and improves S/N

Fig. 5.25 Brillouin scattering spectra of Si (100) surface, where R is Rayleigh scattering and L is Brillouin scattering due to longitudinal acoustic phonons

thin piezoelectric plate, which produces a resonant vibration with a frequency determined by the thickness when a.c. field is applied to the transducer. The transducer (glued onto a sample) excites elastic waves by applying an a.c. electric field and the reflected waves are detected by the transducer. The sound velocity is estimated from the delay time of the round trip of the elastic waves and the thickness of the sample. Longitudinal and transverse elastic waves are excited by choosing the crystallographic direction of the transducer, and the anisotropy of the sound velocities are easily measured by choosing the crystal axis of the samples. From these measurements the elastic constants ci jkl are determined. We have to note here that the frequency range produced by a transducer is limited to a low-frequency region from around 1 MHz to several 10s of MHz. We know that the sound velocity exhibits dispersion and that the sound velocity at high frequency becomes smaller at lower frequencies. Brillouin scattering has been used to investigate the dispersion of the lattice vibrations. Brillouin scattering provides information on the wave vector and the frequency of the lattice vibration and the frequencies are in the region of several GHz. In addition, Brillouin scattering is a kind of non-destructive measurement. From these reasons Brillouin scattering has played an important role in solid state physics.

5.3 Brillouin Scattering

253

Another successful application of Brillouin scattering is the investigation of current instabilities caused by acoustoelectric effect, which was one of the exciting topics in physics in 1960–1970. Phonons or acoustic waves (thermal noise) in a crystal are amplified through the acoustoelectric effect and traveling potential waves are excited when the drift velocity of the electron exceeds the sound velocity. Semiconductors such as CdS, ZnO, GaAs and GaSb have no inversion symmetry and thus exhibit piezoelectricity. When an electric field E is applied to such a crystal, electrons move toward the anode (in the anti-parallel direction to the electric field) with drift velocity vd = μE (μ: drift mobility). When the electron drift velocity vd exceeds the sound velocity vμ , vd > vμ , the electrons move by pushing the potential walls which are produced by the piezoelectric effect and move with the velocity of sound, resulting in an energy flow from electrons to acoustic waves and in the amplification of the acoustic waves. The amplification coefficient is proportional to γ = vd /vμ − 1 and is given by [35] γ K2 , ωσ 2 αe (ωμ , γ) = 2 γ + (ωσ /ωμ + ωμ /ωD )2

(5.118)

where K is the electromechanical coupling coefficient, ωσ = σ/κ 0 , ωD = evμ2 /μkB T , and σ = neμ is the conductivity of the semiconductor. The frequency to √ give the maximum amplification coefficient is given by f m = ωσ ωD /2π, ranging over several GHz. It is well known that the amplification of the acoustic waves excited by a transducer agrees quite well with (5.118). When an electric field is applied to a piezoelectric crystal and the condition γ > 1 is satisfied, acoustic waves with frequencies around f m are amplified. Since a crystal that is not uniform gives rise to a higher electric field in a region with higher resistivity, the amplification coefficient becomes higher, resulting in more strongly amplified acoustic waves, in this region of higher electric field. The higher electric field region, high-field domain, moves with the velocity of sound. The phonon intensity in this domain is very high, by factors of 105 –106 higher than the thermal phonon intensity (which exists as thermal noise), and parametric amplification produces phonons with a frequency of half of f m of intensity about 108 –109 higher than the thermal noise. The parametric mechanism is expressed as the amplification of frequency f /2 through the frequency conversion f = f /2 + f /2. Such high-intensity phonons are observed with a photomultiplier by adjusting the incident and scattered angles appropriately and a Fabry–Perot interferometer is not required. In addition, the domain passes by in several μs and thus the pulse signal is detected with a high signal-to-noise ratio. An example of experimental data is shown in Fig. 5.26, where we find that phonons of f m 1.4 GHz are amplified near the cathode and that lower-frequency phonons are more strongly amplified by the parametric mechanism [36]. The loss mechanisms of the amplified phonons were investigated in detail by using this method in addition to spatial and frequency distributions in GaAs [37–39] and in CdS [40].

254

5 Optical Properties 2

Fig. 5.26 Phonon spectra in acoustoelectric domain in CdS with resistivity 70 cm. Transverse acoustic waves (phonons) with displacement vector parallel to the c axis and wave vector perpendicular to the c axis are amplified by applying a high electric field and travel from the cathode to the anode with the velocity of sound. The phonon spectra are obtained at different positions from the cathode, where domains are formed at d0 = 0.1 cm, and d1 = 0.132 cm, d2 = 0.20 cm, d3 = 0.26 cm, d4 = 0.322 cm, and d5 = 0.386 cm (from [36])

5.3.3 Resonant Brillouin Scattering We have discussed Raman scattering and Brillouin Scattering in semiconductors, where all the experiments were carried out by using a laser for the incident light source. On the other hand, Garrod and Bray [41] have shown that Brillouin scattering is possible by using monochromatic light dispersed with a monochromator, if the phonons amplified via the acoustoelectric effect have sufficient intensity. They succeeded in observing the Brillouin scattering intensity by changing the incident light wavelength near the fundamental absorption edge and discovered a very interesting feature of the scattering efficiency. Figure 5.27 shows the squared photoelastic constant | p44 |2 in GaAs deduced from the Brillouin scattering as a function of incident photon energy, where | p44 |2 is proportional to the Brillouin scattering cross-section. A high electric field is applied in the [110] direction to produce an electron drift velocity faster than the sound velocity and the high-intensity phonon domain produced by the acoustoelectric effect provides strong Brillouin scattering signals, enabling us to observe Brillouin scattering near the fundamental absorption edge by using monochromatic light dispersed with a monochromator. The scattering geometry (incident and scattering angles, and polarization) is chosen to observe TA phonons of frequency 0.35 GHz and the incident light pulse is obtained from a mercury lamp dispersed with a monochromator. Since the Brillouin scattering signals

5.3 Brillouin Scattering

255

Fig. 5.27 Square of photoelastic constant p44 obtained from Brillouin scattering in GaAs as a function of photon energy, where the photoelastic constant is estimated from the Brillouin scattering 2 . Phonons, fast intensity by assuming that the Brillouin scattering intensity is proportional to p44 transverse phonons of 0.35 GHz, are amplified through the acoustoelectric effect and the Brillouin scattering cross-section is corrected by taking the absorption of the light into account. The dashed curve is obtained from piezobirefringence data [41]

are transmitted through the GaAs sample, the absorption has to be corrected near the fundamental absorption edge. The ωi4 dependence of the Brillouin scattering crosssection is also taken into account. The squared photoelastic constant | p44 |2 is thus obtained as a function of the incident photon energy, which is plotted in Fig. 5.27. The dashed curve in the figure is the photoelastic constant | p44 |2 obtained from the piezobirefringence data. We find in Fig. 5.27 that | p44 |2 becomes at minimum at around ωi = 1.38 eV, which produces a sign reversal of p44 at the photon energy. Now we will discuss the relation between the photoelastic constant and piezobirefringence. We have discussed piezobirefringence in Sect. 4.7 and shown that application of stress to a crystal results in a difference in the refractive indices for the directions parallel and perpendicular to the stress. The induced difference of the refractive indices is proportional to the stress when the stress is weak, and the change in the dielectric constant Δκ˜ corresponding to the stress tensor T˜ is written as Δκ˜ = Q˜ · T˜ ,

(5.119)

where Q˜ is called the piezobirefringence tensor and is related to α˜ defined in Sect. 4.7. When we use the strain tensor defined in Appendix C and use the relation e˜ = s˜ T˜ (˜s : elastic compliance constant), (5.102) reduces to Δκ˜ = −κ˜ κ˜ p˜ s˜ T˜ = α˜ T˜ ,

(5.120)

Q˜ = −κ˜ κ˜ p˜ s˜ = α˜ .

(5.121)

and therefore we obtain

256

5 Optical Properties 2

Next we consider two cases: stress applied to the [100] and [111] directions. For the [100] stress we obtain α(100) =

Δκ − Δκ⊥ = Q 11 − Q 12 = −κ2 ( p11 − p12 )(s11 − s12 ) , X

(5.122)

and for the [111] stress we obtain α(111) =

Δκ − Δκ⊥ = Q 44 = −κ2 p44 s44 . X

(5.123)

Now it is apparent from the above results that piezobirefringence experiments will provide the photoelastic constant p, ˜ which determines the Brillouin scattering-cross section. In Fig. 5.27 the photoelastic constants determined from the piezobirefringence experiment by Feldman and Horowitz [42] are plotted by the dashed curve, which agrees quite well with the Brillouin scattering data. In Fig. 5.28 we present experimental result on resonant Brillouin scattering in CdS, where acoustoelectric domains are also used to observe Brillouin scattering cross sections as a function of the incident photon energy. We see very clearly resonant cancellation and resonant enhancement near the fundamental absorption edge in

Fig. 5.28 Brillouin scattering cross-sections obtained from Brillouin scattering by acoustoelectric domains in CdS plotted as a function of incident photon energy. Brillouin scattering is observed by using transverse acoustic phonons (elastic waves) of 1 GHz and 0.5 GHz propagating in the c plane of CdS and the cross-sections are estimated by correcting the absorption near the fundamental absorption edge. The dash-dotted curve is calculated from (5.91) with ωgi = 2.40(2.494) eV and ωgs = 2.38(2.480) eV. The solid curve is calculated by taking the exciton effect in to account and by putting ωgi = 2.494 eV and ωgs = 2.480 eV. Both theoretical curves take into account the resonant cancellation term. (After [43])

5.4 Polaritons

257

Fig. 5.28 [43]. The theoretical curves in Fig. 5.28 are calculated by taking account of the non-resonant term R0 in (5.91): σ B ∝ |Ris − R0 |2 ,

(5.124)

where R0 is a dispersionless term arising from higher-lying critical points, and resonant cancellation occurs when Ris − R0 = 0. The dash-dotted curve in Fig. 5.28 is calculated by putting ωgi = 2.40 eV and ωgs = 2.38 eV, and the solid curve is calculated by taking account of the exciton effect and putting ωgi = 2.494 eV and ωgs = 2.480 eV. The comparison reveals that neglect of the exciton effect requires energy band gaps lower than the experimentally determined values (ωgi = 2.40 eV, ωgs = 2.38 eV) and that the theoretical curve with the exciton effect agrees quite well with the experimental data, where the binding energy of exciton Eex = 28 meV is used. These results indicate the importance of the exciton effect in CdS. In addition to Brillouin scattering by acoustoelectrically amplified phonons, different modes of phonons are excited by bonding a crystal with a different crystallographic axis to the CdS sample and injecting the acoustoelectric domains into the crystal. This phonon injection method provides resonant Brillouin scattering by different phonon modes. The experimental data are interpreted in terms of Loudon’s theory and analysis based on the dielectric function [26, 44–46].

5.4 Polaritons 5.4.1 Phonon Polaritons As discussed in Sect. 6.1.1 of Chap. 6, a crystal with two or more atoms (α atoms) in a unit cell has lattice vibration modes of 3α: 3α − 3 modes of optical phonons in addition to one longitudinal and two transverse acoustic modes. Here we consider a simple case where a crystal has two atoms in a unit cell with the masses M1 and M2 . Such semiconductors as Ge and Si with Oh crystal symmetry have the same masses and same electronic charges, and thus the relative displacement of the atoms will not induce electric polarization. Therefore, longitudinal and transverse optical phonons √ at wave vector q = 0 are degenerate and their angular frequency is given by ω0 = 2k0 /Mr (1/Mr = 1/M1 + 1/M2 , k0 : force constant). In the region q = 0, the degeneracy of the longitudinal and transverse modes are removed due to elastic anisotropy. On the other hand, GaAs has no inversion symmetry (Td group), and electronic polarization is induced due to the difference in ionicity of the atoms, resulting in removable of the degeneracy of the longitudinal and transverse optical phonons at q = 0. Let us assume that the lattice consists of atoms with their masses M+ and M− and with electronic charge +e∗ and −e∗ . In order to take into account the electric

258

5 Optical Properties 2

field induced by polarization, we use the local electric field E loc . The equations of motion for the displacement u+ and u− are then written as d2 u+ = −2k0 (u+ − u− ) + e∗ E loc dt 2 d2 u− M− 2 = −2k0 (u− − u+ ) − e∗ E loc , dt M+

(5.125a) (5.125b)

where the local field is defined by E loc = E + P/3 0 by using the applied external electric field E. From these equations we obtain Mr

d2 (u+ − u− ) = −2k0 (u+ − u− ) + e∗ E loc . dt 2

(5.126)

Now we assume that the external field is an electromagnetic field with angular frequency ω and that the local field is given by E loc exp(−iωt). The relative displacement is therefore given by u+ − u− =

(e∗ /Mr )E loc exp(−iωt) . ω02 − ω 2

(5.127)

Since the dipole moment is given by μ = e∗ (u+ − u− ), the polarization P of a solid with density of unit cells N is P = N e∗ (u+ − u− ) .

(5.128)

The contribution from the electronic polarization is included by taking account of the Clausius–Mossotti equation. The dielectric constant2 is then given by κ(ω) = κ∞ +

κ0 − κ∞ , 1 − (ω/ωTO )2

(5.129)

where κ0 is the static dielectric constant and κ∞ is the high-frequency dielectric constant. The angular frequency of the transverse optical (TO) phonons ωTO is given by κ∞ + 2 2 2 ω , = (5.130) ωTO κ0 + 2 0 where we have κ0 = κ∞ without the contribution of ionic polarization and thus ωTO = ωLO = ω0 . Next, we discuss the contribution of ionic polarization to the longitudinal optical phonon frequency ωLO . The longitudinal optical phonon frequency is defined by the

2

See also Sect. 6.3.6 for the derivation of the following relations.

5.4 Polaritons

259

frequency required to satisfy the condition κ(ω) = 0 in (5.129). Using the angular frequency of the longitudinal optical phonons we find 2 κ0 ωLO = . 2 κ∞ ωTO

(5.131)

This relation is called the Lyddane–Sachs–Teller equation. With this relation the dielectric function is rewritten as 2 ω 2 − ωTO ω2 − ω2 = κ∞ LO . (5.132) κ(ω) = κ∞ 1 + LO 2 2 2 ωTO − ω ωTO − ω2 The dielectric constant becomes negative for ωTO ≤ ω ≤ ωLO , and total reflection occurs in this frequency region. Now, we consider the interaction between the lattice vibrations and an external electric field (5.133) E(r, t) = E 0 exp(i[k · r − ωt]) . In the absence of residual charges, the electric displacement D is div D = 0 ,

(5.134)

κ(ω)(k · E 0 ) = 0 .

(5.135)

and thus we obtain Therefore, one of the two conditions κ(ω) = 0 or (k · E 0 ) = 0 should be satisfied. We will discuss these two cases in the following.

5.4.1.1

(1) Transverse Waves: (k · E 0 ) = 0

Since the wave vector k and electric field vector E 0 are perpendicular, the waves are transverse and the external electric field interacts with the transverse waves excited in the crystal. The dielectric function is given by (5.132). The dielectric constant κ(ω) diverges at ω = ωTO , and the imaginary part of the dielectric constant behaves like a delta function, giving rise to resonance. The resonance frequency is associated with transverse lattice vibrations and thus called transverse resonance frequency.

5.4.1.2

(2) Longitudinal Waves: k E 0 and κ = 0

When the electric field of the excited waves is longitudinal, we have k · E 0 = 0 and κ = 0 is required. The angular frequency ωLO satisfies this condition and is given by (5.131), which tells us that ωLO > ωTO . Since the excited waves are longitudinal, there exists no interaction between the excited waves and the external field. In order

260

5 Optical Properties 2

to understand these features in more detail we use a simplified model. We define the polarization due to the lattice vibrations by P latt and the other polarizations by P ele = κ∞ 0 , which show dispersion in a frequency region higher than the lattice vibrations, where κ∞ is called the high-frequency dielectric constant or optical dielectric constant. The polarizations P ele arise from electronic contributions such as the electronic polarization, optical transition, plasma oscillations, and so on. Using these relations we may express the electric displacement by D = 0 E + P = 0 E + P latt + P ele = κ∞ 0 E + P latt ≡ κ(ω) 0 E .

(5.136)

For ω = ωLO , we have κ(ωLO ) = 0 and thus D = 0. Even if the condition for electric displacement D = 0 holds, the lattice vibrations are excited and we have E = 0. When we define the longitudinal electric field by E latt , we obtain E latt = −

1 P. κ∞ 0

(5.137)

For simplicity we neglect the contribution of the polarizations to the local electric √ field in (5.126) and put E = E loc and we obtain ωTO = 2k0 /Mr . Defining the new variable u˜ = u+ − u− we get d2 2 u˜ = −ωTO u˜ + e∗ E latt . dt 2

(5.138)

Since the polarization of a semiconductor with density of unit cells N is given by ˜ we put E latt = 1/(κ∞ 0 )N e∗ u˜ into (5.138) and obtain for ω = ωLO P = N e∗ u, 2 2 ωLO = ωTO +

N (e∗ )2 . Mr κ∞ 0

(5.139)

This result means that the longitudinal optical phonon frequency ωLO is higher than the transverse optical phonon frequency ωTO . This result may be interpreted as showing that the electric field E latt induced by the polarization P latt is in the reverse direction to the polarization vector and that the restoring forces of the lattice and the electric field add together, resulting in a LO phonon frequency higher than the TO phonon frequency. Using the relation P = (κ 0 − 1)E and the static dielectric constant κ0 , we find N (e∗ )2 κ 0 − κ∞ = (5.140) 2 Mr 0 ωTO and inserting this into (5.139) the Lyddane–Sachs–Teller equation (5.131) is derived.

5.4 Polaritons

261

As stated in Sect. 4.1, electromagnetic waves in a semiconductor are described by Maxwell’s equations and for a plane wave we obtain c2 k 2 = ω 2 κ(ω) .

(5.141)

Inserting (5.131) into the above equation, the following relation is obtained: c k = ω κ∞ + 2 2

2

κ0 − κ∞ . 2 1 − (ω 2 /ωTO )

(5.142)

This relation represents a coupled mode of transverse electromagnetic waves and lattice vibrations and a wave given by this relation is called a phonon polariton. To illustrate the dispersion relations of phonon polaritons we plot (5.142) in Fig. 5.29. Figure 5.29 represents the dispersions of phonons, electromagnetic waves and phonon polaritons. The dashed lines (inclined) are the transverse electromagnetic waves not coupled to TO phonons in vacuum and in a medium of dielectric constant κ∞ , √ respectively, and they are given by ω = kc and ω = kc/ κ∞ , respectively. The horizontal solid line is the uncoupled LO phonon branch and the horizontal dashed line is the uncoupled TO phonon branch. The solid curves UPL and LPL are the upper and lower polariton branches, respectively, which are both coupled to TO phonons. Since the LO phonons are not coupled to photons (electromagnetic waves), it is shown

Fig. 5.29 Dispersion curves of phonon polaritons. The dashed lines (inclined) are ω = kc for √ photons (electromagnetic waves) in vacuum and ω = kc/ κ∞ for photons in a medium with dielectric constant κ∞ , and they are not coupled with phonons (lattice vibrations). The horizontal solid line is for uncoupled LO phonons and the horizontal dashed line is for uncoupled TO phonons. The solid curves UPL and LPL are upper and lower polariton branches, respectively, which are both coupled modes of photons and phonons. LO phonon branch is drawn with a solid line because it is not coupled with photons. The parameters used for the calculation are κ0 = 15 and κ∞ = 10

262

5 Optical Properties 2

by the solid line. The parameters used in the calculation are κ0 = 15 and κ∞ = 10. It is clear from Fig. 5.29 that solutions for the coupled mode of photons and phonons do not exist in the region ωTO ≤ ω ≤ ωLO . In other words, total reflection will occur in this region. In a real material, however, coupled waves are subject to damping and this effect is incorporated by the replacement of ω 2 in the denominator of (5.142) by ω 2 → ω 2 + iωγ (γ is the damping parameter), giving rise to the penetration of electromagnetic waves into a medium and to reflectivity of less than 100% in this region. Measurements of Raman scattering by phonon polaritons have been done in GaP by Henry and Hopfield [47].

5.4.2 Exciton Polaritons Let us begin with the simple case where we can neglect the kinetic energy of an exciton, 2 K 2 /2M, which is called the approximation without spatial dispersion. The dielectric function of the exciton is given by (4.110) of Sect. 4.5 κ(ω) = κ1 (ω) + iκ2 (ω) =

C/π . EG − Eex /n 2 − (ω + iΓ )

(5.143)

Here we will be concerned with the ground state of the exciton and put n = 1. We define EG − Eex = ω0 and the contributions to the dielectric constant except excitons by κ∞ . Therefore, we have κ(ω) = κ∞

Δex 1+ ω0 − (ω + iγ)

,

(5.144)

where we put γ = Γ . As in the case of phonon polaritons, the electromagnetic wave in a medium in which excitons are excited may be obtained by solving Maxwell’s equations. Therefore, we have two solutions, which are the transverse waves of k · E = 0 and κ(ω) = 0, and the longitudinal waves of k E and κ(ω) = 0. For the transverse waves we have (5.145) c2 k 2 = ω 2 κ(ω) , and thus we find the dispersion of exciton polaritons, which are coupled waves of excitons and photons. For the longitudinal waves we have a solution similar to the case of LO phonons: κ(ω) = 0 . (5.146) Therefore, the angular frequency of a longitudinal exciton ωl is given by ωl = ω0 + Δex .

(5.147)

5.4 Polaritons

263

The angular frequency of the transverse exciton is given by ωt = ω0 and Δex is called the longitudinal–transverse (LT) splitting of the exciton. Assuming that the wave vector k of (5.144) is complex, we put k = k1 + ik2 ,

(5.148)

and then we obtain for the real and imaginary parts of (5.144) ω 2 κ∞ c2

1+

Δex = k12 − k22 , ω0 − ω ω 2 κ∞ πδ(ω − ω0 ) 0 2 = 2k1 k2 , c

(5.149a) (5.149b)

where the Dirac delta function in Appendix A is used and κ∞ is the background dielectric constant (related to electronic transition, other than the exciton). The imaginary part is proportional to δ(ω − ω0 ) and exhibits resonance at ω = ω0 (= EG − Eex ). We may neglect the term k2 in the region outside the resonance, and so obtain & ω − ω0 − Δex ck1 =√ . (5.150) ω κ∞ ω − ω0 This equation gives the dispersion of exciton polaritons, which is shown in Fig. 5.30. Figure 5.30 is the dispersion curve of exciton polaritons, where the kinetic energy of the exciton, 2 K 2 /2M, is neglected (or the momentum of the exciton for centerof-mass motion K is regarded to be 0). The dispersion curves are calculated by

Fig. 5.30 Dispersion curves of exciton polaritons, where spatial dispersion is neglected (momentum for center-of-mass motion is neglected: K = 0). The difference, LT splitting Δex , between the angular frequencies of longitudinal excitons ωl and transverse excitons ωt is assumed to be Δex /ω0 = 0.2, where ω0 = EG − Eex . The dashed line shows the photon dispersion in the medium

264

5 Optical Properties 2

assuming LT splitting to be Δex /ω0 = 0.2, where Δex is the LT splitting between the angular frequencies of the longitudinal exciton ωl and the transverse exciton ωt , and Δex /ω0 = 0.2. In the region ω ω0 we find that ck1 ω √ κ∞ (1 + Δex /ω0 )

(5.151)

and that the waves behave like electromagnetic waves (photons) in a material with effective dielectric constant, not equal to κ∞ (1 + Δex /ω0 ), resulting in a slightly √ slower phase velocity compared to that of light, c/ κ∞ . In the region ω0 < ω < ω0 + Δex , we have κ(ω) ≤ 0 and thus no solution, resulting in total reflection, just as in the case of phonon polaritons. In the region ω ω0 the waves behave like √ photons (electromagnetic waves) and the phase velocity is c/ κ∞ . Next, we take into account the kinetic energy of the exciton. The dielectric constant is given by Δex κ(ω) = κ∞ 1 + , (5.152) ω0 + K 2 /2M − ω − iγ and insertion of this equation into (5.145) leads to Δex c2 k 2 . =1+ 2 2 κ∞ ω ω0 + K /2M − ω − iγ

(5.153)

It is difficult to obtain an exact solution for this equation, and we approximate such as ωl2 − ωt2 2ωt Δex by taking account of Δex ω0 . Therefore, we obtain the following quadratic equation with respect to ω 2 : c2 k 2 ωl2 − ωt2 = 1 + . κ∞ ω 2 ωt2 + ωt (K 2 /M) − ω 2

(5.154)

The polariton dispersion calculated from (5.154) is shown in Fig. 5.31, where LT splitting between longitudinal excitons ωl and transverse excitons ωt = 1.515 eV is assumed to be Δ = 0.08 meV and the exciton mass to be M = 0.6. In Fig. 5.31 the upper polariton (UPL) and lower polariton (LPL) branches are indicated by 1 and 2, respectively, and the Stokes transition of the Brillouin scattering is indicated by arrows, where a back-scattering geometry is assumed and thus the wave vector of scattered polaritons is reversed after scattering. The parameters used here are for GaAs, which are determined from Brillouin scattering by polaritons in GaAs [48].

5.5 Free–Carrier Absorption and Plasmon

265

Fig. 5.31 Dispersion curves of exciton polaritons in GaAs, where spatial dispersion is taken into account (momentum for center-of-motion is non-zero: K = 0). The LT splitting, the difference between the angular frequencies of longitudinal excitons ωl and transverse excitons ωt = 1.515 eV, is assumed to be Δ = 0.08 meV and the exciton mass to be M = 0.6. The upper polariton (UPL) and lower polariton (LPL) branches are indicated by 1 and 2, respectively, and the Stokes transitions of Brillouin scattering are indicated by arrows. The back-scattering geometry is used and thus the wave vector of scattered polaritons is reversed after scattering

5.5 Free–Carrier Absorption and Plasmon Consider a system with electrons of density n, effective mass m ∗ and electronic charge −e. When an electric field E = E 0 exp(−iωt) is applied to the system, the equation of motion is written as m∗

d2 m∗ d x = −e E 0 e−iωt , x + dt 2 τ dt

(5.155)

where τ is the relaxation time of the electron. The displacement vector of the electron is then given by −e E x= ∗ . (5.156) m (−ω 2 − iω/τ ) The polarization P associated with this displacement is defined by P = n(−e)x .

(5.157)

In addition to the electronic polarization we have to take account of other contributions to the polarization or dielectric constant. This is done by introducing the background polarization P ∞ and background dielectric constant κ∞ , and their relations 0 E + P ∞ = κ∞ 0 E and 0 E + P ∞ + P = κ 0 E. Using this definition the dielectric constant reduces to

266

5 Optical Properties 2

κ(ω) = κ∞ −

ne2 . 0 m ∗ ω(ω + i/τ )

(5.158)

When we define the plasma frequency by & ωp =

ne2 , κ∞ 0 m ∗

(5.159)

the dielectric constant is rewritten as κ(ω) = κ∞ 1 −

ωp2 ω(ω + i/τ )

.

(5.160)

Let us examine the plasma frequency in semiconductors with electron density n 1 × 1018 cm−3 , m ∗ = m 0 , κ∞ = 12. The plasma frequency is estimated to be ωp 1.6 × 1013 rad/s and the relaxation time in semiconductors is about τ 10−12 s, leading to the condition ωp τ 1 in the region of frequency near the plasma frequency (in metals, this condition is satisfied for the frequency of visible light). Therefore, we may safely approximate as κ(ω) = κ∞ 1 −

ωp2 ω2

,

(5.161)

and the condition κ(ωp ) = 0 is fulfilled at ω = ωp . This result tells us that longitudinal plasma oscillations and thus plasmons are excited in a free electron system as in the cases of phonon polaritons and exciton polaritons. Next we will discuss this longitudinal plasma oscillation in detail. Let us consider the system shown in Fig. 5.32. In the case of a metal, the conduction (free) electrons uniformly occupy the space

Fig. 5.32 Illustration of plasma oscillations in a metal or in a semiconductor. Metal ions or donor ions in a semiconductor are indicated by the + symbol and the conduction electrons are shown by shading. When electrons in the equilibrium state are displaced together by x, a polarization P = n(−e)x results, and a surface charge density ±ne|x| appears. The electric field induced by the displacement acts so that the displaced electrons are restored, resulting in a collective motion of the electrons (plasma oscillations) with plasma frequency ωp

5.5 Free–Carrier Absorption and Plasmon

267

surrounding the positive metal ions. In the case of a semiconductor, the positive donor ions are surrounded uniformly by the conduction electrons. In Fig. 5.32 the positive ions are indicated by the + symbol and the electrons are shown by the shading. There are no excess charges and thus the medium is neutral. Since the positive ions are not able to move, the displacement of the electrons is taken into account. We assume that an external field is not present and that the electron displacement x occurs in the x direction. This displacement will induce a polarization P = n(−e)x. Since the electric displacement is given by D = κ∞ 0 E + P = κ(ωp ) 0 E = 0, an electric field E l = − P/κ∞ 0 = nex/κ∞ 0 is induced, and the direction is anti-parallel to the polarization P. This electric field acts as a restoring force for electrons, and so the electrons are forced to move toward the equilibrium position. This collective motion of electrons results in a resonant oscillation with plasma frequency ωp . This kind of collective motion in a system with equal positive and negative charges is called a plasma oscillation. Plasma oscillations are known to be excited in gases, where the oscillations are associated with the relative displacement between positive and negative charges. Next, we will discuss free-carrier absorption. We substitute the complex dielectric constant κ = κ1 + iκ2 in (5.158) and obtain for the real and imaginary parts ne2 τ 2 , 0 m ∗ (ω 2 τ 2 + 1) ne2 τ κ2 (ω) = . 0 m ∗ ω(ω 2 τ 2 + 1) κ1 (ω) = κ∞ −

(5.162) (5.163)

As stated in Sect. 4.1, the absorption of electromagnetic waves is determined by the imaginary part of the dielectric constant κ2 of a medium and the absorption coefficient is given by (4.21) ne2 τ ωκ2 = . (5.164) α= ∗ n0c 0 m n 0 c(ω 2 τ 2 + 1) When an electromagnetic wave of angular frequency ω is applied to a semiconductor with free carriers (electrons or holes), the electromagnetic wave is absorbed by the free carriers. This phenomenon is called the free-carrier absorption, and the absorption coefficient is given by (5.164). Free-carrier absorption is caused by electron transitions within a conduction band induced by absorbing photons. Using the initial state E(ki ) and final state E(kf ) of an electron, the energy conservation rule ω = E(kf ) − E(ki ) and momentum conservation rule k = kf − ki hold. However, we know that a photon, even with a small wave vector k, has a large energy and thus the transition is a direct transition. This means that the energy and momentum conservation rules are not satisfied at the same time. Therefore, free-carrier absorption occurs when impurity scattering or phonon scattering is involved as an intermediate state. Free carrier absorption is very similar to indirect transitions and involves a higher-order perturbation. The treatment of free-carrier absorption has been reported in detail by Fan et al. [49]. When we assume ωτ 1 in (5.163), κ2

268

5 Optical Properties 2

becomes proportional to ω −3 and thus the absorption coefficient is proportional to ω −2 . We have to note that the result is obtained by assuming that the relaxation time τ is independent of the angular frequency ω. In experiments the observed absorption coefficient has the form α(ω) ∝ ω −1.5∼−3.5 , and this behavior is believed to be due to the difference of the scattering mechanisms. Here we will discuss the mobility of electrons or holes in connection with freecarrier absorption. Let us consider the motion of an electron with effective mass m ∗ in the presence of an electric field E 0 e−iωt . The equation of motion is m∗

m∗v dv + = −e E 0 e−iωt dt τ

(5.165)

and the electron drift velocity under the a.c. field is v=−

eE . + 1/τ )

m ∗ (−iω

(5.166)

The mobility μ defined by v = −μE is given by μ=

m ∗ (1

eτ . − iωτ )

(5.167)

If the electron density is n, the current density is given by J = n(−e)v = neμE = σ E, where the conductivity σ is given by σ = neμ =

ne2 τ . ∗ m 1 − iωτ

(5.168)

Using the relations (4.24), (4.25a) and (4.25b) described in Sect. 4.1, and taking the background dielectric constant κ∞ into consideration, (5.168) leads to (5.162) and (5.163). Since the dielectric constant becomes zero at the plasma frequency, electromagnetic waves are subject to total reflection. Here we assume that τ is large and the absorption is weak. Then the reflection coefficient given by (4.13) is approximated as (n 0 − 1)2 (n 0 − 1)2 + k02 ≈ , (5.169) R= (n 0 + 1)2 (n 0 + 1)2 + k02 where we find that the reflection coefficient becomes R = 1 at the plasma frequency ω = ωp . On the other hand, the reflection coefficient becomes zero at a frequency & ω(R = 0) =

ne2 . m ∗ (κ∞ − 1) 0

(5.170)

5.5 Free–Carrier Absorption and Plasmon

269

Fig. 5.33 Reflection coefficients of nInSb with different electron densities near the plasma edge plotted as a function of wavelength. The electron densities are n = 3.5 × 1017 cm−3 , 6.2 × 1017 cm−3 , 1.2 × 1018 cm−3 , 2.8 × 1018 cm−3 , and 4.0 × 1018 cm−3 . (After Spitzer and Fan [50])

From these results we may conclude that a reflection edge exists between ω(R = 0) and ωp . This feature has been observed in experiments by Spitzer and Fan and their results are shown in Fig. 5.33 [50]. The contribution to the dielectric function from the plasma oscillations is obtained by assuming that there is no dispersion of LO phonons near the region ω = ωp , approximating the background dielectric constant by κ∞ . However, the frequency of plasma oscillations is proportional to the square of the carrier density and it is possible to achieve the condition that the plasma frequency is very close to the LO phonon frequency. Under these circumstances transverse optical (TO) phonons are expected not to couple with plasma oscillations. However, longitudinal optical (LO) phonons are expected to couple with plasma oscillations because both are longitudinal. The coupled mode is obtained as follows. The dielectric function without a damping term is obtained from (5.132) and (5.161) as

ωp2

(κ0 − κ∞ )ωTO κ(ω) = κ∞ 1 − 2 + 2 ω ωTO − ω2 2 ωp2 − ω2 ωLO = κ∞ − 2 + 2 . ω ωTO − ω 2

(5.171)

The coupled mode is longitudinal and the condition κ(ω) = 0 holds, and so we obtain the solution 2 = ω±

1 1 2 2 2 ωLO + ωp2 ± (ωLO + ωp2 ) − 4ωp2 ωTO 2 2

1/2

,

(5.172)

where ω+ and ω− are the resonance frequencies of the plasmon–LO phonon coupled mode, above and below the LO phonon frequency ωLO . Such a coupled mode of plasma oscillations and LO phonons, the plasmon–LO phonon coupled mode, has been predicted by Gurevich et al. [51] and their existence has been proved experimentally by Mooradian and Wright [52, 53]. Figure 5.34 shows the experimental

270

5 Optical Properties 2

Fig. 5.34 Raman shift of GaAs as a function of the electron density at room temperature. L+ and L− are the solutions of plasmons coupled to LO phonons and calculated from (5.172). ◦ and • are experimental data by Mooradian and the solid curve is calculated using the parameters ωLO = 292 cm−1 and ωTO = 269 cm−1 in (5.172). (After [53])

results in GaAs at room temperature by Mooradian [53], where the TO phonons do not couple with the plasmons and the Raman shift is ωTO = 269 cm−1 , and is almost constant, whereas the LO phonons couple with the plasmons and split into two branches. The upper branch L+ extrapolates to ωLO = 292 cm−1 and the lower branch L− approaches zero at lower electron densities. The upper branch L+ approaches the plasma frequency ωp and the lower branch L− approaches the TO phonon frequency ωTO at higher electron densities. The solid curves for the upper L+ and lower L− branches are calculated from (5.172) with ωLO = 292 cm−1 and ωTO = 269 cm−1 , and show good agreement with the experimental data. For a more detailed treatment of plasmon–LO phonon interactions see the paper by Klein [54].

5.6 Problems (5.1) (5.2) (5.3)

(5.4) (5.5)

2D Derive the Joint density of Two-dimensional band Jcv (ω − EG − Ex ) given by (5.15). Calculate Reflectivity near E 0 critical point using (5.27), using the parameters defined for Problems 4.6 of Chap. 4. Compare the calculated curve of Fig. 12.5 of the previous problem with the experimental results shown in Fig. 5.7. Experimental data show a weak peak near the critical point E 0 . Explain the difference between Figs. 12.5 and 5.7. Calculate Seraphin coefficients α(ω) and β(ω) using the model dielectric functions κ1 (ω) and κ2 (ω) for E 0 transition. Electroreflectance experiments provide the critical point energies such as E 0 , E 0 + Δ0 , E 1 , and E 1 + Δ1 . These critical point energies are determine from the analysis based on the spectra ΔR/R. Calculate the electroreflectance spectra using (5.48) for the cases given below. (1) Three dimensional case: m 3 = 5/2, C3 = 0.005, θ3 = 3.0, EG = 3.0 eV, and Γ3 = 0.050.

References

(5.6)

271

(2) Two dimensional case: m 2 = 3, C2 = 0.0015, θ2 = 3.0, EG = 3.0 eV, and Γ2 = 0.050. Calculate reflectivity due to free carrier plasma using following parameters. κ∞ = 10, ωp τ = 10. Plot reflectivity as a function of ωp /ω = λ/λp , where λp is the plasma wavelength.

References 1. M. Cardona, Modulation spectroscopy, in Solid State Physics, Suppl. 11 (Academic, New York, 1969) 2. D.E. Aspnes, Modulation spectroscopy/electric field effects on the dielectric function of semiconductors, in Handbook of Semiconductors, vol. 2, ed. by M. Balkanski (North-Holland, Amsterdam, 1980), pp.109–154 3. P. Yu, M. Cardona, Fundamentals of Semiconductors: Physics and Materials Properties (Springer, Heidelberg, 1996) 4. B.O. Seraphin, Electroreflectance, in Semiconductors and Semimetals, vol. 9, ed. by R.K. Willardson, A.C. Beer. (Academic, New York 1972), pp. 1–149 5. D.F. Blossey, P. Handler, Electroabsorption, in Semiconductors and Semimetals, vol. 9, ed. by R.K. Willardson, A.C. Beer (Academic, New York, 1972), pp.257–314 6. D.E. Aspnes, N. Bottka, Electric-field effects on the dielectric function of semiconductors and insulators, in Semiconductors and Semimetals, vol. 9, ed. by R.K. Willardson, A.C. Beer (Academic, New York, 1972), pp.457–543 7. R. Loudon, The Quantum Theory of Light (Oxford University Press, Oxford, 1973) 8. R. Loudon, The Raman effect in crystals. Adv. Phys. 13, 423–482 (1964); Erratum, Adv. Phys. 14, 621 (1965) 9. C. Hamaguchi, Brillouin scattering in anisotropic crystals. Oyo Buturi (Jpn. Soc. Appl. Phys.), 42(9), 866 (1973) (in Japanese) 10. M. Cardona, Light scattering as a form of modulation spectroscopy. Surf. Sci. 37, 100–119 (1973) 11. M. Abramowitz, I.A. Stegun, Handbook of Mathematical Functions (Dover Publications, New York, 1965), p.446 12. W. Franz, Z. Naturforsch. 13, 484 (1958) 13. L.V. Keldysh, Zh. Eksp. Teor. Fiz. 34, 1138 (1958) [English transl.: Sov. Phys.-JETP, 7, 788 (1958)] 14. B.O. Seraphin, N. Bottka, Phys. Rev. 145, 628 (1966) 15. D.E. Aspnes, Phys. Rev. 147, 554 (1966) 16. Y. Hamakawa, P. Handler, F.A. Germano, Phys. Rev. 167, 709 (1966) 17. H. R. Philipp, H. Ehrenreich, in Semiconductors and Semimetals, vol. 3, ed. by R.K. Willardson, A.C. Beer (Academic Press, New York, 1967) pp. 93–124 18. D.E. Aspnes, Phys. Rev. Lett. 28, 168 (1972) 19. D.E. Aspnes, J.E. Rowe, Phys. Rev. B 5, 4022 (1972) 20. D.E. Aspnes, Surf. Sci. 37, 418 (1973) 21. M. Haraguchi, Y. Nakagawa, M. Fukui, S. Muto, Jpn. J. Appl. Phys. 30, 1367 (1991) 22. H.M.J. Smith, Phil. Trans. A 241, 105 (1948) 23. P.A. Temple, C.E. Hathaway, Phys. Rev. B 6, 3685 (1973) 24. R. Loudon, Proc. Roy. Soc. A275, 218 (1963) 25. G.L. Bir, G.E. Pikus, Sov. Phys.-Solid State 2, 2039 (1961) 26. S. Adachi, C. Hamaguchi, J. Phys. C Solid State Phys. 12, 2917 (1979) 27. B.A. Weinstein, M. Cardona, Phys. Rev. B 8, 2795 (1973)

272 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43. 44. 45. 46. 47. 48. 49. 50. 51. 52. 53.

5 Optical Properties 2

L. Brillouin, Ann. Phys. (Paris) 17, 88 (1922) F. Pockels, Ann. Physik 37 (1889) 144, 372; 39, 440 (1890) G.B. Benedek, K. Fritsch, Phys. Rev. 149, 647 (1966) C. Hamaguchi, J. Phys. Soc. Jpn. 35, 832 (1973) D.F. Nelson, P.D. Lazay, M. Lax, Phys. Rev. B 6, 3109 (1972) R.W. Dixon, IEEE J. Quantum Electron. QE-3, 85 (1967) J.R. Sandercock, Phys. Rev. Lett. 28, 237 (1972) D.L. White, J. Appl. Phys. 33, 2547 (1962) B.W. Hakki, R.W. Dixon, Appl. Phys. Lett. 14, 185 (1969) D.L. Spears, R. Bray, Phys. Lett. 29A, 670 (1969) D.L. Spears, Phys. Rev. B 2, 1931 (1970) E.D. Palik, R. Bray, Phys. Rev. B 3, 3302 (1971) M. Yamada, C. Hamaguchi, K. Matsumoto, J. Nakai, Phys. Rev. B 7, 2682 (1973) D.K. Garrod, R. Bray, Phys. Rev. B 6, 1314 (1972) A. Feldman, D. Horowitz, J. Appl. Phys. 39, 5597 (1968) K. Ando, C. Hamaguchi, Phys. Rev. B 11, 3876 (1975) K. Ando, K. Yamabe, S. Hamada, C. Hamaguchi, J. Phys. Soc. Jpn. 41, 1593 (1976) K. Yamabe, K. Ando, C. Hamaguchi, Jpn. J. Appl. Phys. 16, 747 (1977) S. Adachi, C. Hamaguchi, Phys. Rev. B 19, 938 (1979) C.H. Henry, J.J. Hopfield, Phys. Rev. Lett. 15, 964 (1965) R. Ulbrich, C. Weisbuch, Phys. Rev. Lett. 38, 865 (1977) H.Y. Fan, W. Spitzer, R.J. Collins, Phys. Rev. 101, 566 (1956) W.G. Spitzer, H.Y. Fan, Phys. Rev. 106, 882 (1957) V.L. Gurevich, A.I. Larkin, Y.A. Firsov, Fiz. Tverd. Tela 4, 185 (1962) A. Mooradian, G.B. Wright, Phys. Rev. Lett. 16, 999 (1966) A. Mooradian, in Advances in Solid State Physics, ed. by O. Madelung (Pergamon, New York, 1969), p. 74 54. M.V. Klein, in Light Scattering in Solids, ed. by M. Cardona (Springer, New York, 1975), p. 148

Chapter 6

Electron–Phonon Interaction and Electron Transport

Abstract Semiconductor device operation depends on the drift velocity of carriers, electrons and holes, which is determined by the mobility. The mobility μ is expressed by eτ /m ∗ , where e, τ , and m ∗ are the electronic charge, average of the relaxation time, and the effective mass. The relaxation time or scattering time is limited by various scatterings of carriers. Among them the phonon scattering plays the most important role. In this chapter we begin with the analysis of the lattice vibrations and the derivation of Boltzmann transport equation. Readers who are interested in the detailed treatments of the transport properties are recommended to refer the articles [1–14]. Then collision time, relaxation time and mobility are defined. The transition probabilities and transition matrix elements for the scattering due to various modes of phonons, impurity, electron–electron interaction and so on are evaluated using quantum mechanical approach. These results are used to evaluate scattering rates and relaxation times, and finally respective carrier mobility is obtained. In order to get an better insight into the electron transport, scattering rates and mobilities due to the various processes are evaluated numerically and plotted as functions of electron energy, temperature and carrier densities. In addition, electron mobility is evaluated by taking all the relevant scattering processes. Also a theoretical method to evaluate deformation potentials for phonon scattering is given, where the calculated lattice vibrations and the full band structures in the Brillouin zone are properly employed. Many figures obtained by numerical calculations are very informative for an understanding of semiconductor transport.

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2023 C. Hamaguchi, Basic Semiconductor Physics, Graduate Texts in Physics, https://doi.org/10.1007/978-3-031-25511-3_6

273

274

6 Electron-Phonon Interaction and Electron Transport

6.1 Lattice Vibrations 6.1.1 Acoustic Mode and Optical Mode A crystal consists of a periodic arrangement of atoms and molecules. However, the atoms or molecules of a crystal vibrate around the equilibrium positions at finite temperatures because of their thermal motion. When a atom is displaced from its equilibrium position, the atom is subject to a restoring force depending on the displacement. The restoring force follows Hooke’s law and is proportional to the displacement. When each atom vibrates randomly, each atom suffers random forces and its vibration is immediately damped. On the other hand, if each atom vibrates with a small relative displacement from the neighboring atoms, then the vibration will continue with its small vibration energy. For simplicity we consider the one-dimensional lattice shown in Fig. 6.1, where the mass of the atoms is M and the distance between the nearest neighbor atoms (lattice constant) at equilibrium is a. We assume that the inter–atomic forces act on neighboring atoms only and that the atoms are connected to each other by a spring constant (force constant) k0 . Defining the displacement of the atoms from their equilibrium positions by u 0 , u 1 , u 2 , . . ., u n , u n+1 , . . ., the equation of motion of nth atom M

d2 u n = −k0 (u n − u n−1 ) − k0 (u n − u n+1 ) dt 2 = k0 (n n−1 + u n+1 − 2u n ) .

(6.1)

As stated above, when the displacement of each atom is independent, an atom will be subject to a strong force from the neighboring atoms and the displacement is damped. Therefore the lowest excitation energy of the lattice vibration corresponds to a wavelike displacement, keeping the displacement of neighboring atoms almost in phase, when we see neighboring atoms. In such a case we may write the solution of (6.1) as u n = A exp[i(qna − ωt)],

Fig. 6.1 Displacement of atoms from their equilibrium positions (lattice vibration)

(6.2)

6.1 Lattice Vibrations

275

where q = ω/vs = 2π/λ is the wave vector, ω is the angular frequency, vs is the velocity of sound, and λ is wavelength. Inserting (6.2) into (6.1), we obtain qa . Mω 2 = −k0 eiqa + e−iqa − 2 = 4k0 sin2 2

(6.3)

From this we have following relation: ω=2

k0 M

qa sin . 2

(6.4)

When the wavelength is much longer than the lattice constant (qa 1), the phase velocity vs is given by ω vs = = q

k0 sin(qa/2) ∼ a = M (qa/2)

k0 a M

(qa 1) .

(6.5)

This result indicates that a lattice vibration with long wavelength has a constant phase √ velocity vs = k0 /Ma, which corresponds to the sound velocity. Figure 6.2 shows the calculated curve from (6.4), where we see that the ω − q curve is a periodic function with a period of 2π/a. The whole dispersion curve is the repetition or displacement of the curve in the period −π/a ≤ q ≤ π/a, and thus this feature enables us to discuss lattice vibrations in that period. The region of the period is called the first Brillouin zone, and the second Brillouin zone is shown in Fig. 6.2. The second, third and other Brillouin zones are equivalent to the first Brillouin zone, which is shown in Sect. 1.4 in detail in connection with the reduced zone scheme. Where there are N atoms, N degrees of freedom of motion exist. Adopting cyclic boundary conditions we can define wave vectors by q = 2πn/(N a), where n = (−N /2 + 1) ∼ (+N /2), giving rise to N values of the wave vectors. The above defined wave vectors are obtained from the cyclic boundary condition such that the displacement u n of (6.2) is equivalent for n = 0 and n = N .

Fig. 6.2 Dispersion curve dimensional lattice vibration

of

one-

276

6 Electron-Phonon Interaction and Electron Transport

Next, we consider a lattice consisting of two kinds of atoms with masses M1 and M2 . The atomic distance of the atoms of mass M1 is a and the same is true for the atoms M2 . When the nearest-neighbor interaction is assumed, the equations of motion are written as in the case of the one-dimensional lattice stated above as ⎫ d2 ⎪ M1 2 u 2n+1 = k0 (u 2n + u 2n+2 − 2u 2n+1 ) , ⎪ ⎪ ⎬ dt (6.6) ⎪ ⎪ d2 ⎪ M2 2 u 2n = k0 (u 2n−1 + u 2n+1 − 2u 2n ) ⎭ dt for the atoms M1 and M2 . We assume once again wave-type solutions of the same type as before. In addition we may expect another type of solution where atoms of even order and odd order are displaced in the reverse direction to each other, and thus atoms of even order form a wave and odd order atoms form another wave. To satisfy these vibration types we express the displacement as u 2n+1 = A1 ei{(2n+1)(qa/2)−ωt} , u 2n = A2 ei{(2n)(qa/2)−ωt} .

(6.7)

Inserting these equations into (6.6), we obtain following relations: (M1 ω 2 − 2k0 )A1 + {2k0 cos(qa/2)}A2 = 0 ,

(M2 ω 2 − 2k0 )A2 + {2k0 cos(qa/2)}A1 = 0 .

(6.8)

We easily find that the condition A1 = A2 = 0 correspond to all atoms at a standstill, and therefore we have to find solutions such that both A1 and A2 are not zero simultaneously. This condition is satisfied by requiring the determinant of the simultaneous equations with respect to A1 and A2 in (6.8) to be zero, giving rise to (M1 ω 2 − 2k0 ) 2k0 cos(qa/2) = 0. 2k0 cos(qa/2) (M2 ω 2 − 2k0 )

(6.9)

This equation is regarded as a quadratic equation with respect to ω 2 , and the solutions 2 2 and ω+ are given by ω−

M1 + M2 4M1 M2 2 qa 1− 1− , = k0 sin M1 M2 (M1 + M2 )2 2

qa M1 + M2 4M1 M2 2 1+ 1− sin2 . ω+ = k 0 M1 M2 (M1 + M2 ) 2

2 ω−

(6.10a)

(6.10b)

6.1 Lattice Vibrations

277

Fig. 6.3 Angular frequency versus wave vector relations for the two vibration modes of a lattice consisting of two kinds of atoms

It is evident from (6.10b) and (6.10b) that ω− and ω+ approach zero and a constant not equal to zero as q → 0. Taking account of the fact that the angular frequency is positive, ω− and ω+ are plotted as a function of the wave vector q for several values of α = M1 /M2 as a parameter in Fig. 6.3, where we define 1/Mr = 1/M1 + 1/M2 . Let us consider the two branches ω− and ω+ in the long wavelength limit. For q = 0, (6.8), (6.10b) and (6.10b) lead us to the following results: ⎫ ω− = 0 ⎬ A1 , = 1⎭ A2 1 2k0 1 ≡ + ω+ = 2k0 M1 M2 Mr A1 M2 =− A2 M1

(6.11) ⎫ ⎪ ⎪ ⎪ ⎪ ⎬ ⎪ ⎪ ⎪ ⎪ ⎭

.

(6.12)

When we put M1 = M2 , the ω− branch gives the same result as a lattice consisting of one kind of atom, corresponding to a sound wave, and thus called the acoustic branch, the acoustic mode of vibrations or the acoustic phonon. Since the acoustic branch satisfies the condition (A1 = A2 ), the neighboring atoms move in the same direction and thus the relative displacement is zero in the long wavelength limit. On the other hand, the ω+ branch satisfies A1 /A2 = −M2 /M1 and thus different atoms are displaced in the opposite directions to each other, resulting in zero of the center of mass motion. The ω+ branch exhibits a relative displacement between the different atoms and induces an electric field when the atoms are ionic. The induced electric field interacts strongly with the external electromagnetic field and absorbs the external waves. This often occurs in the infrared region, leading to it to be called the optical branch, optical mode of lattice vibrations or the optical phonon. Figure 6.4 shows a schematic illustration of the atomic displacement for (a) the acoustic mode (acoustic

278

6 Electron-Phonon Interaction and Electron Transport

Fig. 6.4 Schematic illustration of two types of lattice vibrations: a acoustic mode (acoustic phonon) and b optical mode (optical phonon)

phonon) and (b) the optical mode (optical phonon), where we see the difference in the displacement between the two modes of lattice vibrations. The acoustic mode in the limit of qa 1 gives the following relation: ω− ∼ =

2k0 aq (qa 1) , (M1 + M2 )

(6.13)

and thus the sound velocity (phase velocity) is given by ω− vs = = q

2k0 a, (M1 + M2 )

(6.14)

which corresponds to (6.5). In ionic crystals unusual reflectivity has been observed in the infrared wavelength region of 20–100 µm. For example, the reflectivity of NaCl exhibits maxima around 40 and 60 µm, where the angular frequencies of light for the corresponding wavelengths are ω = 2πc/λ ∼ 4 × 1013 s−1 and their wave vectors are q = 2π/λ ∼ 103 cm−1 , which are much smaller than the wave vector at the Brillouin zone edge π/a 108 cm−1 . From the energy and momentum conservation rules, such high energy excitation in the small wave vector region is easily found to correspond to the optical phonon branch ω+ . In general, as stated previously, the optical mode of lattice vibration appears in a crystal with two or more atoms in a unit cell. Since there exist one longitudinal and two transverse acoustic modes, a crystal with s atoms in a unit cell gives rise to 3(s − 1) optical modes of lattice vibration.

6.1 Lattice Vibrations

279

6.1.2 Harmonic Approximation We consider the motion of the lth lattice atom of a crystal with mass Ml . The potential energy V of the crystal is a function of the coordinates of the lattice atom x l and the kinetic energy of the crystal is the sum of the kinetic energy of each atom pl2 /2Ml . Therefore, the total energy of the crystal is given by H=

p2 l + V (x 1 , x 2 , . . . , x l , . . .) . 2M l l

(6.15)

For simplicity, we consider a crystal consisting of N atoms which are bound together by the nearest-neighbor force only. In equilibrium the position of an atom is expressed in terms of the lattice vector a as (6.16) Rl = l a . For another simplicity we assume a one-dimensional lattice and express the potential energy by f (xl+1 − xl ) , (6.17) V (x 1 , x 2 , . . . , x l , . . .) = l

where f (xl+1 − xl ) is a function of the relative distance between the lth and (l + 1)th atoms. We define the displacement u l of the lth atom by u l = xl − la .

(6.18)

Since we assume the equilibrium condition such that the lth atom occupies its lattice point la, the following relation holds for every l: ∂V = 0; u 1 = u 2 = u 3 = · · · = u N = 0 . ∂u l

(6.19)

In the case of a small displacement u l , the potential energy is expanded by the Taylor series ∂2 V 1 ul ul + ··· , (6.20) V (u 1 , u 2 , u 3 , . . . , u N ) = V0 + 2 l,l ∂u l ∂u l where the first derivative term ∂V /∂u l is dropped because of the condition given by (6.19). In addition we may put V0 = 0 by choosing V0 as the origin of the potential energy. Since the relation V =

l

f (xl+1 − xl ) =

f (u l+1 − u l + a)

(6.21)

l

holds, we have ∂ f /∂u l+1 = −∂ f /∂u l ≡ ∂ f /∂u, and the summation is rewritten as

280

6 Electron-Phonon Interaction and Electron Transport

l,l

=

∂2 f ∂u l ∂u l

ul ul

2 u l+1

l

=

∂2 f ∂2 f ∂2 f ∂2 f + u l2 2 + u l+1 u l + u l u l+1 2 ∂u l+1 ∂u l ∂u l ∂u l+1 ∂u l+1 ∂u l

∂2 f 2 + u l2 − u l+1 u l − u l u l+1 u l+1 ∂u 2 l

≡g

(u l+1 − u l )2 ,

(6.22)

l

where g = ∂ 2 f /∂u 2 . Inserting this relation into (6.20) we obtain 1 (u l+1 − u l )2 . V (u 1 , u 2 , u 3 , . . . , u N ) = V0 + g 2 l

(6.23)

From these considerations we find that the Hamiltonian for a crystal of a monoatomic chain can be expressed by the displacement u l and momentum pl . These two parameters are independent and satisfy the following commutation relation: [u l , pl ] = u l pl − pl u l = iδl,l ,

(6.24)

where the crystal consists of atoms with the same mass and the momentum operator is defined by pl = −i∂/∂u l . The Hamiltonian H for a crystal of a mono-atomic chain is given by H=

1 1 pl pl + g (2u l u l − u l u l+1 − u l u l−1 ) . 2M l 2 l

(6.25)

The Hamiltonian derived above is for a one-dimensional lattice connected by a spring force (or force constant) g, and corresponds to the equation of motion given by (6.1). Therefore, the displacement is given by u l = Aei(qla−ωt) .

(6.26)

Here we introduce the cyclic boundary condition: u l+N = u l ,

(6.27)

and the wave vector q has to satisfy exp(iqa N ) = 1 or q =

2π l, aN

(6.28)

6.1 Lattice Vibrations

281

where l is an integer. The same relation is obtained by introducing the cyclic boundary condition to (6.25). Here we show that the Hamiltonian for lattice vibrations given by (6.25) is easily solved by using the Fourier transform. To do this we define 1 −iqal ul e Qq = √ N l

(6.29)

and then the displacement u l is obtained by the inverse transform 1 1 1 u l eiqa(l−l ) = Q q eiqal = u l N δll = u l . √ N N l N q q,l

(6.30)

As shown in Appendix A.2, we have the following relation:

eiqa(l−l ) = N δll .

(6.31)

q

Since this relation is often used in this textbook and is very important for solid state physics, a proof is given here, although a general formula including 3-dimensional case is proved in Appendix A.2. The wave vector is written as q=

2π 2π n= n, aN L

where L = N a is the length of a one-dimensional crystal of N atoms. The wave vector q has N degrees of freedom, which is exactly the same as the number of atoms N . This requires the condition for n such that n ranges from 1 to N , from 0 to N − 1, or from −N /2 + 1 to N /2, resulting in N values for n. This is equivalent to the reduced Brillouin zone scheme and the wave vector q in the first Brillouin zone describes all the features required for lattice vibrations. When we see the wave vectors q corresponding to n in Fig. 6.2, all the features of the relation between ω and q are the repetition of the first Brillouin zone. From this reason the first Brillouin zone is taken in general as π −π , m∗

(6.390)

364

6 Electron-Phonon Interaction and Electron Transport

Fig. 6.29 Electron mobility μpop for polar optical phonon scattering in GaAs is plotted as a function of temperature T , in addition to the mobilities due to acoustic phonon scattering, and piezoelectric potential scattering, where the used parameters are given in Table 6.3. The mobilities due to acoustic phonon scattering for Ξ = 7.0 and Ξ = 14.0 [eV] are shown to see the difference. The electron mobility μtotal due to acoustic (Ξ = 14.0 [eV]), piezoelectric, and polar optical phonon scattering is also shown, which gives mobility μ = 8, 840 [cm2 /Vs] at T = 300 [K]. Data points ◦ are obtained by averaging the reported experimental data from Rode [46]

In addition we plotted electron mobilities due to acoustic phonon scattering using two different values of deformation potentials Ξ = 7.0 [eV] [45] and Ξ = 14.0 [eV], and piezoelectric potential scattering. The mobility due to acoustic phonon scattering deduced from Ξ = 7.0 [eV] is too high and the electron mobility due to these three scattering processes does not agree with experimental observation. We calculated the electron mobility due to acoustic, piezoelectric, and polar optical phonon scatterings and Ξ = 14.0 [eV] is quite reasonable value of the electron mobility μ = 8,840 [cm2 /Vs] at T = 300 K, as shown by μtotal = μac+pz+pop in Fig. 6.29. In the calculations we employed numerical integration stated above for the case of combined acoustic deformation potential and polar optical phonon scatterings, where we we find a very good agreement between the present calculation and the experimental data. The experimental data are obtained by averaging the reported values of Rode [46]. Here we have to note that the acoustic deformation potential Ξ = 14.0 eV gives a very good agreement between the calculations and the experimental data.

6.5.4 Piezoelectric Potential Scattering As discussed in Sect. 6.4.4, the effect of screening does not play an important role in the piezoelectric potential scattering, we neglect the effect and estimate the electron

6.5 Mobility

365

Fig. 6.30 Calculated electron mobility due to piezoelectric potential scattering in GaAs plotted as a function of temperature, where the material parameters are given by ∗ =e ∗ Table 6.3, and epz 14 and c = c44 are used without averaging

mobility for piezoelectric potential scattering. Then the mobility is given by the following equation using (6.357). √ 16 2π2 (k T )−1/2 . μpz = ∗2 /c∗ ∗2 B 3m ∗3/2 eepz

(6.391)

Electron mobility due to piezoelectric potential scattering is shown in Fig. 6.30 as a function of temperature T , where we see the mobility decreased with increasing temperature T . Here we neglected the screening effect which is discussed by Ridley ∗ = [8]. In the calculation the piezoelectric coupling constant is obtained by using epz ∗ e14 = 0.16 and c = c44 , neglecting anisotropy.

6.5.5 Inter–Valley Phonon Scattering The mobility for inter–valley phonon scattering is evaluated with a relation similar to that for non–polar optical phonon scattering, and is obtained by replacing the optical phonon deformation potential Dop by the inter–valley phonon deformation potential Di j and the optical phonon energy ωop by the inter–valley phonon energy ωi j . In many–valley semiconductors such as Ge and Si, however, there are four and six equivalent valleys, respectively, and the degeneracy factor of the valleys giivj for scattered electron must be considered. The electron mobility for inter–valley phonon scattering is given by the following equation using (6.361) μint =

√ 4giivj 2πe2 ρ(ωi j )1/2 ∗3/2

3m d

m ∗c Di2j

f (xi j ) ,

(6.392)

366

6 Electron-Phonon Interaction and Electron Transport

where xi j = ωi j /kB T and f (xi j ) is obtained by replacing x0 in (6.377) by xi j . Let us examine the temperature dependence of the electron mobility in Si. As discussed in Sect. 6.4, the conduction bands of Si consist of equivalent valleys located along the 100 direction, and g–type and f–type inter–valley scattering will dominate the other scattering processes at higher temperatures. In order to get an insight into the importance of inter–valley scattering, we calculate the electron mobility by taking account of acoustic phonon scattering and f–type inter–valley phonon scattering ωiv = 51.6 [meV], which is obtained from magnetophonon resonance experiments describe in Sect. 7.4. The assignment of the phonon energy and the types f– and g– are made by assuming that the electrons occupy the lowest Landau level because of the electron density is very low in the used pure samples. The results are summarized in Table 6.4. The deformation potentials for inter–valley phonons listed are from Jacoboni et al. [41] and the intervalley phonon types and energies obtained from magnetophonon experiments are also summarized in Table 6.4. In the present analysis we used the f–type inter–valley phonon energy ωiv,f = 51.6 [meV] and the intervalley deformation potential, where the degeneracy factor of the valleys are included in the deformation potential. This approximation is adopted to calculate the scattering rate in Si shown in Fig. 6.20. Usually, the calculated electron mobility is adjusted to fit the experimental data by changing the deformation potential parameter 2 . The left hand side of Fig. 6.31 shows the electron mobility limited by b = Ξiv2 /Dac lattice scatterings (acoustic and intervalley phonons) as a function of temperature with b = 0, 0.5, 1.0, 2.0 as an adjustable parameter. The right hand side of Fig. 6.31 shows the best fitted temperature dependence of the electron mobility in high purity Si with b = 1.73, where the experimental data • are from Canali et al. [50] and Jacoboni et al. [51]. The deformation potential parameter b is obtained by replacing the deformation potential for non–polar optical phonon scattering by the deformation potential of inter–valley phonon scattering and is defined as follows. b=

E iv2 , 2 Dac

E iv2 =

Div2 vs2 . ωiv2

Here we have to note that the acoustic phonon deformation potential Dac used here is equivalent to the deformation potential Ξ = 9, 0 [eV] determined from the mobility analysis. The parameters used to calculate the scattering rates shown in Fig. 6.20 and the electron mobility in Fig. 6.31 are Ξ = 9.0 [eV] and b = 1.73. When only acoustic phonon scattering is taken into account (b = 0) with acoustic deformation potential Ξ = 9.0 [eV], the calculated mobility at T = 300 K is μ = 2560 cm2 /Vs, which is much larger than the observed mobility 1450 cm2 /Vs, whereas the deformation potential parameter b = 1.73 results in 1452 cm2 /Vs, which is very close to the measured value. In the calculation we take into account of only f–type intervalley phonon ωiv = 51.6 [meV] listed in Table 6.4 which gives rise to the strongest magnetophonon resonance as shown in Sect. 7.4. It is seen in Fig. 6.31 that the electron mobility decreases with increasing b from 0 to 2.0, which means that the electrons

6.5 Mobility

367

Fig. 6.31 a: Calculated temperature dependence of the electron mobility due to acoustic phonon scattering and intervalley phonon scattering in Si for different values of b = 0, 0.5, 1.0, and 2.0 from top to bottom curve. b: Comparison of the temperature dependence of electron mobility in Si between experiments and theoretical calculation with b = 1.73. The the material parameters are given by Table 6.3, and acoustic deformation potential Ξ = 9.0[eV], f–type intervalley phonon energy ωiv,f = 51.6 [meV], and the deformation potential ratio b = 1.73, which gives electron mobility μ = 1452 [cm2 /Vs] at T = 300 K. The experimental data • are from Canali et al. [50] and Jacoboni et al. [51]

are scattered more by inter–valley phonons, resulting in a lower mobility. It may be expected from these results that the calculated electron mobility can be fitted to the experimental results by taking g–type and f–type inter–valley phonon scattering accurately into account and adjusting the deformation potentials. It is also seen in Fig. 6.31 that inter–valley phonon scattering may be disregarded at lower temperatures and that inter–valley phonon scattering affects the electron mobility at temperatures T > 100 K [49].

6.5.6 Ionized Impurity Scattering We have shown that the relaxation time for ionized impurity scattering is given by the Brooks–Herring formula (6.362) and the Conwell–Weisskopf formula (6.363), where these formulae are derived with and without screening by conduction electrons, respectively. The relaxation time becomes a maximum when E in the logarithmic terms is 3kB T and thus the integral is approximated by replacing E by 3kB T except for E in the prefactor. The electron mobility of Brooks–Herring formula is written as μBH

√

−1 ξ0 64 2π 2 3/2 log(1 + ξ (k T ) ) − , = B 0 n I z 2 e3 m ∗1/2 1 + ξ0

(6.393)

368

6 Electron-Phonon Interaction and Electron Transport

where ξ0 =

24 m ∗ (kB T )2 . 2 e 2 n

(6.394)

The electron mobility of the Conwell–Weisskopf formula is given by μCW

−1 √

144π 2 2 kB2 T 2 64 2π 2 3/2 log 1 + = (kB T ) . 2/3 n I z 2 e3 m ∗1/2 z 2 e4 n I

(6.395)

Figure 6.32a is the temperature dependence of calculated mobilities due to ionized impurity scattering by Brooks–Herring formula and by Conwell–Weisskopf formula, evaluated by numerical integration. As expected, however, the logarithmic term is well approximated by replacing E with 3kB T and the difference between the numerical analysis and the approximation is negligible, such as μBH = 2.228 × 105 (numerical) and μBH = 2.262 × 105 (approximation) at T = 10 K for n I = 6.0 × 1013 cm−3 and n = n I /2 in GaAs. Figure 6.32b shows temperature dependence of the electron mobility in GaAs, where ionized impurity scattering, acoustic deformation potential scattering, piezoelectric potential scattering, and polar optical phonon scattering are shown, respectively. The curve μtotal is the theoretical curve due to over all scatterings, and the used parameters are given in Table 6.3. All of the mobilities are evaluated by numerical integration. The points assigned by ◦ is the averaged value of the experimental data of Rode [45, 46]. The total mobility μtotal is numerically evaluated by using τtotal defined by the following equation 1 1 1 1 1 = + ++ + (6.396) τtotal τBH τac τpz τpop and using (6.119), μtotal =

e τtotal . m∗

(6.397)

6.5.7 Neutral Impurity Scattering The relaxation time of the Erginsoy formula for neutral impurity scattering leads to μnI = where a B is Bohr radius.

1 m ∗ /m e e · = , 20anI n nI 20aB κn nI

(6.398)

6.5 Mobility

369

(a)

(b)

Fig. 6.32 a: Calculated temperature dependence of the electron mobilities of GaAs due to ionized impurity scattering by Brooks–Herring formula and Conwell–Weisskopf formula, where density of ionized impurity is n I = 6.0 × 1013 cm−3 and electron density in the conduction band is assumed to be half of the ionized impurity density n = 3.0 × 1013 cm−3 . b: Temperature dependence of electron mobility in GaAs, where ionized impurity scattering, acoustic deformation potential scattering, piezoelectric potential scattering, and polar optical phonon scattering are shown, respectively. The curve μtotal is the theoretical curve due to all the scattering, and the parameters are given in Table 6.3. All the mobilities are evaluated by numerical integration. The averaged values of the experimental data are plotted by ◦ (see Rode [45, 46])

6.5.8 Plasmon Scattering The relaxation time for plasmon scattering is given by (6.368) (the inverse of the scattering rate). However, the electron mobility due to the plasmon scattering is not easily evaluated because of the complicated logarithmic terms and thus here we evaluate the mobility by approximating E(k) by kB T in the logarithmic terms. Then the mobility due to the plasmon scattering is then given by e τpl m∗ √ 32 π2 ∞ √ (kB T )1/2 3 2e(m ∗ )3/2 ωp

μpl =

qc

η+ 2m ∗ kB T /2 − 2m ∗ kB T /2 −1 qc u(η− ) +(n p + 1) ln , (6.399) √ 2m ∗ kB T /2 − η− 2m ∗ kB T /2

× n p ln √

where η± = 1 ± (ωp /kB T ), and other parameters are the same as defined before.

370

6 Electron-Phonon Interaction and Electron Transport

Fig. 6.33 Calculated mobilities limited by plasmon scattering in GaAs are plotted as a function of lattice temperature for electron densities (1) n = 0.5 × 1018 , (2) n = 1.0 × 1018 , and 2.0 × 1018 [cm−3 ]. Used parameters are m ∗ = 0.067m and ∞ = 10.92 0

Fig. 6.34 Calculated mobilities limited by plasmon scattering in GaAs are plotted as a function of electron density at T = 300. Electron energy in the logarithmic terms are approximated by average electron energy E (k) = kB T and thus the electron density n = 3.55 × 1023 (dotted bar in the figure) gives the condition ωp = kB T . In the region of lower electron density, only plasmon absorption is allowed

Calculated temperature dependence of the mobilities limited by plasmon scattering are shown in Fig. 6.33, where we used scalar effective mass m ∗ = 0.067m and dielectric constant ∞ = 10.92 0 , and the curves are obtained for three different electron densities (1) 0.5 × 1018 , (2) 1.0 × 1018 , and (3) 2.0 × 1018 [cm−3 ]. These results indicate that the plasmon limited mobility play an important role at higher temperature, which reflects the the excited number of the plasmon n p . In Fig. 6.34 the electron mobility due to plasmon scattering is plotted as a function of electron density. We see a small step around T = 350 [K] for the electron density

6.5 Mobility

371

n 5.0 × 1017 [cm−3 ], which will be explained in terms that the plasmon emission rate includes the step function u(η− ), where η− becomes 0 at T = 356.2 [K] for ω p = 30.7 [meV]. The discontinuity at lower electron density is explained in terms that plasmon emission process is forbidden for kB T < ωp . In order to obtain the electron mobility limited by plasmon scattering we approximated by replacing electron energy E(k) by kB T . However, we find that the calculated electron mobility due to plasmon scattering does not show any noticeable change when we change the average electron energy from kB T to (3/2)kB T , and thus the approximation is valid for the electron mobility due to plasmon scattering. Now we have to discuss the electron density dependence of the mobility. As shown Figs. 6.33 and 6.34, the electron mobility μpl increases with increasing the electron density n. The mobility behaves as 1 1 μpl ∝ · = ωp n p

ωp m ∗ −1 · exp ne2 kB T

(6.400)

and thus at higher temperatures or lower√electron density such as ωp /kB T 1 the mobility is approximated as μpl ∝ ωp / n and thus electron density dependence is very weak as observed in lower electron density n in Fig. 6.34. On the other hands, at lower temperatures or higher electron √ density such as ωp /kB T 1, the mobility is proportional to exp(ωp /kB T )/ n, and thus the mobility increase with increasing the electron density n because of the exponential term exp(ωp /kB T ) as seen the mobility at higher electron density in Fig. 6.34.

6.5.9 Alloy Scattering The relaxation time for alloy scattering is given by (6.313) or (6.369), and the electron mobility for alloy scattering is evaluated as μalloy

√ 1 16e π4 (kB T )−1/2 , = ∗ 5/2 2 3(2m ) (Va − Vb ) x(1 − x)Ω

(6.401)

where m ∗ is the effective mass of the carrier Ω = a 3 /4 for a zinc blende crystal with the lattice constant a. Since we are not able to estimate |Va − Vb |, we evaluate the electron mobility limited by the alloy scattering by assuming the mobility at 10 K for x = 0.5 is 1.0 × 104 [cm2 /Vs], which gives |Va − Vb | = 3.185 [eV] for m ∗ = 0.067m, a = 5.66 × 10−10 [m]. The calculated electron mobilities due to the alloy scattering are plotted in Fig. 6.35 for x = 0.1 ∼ 0.5. We find in Fig. 6.35 that the alloy scattering becomes very weak at lower temperatures and depends strongly on the alloy composition. The alloy scattering depends strongly on the potential |Va − Vb |2 and the composition x. We may expect that the alloy scattering plays an important role at higher temperatures as shown in Fig. 6.35.

372

6 Electron-Phonon Interaction and Electron Transport

Fig. 6.35 Calculated electron mobility due to alloy scattering as a function of temperature for the alloy composition x = 0.1 ∼ 0.5. The parameter |Va − Vb | is determined to give μ = 10 [m2 /Vs] at T = 10 [K]. Alloy scattering becomes very weak at lower temperatures and depends strongly on the alloy composition

6.6 Problems Chapter 6 deals with the scattering processes and evaluate electron mobilities due to various scattering processes in detail. It is very helpful for readers to summarize the processes in a short version. Here the readers are asked to summarize the respective equations for acoustic phonon scattering as an example. This will help the readers to understand other scattering processes. (6.1)

Show the scattering probability P(k, k ) for the acoustic phonon scattering, using the interaction Hamiltonian H1 = Hel . Describe how to derive the scattering rate wac for an electron by acoustic phonon deformation potential scattering given by (6.332). Discuss the assumptions used to derive the final result.

(6.2)

Show that the relaxation time τac for an electron by acoustic phonon deformation potential scattering is given by (6.341) under the qmax = 2k(1 ± m ∗ vs /k) 2k.

(6.3)

Calculate the relaxation time without the approximation, and compare the result with the above calculations.

(6.4)

Electron mobility of n-GaAs is limited by polar optical phonon scattering. Using the parameters for GaAs listed in Table 6.3, calculate the electron mobility limited by polar optical phonon scattering in GaAs at the range of temperature from 100 to 500 K.

References

(6.5)

373

Calculate conductivity effective mass m c of electrons in Si with 6 (or 3) equivalent valleys and derive the relation (6.372)) 1 1 = mc 3

1 2 + ml mt

(6.402)

(6.6)

Prove (6.402) is valid for the conductivity effective mass of electrons in Ge with 8 (or 4) equivalent valleys.

(6.7)

Evaluate effective density of states mass m ds and effective conductivity mass m c of electrons in Ge and Si.

References 1. J.M. Ziman, Electrons and Phonons (Oxford University Press, Oxford, 1963) 2. E.G.S. Paige, Progress in Semiconductors, vol. 8, ed. by A.F. Gibson, R.E. Burgess (Temple Press Books, London, 1964) 3. B.R. Nag, Theory of Electrical Transport (Pergamon Press, New York, 1972) 4. A. Haug, Theoretical Solid State Physics (Pergamn Press, New York, 1972) 5. E.M. Conwell, High Field Transport in Semiconductors, in Solid State Physics, Suppl. 9 (Academic, New York, 1967) 6. R.A. Smith, Wave Mechanics of Crystalline Solids (Chapman and Hall, London, 1969) 7. K. Seeger, Semiconductor Physics (Springer, Heidelberg, 1973) 8. B.K. Ridley, Quantum Processes in Semiconductors (Oxford University Press, Oxford, 1988) 9. M. Born, K. Huang, Dynamical Theory of Crystal Lattice (Oxford University Press, Oxford, 1988) 10. H. Brooks, Adv. Electron. Electron Phys. 8, 85 (1955) 11. H. Haug, S.W. Koch, Quantum Theory of the Optical and Electronic Properties of Semiconductors (World Scientific, Singapore, 1993) (Chaps. 7 and 8) 12. G.D. Maham, Many-Particle Physics (Plenum Press, New York, 1986) (Chap. 5) 13. D.K. Ferry, R.O. Grondin, Physics of Submicron Devices (Plenum Press, New York, 1991) (Chap. 7) 14. C. Kittel, Quantum Theory of Solids (Wiley, New York, 1963) (Chap. 2) 15. E.M. Conwell, V.F. Weisskopf, Phys. Rev. 77, 388 (1950) 16. C. Herring, E. Vogt, Phys. Rev. 101, 944 (1956) 17. O. Madelung (ed.), Semiconductors. Landolt–Börnstein:Numerical Data and Functional Relationships in Science and Technology, vol. 17 (Springer, Berlin, 1982) 18. M.V. Fischetti, J. Appl. Phys. 80, 2234 (1996) 19. W. Pötz, P. Vogl, Phys. Rev. B 24, 2025 (1981) 20. S. Zollner, S. Gopalan, M. Cardona, Appl. Phys. Lett. 54, 614 (1989); J. Appl. Phys. 68, 1682 (1990); Phys. Rev. B 44, 13446 (1991) 21. M. Fischetti, S.E. Laux, Phys. Rev. B 38, 9721 (1988) 22. H. Mizuno, K. Taniguchi, C. Hamaguchi, Phys. Rev. B 48, 1512 (1993) 23. M.L. Cohen, T.K. Bergstresser, Phys. Rev. 141, 789 (1966) 24. K. Kunc, O.H. Nielsen, Comput. Phys. Commun. 16, 181 (1979) 25. G. Dolling, J.L.T. Waugh, in Lattice Dynamics, ed. by R.F. Wallis (Pergamon, Oxford, 1965), pp. 19–32

374

6 Electron-Phonon Interaction and Electron Transport

26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39.

K. Kunc, H. Bilz, Solid State Commun. 19, 1027 (1976) W. Weber, Phys. Rev. B 15, 4789 (1977) O.H. Nielsen, W. Weber, Comput. Phys. Commun. 17, 413 (1979) O.J. Glembocki, F.H. Pollak, Phys. Rev. Lett. 48, 413 (1982) S. Bednarek, U. Rössler, Phys. Rev. Lett. 48, 1296 (1982) Hiroyuki Mizuno: MS Thesis, Osaka University (1995) J. Lindhard, Mat. Fys. Medd. 28, 8 (1954) E.M. Conwell, A.L. Brown, J. Phys. Chem. Solids 15, 208 (1960) H. Callen, Phys. Rev. 76, 1394 (1949) J. Zook, Phys. Rev. 136, A869 (1964) A.R. Hutson, J. Appl. Phys. 32, 2287 (1961) A.R. Hutson, D.L. White, J. Appl. Phys. 33, 40 (1962) C. Hamaguchi, J. Appl. Phys. 130, 125701 (2021) L. Eaves, R.A. Hoult, R.A. Stradling, R.J. Tidey, J.C. Portal, S. Askenazy, J. Phys. C Solid State Phys. 8, 1034 (1975) C. Hamaguchi, Y. Hirose, K. Shimomae, Jpn. J. Appl. Phys. 22(Suppl. 22–3), 190 (1983) C. Jacoboni, L. Reggiani, Rev. Mod. Phys. 55, 645 (1983) C. Erginsoy, Phys. Rev. 79, 1013 (1950) N. Sclar, Phys. Rev. 104, 1548 (1956) T.C. McGill, R. Baron, Phys. Rev. B 11, 5208 (1975) D.L. Rode, Phys. Rev. B 2, 1012 (1970) D.L. Rode, Semiconductors and Semimetals, vol. 10, ed. by R.K. Willardson, A.C. Beer (Academic, New York, 1975), pp. 1–89 D.M. Brown, R. Bray, Phys. Rev. 127, 1593 (1962) F.J. Morin, Phys. Rev. 93, 62 (1954) D. Long, Phys. Rev. 120, 2024 (1960) C. Canali, C. Jacoboni, F. Nava, G. Ottavani, A. Alberigi Quaranta, Phys. Rev. B 12, 2265 (1975) C. Jacoboni, C. Canali, G. Ottaviani, A.A. Quaranta, Solid-State Electron. 20, 77 (1977)

40. 41. 42. 43. 44. 45. 46. 47. 48. 49. 50. 51.

Chapter 7

Magnetotransport Phenomena

Abstract Electron transport in a magnetic field exhibits various interesting characteristics, which is called magnetotransport phenomena. In this chapter we deal with Hall effect, magnetoresistance, and oscillatory magnetoresistance effects in detail. Hall effect is very useful to determine the mobility and density of carriers. Shubnikov–de Haas oscillations are observed in degenerate semiconductors and provide the information of Fermi energy. Magnetophonon resonance arises from inter–Landau level transitions of non-degenerate electron gas and gives the effective mass. Once we know the effective mass we can deduce phonon energy involved with the magnetophonon resonance. These two oscillatory magnetoresistance effects are very widely used to investigate semiconductor parameters. Quantum Hall effect is not dealt with here but discussed in detail in Chap. 8. For more detailed treatments, readers are recommended to refer the articles [1–3] for basic treatments, and other review articles [4–12].

7.1 Phenomenological Theory of the Hall Effect The application of a magnetic field perpendicular to the current through a conducting material results in the generation of an electric field perpendicular to both the current and the magnetic field. This phenomena was discovered in 1879 by E. H. Hall and is called the Hall effect. This phenomena has been successfully used to investigate the electronic properties of semiconductors and metals. In this section, first we deal with the Hall effect in a simple way in which all the electrons have the same velocity and later we will discuss a more accurate treatment using the Boltzmann transport equation. First, let us consider an infinitely long sample, as shown in Fig. 7.1, and assume that a uniform current density J flows along the sample. An electron with drift velocity v experience the Lorentz force F = −ev × B, where −e is the charge of the electron. Let the electron density be n; the current density is then given by J = n(−e)v. When the current flows in the +x direction, the velocity component is vx < 0 and thus the electron drifts in the −x direction. In a magnetic field applied in the z direction, the Lorentz force for the electron is given by Fy = −e(|vx |Bz ) = −e|vx |Bz < 0, and © The Author(s), under exclusive license to Springer Nature Switzerland AG 2023 C. Hamaguchi, Basic Semiconductor Physics, Graduate Texts in Physics, https://doi.org/10.1007/978-3-031-25511-3_7

375

376

7 Magnetotransport Phenomena

Fig. 7.1 Hall effect in semiconductors. Hall fields for a electron (n-type semiconductor) and b hole (p-type semiconductor) are reversed

thus the electron is forced to move in the −y direction. Noting that the Hall effect is normally measured as the electric field induced in the y direction without any flow of current in this direction, negative charges due to the electrons will accumulate on the front surface as shown in Fig. 7.1 and immobile positive charges (donors) will appear on the back surface, resulting in an electric field in the −y direction. The induced electric field (Hall field) E y < 0 will balance the Lorentz force and a steady state will be achieved so that Fy + (−e)E y = 0. This electric field E y is called the Hall Field, and we find the following relation: E y = v x Bz = −

Bz Jx = RH Jx Bz , ne

(7.1)

where RH is called the Hall coefficient,. For electrons the Hall coefficient is given by 1 (7.2) RH = − . ne The angle θH between E x and E y is called the Hall angle, which is given by tan θH =

Ey = −μe Bz = ωc τ . Ex

(7.3)

In the above equation Jx = neμe E x , vx = −μE x and ωc =

eBz eτ , μe = ∗ m∗ m

(7.4)

are used and ωc is the cyclotron angular frequency defined in Chap. 2. The Hall effect is schematically shown in Fig. 7.1a for negative charge carriers (electrons in n-type semiconductors). On the other hand, Fig. 7.1b shows the Hall effect for holes (p-type semiconductors). A hole current in the +x direction is produced by hole drift in the +y direction (vx > 0), and the Lorentz force for a hole in the presence of a magnetic field in the z direction directs it along the −y direction, resulting in positive and negative charge accumulation on the +y surface and −y surface, respectively. This charge accumulation gives rise to a Hall field in the +y direction, which is opposite

7.1 Phenomenological Theory of the Hall Effect

377

to the case for electrons. The Hall coefficient for holes with density p is therefore given by 1 RH = . (7.5) pe If we let the width in the y direction of a semiconductor sample be w and the thickness in the z direction be t, then we obtain the Hall voltage in the y direction VH = wE y . From current Ix = Jx wt and from (7.1) the Hall voltage is expressed as VH =

RH I x Bz . t

(7.6)

Measurement of the Hall effect gives the Hall coefficient RH from (7.6) and the electron density n or hole density p are determined from (7.2) or (7.5), respectively. It should be noted here that the Hall coefficient given by (7.2) and (7.5) are derived under the assumption that the carrier relaxation time τ is independent of the carrier energy. When the relaxation time τ depends on the carrier energy and the effective mass is not scalar, the Hall coefficient is given by the following relation instead of (7.2): rH (7.7) RH = − , ne where rH is called the scattering factor of the Hall coefficient, and is determined from the scattering mechanisms and distribution function of the carriers. A detailed treatment will be given in next section. Using (6.121) for the conductivity σ the Hall coefficient (7.2) is rewritten as |RH | σ = μ.

(7.8)

This relation is valid only for rH = 1 as seen from (7.7), and in general use the relation |RH | σ = rH μ. (7.9) As discussed later, it is very difficult to determine the scattering factor rH in semiconductors. We define the Hall mobility by |RH | σ = μH

(7.10)

where μH is called the Hall mobility. The Hall mobility defined above has the same dimensions as the drift mobility but differs by a factor rH , or in other words, the following relation holds. μH = rH . (7.11) μ Although the treatment stated above is based on a simplified model, the results give good information to interpret the Hall effect. In the following we will derive

378

7 Magnetotransport Phenomena

relations useful for understanding magnetotransport in semiconductors, which may be extended to the more detailed general case. The equation of motion for an electron is written as dv m∗v + = −e(E + v × B). (7.12) m∗ dt τ When a static electric field is applied to a semiconductor, the steady state condition dv/dt = 0 gives rise to a steady-state drift velocity v given by v=−

eτ E = −μE. m∗

(7.13)

Applying the averaging procedure on this relation used in Sect. 6.2.2 gives the same result for the drift mobility as (6.118). Therefore, the velocity is interpreted as the drift velocity In the presence of a magnetic field B, the velocity is given by v=−

eτ (E + v × B). m∗

(7.14)

If the magnetic field is along the z direction, the above equation leads to eτ (E x + v y Bz ), m∗ eτ v y = − ∗ (E y − vx Bz ), m eτ vz = − ∗ E z . m vx = −

These relations are rewritten as τ e ωc τ 2 vx = − ∗ Ex − Ey , m 1 + ωc2 τ 2 1 + ωc2 τ 2 ωc τ 2 e τ vy = − ∗ E + E x y , m 1 + ωc2 τ 2 1 + ωc2 τ 2 e vz = − ∗ τ E z . m

(7.15a) (7.15b) (7.15c)

(7.16a) (7.16b) (7.16c)

Since the current density is given by J = n(−e)v, we obtain τ ne2 ωc τ 2 Jx = ∗ Ex − Ey , m 1 + ωc2 τ 2 1 + ωc2 τ 2 ωc τ 2 ne2 τ Jy = ∗ E + E x y , m 1 + ωc2 τ 2 1 + ωc2 τ 2 ne2 Jz = ∗ τ E z . m

(7.17a) (7.17b) (7.17c)

7.1 Phenomenological Theory of the Hall Effect

379

Therefore, writing the i component of the current as Ji = σi j E j , we find

[J ] = [σ][E]

(7.18)

⎡

⎤ σx x σx y 0 [σ] = ⎣ σ yx σ yy 0 ⎦ , 0 0 σzz

σx x = σ yy = σx y = −σ yx σzz =

ne2 τ · , m ∗ 1 + ωc2 τ 2 ne2 ωc τ 2 =− ∗ · , m 1 + ωc2 τ 2

ne2 τ = σ0 . m∗

(7.19)

(7.20a) (7.20b) (7.20c)

Next, we will discuss the Hall effect, where we assume the current is in the x direction and the magnetic field is applied in the z direction. The current density in the x and y directions are then given by Jx = σx x E x + σx y E y , Jy = σ yx E x + σ yy E y .

(7.21a) (7.21b)

Since the Hall effect is measured without current flow in the y direction, i.e. Jy = 0, this condition gives rise to the following relation Ey = −

σ yx σx y Ex = E x = −ωc τ E x . σ yy σx x

(7.22)

Inserting E y into Jx of (7.21b), we get Jx =

σx2x + σx2y σx x

Ex .

(7.23)

It is very interesting to point out that (7.20a) and (7.20b) result in Jx =

ne2 τ E x = neμE x = σ0 E x . m∗

(7.24)

This result means that the current density Jx is independent of the magnetic field Bz under the assumption we have used above, and that the resistivity is not changed by the application of a magnetic field, resulting in no magnetoresistance effect. We know that this conclusion conflicts with the experimental observations and that all

380

7 Magnetotransport Phenomena

semiconductors exhibit magnetoresistance. This conflicting conclusion arises from the following incorrect assumptions: (1) isotropic effective mass (spherical energy surface), (2) electron relaxation time τ independent of electron energy and all electrons drifting with the same velocity v, (3) shape of the sample not considered (the length is infinite). Although these assumptions will lead to wrong conclusions, the relations derived here give the correct expressions when we introduce the averaging procedures later. For this reason we shall proceed with the theoretical analysis of magnetotransport with the above simplified assumptions. From (7.21b) and (7.23) we have Ey =

σx y σx y Ex = 2 Jx = RH Bz Jx , σx x σx x + σx2y

(7.25)

and the Hall coefficient is generally expressed as RH =

σx y 1 . σx2x + σx2y Bz

(7.26)

Under the above assumption, substituting (7.20a), (7.20b) or (7.24) into (7.25) we obtain Jx 1 = − Bz Jx (7.27) E y = −ωc τ E x = −μBz σ0 ne and thus RH = −1/ne, which is equivalent to (7.2). Next, we will consider the case where two types of carriers are present. Let us identify two types of carriers by using subscripts 1 and 2. We therefore obtain (1) (2) Jx = σx(1)x + σx(2) x E x + σx y + σx y E y , (1) (2) Jy = σx(1)y + σx(2) y E x + σx x + σx x E y .

(7.28a) (7.28b)

Let us define the electrical conductivity for each carrier by σ1 and σ2 , and the Hall coefficient by R1 and R2 . Then, from (7.20a) and (7.20b) we have for carrier 1 σx(1)x =

σ1 σ12 R1 Bz (1) , σ = − x y 1 + σ12 R12 Bz2 1 + σ12 R12 Bz2

(7.29)

and similar relations for carrier 2. From the condition for achieving the Hall effect we put Jy = 0 and in the same way as we derived (7.26) we obtain R H Bz =

σx(1)y + σx(2) y 2 . (1) (1) (2) 2 σx x + σx x + σx y + σx(2) y

(7.30)

7.1 Phenomenological Theory of the Hall Effect

381

Inserting (7.29) and the same expression for carrier 2 in this equation we find RH =

σ12 R1 (1 + σ22 R22 Bz2 ) + σ22 R22 (1 + σ12 R12 Bz2 ) . (σ1 + σ2 )2 + σ12 σ22 (R1 + R2 )2 Bz2

(7.31)

It is very important to point out here that (7.31) is valid even if the relaxation time τ (τ1 and τ2 ) depends on the carrier energy, and thus it gives the general expression for the Hall coefficient with two types of carriers. Since σ1 |R1 | = μ1 and σ2 |R2 | = μ2 , in the weak magnetic field case such as μ1 Bz 1 and μ2 Bz 1, (7.31) may be approximated as RH (0) =

σ12 R1 + σ22 R2 . (σ1 + σ2 )2

(7.32)

On the other hand, in the high magnetic field case such that σ1 |R1 |Bz = μ1 Bz 1 and σ2 |R2 |Bz = μ2 Bz 1 are satisfied, we obtain

RH (∞) =

1 1 + R1 R2

−1

.

(7.33)

As an example, we consider the case of two carriers, electrons and holes, with respective mobilities μe and μh , densities n and p, and assume r H = 1 for simplicity. Inserting σ1 = neμe , σ2 = peμh , R1 = −1/ne and R2 = 1/ pe into (7.31) we obtain RH =

( p − nb2 ) + b2 μ2h Bz2 ( p − n) 1 · , (bn + p)2 + b2 μ2h Bz2 ( p − n)2 e

(7.34)

where b = μe /μh is the mobility ratio. Due to the assumptions described above, the above equation is valid for rH = 1 and thus for the case where the relaxation times are independent of energy and are constant. From this equation we find that the Hall coefficient becomes zero or RH = 0, when the following relation is satisfied: p=

nb2 (1 + μ2h Bz2 ) . 1 + b2 μ2h Bz2

(7.35)

The Hall coefficients at low magnetic fields, RH (0), and at high magnetic fields, R H (∞), are given as follows from (7.32) and (7.33): respectively. pμ2h − nμ2e p − b2 n = , 2 e( pμh + nμe ) e(nb + p)2 1 . RH (∞) = e( p − n) RH (0) =

(7.36) (7.37)

382

7 Magnetotransport Phenomena

7.2 Magnetoresistance Effects 7.2.1 Theory of Magnetoresistance We have discussed the current density in the presence of a magnetic field in Sect. 7.1, where we assumed free electrons with scalar effective mass m ∗ and constant drift velocity v. Under this assumption we have shown that no magnetoresistance effect appears. Here we discuss a more exact treatment of the magnetoresistance effect with the help of the Boltzmann transport equation. In the presence of a d.c electric field E and magnetic field B, the Lorentz force acting on the electrons given by the right-hand side of (7.12), and insertion of this relation into (6.90) results in e −

1 ∂E ∂f f − f0 f1 E+ ×B · =− =− . ∂k ∂k τ τ

(7.38)

Here, the distribution function f 0 under thermal equilibrium is a function of the electron energy E(k) and we find ∂ f 0 ∂E ∂ f0 = · . ∂k ∂E ∂k

(7.39)

The right-hand side of (7.38), − f 1 /τ , is obtained from the first-order approximation by inserting f 0 into f of the right-hand side: −

e f1 =− 2 τ

∂E ∂E ∂ f 0 ×B · . ∂k ∂k ∂E

(7.40)

Since [∂E(k)/∂k] × B is orthonormal to ∂E(k)/∂k, (7.40) becomes zero. Therefore, only the term f 1 of the distribution function f = f 0 + f 1 will contribute to the magnetic effect and (7.38) is approximated as −

∂ f0 e ∂E f1 f1 e E· − 2 ×B· =− . ∂k ∂k ∂k τ

(7.41)

In the following we will solve this equation under the assumption that the distribution function is not significantly changed in a weak electric field. In addition, we will not take account of the quantization of the electronic states.

7.2 Magnetoresistance Effects

383

7.2.2 General Solutions for a Weak Magnetic Field In a weak magnetic field B, except for B = 0, we may obtain solutions by an iterative method. We start from the solution for zero magnetic field. In zero magnetic field we have from (7.41) f1 =

eτ ∂ f0 eτ E· = ∂k

E·

∂E ∂ f 0 ∂E ∂ f 0 eτ Ej = ∂k ∂E ∂k j ∂E j

= f 1(0) ,

(7.42)

where E j and ∂E/∂k j represent the j component of E and ∂E/∂k, respectively. In the following we have omitted the symbol of summation. Inserting this f 1 into (7.41), the distribution function in the case of B = 0 is obtained in the first order of B, which is given by

∂ f 1(0) eτ ∂E × B · 2 ∂k ∂k

2

∂ ∂ f 1(0) e τ ∂E ∂E ×B · ×B · + 4 τ ∂k ∂k ∂k ∂k

f 1 = f 1(0) +

= f 1(2) .

(7.43)

Inserting this in the equation of current density e J =− 3 4π

e v f1d k = − 3 4π 3

1 ∂E f 1 d3 k, ∂k

(7.44)

we obtain the current density in the general form in the presence of a weak magnetic field. The equation may be written in the tensor form Ji = σi j E j + σi jl E j Bl + σi jlm E j Bl Bm ,

(7.45)

where the first, second and third terms on the right-hand side are respectively obtained from the first, second and third terms on the right-hand side of (7.43). Rewriting (7.44) as e ∂E f 1 d3 k, (7.46) Ji = − 3 4π ∂ki we obtain the following relations:

384

7 Magnetotransport Phenomena

σi jl σi jlm

∂ f 0 ∂E ∂E τ , ∂E ∂ki ∂k j

∂E ∂ ∂E e3 3 ∂ f 0 ∂E τ rls , τ =− 3 4 d k 4π ∂E ∂ki ∂kr ∂ks ∂k j e4 ∂ f 0 ∂E τ = − 3 6 d3 k 4π ∂E ∂ki

∂E ∂ ∂ ∂E ∂ τ τ mr s ltu , × ∂kr ∂ks ∂kt ∂ku ∂k j

e2 σi j = − 3 2 4π

d3 k

(7.47a) (7.47b)

(7.47c)

where lr s is called the permutation tensor and has the following relations. When two of the subscripts lr s are the same, lr s = 0. When the subscripts are in the order 12312 · · · and 21321 · · · , lr s are 1 and −1, respectively. The coefficients defined in (7.47b)–(7.47c) are general expressions for the electrical conductivity tensor in the presence of a magnetic field, and its i j component is given by (σi j + σi jl Bl + σi jlm Bl Bm ). Here, σi j is the second-rank tensor of the electrical conductivity and the equivalent to the conductivity for B = 0. σi jl is the third-rank Hall effect tensor and σi jlm is the fourth-rank magnetoconductivity tensor. The physical meaning of these tensors can be understood from the following examples.

7.2.3 Case of Scalar Effective Mass The constant energy surface of conduction band is assumed to be spherical and expressed as 2 2 k , (7.48) E(k) = 2m ∗ where m ∗ is the scalar effective mass. Then we have the following relations: 2 ∂E = ∗ ki , ∂ki m

∂2 2 = ∗ δi j . ∂ki ∂k j m

(7.49)

Inserting these relations into (7.47b)–(7.47c), we carry out the integration using polar coordinates with the polar axis along the electric field E and with the angle θ between k and E. In other words, we may put d3 k = k 2 sin θdθdφdk and we obtain from (7.47b) 2π ∞ π e 2 2 ∂ f0 2 τ δi j dk · k dθ · sin θ dφ · k 2 · cos2 θ 3 ∗2 4π m ∂E 0 0 0 ∞ ∞ 2ne2 3/2 ∂ f 0 1/2 dE =− τ E E f dE δi j . (7.50) 0 3m ∗ ∂E 0 0

σi j = −

7.2 Magnetoresistance Effects

385

Using (6.103) in the above equation, we find the same result as (6.106). In the case of non-degenerate semiconductors, the above result leads to (6.114). In a similar fashion, we may calculate (7.47c) and (7.47c), giving rise to the following relations: ne2 τ δi j = σ0 δi j , m∗ ne3 = − ∗2 τ 2 i jl = γ0 i jl , m ne4 3 = ∗3 τ mis ls j = β0 mis ls j . m

σi j =

(7.51a)

σi jl

(7.51b)

σi jlm

(7.51c)

Therefore, if we write the current density tensor in a weak magnetic field as [J ] = [σ(B)][E],

(7.52)

we obtain the electrical conductivity tensor [σ(B)] given by [σ(B)] =

⎡

σ0 + β0 [B y2 + Bz2 ] γ0 Bz − β0 Bx B y

−γ0 B y − β0 Bx Bz

⎤

⎢ ⎥ ⎣ −γ0 Bz − β0 Bx B y σ0 + β0 (Bx2 + Bz2 ) γ0 Bx − β0 B y Bz ⎦ .(7.53) γ0 B y − β0 Bx Bz −γ0 Bx − β0 B y Bz σ0 + β0 (Bx2 + B y2 )

Here we will separate the conductivity tensor into terms independent of the magnetic field B, and terms proportional to B and to B 2 , and then we find the following relations: ⎡ ⎡ ⎤ ⎤ σ0 0 0 0 γ0 Bz −γ0 B y 0 γ0 Bx ⎦ , σi j = ⎣ 0 σ0 0 ⎦ , σi jl Bl = ⎣ −γ0 Bz γ0 B y −γ0 Bx 0 0 σ0 ⎡ ⎤ −β Bx Bz β0 (B y2 + Bz2 ) −β0 Bx B y σi jlm Bl Bm = ⎣ −β0 Bx B y β0 (Bx2 + Bz2 ) −β0 B y Bz ⎦ . (7.54) −β0 Bx Bz −β0 B y Bz β0 (Bx2 + B y2 ) Next, we discuss the Hall effect in a weak magnetic field. In order to compare the results of Sect. 7.1, we assume that the magnetic field B is applied in the z direction and Bx = B y = 0. Then we obtain from (7.53) and (7.54) Jx = (σ0 + β0 Bz2 )E x + γ0 Bz E y , Jy = −γ0 Bz E x + (σ0 +

β0 Bz2 )E y .

(7.55a) (7.55b)

Comparing this with (7.20a)–(7.20c), (7.21b) and (7.21b) the following results are derived.

386

7 Magnetotransport Phenomena

ne2 ne2 ωc2 3 τ − τ , m∗ m∗ 2 ne ωc 2 = γ0 Bz = − τ . m∗

σx x = σ yy = σ0 + β0 Bz2

(7.56a)

σx y = −σ yx

(7.56b)

Here the final expressions of the above equations are rewritten by using (7.51b)– (7.51c) and the cyclotron frequency ωc = eBz /m ∗ . When τ is independent of the electron energy, we have τ n = τ n and thus (7.20a) and (7.20b) agree with (7.56b) and (7.56b) in the limit of a weak magnetic field ωc τ 1. The Hall coefficient is also obtained by introducing the condition Jy = 0 as follows. Putting Jy = 0 in (7.55b), we calculate E x and insert it into (7.55b) to obtain σx y γ0 Jx = Jx Bz . σx2x + σx2y (σ0 + β0 Bz2 )2 + γ0 Bz2

Ey =

(7.57)

Therefore, the Hall coefficient RH is given by RH =

σx y γ0 γ0 ∼ Jx = = 2, σx2x + σx2y (σ0 + β0 Bz2 )2 + γ02 Bz2 σ0

(7.58)

where the final result is obtained by taking account of the fact that σ0 β0 Bz2 and σ0 γ0 Bz in the weak magnetic field limit. Substituting (7.51c) in (7.58), the Hall coefficient in a weak magnetic field is written as rH , ne

(7.59)

τ 2 . τ 2

(7.60)

RH = − where rH is defined by rH =

According to the above results we find that the scattering factor of the Hall effect rH may be calculated when the distribution function and energy dependence of the relaxation time τ are known. As an example, we assume a Maxwellian distribution function and τ = aE −s , and then from (6.116) the following result is obtained: rH =

Γ (5/2 − 2s)Γ (5/2) . [Γ (5/2 − s)]2

(7.61)

In the case of acoustic phonon scattering as discussed in Sect. 6.4 (see (6.341)), we have s = 1/2 and rH =

3π = 1.18, 8

(7.62)

7.2 Magnetoresistance Effects

387

Fig. 7.2 a: Hall coefficients of n-Ge are plotted as a function of inverse temperature 1/T for five samples with different doping. The straight line shows the intrinsic region where electrons n and holes p satisfy n = p. b: Measured resistivity as a function of 1/T

Fig. 7.3 Carrier density n = 1/(RH e) are plotted as a function of 1/T for five samples. b: Hall mobility μ = RH σ is plotted and theoretical Hall mobility due to acoustic phonon scattering with deformation potential Ξ = 11.5 eV is plotted as a function of temperature T

which is very close to 1. In the case of impurity scattering, however, we have s = −3/2, as derived in Sect. 6.4, and rH =

315π = 1.93, 512

(7.63)

which means that the Hall mobility is almost twice the drift mobility. Here we present the most famous and the most important Hall effect measurement and its analysis reported by Debye and Conwell [13]. Figure 7.2a shows the reproduction of the reported Hall coefficients as a function of inverse temperature for different samples shaped of Hall bar as seen in the inset. The sharp drop of RH at higher temperatures indicates intrinsic region (electron density n and hole density p satisfies n = p). Measured resistivity ρ = 1/σ is plotted in Fig. 7.2b. Using the experimental data the carrier (electron) density is obtained by n = 1/(RH e), which is shown in Fig. 7.3a and obtained carrier (electron) Hall mobility by the relation (7.10), μH = RH · σ, is plotted in (b) as a function of temperature T . The flat region of n corresponds th the case where electrons are excited completely from the doped donors ND except the electrons captured by acceptors NA , in other words, n = ND − NA . Electron Hall mobility calculated with the deformation potential Ξ = 11.5 eV and rH = 1.18 is plotted by red dashed curve. The doping densities, or

388

7 Magnetotransport Phenomena

effective donor densities, ND − NA , are 1.0 × 1013 for sample number 55, 1.4 × 1014 for 51, 1.7 × 1015 for 64, 7.5 × 1015 for 54, and 5.5 × 1016 1/cm3 for 61. Samples with higher doping exhibit lower mobility at lower temperature, which means electron mobility is strongly affected by impurity scattering at low temperatures.

7.2.4 Magnetoresistance Here we will derive the Hall coefficient and magnetoresistance in a semiconductor with scalar mass in an arbitrary magnetic field. Let us assume the distribution function f 1 = c · k,

(7.64)

and determine the coefficient c. Inserting this f 1 into (7.41) we obtain

e ∂ f 0 ∂ e c · k = 0. E+ ∗B× (c · k) − m ∗ ∂E m ∂k τ

(7.65)

The coefficient c is determined by dividing (7.65) into its components and solving the simultaneous equations of cx , c y and cz . Inserting the components cx , c y and cz into (7.64) and rewriting again in a vector form we obtain f1 =

τ ∂ f0 e m ∗ 1 + (eτ /m ∗ )2 B 2 ∂E eτ 2 eτ (B · E)B · k. × E+ ∗B×E+ m m∗

(7.66)

Here we show that the above result coincides with that obtained for the weak magnetic field case. Rewriting the coefficient of the above equation as ωc2 τ 3 τ =τ− , 2 2 1 + ωc τ 1 + ωc2 τ 2 we easily find that it may be approximated τ − ωc2 τ 3 in the case of ωc τ 1, leading to conductivity tensor (7.53) for low magnetic field case. From such a comparison the conductivity tensor for an arbitrary magnetic field is obtained from (7.53) by replacing τ2 ne3 , m ∗2 1 + ωc2 τ 2 τ3 ne4 , β0 → β = − ∗3 m 1 + ωc2 τ 2 γ0 → γ = −

(7.67a) (7.67b)

where · · · is the averaged value over the distribution function as given by (6.116).

7.2 Magnetoresistance Effects

389

In the case of Bx = B y = 0, Bz = 0, and E z = 0, we obtain Jx = (σ0 + β Bz2 )E x + γ Bz E y τ ne2 ωc τ 2 Ex − Ey , = ∗ m 1 + ω2 τ 2 1 + ωc2 τ 2 Jy = −γ Bz E x + (σ0 + β Bz2 )E y ωc τ 2 ne2 τ E Ey . = ∗ + x m 1 + ωc2 τ 2 1 + ωc2 τ 2

(7.68a)

(7.68b)

From a comparison of these relations with (7.17b) and (7.17c), we find that the difference is the averaging by the distribution function. Therefore, we obtain for the Hall coefficient τ2 1 1 + ωc2 τ 2 RH = − (7.69) 2 2 ne τ τ2 2 + ωc 1 + ωc2 τ 2 1 + ωc2 τ 2 and thus the scattering factor of the Hall coefficient rH is given by τ2 1 + ωc2 τ 2 rH = 2 2 . 2 τ τ + ωc2 1 + ωc2 τ 2 1 + ωc2 τ 2

(7.70)

Next, deriving E y from the condition Jy = 0 and inserting it into (7.68b), we obtain Jx =

σ(B) =

σx2x + σx2y σx x ne2 m∗

E x = σ(B)E x ,

2 2 τ τ2 2 + ω c 1 + ωc2 τ 2 1 + ωc2 τ 2 . τ 1 + ωc2 τ 2

(7.71a)

(7.71b)

Equation (7.69) leads to the Hall coefficient in two extreme cases. In a weak magnetic field such that ωc τ 1, (7.59) and (7.60) are deduced. On the other hand, in a strong magnetic field such that ωc τ 1, we obtain 1 RH ∼ =− , ne

(7.72)

390

7 Magnetotransport Phenomena

and the Hall coefficient is independent of the scattering mechanisms and exhibits saturation. The magnetoresistance is calculated from (7.71b). Since the resistivity ρ is related to the conductivity σ by the relation ρ = 1/σ, expressing these by

Δσ , σ = σ0 1 − σ0

Δρ , ρ = ρ0 1 + ρ0

(7.73a) (7.73b)

the magnetoresistance and magnetoconductance in a weak magnetic field are obtained from (7.71b) and from the assumption of Δσ/σ0 1 as −

τ 3 τ − τ 2 2 Δρ Δσ = = ωc2 . σ0 ρ0 τ 2

(7.74)

This may be rewritten as the following by defining the Hall coefficient given by (7.59) at low magnetic field as RH (0) and using (7.60): Δρ Δσ =− = ξ RH (0)2 σ02 Bz2 = ξ(μH Bz )2 , ρ0 σ0 τ 3 τ − 1. ξ= τ 2 2

(7.75a) (7.75b)

When we assume a relation τ = aE −s , ξ is given by ξ=

Γ (5/2 − 3s)Γ (5/2 − s) − 1. [Γ (5/2 − 2s)]

(7.76)

For acoustic phonon scattering, s = 1/2, the above expression reduces to ξ=

4 − 1 = 0.273, π

(7.77)

and for ionized impurity scattering, s = −3/2, we obtain ξ=

32768 − 1 = 0.577. 6615π

(7.78)

In general, τ 3 τ is larger than τ 2 2 , and the relation ξ ≥ 0 holds. Therefore, in the presence of a magnetic field, the resistivity increases, showing positive magnetoresistance. It is also clear that no magnetoresistance appears in the case of constant τ (τ is independent of electron energy) because we have ξ = 0 for this case. Another important conclusion is drawn for a degenerate semiconductor. Since

7.3 Shubnikov–de Haas Effect

391

∼ τn ∂ f 0 /∂E is approximated by the δ-function in degenerate semiconductors, τ n = F and ξ ∼ = 0, indicating that the magnetoresistance is extremely small for a degenerate semiconductor with scalar effective mass. The physical meaning of the magnetoresistance is as follows. In a transverse magnetic field an electron is exposed to a Lorentz force, moving in the direction perpendicular to the magnetic field and the current, and induces the Hall field. When the force due to the Hall field balances the Lorentz force, the electron will move straight through the sample. However, the electrons are distributed over the energy range determined by the distribution function and thus there exist electrons with lower and higher velocities compared to the average velocity which produces the Hall field. The Lorentz force of the electrons with lower and higher velocities will not balance the force due to the Hall field and and thus they spread out, resulting in increasing resistivity (magnetoresistance: Δρ/ρ0 ≥ 0). Finally, we derive the magnetoresistance in a high magnetic field. From (7.71b) the conductivity σ∞ and resistivity ρ∞ in the limit of ωc τ 1 are given by σ0 ρ∞ = = 1/τ τ , σ∞ ρ0

(7.79)

and again assuming the relation τ = aE −s we obtain ⎧ 32 ⎪ ⎪ ⎪ ⎨ 9π = 1.13 (s = 1/2),

ρ∞ Γ (5/2 + s) · Γ (5/2 − s) = = ⎪ ρ0 [Γ (5/2)]2 ⎪ 32 ⎪ ⎩ = 3.39 (s = −3/2). 3π

(7.80)

7.3 Shubnikov–de Haas Effect 7.3.1 Theory of Shubnikov–de Haas Effect In Sect. 2.5 we have discussed electron motion in a magnetic field and explained that the electron cyclotron motion is quantized to form Landau levels. In addition the density of states for the quantized electrons is given by (2.132) and the features are shown in Fig. 2.15. Considering a degenerate semiconductor, and letting the electron density be n and the Fermi energy be E F , we have in the limit of temperature T = 0 EF =

2 2 2/3 3π n . 2m ∗

(7.81)

When a magnetic field applied to the semiconductor is changed, the Fermi energy passes through the bottoms of the Landau levels. In a magnetic field such that the Fermi energy is located at the bottom of one of the Landau levels, where the density

392

7 Magnetotransport Phenomena

of states is a maximum, the scattering rate for electrons is high because there are many final states for scattered electrons. If the Fermi energy is not changed by the presence of magnetic field, the above condition is written as

EF = ωc

1 N+ 2

eB = ∗ m

1 N+ , 2

N = 0, 1, 2, . . .

(7.82)

and therefore the magnetoresistance oscillates periodically with the inverse magnetic field 1/B. The period is then given by Δ

e 1 2e 2 −2/3 = ∗ = 3π n . B m EF

(7.83)

This phenomenon is called the Shubnikov–de Haas effect. It is not possible to explain the Shubnikov-de Haas effect by the classical theory of the Boltzmann transport equation. One of the most well-known and understandable methods for this is the density matrix method. The Kubo formula, a generalized linear theory, has been widely used to understand quantum transport including the Shubnikov–de Haas effect and the detail is found in references [2, 3]. Here we will try to explain it in a simplified manner. Using the result of the previous section, in a magnetic field applied in the z direction, the transverse magnetoresistance ρ⊥ , longitudinal magnetoresistance ρ and Hall coefficient RH are, respectively, given by ρ⊥ =

σx2x

σx x , + σx2y

1 , σzz σ yx 1 RH = − . 2 Bz σx x + σ 2yx ρ =

(7.84a) (7.84b) (7.84c)

As described later, not only the Shubnikov-de Haas effect but also other quantum effects, namely the quantum galvanomagnetic effect, are observed under the condition ωc τ = μBz 1. Under this condition σx y σx x is satisfied and thus we obtain the relations σx x ρ⊥ ∼ = 2 , σx y 1 . RH ∼ =− Bz σ yx

(7.85a) (7.85b)

In the a case where ωc τ 1 is satisfied, the magnetoresistance effect cannot be treated by classical theory. This is understood from the discussion stated in Sect. 2.5. When ωc τ 1 is satisfied, the electron motion of the Landau orbit results in the

7.3 Shubnikov–de Haas Effect

393

formation of Landau levels. When an electric field E x is applied in the x direction, perpendicular to the magnetic field applied in the z direction, the electron will move with a velocity E x /Bz in the y direction as shown on the left of Fig. 2.14. In other words, as shown by (2.127), the cyclotron center coordinates (X, Y ) are given by Ex , Y˙ = Bz

X˙ = 0,

(7.86)

and the electron moves with a constant velocity in the y direction. This gives us the current density Jy = neE x /B y = σ yx E x , and therefore we obtain the conductivity σ yx ne σ yx = . (7.87) Bz Inserting this conductivity tensor into (7.85b), we find that the result agrees with the Hall coefficient (7.72) for high magnetic field obtained in Sect. 7.2: 1 RH ∼ =− . ne

(7.88)

Since no current flows in the x direction, we have σx x = 0. In experiments we observe current in the x direction, which may be interpreted as follows. As shown on the right of Fig. 2.14, scattering of an electron results in a change of its cyclotron center, and its component along the x direction gives rise to a current component Jx and thus to σx x = 0. It is very interesting to point out that the current due to the drift motion is disturbed by scattering according to the classical transport theory, whereas in the presence of a high magnetic field a current component along the electric field direction is induced by electron scattering. From the example stated above, we find that quantum magnetotransport phenomena are completely different from classical transport phenomena. Also, we have to note again that the electron motion is quantized due to cyclotron motion in the plane perpendicular to the magnetic field, giving rise to one-dimensional motion allowed only along the z direction. This quantization leads to the density of states shown in Fig. 2.15. The one-dimensional density of states results in a divergence of the electron scattering rate at the bottom of the Landau level. To calculate the current density by solving a transport equation, the current density is evaluated with the electron density of states by averaging over the electron energy. Therefore, the density of states appears twice in the calculations, resulting in a logarithmic divergence of the current. This means that the current and thus the conductivity plotted as a function of inverse magnetic field oscillate periodically. Although magnetotransport phenomena are often analyzed by the density matrix method or Kubo formula [3] as stated earlier, here we describe the outline of the method adopted by Roth and Argyres [2]. We define the one-electron Hamiltonian in a magnetic field by H0 , which is written as 1 (7.89) H0 = ( p + e A)2 + gμB s · B, 2m ∗

394

7 Magnetotransport Phenomena

where the electron spin is considered, g is the effective g-factor, and μB = e/2 m. The eigenvalues for the Hamiltonian (7.89) may be given by the following equation from the analogy of the treatment stated in Sect. 2.5:

Enk± =

2 k z2 1 ν ωc + Ez ; Ez = N+ ± , 2 2 2m ∗

(7.90)

where ν = m ∗ g/2m. Also, it is evident that the density of states is given by 1 δ[E N k± − E] V N k±

−1/2

∗ 1/2 1 ν 2m 1 E− N+ ± ωc = . 2 (2πl)2 N ,± 2 2

g(E, Bz ) =

(7.91)

Here, V = L 3 is the crystal volume and l = (/eB)1/2 = (/m ∗ ωc )1/2 is defined by (2.108), which corresponds to the classical cyclotron radius. In general we may express the density of states g (d) for a d-dimensional band as g

(d)

2 2 = δ[Ek − E] = dd k V (2π)d

(7.92)

k

and for a three-dimensional band we have g (3) (E) =

2 (2π)3

d3 k =

2 (2π)3

4πk 2 dk =

1 2π 2

2m ∗ 2

3/2 E 1/2 .

(7.93)

The one-dimensional density of states in a magnetic field is evaluated by using the Poisson summation formula:

∞ +∞ 1 = Φ m+ (−1)r Φ(x)e2πir x dx 2 0 −∞ m=0 ∞

(7.94)

and the following relation is obtained in the limit of ωc 1 using the threedimensional density of states, g (3) : g(E, Bz ) =

g (3) 1 +

∞ 2πE π ωc 1/2 (−1)r cos(πνr ) . (7.95) cos r − 2E ωc 4 r 1/2 r =1

From these results we find that the density of states oscillates periodically with inverse magnetic field 1/Bz . This oscillatory feature is reflected in the magnetoresistance oscillations.

7.3 Shubnikov–de Haas Effect

395

The one-electron density matrix, ρT (t), satisfies (see Appendix F for the density matrix) dρT = H0 + H + F, ρT , i (7.96) dt where H is the scattering potential, and F represents the interaction with an electric filed E given by F = e E · r. (7.97) The current density J is evaluated from J =−

e Tr(ρT v), V

(7.98)

where V is the crystal volume, and v = ( p + e A)/m ∗ is the velocity operator stated in Sect. 2.5 and given by v=

1 px , k y + eBx, k z . m∗

(7.99)

Since the total number of electrons is conserved, we have for the electron density n 1 Tr(ρT ) = n. V

(7.100)

ρT = ρ0 + ρ(t),

(7.101)

Rewriting the density matrix as

ρ0 is written using the Fermi–Dirac distribution function as ρ0 =

1 . e(E−EF )/kB T + 1

(7.102)

Using these results (7.96) is rewritten as i

dρ(t) = [H0 + H , ρ(t)] + [F, f (H0 + H )]; ρ(0) = 0, dt

(7.103)

where f is the Fermi–Dirac distribution function. Solving the above equation for the one-electron density matrix for the electron–phonon interaction, the current density is evaluated from (7.98) and so we derive the magnetoconductivity.

396

7 Magnetotransport Phenomena

7.3.2 Longitudinal Magnetoresistance Configuration The case where the magnetic and electric fields are applied in the same direction, the z direction, is called the longitudinal configuration and the magnetoresistance is called the longitudinal magnetoresistance. For simplicity we define a new subscript μ instead of the subscripts N k±. Then the equation of motion for the diagonal element of the density matrix ρμ is written as the following [11]:

wμν ρμ (1 − ρν ) − wνμ ρν (1 − ρμ ) = eE z vμz

ν

d f (Eμ ) , dEμ

(7.104)

where vμz is the z component of the velocity operator v μ for the Landau state |μ = |N k± and wμν is the scattering rate of an electron between the Landau states |μ and |ν which is given by wμν = wνμ =

2π 2 |H | δ[Eμ − Eν ]. μν

(7.105)

Measurements of the Shubnikov–de Haas effect in semiconductors have been carried out at low temperatures to achieve the condition ωc τ 1, where impurity scattering and acoustic phonon scattering are dominant. The scattering probabilities are obtained from the method described in Sect. 6.2. It should be noted that electron spin is conserved in the scattering. For impurity scattering we have wμν =

!" ! ! #!2 2π N I |H (q)|2 ! μ !eiq·r ! ν ! δ[Eμ − Eν ], V q

(7.106)

and for acoustic phonon scattering we obtain wμν =

!" ! ! #!2 2π |C(q)|2 ! μ !eiq·r ! ν ! q × (n q + 1)δ[Eμ − Eν − ωq ] + n q δ[Eμ − Eν + ωq ] ,

(7.107)

which are shown in Chap. 6. Here, q = ( j, q) represents mode j and wave vector q for an acoustic phonon with energy ωq , and n q is the Bose–Einstein distribution function given by n q = 1/[exp(ωq /kB T ) − 1]. The matrix element μ| exp(iq · r)|ν appearing in both impurity and acoustic phonon scattering is evaluated from the eigenfunctions of (2.120). The detail of the evaluation is given by Kubo et al. [3]. We expand the diagonal element of the density matrix as ρμ = f (Eμ ) + ϕμ

d f (Eμ ) , dEμ

(7.108)

7.3 Shubnikov–de Haas Effect

397

where f (E) = 1/[exp{(E − EF )/kB T } − 1] is the Fermi–Dirac distribution function and d f /dE is given by (6.103). Impurity scattering is known to be elastic scattering. Assuming that the acoustic phonon scattering is elastic, we find that f (Eμ ) before scattering is equal $ to f (Eν ) after scattering. Therefore, the left-hand side of (7.104) is rewritten as ν wμν (ρμ − ρν ), and (7.104) reduces to

wμν (ϕμ − ϕν ) = eE z vμz .

(7.109)

ν

When we adopt the relaxation time approximation as in Sect. 6.2, which is used for solving the classical Boltzmann transport equation, it is possible to express the above relation as ϕμ wμν (ϕμ − ϕν ) = , (7.110) τμ ν where the following relation holds between the relaxation time τμ and scattering probability wμν :

k 1 = w N k±,N k ± 1 − z . (7.111) τ N k± kz N k

As described in Sect. 6.4, the inverse of the relaxation time is equivalent to the scattering rate in the case of isotropic and elastic scattering and therefore we have ϕμ = eE z τμ vμz .

(7.112)

Inserting this into (7.108) and using the result to evaluate (7.98), we obtain the longitudinal magnetoresistance given by ρ−1

= σzz = −

2 e2 d f τ ± (E N k ) v Nz k . V dE N k±

(7.113)

N k±

The Fermi energy of electron in the presence of a magnetic field is determined from (7.91) as ∞ n= f (E)g(E, Bz )dE. (7.114) 0

Assuming that the electron density is conserved, the Fermi energy in a magnetic field EF differs from the Fermi energy for zero magnetic field EF0 and depends on the magnetic field. In general, we may expand the Fermi energy in a magnetic field as EF = EF(0) + EF(1) Bz2 + EFosc ,

(7.115)

398

7 Magnetotransport Phenomena

where EFosc is is a sum of quasi-periodic functions in 1/Bz , whose amplitude is proportional to (ωc /EF(0) )3/2 EF(0) and is small compared to EF(0) . In general, neglecting the terms beyond the first term on the right-hand side of (7.115), the Fermi energy is often approximated as EF = EF(0) . As discussed in Sect. 6.2.2, d f /dE in (7.113) is given by −(1/kB T ) f (1 − f ), which behaves like a δ-function, and thus in the limit of kB T ωc we obtain ρ−1

% 4 EF(0) n± −1 = ρ0 , nωc ± $ EF − (N + 1 ± 1 ν)ωc −1/2 N 2 2

(7.116)

where ρ0 = m ∗ /ne2 τ0 (EF(0) ) is the resistivity for Bz = 0, τ0 (EF(0) ) is the relaxation time for electrons with Fermi energy at Bz = 0, n ± are the electron densities for electron spins ±, and n = n + + n − . In the case of EF ωc , the longitudinal magnetoresistance for an arbitrary value of kB T /ωc is written as

∞ 2πEF π ∼ ρ = ρ0 1 + br cos r− , ωc 4 r =1

(7.117)

where br =

(−1)r r 1/2

ωc 2EF

1/2

2π 2 r kB T /ωc cos(πνr )e−2πr Γ /ωc , sinh(2π 2 r kB T /ωc )

(7.118)

and the broadening of the density of states for electrons (broadening energy Γ ) is taken into account. We find from this equation that the longitudinal magnetoresistance oscillates periodically when plotted versus 1/Bz , as stated earlier.

7.3.3 Transverse Magnetoresistance Configuration In the transverse magnetoresistance configuration, the electric field is applied perpendicular to the magnetic field and the observed magnetoresistance is called the transverse magnetoresistance. Calculations of the transverse magnetoresistance is complicated compared to the longitudinal magnetoresistance. This is understood from the following. In a magnetic field in the z direction, the application of an electric field in the x direction, for example, causes an electron quantized in the x, y plane to move in the y direction with a constant velocity E x /Bz in the absence of electron scattering and thus to no current flow in the x direction. The electron current is induced by scattering, which gives rise to a change of the cyclotron center in the x direction, and results in the current in the x direction and in σx x = 0. In the transverse magnetoresistance configuration, Kubo et al. derived the solution of (7.96) for the elastic scattering case [3, 12]:

7.3 Shubnikov–de Haas Effect

σx x

πe2 = V

∞

dE −∞

399

df Tr δ(E − H )[H , X ]δ(E − H )[H , X ] , dE

(7.119)

where H = H0 + H and X is the operator for the x component of the cyclotron center coordinate. From the above equation the following relation is obtained by taking in account the broadening effect due to collisions [2]:

∞ 2πEF π 5 +R , br cos r− ρ⊥ = ρ0 1 + 2 r =1 ωc 4 ∞

3 ωc 2πEF 2πEF R= br αr cos r + βr sin r 4 2EF r =1 ωc ωc 4πΓ /ωc . −log 1 − e

(7.120a)

(7.120b)

Here, br is given by (7.118), and coefficients αr and βr are given by αr = 2r 1/2

∞ s=1

βr = r 1/2

r −1 s=1

1 e−4πsΓ /ωc , [s(r + s)]1/2

1 . [s(r − s)]1/2

(7.121a)

(7.121b)

These results mean that the transverse magnetoresistance oscillates periodically in the plot versus 1/Bz as in the case of longitudinal magnetoresistance. The second term on the right-hand side in (7.120b) is the oscillatory component due to the transition induced by a change in the quantum number N , whereas R is due to the transition without changing the quantum number N and diverges when Γ is zero. This divergence arises from the fact that the integral with respect to the onedimensional density of states appears twice in the integral containing the scattering rate and distribution function, resulting in a logarithmic divergence for N = N . The contribution from each component depends on the magnitude of Γ /EF and the contribution from R becomes smaller for r > 1 (higher harmonic oscillatory component). Usually, therefore, the analysis has been carried out by neglecting the contribution from R. The amplitude of the oscillatory component of both the longitudinal and transverse magnetoresistance depends on the magnetic field and the temperature through the term T exp{−2π 2 kB (T + TD )/ωc }, 1/2 Bz where TD =

Γ πkB

(7.122)

400

7 Magnetotransport Phenomena

is called the Dingle temperature. On the other hand, the phase of the oscillatory component is −π/4 for both longitudinal and transverse configurations, but we have to note that the spin g factor is not included in the above calculations and that a comparison with experiment may be difficult. Next, a comparison of the theory with experiment is described. In experiments we have to apply electrodes to measure the resistivity in addition to the electrodes for current supply. Measurements of the Shubnikov–de Haas effect are strongly affected by the sample uniformity and thus require many electrode contacts for the resistivity measurement. Applying a constant current, the voltage drops between the pairs of contacts are measured and we choose the pair which shows the largest oscillation. The Shubnikov–de Haas effect is normally observed at low temperatures and measurements of the temperature dependence of the oscillations are required to estimate the effective mass. It is expected from the theory given above that the oscillation amplitude decreases exponentially with temperature, and thus the magnetic field modulation technique is often adopted in order to observe such a weak oscillatory behavior, where the second derivative magnetoresistance is detected. Recently it has been shown that the second-derivative signals directly obtained by computer analysis provides a good signal-to-noise ratio and a good quality of oscillatory structure. As an example, we show in Fig. 7.4 the experimental results on the Shubnikov–de Haas effect in n-GaSb [14], where the longitudinal and transverse magnetoresistance is plotted as a function of the inverse magnetic field and periodic oscillations in the inverse magnetic field 1/B are clearly observed, showing good agreement with the theoretical prediction stated above. From the period 2.75 T−1 and with the help of (7.83), the electron density n = 1.3 × 1018 cm−3 is obtained. Here we will discuss how to deduce the effective mass from the analysis of the Shubnikov–de Haas effect. When we put χ=

Fig. 7.4 Shubnikov–de Haas effect in nGaSb (n = 1.3 × 1018 cm−3 ), where the longitudinal and transverse magnetoresistance is plotted as a function of inverse magnetic field 1/B. (After Becker and Fan [14])

2π 2 kB T , ωc

7.3 Shubnikov–de Haas Effect

401

the temperature dependence of the oscillation amplitude is written as χ sinh χ =

2π 2 kB T /ωc . sinh(2π 2 kB T /ωc )

(7.123)

Inserting the relation ωc = eB/m ∗ into the above equation, it is easily seen that the effective mass m ∗ is estimated from the temperature dependence of the amplitude. The electron effective obtained by this method in n-GaSb is m ∗ = 0.05 m and the effective mass is found to depend on the electron density, probably due to the nonparabolicity of the conduction band. In general, the amplitude of the oscillatory magnetoresistance decays exponentially as the inverse magnetic field 1/B. This decay is due to the collision broadening of the Landau levels. The amplitude of the oscillatory components of the magnetoresistance due to the Shubnikov–de Haas effect depends on the magnetic field as

ωc EF

1/2

χ −2πΓ /ωc = e sinh χ

ωc EF

1/2

×e−2π

2π 2 kB T /ωc sinh(2π 2 kB T /ωc )

2

kB TD /ωc

,

(7.124)

where TD = Γ /πkB is the Dingle temperature defined before. Therefore, when the amplitude of the oscillatory components divided by [(ωc /EF )1/2 (χ/ sinh χ)] is plotted against 1/B, it will result in a straight line. From the slope of the plot we may estimate the Dingle temperature and thus the strength of the broadening. In Fig. 7.5 such a plot is shown for different electron densities in n-GaSb estimated from the Hall coefficient RH for n-GaSb at T = 4.2 K [14], where we find good agreement with the prediction of the theory. From the analysis the Dingle temperature TD = 6.6 K is obtained for an electron density n = 1.3 × 1018 cm−3 . We have define the Dingle temperature to express the Landau broadening and shown how to estimate it from experimental data. Another parameter to give the collision broadening may

Fig. 7.5 The oscillation amplitude of the longitudinal magnetoresistance in n-GaSb plotted as a function of the inverse magnetic field 1/B, where we find the exponential decay (Dingle temperature) depends on the electron density estimated from the Hall coefficient RH (after Becker and Fan [14])

402

7 Magnetotransport Phenomena

be estimated from the electron mobility; it is called the mobility temperature. The mobility temperature is defined by the relation Tm = /2πkB τm , where the relaxation time τm is estimated from the electron mobility. Becker and Fan have deduced the mobility temperature Tm = 4.9 K for n-GaSb with n = 1.3 × 1018 cm−3 .

7.4 Magnetophonon Resonance 7.4.1 Experiments and Theory of Magnetophonon Resonance In the previous section we discussed the Shubnikov–de Haas effect, where electrons quantized into Landau levels in the presence of a magnetic field are scattered elastically in the Landau levels and result in a periodic oscillation of the magnetoresistance with the inverse magnetic field 1/B. On the other hand, we will now consider the oscillatory magnetoresistance induced by inelastic electron scattering, which is known as magnetophonon resonance. The magnetophonon resonance is caused by the scattering of electrons between the Landau levels induced by optical phonon absorption and emission, and therefore magnetoresistance maxima appear when the multiple of the Landau level spacing is equal to the optical phonon energy. Strong resonance has been observed in III–V compound semiconductors, where the electron–LO phonon interaction is dominant. The resonance condition is then given by the following relation: N ωc = ωLO ,

N = 1, 2, 3, . . .

(7.125)

where LO is the LO phonon energy and ωc = eB/m ∗ is the cyclotron frequency of an electron with effective mass m ∗ . Observation of the magnetophonon resonance requires excitation of a sufficient number of LO phonons involved with the scattering. Since the excitation number of phonons is given by the Bose–Einstein distribution function 1 , (7.126) n LO = ω /k T e LO B − 1 the number of phonons is very small at such low temperatures that ωLO > kB T . At such low temperatures the broadening of the Landau levels is quite small and thus the quantum effect is clearly observed. But the number of excited phonons is limited, resulting in difficulty in observing the magnetophonon resonance at such low temperatures. On the other hand, at higher temperatures, there exist enough phonons to interact with electrons, but the Landau level broadening is quite large, and thus the quantization effect (magnetophonon resonance) is smeared out. Up to now magnetophonon resonance has been observed in most III–V semiconductors in which the electron–LO phonon interaction is strong, and the amplitude of the

7.4 Magnetophonon Resonance

403

∼ 150 K for magnetophonon oscillations exhibits a maximum at the temperature T = the reason stated above. It is well known that the observation of magnetophonon resonance is very difficult at temperatures below 40 K and above 350 K. However, at temperatures T ≤ 40 K, hot electrons produced by a high applied electric field application make transitions between the Landau levels by emitting LO phonons and exhibit magnetophonon resonance, which is called hot electron magnetophonon resonance. Magnetophonon resonance was first predicted theoretically in 1961 by Gurevich and Firsov [15], and then in 1963 Puri and Geballe [16] succeeded in observing the oscillatory behavior of the thermoelectric power in InSb in a magnetic field, which is caused by the magnetophonon effect. Magnetophonon resonance in the magnetoresistance in n-InSb was subsequently observed in 1964 by Firsov et al. [17]. When the LO phonon energy involved with the resonance is known, the effective mass of the electron is determined from (7.125) by analyzing the period of oscillation in the plot versus the inverse magnetic field. In addition magnetophonon resonance is observed at temperatures around T = 150 K; it provides information about the temperature dependence of the effective mass and about various electron–phonon interactions, as will be mentioned later. For this reason the study of magnetophonon resonance provided very important information in the period 1960–1970 and established its position for semiconductor research, especially in the field of quantum transport. The most important contribution to the study of magnetophonon resonance is the discovery of the empirical formula by Stradling and Wood [4], who obtained the following relation to express the oscillatory component from a series of experiments in III–V compound semiconductors:

ωLO ωLO cos 2π . ∝ exp − γ ¯ ρosc xx ωc ωc

(7.127)

This relation is called the empirical formula of Stradling and Wood. In (7.127) γ¯ represents the exponential decay of the oscillatory component in the plot versus the inverse magnetic field which arises from the Landau level broadening and corresponds to the Dingle temperature for the Shubnikov–de Haas effect. Magnetoresistance in the presence of magnetophonon resonance consists of monotonic increase with the magnetic field and an oscillatory component which is periodic with the inverse magnetic field. Clear signals are obtained by removing the monotonic component, and several methods have been proposed to observe the oscillatory components accurately. Stradling and Wood adopted the following method to detect the oscillatory component of the magnetoresistance by removing the monotonic component. The Hall voltage, proportional to σx−1 y , was subtracted from the voltage drop between the sample electrodes. Here the voltage drop is proportional to the magnetoresistance ρx x and the Hall voltage is proportional to the magnetic field which contains no oscillatory component in it, Later, magnetic field modulation and second-harmonic detection by a lock-in amplifier were successfully used for magnetophonon resonance measurements, where the second-harmonic component is proportional to the second derivative of the magnetoresistance with respect to the

404

7 Magnetotransport Phenomena

magnetic field. Recently, however, the numerical derivative of the magnetoresistance calculated by using a personal computer has provided an excellent method for such purposes. The magnetic field modulation technique is based on a superposition of a weak ac magnetic field B1 cos(ωt) with modulation frequency ω upon a dc magnetic field B and on the detection of the second-harmonic signals (2ω). In general, the magnetoresistance under the application of such a magnetic field is written as ρ[B + B1 cos(ωt)] dρ 1 d2 ρ = ρ(B) + B1 cos(ωt) + [B1 cos(ωt)]2 + · · · , dB 2 dB 2

(7.128)

where the third term of the right-hand side contains the component oscillating as cos(2ωt). Therefore, when the second-harmonic component is detected by a lock-in amplifier, the signal is proportional to the second derivative of the magnetoresistance. This method discriminate the monotonic component from the magnetoresistance and gives −d2 ρ/dB 2 , or the signals very close to the oscillatory component given by (7.127). We have to note here that the second derivative of (7.127) has a contribution from the exponential term and thus the experimentally observed second derivative will not give (7.127). However, a correction is possible to estimate all the parameters ¯ required for the analysis of magnetophonon resonance such as ωLO and γ. As an example, Fig. 7.6 shows the experimental results for magnetophonon resonance in n-GaAs at T = 160 K [18]. In Fig. 7.6 three curves are compared: the

Fig. 7.6 Magnetophonon resonance observed in n-GaAs at T = 77 K. ρ(B) is the transverse magnetoresistance as a function of magnetic field, dρ/dB is the first derivative of the magnetoresistance measured by magnetic field modulation technique and −d2 ρ/dB 2 is the second-derivative of the magnetoresistance. The second derivative signals reveal magnetophonon resonance very clearly. (After Hazama et al. [18])

7.4 Magnetophonon Resonance

405

transverse magnetoresistance and it first derivative and second derivative signals. ρ(B) is the measured transverse magnetoresistance in which slight oscillations are observed as the magnetic field is increased. dρ/dB is the first derivative of the magnetoresistance observed by detecting the fundamental frequency component by a lock-in amplifier and shows clear oscillations, but the signals are 90◦ out of phase compared to the oscillations of the magnetoresistance. On the other hand, the secondderivative signals −d2 ρ/dB 2 exhibit very clear oscillations that are in phase with the original transverse magnetoresistance. Using the magnetic field modulation technique, magnetophonon resonance has been observed for up to N = 18 ∼ 20 peaks of (7.125), and thus it has provided a very accurate determination of the effective mass. Although cyclotron resonance is well known as the most suitable method to determine the effective mass, only one peak is observed. On the other hand, magnetophonon resonance measurements will provide many peaks and thus it is possible to discuss the non-parabolicity of the conduction band in addition to the accurate determination of the effective mass. When the inverse magnetic field of the resonance peak is plotted as a function of N (Landau plot), the electron has a scalar effective mass and the plot exhibit a straight line. However, when the conduction band is nonparabolic, the Landau plot deviates from a straight line and the analysis provides information about the non-parabolicity of the conduction band. Since magnetophonon resonance is observed under the condition ωc τ > 1, the relation |σx y | > σx x is satisfied and we may approximate as σx x ρx x ∼ = 2 . σx y

(7.129)

In the explanation of the Shubnikov–de Haas effect we have shown that (7.87), σ yx ∼ = ne/B, holds in a high magnetic field. This relation is valid in the second order of scattering potential V [19]. Therefore we may conclude that the oscillatory component of magnetophonon resonance arises from the oscillatory component of σx x . As mentioned earlier, in the absence of scattering, an electron moves in the y direction with a constant velocity E/B, and thus we have no current flow in the x direction, giving rise to σx x = 0. The current component along the x direction is caused by a change in the cyclotron center induced by electron scattering, resulting in σx x = 0. This fact means that the conductivity σx x is proportional to the electron scattering rate. A detailed treatment of the magnetoconductivity will be given later, the above considerations yield the following qualitative conclusions. The electron– LO phonon scattering rate is proportional to the strength of the electron–LO phonon interaction given by (6.239) and to the excitation number of phonons, n LO + 1 for phonon emission and n LO for phonon absorption. The scattering rate for the electron– LO phonon interaction is given by the sum of the two terms, absorption and emission. For simplicity, we assume that the scattering rate is proportional to n LO . Expressing the Landau level broadening by Γ and following the treatment of the Shubnikov–de Haas effect, the oscillatory component of the magnetophonon resonance is written as (usually we may put r = 1 in the following equations)

406

7 Magnetotransport Phenomena

σx x

ωLO cos 2πr ωc

∞ 1 ωLO ωLO = cos 2πr , (7.130) exp −γr ¯ exp(ωLO /kB T ) − 1 r =1 ωc ωc ∞

Γ ∼ n LO exp −2πr ωc r =1

where γ¯ = 2πΓ /ωLO . This simplified estimate of the magnetophonon resonance amplitude is found to agree with the empirical formula of Stradling and Wood for r = 1, and the exponential decay of the oscillatory component is well explained in terms of the Landau level broadening (Γ ) at low magnetic fields. In addition, the relation explains the temperature dependence of the magnetophonon resonance amplitude. At low temperatures the broadening is small but the number of phonon excitations is low, and thus the oscillations are very weak. At high temperatures, the number of phonon excitations is high but the increase in the broadening constant Γ due to various scattering mechanisms results in an exponential decay of the magnetophonon oscillations. It may be explained also that the oscillation amplitude of magnetophonon resonance exhibits a maximum at around T = 150 K, decreasing below and above this temperature. The feature is shown in Fig. 7.7, which is obtained from magnetophonon experiments in n-GaAs. Now we discuss the theory of magnetophonon resonance. According to the Kubo formula [3, 5], the conductance σx x is given by σx x =

2π 2 l 2 q y n LO (1 + n LO ) [ f (E) − f (E + ωLO )] −∞ q ! !2 ×δ(E + ωLO − Eν )δ(E − Eν ) !ν |C(q)e−iq·r |ν! , (7.131) e2 kB T

+∞

dE

Fig. 7.7 Temperature dependence of the N = 3 magnetophonon resonance peak for several n-GaAs samples (after Stradling and Wood [4])

7.4 Magnetophonon Resonance

407

where l = (/eB)1/2 and C(q) represents the strength of the electron–LO phonon interaction defined by (6.239). Converting the summation over q into an integral and using (2.120) for the electron wave functions in a magnetic field, the above equation reduces to +∞ 1 2π e2 dq dq dE n LO (n LO + 1)(l 2 q y )2 |C(q)|2 dq σx x = x y z 3 kB T (2π) −∞ × [ f (E − ωLO ) − f (E)] δ(E − ωLO − E N , pz ) N ,M X, pz

! !2 ×δ(E − E M, pz −qz ) ! JN M (X, qx , X − l 2 q y )! ,

(7.132)

where JN M (X, qx , X − l 2 q y ) is defined by the following equation by using (2.120): N , X, pz |eiq·r |M, X , pz = JN M (X, qx , X − l 2 q y ) ×δ pz −qz , pz δ X −l 2 q y ,X .

(7.133)

In the case of a scalar electron effective mass, we find ! ! ! JN M (X, qx , X − l 2 q y )!2 = N ! ζ M−N e−ζ L M−N (ζ) 2 , N M!

(7.134)

2 2 2 where L M N (ζ) is the Laguerre polynomial and ζ = l (q x + q y )/2 [5]. The integral in (7.132) is evaluated to give [5]

σx x

1 exp −α(M ¯ − N − P − δP) = σ1 exp −2α¯ N + 2 N ,M

¯ + P − M + δ P |), ×K 0 (α|N

ωLO 3/2 ne2 α σ1 = ∗ √ n LO sinh α, ¯ m kB T πωc

(7.135a) (7.135b)

where α¯ = ωc /2kB T and α is defined by (6.240) which is a dimensionless quantity to give the strength of the electron–LO phonon interaction. δ P = ωLO /ωc − P and P is the largest integer contained in ωLO /ωc . The function K 0 (x) is the modified Bessel function of order of zero. The function K 0 (x) in (7.135b) exhibits a logarithmic divergence in the limit x → 0. Therefore, (7.135b) diverges when P = N − M and δ P = 0, or when P = M − N − 1 and δ P = 1. This divergence has been already mentioned for the case of the Shubnikov–de Haas effect and arises from the singularity of the density of states. In order to avoid this divergence for evaluation of the equation, the broadening effect of the Landau levels is taken into account and Barker has derived the oscillatory component of the magnetophonon resonance [5] written as

∞ 1 ωLO exp(−2πr Γ /ωc ) cos 2πr , (7.136) σosc ∼ r ωc r =1

408

7 Magnetotransport Phenomena

which is called Barker’s formula. When we keep the term for r = 1 only in (7.136), it gives the empirical formula of Stradling and Wood. Barker has calculated the broadening constant for various scattering mechanisms. Here we note that we have the following relation between γ, Γ and γ: ¯ 2πγ = 2π

ωLO Γ = γ¯ . ωc ωc

(7.137)

The values of γ¯ for various types of scattering are summarized below. For longitudinal optical phonon scattering γ¯ = 2π

&α 2

(1 + n LO )

'2/3 ω 2/3 c , ωLO

(7.138)

for acoustic phonon scattering γ¯ = 2π

2/3

2

2m ∗ kB T 3/2 ωc 2/3 Dac −1/2 (ω k T ) , c B 8πρvs2 2 ωLO

(7.139)

and for a single impurity, where an electron does not feel two or more impurities at the same time,

2 1/2 2/5 e4 2π 2/5 NI , (7.140) γ¯ = ωLO 4π(κ0 )2 2m ∗ where NI is the density of impurities. In a semiconductor with a higher density of impurities, an electron is scattered at the same time by two or more impurities and this phenomenon is called the band-tailing effect. For the band-tailing effect √ 3/2

1/4 2 1/4 NI πe 3/4 kB T γ¯ = (κ0 ) , ωLO 4 n

(7.141)

where n is the electron density. At the beginning of this section we mentioned that the electron effective mass is evaluated from (7.125) when we know the LO phonon energy. Since the LO phonon energy has been accurately determined from Raman scattering, magnetophonon resonance experiments provide information about effective mass, non-parabolicity, energy band parameters and so on [4, 6]. In many compound semiconductors, their conduction band minima are located at k = 0 (at the Γ point) and the effective mass is given by (2.82) as discussed in Sect. 2.4. When we use this relation, we may estimate the momentum matrix element P. A more accurate expression for the conduction band non-parabolicity is derived by Herman and Weisbuch by the following relation by taking account of contributions from higher-lying conduction bands [20], which is given by (2.239a) and (2.239b)

7.4 Magnetophonon Resonance

409

P12 2 m P02 2 1 1 + −1 = + + m∗ 3 E0 E0 + Δ0 3 E(Γ8c ) − E0 E(Γ7c ) − E0 +C, (7.142) where E0 is the energy gap between the Γ6c conduction band and the Γ8v valence band, Δ0 is the spin-orbit splitting energy of the valence bands, E(Γ8c ) and (Γ7c ) are the energies of the conduction bands located above the Γ6c conduction band, and P0 , (P1 ) is the momentum matrix element between the conduction band (higher-lying conduction band) and the valence bands. The constant C represents a contribution from the other higher-lying conduction bands and is determined to be C = 2. We have to note here that (7.142) is valid for diamond type crystals and not for III– V compound semiconductors which have no inversion symmetry, and that another consideration is required to validate the similar equation for III–V semiconductors. From the analysis of magnetophonon resonance experiments, Shantharama et al. [21] has reported that P12 and C are much smaller that the values predicted by Herman, Weisbuch [20]. Hazama et al. [22] have derived a similar expression for zinc blende crystals and evaluated P0 and P1 of (7.142) from the k · p theory for GaAs, InSb and InP, where they found that P02 = 23.55 eV and P12 = 0.13 eV for GaAs and C is −0.8, whereas for InSb and InP they obtained C = 0. These values show a good agreement with the values experimentally determined by Shantharama et al.

7.4.2 Various Types of Magnetophonon Resonance The magnetophonon resonance effect discussed above has been theoretically predicted and experimentally observed in various semiconductors, mainly at temperatures T > 77 K. In addition to this magnetophonon resonance (usually referred to as ordinal magnetophonon resonance), various types of magnetophonon resonance have been observed as discussed below.

7.4.2.1

(a) Impurity Series

At low temperatures T < 40 K a high electric field applied to a semiconductor produces hot electrons whose average energy is higher than the lattice temperature. Such a hot electron will make a transition from a Landau level to a donor state of an impurity by emitting an LO phonon, resulting in oscillatory behavior of the magnetoresistance. This oscillatory magnetoresistance is called the impurity series of magnetophonon resonance [23–25]. The resonance condition is given by N ωc + E I (B) = ωLO ,

N = 1, 2, 3, . . . ,

(7.143)

410

7 Magnetotransport Phenomena

Fig. 7.8 Magnetophonon resonance in the longitudinal magnetoresistance configuration in n-GaAs at T = 12 K, where the second derivative of the magnetoresistance is plotted as a function of magnetic field. At low electric fields, the 2TA phonon series, indicated by 3T, 4T, . . ., are observed; they are caused by a hot electron transition between Landau levels accompanied by simultaneous two transverse acoustic phonon emission. At higher electric fields, the 2TA series disappears and instead the impurity series, indicated by N , is observed which is caused by an electron transition from a Landau level to the impurity state by emitting an LO phonon. (After [25])

where E I (B) is the ionization energy of a donor in a magnetic field B. From the analysis of the impurities series, information about impurities, especially the magnetic field dependence of impurity states, has been investigated. An example of the impurity series in the longitudinal magnetoresistance configuration is shown in Fig. 7.8 [25].

7.4.2.2

(b) Two-TA-Phonon Series

In experiments on impurity series other magnetophonon resonance peaks have been often observed by changing the magnitude of the applied electric field, this series is well understood in term of the simultaneous emission of transverse acoustic (TA) phonons. This kind of magnetophonon resonance was first observed by Stradling and Wood [24] and they named it 2 TA magnetophonon series. Such TA phonons have a high density of states, sometimes at the edge of the Brillouin zone, and the transition probability of the simultaneous emission of the TA phonons is high, enabling us to observe the 2 TA series of magnetophonon. The resonance condition of the 2 TA series is given by (see [24]) Mωc = 2ωTA , here ωTA is the TA phonon energy.

M = 1, 2, 3, . . . ,

(7.144)

7.4 Magnetophonon Resonance

411

The 2 TA series is well observed in Fig. 7.8, where the second derivative of the longitudinal magnetoresistance is obtained by means of magnetic field modulation and the results for n-GaAs at T = 12 K are plotted as a function of the magnetic field. Hot electrons are produced by applying an electric field from 1.6 to 8.1 V/cm. At lower electric fields the 2 TA series indicated by 3 T, 4 T, . . . , is clearly seen. At higher electric fields, the 2 TA series disappears and the impurity series is observed. From the 2 TA series and from (7.144), the phonon energy ωTA(X) = 9.8 meV is determined and this value agrees well with the neutron scattering data, ωTA(X) = 9.7 meV [26].

7.4.2.3

(c) Inter-Valley Phonon Series

We have already shown from the energy band calculations in Chap. 1 and from the analysis of cyclotron resonance in Chap. 2 that the conduction band minima in Si and Ge are not located at the Γ point but on the Δ axes of the 100 direction and the L point in the 111 direction of Brillouin zone, respectively. Therefore, there are six equivalent valleys in Si and four equivalent valleys in Ge. As stated previously, such conduction bands are called many-valley structures. In a semiconductor with such a many-valley conduction band structure, the electrons are scattered between the equivalent valleys by absorbing or emitting phonons, which is called inter-valley phonon scattering. There are several types of phonons with specific energies involved in the inter-valley scattering, resulting in the magnetophonon resonance. We have shown in Chap. 6 that the electron mobility in Si is determined by acoustic phonon scattering at low temperatures and by inter-valley phonon scattering at higher temperatures. Magnetophonon resonance due to inter-valley phonon scattering has been reported by Portal et al. [27], Eaves et al. [28] and Hamaguchi et al. [29]. From the analysis of electron mobility in Ge, the inter-valley scattering is found to be very weak, but the magnetophonon resonance in Ge reveals very clearly the inter-valley phonon series [28, 30]. Figure 7.9 shows a typical example of magnetophonon resonance in Si at 77 K due to inter-valley phonon scattering, where the second-derivative signals obtained by the magnetic field modulation technique are plotted against the magnetic field and a clear resonance is seen. The resonance condition for magnetophonon resonance due to inter-valley phonon scattering is given by the following relation, taking into account the anisotropy of the effective mass:

1 1 ωc1 − N + ωc2 = ±ωint , M, N = 0, 1, 2, . . . , (7.145) M+ 2 2 where ωci = eB/m ci is cyclotron frequency for the effective mass m ci (in the plane perpendicular to the magnetic field) of the ith valley, and ωint is the inter-valley phonon energy. From (7.145) two different series of magnetophonon resonance are expected, which are obtained by keeping M or N constant as shown below. The resonance condition for the electron transition from a fixed Landau number N of the

412

7 Magnetotransport Phenomena

Fig. 7.9 Magnetophonon resonance due to inter-valley phonon scattering (inter-valley phonon series) in n-Si at 77 K, where the second-derivative signals of longitudinal magnetoresistance, J B100, are obtained by the magnetic field modulation technique. Several difference series are recognized in the oscillations. The series due to the fundamental magnetic field 84.7 T obtained from the Fourier transform analysis shown in Fig. 7.10 are indicated by 12–28 and the fundamental magnetic field 21.4 T by 8’–11’. Experimental data are obtained at electric fields 35 V/cm and 141 V/cm

valley (2) to Landau levels M of the valley (1) gives the resonance magnetic field BM 1 1 = (M + γ N ), (7.146) BM Bf M where

1 e = , Bf M B 1 m c1 ωint

1 m c1 1 . γN = − N + 2 2 m c2 1

=Δ

(7.147a) (7.147b)

On the other hand, for the case of a fixed Landau level M we have 1 1 = (N + γ M ), BN Bf N

(7.148)

where

1 e 1 =Δ = , Bf N B 2 m c2 ωint

1 m c2 1 . γM = − M + 2 2 m c1

(7.149a) (7.149b)

7.4 Magnetophonon Resonance

413

Fig. 7.10 Fourier transform of the data shown in Fig. 7.9. The peaks give the fundamental magnetic fields for the magnetophonon resonance and their higher harmonic components. The types and energies of the inter-valley phonons are elucidated from the fundamental field and the series scattering. The fundamental magnetic fields 84.7 T and 21.4 T give rise to the magnetophonon series 12–28 and 8’–11’, respectively, in Fig. 7.10

As stated above, inter-valley magnetophonon resonance involves two different valleys with the Landau level indices M and N , and therefore the magnetophonon resonance series are expected to arise from the inter-valley scattering in which the Landau index M or N is changed. In addition there are various kinds of inter-valley phonons; in Si, for example, f - and g-types of acoustic phonons and optical phonons are involved, resulting in many series of magnetophonon resonance and in a very complicated structure of the magnetophonon oscillations. Therefore, it is very difficult to identify the phonon types and the Landau indices from the experimental data. One of the most popular methods to analyze such complicated data is to produce about 200–400 magnetoresistance data points equally spaced with respect to the inverse magnetic field and to obtain the fundamental frequencies (fundamental magnetic fields B f M and B f N ) from the Fourier transform. As an example, the magnetophonon resonance data for n-Si in Fig. 7.9 are Fourier transformed and the Fourier spectra are shown in Fig. 7.10. From the Fourier analysis, we obtain the fundamental magnetic field B f = 21.4 and 84.7 T, and at lower electric fields peaks at 70 T and 106 T. The peak at 170 T is due to the second harmonic of the fundamental magnetic field 84.7 T. These fundamental fields are used to assign the magnetophonon resonance series as shown in Fig. 7.9. Using B f = 21.4 [T] we obtain ωiv = 13.04 [meV] for m c1 = m t and 2.53 [meV] for m c1 = m l (too small and thus no involved phonons for this), and the former energy gives g–TA phonon scattering. For B f = 84.7 [T], we find f–LA (or f–TO) phonon energy ωiv = 51.6 [meV] for m c1 = m t and g–TA phonon energy 10.0 [meV] for m c1 = m l , respectively. These value are listed in Table 6.4 of Chap. 6. Let us discuss the inter-valley magnetophonon resonance in n-Si in more detail. As stated in Sect. 6.3.7, g- and f -type inter-valley phonons are involved in the magnetophonon processes, where g-type phonons result in the inter-valley scattering between the valleys along the same principal axis, and f -type phonons are associated

414

7 Magnetotransport Phenomena

with the inter-valley scattering between the valleys whose principal axes are perpendicular. When a magnetic field is applied in the 100 direction, two different series of g-type magnetophonon resonance are expected. One is the inter-valley scattering between the valleys along the 100 valleys and the other is inter-valley scattering between the valleys in the 010 (and 001) axis whose cyclotron frequency is different from that of the 100 valleys. In g-type magnetophonon resonance, the cyclotron resonance condition reduces to (7.125) derived for magnetophonon resonance due to LO phonon scattering in GaAs. On the other hand, f -type inter-valley phonon scattering involves initial and final Landau levels whose cyclotron masses are different in the case of the transition from the 100 valley to the other valleys along the different axis. However, for a transition between the 010 and 001 valleys, the cyclotron masses of the initial and final states are the same. Therefore, f -type inter-valley magnetophonon gives rise to different series. Since the conduction band minima in Si are located at 0.85 × k100 from the Brillouin zone edge k100 on the Δ axis, the wave vector of the g-type inter-valley phonon is given by qg = 0.3 × k100 in the 100 direction. √ On the other hand, defining the band-edge wave vector along Σ by k110 (=√3/2 2 × 2π/a), the f -type inter-valley phonon wave vector is given by qf = 0.85 2 × 2π/a and thus we have qf = 0.92 × k110 . It may be possible to estimate the inter-valley phonon energy from the dispersion curves determined from neutron scattering experiments. Since the effective masses of Si are determined very accurately from the cyclotron experiments, the inter-valley phonon energies are estimated from magnetophonon resonance experiments. The analysis of magnetophonon resonance provides various types of phonon modes and their energies, and the assignment is made with the help of neutron scattering data [29]. However, the assignment is ambiguous and will not produce a definite conclusion. We have to note here that the magnetophonon resonance in n-Si has been obtained in very pure single crystals and thus the electrons are not degenerate. In such a case we may expect that the magnetophonon resonance arises from electrons in initial states with a low Landau index (0 or 1).

7.4.3 Magnetophonon Resonance Under High Electric and High Magnetic Fields The magnetophonon resonance described above is observed under low electric fields and high magnetic fields, and the magnetophonon resonance due to hot electrons is observed at low temperatures in electric fields of up to several 100 V/cm. Several attempts have been made to investigate the high electric field effect in bulk semiconductors where it is not easy to apply a high electric field. In order to overcome this difficulty Eaves et al. [31] proposed to use an n+ nn+ structure of epitaxially grown GaAs. They succeeded in observing magnetophonon resonance at high electric and high magnetic fields by applying the current in the direction perpendicular to the layers (x direction) and the magnetic field perpendicular to the current

7.4 Magnetophonon Resonance

415

Fig. 7.11 Magnetophonon resonance in an epitaxially grown n + nn+ GaAs structure for a transverse magnetoresistance configuration ( J ⊥ B), and high electric and magnetic fields (T = 300 K). The high applied electric field is achieved by a high current flow perpendicular to the epitaxial layers. At low electric fields (low current) the ordinal magnetophonon resonance is observed, whereas at higher electric fields, increasing the current, the peaks are depressed (see [31]). The effect was first explained by Eaves et al. in terms of quasi-elastic inter-Landau-level scattering, and later Mori et al. [32] explained it in terms of inelastic inter-Landau-level scattering, resulting in a double-peak structure due to inelastic LO phonon scattering

(z direction). Figure 7.11 shows the experimental results of Eaves et al., where at low electric fields (low current flow) the ordinal magnetophonon resonance due to LO phonon scattering is observed, whereas at high electric fields (high current flow) the ordinal magnetophonon resonance peaks seem to be depressed and to decay. Eaves et al. interpreted this phenomenon as showing that elastic or quasi-elastic scattering such as impurity scattering and acoustic phonon scattering dominate the transitions between the Landau levels. This process is more clearly explained with the help of Fig. 7.12 as follows. The spatial superposition of the wave functions between the adjacent Landau levels, which is small at low electric fields, increases at higher electric fields, and quasi-inelastic scattering therefore dominates the other scattering mechanisms. As a result, the ordinal magnetophonon resonance due to LO phonon scattering is weakened, causing depression of the magnetophonon peaks. This process is called QUILLS (QUasi-elastic Inter-Landau-Level Scattering). In contrast to this model, Mori et al. [32, 33] proposed the different model named IILLS (Inelastic Inter-Landau-Level Scattering) shown in Fig. 7.13. In this model, two facts are taken into account: (1) Landau levels incline in the presence of a magnetic field, and (2) current (conductivity σx x ) is induced by a change in the electron cyclotron center along the electric field by electron scattering. These two facts are shown schemat-

416

7 Magnetotransport Phenomena

Fig. 7.12 Landau levels (adjacent 3 Landau levels for fixed k z ) a at a low electric field and b at a high electric field. At a high electric field the wave functions of the two adjacent levels overlap, resulting in the increase in transition probability between the (n + 1)th and nth Landau levels at the same energy (QUILLS)

ically in Fig. 7.13, where two different resonances due to LO phonon emission or absorption appear at lower and higher magnetic fields compared to the ordinal magnetophonon resonance. The IILLS model is based on the fact that σx x is proportional to (ΔX )2 = (l 2 q y )2 according to (7.131). Therefore a vertical transition gives ΔX = 0 and will not contribute to σx x . We have described theory of magnetophonon resonance due to LO phonon scattering and the theory of Barker given by (7.131), which is derived from the Kubo formula. Here we will consider the IILLS theory based on the magnetophonon theory. As is well known, the Kubo formula is a kind of linear response theory and the following calculations of σx x are assumed to be approximated by a linear theory although the Landau levels are changed by the application of an electric field. Equation (7.131) is rewritten as σx x =

e2 β 2 2 em ab l q y ) (Pi→ f + Pi→ f , 2 i f q

(7.150)

where β = 1/kB T , the second terms on the right-hand side are respectively the probabilities of LO phonon emission and absorption, and i and f represent the initial and final electronic states, respectively. The rates of LO phonon emission and absorption are written as

7.4 Magnetophonon Resonance

417

Fig. 7.13 In-elastic inter-Landau-level scattering (IILLS), where three adjacent Landau levels for fixed k z and classical Landau orbits (N = 0, 1, 2) are shown. a At low electric fields, a vertical transition will not contribute to σx x . b At a high electric field, a non-vertical transition (i) the high magnetic field side and (ii) the low magnetic field side satisfies the magnetophonon resonance condition, resulting in a double-peak structure. In the figure the separation between the Landau levels of N = 0 and N = 2 is equal to the LO phonon energy ω0

!" #!2 2π (n LO + 1) ! f |C ∗ (q)e−iq·r |i ! × f (Ei ) [1 − f (Ei − ωLO )] δ[E f − (Ei − ωLO ], !" #!2 2π n LO ! f |C(q)eiq·r |i ! = × f (Ei ) [1 − f (Ei + ωLO )] δ[E f − (Ei + ωLO )],

em Pi→ f =

ab Pi→ f

(7.151)

(7.152)

where n LO is the Bose–Einstein distribution function of the LO phonons and f (E) is the Fermi–Dirac distribution function of the electrons, which is approximated by the Maxwell–Boltzmann distribution function in the types of semiconductor we are concerned with. Ei and E f are the electron energies of the initial and final states. The two terms of the above equation contribute to σx x in a similar way and we take into account the absorption term only for simplicity. In the presence of an electric field (E x) and magnetic field (B z), and defining the vector potential by A = B(0, x, 0), the Hamiltonian is written as H=

1 ( p + e A)2 + ex E. 2m ∗

(7.153)

418

7 Magnetotransport Phenomena

The eigenfunctions and eigenvalues for the Hamiltonian are given by ψn = exp(ik y y) exp(ik z z)φn (x − X ),

2 k z2 1 1 ∗ E 2 Eν = n + ω0 + + eE X ν + m , 2 2m ∗ 2 B

(7.154) (7.155)

where φn (x) is the solutions for a simple harmonic oscillator and n = 0, 1, 2, . . . . In the y direction the cyclic boundary condition is satisfied and k y = 0, ±2π/L, ±4π/L, . . . , and k z is the electron wave vector in the direction parallel to the electric field. The center coordinate of the cyclotron motion X ν is given by

E 2 , X = − lB ky + ωc B

(7.156)

and L is the sample length in the y direction. Considering these results and following the treatment of Barker [5] to derive magnetophonon resonance theory, we obtain the following relations (see Mori et al. [32]): σosc

√

3 ( exp(−2πr γ) cos 2πr ω¯ 0 + e¯ ω¯ 0 + 1 ∼ r 2 r =1 √

3 ( e¯ ω¯ 0 + 1 , + cos 2πr ω¯ 0 − 2 ∞ 1

(7.157)

where √ 2eEl B e¯ = , ωc ω0 ω¯ 0 = ωc

(7.158)

and in the limit of low electric field e¯ = 0, which gives rise to Barker’s formula (7.136). In addition, from (7.157) the resonance condition is given by √ ω¯ 0 ±

3 ( e¯ ω¯ 0 + 1 = N , 2

(7.159)

and thus the resonance magnetic field is given by B N±

B0 ± ∼ N

)

3 m∗ E. 2 el0 B0

(7.160)

Here, B0 /N = B N is the resonance magnetic field for ordinal magnetophonon resonance at low electric fields. At high fields, it is seen from (7.157) and (7.160) that the electric field-induced magnetophonon resonance due to inelastic LO phonon

7.4 Magnetophonon Resonance

419

Fig. 7.14 Electric field-dependence of the resonance peaks for electric field-induced magnetophonon resonance due to inelastic inter-Landau-level scattering (IILLS), where the experimental results of Eaves et al. [31] are compared with the theoretical calculations (solid curves). The peak splitting is near the N = 2 ordinal magnetophonon resonance

scattering appears at both sides of the ordinal low electric field magnetophonon resonance peak. The oscillatory magnetoconductance σosc in GaAs in the IILLS model is calculated from (7.157) for electric fields of 0–3.5 kV/cm, and the second derivative of the magnetoconductance with respect to the magnetic field B is plotted in Fig. 7.14 in the magnetic field region near the N = 2 ordinal magnetophonon resonance. We find in Fig. 7.14 that the low electric magnetophonon peak at 11 T splits into two peaks on the lower and higher magnetic field sides of the ordinal magnetophonon peak as shown by the arrows. Figure 7.15 shows a plot of the peak positions as a function of the magnetic field, where the experimental data points are compared with the theoretical calculation (solid curves) and a good agreement is seen. We have to note here that the QUILLS model is disproved by these considerations and that the IILLS model is based on the linear theory and its validity has not yet been confirmed. In addition the IILLS model is derived by taking only LO phonon absorption into account and the contribution of LO phonon emission is not considered. Taking account of these factors, Wakahara and Ando [34] adopted a more elaborate theory to understand the magnetophonon resonance at high electric and high magnetic fields, and found that the most important mechanism for the peak splitting is due to the IILLS process.

7.4.4 Polaron Effect In magnetophonon resonance the electrons and phonons are strongly coupled, the electrons being coupled strongly with the phonons by emitting or absorbing LO phonons. Under such conditions an electron is thought of as moving with phonon cloud around it and such a state is called a polaron. Once a polaron is formed, the

420

7 Magnetotransport Phenomena

Fig. 7.15 Calculated result of electric-field induced magnetophonon resonance due to inelastic inter-Landau-level scattering (IILLS), where the second derivative of the oscillatory magnetoconductivity ∂ 2 σosc /∂ B 2 in GaAs is plotted as a function of magnetic field B near the N = 2 resonance. The peak of 11 T due to ordinal magnetophonon resonance due to LO phonon scattering at zero electric field splits into two peaks with increasing electric field

electron moves with the phonons and thus the band-edge effective mass is increased. This feature is explained with the help of the diagrams shown in Fig. 7.16. In general, electron-phonon interaction is represented by two processes shown in Fig. 7.16, where (a) is the process where an electron of state |k emits a phonon of wave vector q and is transferred to a state |k − q and (b) is the process where an electron of |k − q absorbs a phonon of wave vector q and is transferred to a state |k. These two processes are independent. On the other hand, in a system where electrons are strongly coupled with phonons, an electron of |k emits a phonon of wave vector q and subsequently absorbs the phonon and returns to the initial state |k. This is a kind of composite state, the polaron state, as shown in Fig. 7.16c. It is evident from Fig. 7.16c that the polaron state is calculated by second-order perturbation theory. In the following analysis we assume the very simplified case of a conduction band represented by a parabolic approximation with scalar effective mass; we also assume T = 0 and B = 0. The Hamiltonian of electron–phonon system under interaction is written as (7.161) H = H0 + H , where H0 is the Hamiltonian for a non-interacting electron and phonon and is given by

p2 1 † . (7.162) a + ω a + H0 = LO q q 2m ∗ 2 q

7.4 Magnetophonon Resonance

421

Fig. 7.16 Diagrams for the electron–LO phonon interaction. a An electron |k emits a phonon of wave vector q and is scattered to a state |k − q. b an electron |k − q absorbs a phonon of wave vector q and is scattered to a state |k. c When the electron–phonon interaction is strong, an electron |k subsequently emits and absorbs a phonon of wave vector q, and returns to the initial state |k. This is a kind of composite state and the electron moves accompanied by the phonon cloud, and a polaron state is formed

The term H is the Hamiltonian for the electron–phonon interaction and for the Fröhlich-type interaction it may be written as H =

Vq aq eiq·r + aq† e−iq·r ,

(7.163)

q

where the term Vq is expressed by using (6.239) and (6.240) as 1/4

iωLO (4πα)1/2 , q 2m ∗ ωLO

1/2 1 m∗ e2 1 α= − . 0 κ∞ κ0 2ωLO

Vq =

(7.164) (7.165)

The eigenstate for H0 is specified by the electron wave vector k and the phonon number n q of phonon wave vector q and is expressed as |k, n q , and its eigenenergy is given by

2 k 2 1 n . (7.166) + ω + E(k, n q ) = LO q 2m ∗ 2 q Since we are concerned with a state at T = 0, the phonon system is in the vacuum state and the eigenstate for the unperturbed system is given by |k, 0. Then the perturbing energy is obtained as ΔE = k, 0|H |k, 0 k, 0|H |k , n q k , n q |H |k, 0 + . E(k, 0) − E(k , n q )

(7.167)

n q =0,k

It is apparent that the second term on the right-hand side of the above equation corresponds to the diagram shown in Fig. 7.16c. The first-order perturbation given

422

7 Magnetotransport Phenomena

by the first term on the right-hand side becomes zero because H contains the creation and annihilation operators of the phonon. The second term on the right-hand side of (7.167) vanishes except for the term for n q = 1, and the matrix element of the numerator reduces to k , 1q |H |k, 0 = Vq δ(k − k − q), k, 0|H |k , 1q = Vq δ(−k + k + q),

(7.168) (7.169)

where (7.168) and (7.169) represent phonon emission and absorption, respectively, and correspond to the diagram of Fig. 7.16c. From the δ-function we obtain the electron wave vector of the virtual state, k = k − q. The energies of the initial and final states are E(k, 0) = E(k) =

2 k 2 , 2m ∗

(7.170)

and the energy of the intermediate state |k − q, where a single phonon of q is excited, is given by E(k , n q ) = E(k − q, 1q ) =

2 (k − q)2 + ωLO . 2m ∗

(7.171)

Inserting these results into (7.167) we obtain the following relation: ΔE(k) =

q

|Vq |2 . E(k) − E(k − q) − ωLO

(7.172)

Converting the summation over k into a summation over q with the use of the momentum conservation * 3 rule and the summation into an integral by using the relation $ 3 3 q = (L /8π ) d q, the following result is obtained: 1 d3 q αωLO u · 2π 2 k 2 − (k − q)2 − u 2 q 2 q 2 ∞ 2kq − q 2 − u 2 1 αωLO u log dq. = 2πk q 2kq + q 2 + u 2 0

ΔE(k) =

(7.173)

The derivation of this equation may be done by following the treatment given by √ (6.296)–(6.299) shown in Sect. 6.3.10. Here, u = 2m ∗ ωLO / and the upper limit of the integral is set to qmax → ∞. When the integration is carried out, we obtain1

1 In order to carry out the integration, we assume that the term to be integrated is a function of k and q. We then differentiate it with respect to k and integrate the result with respect to q, and then integrate it with respect to k.

7.5 Problems

423

ΔE(k) = −αωLO

sin−1 (k/u) . k/u

(7.174)

Putting u = k, we have 2 k 2 /2 m ∗ = ωLO . In the region where the electron energy is less than the LO phonon energy, k < u, we may use the asymptotic form sin−1 x = x + 16 x 3 + · · · , and so the electron energy is approximated as E=

α 2 k 2 2 k 2 + O(k 4 ). 1 − + ΔE = −αω + LO 2m ∗ 2m ∗ 6

(7.175)

Such an energy in which the perturbation energy is included in the electron energy is called the self-energy of the polaron. The effective mass of the polaron, m ∗pol is then given by m∗ , (7.176) m ∗pol = 1 − α/6 or it may be expressed as

α ∗ m ∗pol = 1 + m . 6

(7.177)

The effective mass observed by magnetophonon resonance is affected by the polaron effect and thus the band edge effective mass should be corrected by (7.177). In addition (7.175) shows that the polaron state is lower than the bottom of the conduction band by αωLO and that the polaron can be excited by incident light with photon energy lower than the band gap.

7.5 Problems (7.1)

In order to understand Hall effect, analyze Hall measurement carried out using a device shown in Fig. 7.17. The dimensions of the sample are thickness t = 1 mm, width w = 4 mm, and length l = 10 mm. When magnetic field Bz = 0.4 T and current Ix = 1.0 mA are applied, Hall voltage VH = 1.0 mV. Hall field is E y < 0. Observed voltage difference Vx between the voltage probes (distance l x ) is 25 mV without the magnetic field. Answer the following questions: (1) Which is the type of carriers, electrons (n–type) or holes (p–type)? (2) Calculate the density of the carriers. (3) Calculate the conductivity σ of this sample. (4) Calculate Hall mobility μH of the carriers.

(7.2)

Derive equation (7.51c) for a parabolic band band with isotropic effective mass.

424

7 Magnetotransport Phenomena

Fig. 7.17 Schematic illustration of Hall effect measurement for a typical sample. Application of magnetic field Bz and current flow I x , produces Hall voltage VH

(7.3)

Derive equation (7.51c) for a parabolic band band with isotropic effective mass..

(7.4)

Shubnikov–de Haas oscillations appear periodically with respect to the applied magnetic field B. Consider a material with electron density n = 2 × 1018 [cm−3 ] and assume the electrons with effective mass m ∗ = 0.0135m (for InSb) are degenerate. (1) Calculate Fermi energy EF of this material. (2) Calculate the period of the Shubnikov–de Haas oscillations (1/B). (3) Calculate EF and (1/B) for GaSb shown in Fig. 7.4, where the electron effective mass at the Γ point is known m ∗ = 0.039

(7.5)

Calculate oscillatory term for r = 1 of magnetophonon resonance given by (7.136) and plot it as a function of magnetic field. Use the parameters 2πr Γ /ωc = 0.5ωLO /ωc , m ∗ = 0.067m, ωLO = 35.4 [meV] (for GaAs).

(7.6)

Estimate polaron masses in GaAs and InAs using material parameters in Table 6.3 and describe the effective mass correction.

References 1. K. Seeger, Semiconductor Physics (Springer, New York, 1973) 2. L.M. Roth, P.N. Argyres, in Semiconductors and Semimetals, vol. 1, ed. by R.K. Willardson, A.C. Beer (Academic, New York, 1966), pp. 159–202 3. R. Kubo, S.J. Miyake, N. Hashitsume, in Solid State Physics, vol. 17, ed. by F. Seitz, D. Turnbull (Academic, New York, 1965), p. 279 4. R.A. Stradling, R.A. Wood, J. Phys. C 1, 1711 (1968) 5. J.R. Barker, J. Phys. C Solid State Phys. 5, 1657 (1972) 6. P.G. Harper, J.W. Hodby, R.A. Stradling, Rep. Prog. Phys. 36(1), 1 (1973) 7. R.V. Parfenev, G.I. Kharus, I.M. Tsidilkovskii, S.S. Shalyt, Sov. Phys.-USP 17, 1 (1974) 8. R.L. Peterson, in Semiconductors and Semimetals, vol. 10, ed. by R.K. Willardson, A.C. Beer (Academic, New York, 1975), p. 221 9. R.J. Nicholas, Prog. Quantum Electron. 10, 1 (1985) 10. C. Hamaguchi, N. Mori, Physica B 164, 85 (1990) 11. P.N. Argyres, Phys. Rev. 117, 315 (1960) 12. R. Kubo, H. Hasegawa, N. Hashitsume, J. Phys. Soc. Jpn. 14, 56 (1959) 13. P.P. Debye, E.M. Conwell, Phys. Rev. 93, 693 (1954)

References

425

14. W.M. Becker, H.Y. Fan, in Proceeding of the 7th International Conference on the Physics of Semiconductors, Paris, 1964 (Dumond, Paris and Academic, New York, 1964), p. 663 15. V.L. Gurevich, Y.A. Firsov, Zh. Eksp. Teor. Fiz. 40, 198 (1961) [Sov. Phys.-JETP 13, 137 (1961)] 16. S.M. Puri, T.H. Geballe, Bull. Amer. Phys. Soc. 8, 309 (1963) 17. Y.A. Firsov, V.L. Gurevich, R.V. Pareen’ef, S.S. Shalyt, Phys. Rev. Lett. 12, 660 (1964) 18. H. Hazama, T. Sugimasa, T. Imachi, C. Hamaguchi, J. Phys. Soc. Jpn 54, 3488 (1985) 19. P.N. Argyres, L.M. Roth, J. Phys. Chem. Solids 12, 89 (1959) 20. C. Herman, C. Weisbuch, Phys. Rev. B 15, 823 (1977) 21. L.G. Shantharama, A.R. Adams, C.N. Ahmad, R.J. Nicholas, J. Phys. C 17, 4429 (1984) 22. H. Hazama, T. Sugimasa, T. Imachi, C. Hamaguchi, J. Phys. Soc. Jpn. 55, 1282 (1986) 23. R.A. Stradling, R.A. Wood, Solid State Commun. 6, 701 (1968) 24. R.A. Stradling, R.A. Wood, J. Phys. C 3, 2425 (1970) 25. C. Hamaguchi, K. Shimomae, Y. Hirose, Jpn. J. Appl. Phys. 21(Suppl. 21–3), 92 (1982) 26. J.L.T. Waugh, G. Dolling, Phys. Rev. 132, 2410 (1963) 27. J.C. Portal, L. Eaves, S. Askenazy, R.A. Stradling, Solid State Commun. 14, 1241 (1974) 28. L. Eaves, R.A. Hoult, R.A. Stradling, R.J. Tidey, J.C. Portal, S. Skenazy, J. Phys. C 8, 1034 (1975) 29. C. Hamaguchi, Y. Hirose, K. Shimomae, Jpn. J. Appl. Phys. 22(Suppl. 22–3), 190 (1983) 30. Y. Hirose, T. Tsukahara, C. Hamaguchi, J. Phys. Soc. Jpn. 52, 4291 (1983) 31. L. Eaves, P.P. Guimaraes, F.W. Sheard, J.C. Portal, G. Hill, J. Phys. C 17, 6177 (1984) 32. N. Mori, N. Nakamura, K. Taniguchi, C. Hamaguchi, Semicond. Sci. Technol. 2, 542 (1987) 33. N. Mori, N. Nakamura, K. Taniguchi, C. Hamaguchi, J. Phys. Soc. Jpn. 57, 205 (1988) 34. S. Wakahara, T. Ando, J. Phys. Soc. Jpn. 61, 1257 (1992)

Chapter 8

Quantum Structures 1

Abstract In this chapter and the following Chap. 9 we deal with semiconductor quantum structures. First, two–dimensional electron gas (2DEG) in MOSFET and single heterostructure (High Electron Mobility Transistor: HEMT) are discussed by solving Schrödinger equation, and then transport properties are described by evaluating scattering rate and mobility. Mesoscopic phenomena observed in a semiconductor structure of the scale in between micro– and macro–structure is discussed by Landauer and Landauer Büttiker formulas. Aharonov–Bohm effect and ballistic transport are also discussed. Quantum Hall effect has attracted many scientists from the reasons due to the development in new physics of semiconductors in addition to the resistance standard, von Klitzing constant. Integral and fractional quantum Hall effects are discussed in different models. In Chap. 9 we deal with superlattices and quantum dots.

8.1 Historical Background The words “quantum structures” or “quantum effect devices” have been cited very often since the 1980s [1–12]. Early work on the quantization of electrons was initiated in the 1960s, when electrons in the inversion layer of the MOSFET (MetalOxide-Semiconductor Field Effect Transistor) [13] were found to be quantized at the interface and to exhibit two-dimensional properties. Historical review of the early work is well described by Ando, Fowler and Stern [1]. Then the Quantum Hall effect was discovered in 1980 by van Klitzing et al. [14] by using a Si-MOSFET and thereafter the transport properties of a two-dimensional electron gas has received a great deal of attention. Another attempt to fabricate quantum structures, which has led to the most important applications in semiconductor physics and devices, was initiated in 1960 by Esaki and Tsu [15], who introduced the molecular beam epitaxial (MBE) technology to grow layered structures, named superlattices, and succeeded in observing Bloch oscillations. Since then MBE growth techniques have been used by many people to tailor various types of quantum structure and the electron transport and optical properties arising from the quantization effect have been observed. For example, the © The Author(s), under exclusive license to Springer Nature Switzerland AG 2023 C. Hamaguchi, Basic Semiconductor Physics, Graduate Texts in Physics, https://doi.org/10.1007/978-3-031-25511-3_8

427

428

8 Quantum Structures 1

two-dimensional transport, the quasi-one-dimensional structure (quantum wire), the zero-dimensional structure (quantum dot), and superlattices have been extensively investigated. This research is still in progress and it is very difficult for the author to review them by the two chapters of the present textbook. Therefore, in this textbook we will deal with several important phenomena of quantum structures and introduce the basic physics which is required for readers who want to investigate in more detail. It is best to understand the physics of the two-dimensional electron gas in the MOSFET first and then to investigate the physics of the quantum effects of heterostructures. Therefore, we will study the two-dimensional electron gas in the MOSFET in detail and then look at several important quantum effects in heterostructures. Readers who are interested in more detail are recommended to read the references.

8.2 Two-Dimensional Electron Gas Systems 8.2.1 Two-Dimensional Electron Gas in MOS Inversion Layer The two-dimensional characteristics of electrons were first observed in MOSFETs and various properties of quantum effects have been investigated in MOSFETs. It is best to study the two-dimensional properties of electrons in the MOSFET for a detailed understanding of the quantum effects in quantum structures fabricated from heterostructures. Therefore in this section we will deal with the two-dimensional electron gas in the MOFSFET. The structure of the MOSFET is shown in Fig. 8.1, and consists of an insulating SiO2 film, a metal gate, a source and a drain formed on a p-Si substrate. The gate electrode controls the electron density in the inversion layer (channel) induced below

Fig. 8.1 Structure of MOS field effect transistor (MOSFET). The MOSFET is fabricated on a p-Si substrate, with a SiO2 thin film (insulating film) on the p-Si and a metal gate electrode on the SiO2 . The source and drain electrodes are formed by diffusing p-Si n+ impurities into the p-Si substrate and then putting metal contacts on the diffused surfaces. Application of a positive voltage bias to the gate electrode induces an n-channel of electrons under the gate electrode, resulting in electron current flow between the source and the drain

8.2 Two-Dimensional Electron Gas Systems

429

Fig. 8.2 Energy diagram of the MOSFET of Fig. 8.1. It is shown for a positive gate bias, where an inversion layer of electrons is formed near the surface of the p-Si at the interface between the semiconductor (p-Si) and the insulator (SiO2 ). The induced electrons are confined in a narrow region at the interface and move only parallel to the interface, exhibiting two-dimensional characteristics. In the region near the interface of the p-Si substrate, the bands bend and holes are depleted leaving ionized acceptors in the region from the surface to z d . Charge neutrality is achieved by holes and acceptors in the region beyond the depletion layer

the insulating SiO2 film by applying a bias, and it thus controls the current flow through the channel. The FET characteristics are similar to those of a triode vacuum tube, which are well described in the textbook of Sze [13]. The energy diagram for the device is shown in Fig. 8.2 for a positive bias applied to the gate electrode. The application of the gate bias lowers the energy of the gate electrode and bends the energy of the semiconductor surface at the interface between the semiconductor and the insulating layer. As a result electrons are induced at the interface of the p-Si, and the layer (or channel) of the electrons is called the inversion layer. The valence band is also bent so that the valence band is filled by electrons, depleting holes in this region, and negatively charged acceptors are left. This layer is therefore called the depletion layer, which is indicated by the depth z d . Beyond the depletion layer (z d ≤ z ≤ ∞) charge neutrality is preserved by the holes and ionized acceptors, where the Fermi energy is given by the bulk Fermi energy E F . The electrons in the inversion layer confined at the interface are quantized in the z direction and can move only in the direction x and y (parallel to the interface). From this the electrons in the inversion layer form a two-dimensional state and are called a two-dimensional electron gas.

8.2.1.1

Triangular Potential Approximation

It is seen in Fig. 8.2 that electrons in the inversion layer are confined within a narrow region of the interface and that the confining potential looks like a triangular potential. Let the electric field at the interface be E s and the direction of the confinement be z. The confining potential is then approximated as

430

8 Quantum Structures 1

φ(z) = −E s z .

(8.1)

Assuming that the ionized acceptors NA and donors ND (NA ND ) are distributed uniformly along the direction of z from the interface to the position z d , the potential distribution is obtained by solving Poisson’s equation: φd (z) =

e(NA − ND ) 2 z , 2κs 0

(8.2)

where κs is the dielectric constant of Si. Analysis of the potential distribution in this section is carried out by neglecting the contribution of the charge in the depletion region and by taking the contribution of the electrons themselves. The electrons are confined in the z direction and are mobile only in the x, y plane. Letting the area of the x, y plane be A and writing the wave function of an electron in the inversion layer as (8.3) ψ(x, y, z) = A−1/2 exp(ik x x + ik y y)ζi (z) , The Schrödinger equation in the z direction reduces to −

2 d 2 ζi (z) − eφ(z)ζi (z) = Ei ζi (z) , 2m 3 dz 2

(8.4)

where m 3 is the electron effective mass in the z direction. Inserting the triangular potential given by (8.1) into the potential energy of (8.4), we obtain the following relation: 2m 3 eE s Ei d2 ζ (z) + − z ζi (z) = 0 . (8.5) i dz 2 2 eE s We have to note here that (8.5) is exactly the same as (5.3a) used to describe the Franz–Keldysh effect in Sect. 5.1.2. Defining z = (8.5) reduces to

2m 3 eE s 2

1/3 z−

Ei eE s

,

d2 ζi (z ) − z ζi (z ) = 0 . dz 2

(8.6)

(8.7)

The solution of this equation is given by the Airy function as described in Sect. 5.1.2, and is written as (8.8) ζi (z ) = Ci · Ai(z ) . This is rewritten as ζi (z) = Ci · Ai [2m 3 eE s /2 ]1/3 [z − Ei /eE s ] .

(8.9)

8.2 Two-Dimensional Electron Gas Systems

431

The constant Ci is determined by the normalization condition of (8.9) and given by1 2m 3 eE s 1/6 1 1 Ci = √ = 2 Ai (xi ) λAi (xi )

(8.10)

The potential barrier at the interface of the insulating SiO2 film and the p-Si surface is very high and may be approximated an infinite barrier height, enabling us to put ζ (z = 0) = 0. This assumption gives rise to the solution (see [16]) Ei ≈

2 2m 3

1/3

3 3 2/3 . π eE s i + 2 4

(8.11)

This solution gives a good approximation for a large value of i, and also a reasonably good result for small i. For i = 0, for example, the solution is obtained by putting i + 3/4 = 0.75, whereas the exact solution is given by inserting 0.7587. The other approximate solutions are closer to the exact solutions. It is concluded from the above results that the energy levels of a confined electron in the z direction are given by discrete values due to the quantization. Adding the electron energies of the x and y directions, the total energy of the electron, in the two-dimensional electron gas, is given by 2 k 2y 2 k x2 + . (8.12) E = Ei + 2m 1 2m 2 Next we will discuss the density of states for a two-dimensional electron gas and the potential acting on the electrons. The density of states for a two-dimensional electron gas is derived as follows. When the cyclic boundary condition is introduced

1

The normalization constant (5.8) is evaluated by integrating the squared wave function in the whole region, −∞ ∼ +∞, whereas the normalization in MOSFET should be carried out in the region 0 < z < ∞. Introducing variables, λ = [2m 3 eE s /2 ]−1/3 and xi = −E /(λeE s ), where xi is i–th solution of Ai(xi ) = 0, (i = 0, 1, 2, . . .). Then (8.9) is rewritten as z ζi (z) = Ci · Ai + xi . λ Normalization of the wave function (8.9) in the region 0 < z < ∞ is given by

∞

∞ z 1= |ζi (z)|2 dz = Ci2 Ai2 + z i dz λ 0 0 Here we change the variable as x = z/λ, and then

∞

1 = Ci2 λ Ai2 (x + xi )dx = Ci2 λ 0

∞

Ai2 (x)dx

xi

∞ = Ci2 λ{Ai (xi )}2 . = Ci2 λ −{Ai (x)}2 + xAi2 (x) xi

From this we find the normalization constant Ci given by (8.10).

432

8 Quantum Structures 1

to a semiconductor of the volume L 3 , the number of states in the region between (k x , k y ) and (k x + dk x , k y + dk y ) is given by 2L 2 dk x dk y . (2π )2 Therefore, the density of states per unit area is given by 2 dk x dk y , (2π )2

(8.13)

where the factor 2 in the above √ equation arises from √the spin degeneracy. When we convert the variables by k x / m 1 /m = k x and k y / m 2 /m = k y , (8.12) is reduced to 2 2 2 2 E = Ei + (k x + k 2 k . y ) = Ei + 2m 2m √ Taking account of the relations, dk x dk y = ( m 1 m 2 /m)dk x dk y and 2π k dk = π d(k 2 ) = π(2m/2 )d(E − Ei ), the following relation is obtained: 2 2 md md 2π k dk = dk x dk y = d(E − Ei ) , 2 2 (2π ) (2π ) m π 2

(8.14)

√ where the density-of-states mass defined by m d = m 1 m 2 is used. This relation gives the density of states for a two-dimensional electron gas, which is shown schematically in Fig. 8.3. As shown in Fig. 8.3, the three-dimensional density of states is expressed by a parabolic curve (dashed curve) but the two-dimensional density-of-states curve

Fig. 8.3 Density of states (solid curve) for a two-dimensional electron gas is shown by the solid curve, a combination of step functions. The step function is called a subband. The energy of the 2 bottom of the subband is given by Ei and each subband has the step √ m d /π . The density of states for three-dimensional electrons (dashed curve) is proportional to E and thus given by a parabolic curve. In the limit of narrow subband spacing, the two-dimensional density of states approaches the three-dimensional density of states

8.2 Two-Dimensional Electron Gas Systems

433

(solid curve) is given by step functions. Each step function is called a subband and Ei is the energy of the bottom of the subband and is called the subband energy. As shown in Fig. 2.8, the conduction bands of Si consist of six equivalent valleys, and thus the density of states should be calculated by taking account of the valley degeneracy n v . For example, in the Si-MOSFET, where the insulating SiO2 is grown on the (001) surface of Si, we obtain two different series of subbands which are the two equivalent valleys with their principal axis in the direction perpendicular to the interface and four equivalent valleys with the valley axes parallel to the interface; their effective masses in the quantization directions are, respectively, m 3 = m l (n v = 2) and m 3 = m t (n v = 4). Letting the valley degeneracy be n vi for the subband series Ei , the density of states for a two-dimensional electron gas is written as i J2D (E)d(E − Ei ) =

n vi m di d(E − Ei ) . π 2

(8.15)

Since electrons obey Fermi–Dirac statistics, the sheet density of the two-dimensional electron gas Ni of the subband E i is calculated as

Ni =

∞ Ei

=

i J2D (E)

1 dE , exp [(E − EF )/kB T ] + 1

n vi m di kB T F0 [(EF − Ei )/kB T ] , π 2 F0 (x) = log(1 + ex ) ,

(8.16) (8.17)

where EF is the Fermi energy. Then the sheet density of electrons in the inversion layer Ninv is given by

Ninv = Ni . (8.18) i

Since the charge density in the depletion layer is given by ρdepl (z) =

−e(NA − ND ), 0 < z ≤ z d 0,

z > zd

(8.19)

the corresponding sheet density of the ionized impurities in the depletion layer Ndepl is defined by (8.20) Ndepl = (NA − ND )z d , and the depth of the depletion layer z d is estimated from the curvature of the potential φd in (8.2) [17]. As seen in Fig. 8.2, the potential curvature is given by the following relation assuming the energy at z → ∞ (the bulk region of the semiconductor) as (Ec − EF )bulk and neglecting the contribution from the inversion electrons. At T = 0 and at zero bias between the source and drain, the potential curvature is determined as

434

8 Quantum Structures 1

φd = (Ec − EF )bulk + EF −

eNinv z av , κ s 0

(8.21)

where EF is the Fermi energy measured from the bottom of the conduction band at the Si–SiO2 interface, and the following parameters are used z av =

zi =

i Ni z i , Ninv

(8.22)

z|ζi (z)|2 dz

|ζi (z)|2 dz .

(8.23)

The electric field at the Si surface is determined by the total sheet density of the charges. When we define it by −E s , it is given by Es =

e(Ninv + Ndepl ) , κ s 0

(8.24)

where Ndepl = z d (NA − ND ). The potential distribution φ(z) is determined by Poisson’s equation

1 d2 φ(z) 2 ρdepl (z) − e =− Ni ζi (z) . (8.25) dz 2 κ s 0 i 8.2.1.2

Solutions by the Variational Method

More accurate solutions may be obtained by using the variational principle. The variational principle is based on the assumption of a trial wave function and on determination of the wave function to minimize the energy. The most popular trial function is the Fang–Howard function [18] ζ0 (z) for the ground state given by the following equation, where ζ (z = 0) = 0 at z = 0 and ζ (z = ∞) = 0 at z → ∞: ζ0 (z) =

1 3 −bz/2 b ze . 2

(8.26)

This assumption gives a good result when the electron density in the inversion layer is low and the electrons occupy the lowest subband. The variational parameter b of the trial function is determined to minimize the subband energy. Inserting (8.26) into the one-dimensional Schrödinger Equation (8.4), the expectation value of the energy is evaluated as 2 b 2 3e2 11 2 Ndepl + Ninv − (NA − ND ) . + (8.27) E0 = 8m 3 κ s 0 b 16 b Various parameters are determined to minimize the energy E0 and are given below:

8.2 Two-Dimensional Electron Gas Systems

12m 3 e2 N ∗ 1/3 b0 = , κ s 0 2 9κs 0 2 1/3 z0 = , 4m 3 e2 N ∗ 2/3 5/3 e2 1 3 55 E0 = Ndepl + , Ninv 1/2 ∗1/3 2 96 N m 3 κ s 0

435

(8.28a) (8.28b) (8.28c)

11 where N ∗ = Ndepl + 32 Ninv . It has been shown by Stern [17] that the subband energy E0 in Si calculated by this method shows good agreement with the result of selfconsistent calculations.

8.2.1.3

Solutions by the Self-Consistent Method

The Schrödinger equation, Poisson’s equation and the electron sheet density are written as 2 d2 + [E − eφ(z)] ζi (z) = 0 , (8.29) − i 2m 3 dz 2

1 d2 φ(z) 2 =− Ni |ζi (z)| , ρdepl − e (8.30) dz 2 κ s 0 i n v m d kB T E F − Ei . (8.31) Ni = log 1 + exp π 2 kB T The simultaneous equations may be solved self-consistently by using numerical analysis as follows. Let the Si/SiO2 interface be at the origin z = 0, and choose a distance z = L where the wave function converges (for example, 20 nm). The region [0, L] is discretized into 200 meshes and we define h = L/200. The following calculations are usually solved by introducing dimensionless values for energy and distance. Here we show how to solve by the difference method. Differentiation of a function f (z) is expressed as f ( j+1) − f ( j) df → , dz h f ( j+1) − 2 f ( j) + f ( j−1) d2 f → . 2 dz h2

(8.32) (8.33)

The Schrödinger equation (8.29) and Poisson’s equation (8.30) are then expressed as 200 × 200 matrix equations. Since both equations are second-order differential equations, the corresponding matrices have diagonal elements and adjacent components, or in other words the matrices are tridiagonal, and thus the solutions are easily obtained by diagonalization. From those procedures we obtain 200 eigenvalues and

436

8 Quantum Structures 1

200 eigenfunctions from the Schrödinger equation because we have discretized the equation into 200 meshes. Therefore, this difference method gives the solutions of the Schrödinger equation with the accuracy of the 200 mesh discretization. This procedure provides smooth solutions for lower eigenstates.2 On the other hand, Poisson’s equation is solved easily by the iteration method when the initial value E s is known. Another method to solve Poisson’s equation is to diagonalize the tridiagonal matrix using the values at z = 0 and z = L. The simultaneous equations, (8.29) and (8.30), contain the wave function ζi (z) and potential φ(z) and they are not independent. Here we will show a method to obtain self-consistent solutions for the simultaneous equations. 1. Determine the surface of Si. In the case of the (001) surface of Si, we have to solve two Schrödinger equations for m 3 = m l , n v = 2 and m 3 = m t , n v = 4. 2. Determine the initial values of Ninv and NA − ND . 3. The total sheet electron density Ninv is assumed to occupy the ground state subband E0 , and parameters such as z av , z d , φd , Ndepl , and Es are determined using the Fang– Howard trial function. In the next iteration these parameters are replaced by new values. 4. Using these initial parameters, solve Poisson equation, (8.30), and obtain an approximate solution of the potential φ(z).3 5. Inserting the potential into the Schrödinger equation, (8.29), obtain the wave function ζi (z) and eigenvalue Ei . 6. Calculate the electron sheet density of each subband from (8.31). 7. Replace the data of (3) by new data, and repeat the processes (3–6). This iteration is continued till the energy Ei converges. Self-consistent solutions for the electronic states in Si-MOSFET fabricated on the (100) surface are shown in Fig. 8.4, where the electron sheet density Ninv = 1.0 × 1013 cm−2 , NA = 5.0 × 1017 cm−3 and the parameters used are m l = 0.916 m, m t = 0.190 m and κs = 11.7. In the case of the Si (001) surface, we have a subband series of E0 , E1 , E2 , . . . for m 3 = m l and n v = 2, and series of E0 , E1 , E2 , . . . for m 3 = m t and n v = 4. The solid curve in Fig. 8.4 is the conduction band profile V (z), where the conduction band energy at the Si/SiO2 interface is set to be zero. The horizontal solid lines are Ei (i = 0, 1, 2) and the horizontal dashed lines are Ei (i = 0, 1), and the Fermi energy is shown by the dot-dashed line. The squared wave functions for the Ei series are plotted by solid curves and those for the Ei series by dashed curves. It is very interesting to point out that the subband energies E1 and E0 are very close. In Table 8.1 the self-consistent solutions for the subband energies, 2

Although the Schrödinger equation is a continuous function, the method discretizes the wave function into 200 meshes, giving rise to a 200 × 200 matrix equation. The eigenvalues and eigenfunctions are obtained by diagonalizing the matrix. In general we are interested in the lower energy states and some of the lowest values of the energies and wave functions. Details of the calculations are found in textbooks of numerical analysis. 3 Neglecting the contribution from N depl and assuming −E s = eNinv /κs 0 and a triangular potential, the Schrödinger equation may be solved by the iteration method to give converged solutions.

8.2 Two-Dimensional Electron Gas Systems

437

Fig. 8.4 Self-consistent solutions for inversion electrons in the Si (001) surface. The potential energy V (z), wave function |ζi (z)|2 , subband energy Ei and Fermi energy (horizontal dot-dashed line) are shown. The subband energies of the Ei series are indicated by the horizontal solid lines and the Ei series by the horizontal dashed lines, and the corresponding wave functions are shown by the solid and dashed curves. Ninv = 1.0 × 1013 cm−2 , NA = 5.0 × 1017 cm−3 , and T = 300 K. The Fermi energy is determined to be EF = 277 meV Table 8.1 Self-consistent solutions for the electronic states in the inversion layer of the (001) surface of Si-MOSFET. Ninv = 1.0 × 1013 cm−2 , NA = 5.0 × 1017 cm−3 , and T = 300 K Notation Subband energy Subband occupation Average distance z i (meV) (%) (nm) E0 E1 E2 E0 E1 E2

232 339 404 336 462 555

78.3 3.6 0.0 18.1 0.0 0.0

1.13 2.47 3.60 2.34 4.66 6.51

electron occupation and the average extension (distance) of the wave function z i are summarized. The Fermi energy is EF = 277 meV. From these results it is clear that electrons in the inversion layer of Si-MOSFET are quantized to form a two-dimensional electron gas. Experiments on the Shubnikov–de Haas effect and so on have been reported so far. The most prominent work has been the discovery of the quantum Hall effect in 1980, which will be discussed in detail later.

8.2.2 Quantum Wells and HEMT The semiconductors which exist in nature are elements and compound materials with periodic structures such as Si, Ge, and GaAs. In the late 1960s to early 1970s,

438

8 Quantum Structures 1

however, Esaki and Tsu proposed a completely new idea for growing new materials called superlattices, which do not exist in nature, which is based on the crystal growth technique, molecular beam epitaxy. They fabricated a new structure, called the superlattice, where n layers of GaAs and m layers of AlAs were grown periodically in a very high vacuum. Since then various types of quantum structures have been proposed and investigated experimentally. The purpose of Esaki and Tsu was to observe Bloch oscillations in superlattices. Bloch oscillations are achieved when electrons are accelerated from the bottom of a conduction band to the Brillouin zone edge without any scattering, and thus a very high field is required. In such a high electric field electrical breakdown readily occurs in a bulk semiconductor. On the other hand, in a superlattice, where the Brillouin zone is folded as stated later and mini-bands are formed, it may become possible to observe Bloch oscillations. Here we have to note that there exist several restrictions in order to grow a different semiconductor on a substrate. When different materials A and B are grown on a same substrate, the structure is called a heterostructure, and the characteristics of the heterostructure depend strongly on the physical and chemical properties of both materials. In order to get a good structure it is essential that the lattice constants of both materials are equal or, in other words, the two materials are lattice matched. Under the lattice-matched condition, controlled crystal growth provides lattice-matched crystal growth, pseudomorphic growth. Lattice mismatch of crystal A with lattice constant aA and B with lattice constant aB is defined by η = 2|aA − aB |/(aA + aB ). For a heterostructure with a small lattice mismatch, pseudomorphic growth is achieved, while for a heterostructure with a large lattice mismatch lattice defects (misfit dislocation) are introduced in order to relax the strain due to the lattice mismatch. In order to avoid the defects, thin layer superlattices are grown alternately by limiting the number of the layers to less than the critical layer thickness. Such a superlattice grown without strain relaxation is called a strained-layer superlattice. From these considerations we find that the growth of superlattices and quantum structures without strain effects is achieved by choosing materials with small lattice mismatch, or lattice-matched materials. In Fig. 8.5 the energy gaps versus the lattice constants are plotted for typical III–V compound semiconductors (cubic zinc blende crystals), where the solid and open circles represent direct and indirect band gaps, respectively. For example, the lattice constants of GaAs and AlAs are 5.653 and 5.660 Å, respectively, and the lattice mismatch is η = 0.12%. In the case of such a small lattice mismatch, pseudomorphic crystal growth is possible. From this reason early studies of quantum structures have been carried out intensively in heterostructures with GaAs and Alx Ga1−x As (x = 0 − 1). In materials of large lattice mismatch, it is possible to achieve latticematched crystal growth by using ternary alloys, such as a combination of GaInAs and InP. Compounds of four elements will provide a wide variety of pseudomorphic crystal growth. The energy band diagrams of heterostructures with lattice match are classified into three cases, as shown in Fig. 8.6, which are type I, type II and type II after the notation of Esaki et al. In type I the conduction band of semiconductor B with the smaller band gap becomes a minimum and the valence band a maximum, and therefore electrons and holes are excited in this region. In type II (staggered) the minimum of

8.2 Two-Dimensional Electron Gas Systems

439

Fig. 8.5 Energy band gaps plotted as a function of the lattice constant for typical III–V compound semiconductors, where the solid and open circles represent direct and indirect gaps, respectively

Fig. 8.6 Three types of heterostructure. a type I: electrons and holes are confined in the same space. b type II (staggered): Confinement of electrons and holes are spatially different, resulting in spatially indirect transition. c type III (misaligned): zero-gap

the conduction band of semiconductor A and the maximum of the valence band of semiconductor B are spatially different, resulting in a spatially indirect band gap. In type III (misaligned) the heterostructures behave as a zero-gap material (semimetal) or as a narrow gap material. Of these three types the type I heterostructures have been most intensively investigated. Here we will consider the quantum wells of type I heterostructures. The regions of the conduction band minimum and maximum are called the well layer and barrier layer, respectively. When the barrier layer is thick, electrons are not able to penetrate and are confined in the quantum well region, resulting in quantization of the electron motion perpendicular to the heterointerface, forming a subband structure. Since electrons are able to move in the plane parallel to the heterointerface, the electrons exhibit two-dimensional characteristics. These features are shown in Fig. 8.7. Figure 8.7a is the case for a non-doped heterostructure and both the well and barrier regions are electronically neutral, giving rise to zero electric field. Figure 8.7b is the uniformly

440

8 Quantum Structures 1

Fig. 8.7 Modulation doping in heterostructures. a non-doped case, where no electric field exists. When low densities of electrons and holes are excited by photon absorption, they occupy the subbands in the conduction band and the valence band, respectively, and they recombine to end up at the initial states. b is the case where impurity donors are uniformly doped in both the well and barrier regions. The electrons confined in the well regions form two-dimensional states and are subject to impurity scattering in the well region, resulting in reduction of the electron mobility at low temperatures. c is the case called modulation doped, where donor impurities are doped only in the barrier regions, and electrons confined in the well regions are separated from the ionized impurities. Therefore, the high mobility of two-dimensional electron gas is achieved

doped case in which donors and electrons excited from the donors are confined in the well region, giving rise to two-dimensional electron gas formation in the well region. The electron mobility in such a structure is affected by ionized impurity scattering due to the donors in the well region and is reduced at low temperatures. To avoid this decrease in mobility a new idea was proposed, which is shown in Fig. 8.7c, where electrons in the well regions are supplied from donors in the barrier regions and confined in the well regions, resulting in a reduction of the impurity scattering and an increase of the mobility at low temperatures. Note that impurity potential is a longrange force and thus electrons are affected by the ionized donors in the barrier region. A more dramatic reduction of impurity scattering is achieved by putting a non-doped spacer region near the well region. This method is called modulation doping [19]. In such structures, electrons are confined in the well region by the potential walls of the conduction band discontinuity ΔEc at the interface and are quantized in the direction perpendicular to the barriers, whereas the electrons can move in the plane parallel to the interface. Therefore, a two-dimensional electron gas is formed in the well regions. For simplicity, we assume that the potential wall is infinity and that the well region is from z = 0 to z = L (well width L). Then the electron wave functions (called envelope functions) ζn (z) are obtained by solving the one-dimensional Schrödinger equation

8.2 Two-Dimensional Electron Gas Systems

−

441

2 d 2 ζn (z) = En ζn (z) , 2m ∗ dz 2

which will give solutions ζn (z) = A sin

π

nz ,

(8.34) L √ where A is the normalization constant, A = 2/L. The corresponding eigenvalues are 2 π 2 n (8.35) En = 2m ∗ L and the total electron energy is given by E=

2 2 2 π 2 2 2 2 2 n k + k + En . + k ≡ + k x y x y 2m ∗ 2m ∗ L 2m ∗

(8.36)

The eigenfunctions ζn (z) are orthogonal for different n. The ground state is given by n = 1 and the number of nodes of the function is n − 1. In other words, the greater is the number of nodes (n − 1), the higher is the energy. This relation holds for the self-consistent solutions described next. Now, we will deal with self-consistent calculations of the two-dimensional electron gas in heterostructures. We adopt the effective mass approximation to obtain the states of the two-dimensional electron gas. In general the electron effective mass and dielectric constant depend on the materials. Assuming that the particle velocity and electric field are along the direction perpendicular to the heterointerface, the simultaneous equations to be solved are as the following. The Schrödinger equation is given by 2 d 1 d ζn (z) + V (z)ζn (z) = En ζn (z) , (8.37) − 2 dz m ∗ (z) dz and Poisson’s equation for the potential φ(z) = −(1/e)V (z) is written as

d 1 d ρ(z) + e κ(z) φ(z) = − Nn |ζn (z)|2 , dz dz 0 n

(8.38)

where the spatial dependence of the effective mass m ∗ (z) and the dielectric constant (z) are taken into account. The simultaneous equations are solved in a similar fashion to the self-consistent calculations for the MOSFET. Here we will show the results for quantum wells of well width L = 20 and 50 nm in Figs. 8.8 and 8.9, respectively. In the calculations, the effective mass m ∗ = 0.068 m and the dielectric constant κ = 12.9 are assumed to be spatially uniform, for simplicity. The barrier height and electron sheet density are set to be ΔEc = 0.3 eV and Ns = 1012 cm−2 , respectively and the solutions are obtained for T = 4.2 K. The subband energy En , Fermi energy EF and electron sheet density Nn in each subband obtained from the self-consistent calculations are summarized in Table 8.2.

442

8 Quantum Structures 1

Fig. 8.8 Self-consistent solutions for a two-dimensional electron gas in an Al0.3 Ga0.7 As/GaAs modulation-doped quantum well with well width 20 nm. The results are at T = 4.2 K for electron sheet density Ns = 1012 cm−2 and spacer layer of 10 nm in the AlGaAs barriers. The subband energies and Fermi energy are indicated by the horizontal lines and the square of the wave function |ζn (z)|2 is plotted

Fig. 8.9 Self-consistent solutions for a two-dimensional electron gas in an Al0.3 Ga0.7 As/GaAs modulation-doped quantum well with well width 50 nm. The results are at T = 4.2 K for electron sheet density Ns = 1012 cm−2 and spacer layer of 10 nm in the AlGaAs barriers. The subband energies and Fermi energy are indicated by the horizontal lines and the square of the wave function |ζn (z)|2 is plotted Table 8.2 Fermi energy, subband energies and electron sheet density in each subband obtained from self-consistent calculations for Al0.3 Ga0.7 As/GaAs quantum wells with well width 20 nm and 50 nm. The parameters used are m ∗ = 0.068 m, = 12.9, Ns = 1012 cm−2 , and T = 4.2 K L = 20 nm L = 50 nm n 0 1 2 EF

En (eV)

0.042 0.065 0.116 0.071

Nn (1011 cm−2 ) 8.3 1.7 0.0

En (eV)

0.049 0.050 0.064 0.066

Nn (1011 cm−2 ) 4.8 4.7 0.55

8.2 Two-Dimensional Electron Gas Systems

443

Fig. 8.10 a Structure of HEMT, and b its energy band diagram (see [21])

We have already mentioned that the modulation doping will improve the electron mobility. Mimura has been involved with the development of the high frequency GaAs MESFET (Metal Semiconductor Field Effect Transistor) and arrived at the conclusion that the surface states of GaAs play the most important role in its performance. During the process to find a method for improvement, he got the idea of using an AlGaAs/GaAs heterostructure. With the help of Hiyamizu, they grew a heterostructure FET and confirmed its FET characteristics in 1980 [20]. They named the device the High Electron Mobility Transistor (HEMT). The structure of the HEMT is shown in Fig. 8.10a. High purity GaAs is grown on a GaAs substrate, and an Alx Ga1−x As (x ∼ = 0.3) layer of 60–100 Å thickness is then grown, followed by the growth of an Alx Ga1−x As layer with Si donors. Usually a cap layer of the GaAs is grown on the surface of AlGaAs in order to avoid oxidation of the AlGaAs. Metals such as AuGeNi are deposited on the GaAs surface and the ohmic contacts of the source and drain are formed by thermal diffusion. The gate electrode is fabricated by the deposition of Al metal between the source and drain contacts, which controls the sheet density of the two-dimensional electron gas by the gate voltage. The energy band diagram near the region of the AlGaAs/GaAs interface is shown in Fig. 8.10b, where the ionized donors in the AlGaAs layer and the two-dimensional electron gas in the GaAs layer are separated. The electron mobility and sheet electron density of such a HEMT structure are plotted as a function of temperature in Fig. 8.11. The electron sheet density is almost constant in the temperature region shown, whereas the electron mobility becomes very high at low temperature because of the reduction of impurity scattering [21]. Later, improvements in the crystal growth and the structure led to a high electron mobility greater than 1 × 107 cm−2 /Vs. In Fig. 8.11, the effect of light illumination on the electronic characteristics is shown, causing an increase in the electron sheet density and electron mobility as indicated by the symbols and , respectively [21]. An example of a self-consistent calculation of the two-dimensional electron gas in a HEMT at T = 4.2 K is shown in Fig. 8.12, where we have assumed Ns = 6 × 1011 cm−2 and Δt = 10 nm. The Fermi energy is EF = 0.085 eV and all the electrons occupy only the lowest subband below the Fermi energy, resulting in a degenerate condition. These electrons are confined in a narrow region about 15 nm thickness at the interface and thus the reason for the two-dimensionality of the electrons is clear. In addition, the electrons are well separated from the ionized donors in the

8 Quantum Structures 1

⁄

444

Fig. 8.11 Temperature dependence of the electron sheet density and electron mobility in a HEMT, where and are the electron sheet density and electron mobility under illumination, respectively. (After [21])

Fig. 8.12 Self-consistent solutions for a two-dimensional electron gas in a HEMT fabricated from Alx Ga1−x As/GaAs (x = 0.3), where Ns = 6 × 1011 cm−2 , T = 4.2 K, ΔEc = 0.3 eV, spacer layer thickness Δt = 10 nm, and m ∗ = 0.068 m. The bottom of the conduction band is plotted by the solid curve and the squared wave functions for each subband are shown. The values obtained are EF = 0.085, E0 = 0.064, E1 = 0.095, E2 = 0.115 eV, N0 = 6 × 1011 cm−2 , and N1 , N2 ≈ 0

AlGaAs layer and the impurity scattering is reduced. We have to note that impurity scattering is a long-range force interaction and thus remote impurity scattering plays an important role in the mobility at low temperatures.

8.3 Transport Phenomena of Two-Dimensional Electron Gas

445

8.3 Transport Phenomena of Two-Dimensional Electron Gas 8.3.1 Fundamental Equations In this section we will consider transport phenomena in a two-dimensional electron gas; the theoretical calculations are based on references [2–7]. After these original works many papers have been published, and more detailed calculations are found in [22, 23] (see also references therein). The electrons in the conduction bands of GaAs and AlAs are treated by the effective mass approximation and the wave function of the bulk state is expressed as Ψ = V −1/2

C k exp(ik · r) ,

(8.39)

k

where Ψ is normalized by the volume V and |C k |2 = 1. The band-edge energy is given by 2 k 2 . (8.40) E(k) = 2m ∗ In the following we assume that the effective mass approximation is valid for heterostructures. When electrons are confined in the z direction, the wave function of the two-dimensional electron gas is given by (8.3) and written as Ψ = ζ (z)A−1/2 exp(ik · r ) ,

(8.41)

where A is the area of the x, y plane, L is the width of the z direction, and the volume is given by V = AL. The normalization condition is written as

|ζ (z)|2 dz = 1 .

(8.42)

Writing the subband energy as En , we have shown that the electron energy in the quantum well of the heterostructure is defined by E(k) = En + E(k ) ,

(8.43)

where k is the wave vector parallel to the heterointerface given by k2 = k x2 + k 2y and the energy in the plane parallel to the heterointerface is given by

(8.44)

446

8 Quantum Structures 1

E(k ) =

2 2 (k + k 2y ) . 2m ∗ x

(8.45)

Next, we assume infinite barriers and a well width of W for simplicity. Under this assumption, the wave function and energy are given by the following relations as shown in Sect. 8.2.2: nπ 2 sin z , (8.46) ζn (z) = W W 2 π 2 2 En = n . (8.47) 2m ∗ W In the following we show the calculations based on (8.46). It is very easy to perform numerical calculations with the use of self-consistent solutions. First, we present the fundamental equations derived by Price [2]. Phonons are assumed to be three dimensional and their wave vector is defined by q 2 = q 2 + qz2 for the purpose of the calculations. The wave vector of an electron is changed by q after phonon emission or absorption, but such a conservation rule does not hold in the z direction. Instead, the following integral results from the matrix element:

W ζm (z)∗ ζn (z) exp(iqz z)dz , (8.48) Imn (qz ) = 0

where m = n corresponds to an intra-subband transition and m = n corresponds to an inter-subband transition. From the conditions of normalization and orthogonality, the integral has the property of a δ-function, i.e. Imn (0) =

1 (for m = n) 0 (for m = n) .

(8.49)

Next, we will present some important relations for the calculations of the scattering probability and the numerical results.

∞

−∞

where

|Imn (qz )|2 dqz = 2π

W

0

2 Φmn dz ,

Φmn (z) = ζm∗ (z)ζn (z) .

(8.50)

(8.51)

It is very convenient to introduce the following coefficient: 1 =2 bmn

0

W

2 Φmn dz .

Using this relation we may obtain the following relation

(8.52)

8.3 Transport Phenomena of Two-Dimensional Electron Gas

∞

−∞

In a similar fashion

∞

−∞

447

|Inn |2 dqz =

π . bnn

(8.53)

|Imn |2 dqz =

π . bmn

(8.54)

Using (8.46) for the wave function ζn (z), we find W , 3 W = , (n = m) 2

bnn =

(8.55)

bmn

(8.56)

which are independent of the subband indices m and n. The above results indicate that the coefficient bmn is different for intra-subband transitions (m = n) and intersubband transitions (m = n). It may be understood that the value 1/b gives a measure of the decay of |I |2 with q. When we use the wave function given by (8.46), Imn (q) is written as Inn (q) = Imn (q) =

sin( 21 W q) 1 Wq 2 sin 1 cos ( 2 W q) 1 Wq 2

n2 P, n 2 − (W q/2π )2

(8.57)

4mn(W q/π )2 2 P , 4m 2 n 2 − m 2 + n 2 − (W q/π )2

(8.58)

where sin() in the symbol sin cos () appearing on the right-hand side of Imn (q) is for the case that both m and n are even or odd, and cos() is for the case that one of the m and n is even and the other is odd, and P is the phase factor such that |P| = 1 with phase angle ± 21 W q.

8.3.2 Acoustic Phonon Scattering and Non-Polar Optical Phonon Scattering Detailed discussion has been given of the matrix elements of electron scattering in the case of three-dimensional (bulk) semiconductors in Sect. 6.3. Here, we will calculate the scattering rates for a two-dimensional electron gas using the result for the three-dimensional case. Therefore, we first summarize the results for the threedimensional case. Letting the electron–phonon interaction Hamiltonian be H1 and using (6.156), the scattering matrix element is written as k

|H1± |k

1 1 1/2 ± = n(q) + ± δk,k ±q C q , 2 2

(8.59)

448

8 Quantum Structures 1

where the upper (lower) symbol of ± corresponds to phonon emission (absorption) of a phonon with wave vector q and energy ω, k and k represent the electron initial and final states, respectively, and n(q) is the excitation number of phonons, which is given by the Bose–Einstein distribution function. The wave vector q is expressed as ± q = k − k .

(8.60)

The scattering rate is derived as follows from the results stated in Sect. 6.4: + − + wIII wIII (k, k ) = wIII 2π 2 C q n(q)δ E(k) − E(k ) + ω =

k

+ (n(q) + 1) δ E(k) − E(k ) − ω .

(8.61)

Noting that electron spin is conserved in scattering, and using (8.60) and replacing the summation of the final states with an integral, we find

k

=

1 (2π )3

d3 k =

1 (2π )3

d3 q .

(8.62)

When the excitation number of phonons is approximated as n(q) ∼ n(q) + 1 ∼ k B T /ω, the scattering rate reduces to wIII

2π 2 = SIII (2π )3

where SIII =

d3 k δ E(k) − E(k ) ,

2 kB T kB T Dac |C|2 = ω 2ρvs2

(8.63)

(8.64)

and the integral, which includes the δ-function, gives rise to the three-dimensional density of states gIII =

1 (2π )3

=

1 (2π )3

δ E(k) − E(k ) d 3 k = 2π(2m ∗ )3/2 E 1/2 . 3

dk 1 4π k 2 3 (2π ) dE (8.65)

The result means that the number of states in the energy range E and E + dE per unit volume is given by gIII dE, where the spin flip transition is disregarded and the spin degeneracy is set to be 1. In scattering in a two-dimensional electron gas, the spatial integration of the Bloch function (8.41) is divided into integrals for the perpendicular direction dz to the het-

8.3 Transport Phenomena of Two-Dimensional Electron Gas

449

erointerface and for the parallel direction dr . Therefore, two terms, Imn (qz ) defined in Sect. 8.3.1 and k δ[E(k ) + Em − E(k ) − En ± ω], appear in the matrix element, where k (q ) and k (q ) represent the wave vectors parallel to the heterointerface. Replacing the summation of the final states by (1/(2π )3 )d2 q dqz and integral with respect to q by d2 k using the property of the δ-function, we obtain the following results: wII =

2π 1 |Imn (qz )|2 dqz (2π )3

× |C|2 n(q)δ E(k ) − E(k ) + ΔEmn + ω + (n(q) + 1) δ E(k ) − E(k ) + ΔEmn − ω d2 k ,

(8.66)

where ΔEmn = Em − En = −ΔEnm .

(8.67)

Adopting the same assumption as for the three-dimensional case, it may be evident that we have the result

(8.68) SII = SIII |Imn (qz )|2 dqz . Since the two-dimensional density of states is given by

gII dE =

δ E(k ) − E(k ) d2 k =

we have wII =

2 m∗ 2π k dk = dE , (2π )2 π 2

2 1 m ∗ kB T Dac u(E(k ) − ΔEnm ) , 3 2 b 2ρvs

(8.69)

(8.70)

where u(x) is the step function which satisfies u(x ≥ 0) = 1 and u(x < 0) = 0. Here we discuss b in detail. In the case of intra-subband scattering within the nth subband, 1/b may be written as 1/b = 3/W , and thus this relation is used for scattering within the ground-state subband. In the case of inter-subband scattering, on the other hand, we have 1/b = 2/W , and thus the effective value of b is given by the following relation when the electron with energy E in the range En < En+1 is scattered into the mth subband by acoustic phonons:

π 2π π 3π π + (n − 1) , = gII + gII · = gII b bmm bm j W W j

(8.71)

where m ≤ n. For a large value of n, the prefactor of gII in the above equation reduces to ∼ = gIII , giving = (2m ∗ E)1/2 2/ = gIII /gII and (8.71) is approximated as ∼ rise to three-dimensional scattering.

450

8 Quantum Structures 1

A similar treatment is possible for non-polar optical phonon scattering and the scattering rate for a two-dimensional electron gas is written as wop =

2 m∗ 1 Dop 1 1 n(ω ± u(E(k ) ∓ ω0 − ΔEnm ) . ) + 0 b 4ρ2 ω0 2 2

(8.72)

Here we introduce new parameter x0 =

ω0 1 , n(x0 ) = x , kB T e 0 −1

(8.73)

and we find that 1 1 Nopnm = n(x0 ) + ± u(E ∓ ω0 − ΔEnm ) 2 2 1 = x 1 + ex0 u(x − x0 − xnm ) , e 0 −1

(8.74)

and for intra–subband transitions, putting ΔEnm = 0 we obtain Nop =

ex0

1 1 + ex0 u(x − x0 ) , −1

(8.75)

where we used xmn = ΔEnm /ω0 . Therefore (8.72) is rewritten as wop =

2 2 m∗ m∗ 1 Dop 1 Dop N , w = Nop (for xnm = 0) . opmn op b 4ρ2 ω0 b 4ρ2 ω0

(8.76)

See evaluation of the electron mobility for Problems and Answers of this Chapter.

8.3.3 Inter-Valley Phonon Scattering In many-valley conduction bands such as in Si, electrons are scattered between the valleys, absorbing or emitting a large wave vector phonon. This inter-valley phonon scattering is described in detail in Sect. 6.3.7 for the case of bulk semiconductors and is well interpreted in terms of deformation potential theory. Defining the involved phonon angular frequency as ωi j and the deformation potential as Di j , the scattering rate wint = 1/τint from the initial state of an electron in valley i, subband m and wave vector k to the final sate in valley j, subband n and wave vector k is calculated as follows. The strength of the interaction for inter-valley phonon scattering may be expressed as

8.3 Transport Phenomena of Two-Dimensional Electron Gas

Cq =

Di j . 2ρωi j

451

(8.77)

The energies of the initial and final states of the electron are respectively written as Eim (k ) =

2 k2 2m i∗

+ Eim ,

(8.78)

+ E jn ,

(8.79)

E jn (k ) =

2 k2 2m ∗j

where m i∗ and m ∗j are the isotropic effective masses of the valley i and j, and in the presence of anisotropy the final results may be obtained by replacing the effective masses with the density of states masses. Note that Eim and E jn are the energies of the bottom of the subbands m and n. Using these results the scattering rate is calculated as wint =

2 2π Di j ν j 2ρωi j (2π )2

k

1 2π

|Imn (qz )|2 qz

1 1 dqz d2 k , ×δ E jn (k ) − Eim (k ) ± ωi j n q + ∓ 2 2

(8.80)

where ν j is the valley degeneracy of the final state. When we put D=

m ∗j

2 ∗ k +

mi

2m ∗j Eim − E jn ∓ ωi j , 2

(8.81)

the integral of (8.80) with the δ-function reduces to

∞ 2 2 2 2 2 δ δ ∗ (k − D) d k = ∗ (k − D) 2π k dk 2m 2m 0 k j j =

2π m ∗j 2

u(D) .

(8.82)

Since the integral with respect to qz is the same as for the case of acoustic phonon scattering, the inter-valley phonon scattering rate is given by wint = =

ν j Di2j m ∗j 2ρ2 ωi j ν j Di2j m ∗j 2ρ2 ωi j

1 · 2bmn ·

1 1 nq + ∓ · u(E(k ) ∓ ωi j − ΔEnm ) 2 2

1 Ni j . 2bmn

(8.83)

452

8 Quantum Structures 1

where Ni j is the excited number of the intervalley phonons and given by (8.74) replacing ωop with ωi j .

8.3.4 Polar Optical Phonon Scattering Next, we will discuss polar optical phonon scattering. Since the matrix element for polar optical phonon scattering is proportional to the inverse of the phonon wave vector, q −1 , the previous treatments cannot be applied. From (6.239) derived in Sect. 6.3.6, we obtain the electron–polar optical phonon interaction |Cpop (q)| = α(ωLO ) 2

1 L3

3/2

2 2m ∗

1/2

1 , q2

(8.84)

where α is dimensionless quantity and is given by (6.240) and L 3 = V is the volume of the three-dimensional crystal. In the present case we are using the normalized wave function given by (8.41), and thus we can disregard the factor L 3 . Therefore we rewrite it as |Cpop (q)| = α(ωLO ) 2

e2 ω0 = 20

3/2

2 2m ∗

1 1 − κ∞ κ0

1/2

1 q2

1 , q2

(8.85)

and calculate the scattering rate as follows. Separating the phonon wave vector q into the component perpendicular to the heterointerface, qz , and the component parallel to the interface, Q = ±(k − k ), we obtain

Jmn (Q) ≡

+∞

−∞

|Imn (qz )|2 dqz . qz2 + Q 2

(8.86)

Then the scattering rate for a two-dimensional electron gas for polar optical phonon scattering is given by 1 e2 ω0 2 2(2π ) 0 κ∞ 1 × n(ω0 ) + ± 2

wpop =

1 Jmn (Q)d2 k κ0 1 δ E(k ) − E(k ) ∓ ω0 − ΔEnm . (8.87) 2 −

Equation (8.86) may be rewritten as the following by using (8.51):

8.3 Transport Phenomena of Two-Dimensional Electron Gas

Jmn (Q) =

π Q

453

dz 1 dz 2 Φmn (z 1 )Φmn (z 2 ) exp(−Q|z 1 − z 2 |) .

(8.88)

Following the treatment of Price [2], we discuss the following two extreme cases. As stated before, |Imn |2 decreases rapidly with increasing q. When the parameter Q is smaller than the critical value of q, |Inn (qz )|2 may be replaced with the value at qz = 0 and put outside the integral, giving rise to the approximate result Jnn (0)

π (for small Q) . Q

(8.89)

The value of Jmn (0) may be approximated by expanding the exponential term as 1 − Q|z 1 − z 2 | + · · · to give Jmn (0)

2W m 2 + n 2 (for small Q) , π (m 2 − n 2 )2

(8.90)

where the wave function derived for a quantum well with infinite barrier height, (8.46), is used. On the other hand, for large values of Q, sin(W qz /2)/(W qz /2) in Imn (qz ) behaves like a δ-function and it may be approximated as Jmn

π (for large Q) . bmn Q 2

(8.91)

Using these results, |Inn (qz )|2 and Jnn (Q) which determine the strength of intrasubband scattering and |Imn (qz )|2 and Jmn (Q) (m = n) which determine the strength of inter-subband scattering are calculated and plotted in Figs. 8.13 and 8.14 for several parameters, respectively. For the intra-subband scattering, J11 (Q) and J22 (Q) are almost the same in magnitude and therefore the former values are plotted in Fig. 8.13. The curves of |Imn (qz )|2 represent intra-subband (m = n) and inter-subband scattering (m = n) for acoustic phonon scattering and non-polar optical phonon scattering. The curves of Jmn (Q) represent the strength of the polar optical phonon scattering. Here we will estimate the scattering rate for polar optical phonon following the treatment of Price [2]. It is evident from (8.87) that the scattering rate depends on Q = |k − k |. We will consider the case where the inter-subband transition plays an important role and we will consider the temperature range T

1. Then using (8.91), (8.95) reduces to wpop

1 1 1 3 e2 1 Npop = Npop − − κ∞ κ0 W 80 κ∞ κ0 1 Npop s−1 . (8.97) ∼ 1.45 × 105 × W π e2 b11 8π 0

For example, in a quantum well of 10 nm well width, the phonon excitation number at T = 300 K is n(ω0 ) = 0.342, which gives wpop = 4.95 × 1012 s−1 , and n(ω0 ) = 0.0168 at T = 100 K, which gives wpop = 2.43 × 1011 s−1 . In a narrow quantum well, on the other hand, using (8.89), (8.95) reduces to wpop

e2 = k0 80

1 1 − κ∞ κ0

Npop ∼ 1.20 × 1013 × Npop s−1 .

(8.98)

456

8 Quantum Structures 1

In a similar fashion to the wide well case, wpop may be estimated as 4.12 × 1012 s−1 at T = 300 K and 1.85 × 1011 s−1 at T = 100 K. From these results we may conclude that both approximations give almost the same magnitude for the scattering rate. For deformation-potential type acoustic phonon scattering, the scattering rate in a quantum well with well width W = 10 nm is estimated from (8.70) to be 1.16 × 1012 s−1 at T = 300 K and 0.202 × 1012 s−1 at T = 100 K. Optical phonon scattering, polar and non-polar, is reduced very rapidly at lower temperatures because of the low excitation number of phonons involved. Therefore, in the lower temperature range (T < 100 K), acoustic phonon scattering dominates, but at higher temperatures optical phonon scattering plays an important role. See Problems and Answers of this Chapter for evaluation of electron mobility of the respective model.

8.3.5 Piezoelectric Potential Scattering Many III–V compound semiconductors belong to the zinc blende crystal structure, and piezoelectric field waves are excited along with the acoustic phonon propagation. These piezoelectric potential waves induce electron scattering and the scattering processes in the three-dimensional case is described in detail in Sect. 6.3.4. Here the lattice vibrations are dealt with as three-dimensional phonons to derive the scattering rate in a two-dimensional electron gas for piezoelectric potential scattering. Using (6.197) we may write |Cpz (q)| = 2

∗ e · epz

∗

2

, 2M N ωq

(8.99)

∗ is the effective piezoelectric constant, and where M N = ρ is the crystal density, epz = κ0 . Using the relation ωq = v s · q and approximating as n(ωq ) = kB T /ωq (assumption of equipartition rule), and from the comparison with the deformation potential type acoustic phonon scattering, we obtain the relation 2 → Dac

e · e 2 14

A , Q 2 + qz2

(8.100)

where A( Q, qz ) is a dimensionless parameter of anisotropy which depends on the phonon propagation direction. In the case of acoustic phonon scattering for intrasubband transitions, the associated phonon wave vector Q is small and all the terms except |Inn |2 in the integral decrease rapidly, enabling us to approximate |Inn |2 = 1. Then we have e · e 2 π 14 2 π → B, (8.101) Dac b Q where

8.3 Transport Phenomena of Two-Dimensional Electron Gas

B=

Q π

∞

−∞

Q2

457

A dqz . + qz2

(8.102)

Since transverse and longitudinal acoustic waves contribute to the piezoelectric scattering, defining the respective term as Bt and Bl , we may rewrite SII =

kB T π 2 Q 2

(e · el )2 Bl (e · et )2 Bt +2 2 ρvl ρvt2

,

(8.103)

where el and et are the piezoelectric constants for longitudinal and transverse acoustic waves, respectively, and in the case of GaAs, for example, et = e14 and el = 0. The piezoelectric constant e14 of GaAs is known to be −0.160 C/m2 . According to the calculations of Price [2] the coefficients Bl and Bt are Bl =

9 13 , 2Bt = . 32 32

(8.104)

In Chap. 11 we discuss piezoelectric potential scattering in GaN, where the normal mode analysis (Debye model) of the elastic anisotropy is discussed. Subband transitions due to the piezoelectric potential may be treated as elastic scattering and we have the following relation between Q and k : Q 2 = 2(1 − cos θ )k2 ,

(8.105)

where θ is the angle between the electron wave vectors k of the initial and final states. The scattering rate in a two-dimensional electron gas due to the piezoelectric potential is given by m∗ SII , (8.106) wpiez = π 3 where is the average over the angle θ . The relaxation time which determines the electron mobility is obtained from the scattering rate multiplied by (1 − cos θ ) and is averaged as shown in Sect. 6.2. Therefore, the relaxation time is given by 1 m∗ (1 − cos θ )SII . = τ π 3

(8.107)

As seen in (8.103), the scattering factor for the piezoelectric potential SII is proportional to 1/Q. Using the relation of (8.105), the average of (8.107) results in

k 2 (1 − cos θ ) = . Q π

(8.108)

Therefore, the relaxation time of the electron in the subband Em is given by the following relation:

458

8 Quantum Structures 1

1 τpiez

m∗ 2 1 (Q SII ) 3 π π k √ (e · el )2 Bl kB T m∗ 2(e · et )2 Bt = √ + . √ 2 2 2 2 ρvl ρvt E − Em 2π =

(8.109)

8.3.6 Ionized Impurity Scattering Electrons are scattered by the Coulomb potential induced by ionized impurities [3, 24, 25]. Assuming that a point charge +e is located at the position (r 0 , z 0 ), the static potential induced by the charge φ(r , z) is written as φ(r , z) =

1 e , 4π κ0 (r − r 0 )2 + (z − z 0 )2

(8.110)

where κ0 is the dielectric constant of the semiconductor we are interested in. The scattering Hamiltonian for this ionized impurity is written as Hion = −eφ ,

(8.111)

and the scattering matrix element of an electron from a state in subband m and wave vector k into a state in subband n and wave vector k is given by

e2 ζn∗ (z)ζm (z)dz 4π κ0 A

exp[i(k − k ) · r ] × d2 k , (r − r 0 )2 + (z − z 0 )2

n, k |Hion | m, k = −

(8.112)

where A is the area of normalization. Putting Q = k − k , the squared matrix element is n, k |Hion | m, k 2 =

where Imn (Q, z 0 ) =

e2 2π κ0

2

1 A2 Q 2

|Imn (Q, z 0 )|2 ,

ζm∗ (z)ζn (z) exp(−Q|z − z 0 |)dz .

(8.113)

(8.114)

The scattering rate for a two-dimensional electron from a state |m, k to a state |n, k scattered by a point charge +e located at (r 0 , z 0 ) is then given by

8.3 Transport Phenomena of Two-Dimensional Electron Gas

459

P(m, k → n, k ; z 0 ) =

2 2π n, k |Hion |m, k δ E(k ) − E(k ) ,

(8.115)

where E(k ) = E(k ) =

2 k2 2m ∗ 2 k2 2m ∗

+ Em ,

(8.116)

+ En .

(8.117)

When the ionized impurities are distributed uniformly in the x, y plane and the volume density in the z direction is given by gion (z), the scattering probability of (8.115) reduces to

P(m, k → n, k ) = A P(m, k → n, k ; z 0 )gion (z 0 )dz 0 (8.118) =

2π

e2 2π κ0

2

1 Q2

A

ion Jmn (Q)δ E(k ) − E(k ) ,

where gion (z 0 ) is the density of ions per unit volume and Nion = ion (Q) is given by ion density per unit area. Jmn

ion Jmn (Q)

W

=

|Imn (Q, z 0 )|2 gion (z 0 )dz 0 .

gion (z 0 )dz 0 is the

(8.119)

0

When impurity ions are uniformly distributed and gion (z 0 ) = n ion , the above integration leads to (assuming Q = 0, Inn = 1) ion (Q) = An ion W . Jnn

(8.120)

Since the impurity scattering in a two-dimensional electron gas can be treated as elastic scattering, the relaxation time is given by 1 τion

=

n

k

k P(m, k → n, k ) 1 − x . kx

(8.121)

Replacing the summation with respect to k by an integral and defining the scattering angle by k x /k x = cos θ , we obtain

460

8 Quantum Structures 1

1 τion

2π e2 2 1 2 k2 2 k2 ion = J (Q)δ En − Em + − 2π κ0 AQ 2 mn 2 m∗ 2m ∗ n ×(1 − cos θ )d2 k .

(8.122)

When we define 2m ∗ (En − Em ) , 2 √ k 2 + D − 2k D cos θ ,

D = k2 −

(8.123)

Q=

(8.124)

the property of the δ-function gives rise to the following result: 1 τion

=

n

e4 2π (κ0 )2

ion (Q) m∗ Jmn (1 − cos θ )dθ · u(D) . A[Q(θ )]2 π 2

(8.125)

As will be discussed later, the screening by a two-dimensional electron gas of sheet density Ns modifies the relaxation time as 1 τion

=

n

e4 2π (κ0 )2

ion m∗ Jmn (Q(θ )) (1 − cos θ ) dθ · u(D) , (8.126) A [Q(θ ) + P Hmn (Q(θ ))]2 π 2

where the screening parameters P and Hmn are given by e2 Ns , 2κ k T

0 B Hmn (Q(θ )) = ζm (z 1 )ζm (z 2 )ζn (z 1 )ζn (z 2 ) P=

× exp [−Q(θ )|z 1 − z 2 |] dz 1 dz 2 .

(8.127)

(8.128)

8.3.7 Surface Roughness Scattering A two-dimensional electron gas is confined by potential barriers, which are the interface of SiO2 and Si in the case of a Si-MOSFET and are the GaAs/AlGaAs interfaces in the case of heterostructures. It is almost impossible to grow such surfaces with flatness of atomic order and thus the electrons are subject to scattering due to the surface roughness. The surface roughness scattering has been investigated theoretically by Ando and Matsumoto [1, 26, 27]. Let the plane parallel to the interface be the x, y plane and the perpendicular direction be the z axis. When the interface has an irregular fluctuation Δ(x, y) in the z direction, the fluctuation results in a fluctuation in the potential V (z), which

8.3 Transport Phenomena of Two-Dimensional Electron Gas

461

induces electron scattering. Assuming that the fluctuation Δ(x, y) is small and varies very slowly, then the expansion of Δ(x, y) may be approximated to the first order, which gives the perturbation Hamiltonian for surface roughness Hsr as Hsr = −

dV Δ(x, y) . dz

(8.129)

In the following we will consider intra-subband transitions for simplicity. The matrix element between the initial state of wave vector k and the final state k is written as k |Hsr |k = −

∞ −∞

1 dV ζ (z)dz dz A

ζ ∗ (z)

= −Feff Δ(k −

Δ(x, y)ei(k −k )·r d2 r A

k ) ,

(8.130)

where

Feff = Δ( Q) =

∞ −∞

1 A

ζ ∗ (z)

dV ζ (z)dz , dz

(8.131)

Δ(r )ei Q·r d2 r .

(8.132)

A

Here, Q = k − k , r is the position vector in the x, y plane, A is the area of normalization and ζ (z) is the envelope function obtained by solving the one-dimensional Schrödinger equation in the effective mass approximation. Feff /e is expressed by the effective electric field at the interface E eff as follows [26]: Feff

e2 = κ0

1 Ns + Ndepl 2

= eE eff ,

(8.133)

where Ns is the sheet electron density and Ndepl is the space charge density in the depletion layer. Note that this relation is derived for electrons in the inversion layer of a Si-MOSFET. Usually the correlation of the surface roughness is expressed by using a Gaussian function, which leads to the result !

"

(r − r )2 Δ(r)Δ(r ) = Δ exp Λ2

2

,

(8.134)

where Δ is the average height of the roughness in the z direction and Λ is the spatial extent of the roughness in the direction parallel to the interface. The Fourier transform of (8.134) reduces to " π Δ2 Λ2 Q 2 Λ2 |Δ( Q)|2 = exp − . A 4

!

(8.135)

462

8 Quantum Structures 1

With this approximation the scattering rate or the relaxation time τsr due to surface roughness scattering is derived as 2 2π k x 1 k |Hsr |k δ E(k ) − E(k ) 1 − . = τsr kx

(8.136)

k

Replacing (1 − k x /k x ) in (8.136) with (1 − cos θ ), taking account of the screening effect, and replacing the summation with respect to k by an integral with respect to Q, we obtain 2 1 2π π ΔΛe2 N ∗ Q 2 Λ2 = exp − τsr Q A (Q) 4 ×δ E(k − Q) − E(k ) (1 − cos θ ) ,

(8.137)

where N ∗ = (Ns /2 + Ndepl ) and (Q) is the dielectric constant with screening effect given by 1 1 e2 m ∗ F(Q) , (8.138) (Q) = κ0 1 + κ0 Q 2π 2 and κ0 is the dielectric constant of the semiconductor without the screening effect.4 F(Q) is defined by

F(Q) =

dz 1

dz 2 |ζ (z 1 )|2 |ζ (z 2 )|2 exp(−Q|z 1 − z 2 |) .

(8.139)

Approximation of (8.137) leads to the following relation: 1 π m ∗ Δ2 Λ2 e4 N ∗2 Q 2 Λ2 . exp − τsr (Q) 4 3 [(Q)]2

(8.140)

From these results we find that the surface roughness scattering results in an electron mobility proportional to 1/N ∗2 and therefore the electron mobility is expected to decrease with the square of the electron density. This feature has been experimentally confirmed in the Si-MOSFET. For example, Hartstein et al. [28] have reported that the decrease in electron mobility is explained in terms of (Ns + Ndepl )2 instead of (Ns + 2Ndepl )2 [1]. It has been pointed out that the surface roughness approximated by an exponential function explains the experimental data better than the Gaussian function approximation [29, 30].

4

In the case of a Si-MOSFET the dielectric constant should be estimated by taking contributions from the semiconductor and the insulator (SiO2 ). See reference [1].

8.3 Transport Phenomena of Two-Dimensional Electron Gas

463

8.3.8 Screening Effect Here we will discuss the effect of screening on the impurity potential. We assume that a change in the potential δφ(r) is induced by an ionized impurity and that the occupation of electrons is modified by the potential change. Then the subband energy Ei of the subband i is changed by the amount ¯ ) = −e δEi (r ) = −eφ(r

∞

−∞

δφ(r)|ζi (z)|2 dz .

(8.141)

Therefore, the charge density induced by the ionized impurity is given by ρind (r) = −e

δ Ni |ζ (z)|2 = −e

i

= e2

i

∂ Ni i

∂ Ni

∂Ei

∂Ei

φ¯ i (r )|ζ (z)|2 = −e2

δEi |ζ (z)|2

∂ Ni i

∂EF

(8.142)

φ¯ i (r )|ζ (z)|2 ,

where the sheet electron density Ni of the subband i is given by (8.16) and thus we have 1 m di n vi ∂ Ni . (8.143) = ∂EF π 2 1 + exp [(Ei − EF )/kB T ] Inserting this relation into (8.143), the induced charge density is reduced to ρind (r) = −2κ0

¯ )|ζ (z)|2 , Pi φ(r

(8.144)

i

where Pi is defined by the following equation: Pi =

1 e2 m di n vi . 2 2κ0 π 1 + exp [(Ei − EF )/kB T ]

(8.145)

Using these results, Poisson’s equation under the influence of the screening effect is obtained as 1 ∇ 2 δφ(r) = − (8.146) [ρext (r) + ρind (r)] . κ0 ˜ Replacing the potential due to ionized impurity δφ(r) with φ(r) and inserting (8.144) into (8.146), we obtain ˜ ∇ φ(r) −2 2

i

Pi |ζ (z)|

2

∞ −∞

˜ φ(r)|ζ (z)|2 dz = −

The positive charge at z = z 0 is defined by

1 ρext (r) . κ0

(8.147)

464

8 Quantum Structures 1

ρext (r) = e · δ(r )δ(z − z 0 ) .

(8.148)

Inserting this into (8.147) we find ˜ −2 ∇ 2 φ(r)

Pi |ζi (z)|2

i

=−

∞ −∞

2 ˜ φ(r)|ζ i (z)| dz

e δ(r )δ(z − z 0 ) . κ0

(8.149)

We apply the Fourier transform ˜ Q, z) = Φ(

˜ , z)ei Q·r d2 r φ(r

(8.150)

to both sides of (8.149), and the result is

∂2 e 2 ˜ Q, z) − 2 ¯ Q) = − Φ( − Q Pi |ζi (z)|2 Φ( δ(z − z 0 ) , 2 ∂z κ 0 i

where Φ¯ i ( Q) = Defining f (z) = − (8.151) reduces to

∞

−∞

˜ Q, z)|ζi (z)|2 dz . Φ(

e δ(z − z 0 ) + 2 Pi |ζi (z)|2 Φ¯ i ( Q) , κ0 i

∂2 2 ˜ Q, z) = f (z) . − Q Φ( ∂z 2

(8.151)

(8.152)

(8.153)

(8.154)

Using the Fourier transform of the above equation ˆ Q, qz ) = ψ( fˆ(qz ) =

∞

−∞ ∞

−∞

˜ Q, z)eiqz z dz , Φ(

(8.155)

˜ Q, z)eiqz z dz , Φ(

(8.156)

(8.154) is rewritten as ˆ Q, qz ) = − ψ(

fˆ(qz ) . qz2 + Q 2

(8.157)

The inverse Fourier transform of the above equation leads to the following relation:

8.3 Transport Phenomena of Two-Dimensional Electron Gas

465

fˆ(qz )e−iqz z dqz 2 2 −∞ −∞ qz + Q

∞ −Q|z−z |

∞

∞ e−iqz z e 1 f (z )dz =− f (z )dz dq = − z 2 + Q2 2π −∞ q 2Q −∞ z −∞

∞ −Q|z−z |

e e 2 ¯ =− δ(z − z 0 ) + 2 Pi |ζi (z )| Φi ( Q) dz − 2Q κ 0 −∞ i

˜ Q, z) = Φ(

1 2π

∞

ˆ Q, qz )e−iqz z dqz = − ψ(

e e−Q|z−z0 | − = Pi Φ¯ i ( Q) κ0 2Q i

1 2π

∞ −∞

∞

e−Q|z−z | |ζi (z )|2 dz . Q

(8.158)

Let us consider the scattering rate due to ionized impurities with the screening effect. The matrix element M˜ for impurity scattering from an initial state in subband m and with wave vector k to a final state in subband n and with wave vector k is given by ˜ k = M˜ = n, k |eφ|m,

∞

=

e A

=

e2 2κ0 Q A −

−∞

∞ −∞

ζn∗ (z)ζm (z) ·

e A

i(k −k ) ˜ φ(r)e · r d2 r A

˜ Q, z)dz ζn∗ (z)ζm (z)Φ(

∞ −∞

ζn∗ (z)ζm (z)e−Q|z−z0 | dz

∞

e 1 ∞ ¯ Q) Pi Φ( dz dz ζn∗ (z)ζm (z)|ζi (z )|2 e−Q|z−z | A Q −∞ −∞ i

= n, k |eφ|m, k −

˜ k Pi i, k |eφ|i,

i

i (Q) Hmn . Q

(8.159)

Now we define following relations M = n, k |eφ|m, k ,

(8.160)

M˜ =

(8.161)

i Hmn (Q) =

˜ k , n, k |eφ|m,

∞ ∞ dz dz ζn∗ (z)ζm (z)|ζi (z )|2 e−Q|z−z | −∞ −∞

,

(8.162)

where φ and M are the potential and matrix element without screening by the twodimensional electron gas. Therefore, the matrix element is rewritten as follows by using the above relations and (8.159).

466

8 Quantum Structures 1 i

H M˜ = M − Pi M˜ mn , Q Q M˜ = M. i Q + Pi Hmn

(8.163) (8.164)

8.3.9 Remote Ionized Impurity Scattering The discovery of modulation doping by Dingle et al. [19] in 1978 has enabled to improve the low-temperature mobility in AlGaAs/GaAs heterostructures. The most important factor to achieve high electron mobility is to separate 2DEG from ionized impurities in modulation-doped AlGaAs/GaAs heterostructures, where the 2DEG in GaAs layer at the interface is supplied from the donors doped in the barrier layer AlGaAs. This structure will reduce ionized impurity scattering because the GaAs layer is not doped intentionally and thus very low density of acceptors is introduced unintentionally. At low temperatures 2DEG is suffered from acoustic phonon scattering and ionized impurity scattering. Therefore the ionized impurities introduced in AlGaAs layer are the most important source of electron scattering. Interaction potential of 2DEG with such remote ionized impurities in AlGaAs is long range and expected to be the source of scattering potential for 2DEG in GaAs layer. It is well known that the introduction of a spacer layer, non-doped layer in the barrier AlGaAs at the interface, will increase the electron mobility quite a bit [21]. The first observation of electron mobility exceeding106 cm2 /Vs was made by Hiyamizu et al. [21]. In addition they reported an increase in the electron mobility after light exposure. Improvement of molecular beam epitaxy has let to produce heterostructures with low temperature mobility values exceeding 1 × 107 cm2 /Vs. Pfeiffer et al. [31] observed Hall mobility of 1.17 × 107 cm2 /Vs at carrier density of 2.4 × 1011 electrons/cm2 with a spacer layer of 700 Å after exposure to light at 0.35 K. Saku el al [32] reported electron mobility 1.05 × 107 cm2 /Vs in modulation-doped AlGaAs/GaAs with a spacer layer thickness 750 Å and with an electron sheet density of 3 × 1011 cm−2 . Umansky et al. [33] reported a maximum electron mobility of 1.44 × 107 cm2 /Vs at 0.1 K with a spacer thickness of 680 Å and a sheet electron density of 2.4 × 1011 cm−2 . All the data reported so far have revealed the importance of the doping profile in the barrier layer AlGaAs and thus the electron mobility is affected strongly by the remote ionized impurities. Hess [24] was the first to calculate the remote impurity scattering, but the results did not agreement with experimental observation. Ando et al. [1] reported a detailed model how to deal with the remote ionized impurity scattering, but they did not show any calculated results. Using the model Ando [34] reported an elaborate analysis of Coulomb scattering in addition to interface-roughness scattering and alloy-disorder scattering, and concluded that the Coulomb scattering due to remote impurities plays an important role in determining the low-temperature mobility. In the calculations two subbands are taken into account. Lee et al. [35] reported detailed analysis of

8.3 Transport Phenomena of Two-Dimensional Electron Gas

467

low field mobility of 2DEG in modulation doped AlGaAs/GaAs layer, where they took into account of remote impurity scattering, scattering due to background impurities, acoustic deformation potential scattering, polar optical phonon scattering and piezoelectric scattering. They pointed out that the low temperature mobility is well explained in terms of scattering by remote and background impurities. In addition they point out the importance of acoustic phonon scattering. Gold [36] also has reported theoretical analysis of the electron mobility of 2DEG in AlGaAs/GaAs heterostructures and interpreted experimental data in terms of multiple scattering mechanisms including remote impurity scattering. These reported analyses [31, 33, 35, 36] reveal that the scattering by background impurities plays an important role in the low temperature mobility. Here the scattering rate of 2DEG by ionized impurities is derived along the theoretical treatment made by Ando et al. [1]. For simplicity we assume that there exists only one type of impurities with the electronic charge +Z e. The dimensions of the sample are taken to be L for the length, A = L 2 for the area and V = L 3 for the volume. An impurity located at (r i , z i ) will produce a potential energy given by the following relation for z i < 0 V (r, z) =

Vi (r − r i , z − z i ),

(8.165)

i

Vi (r, z) = −

Z e2 , 4π (r − r i )2 + (z − z i )2

(8.166)

where = κ0 is the average dielectric constant of AlGaAs and GaAs layers and the dielectric constants of the two materials are assumed to be the same for simplicity in the following numerical calculations. Since we are interested in the electron mobility at low temperatures, the electrons are assumed to occupy the lowest subband (the electric quantum limit) with the wave function ζ0 (z) and the subband energy E0 , and thus the effective potential for the 2DEG is given by

∞ |ζ0 (z)|2 Vi (r, z) dz . (8.167) vi (r) = 0

Fourier transform of the above equation with respect to two-dimensional directions r = (x, y) will give the following relation vi (r) =

v Q (z i )ei Q·(r−r i ) .

Q

The inverse transform of the above equation results in

(8.168)

468

8 Quantum Structures 1

Fig. 8.15 The screening factor H00 (Q) given by (8.174) is plotted as a function of Q/b

1 Z e2 F(Q, z i ), L 2 2 Q

∞ F(Q, z i ) = e−Q|zi | e−Q|z| |ζ0 (z)|2 dz . v Q (z i ) = −

(8.169) (8.170)

0

When the screening of the potential energy by the 2DEG is taken into account, Q in the denominator of (8.169) should be replaced as follows [4] (and see Sect. 8.3.8) Q → Q + P Hmn ≡ Q + Q s ,

(8.171)

where 1 e2 m ∗ e2 ∂ Ns , (8.172) = 2 2 ∂EF 2 π 1 + exp [(E0 − EF )/kB T ] = Hmn (Q(θ ))

= ζm (z 1 )ζm (z 2 )ζn (z 1 )ζn (z 2 ) exp(−Q|z 1 − z 2 |)dz 1 dz 2 . (8.173)

P= Hmn

Here we evaluate Hmn (m = n = 0) given by (8.173) using the Fang-Howard formula (8.26) [18] for the ground state of the 2DEG and obtain the following relation: H00 =

1 + (9/8)(Q/b) + (3/8)(Q/b)2 . (1 + Q/b)3

(8.174)

The result is shown in Fig. 8.15, where H00 (Q) is plotted as a function of Q/b. Now we evaluate the relaxation time due to remote ionized impurity scattering. A schematic drawing of the modulation-doped heterostructure used in the present calculations is shown in Fig. 8.10a and b, where we assume AlGaAs layer is uniformly doped by Si donors (n rmt [cm−3 ]) from z = −ds to z = −(dN + ds ). The layer with thickness ds is called the spacer layer. The relaxation time due to the remote ionized impurity scattering is then written as

8.3 Transport Phenomena of Two-Dimensional Electron Gas

1 τrmt

469

2π −ds = L 2 n rmt (z i )dz i −(ds +dN ) k ×|vk−k (z i )|2 (1 − cos θkk )δ E(k) − E(k ) ,

(8.175)

where θkk is the angle between the wave vectors of 2DEG k and k , and the energy of the 2DEG is given by E(k) = 2 k 2 /2m ∗ . Summation with respect to k in (8.175) is expressed in an integral form shown below.

k

L2 = (2π )2

d2 k .

(8.176)

When the distribution of the ionized impurities is uniform with the density n rmt , (8.175) is reduced to 1 τrmt

2π L 2 = (2π )2

2

2

d k L n rmt

−ds

−(ds +dN )

dz i

×|vk−k (z i )|2 (1 − cos θkk )δ E(k ) − E(k) ,

(8.177)

where we used the conservation laws for the wave vectors of 2DEG k = k ± Q and the energy E(k ) = E(k). Using Fang-Howard formula (8.26) for the ground state of 2DEG, (8.170) is written as F(Q, z i ) = e−Q|z i |

b3 . (Q + b)3

(8.178)

The average wave vector of 2DEG is given by k = 2m ∗ kB T /2 (k < 108 [1/m], T < 50) for non-degenerate √case (Boltzmann statistics) and given by the Fermi wave √ vector kF = 2m ∗ EF / = 2π Ns (Ns is the sheet density of 2DEG) for degenerate case. Since b = 5.3 × 108 [1/m] and kF ∼ 2.5 × 108 [1/m] for Ns = 1016 [1/m2 ], the relation b > Q = 2k sin(θ/2) holds at low temperatures or for the sheet electron density Ns < 2 × 1012 [1/cm2 ], and thus we may approximate b3 /(b + Q)3 1 in (8.178) and H00 (Q) 1. Then, (8.177) reduces to the following relation with Q = 2k cos θk k , where we used θk k = θ for simplicity. 1 τrmt

2

2π

Z e2 dθ n rmt k dk dz i e−4k sin(θ/2)|z i | 2 0 2 (1 − cos θ ) |k δ | − |k|)(|k | + |k|) . (8.179) × 2m ∗ (2k sin(θ/2) + Q s )2

1 = 2π

Using the property of the δ-function and integrating over z i , the above equation reduces to

470

8 Quantum Structures 1

1 τrmt

2 2π n rmt m ∗ Z e2 2 sin2 (θ/2) = dθ 8π 3 [2k sin(θ/2) + Q s ]2 0 exp[−4ds k sin(θ/2)] − exp[−4(ds + dN )k sin(θ/2)] × 4k sin(θ/2)

2π ∗ 2 2 Ze n rmt m 2 sin(θ/2) = d(θ/2) 64π 3 k3 0 [sin(θ/2) + Q s /2k]2 × {exp[−4ds k sin(θ/2)] − exp[−4(ds + dN )k sin(θ/2)]} . (8.180)

Replacing θ/2 by θ and taking into account of the symmetry of the function and changing the range of integration into [0, π/2], we obtain the following relation. 1 τrmt

2

π/2 1 n rmt m ∗ Z e2 sin θ = dθ 16π 3 k3 0 [sin θ + Q s /2k]2 × {exp[−4ds k sin θ ] − exp[−4(ds + dN )k sin θ ]} .

(8.181)

Equation (8.181) is shown to be equivalent to Eq. (6) of Hess [24] and to Eq. (6) of Lee et al. [35]. Integral with respect to θ of the above equation will not give an analytical solution and thus we carry out the integral numerically to evaluate the electron mobility in two cases, degenerate and non-degenerate 2DEG. (1) Degenerate Case: When the 2DEG is degenerate (EF − E0 > 0) and occupies only the ground subband, we obtain the following relations m∗ (EF − E0 ) , π 2 e2 m ∗ e2 ∂ Ns = ≡ Qs , P= 2 ∂EF 2 π 2

Ns =

(8.182) (8.183)

where m ∗ /π 2 is the density of states of 2DEG. The electron mobility of degenerate 2DEG is calculated by replacing k of τ (k) by Fermi wave vector kF as shown later in ∗ 2 1/2 (8.212). Since √Fermi wave vector is defined by kF = [2m (EF − E0 )/ ] , we obtain k = kF = 2π Ns from (8.182). The mobility is, then, evaluated by numerical integration of (8.181). We introduce I1 (Q s /2kF , d) defined by

I1 (Q s /2kF , d) =

π/2

dθ 0

sin θ exp[−4d kF sin θ ] , [sin θ + Q s /2kF ]2

(8.184)

where d is ds or ds + dN . Inserting (8.181) and (8.184) into (8.212), the mobility of degenerate 2DEG is given by

8.3 Transport Phenomena of Two-Dimensional Electron Gas

471

eτ (kF ) m∗ kF3 16π 3 e 2 = . (8.185) n rmt m ∗2 Z e2 I1 (Q s /2kF , ds ) − I1 (Q s /2kF , ds + dN )

μrmt =

As stated earlier higher electron mobility is achieved by introducing different doping profile. Among them Pfeiffer et al. [31] reported that δ-doping in AlGaAs layer results in a high electron mobility of 11.7 × 106 cm2 /Vs at a carrier density of 2.4 × 1011 electrons/cm2 with a spacer layer of 700 Å after exposure to light at 0.35 K. Electron mobility limited by δ-doped remote impurity scattering is easily calculated. The integral with respect to z i in (8.179) is evaluated as

dz i n rmt e−4k sin(θ/2)z i = Nrmt e−4k sin(θ/2)ds ,

(8.186)

where Nrmt is the sheet density of δ-doped impurities, which supply 2DEG carriers and thus Nrmt = Ns . Note the difference between n rmt and Nrmt . Using this relation, (8.180) is written as 1 τrmt

=

2

2π 1 Nrmt m ∗ Z e2 sin2 (θ/2) d(θ/2) 8π 3 k3 0 [sin(θ/2) + Q s /2k]2 × exp[−4ds k sin(θ/2)] .

(8.187)

The integral with respect to θ of (8.187) does not give any analytical expression and thus we carry out integration for typical values of Q s , k = kF and ds , defining I (Q s /2kF ) by

π/2

I2 (Q s /2kF ) = 0

sin2 θ exp(−4ds kF sin θ )dθ . (sin θ + Q s /2kF )2

(8.188)

Using (8.212) electron mobility due to a δ-doped heterostructure at low temperatures is therefore given by μrmt =

1 eτ (kF ) 4π 3 e 2 3 . = kF m∗ Nrmt m ∗2 Z e2 I2 (Q s /2kF )

(8.189)

(2) Non-degenerate Case: In this case the Fermi energy is lower than the ground subband energy, (EF < E0 ), and the Fermi–Dirac distribution function may be approximated as 1/[1 + exp{(E − EF )/kB T }] exp{−(E − EF )/kB T }. Since Hmn 1 (m = n = 0) for b Q, we obtain P Hmn ∼ P ≡ Q s and the following relations

472

8 Quantum Structures 1

Ns =

m∗ π 2

∞ E0

m∗ E − EF −(E0 − EF ) dE = , (8.190) exp − k T exp B kB T π 2 kB T

e2 Ns e2 ∂ Ns = P= ≡ Qs , 2 ∂EF 2kB T

(8.191)

where m ∗ /π 2 is the density of states for 2DEG as shown before for degenerate 2DEG. Here only the ground subband with its energy E0 is considered. Inserting (8.181) into (8.209) and (8.210) we may evaluate the mobility. However, the integral of (8.180) does not give an analytical solution we assume that k in the integrand is given by using the average k-vector k = [2m ∗ kB T /2 ]1/2 . Replacing kF by k in (8.184), the electron mobility is evaluated from (8.209) and (8.210) as μrmt

√ 60 2 π 3/2 2 (kB T )3/2 = √ n rmt m ∗ e3 ×

1 . I1 (Q s /2k, ds ) − I1 ((Q s /2k, ds + dN )

(8.192)

Now we evaluate the mobility numerically and compare with experimental results shown in Fig. 8.11. For the purpose of comparison with the experimental data of Hiyamizu et al. [21] as an example, we assume m ∗ = 0.067 m, = κ0 with κ = 13, and the spacer layer thickness 200 Å. When a perfect ionization of donors is assumed, we obtain the thickness dN from the relation Ns = dN n rmt , which gives dN = 0.5 × 10−6 cm =50 Å for n rmt = 1018 cm−3 and Ns = 5 × 1011 cm2 and dN = 30 Å for Ns = 3 × 1011 cm−2 . The former and latter cases of Ns correspond to the parameters of Hiyamizu et al. [21] with and without exposure to light, respectively. Fermi energy at low temperatures is EF − E0 = 3.55 meV for the 2DEG density Ns = 1011 cm−2 and 35.5 meV for Ns = 1012 cm−2 from (8.182). In such cases 2DEG is treated as degenerate. The mobility of 2DEG limited by the remote ionized impurity scattering calculated from (8.185) is shown in Fig. 8.16, where the mobility is plotted as a function of 2DEG sheet density Ns for three different spacer layer thickness ds = 200, 250, 300 Å, and for the impurity density n rmt = 1018 cm−3 . For comparison calculated mobility for n rmt = 1.5 × 1017 cm−3 and ds = 300 Å, is plotted by the dashed curve. The calculated mobility increases with increasing the 2DEG sheet density, which is interpreted in terms of screening effect. Higher the sheet density is, the screening becomes more effective, resulting in higher electron mobility. Here we compare with the experimental data of Hiyamizu et al. [21]. Their data are plotted by the solid circles in Fig. 8.16, where μ = 1.25 × 106 (2.12 × 106 ) cm2 /Vs at T ∼ 5 K for a sample with the impurity density n rmt = 1.0 × 1018 cm−3 , Ns = 3 × 1011 cm−2 (5.04 × 1011 cm−2 after light exposure) and the spacer layer thickness ds = 200 Å. The calculated mobility is μrmt = 0.55 × 106 cm2 /Vs for Ns = 3 × 1011 cm−2 and 0.81 × 106 cm2 /Vs for Ns = 5.04 × 1011 cm−2 when the ionized impurity density is assumed to be the doped donor density n rmt = 1018 cm−3 . The calculated mobility is very small compared with the experimental data. This discrepancy may be

8.3 Transport Phenomena of Two-Dimensional Electron Gas

473

Fig. 8.16 Calculated mobility μrmt of 2DEG limited by the remote ionized impurity scattering in modulation-doped AlGaAs/GaAs heterostructures (HEMT) is plotted as a function of the electron sheet density Ns . Three curves are calculated for different spacer layer thickness ds = 200, 250, 300 Å. The donor density in AlGaAs layer is n rmt = 1018 cm−3 and the mobility is calculated from (8.185) assuming that 2DEG is degenerate. The donors are assumed to be completely ionized and the doped layer thickness is estimated by using the relation dN = Ns /n rmt . The mobility increases with increasing the spacer layer thickness ds . Experimental data of Hiyamizu et al. [21] are plotted by brown circles. The calculated mobility for n rmt = 1.5 × 1017 cm−3 and ds = 200 Å is plotted by the dashed curve for comparison

understood when we take into account of the ionization rate of the donors. As shown later the ionization of the donors is not perfect and expected to be 14 to 25 % in the case of δ-doped AlGaAs/GaAs. The dashed curve in Fig. 8.16 is calculated assuming the ionized donor density of n rmt = 1.5 × 1017 cm−3 in the sample of Hiyamizu et al. [21]. The calculated electron mobility is μrmt = 1.1 × 106 cm2 /Vs for Ns = 3 × 1011 cm−2 and 2.09 × 106 cm2 /Vs for Ns = 5.04 × 1011 cm−2 after exposure to light. These values are in good agreement with the experimental observation of Hiyamizu et al. [21]. The present results show an importance of the spacer layer to achieve high electron mobility in modulation-doped heterostructures. We have to note here that the ionized donor density after exposure to light is higher than 1.5 × 1017 cm−3 , which will reduces the mobility a little bit. As stated earlier Ando [34] reported the calculations of the mobility in AlGaAs/GaAs heterostructure using trial functions of the electron ground state given by Fang and Howard (8.26) and by the wave function with a nonvanishing amplitude in AlGaAs, here referred to as “Ando”. The results are shown in Fig. 8.17. We find there exists only a slight difference between the two approximations of the wave functions “Ando” and “Fang-Howard”. The most important difference in the assumption between the analysis shown in Figs. 8.16 and 8.17 is the acceptors impurities in GaAs and AlGaAs layers. Ando takes account of the ionized acceptors of the depletion region in the GaAs layer and the compensation in the AlGaAs layer. Therefore the calculated mobility Fig. 8.17 is lower than the result shown in Fig. 8.16. However, the overall features of the results are very similar and reveal the importance of the screening effect in the Coulomb scattering. The solid and dashed curves in Fig. 8.17

8 Quantum Structures 1

cm ⁄ Vs

474

cm Fig. 8.17 Mobility calculated by Ando [34] including Coulomb scattering by impurities in GaAs and AlGaAs layers. Wave function “Ando” takes account of penetration into AlGaAs layer (solid curves) and “Fang-Howard” is given by (8.26) (dashed curves). In the calculations ionized impurities in GaAs, depletion charge density Ndepl = 5 × 1010 cm−2 and compensated donors in AlGaAs, ND − NA = 2 × 1017 cm−3 with the compensation rate K = 0.25 are assumed. Calculated mobilities are plotted as a function of the electron sheet density Ns for different spacer layer thickness ds = 200, 150, 100, 50, and 0 A. Experimental data of Hiyamizu et al. [21] and Tsui et al. [37] are also plotted for comparison. After Ando [34]

are calculated for the wave functions of “Ando” and “Fang-Howard”, respectively. Experimental data of Hiyamizu et al. [21] and Tsui et al. [37] are plotted along with the calculated curves, where the black dot corresponds to the electron sheet density under the equilibrium condition (in the dark) and the open circles are obtained under exposure to light. The calculated curves by Ando [34] shows a reasonable agreement with the experimental data, except the decrease in mobility at high electron density observed by Hiyamizu et al. Next we calculate electron mobility in δ-doped AlGaAs/GaAs. In the calculation we have to estimate the ionized donor density in the δ-doped AlGaAs. Since the 2DEG in GaAs is supplied by the ionized donors, it is very reasonable to assume that Nrmt = Ns . The calculated result is shown by the solid curve in Fig. 8.18 as a function of the sheet density of 2DEG Ns , and the experimental date of Pfeiffer et al. [31] are plotted by the solid circles. We find in Fig. 8.18 that the calculated mobility increases with increasing the sheet density of 2DEG and that the calculated result agrees well with the experimental values. The calculated mobility is μrmt = 12.5 × 106 cm2 /Vs which is in good agreement with the observed mobility 11.7 × 106 cm2 /Vs (Ns = 2.4 × 1011 cm−2 ) at T = 0.35 K. The mobility of the same sample in the dark is estimated to be and 4.9 × 106 cm2 /Vs (Ns = 5.4 × 1010 cm−2 ) which is also in good agreement with the calculated mobility 5.8 × 106 cm2 /Vs. We can conclude here again that the spacer layer plays an important role in achieving high electron mobility in modulation-doped heterostructures.

8.3 Transport Phenomena of Two-Dimensional Electron Gas

475

Fig. 8.18 Calculated mobility μrmt of 2DEG limited by remote ionized impurity scattering in the δ-doped AlGaAs/GaAs heterostructures is plotted as a function of the electron sheet density Ns . The solid curves are calculated for spacer layer thickness ds = 700, 600 and 500 Å. For comparison the experimental data of Pfeiffer et al. [31] with μ = 11.7 × 107 [cm2 /Vs] (ds = 700 Åat T = 0.35 K with light illumination and with μ = 4.9 × 106 [cm2 /Vs] in the dark are plotted by the solid circles. Theoretical curves are obtained by assuming that the ionized donor density is Nrmt = Ns . The calculated mobility increases with increasing 2DEG density due to the screening effect

Fig. 8.19 Mobility μrmt of nondegenerate 2DEG limited by remote impurity scattering in modulationdoped AlGaAs/GaAs heterostructure (HEMT), where the mobility is evaluated from (8.192) for n rmt = 1017 cm−3 , ds = 200 Å, and electron sheet density Ns = 1.0 × 1010 , 5.0 × 1010 , and 1.0 × 1011 cm−2

2DEG of AlGaAs/GaAs heterostructures is usually degenerate as shown above. Here we will show the mobility of non-degenerate 2DEG limited by the remote impurity scattering for comparison. The calculated mobility of non-degenerate 2DEG limited by remote impurity scattering using (8.192) is shown in Fig. 8.19, where the doping density in AlGaAs layer is n rmt = 1.0 × 1017 cm−3 , spacer layer thickness ds = 200 Å and sheet density of 2DEG Ns = 1.0 × 1010 , 5.0 × 1010 , and 1.0 × 1011 cm−2 . We find in Fig. 8.19 that the mobility increases with increasing the 2DEG density Ns at low temperatures due to screening effect. At high temperatures the screening effect is weakened for lower 2DEG density and thus the mobility behaves like μrmt ∝ T 3/2 as in the case of 3D electrons.

476

8 Quantum Structures 1

8.3.10 Mobility of a Two-Dimensional Electron Gas In general the electron mobility can be evaluated by solving the Boltzmann transport equation. We have already presented the treatment of three-dimensional and bulk semiconductors in Chap. 6. A similar treatment is possible for the case of a twodimensional electron gas and the difference arises from the relaxation time τ and the density of states of the two-dimensional electron gas. According to the treatment of Sect. 6.2, we assume that the external electric field is weak and that the change in the distribution function due to the external field is small compared to the thermal equilibrium value f 0 . The distribution function is written as f = f 0 + f 1 , ( f 1 U , 2k1 k2

(9.1)

k12 − κ 2 sin(k1 a) sinh(κb) for E < U , 2k1 κ

(9.2)

and cos(kd) = cos(k1 a) cosh(κb) −

where k1 , k2 and κ are defined by the following relations: 2 k12 , 2m ∗A

(9.3a)

E −U =

2 k22 for E > U , 2m ∗B

(9.3b)

U −E =

2 κ 2 for E < U . 2m ∗A

(9.3c)

E=

Equations (9.1) and (9.2) are easily solved numerically. For simplicity we assume a = b, d = 2a and m ∗A = m ∗B = m ∗ = 0.067 m in Fig. 9.1 and the calculated result is shown in Fig. 9.2, where the horizontal axis is the well width or the barrier width a and the shaded areas represent the regions where energy eigenvalues exist. When the barrier width a is large, the probability for electrons to penetrate through the barrier decreases and electrons are confined in the well, giving rise to discrete energy levels. In this case, therefore, electrons are confined in the well regions and the electronic

9.1 Superlattices

517

Fig. 9.2 Electronic states of superlattices calculated from the Kronig–Penney model plotted as a function of the barrier width (well width), with the assumption of the same width for the well a and the barrier b (a = b), a superlattice period d = a + a, the same effective mass of the conduction band edges, m ∗ = 0.067 m, and a conduction band discontinuity U = 0.3 eV. For large a, the electrons are confined within the well layers, resulting in discrete energy levels, whereas for higher energies or smaller a, the electrons penetrate into the barrier layers and form mini-bands

states are the same as the two-dimensional electron gas we have already discussed. Even in the case of large a, electrons with high energy feel effectively lower barrier height and such electrons can penetrate into the barrier, resulting in the formation of energy bands (mini-bands). On the other hand, when the barrier width a is thin, electrons can penetrate into the barrier and form energy bands (mini-bands). Such bands are called mini-bands.

9.1.2 Effect of Brillouin Zone Folding As seen in the discussion of the previous section, a superlattice consisting of materials with lattice constants a and b has a period a + b. Therefore, the first Brillouin zone edge of such a superlattice is given by 2π/(a + b), indicating that a larger unit cell results in a smaller Brillouin zone. In other words, Brillouin zones of bulk materials, 2π/a and 2π/b, are folded into a smaller zone with 2π/(a + b) in a superlattice. As a result, many mini-bands are formed in a superlattice. This is a typical feature for superlattices and is called the zone-folding effect. It is very interesting to investigate the zone-folding effect of direct and indirect transition semiconductors. Figure 9.3a, b shows the energy band structures of direct and indirect bad gap semiconductors, respectively. Let us assume that we have two semiconductors with similar electronic properties and that a superlattice with mono-atomic layers is grown layer by layer. Therefore, the energy band structure is zone-folded at the point 2π/2a, as shown

518

9 Quantum Structures 2

Fig. 9.3 Brillouin zone-folding effect in superlattices, where the band structures are illustrated for the change in the lattice constant from a to 2a, for a a direct band gap semiconductor and b an indirect band gap semiconductor, where the dotted curves show zone-folded bands schematically

by the dotted curves in Fig. 9.3a or b. As a result, the zone-folding of indirect gap semiconductors causes the conduction band minimum of the superlattice to be located at k = 0 and therefore to a quasi-direct transition. For example, GaAs and AlAs have almost the same lattice constant and it is well known that GaAs and AlAs are respectively direct and indirect gap semiconductors. From the above considerations, therefore, we may expect a quasi-direct transition in the superlattice (GaAs)1 /(AlAs)1 due to the zone-folding effect in which the conduction band edge at the X point of AlAs is folded to the point. It has been pointed out that the use of superlattices makes it possible to control energy band structures and to produce materials with new properties. For this reason, this kind of technology is sometimes called band gap engineering. The crystal structure of GaAs and AlAs is the zinc blende type as shown in Fig. 1.4, where face-centered cubic lattices with different atoms are displaced by a distance of a/4 from each other in the diagonal direction. The bulk crystals belong ¯ m) but the superlattices of the layer structures of these to the point group Td (43 crystals have lower symmetry. For example, the Bravais lattice of a superlattice (GaAs)n /(AlAs)m with n layers of GaAs and m layers of AlAs depends on the total number of layers in a period, n + m. If it even, the lattice is simple tetragonal, 5 ¯ (P 4m2); if it is odd, the lattice is body-centered belonging to the space group D2d 9 ¯ (I 4m2). In the following we assume tetragonal, belonging to the space group D2d that GaAs and AlAs are lattice matched with the lattice constant a0 . Figure 9.4 shows the crystal structure of the (GaAs)1 /(AlAs)1 superlattice. We may show that √ the lattice constants of the superlattice (GaAs)n /(AlAs)m are given by a = a0 / 2 and c = (n + m)a0 /2. Therefore, the unit cell volume of the superlattice (GaAs)n / (AlAs)m is evaluated to be a03 /4 multiplied by n + m. The reciprocal lattice vectors are easily calculated from this result. Using the reciprocal lattice vectors, the first Brillouin zone of the (GaAs)n /(AlAs)m superlattice is calculated which is presented in Figs. 9.5 and 9.6. Figure 9.5 shows the first Brillouin zone for n + m = 2 (n = m = 1) and Fig. 9.6 is for n + m = 3, where the points at the zone boundaries of the superlattice are marked by labels such as Z and X in order to distinguish the critical points of the superlattice from those

9.1 Superlattices

519

Fig. 9.4 Crystal structure of superlattice (GaAs)1 /(AlAs)1 . Two zinc blende crystals are layered along the growth direction

Fig. 9.5 The first Brillouin zone of the (GaAs)n /(AlAs)m superlattice for n + m = 2 along with the first Brillouin zone of the zinc blende crystal. In general, the first Brillouin zone of a superlattice with an even value of n + m differs only in the folding in the direction X z , resulting in a simple tetragonal lattice

of zinc-blende crystal. In the text, the notation without an underline is used for the energy band structures shown later. The first Brillouin zone for other combinations, n + m, of the (GaAs)n /(AlAs)m superlattice may be calculated in a similar fashion, giving rise to a simple tetragonal the Bravais lattice for an even value of n + m and to a body-centered tetragonal for an odd value of n + m. With these results the energy band structures of superlattices are calculated. Here and in the following sections we will compare the theoretical calculations with the experimental results for (GaAs)n /(AlAs)n superlattices as an example. There have been published many papers on the theoretical calculations of superlattice energy band structures and experiments so far, and it is not the aim of this textbook to cover all of them. Therefore, we will present the theory of the tight binding approximation and compare the calculations with the experimental results for the photoreflectance and photoluminescence [5–7]. The bottom of the conduction band of GaAs is located at the point and that of AlAs is at the X point. Therefore, if we change the layer number n of the (GaAs)n /(AlAs)n superlattice, we can expect a crossing of the two conduction band edges, resulting in a crossing between type I and type II superlattices. A typical experiment to show the crossing is the photoluminescence

520

9 Quantum Structures 2

Fig. 9.6 The first Brillouin zone of the (GaAs)n /(AlAs)m superlattice for n + m = 3 along with the first Brillouin zone of the zinc blende crystal. In general, the first Brillouin zone of a superlattice with an odd value of n + m differs only in the folding in the direction X z , resulting in a body-centered tetragonal lattice

method [8–19]. On the other hand, energy band calculations for (GaAs)n /(AlAs)n superlattices have been carried out by the envelope function model [20], tight binding approximation [21–28], empirical and self-consistent pseudopotential methods [29– 32], local density functional method [33–38] and augmented-spherical-wave method [39].

9.1.3 Tight Binding Approximation The tight binding approximation is based on the linear combination of atomic orbitals, where the chemical bonds of a few atomic orbitals are considered, and has been successfully applied to calculation of the energy band structures of solids [40]. Although an increase in the number of atomic orbitals gives better accuracy for the calculated energy band structure, the time required for computation increases. The most popular tight binding method to calculate the energy band structure of semiconductors takes account of four atomic orbitals of s, px , p y and pz . In general a set of orthogonal and normalized atomic orbitals is obtained by the method of Löwdin [41]. The wave functions |ψ of a system satisfy the following eigenvalue equation: H |ψ = E|ψ ,

(9.4)

where E is the energy eigenvalue. When the wave function |ψ is expanded in atomic orbital functions |φ j (r), we obtain |ψ =

j

C j |φ j .

(9.5)

9.1 Superlattices

521

According to the variational principle, the energy E=

ψ|H |ψ , ψ|ψ

(9.6)

is minimized by changing the expansion coefficient C j . From this we find

Hi j − Eδi j C j = 0 .

(9.7)

The condition for the above equation to have a reasonable solution is det Hi j − Eδi j = 0 ,

(9.8)

Hi j = φi |H |φ j .

(9.9)

where When the basis functions |φ j consist of a limited number of atomic orbitals, the functions do not satisfy the condition of normalization, orthogonality and completeness. Therefore, a set of basis functions which satisfy normalization and orthogonality should be chosen. Usually the energy band calculations are carried out for Löwdin orbitals composed of atomic orbitals. The Löwdin orbital is defined by the following relation: Si−1 (9.10) |φiL = j |φ j , ij

Si j = φi |φ j .

(9.11)

Using the Löwdin orbitals |φiL for the basis functions, (9.8) reduces to det HiLj − Eδi, j = 0 ,

(9.12)

HiLj = φiL |H |φ Lj .

(9.13)

where

In the following tight binding approximation, the Löwdin orbitals are used as the atomic orbitals. Energy band calculations have been carried out utilizing the cyclic boundary condition. Here we assume zinc blende crystals and define the Bloch sum (quasiatomic functions) defined by the following relation, which are composed of atomic orbitals and satisfy the cyclic boundary condition: 1 exp [ik · (Ri + v b )] |nb Ri ) , |nbk) = √ N Ri

(9.14)

522

9 Quantum Structures 2

where N is the number of unit cells, b represents a (anion) or c (cation), Ri is the position of the anion, v b is δb,c (a0 /4)(1, 1, 1), and n is the orbital function s, px , p y or pz . The Schrödinger equation for the Bloch function |kλ is written as [H − E(k, λ)] |kλ = 0 ,

(9.15)

where λ is the band index. The above equation may be expressed by matrix representation as (9.16) (nbk|H |n b k) − E(k, λ)δn,n , δb,b (n b k|kλ = 0 . n,b

The Bloch function |kλ is written as the following with the use of the Bloch sum |nbk): |λk = |nbk)(nbk|kλ . (9.17) n,b

The matrix element (nbk|H |n b k) is written as (nbk|H |n b k) =

1 ik·(Ri −R j +vb −vb ) e (nb R j |H |n b Ri ) . N R ,R i

(9.18)

j

Here, we assume that (nb R j |H |n b Ri ) depends only on R m = Ri − R j + v b − v b . This assumption is called the two-center approximation [40]. Using this assumption (9.18) reduces to (nbk|H |n b k) =

exp(ik · Rm )(nb0|H |n b Rm ) ,

(9.19)

Rm

where (nb0|H |n b Rm ) is called the inter-atomic matrix element and is given by Table 9.1. (nn σ ) and (nn π ) are, respectively, the inter-atomic matrix elements for the σ bonding and π bonding between the atomic orbitals n and n . These inter-atomic matrix elements are determined empirically or semi-empirically and the accuracy of the tight binding approximation is determined by these values. It should be pointed out here that the inter-atomic matrix elements are proportional to the square of the bond length d (d −2 ) [3]. Chadi and Cohen [42] have calculated the energy band structures of semiconductors by taking account of the atomic orbitals s, px , p y and pz and the nearest-neighbor interactions, but they failed to obtain the band structures of indirect band gap semiconductors. Two different methods have been reported in order to solve this inconsistency. One is to take account of the second nearest-neighbor interactions of the atomic orbitals in addition to the nearest neighbor interaction [5]. The other is to use the excited state s ∗ in addition to the sp 3 orbitals [4]. In the following we will discuss the sp 2 s ∗ tight binding approximation first and then the second nearest-neighbor approximation in connection with the energy band calculation of superlattices.

9.1 Superlattices

523

Table 9.1 Inter-atomic matrix elements (nb0|H |n b Rm ). l, m and n are the direction cosines of Rm and the notation in the right-hand column is the representation of Slater-Koster. (After [40]) Ess ≡ (sb0|H |sb Rm ) (ssσ ) Esx ≡ (sb0|H | px b Rm ) l(spσ ) Ex x ≡ ( px b0|H | px b Rm ) l 2 ( ppσ ) + (1 − l 2 )( ppπ ) Ex y ≡ ( px b0|H | p y b Rm ) lm( ppσ ) − lm( ppπ ) Ex z ≡ ( px b0|H | pz b Rm ) ln( ppσ ) − ln( ppπ )

9.1.4 sp3 s∗ Tight Binding Approximation It has been pointed out that the tight binding approximation interprets the valence band structure but fails in describing conduction bands with high energy [3]. The reason for this disagreement is understood to be that the wave function of an electron in a conduction band, not localized in the crystal, cannot be described by the wave functions localized around the atoms. This is also the reason why the sp 3 tight binding approximation fails in describing the conduction band in indirect gap semiconductors. Vogl et al. [4] have proposed a new method to describe the conduction band by introducing an excited s state, the s ∗ orbital, in addition to the s and p orbitals for the tight binding basis functions. This method is called the sp 3 s ∗ tight binding approximation. First we will show the method proposed by Vogl et al. and the energy band structures of III–V compound semiconductors. In the calculation of the sp 3 s ∗ tight binding approximation, the atomic orbitals n of (9.17) are five orbitals for the anion and 5 orbitals for cations, a total of ten orbitals. Therefore, Hamiltonian matrix for the basis functions |nbk) results in a 10 × 10 matrix. These elements are given by Table (A) of reference [4], and are also shown in Sect. 9.1.5 of this textbook. From the solutions of the determinant the band structures of III–V semiconductors are obtained. As an example, the band structures of GaAs and AlAs are calculated by using the parameters given by Vogl et al. [4], which are shown in Figs. 9.7 and 9.8, respectively. It is found in Fig. 9.8 that the sp 3 s ∗ tight binding approximation gives the indirect band gap band structure for AlAs, which explains the experimental results quite well, whereas the sp 3 tight binding approximation failed in explaining it. The conduction band minima are located near the X point.

9.1.5 Energy Band Calculations for Superlattices Let us consider a superlattice (ca)n /(CA)m consisting of a layer structure of two different zinc blende-type materials such as n layers of ca and m layers of CA, periodically grown on the (001) surface, where c and C are cations, and a and A are anions. The superlattice (ca)n /(CA)m has 2(n + m) atoms in the unit cell (the

524

9 Quantum Structures 2

Fig. 9.7 Energy band structure of GaAs calculated by the sp 3 s ∗ tight binding approximation, which gives the direct band gap at the point

Fig. 9.8 Energy band structure of AlAs calculated by the sp 3 s ∗ tight binding approximation, which gives the indirect band gap in contrast to the sp 3 tight binding approximation

position vector is Ri and i is the index for each unit cell) and the respective atom has five orbitals of s, px , p y , pz and s ∗ . Then the Bloch sum is written as the following: 1 |χ αj (k) = √ exp ik · (Ri + τ j ) |α j , N Ri

(9.20)

where α = s, px , p y , pz , s ∗ and the subscript j indicates the atom in the unit cell with the position vector τ j . The Hamiltonian matrix of the superlattice for the basis functions is given by

9.1 Superlattices

525

1 2 3 . . . . . . 2n 1 2 3 . . . . . . 2m † a ac Ca ⎜ c ca ⎜ .. ⎜ . 3 ⎜ aˆ 0 .. ⎜ .. .. ⎜ . . . ⎜ .. ⎜ . . . ac . ⎜ ⎜ ⎜ 2n c c A ⎜ Hˆ = 1 ⎜ A AC ⎜ C

2 ⎜ C A ⎜ ⎜ ... 3 ⎜ A .. ⎜ .. .. . . . ⎜ ⎜ .. ⎜ . ⎝ h.c. A AC 2m C 1 2

⎛

⎞ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎠

(9.21) where h.c. means the Hermite conjugate and the matrix elements of the above equation are given by the following matrix:

s px a = py pz s∗

s px c = py pz s∗

s px ac = py pz s∗

⎛

s

s p x p y pz s ∗ ⎞ Esa 0 0 0 0 ⎜ 0 E pa 0 0 0 ⎟ ⎜ ⎟ ⎜ 0 ⎟ 0 E 0 0 pa ⎜ ⎟ ⎝ 0 0 0 E pa 0 ⎠ 0 0 0 0 Es ∗ a ⎛

(9.22a)

s p x p y pz s ∗ ⎞ Esc 0 0 0 0 ⎜ 0 E pc 0 0 0 ⎟ ⎜ ⎟ ⎜ 0 ⎟ 0 E 0 0 pc ⎜ ⎟ ⎝ 0 0 0 E pc 0 ⎠ 0 0 0 0 Es ∗ c ⎛

px

py

pz

(9.22b)

s∗ 0

⎞ Vss g0 Vsapc g1 Vsapc g1 Vsapc g0 ⎜ −Vscpa g1 Vx x g0 Vx y g0 Vx y g1 −Vs ∗ cpa g1 ⎟ ⎜ ⎟ ⎜ −Vscpa g1 Vx y g0 V g Vx y g1 −Vs ∗ cpa g1 ⎟ xx 0 ⎜ ⎟ ⎝ −Vscpa g0 Vx y g1 Vx y g1 Vx x g0 −Vs ∗ cpa g0 ⎠ 0 Vs ∗ apc g1 Vs ∗ apc g1 Vs ∗ apc g0 0

526

9 Quantum Structures 2

s px ca = py pz s∗

⎛

s

px

py

pz

s∗ 0

⎞ Vss g2 −Vscpa g3 Vscpa g3 Vscpa g2 ⎜ Vsapc g3 Vx x g2 −Vx y g2 −Vx y g3 Vs ∗ apc g3 ⎟ ⎜ ⎟ ⎜ −Vsapc g3 −Vx y g2 Vx x g2 Vx y g3 −Vs ∗ apc g3 ⎟ ⎜ ⎟ ⎝ −Vsapc g2 −Vx y g3 Vx y g3 Vx x g2 −Vs ∗ apc g2 ⎠ 0 −Vs ∗ cpa g3 Vs ∗ cpa g3 Vs ∗ cpa g2 0

The phase factors gi (i = 0 . . . 4) are given by the following equations with k = (ξ, η, ζ )2π/a0 : (see footnote1 for the derivation) ζ ξ +η 1 exp i cos , 2 2 2 ζ ξ +η i sin , g1 = exp i 2 2 2 ζ ξ −η 1 cos , g2 = exp i 2 2 2 ζ ξ −η i sin . g3 = exp i 2 2 2 g0 =

(9.23a) (9.23b) (9.23c) (9.23d)

The position vectors of a superlattice are also obtained in a similar fashion. In addition the position vectors of the next nearest neighbors g4 . . . g11 are also derived in a similar way. The matrix elements ac, ca and so on represent the nearest neighbor interaction indicate the interaction at the heterointerface. in a bulk material, and c A and Ca We have derived the Hamiltonian matrix to calculate the energy band structure of an arbitrary n + m superlattice, which will give us eigenvalues and eigenstates at an arbitrary point k in the Brillouin zone. However, we have to note that the energy band calculations require several parameters to be determined empirically. Before calculating the energy band structures of superlattices, we shall derive the Hamiltonian matrix of a bulk semiconductor such as GaAs and AlAs. The bulk matrix elements are obtained by putting n = 1 and m = 0. + ca † a + a a + a a † ac H (bulk) = H (n = 1, m = 0) = ac † + ca c + cc + cc† 1

(9.24)

The phase factors are obtained as follows. For example, in a bulk material, let the position vectors ¯ 1)a/4, ¯ ¯ of the four atoms next to a central anion d 1 = (111)a/4, d 2 = (11 d 3 = (1¯ 11)a/4, d4 = ¯ (11¯ 1)a/4 and we have g0 = eik·d 1 + eik·d 2 + eik·d 3 + eik·d 4 g1 = eik·d 1 + eik·d 2 − eik·d 3 − eik·d 4 g2 = eik·d 1 − eik·d 2 + eik·d 3 − eik·d 4 g3 = eik·d 1 − eik·d 2 − eik·d 3 + eik·d 4

9.1 Superlattices

527

represents the bulk Hamiltonian matrix elements of the tight binding approximation for a bulk semiconductor such as GaAs, and reduces to the matrix of Table (A) of Vogl et al. [4]. The parameters for the tight binding approximation are given by the following, which are determined empirically: Es± = E(1c ) + E(1v ) ± Es , c c v E p± = Ex x± = E(15 ) + E(15 )15 ± E p , 1 1 1 = − Es+ Es− − E(1c )E(1v ) , Vss = 4Ess 222 1 1 1 c v Vx x = 4Ex x = E p+ E p− − E(15 )E(15 ), 222 1 1 1 Vx y = 4Ex y = E p+ E p− − E(X 5c )E(X 5v ) , 222 1 1 1 Vs± p∓ = 4Es± p∓ = [Es± C± − D± ]/[Es± − Es ∗ ± ] , 222 1 1 1 Vs ∗ ± p∓ = 4Es ∗ ± p∓ = [Es ∗ ± C± − D± ]/[Es ∗ ± − Es± ] . 222

(9.25a) (9.25b) (9.25c) (9.25d) (9.25e) (9.25f) (9.25g)

where v c )E(X ± ) C± = Es± E p∓ − E(X ± v c v c +[Es± + E p∓ − E(X ± ) − E(X ± )][Es ∗ ± − E(X ± ) − E(X ± )] , c v Es± E(X ± ) E(X ± ) c v ) E p∓ E(X ± ) . [3 pt]D± = det E(X ± E(X c ) E(X c ) E ∗ ±

±

(9.26a) (9.26b)

s ±

Here E(X + ) = E(X 3 ), E(X − ) = E(X 1 ), where the subscripts + and − represent the anion and the cation, respectively, and E(α) = Eαc − Eαa . In the above equation the representation of Slater–Koster is used (see [40]). A convenient method to deduce the parameters of the tight binding approximation has been reported by Yamaguchi [26]. A comparison between the energy band structures of superlattices calculated from the sp 3 s ∗ tight binding approximation and deduced from experiment has been reported by Fujimoto et al. [6], where the transition energies determined from photoreflectance and photoluminescence experiments on (GaAs)n /(AlAs)n (n = 1 . . . 15) are compared with the theoretical calculations. Later Matsuoka et al. [7] pointed out that the assumptions used for the calculations are not correct. Photoreflectance signals are produced by the following mechanisms. Electron–hole pairs are excited by illumination of a weak intensity laser with photon energy larger than the energy band gap. The excited electrons (or holes) recombine at the sample surface and the other carriers, i.e. holes (electrons) induce an electric field at the surface, and thus the surface electric field is modulated without electrode contacts. Photoreflectance is therefore one of the techniques of modulation spectroscopy.

528

9 Quantum Structures 2

The experimental results at T = 200 K for photoreflectance (PR) and photoluminescence (PL) on (GaAs)n /(AlAs)n superlattices with n = 8 and n = 12 are shown in Figs. 9.9 and 9.10, respectively, where the best fit theoretical curves based on the Aspnes theory described in Sect. 5.1.3 are also plotted and the transition energies obtained from the best fit curves are indicated by the arrows. The arrows in Fig. 9.9 for the (GaAs)8 /(AlAs)8 superlattice indicate the transition energies, 1.797 eV, 1.897 eV, 1.915 eV, and 1.951 eV, which are determined from the best fit of the theoretical curve to the experimental data. In this superlattice we find a weak structure around 1.797 eV below the main peak at about 1.9 eV. Since the direct transition results in a strong peak in the PR spectra, the weak structure seems to arise from a direct transition with a very weak transition probability. In other words, the weak transition is ascribed to the quasi-direct transition between the zone-folded X z conduction band and the heavy-hole band (X z –h transition). The main peak is ascribed to the direct transition between the conduction band and the heavy-hole band (–h transition), and the peak at about 1.95 eV is due to the direct transition between the conduction band and the light-hole band (zone-folded valence band) (–l transition). We find in Fig. 9.9 that PL peaks appear at 1.8515 eV and 1.902 eV and these peaks exhibit good agreement with the weak structure at 1.797 eV and the main peak at 1.9 eV observed in the PR spectra. Figure 9.10 shows the PR and PL spectra at 200 K for (GaAs)12 /(AlAs)12 superlattice along with the best fit PR curve from the Aspnes theory. From the analysis of the PR spectra three transitions at 1.740 eV, 1.754 eV and 1.793 eV are obtained in the narrow region of photon energy from 1.7 eV to 1.85 eV. However, it is very interesting to point out that any weak structure such as observed in the PR spectra of the (GaAs)8 / (AlAs)8 superlattice of Fig. 9.9 has not been resolved in the (GaAs)12 /(AlAs)12 superlattice. This may be interpreted as showing that the X z conduction band is located on the higher energy side than the conduction band or that these two bands are mixed.

Fig. 9.9 Photoreflectance (PR) and photoluminescence (PL) spectra of the (GaAs)8 /(AlAs)8 superlattice, where the solid curves are the theoretical results based on the Aspnes theory and the arrows indicate the transition energies determined from the analysis. The dot-dashed curves are photoluminescence data. (T = 200 K)

9.1 Superlattices

529

Fig. 9.10 Photoreflectance (PR) and photoluminescence (PL) spectra of the (GaAs)12 / (AlAs)12 superlattice, where the solid curves are the theoretical results based on the Aspnes theory and the arrows indicate the transition energies determined from the analysis. The dot-dashed curves are photoluminescence data. (T = 200 K)

The PL spectra show a peak at about 1.75 eV which is in good agreement with the peaks at 1.74 eV and 1.754 eV of the PR spectra. In the following a comparison will be described between these experimental results and calculations based on the tight binding approximation. A comparison between experiments and calculations based on the sp 3 s ∗ tight binding approximation is shown in Fig. 9.11, where a similar comparison has been

Fig. 9.11 Transition energies of (GaAs)n /(AlAs)n superlattices calculated by the sp 3 s ∗ tight binding approximation are shown as a function of the layer number n, where the solid, dotted and dot-dashed curves are for direct allowed, quasi-direct, and indirect transition energies. In the figure the experimental data obtained by Matsuoka et al. [7] are also shown. The calculations based on the sp 3 s ∗ tight binding approximation show that a crossing from direct to indirect transitions occurs at n = 8 and the quasi-direct transition appears on the lower-energy side for n < 5

530

9 Quantum Structures 2

reported by Fujimoto et al. [6]. In the calculations the valence band discontinuity is assumed to be 0.54 eV. It is found in Fig. 9.11 that the theoretical calculations reveal a crossing from direct to indirect transitions occurs at n = 8 and to a quasidirect transition for n < 5. However, the experimental results exhibit the crossing between the direct and indirect or quasi-direct (X z ) transitions around n = 12 and that there exists a considerable disagreement between the experimental data and the calculations in the region of small n. The calculations show that the indirect transition energy is the lowest for n < 8, which corresponds to the R point for n = 1 and the M point otherwise. The reason for this disagreement may be ascribed to the fact that the sp 3 s ∗ tight binding approximation does not take account of the correct value of the effective mass of the X valleys of AlAs [7, 43].

9.1.6 Second Nearest-Neighbor sp3 Tight Binding Approximation We have already pointed out that Brillouin zone folding plays an important role in the electronic and optical properties of superlattices. In particular, the states X z and X x y strongly reflect the magnitude and anisotropy of the effective mass of the X valleys. Therefore, the energy band calculations require the exact effective mass of the X valleys. It has been shown that the sp 3 s ∗ tight binding approximation explains the indirect transition in some III–V semiconductors. However, the method will not guarantee the anisotropy of the effective mass at the bottom of the conduction band valleys. We may easily understand that more parameters are required to calculate the effective mass anisotropy of the X valleys from the tight binding theory. The states X z and X x y in superlattices may be calculated accurately by taking account of the precise anisotropy of the effective mass at the X point. Focusing on this point, Lu and Sham [5] have calculated the energy band structure by using the second nearest-neighbor sp 3 tight binding approximation and succeeded in obtaining good agreement with the experimental results. Also Matsuoka et al. [7] have performed energy band calculations for (GaAs)n /(AlAs)n superlattices by the second nearest-neighbor sp 3 tight binding approximation and explained their experimental results. The (ca)n (CA)m superlattice contains 2(n + m) atoms in a unit cell Ri (i indicates the ith unit cell), and in the second nearest-neighbor approximation four orbitals s, px , p y and pz are taken into account. The Hamiltonian matrix of a superlattice for these orbitals is similar to that for the sp 3 s ∗ tight binding approximation and reduces to a similar expression to (9.21). However, the elements are different and given by

s p b= x py pz

s px py pz ⎞ Esb + Esbsb g7 Esbxb g10 Esbxb g11 0 ⎟ ⎜ −Esbxb g10 E pb + Exbxb g7 −iλb + Exbyb g4 λb ⎟ ⎜ ⎠ ⎝ −Esbxb g11 iλb + Exbyb g4 E pb + Exbxb g7 −iλb 0 λb iλb E pb + Ezbzb g7 ⎛

9.1 Superlattices

531

s px py pz ⎞ ⎛ s Vss g0 Vsapc g1 Vsapc g1 Vsapc g0 p ⎜ −Vscpa g1 Vx x g0 Vx y g0 Vx y g1 ⎟ ⎟ ac = x⎜ p y ⎝ −Vscpa g1 Vx y g0 Vx x g0 Vx y g1 ⎠ pz −Vscpa g0 Vx y g1 Vx y g1 Vx x g0 s

⎛

px

py

pz

⎞ s Vss g2 −Vscpa g3 Vscpa g3 Vscpa g2 p ⎜ Vsapc g3 Vx x g2 −Vx y g2 −Vx y g3 ⎟ ⎟ ca = x⎜ ⎝ p y −Vsapc g3 −Vx y g2 Vx x g2 Vx y g3 ⎠ pz −Vsapc g2 −Vx y g3 Vx y g3 Vx x g2

s = px bb py pz

py pz s px ⎞ Esbsb (g8 + g9 ) −Esbxb g5 −Esbxb g6 Esbxb (g8 + g9 ) ⎜ Esbxb g5 Exbxb g8 + Ezbzb g9 0 −Exbyb g5 ⎟ ⎟ ⎜ ⎝ Esbxb g6 0 Exbxb g9 + Ezbzb g8 −Exbyb g6 ⎠ −Esbxb (g8 + g9 ) −Exbyb g5 −Exbyb g6 Exbxb (g8 + g9 ) ⎛

where Eαb = Eα (000)b ,

Vss = 4Ess ( 21 21 21 ),

Vx x = 4Ex x ( 21 21 21 ),

Vx y = 4Ex y ( 21 21 21 ),

Vsapc = 4Esx ( 21 21 21 )ac , Vscpa = 4Esx ( 21 21 21 )ca ,

Esbsb = 4Ess (110)b ,

Esbxb = 4Esx (110)b ,

Exbxb = 4Ex x (110)b ,

Exbyb = 4Ex y (110)b , Ezbzb = 4Ex x (011)b , and λb is the spin–orbit interaction of the p orbitals. The renormalized spin–orbit splitting of the anion and cation, a and c , is defined by λb =

1 b , (b = a, c) 3

(9.27)

and the following relations hold for | px bα), | p y bα) and | pz bα) ( px bα|Hso | p y bα) = −iλb , ( px bα|Hso | pz bα) = λb , ( p y bα|Hso | px bα) = iλb ,

(9.28a) (9.28b) (9.28c)

( p y bα|Hso | pz bα) = −iλb , ( pz bα|Hso | px bα) = λb ,

(9.28d) (9.28e)

( pz bα|Hso | p y bα) = iλb .

(9.28f)

The renormalized spin–orbit splitting energies for the p orbitals are tabulated in Table 9.2. The phase factors gi (i = 0 . . . 11) are given by (9.23a–9.23d) for g0 . . . g3 , and the other factors are as follows:

532

9 Quantum Structures 2

g4 = sin(ξ ) sin(η) ,

(9.29a)

i g5 = − exp(iζ ) sin(ξ ) , 2 i g6 = − exp(iζ ) sin(η) , 2

(9.29b) (9.29c)

g7 = cos ξ cos η ,

(9.29d)

1 exp(iζ ) cos ξ , 2 1 g9 = exp(iζ ) cos η , 2 g8 =

(9.29e) (9.29f)

g10 = i sin ξ cos η ,

(9.29g)

g11 = i cos ξ sin η .

(9.29h)

The parameters used in the calculations are those determined by Lu and Sham, which are shown in Table 9.3. The other parameters not shown in the table are assumed to be 0. Also, the spin–orbit interaction is neglected for simplicity.

Table 9.2 The renormalized spin–orbit splitting energies for the p orbitals [eV] Al

Si

P

S

Zn

Ga

Ge

0.024 0.044 0.067 0.074 0.074 0.172 0.29

As

Se

0.421 0.48

Cd

In

Sn

0.227 0.392 0.80

Sb

Te

0.973 1.10

Table 9.3 Parameters for the tight binding approximation shown with the notation of Slater-Koster (see [40]) SK notation GaAs AlAs Ess (000)a Ess (000)c Ex x (000)a Ex x (000)c Ess ( 21 21 21 ) Ex x ( 21 21 21 ) Ex y ( 21 21 21 ) Esx ( 21 21 21 )ac Esx ( 21 21 21 )ca Ess (110)a Esx (110)a Ex x (110)a Ex x (011)c

7.0012 7.2004 −0.6498 5.7192 0.6084 −0.5586 −1.2224 −0.6375 −1.8169 −0.3699 −0.5760 0.2813 −0.6500

7.3378 6.1030 0.4592 6.0433 0.4657 −0.5401 −1.4245 −0.4981 −1.8926 −0.2534 −0.8941 0.1453 −0.7912

9.1 Superlattices

533

Here we have to point out that some additional parameters are required to calculate the energy band structure of a superlattice such as GaAs/AlAs. The additional parameters to be determined are those of the atom at the interface (As atom in the case of GaAs/AlAs superlattice), which are usually approximated by the following method. 1. The parameters Esb , E pb and λb of the interface atom As are estimated from the average values of GaAs and AlAs. 2. The nearest-neighbor interaction between the interface atom As and the Ga atom or Al atom is approximated by the interaction in GaAs or AlAs, respectively. 3. The second nearest-neighbor interaction between the Ga atom and the Al atom is approximated by the average value of the Ga–Ga interaction in GaAs and the Al–Al interaction in AlAs. 4. The second nearest-neighbor interaction between the As atoms at the interface is approximated by the average value of the second nearest-neighbor interaction in GaAs and AlAs. The second nearest-neighbor interaction between the interface atom As and the As atom in GaAs or AlAs is approximated by the interaction in GaAs and AlAs. These approximations will give a good result when the parameters associated with the As atoms of GaAs and AlAs are almost the same. Lu and Sham [5] have reported that such approximations will not introduce a considerable effect in the case of n > 3. In addition, the approximations are essential for the wave functions which are required to satisfy their symmetry [43]. Using the parameters estimated from these assumptions and those reported by Lu and Sham [5], and assuming the valence band discontinuity Ev = 0.55 eV, the energy band structures of (GaAs)n /(AlAs)n are calculated. Typical examples of the energy band structures are shown in Figs. 9.12, 9.13, 9.14 and 9.15 for superlattices of n = 1, 3, 8 and 12. In Fig. 9.16 the transition energies of (GaAs)n /(AlAs)n superlattices as a function of the atomic layer number n calculated from the second nearest-neighbor sp 3 tight binding approximation, along with the experimental data, where the experimental data are the same as those shown in Fig. 9.11, which are obtained from photoreflectance (PR) and photoluminescence (PL) experiments. It is found from the calculated results that the lowest transition energy is associated with a quasi-direct transition involving the X z conduction band for n < 12 except n = 1. In addition, we find that the conduction band at the Z point (indirect band) lies almost at the same level as the X z conduction band for n = 3 . . . 12 and that the X z conduction band is lower than the X x y conduction band (M point) except for n = 1. These calculated results show good agreement with the calculations based on the effective mass approximation [44, 45], and indicate the importance of the effective mass anisotropy of the X valleys in AlAs. It should be noted that the lowest conduction band for n = 1 is the X x y conduction band located at the M point, but the results depend strongly on the parameters used. In addition, it seems to be almost impossible to grow a perfect superlattice of (GaAs)1 /(AlAs)1 and thus we are not able to determine conclusively the band structure of the superlattice for n = 1. Ge et al. [46] have reported experiments on PL, PLE (photoluminescence excitation spec-

534

9 Quantum Structures 2

Fig. 9.12 Energy band structure of the (GaAs)1 /(AlAs)1 superlattice calculated by the second nearest-neighbor sp 3 tight binding approximation

Fig. 9.13 Energy band structure of the (GaAs)3 /(AlAs)3 superlattice calculated by the second nearest-neighbor sp 3 tight binding approximation

tra) and PL under the application of pressure and explained the results as showing that the lowest conduction band is X x y for n < 3 and thus that the superlattices are the indirect transition type. In order to draw this conclusion we need to do accurate band structure calculations by taking into account the conduction band at the L point and by making a careful comparison between experiment and theory.

9.1 Superlattices

Fig. 9.14 Energy band structure of the (GaAs)8 /(AlAs)8 superlattice calculated by the second nearest-neighbor sp 3 tight binding approximation

Fig. 9.15 Energy band structure of the (GaAs)12 /(AlAs)12 superlattice calculated by the second nearest-neighbor sp 3 tight binding approximation

535

536

9 Quantum Structures 2

Fig. 9.16 Transition energies as a function of layer number n in the (GaAs)n /(AlAs)n superlattice calculated by the second nearest-neighbor sp 3 tight binding approximation. The solid and dashed curves are respectively the direct () and quasi-direct (X z ) transitions calculated by the second nearest-neighbor sp 3 tight binding approximation and the dot-dashed curve is the indirect transition energy associated with the M point. Experimental results for photoreflectance (PR) and photoluminescence (PL) are also shown for comparison. The theory indicates that the crossing between the direct allowed and quasi-direct transitions occurs at n = 12 and that the bottom of the X x y conduction band (M point) is higher that the bottom of the X z conduction band except for n = 1. The conduction band at the Z point (indirect band) lies at almost the same level as the X z conduction band for n = 3–12 (see [7])

Finally, we will discuss the contribution of the atomic orbitals to the band edges of superlattices. The eigenstates of the eigenvalues consist of the mixture of the atomic orbitals which give the measure of the contribution by the eigenstates. Therefore, the electron distribution in the unit cell is given by |λk|λk|2 =

|(nbj k|λk|2 ,

(9.30)

n

where n = s, px , p y and pz , b = a or c, and j indicates the atom position in the unit cell with j = 1 − 2(n + m). Figure 9.17a–c shows respectively the density distribution of the atomic orbitals at the top of the valence band (v ), at the bottom of the X z conduction band and at the bottom of the conduction band (c ) in the (GaAs)8 /(AlAs)8 superlattice. From the figure we find the following result. The top of the valence band (v ) dominated by the atomic orbitals in GaAs, the X z conduction band edge (X z is zone folded at the point) consists of the atomic orbitals in the AlAs layer, especially of the orbitals of the As atoms, and the c conduction band edge consists of the atomic orbitals in GaAs, mostly of As atom orbitals. From these considerations we find the contribution of the bands from the atomic orbitals, the

9.1 Superlattices

537

Fig. 9.17 Contribution of electrons from each atom in the superlattice (GaAs)8 /(AlAs)8 . The electron contribution is shown a the valence band (v ), where the valence band v is found to consist mostly of electrons in the Ga and As atoms, b the X z conduction band (the X is zone folded at the point), where the electrons of the Al atoms in AlAs mostly contribute to the zone-folded X z conduction band, and c the c conduction band, where the contribution of electrons from the As atoms in GaAs dominates

symmetry of the valence and conduction bands, and the contribution of the energy bands from the X point in AlAs and the point of GaAs. In addition, we find that the electron distributions satisfy the symmetry operation I C4 , indicating the correctness of the assumptions.

538

9 Quantum Structures 2

9.2 Quantum Dots In this section we present a good example of an artificial atom and discuss Coulomb interaction of electrons confined in a disk composed heterostructure GaAs/AlGaAs/ InGaAs.2 It was pointed out that electrons in a quantum dot with a good symmetry exhibit the shell structure of atoms and thus the electronic states reflect Hund’s rule [47–49]. From this reason such a quantum dot is called an artificial atom, in which electronic states are controlled by the unit of an electron. Here we summarize the experimental date of Tarucha et al. [49] and theoretical explanation of the observed results. Figure 9.18 shows the quantum dot structure used by Tarucha et al. [49], where double barrier tunnel structure is cut into a disk shape and the side gate confines electrons with its parabolic potential. First we disregard Coulomb interaction and show that the assumption fails in explaining typical features. Then we deal with many electron system by the method of diagonalization of the coupled N –electron Hamiltonian with Coulomb interaction.

9.2.1 Addition Energy Tarucha et al. used devices such as shown in Fig. 9.18, where the double barrier heterostructure (DBH) consists of an undoped 12.0 nm In0.05 Ga0.95 As and undoped Al0.22 Ga0.78 As barriers of thickness 9.0 (upper barrier) and 7.5 nm (lower barrier). Figure 9.19 shows the current flowing through the device as a function of the gate voltage under the drain bias of V = 150 µV, where we see clear Coulomb oscillations for Vg > −1.6 V with each peak corresponding to a change of exactly one electron in the dot. The spacing between the current peaks in Fig. 9.19 reflects the energy

Fig. 9.18 Quantum dot structure used by Tarucha et al. [49] for the investigation of Coulomb oscillations and addition energy versus electron number. Electrons are confined in the z direction by the double barrier heterostructure AlGaAs/In0.05 Ga0.95 As/AlGaAs and then the side gate confines electrons in the (x, y) plane, forming quantum dot disk 2

This section is based on the Ph.D Thesis (in Japanese) by Tatsuya Ezaki, submitted to Osaka University (1997).

9.2 Quantum Dots

539

Fig. 9.19 Coulomb oscillations observed in the quantum dot of D = 0.5 µm shown in Fig. 9.18, where the current through the dot is plotted as a function of the gate voltage under the drain voltage of Vd = 150 µV [49]

Fig. 9.20 Chemical potential difference versus electron number for two different dots with D = 0.5 and 0.44 µm. See text for the definition of the addition energy and the chemical potential difference [49]

Fig. 9.21 Relation between electronic state E N of N electrons, the chemical potential (addition energy) μ N and the chemical potential difference Δμ N are illustrated

required to add one more to a dot containing N electrons. The spacing at N = 2 and 3, N = 4 and 5, and N = 6 and 7 are larger than the other spacing, which means the difference in the addition energy defined by Δμ N below is higher at N = 2, 4, 6, . . . than the other spacing. Tarucha et al. estimated the chemical potential difference (difference in addition energy) from their experiments and plotted as a function of electron number in Fig. 9.20 for two different devices. Addition energy μ N and the chemical potential difference Δμ N are defined below, which are illustrated in Fig. 9.21. When we neglect Coulomb interaction, the energy E N of N electrons is given by summing up the energy levels ε j of the one–electron states, N εj . (9.31) EN = j=1

540

9 Quantum Structures 2

Then the addition energy (chemical potential) required for adding the N –th electron to the electronic state with N -1 electrons is define by μ N = E N − E N −1 = ε N .

(9.32)

In the presence of Coulomb interaction we have to calculate the total energy E N by taking account of many body effects, which will be discussed later. Figure 9.21 illustrates schematically, the electronic energies for N -1, N and N +1 electrons, the chemical potentials and the difference in chemical potential. The difference in the chemical potential Δμ N is given by Δμ N = μ N +1 − μ N .

(9.33)

In Fig. 9.20 we find that the chemical potential difference exhibits clear peaks at N = 2, 4, 6, and, 12. These features may be understood by investigating the filling of the shell structure. Let’s consider electronic states without Coulomb interaction, and then one electron Hamiltonian h 0 (r, s) in the presence of a magnetic field B is written as h 0 (r, s) =

1 ( p + e A)2 + V (x, y) + V (z) , 2m ∗

(9.34)

where r is the three dimensional coordinates and s is the spin coordinate. In the z direction the electrons in the disk are confined by the double barriers of the heterostructure as shown earlier. Here we are interested in the system of few electrons, and then the lowest subband is taken into account. In the (x, y) plane, the potential V (x, y) is produced by the depletion layer controlled by the gate voltage, and the shape is parabolic. For the purpose of the later discussion we express the potential defined by Ezaki et al. [50] and Ezaki [51], V (x, y) =

2 1 ∗ 2 2 m ωx x + ω2y y 2 1 + α cos(3φ) , 2 7

(9.35)

where ωx and ω y are the confinement potentials in the x and y directions, respectively, and α is introduced to modify the potential shapes as follows. When we put α = 0, we obtain a circular dot for ωx = ω y and an ellipsoidal disk for ωx = ω y , and a triangular dot for α = 1 and ωx = ω y . First we consider the simplest case of a circular dot, and put ωx = ω y = ω0 . Also note that ωL is the Larmor frequency and related to the cyclotron frequency by ωL = ωc /2. In the z direction we assume infinite barrier potentials with the well width W , and thus ζ (z) =

π 2 sin z . W W

(9.36)

9.2 Quantum Dots

541

Since the system is symmetrical in the (x, y) plane, we use the polar coordinate (ρ, φ), and then we may write the wave function of the electron in the disk as

2! 1 ρ 2 exp − (|m| + n)! 2 l0 |m| ρ ρ × L |m| ϕm (φ)ζ (z) , n l0 l0 1 ϕm (φ) = √ e−imφ , 2π , l0 = m∗ 2 = ω02 + ωL ,

1 ψmn (ρ, φ, z) = l0

ωL =

eB , 2m ∗

(9.37a) (9.37b) (9.37c) (9.37d) (9.37e)

|m|

where L n is the generalized Laguerre polynomial. The energy of one–electron state is (9.38) εmn = (2n + |m| + 1) − mωL + εz , where εz is the ground subband energy of electrons confined in the z direction. The potentials for elliptic and triangular shapes are also expressed as follows for the purpose to expand the electronic states by Slater determinant. In the case of elliptic potential V (ρ, φ) =

1 ∗ 2 2 1 ∗ 2 m ω ρ + m ωx − ω2y ρ 2 cos(2φ) , 2 4

(9.39a)

ω=

(9.39b)

ωx2 + ω2y 2

,

and for the triangular potential V (ρ, φ) =

1 ∗ 2 2 1 ∗ 2 2 m ω0 ρ + m ω0 ρ cos(3φ) . 2 7

(9.39c)

In order to understand the peaks of the chemical potential difference in Fig. 9.20, we first deal with the case of no Coulomb interaction in a circular disk. Then the one–electron energy is given by εmn = ω0 (2n + |m| + 1)

(+εz ) .

(9.40)

542

9 Quantum Structures 2

Fig. 9.22 Electronic states in a circular disk with parabolic confinement potential. The lower left figure shows the quantized energy levels with equal spacing ω0 and several energy states are shown by the quantum number (n, m) in the lower right figure. The upper right figure shows the filling of 9 electrons with spin up and down, where the Coulomb interaction is neglected

Fig. 9.23 Shell structure is shown, where the energy is given by εnm = ω0 (2n + |m| + 1). The filled shells are illustrated with the spin orientations. From this figure the chemical potential difference without Coulomb interaction in a circular disk is easily deduced, which is shown in Fig. 9.24

Therefore the electronic states are well expressed by the quantum number (n, m). The lower states are then expressed by (n, m) = (0, 0), (0, ±1), (0, ±2), (1, 0), (0, ±3), (1, ±1), . . ., which are illustrated in Fig. 9.22. In Fig. 9.23 such a shell filling is represented by using an atomic orbital model. We may easily evaluate the difference in addition energies Δμ N as shown in Fig. 9.24, where we find the peaks with the height of ω0 at N = 2, 4, and 6. Therefore the peaks found by Tarucha et al. shown in Fig. 9.20 are qualitatively explained. In order to explain the detailed features of Fig. 9.20, however, we have to take into account the Coulomb interaction of N electrons in a disk.

9.2 Quantum Dots

543

Fig. 9.24 The shell structure of the electronic states in a circular disk and the chemical potential difference is plotted as a function of electron number, where the Coulomb interaction is neglected

9.2.2 Exact Diagonalization Method It is well known that the electron–electron interaction plays an important role in many electron system and that the energy eigenstates derived for a single electron Hamiltonian fail in explaining various aspect of the observed features. In 9.2.1 such a single electron approximation fails in quantitative explanation of the experimental data on the chemical potential change in a quantum dot. In order to analyze a many electron system with including Coulomb interaction, we have to use many electron wave functions. We know that Slater determinant describes the properties of fermion system, which is written for N electrons as χ1 (x 1 ) χ2 (x 1 ) χ1 (x 2 ) χ2 (x 2 ) 1, 2, · · · , N = √1 .. .. N ! . . χ1 (x N ) χ2 (x N )

· · · χ N (x 1 ) · · · χ N (x 2 ) , .. .. . . · · · χ N (x N )

(9.41)

where x i denotes the Cartesian coordinates r i plus spin coordinates for electron i and is equivalently expressed as χi (x i ) = ψi (r i )|α or χi (x i ) = ψi (r i )|β with one–electron eigenfunction ψi (r i ) and spin functions |α and |β. One–electron eigenfunction ψi (r) is given by h 0 (r)ψi (r) = εi ψi (r) ,

(9.42)

where h 0 (r) is one–electron Hamiltonian and εi is the eigenenergy. Using the solutions of one–electron Hamiltonian h 0 (x), we rewrite the eigenfunction as ψiσ (x) and the eigenenergy as εiσ , where we introduced spin quantum number σ . Then the second quantized Hamiltonian is written as H0 =

iσ

† εiσ Ciσ Ciσ ,

(9.43)

544

9 Quantum Structures 2

where i is the quantum number for the spatial part of wave function and σ is the † and Ciσ represent the creation and annihilation operators spin quantum number. Ciσ of the electron state iσ , respectively. When 2 or more electrons are contained in a quantum dot, we have to take into account of the electron–electron interactions, among which Coulomb interaction plays the most important role. The Hamiltonian with Coulomb interaction is written as 1 u i j ji Ci† σ C †j σ C jσ Ciσ , 2 i j ji σ σ

(9.44a)

ψi∗ (r 1 )ψ ∗j (r 2 )u(r 1 − r 2 )ψ j (r 2 )ψi (r 1 ) d r 1 d r 2 ,

(9.44b)

HC = u i j ji =

u(r 1 − r 2 ) =

e2 . 4π |r 1 − r 2 |

(9.44c)

Then the total Hamiltonian is given by H=

† εiσ Ciσ Ciσ +

iσ

1 u i j ji Ci† σ C †j σ C jσ Ciσ . 2 i j ji σ σ

(9.45)

The wave function | of N electrons in a quantum dot is expressed by a linear combination of the orthonormal system |I (a linear combination of Slater determinants) d I |I . (9.46) | = I

In this book the basis function of N electrons is given by |I = |n λ1 , n λ2 , · · · , n λk , · · · = Cλ†N Cλ†N −1 Cλ†1 |0 ,

n λi = 1, (i = 1, 2, · · · , N ) n λj = 0, (λj = λi )

(9.47a) (9.47b)

where λ1 < λ2 < · · · < λ N and |0 is the vacuum state. Using the orthonormal system of N particles |I we may solve the Hamiltonian matrix H I J = I |H|J = I |H0 + HC |J and obtain the many particle states exactly.

9.2 Quantum Dots

545

9.2.3 Hamiltonian for Electrons in a Quantum Dot As described in 9.2.2, Hamiltonian for interacting electrons is given by H=

† εiσ Ciσ Ciσ +

iσ

1 u i j ji Ci† σ C †j σ C jσ Ciσ , 2 i j ji σ σ

(9.48)

where the second term on the right hand side is the energy of Coulomb interaction. Here we will expand the states of N electrons in terms of orthonormal sets, which is done by using Slater determinant of N electrons. We compose Slater determinant of N electrons by the wave functions of (9.37e) obtained for one–electron solutions confined in the two dimensional simple harmonic type potential (ωx = ω y = ω0 ) in the plane parallel to the hetero–interfaces and in the infinite potentials perpendicular to the hetero–interfaces (z direction). In the later section we mention the results on the disks with elliptic and triangular potentials. For this purpose we divide the potentials into two terms, circularly symmetric and asymmetric parts, which are given for the elliptic potential V (ρ, φ) =

1 ∗ 2 2 1 ∗ 2 m ω ρ + m (ωx − ω2y )ρ 2 cos 2φ , 2 4 ωx2 + ω2y

ω=

2

,

(9.49a) (9.49b)

and for the triangular potential V (ρ, φ) =

1 ∗ 2 2 1 ∗ 2 2 m ω0 ρ + m ω0 ρ cos 3φ . 2 7

(9.50)

Expressing the asymmetric part of the potential by V (r), Hamiltonian of N electrons is given by H=

iσ

† εiσ Ciσ Ciσ +

i i

σ

vi i Ci† σ Ciσ

1 + u i j ji Ci† σ C †j σ C jσ Ciσ , (9.51a) 2 i j ji σ σ u i j ji = ψi∗ (r 1 )ψ ∗j (r 2 )u(r 1 − r 2 )ψ j (r 2 )ψi (r 1 ) d3 r 1 d3 r 2 , (9.51b) vi i = ψi∗ (r)V (r)ψi (r) d3 r , (9.51c) where Fourier expansion of the Coulomb interaction is written as

546

9 Quantum Structures 2

u(r 1 − r 2 ) =

e2 ei Q·(ρ 1 −ρ 2 ) e−Q|z1 −z2 | . 2 Q Q

(9.52)

Inserting the one–electron wave functions of (9.37e) into (9.51b), we obtain u i j ji

e2 = 4π

0

∞

F(Q)gi i (Q)g ∗j j (Q) dQ × δm i +m j ,m i +m j , ∞ ψi∗ (ρ)ψi (ρ)Jm i −m i (Qρ)ρ dρ ,

(9.53a)

gi i (Q) = i m i −m i (9.53b) 0 F(Q) = |ξ(z 1 )|2 |ξ(z 2 )|2 e−Q|z1 −z2 | dz 1 dz 2 3 (2π )2 (2π )4 2 −x x+ − 2 2 (1 − e ) (9.53c) = 2 x + (2π )2 2 x x (x + (2π )2 ) x = QW , where Jn (x) is Bessel function and δm i +m j ,m i +m j of (9.53a) represents the momentum conservation rule. The asymmetric part of the elliptic confinement potential V (r) is written by using (9.49a) and (9.50) as V (r) =

1 ∗ 2 m (ωx − ω2y )ρ 2 cos 2φ , 4

(9.54)

and inserting it into (9.51c) we obtain the matrix element of the asymmetric potential vi i =

1 ∗ 2 m (ωx − ω2y ) 8

ψi∗ (ρ)ψi (ρ)ρ 3 dρ × (δm ,m+2 + δm ,m−2 ) .

(9.55)

In the case of the triangular confinement potential, the asymmetric part is V (r) =

1 ∗ 2 2 m ω0 ρ cos 3φ , 7

(9.56)

and inserting it into (9.51c) we obtain the matrix element of the asymmetric part of potential vi i vi i =

1 ∗ 2 m ω0 14

ψi∗ (ρ)ψi (ρ)ρ 3 dρ × (δm ,m+3 + δm ,m−3 ).

(9.57)

In the following analysis we use a quantum dot model shown in Fig. 9.25, where the dot is formed by AlGaAs/In0.05 Ga0.95 As/AlGaAs double heterostructure and constriction in the (x, y) plane. The double heterostructure confines electrons in the z direction with the well width W . The bird’s–eye–view of the model potential in the (x, y) plane is calculated from (9.35) and plotted in Fig. 9.26 for the ellipsoidal

9.2 Quantum Dots

547

Fig. 9.25 A model of a quantum dot used for the analysis. The dot is formed by AlGaAs/InGaAs/ AlGaAs double heterostructure and constricted in the (x, y) plane by etching and gate voltage [50]

Fig. 9.26 Elliptic confining potential in the (x, y) plane sandwiched by the double heterostructure. The potential is calculated by putting α = 0 and ωx = ω y in (9.35). When we put ωx = ω y , we obtain the circular confining potential [50]

Fig. 9.27 Triangular confining potential in the (x, y) plane sandwiched by the double heterostructure. The potential is calculated by putting α = 1 and ωx = ω y in (9.35) [50]

potential and in Fig. 9.27 for the triangular potential, where the equi–energy lines are shown. The elliptic potential is obtained by putting α = 0 and ωx = ω y in (9.35) and the circular potential is obtained by putting ωx = ω y . The triangular potential is shown in Fig. 9.27, where we put α = 1 and ωx = ω y in (9.35).

9.2.4 Diagonalization of N Electrons Hamiltonian Matrix The wave function | of N electrons is expressed by a linear combination of the orthonormal system, in other words N particle Slater determinant |I given by (9.46), | =

I

d I |I .

(9.58)

548

9 Quantum Structures 2

Here we define the difference |I − J | between Slater determinants of N electrons |I and |J by the number of the different pairs of one–electron states. |I = |m 1 , m 2 , · · · , m k , · · · ,

(9.59)

|J = |n 1 , n 2 , · · · , n k , · · · .

(9.60)

Using the above expressions we find the following results. When m i = n i ( i = 1, 2, · · · ) and thus |I = |J , we obtain |I − J | = 0. When n p –th and n q –th one electron states of |I and |J are interchanged, for example, np

nq

np

|I = | · · · , 1 p , · · · , 0q , · · · ,

nq

|J = | · · · , 0 p , · · · , 1q , · · · ,

(9.61)

we obtain |I − J | = 1. For the purpose of further calculations we classify the matrix elements of N electrons Hamiltonian HI J = I |H|J = I |H0 + V + HC |J into the following four cases by using the difference between Slater determinants |I − J |. 1. |I − J | = 0 (diagonal elements) I |H0 |J =

N

ελi ,

(9.62a)

vλ i λi ,

(9.62b)

i=1

I |V |J =

N i=1

I |HC |J =

N −1 N

u λi λ j λ j λi , −u λi λ j λi λ j δσλi σλ j

.

(9.62c)

i=1 j=i+1

2. |I − J | = 1

np

nq

np

nq

|I = | · · · , 1 p , · · · , 0q , · · · , |J = | · · · , 0 p , · · · , 1q , · · · ,

I |H0 |J = 0 , I |V |J = (−1)n p +nq vq p δσ p σq , I |HC |J = (−1)n p +nq

(9.63a)

(9.63b) (9.63c)

N u qλi λi p δσ p σq − u λi qλi p δσq σλi .

(9.63d)

i=1

3. |I − J | = 2 np

nr

nq

ns

np

nr

nq

ns

|I = | · · · , 1 p , · · · , 0r , · · · , 1q , · · · , 0s , · · · , |J = | · · · , 0 p , · · · , 1r , · · · , 0q , · · · , 1s , · · · ,

(9.64a)

9.2 Quantum Dots

549

I |H0 |J = I |V |J = 0 , I |HC |J = (−1)

4. |I − J | ≥ 3

(9.64b)

n p +n q +nr +n s

× u r sq p δσ p σr δσq σs − u srq p δσ p σs δσq σs .

I |H0 |J = I |V |J = I |HC |J = 0 .

(9.64c)

(9.65)

9.2.5 Electronic States in Quantum Dots Here we will show the results calculated by means of the exact diagonalization. The parameters of In0.05 Ga0.95 As such as the effective mass and dielectric constants are estimated by extrapolating the parameters of InAs and GaAs, and we use the effective mass m ∗ = 0.065m 0 and the dielectric constant = 12.90 . The confinement potential is determined so that the average value of ωx and ω y remains constant and we set (ωx + ω y )/2 = ω0 = 3 [meV]. The well width in the z direction is assumed to be W = 12 [nm]. Slater determinant is composed by 20 one–electron states from the lowest ground state to upper 20–th states. The separation of the energy levels between the ground state and the first excited state levels due to the confinement by the heterobarriers in the z direction estimated from (9.36) is 121 [meV], while the energy difference between the ground state and the 20–th state is 9 [meV]. Therefore we consider only the ground state in the z direction confinement. First we present a comparison between the calculated results by the exact diagonalization method and the experimental data of Tarucha et al. for a circular quantum dot. Figure 9.28 shows the chemical potential difference Δμ N = μ N +1 − μ N as a function of electron number N , where the calculated results are shown by ◦ and the experimental data of Tarucha et al. [49] by •. Here we note again that the chemical potential μ N of a quantum dot with N electrons is defined by μ N ≡ E N +1 − E N where

Fig. 9.28 The chemical potential difference Δμ N = μ N +1 − μ N calculated by the exact diagonalization method (◦) versus electron number N in a circular dot is compared with the experimental data (•) of Tarucha et al. [49]. In the calculation the confinement potential by the heterointerfaces is assumed to be ω0 = 3 meV

550

9 Quantum Structures 2

the ground state energy of the quantum dot with N electrons is given by E N . Therefore the chemical potential difference Δμ N is the energy required to add another 1 electron to the dot and thus called charging energy. A state of a large chemical potential difference Δμ N corresponds to a state with more stable energy. In Fig. 9.28 we find that the chemical potential difference Δμ N exhibits a large value for electron number N = 2 and 6, and thus the states are more stable. This feature may be easily understood from the results shown in Figs. 9.23 and 9.24, where the shell structure is calculated in the case of no–Coulomb interaction or one–electron approximation. As given by (9.40) the one–electron energy states are expressed by the quantum number (m, n) or εmn = ω0 (2n + |m| + 1), and thus the energy is degenerate by the factor 2(2n + |m| + 1) with the spin degeneracy 2. A circular quantum dot with electrons N = 2, 6, 12, · · · exhibits closed shell structures, and the energy states become stable, resulting in a large chemical potential difference Δμ N . In addition to N = 2 and N = 6, we find weak peaks at N = 4 and N = 9. These two peaks are stable a little and interpreted in the following way. Let’s consider the case of N = 4 electrons. Two of them will occupy the lowest state and the other 2 electrons will occupy a half of the states of 2n + |m| = 1, resulting in a half–filled shell structure. The exact diagonalization shows that the spin triplet state of the total spins S = (Sz = 0, ±) is the ground state. The outer shell in the quantum dot with N = 4 electrons contains 2 electrons with the same spin orientation. This may be explained in terms of Pauli’s exclusion principle as follows. Since the 2 electrons with the parallel spins of the outer–shell keep away due to Pauli’s exclusion principle, and thus the Coulomb energy becomes smaller, resulting in a stable state of the spin– triplet state S = (Sz = 0, ±). When the quantum dot contains 9 electrons, the ground state is formed by the spin quadruplet state with the total spins S = 3/2 (Sz = ±/2, ±3/2) and a more stable state is achieved. We know that the atomic states obey Hund’s rule. From the exact diagonalization method, a ground state of an incomplete shell in a quantum dot is formed so that the total spin becomes a maximum and thus quantum dot states also obey Hund’s rule [50, 51].

9.2.6 Quantum Dot States in Magnetic Field When a magnetic field is applied in the z direction, the one–electron energy levels of a quantum dot are given by (9.38), which are shown in Fig. 9.29a. Since each state is doubly degenerate with respect to spin, total number of the electrons filling the levels at B = 0 is N = (0), 2, 6, 12, 20, · · · as discussed before. The degenerate energy states with the same value n at B = 0 split into several levels at B = 0 and the energy level with the angular momentum parallel to the magnetic field (m > 0 becomes the lowest). Such a simple feature is dramatically changed when we take Coulomb interaction into account. Here we present the results calculated by the exact diagonalization method for electrons N = 4 in Fig. 9.29b, where the quantum dot model is the same as the circular dot used for the results of B = 0 and the calculated energy levels are plotted as a function of magnetic Field B. In Fig. 9.29b, •, and ◦ are the states with the total angular momentum 0, ± and ±2, respectively. Δ

9.2 Quantum Dots

551

Fig. 9.29 a One–electron states of a quantum dot in magnetic field, where the states are doubly degenerate with respect to spins. The state with the angular momentum parallel to the magnetic field (m is positive) is lower than the other states with the same n. b Energy states in a circular dot with 4 electrons calculated by exact diagonalization method, where •, and ◦ are the states with the total angular momentum 0, ± and ±2, respectively. Δ is the energy difference between the singlet and triplet states due to the exchange interaction. The ground state energy of the spin triplet S = 1 with the total angular momentum M = 0 increases with the magnetic field, while the singlet state S = 0 with total angular momentum M = 2 decreases, and the transition of the ground state occurs at B ≈ 0.25 [T]

is the energy difference between the singlet and triplet states due to the exchange interaction, which is estimated to be Δ = 0.44 [meV]. The ground state energy of the spin triplet S = 1 with the total angular momentum M = 0 increases with the magnetic field, while the singlet state S = 0 with total angular momentum M = 2 decreases, and the transition of the ground state occurs at B ≈ 0.25 [T]. It is also shown by the exact diagonalization that transition of the ground state for electrons N = 5 occurs from the state of the total angular momentum M = 1 to the state M =4 at B ≈ 0.6 [T].

9.2.7 Electronic States in Elliptic and Triangular Quantum Dots As described before we may expect the chemical potential difference depends on the structure of quantum dots, and therefore it is very interesting to show the calculated results on elliptic and triangular quantum dots. In Fig.refDmuNspselliptic the chemical potential difference is shown as a function of electron number N in the two different elliptic dots with (ωx , ω y ) = (2.5 meV, 3.5 meV) and (ωx , ω y ) = (2 meV, 4 meV) by and , respectively, where the data of • are the chemical potential difference in a circular quantum dot with ωx = ω y = 3 meV. The well width in the z direction is the same for the above three quantum dots and W = 12nm.

552

9 Quantum Structures 2

Fig. 9.30 Calculated chemical potential difference Δμ N in two kinds of elliptic dots compared with the results of a circular dot. and ◦ are the results for the elliptic dots with the confinement potentials in x and y directions (ωx , ω y ) = (2.5 meV, 3.5 meV) and (2 meV, 4 meV), respectively. The results for the circular dot of ω0 = 3 meV are shown by • for comparison [50]

Fig. 9.31 Calculated electron distributions for N = 4 in a the circular dot (ω0 = 3 meV) and b the elliptic dot (ωx , ω y ) = (2 meV, = 4 meV), where 0 = 20nm

We find in Fig. 9.30 that peaks except N = 6 are not well resolved compared to the case of the circular dot. This feature is explained in terms that the degeneracy of one–electron states is removed due to the weakened symmetry in elliptic quantum dots, resulting in orbits of mixed angular momentum. The electron distributions of (a) the circular and (b) elliptic dots in the (x, y) plane calculated by the exact diagonalization method are shown in Fig. 9.31, where 4 electrons are contained in the circular dot (a) of ω0 = 3 meV and in the elliptic dot (b) of (ωx , ω y ) = (2 meV, 4 meV). As seen in Fig. 9.31a the electron distribution in the circular dot is symmetric in the plane, while (b) in the elliptic dot the electron distribution has double peaks along the long axis. For comparison, calculated results of the chemical potential difference for a triangular dot (•) with ω0 = 3 meV are shown together with the results for a circular dot () in Fig. 9.32. We find no significant difference between the two dots in Fig. 9.32. Here we have to note that the corners of the potential of the triangular dot used in

9.2 Quantum Dots

553

Fig. 9.32 Calculated chemical potential difference Δμ N in a triangular dot is plotted as a function of electron number N , where the confinement potential is assumed to be ω0 = 3 meV. Calculated results for the circular dot (Fig. 9.28) are shown for comparison. and • are the results for the triangular dot and the circular dot

the calculations is smoothed, resulting in a small change in the chemical potential difference compared to the circular dot. However, we find that the states for electrons N = 3, 6 and 9 are stable a little compared to the circular dot. This feature may be explained in terms of the electron distribution shown in Fig. 9.33, where the results for N = 3 are shown in Fig. 9.33a for the circular dot and in Fig. 9.33b for the triangular dot. The electron distribution of the circular dot in Fig. 9.33a is symmetric but the central part of the distribution is low due to the Coulomb repulsion. In the triangular dot, on the contrarily, each electron occupies the corner as shown in Fig. 9.33b, resulting in a little bit stable states for electrons 3, 6 and 9.

Fig. 9.33 A comparison of the electron wave function distribution for electrons N = 3 in a circular dot (left curve) and in a triangular dot (right curve), where,0 = 20nm

554

9 Quantum Structures 2

9.3 Coulomb Blockade and Single Electron Transistor The semiconductor devices in common use utilize many electrons in each device. For example, 1011 to 1012 electrons exist in the 1 cm2 area of a typical MOSFET device, and thus in a MOSFET with an area as small as 1 µm × 1 µm 103 –104 electrons are involved in the device operation. If device fabrication technology continues to advance and a device size below 0.1 µm becomes possible, then the number of electrons involved in the operation decreases and in the limit a device operated by a single electron will be achieved in the future. However, it is expected that new devices based on operating principles different from those in present devices may be developed, where single or several electrons take part in the device operation. Research projects on new functional devices with few electrons are in progress. The most important principle for such devices is believed to be the Coulomb blockade [52, 53]. In this section the basic principle of the Coulomb blockade will be described [54–56]. First, consider the tunnel junction shown in Fig. 9.34. The energy stored in the junction is given by Q2 . (9.66) U= 2C In the presence of a bias voltage V , an electron at the source electrode with kinetic energy Es (k) will tunnel into the state at the drain electrode with kinetic energy Ed (k ), and thus we find the following relation: 1 (C V − e)2 Es (k) + C V 2 = Ed (k ) + . 2 2C

(9.67)

Since the electron tunneling through the junction has to satisfy the Pauli exclusion principle the following inequalities are required.

Fig. 9.34 Schematic illustration of a tunnel junction biased by a voltage V . The lower part shows its equivalent circuit

9.3 Coulomb Blockade and Single Electron Transistor

555

Fig. 9.35 A finite energy is required for an electron to tunnel through the junction and in the limit of temperature T = 0 no electron current flows at the bias voltage below V = e/2 C. This bias region is called the Coulomb gap

This will lead to

Es (k) < EF − kB T , Ed (k ) > EF + kB T .

(9.68)

Ed (k ) − Es (k) > 2kB T .

(9.69)

Therefore, the tunneling condition is given by eV ≥

e2 − 2kB T , 2C

(9.70)

and no current flows at a bias below a threshold voltage which depends on the temperature. At T = 0, no current results below V = e/2 C. This bias region is called the Coulomb gap and the tunneling characteristics of the Coulomb gap are schematically illustrated in Fig. 9.35. The prohibition of tunneling is called the Coulomb blockade. We discuss the Coulomb blockade phenomenon in a little more detail by investigating the change in the electrostatic energy at the tunnel junction shown in Fig. 9.34. Letting the electrostatic capacitance of a small junction be C, we calculate the change in the electrostatic energy due to the tunneling of an electron. In this system the change in electrostatic energy before and after the tunneling is estimated to be of the order of the Coulomb energy of an electron given by EC =

e2 . 2C

This energy is quite small in a junction of macroscopic size and thus the energy is washed by the thermal noise, making detection impossible. However, in a tunneling junction with an area of 0.01 µm2 with an insulating film of 1 nm thickness, the energy

556

9 Quantum Structures 2

becomes equivalent to temperature of about 1 K. Therefore, if the temperature of the tunnel junction is kept below 1 K, it is expected that the tunneling probability will be controlled by the Coulomb energy EC . When charges of ±Q are stored at the junction surfaces, the electrostatic energy of this system is given by Q 2 /2 C. Let us consider the case where an electron tunnels from the negative electrode to the positive electrode in this system. The charges at the positive and negative electrodes will therefore be changed to ±(Q − e). The change in the electrostatic energy before and after the tunneling is then given by E =

Q2 e e (Q − e)2 − = − Q = EC − eV , 2C 2C C 2

(9.71)

where the final relation is rewritten by using the voltage applied to the junction V = Q/C. This result tells us the following fact. When an electron tunnels in the system, the system loses its own Coulomb energy EC and receives energy eV from the voltage source. Therefore, the tunneling condition for an electron in this system is such that the voltage applied to the junction has to satisfy V > EC /e. In other words, under the condition EC , (9.72) V < e and at low temperatures such that kB T EC , the electron is not allowed to tunnel through the junction. In a similar fashion, the change in the charges due to the tunneling of an electron from the positive electrode to the negative electrode is given by ±(Q + e) and thus the change in the electrostatic energy is shown to be E =

Q2 (Q + e)2 − = eV + EC . 2C 2C

(9.73)

Therefore, for an applied bias voltage such that −

EC 0, electron tunneling is not allowed. Assume that there are n excess electrons and thus −ne charges in the Coulomb island. Four tunneling processes, t1 , t2 , t3 and t4 , are possible, as shown in Fig. 9.36, where an electron is added to or removed from the n electrons due to the tunneling. We define the change in the electrostatic energy due to the four tunneling processes by E1 , . . . , E4 . When all of them are positive, tunneling is forbidden and the number of electrons in the Coulomb island is unchanged, giving rise to zero electron current. For example, the change in electrostatic energy E1 due to the tunneling process t1 is given by e C 1 V − CG VG − e n + , C 2 2 C = 2C + CG ,

E1 =

(9.75) (9.76)

where C is the total electrostatic capacitance seen from the Coulomb island. In a similar fashion, E2 , E3 and E4 are also calculated, and the results are given by (9.75) by replacing the last term on the right–hand side with one of the terms ±(n ± 1/2). Equation (9.75) is plotted in Fig. 9.37a with horizontal axis CG VG and vertical axis C V , where the hatched region satisfies E1 > 0 and tunneling is forbidden. The region where all the four tunneling processes are forbidden is shown by the hatched diamonds in Fig. 9.37b. This region is called the Coulomb diamond.

558

9 Quantum Structures 2

Fig. 9.37 Operating characteristics of the single electron transistor circuit shown in Fig. 9.36. a The hatched region indicates the condition under which the tunneling process t1 does not occur, where n electrons exist in the Coulomb island shown in Fig. 9.36. b The hatched region shows the condition under which any of the tunneling processes t1 , t2 , t3 and t4 will not occur. c Condition for no tunneling is shown by the hatched region for different values of the number n

Fig. 9.38 SET characteristics when the source and drain currents are controlled by the gate voltage VG . Keeping source– drain voltage constant and changing the gate voltage VG , the characteristics pass through the forbidden and allowed tunneling regions alternately. When the gate voltage VG passes through the region without hatching, the tunneling current and source–drain current flow as shown in the lower part of the figure

When the number of electrons n is not fixed, we find the region for forbidden tunneling for different n as shown in Fig. 9.37c. Next, we discuss the tunneling current in the SET device. Keeping the voltage applied to the source–drain electrodes constant and changing the gate voltage VG , the SET characteristics pass through along the dotted line in Fig. 9.38 and thus pass through the diamond of forbidden tunneling and outside the diamond, allowing tunneling, alternately. Therefore, the source–drain current flows periodically as shown in the lower part of Fig. 9.38. It is therefore evident from Fig. 9.38 that the change in the electronic charge at the gate electrode is less than e, the charge of one electron. It means that the device is operated by a charge of less than a single electron. The term “single electron transistor” (SET) was named after the fact that such a circuit consisting of tunneling junctions is operated by controlling the source–drain current by the gate voltage, and the device characteristics are comparable to those of the MOSFET and MESFET. In order to apply the Coulomb blockade effect to a real device operated at a temperature near 300 K, e2 /2 C is required to be larger than kB T and thus we have to

9.4 Surface modulation of Two-dimensional Electron Gas and Weiss Oscillation

559

achieve a device with very small capacitance. At T = 300 K, the capacitance should be C ≤ 3.1 × 10−18 F = 3.1 aF. It may be possible to fabricate a device of this size by using microfabrication technology, but its large scale integration seems to be impossible. This is because in such a small device the noise, radiation hardness, reproducibility and uniformity of large scale integration pose very serious problems for fabrication process. There have been reported so far various types of SET circuits and related functional devices, but most of them are concerned with the investigation of the physical properties of the devices. Recently several important results for SET devices have been reported. Transistors operated by a single electron have been fabricated and the device operation has been confirmed by observing the Coulomb blockade phenomenon at room temperature [57–61]. In addition Yano et al. have succeeded in fabricating very small MOSFETs by using poly Si and in observing SET characteristics by charging and discharging one electron at a trap near the channel, resulting in a change in the threshold voltage. They have integrated SETs and fabricated SET memories [62].

9.4 Surface modulation of Two-dimensional Electron Gas and Weiss Oscillation As discussed in Sect. 8.5 (two-dimensional electron gas) exhibits clear Shubnikov– de Haas (SdH) oscillations in ρx x periodic in inverse magnetic field 1/B and Quantum Hall plateaus in Hall resistance ρx y . When surface of a heterostructure with confined 2DEG is modulated by a laser illumination or a periodic lattice by lithographic processing, the transport of 2DEG is affected by the modulated surface potentials, resulting in Weiss oscillations. The first observation of the Weiss oscillation in AlGaAs/GaAs heterostructure was carried out by D. Weiss, K. von Klitzing, K. Ploog, and G. Weimann in 1989 [63], and followed by Gerhardt et al. [64] and Weiss et al. [65]. They introduced a lateral periodic potential modulation in one direction formed by a well-defined fringe pattern of two laser beams at low temperature, which gives rise to the persistent excited positive charges in AlGaAs layer. 2DEG sheet density increases to Ns = 3.16 × 1011 c˙ m−2 from the dark value Ns = 2.35 × 1011 c˙ m−2 and the electron mobility is μ = 1.3 × 106 c˙ m2 /(V·s). The period of the modulation is determined to be a = 382 nm. The shape of the sample used by them are shown in the inset of Fig. 9.39. Figure 9.39 shows the measured magnetoresistance curves for current perpendicular (ρ⊥ , red curve) and parallel (ρ , green curve) due to the interference fringes in low magnetic field region. Shubnikov–de Haas oscillations and Quantum Hall effect plateaus disappear in the low magnetic field, but new oscillations in ρ⊥ come out instead with a periodicity and a weaker oscillations in ρ with wavelength by 2π/kF which is related 180◦ phase shifted from ρ⊥ . Define the Fermi √ to the 2DEG sheet density Ns by kF = 2π Ns (see (8.182) and its definition), and the observed extrema of ρ⊥ appear at the magnetic field Bλ

560

9 Quantum Structures 2

Fig. 9.39 Magnetoresistance curves for current perpendicular (ρ⊥ , red curve) and parallel (ρ , green curve) due to the interference fringes, as shown in the inset (redrawn from the figures of Gerhardt et al. [64]

1 ea = (λ + φ), Bλ 2kF

(9.77)

where φ = −0.25 ± 0.06) for the minima and φ = +0.17 ± 0.06 for the maxima. It should be noted that new magnetoresistance oscillations below 1 T seems to suppress the SdH oscillations and no additional structure appears in the Hall resistance (QHE). These new oscillations are called as “Weiss oscillations” after his discovery. Different structures of gated superlattice array are reported by Beton et al. [66] and Winkler et al. [67]. The above Weiss oscillations observed in surface modulated 2DEG is analyzed by Gerhardt et al. [64] by using a harmonic modulated potential V (x) = V0 cos(K x), K = 2π/a.

(9.78)

Putting the potential to 2DEG Hamiltonian, the eigen values are given by the perturbed term with Laguerre polynomial in addition to the Landau level energies, and the density of states√is peaked under √ the condition (flat-band energies) for the cyclotron radius Rn = l 2n + 1 (l = /eBz for the ground state and called “magnetic length”, and n is the Landau level index) Rnλ

1 a λ− , λ = 1, 2, 3. . . . . = 2 4

(9.79)

When we use the classical cyclotron orbit with cyclotron angular frequency ωc = eB/m ∗ , cyclotron radius Rc = vF /ωc , and Fermi velocity vF = kF /m ∗ , the relation (9.79) reduces to (9.77). The Weiss oscillations appear more clearly in the heterostructures with antidots arrays on the surface [68, 69]. Figure 9.40a shows an example how to fabricate

9.4 Surface modulation of Two-dimensional Electron Gas and Weiss Oscillation

561

Fig. 9.40 a Schematic illustration of antidot array fabrication by electron beam lithography and b antidot model potential, where a is the period of the antidots and d is an effective diameter the antidot

Fig. 9.41 Magnetoresistance observed in three different samples, where the periods of antidots are a = 200 nm for sample 1 and a = 300 nm for samples 2 and 3. The three samples show different resistivity at vanishing magnetic field B = 0. The inset illustrate the commensurate electron cyclotron orbits, surrounding 1, 2, 4, 9, and 21 antidots

antidots arrays by using electron beam lithography, and (b) illustration of fabricated antidot array. Magnetoresistance oscillations of 2DEG with antidots exhibit similar behavior to the above case of heterostructures with lateral surface superlattices and Weiss oscillations appear in low magnetic field less than 1T instead of SdH effect as shown in Fig. 9.41. It may be expected that the oscillatory phenomena is related to the cyclotron

562

9 Quantum Structures 2

Fig. 9.42 The effective cyclotron radius rˆc = Rc /a is plotted as a function of magnetic field for a = 300 nm. The circled points correspond to the commensurate orbits 1, 2, 4, 9, and 21

orbit surrounding antidots and thus the cyclotron radius Rc , antidot period a, and effective diameter d of the antidot. The inset of Fig. 9.41 shows typical cyclotron orbits, where the number of included in the commensurate orbits are, 1, 2, 4, 9, and 21. Here we mention the physical parameters to understand the commensurability √ of the electron orbits. The cyclotron radius is defined by Rc = 2π Ns /B, the electron √ mean free path le = vF τ with relaxation time τ , and the Fermi wavelength kF = 2π/Ns . As an example, we assume Ns = 2.4 × 1011 1/cm2 , electron mobility μ = 1.3 × 106 cm2 /Vs, and we obtain vF = 2.12 × 107 cm/s, le = lF = 10.5 μm, lF = 51.2 nm, and Rc = 80.8 nm, ωc = 2.63 × 1012 s−1 and ωc τ = 130 at magnetic field B = 1 T. We note here that an electron satisfies the condition ωc τ 1 at B = 1 T. Weiss oscillations in quantum dots array are expected to depend on the parameter rˆc = Rc /a. Another parameter is the normalized antidot cross section dˆ = d/a. When ωc τ < 2π , cyclotron motion of an electron is not completed, resulting in drift motion with scattering. In the case of ωc τ > 2π , however, an electron cyclotron motion is completed and drift motion vd = E H /B of the orbits results in the Hall field. In the latter case, electrons are expected to make cyclotron motion under the commensurate states as shown in the inset of Fig. 9.41. Weiss et al. [68] found the commensurate states for the sample with dˆ = 1/3, the extrema of the magnetoresistance oscillations appear at Rˆ c = 0.5, 0.8, 1.14, 1.7, and 2.53 for the commensurate orbits with n = 1, 2, 4, 9, and 21 as shown in the inset of Fig. 9.41. In Fig. 9.42 the effective cyclotron radius Rˆ c is plotted as a function of magnetic field B. Commensurablity of the Weiss oscillations is discussed in detail by Ando et al. [70], and related references are therein.

9.5 Wannier–Stark Effect in Superlattices

563

9.5 Wannier–Stark Effect in Superlattices Stark [71] discovered the splitting of atomic levels in high electric field in 1913. Later, in 1960, Wannier studied electric field effect on the electronic states in the presence of uniform high electric field and predicted that eigen states are localized along the direction of the electric field [72]. The quantized energy levels are called Wannier–Stark ladders and given by En = neEd,

(9.80)

where n is an integer, E the applied electric field,and d the lattice period along the electric field. Discussion on the Wannier–Stark effect has been very controversial, and many papers have been published about the possibility to observe the effect. Zak [73] claimed that such Stark ladder states cannot exist because they will decay rapidly due to Zener tunneling caused by interband mixing. Another paper published by Emin and Hart [74] claimed that such interband effects are totally absent and no Zener tunneling is observable. On the other hand, the result was claimed by Argyres et al. [75] and Leo et al. [76] and concludes that Zener tunneling is possible in Stark ladders. A number of experimental challenges were carried out in order to observe the Stark ladder in bulk materials, but no clear evidence was found. In stead only weak oscillation of conductivity was observed in ZnS and attributed to the hopping motion of electrons between Stark ladder states [77, 78]. The failure of observation is attributed to scattering of electrons by impurities or phonons, which prevent the acceleration of electrons up to Brillouin zone edge. Mendez et al. [79, 80] observed that Photoluminescence and photocurrent peaks of a GaAs/AlGaAs superlattice, which was explained by a field–induced localization of carriers to isolated quantum wells (Stark ladders) as shown in Fig. 9.43. Schematic illustration of the superlattice structure is depicted in Fig. 9.43, where (a) shows only one miniband of the conduction band, and one level of heavy hole band and one miniband associated with the light hole band, (b) localized with extended states (Stark ladders) allows multiple peaks in the photoluminescence and photocurrent, and (c) in high electric field Stark ladders are formed and electronic state is localized in each well region or interband tunneling is expected. Their experiment is believed to be the first observation of Wannier–Stark effect. At the same time, Bleuse et al. reported a possibility of electric–field–induced localization (Stark ladder formation) in superlattice by the tight–binding theory [81]. Since then, a number of optical measurements on Wannier–Stark effect in semiconductor superlattices have been performed using various techniques such as photoluminescence, photocurrent, and electroreflectance [82–85]. In the following, we present the electroreflectance (ER) measurements in two different superlattices and compare with the theoretical calculations based on the tight–binding theory.

564

9 Quantum Structures 2

Fig. 9.43 Schematic illustration of optical transition in a superlattice under high electric field. a A structure of multiquantum wells of GaAs/AlGaAs. b The Wannier–Stark ladders are formed in a moderate electric field as shown in this figure, where the localized states (thick bars) spread into the next well region (dashed bars) and optical transition occurs from the state of valence band to the extended ladder. c in high electric field Stark ladders are formed electronic state is localized in each well region or interband tunneling is expected. (after Mendez et al. [79])

One of the best way to observe Wannier Stark effect is the ER measurement (modulation spectroscopy) as discussed in 5.1, which reveals the shift of optical transition in detail. Figure 9.44 shows an example of the ER spectra observed in a GaAs(40 Å)/Al0.3 Ga0.7 As(20 Å) superlattice [85], where we see the signal peaks in the energy region 1.5 ∼ 1.8 eV shift in proportion to the applied the applied voltage toward both lower and higher energies as reported by Mendez et al. [79]. This behavior of the ER spectra arises from the oblique transition between states localized in adjacent quantum wells shown in Fig. 9.43b and clearly indicates formation of Stark ladder states. Complex signals are also observed in higher energy region 1.8 ∼ 2.2 eV [85]. The peak shift is plotted in Fig. 9.45 as a function of electric field. The results indicate complicated stark ladders are formed in superlattice with high electric field and assignment of the transition seems to be impossible. Therefore we proposed to use tight–binding theory to analyse the Stark ladders in the conduction band and valence bands of the superlattice. It is very important to point out that the detailed theoretical analysis is required to explain the experimental observation because of the complicated band structures due to the zone folding effect [86, 87] (the zone folding effect is discussed in 9.1.2 of this textbook). Since the valence band structure is very complicated, we need detailed

9.5 Wannier–Stark Effect in Superlattices

565

Fig. 9.44 Electroreflectance spectra observed in GaAs(40 Å)/Al0.3 Ga0.7 As(20 Å) superlattice at various applied voltages from +0.6 to −3.0 at 77 K. The left and right shifts of the peaks indicate oblique transitions between Stark ladder states in adjacent quantum wells [85]

Fig. 9.45 Experimental results of the transition energies obtained from Fig. 9.44 are plotted by open circles. Calculated transition energies between ladder states of the valence bands and the conduction bands are obtained by the tight binding theory, where a H1 E1 0, H1 E1 ± 1, and H1 E1 ± 2, b L1 E1 0, L1 E1 ± 1, and H1 E1 + 2, c H2 E1 + 1, d L2 E1 + 1, e H2 E2 0, H2 E2 ± 1, f L2 E2 − 1, and g the localized spin–orbit split–off states to the conduction band states. See text for the notation Hm En ν and Lm En ν [85]

study of energy band structures of the conduction band, heavy hole band, light hole band, and spin–orbit split-off band in superlattices [85, 87, 88]. The tight binding theory is given in the first part of this chapter in detail, where basis functions are taken as a three–dimensional Fourier transformation of the atomic orbitals, and thus the basis functions are labelled by three–dimensional wavevectors. On the other hand, when an electric field applied along the growth direction (z axis), the translational symmetry in the direction of the electric field is lost. In such a case we are not able to apply the Fourier analysis in the z–direction, although it is still valid in the x– and y–directions. Therefore the basis functions are specified by the atomic position l along the z–axis, and a two–dimensional wavevector k as

566

9 Quantum Structures 2

1 bμ bμ ψk ,l (r) = √ exp(ik · r)φi, j,l (r), N i, j

(9.81)

where φi,bμj,l (r) is an atomic orbital located at the site of the crystal (i, j, l), and b and μ denotes the kind of atom (b = cation (c) or anion (a)) and the type of atomic orbital (μ =, s, px , p y , or pz ). The optical properties are mainly governed by the band structure at the point, we set k = 0. The eigen states and energy eigenvalues of the Wannier Stark localized states are then calculated by solving the secular equation det|Hlbμ;l b μ − δl,l δb,b δμ,μ E| = 0, where

Hlbμ;l b μ = ψlbμ (r)|H |ψlb μ (r).

(9.82)

(9.83)

The effect of the electric field is included in the diagonal elements of the Hamiltonian matrix, and the Hamiltonian contains the intra–atomic spin–orbit interaction. We have neglected a contribution from field–induced intra–atomic mixing between s and pz orbitals, since it is expected to be very small. In order to solve the secular equation (9.83), we consider a finite domain in the z–direction, because the number of superlattice periods of a real system is finite and no translational symmetry exists along the z–direction. The superlattice used in the present work is rewritten as (GaAs14 )/(Al0.3 Ga0.7 As)7 , and the AlGaAs layers are treated by a virtual crystal approximation in which the tight binding parameters are replaced by an average value of GaAs and AlAs. The energy band analysis of the superlattice is made for ten periods of (GaAs14 )/(Al0.3 Ga0.7 As)7 . The valence band offset is set to be 0.144 eV. Figure 9.45 shows a comparison between the experimental data (◦) from Fig. 9.44 and the results of the tight binding calculation (lines). In order to classify the transition we used the notation Hm En ν for the transition from the localized heavy hole state Hm to the localized conduction band state En and Lm En ν for the transition from the localized light hole state Lm to the localized conduction band state En . The lines are then classified as (a) H1 E1 0, H1 E1 ± 1, and H1 E1 ± 2, (b) L1 E1 0, L1 E1 ± 1, and H1 E1 + 2, (c) H2 E1 + 1, (d) L2 E1 + 1, (e) H2 E2 0, H2 E2 ± 1, (f) L2 E2 − 1, and (g) the localized spin–orbit split–off states to the conduction band states. We find in Fig. 9.45 that the Wannier–Stark localization is clearly seen in a superlattice, and that Stark ladders are formed in the spin–orbit split-off band, in addition to the heavy and light hole bands. Another interesting observation is the Brillouin zone folding effect. As pointed out in 9.1, AlAs is an indirect gap material and the conduction band minimum is located at X point which is lower that the conduction band at the point, and therefore so called “Xz ” point plays a very important role in the formation of Stark ladders as pointed out by Morifuji et al. [88]. This effect was clearly observed in the ER measurements carried out by Nagasawa et al. [89] as shown in Fig. 9.46 for (GaAs)5 )/(AlAs)2 superlattice. The sample consists of 10 periods of an undoped (GaAs)5 )/(AlAs)2 superlattice sandwiched by 30 Å nondoped GaAs spacer layers. The superlattice is

9.6 Bloch Oscillation

567

Fig. 9.46 ER measurements in (GaAs)5 )/(AlAs)2 superlattice under a applied electric field at 15 K. The solid lines correspond to the transitions and the zone folded Xz points calculated by the tight binding method, respectively

placed between a p+ – and an n+ –GaAs layer doped with 5.0 × 1018 (Be–doped) and 5.0 × 1018 (Si–doped), respectively. The thickness of the doped layers is 5000 Å for the n-regions and the thickness of the cap layers is 500 Å so as to perform optical measurements. The calculated transition energies by the tight binding theory are shown by the solid lines (, and Xz points). Here we see clearly the zone folded conduction band in the superlattice, and the importance of and X point mixing. The Zener tunneling through a p-i-n diode under a reverse voltage bias has been studied in a tight binding model by Schulman and Chang [90], and Di Carlo et al. [91]. Measurements of the Zener tunneling were carried out using a thin (GaAs)5 )/(AlAs)2 superlattice at T = 4.2 K [89, 92–94].

9.6 Bloch Oscillation Since superlattice in which the Brillouin zone is very narrow due to the band folding effect, the Bloch oscillation is expected. However, the frequency of Bloch oscillation is very high and experimental observations have been achieved by optical method. Here we will discuss the Bloch oscillation in two simplified models. The prediction of Bloch oscillation [95] is based on the periodic motion of an electron in a one dimensional energy band. Let’s consider a simplified model of a conduction band E = A sin(dk) and the electron moves in the k space along with k˙ = −eE/ with its group velocity v given by (see Sect. 3.5 of this textbook)

568

9 Quantum Structures 2

1 dE Ad = cos(dk), dk eE t. k = k(0) −

v(k) =

(9.84) (9.85)

When an electron is not affected by scattering, the electron position x is given by

t

x(t) =

v(k(t ))dt = x(0) +

0

A eEd sin t . eE

(9.86)

The result gives the oscillatory electron motion with the angular frequency ωB = e|E|d/ in real space. This electron motion is called as “Bloch oscillation” [95]. Here we follow the treatment employed by Esaki and Tsu [1] and discuss electron transport in a miniband band given by the following dispersion relation E(k) =

E1 (1 − cos(k · d)), 2

(9.87)

where the first Brillouin zone is defined by [−π/d, +π/d] with the miniband width E1 and superlattice period d. Using the relation v = −1 ∂ E/∂k, the velocity increment in a time interval dt is given by (see (3.111)) dv =

eE ∂ 2 E dt. 2 ∂k 2

(9.88)

The effective mass of the conduction band is given by 1 ∂ 2E 1 = , m ∗ (k) 2 ∂k 2 E1 d 2 1 cos(kd), = cos(kd) = ∗ 22 m (0)

(9.89)

where m ∗ (0) = 22 /E1 d 2 is the band edge effective mass. We evaluate drift velocity following the method proposed by Esaki and Tui [1]. Since the electron energy is given by E(k) and k depends on the time by k = (eE/)t vd =

∞

exp(−t/τ )dv ∞ eE = ∗ cos(eEd · t/) exp(−t/τ )dt, m (0) 0 0

and then we obtain

(9.90)

9.6 Bloch Oscillation

569

Fig. 9.47 Electron velocities in the minibands of the dispersion E = (E1 /2)(1 − cos(k · d) for the period d = 100 Å and d = 50 Å are plotted as a function of the reduced electric field ξ = eEdτ/, where E1 is the band width and d the superlattice period

/d ξ , · m ∗ (0) 1 + ξ 2 eEdτ . ξ=

vd =

(9.91) (9.92)

Calculated electron velocities of (9.91) are plotted in Fig. 9.47 as a function of the reduced electric field ξ for the period d = 100 Å and d = 50 Å, where we see that the maximum velocity is 3.8 × 107 cm/s for d = 100 Å and 1.9 × 107 cm/s for d = 50 Å, and negative differential conductivity appears for ξ > 1. The maximum electron velocity is about 10 to 20 times higher than the drift velocity observed in bulk semiconductors. Here we discuss the electron motion in the model band with E1 = 0.1 eV and miniband under the condition without scattering. Then, the time τB required to travel from the bottom of the miniband with k(0) = 0 to the Brillouin zone edge k = π/d using the relation (9.85)

τB 0

π eE π dt = , τB = . d 2eEd

(9.93)

In the following we estimate various parameters in the case of the superlattice period d = 100 Å. we obtain the band edge effective mass m ∗ (0) = 0.0152 m. Under the applied electric field E = 1000 V/cm (1.0 × 105 V/m), we obtain τB = 2.07 ps. Assuming the relaxation time τ = τB , the electron mobility at the bottom of the miniband is μB = 2.4 × 105 cm2 /Vs and the electric field corresponding to give maximum drift velocity (at ξ = 1) is given by E B = 318 V/cm. The frequency of the Bloch oscillation is νB = ωB /2π = e|E|d/ = 242 GHz. The Bloch oscillation occurs under the condition e|E|τ d/ 2π , while e|E|τ d/ = π for τ = τB . Since τB is the time required for an electron to travel from k = 0 to the miniband edge k = π/d (the first Brillouin zone edge), the condition is expressed as τ τB as concluded by Esaki and Tsu [1]. The Bloch oscillations have been observed by using the four–wave mixing measurements in GaAs/Al0.3 Ga0.7 As superlattices [96, 97].

570

9 Quantum Structures 2

9.7 Problems (9.1) In order to understand zone folding effect, consider crystals A an B with the same lattice constant a. Draw free electron band E(k) = k 2 for A or B crystal in the first Brillouin zone [−2π/a, +2π/a]. Then, calculate and plot free electron bands of a superlattice ABABABAB. . . defined in the first Brillouin zone [−π/a, +π/a]. (9.2) The tight-binding theory is described in detail in the textbook by Harrison [3] and used for calculation of the energy band structures in various materials. The most popular method is to use sp3 orbitals for the basis functions, However, calculated results do not explain the indirect band gap such as GaP, AlAs, and so on. Vogl et al. [4] proposed to add one more orbital s∗ to the basis functions and obtained reasonable energy band structures of the indirect band gaps materials. The matrix elements of sp3 s∗ are listed in the paper by Vogl et al. [4]. Using the listed material parameters, and calculate energy band structures of GaAs and AlAs. (9.3) Consider a circular dot and the potential V (x, y) of (9.35) is rewritten as V (ρ) =

1 ∗ 2 2 m ω0 ρ , 2

(9.94)

where ω0 = ω y = ω y , and ρ 2 = x 2 + y 2 . Then, show that the Hamiltonian of an electron with the effective mass m ∗ and momentum p confined in the potential of (9.94) is given by the Hamiltonian of a simple harmonic oscillator and derive the eigen values of the electron states. (9.4) Calculate the cyclotron radius rˆc of a surface antidot arrays (Weiss oscillation device) with array period a = 200 nm as a function of applied magnetic filed. Use the same parameters as for Fig. 9.42.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10.

L. Esaki, R. Tsu, IBM J. Res. Dev. 14, 61 (1970) P.Y. Yu, M. Cardona, Fundamentals of Semiconductors (Springer, Heidelberg, 1996), Chap. 9 W. Harrison, Electronic Structure and the Properties of Solids (Freeman, San Francisco, 1980) P. Vogl, H.P. Hjalmarson, J.D. Dow, A semi-empirical tight-binding theory of the electronic structure of semiconductors. J. Phys. Chem. Solids 44, 365 (1983) Y.-T. Lu, L.J. Sham, Phys. Rev. B 40, 5567 (1989) H. Fujimoto, C. Hamaguchi, T. Nakazawa, K. Taniguchi, K. Imanishi, Phys. Rev. B 41, 7593 (1990) T. Matsuoka, T. Nakazawa, T. Ohya, K. Taniguchi, C. Hamaguchi, Phys. Rev. B 43, 11798 (1991) A. Ishibashi, Y. Mori, M. Itahashi, N. Watanabe, J. Appl. Phys. 58, 2691 (1985) E. Finkman, M.D. Sturge, M.C. Tamargo, Appl. Phys. Lett. 49, 1299 (1986) E. Finkman, M.D. Sturge, M.-H. Meynadier, R.E. Nahory, M.C. Tamargo, D.M. Hwang, C.C. Chang, J. Lumin. 39, 57 (1987)

References

571

11. G. Danan, B. Etienne, F. Mollot, R. Planel, A.M. Jeaqn-Louis, F. Alexandre, B. Jusserand, G. Le Roux, J.Y. Marzin, H. Savary, B. Sermage, Phys. Rev. B 35, 6207 (1987) 12. J. Nagle, M. Garriga, W. Stolz, T. Isu, K. Ploog, J. Phys. (Paris) Colloq. 48, C5-495 (1987) 13. F. Minami, K. Hirata, K. Era, T. Yao, Y. Matsumoto, Phys. Rev. B 36, 2875 (1987) 14. D.S. Jiang, K. Kelting, H.J. Queisser, K. Ploog, J. Appl. Phys. 63, 845 (1988) 15. K. Takahashi, T. Hayakawa, T. Suyama, M. Kondo, S. Yamamoto, T. Hijikata, J. Appl. Phys. 63, 1729 (1988) 16. M.-H. Meynadier, R.E. Nahory, J.M. Workock, M.C. Tamargo, J.L. de Miguel, M.D. Sturge, Phys. Rev. Lett. 60, 1338 (1988) 17. J.E. Golub, P.F. Liao, D.J. Eilenberger, J.P. Haribison, L.T. Florez, Y. Prior, Appl. Phys. Lett. 53, 2584 (1988) 18. K.J. Moore, P. Dawson, C.T. Foxon, Phys. Rev. B 38, 3368 (1988); K.J. Moore, G. Duggan, P. Dawson, C.T. Foxon, Phys. Rev. B 38, 5535 (1988) 19. H. Kato, Y. Okada, M. Nakayama, Y. Watanabe, Solid State Commun. 70, 535 (1989) 20. G. Bastard, Phys. Rev. B 25, 7584 (1982) 21. J.N. Schulman, T.C. McGill, Phys. Rev. Lett. 39, 1681 (1977); Phys. Rev. B 19, 6341 (1979); J. Vac. Sci. Technol. 15, 1456 (1978); Phys. Rev. B 23, 4149 (1981) 22. H. Rücker, M. Hanke, F. Bechstedt, R. Enderlein, Superlattices Microstruct. 2, 477 (1986) 23. J. Ihm, Appl. Phys. Lett. 50, 1068 (1987) 24. L. Brey, C. Tejedor, Phys. Rev. B 35, 9112 (1987) 25. S. Nara, Jpn. J. Appl. Phys. 26, 690 & 1713 (1987) 26. E. Yamaguchi, J. Phys. Soc. Jpn. 56, 2835 (1987) 27. K.K. Mon, Solid State Commun. 41, 699 (1982) 28. W.A. Harrison, Phys. Rev. B 23, 5230 (1981) 29. E. Caruthers, P.J. Lin-Chung, Phys. Rev. B 17, 2705 (1978) 30. W. Andreoni, R. Car, Phys. Rev. B 21, 3334 (1980) 31. M.A. Gell, D. Ninno, M. Jaros, D.C. Herbert, Phys. Rev. B 34, 2416 (1986); M.A. Gell, D.C. Herbert, Phys. Rev. B 35, 9591 (1987); J.-B. Xia: Phys. Rev. B 38, 8358 (1988) 32. J.S. Nelson, C.Y. Fong, I.P. Batta, W.E. Pickett, B.K. Klein, Phys. Rev. B 37, 10203 (1988) 33. T. Nakayama, H. Kamimura, J. Phys. Soc. Jpn. 54, 4726 (1985) 34. I.P. Batra, S. Ciraci, J.S. Nelson, J. Vac. Sci. Technol. B5, 1300 (1987) 35. D.M. Bylander, L. Kleiman, Phys. Rev. B 36, 3229 (1987) 36. S.-H. Wei, A. Zunger, J. Appl. Phys. 63, 5795 (1988) 37. Y. Hatsugai, T. Fujiwara, Phys. Rev. B 37, 1280 (1988) 38. S. Massidda, B.I. Min, A.J. Freeman, Phys. Rev. B 38, 1970 (1988) 39. R. Eppenga, M.F.H. Schuurmans, Phys. Rev. B 38, 3541 (1988) 40. J.C. Slater, G.F. Koster, Phys. Rev. 94, 1498 (1954) 41. P.O. Löwdin, J. Chem. Phys. 18, 365 (1950) 42. D.J. Chadi, M.L. Cohen, Phys. Status Solidi 68, 405 (1975) 43. T. Matsuoka, Ph.D. Thesis, Osaka University (1991) 44. K.J. Moore, G. Duggan, P. Dawson, C.T. Foxon, Phys. Rev. B 38, 1204 (1988) 45. M. Nakayama, I. Tanaka, I. Kimura, H. Nishimura, Jpn. J. Appl. Phys. 29, 41 (1990) 46. W. Ge, M.D. Sturge, W.D. Schmidt, L.N. Pfeiffer, K.W. West, Appl. Phys. Lett. 57, 55 (1990) 47. M.A. Kastner, Phys. Today 46, 24 (1993) 48. N. Johnson, Condens. Matter 7, 965 (1995) 49. S. Tarucha, D.G. Austing, T. Honda, R.J. van der Hage, L.P. Kouwenhoven, Phys. Rev. Lett. 77, 3613 (1996) 50. T. Ezaki, N. Mori, C. Hamaguchi, Phys. Rev. B 56, 6428 (1997) 51. T. Ezaki, Study on electronic states and electrical conduction in semiconductor quantum devices, pp.44–59. Ph.D. thesis, Osaka University, 1997 52. D.V. Averin, K.K. Likarev, in Mesoscopic Phenomena in Solids, ed. by B.L. Al’tshuler, P.A. Lee, R.A. Webb (Elsevier, Amsterdam, 1991) 53. H. Grabert, M. Devoret (eds.), Single Charge Tunneling (Plenum, New York, 1992)

572

9 Quantum Structures 2

54. M. Stopa, Fundamentals of Mesoscopic Phenomena, ed. by Namba (Ohm-sha, Tokyo, 1994) (in Japanese), pp. 56–66 55. M. Ueda, Oyo Buturi. Jpn. Soc. Appl. Phys. 62, 889–897 (in Japanese) (1993) 56. S. Kastumoto, Kagaku (Science) 63, 530–537 (in Japanese) (1993) 57. T.A. Fulton, G.J. Dolan, Phys. Rev. Lett. 95, 109 (1987) 58. D.C. Ralph, C.T. Black, M. Tinkham, Phys. Rev. Lett. 74, 3241 (1995) 59. W. Chen, H. Ahmed, K. Nakazato, Appl. Phys. Lett. 66, 3383 (1995) 60. D.L. Klein, P.L. McEuen, J.E. Bowen Katari, R. Roth, A.P. Alivisatos, Appl. Phys. Lett. 68, 2574 (1996) 61. K. Matsumoto, M. Ishii, K. Segawa, Y. Oka, B.J. Vartanian, J.S. Harris, Appl. Phys. Lett. 68, 34 (1996) 62. K. Yano, T. Ishii, T. Hashimoto, T. Kobayashi, F. Murai, K. Seki, IEEE Trans. Electron Devices ED-41, 1628 (1994); Appl. Phys. Lett. 67, 828 (1995) 63. D. Weiss, K. v. Klitzing, K. Ploog, G. Weimann, Europhys. Lett. 8, 179 (1989) 64. R.R. Gerhardts, D. Weiss, K. v. Klitzing, Phys. Rev. Lett. 62, 1173 (1989) 65. D. Weiss, K. v. Klitzing, K. Ploog, Surf. Sci. 229, 88 (1990) 66. P.H. Beton, E.S. Alves, P.C. Main, L. Eaves, M.W. Dellow, M. Hinini, O.H. Hughes, S.P. Beaumont, C.D.W. Wilkinson, Phys. Rev. B 42, 9229 (1990) 67. R.W. Winkler, J.P. Katthaus, K. Ploog, Phys. Rev. Lett. 62, 1177 (1989) 68. D. Weiss, M.L. Roukes, A. Menschig, P. Grambow, K. von Klitzing, G. Weimann, Phys. Rev. Lett. 66, 2790 (1991) 69. D. Weiss, K. Richter, E. Vasiliadou, G. Lütjering, Surf. Sci. 305, 408 (1994) 70. T. Ando, Y. Arakawa, S. Komiyamiyama, H. Nakashima (ed.), Mesoscopic Physics and Electronics (Springer, New York, 1998). See Section 2.5 by T. Ando and references therein 71. J. Stark, Annal. Phys. 43, 1914 (1914) 72. G.H. Wannier, Phys. Rev. 117, 432 (1960) 73. J. Zak, Phys. Rev. Lett. 20, 1477 (1968) 74. D. Emin, C.F. Hart, Phys. Rev. B 36, 7353 (1987) 75. P.N. Argyres, S. Sfiat, J. Phys. C: Condens. Matter. 2, 7089 (1990) 76. J. Leo, A. MacKinnon, J. Phys. C: Condens. Matter. 1, 1449 (1989) 77. S. Maekawa, Phys. Rev. Lett. 24, 1175 (1970) 78. M. Saitoh, J. Phys. C: Solid State Phys. 5, 914 (1972) 79. E.E. Mendez, F. Agulló-Rueda, J.M. Hong, Phys. Rev. Lett. 60, 2426 (1988) 80. F. Agulló-Rueda, E.E. Mendez, J.M. Hong, Phys. Rev. B 40, 1357 (1989) 81. J. Bleuse, G. Bastard, P. Voisin, Phys. Rev. Lett. 60, 220 (1988) 82. K. Fujiwara, Jpn. J. Appl. Phys. 28, L1718 (1989) 83. M. Nakayama, I. Tanaka, K. Kawashima, K. Fujiwara, Phys. Rev. B 44, 5935 (1991) 84. H. Schneider, A. Fisher, K. Ploog, Phys. Rev. B 45, 6329 (1992) 85. C. Hamaguchi, M. Yamaguchi, M. Morifuji, K. Taniguchi, C. Gmachl, E. Gornik, Semicond. Sci. Technol. 9, 1994 (1994) 86. A.J. Shields, P.C. Klipstein, M.S. Skolnick, G.W. Smith, C.R. Whitehouse, Phys. Rev. B 42, 5879 (1990) 87. M. Yamaguchi, H. Nagasawa, M.M. Morifuji, H. Kubo, K. Taniguchi, C. Hamaguchi, C. Gmachl, E. Gornik, Semicond. Sci. Technol. 9, 1810 (1994) 88. M. Morifuji, M. Yamaguchi, K. Taniguchi, C. Hamaguchi, Phys. Rev. B 50, 8722 (1994) 89. H. Nagasawa, K. Murayama, M. Morifuji, A. Di Varlo, P. Vogl, G. Böhm, G. Tr"ankle, G. Weimann, C. Hamaguchi, Phys. B 227 206 (1996) 90. J.N. Schulman, Y.-C. Chang, Phys. Rev. B 27, 2346 (1983) 91. A. Di. Carlo, P. Vogl, W. Pötz, Phys. Rev. B 50, 8358 (1994) 92. C. Hamaguchi, M. Yamaguchi, H. Hasegawa, M. Morifuji, A. Di Carlo, P. Vogl, G. Böhm, G. Tränkle, G. Weimann, Y. Nishikawa, S. Muto, Jpn. J. Appl. Phys. 34, 4519 (1995) 93. H. Nagasawa, K. Murayama, M. Morifuji, C. Hamaguchi, A. Di Carlo, P. Vogl, G. Böhm, G. Tränkle, G. Weimann, Solid State Electron. 40, 245 (1996)

References

573

94. K. Murayama, H. Hasegawa, S. Ozaki, M. Morifuji, C. Hamaguchi, A. Di Carlo, P. Vogl, G. Böhm, G. Weimann, Superlattices Microstruct. 20, 493 (1966) 95. F. Bloch, Z. Phys. 52, 555 (1928) 96. J. Feldmann, K. Leo, J. Shar, D.A.B. Miller, J.E. Cunningham, T. Meiser, G. von Plessen, P. Thomas, S. Schmitt-Rink, Phys. Rev. B 46, 7252 (1992) 97. T. Dekorsy, R. Ott, H. Hurz, K. Köhler, Phys. Rev. B 51, 17275 (1995)

Chapter 10

Light Emission and Laser

Abstract In this chapter, physics of luminescence and laser oscillations are treated in detail. First the definition of Einstein coefficients is introduced to connect absorption with spontaneous emission and stimulated emission. Then the spontaneous and stimulated emission rates are derived from the perturbation theory. Absorption and emission rates are strongly affected by the density of states, The density of states in the presence of impurities are shown to result in the band tail effect, where Kane’s model is used. Using these results the gain of laser oscillations are discussed. The results are also used to explain various types of luminescence. Since semiconductor lasers are fabricated in heterostructures and light emission is confined by the heterointerfaces, we discuss optical wave guide analysis to reveal the importance of double heterostructure. Mode analysis of the waveguide is given in detail to explain TE and TM modes and confinement factor, in addition to Fabry–Perot analysis. Since most of the laser diodes (LDs) are fabricated in quantum well structures, confinements of electrons in the conduction band and holes in the valence bands play an important role in the laser mode and the gain. In order to obtain the quantized states in valence bands, we show how to solve 6 × 6 Luttinger Hamiltonian including strain effect. Final part of this chapter is devoted to the physics of GaN based lasers, where we show the strain effect plays an important role in the laser oscillations.

In Chaps. 4 and 5 we dealt with optical properties of semiconductors, where electron transition induced by absorbing photon plays the most important role. It is also possible for an electron to make transition from a higher energy state to a lower energy state by emitting a photon. In other words electrons recombine with holes by emitting light. The latter process gives rise to a light emission (luminescence) and laser action, and provides well known devices such as light emitting diode (LED) and laser diode (LD). In this chapter we deal with light emission from semiconductors and laser diodes. First we deal with spontaneous emission, stimulated emission and absorption, where spontaneous emission is related to luminescence and stimulated emission plays the most important role in the laser action. For better understanding, readers are recommended to refer the articles listed in the references [1–8]

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2023 C. Hamaguchi, Basic Semiconductor Physics, Graduate Texts in Physics, https://doi.org/10.1007/978-3-031-25511-3_10

575

576

10 Light Emission and Laser

10.1 Einstein Coefficients A and B Einstein proposed the optical processes of absorption, spontaneous emission and stimulated emission in 1917.1 In the paper Einstein dealt with emission and absorption of light and pointed out for the first time the concept of stimulated emission. We know that the basic mechanism of the laser action comes from the stimulated emission, but the discovery of lasers was accomplished after his death. The concept proposed by Einstein explains not only the principle on laser action but also the optical processes of absorption and emission. Here we will describe Einstein’s theory first and then derive so called Einstein coefficients A and B. We consider an interaction between radiation field (light or photon) and N atoms or molecules in a cavity, where the atoms or molecules have energy levels E 1 and E2 , and we assume that the atoms or molecules are allowed to make transition between the two levels by absorbing or emitting the photon energy given by ω = E2 − E1 ,

(10.1)

where the atomic energies are degenerate with the degeneracy g1 and g2 , and the number of atoms or molecules are N1 and N2 , respectively. The system is shown schematically in Fig. 10.1. The average density of radiation field W (ω) depends on the thermal equilibrium value WT (ω) and the external excitation WE (ω), and is given by the following relation W (ω) = WT (ω) + WE (ω) .

(10.2)

Here we have to note that WE (ω) is not uniform in the cavity in general case. Emission and absorption of photon are defined in the following way. We define transition rate of an atom from the energy level 2 to the energy level 1 by A21 . An atom of the energy level 1 is not possible to make a transition to the energy level 2 without radiation field, because the energy conservation is not fulfilled in the transition. However, the transition 1 → 2 is possible by absorbing a photon ω. We define the transition rate 1 → 2 by B12 in the presence of photon field with the radiation density W (ω). These two processes are easily understood, but careful consideration is required for the transition from the upper level 2 to the lower level 1

Fig. 10.1 Three optical processes of radiation proposed by Einstein: spontaneous emission, absorption and stimulated emission

1

A. Einstein: “Zur Quantentheorie der Strahlung,” Phys. Z. 18, 121 (1917), The title in English is “On the Quantum Theory of Radiation”.

10.1 Einstein Coefficients A and B

577

in the presence of the radiation W (ω). It is easily expected that the transition 2 → 1 is enhanced in the presence of the radiation field. This transition enhanced by the radiation is called stimulated emission and the rate is defined by B21 . These three transition processes are schematically shown in Fig. 10.1. These optical processes were defined by Einstein in 1917, and the coefficients A21 , B12 and B21 are called Einstein coefficients. We have to note here that the Einstein coefficients A21 , B12 and B21 are independent of the radiation density W (ω). In the above case absorption and stimulated emission are assumed to be proportional to the radiation density W (ω). This assumption is valid when the radiation density is a slowly varying function of transition frequency ω. The transition A21 is called spontaneous emission and independent of the radiation density. The occupation densities N1 of the level 1 and N2 of the levels 2 are governed by the following rate equation, dN1 dN2 =− = N2 A21 − N1 B12 W (ω) + N2 B21 W (ω) . dt dt

(10.3)

In order to investigate the relations between the Einstein coefficients, first we consider the case of thermal equilibrium. In the thermal equilibrium the distribution densities of the two levels are constant and then (10.3) leads to the following relation, N2 A21 − N1 B12 WT (ω) + N2 B21 WT (ω) = 0 . This results in WT (ω) =

A21 . (N1 /N2 )B12 − B21

(10.4)

(10.5)

In the thermal equilibrium, the occupation densities of N1 and N2 are given by Boltzmann statistics, g1 N1 g1 exp(−βE1 ) = = exp(βω) , N2 g2 exp(−βE2 ) g2

(10.6)

where β = 1/kB T . Using this relation (10.5) is rewritten as WT (ω) =

A21 , (g1 /g2 ) exp(βω)B12 − B21

(10.7)

where g1 and g2 represent the degeneracy of the states. We have to note here that the above equation is derived by using Boltzmann statistics and that the result of Einstein theory is easily proved to be consistent with Planck’s radiation theory. From the theory of Planck, the radiation density is given by ¯ WT (ω)dω = nωρ ω dω =

dω nω ¯ 3 ω 3 , dω = 2 3 2 3 π c π c exp(βω) − 1

(10.8)

578

10 Light Emission and Laser

where n¯ is the occupation density of photons. Equation (10.7) should coincide with (10.8), which is validated by the following equations, g1 B12 = B21 , g2 ω 3 B21 = A21 , π 2 c3

(10.9) (10.10)

where the above relations should hold at all temperature range. From these considerations we find that the three Einstein coefficients are related by the above two equations. In addition it is evident from (10.7) that Einstein theory with stimulated emission term is equivalent with Planck’s radiation theory. When g1 = g2 , we obtain the following relation (10.11) B12 = B21 .

10.2 Spontaneous Emission and Stimulated Emission As shown later, laser oscillations in semiconductors are induced by a strong emission by recombination. Recombination emissions consists of two terms, spontaneous emission and stimulated emission. Among them, stimulated emission plays the most important role in the laser oscillations in semiconductors. Here we deal with the recombination emissions in semiconductors in detail. First, we consider the case shown in Fig. 10.2, where excited electrons in the conduction band recombine with the holes in the valence band by emitting light. Figure 10.2 shows a process that an electron in a valence band makes a transition by absorb a light, and the reverse process that the excited electron recombine with the hole by emitting a light. Here the reverse process has two distinct emission processes, spontaneous and stimulated emissions. Before dealing with these processes by quantum mechanics, we will briefly mention how to excite electrons from the valence bands to the conduction band. When we create electron–hole pairs in a semiconductor by light incidence, the resulting recombination emission is called

Fig. 10.2 Optical absorption and recombination emission

10.2 Spontaneous Emission and Stimulated Emission

579

photoluminescence. In the case where an electric field excites electron–hole pairs or the electric field injects electrons and holes in p–n junction, the resulting light emission is called electro-luminescence. Sometimes electron beams are used to excite electron–hole pairs, and the light emission is called cathode luminescence. Light emitting diode (LED) and laser diode (LD) are excited by electron–hole injection. Also we have to note that excited electrons or holes recombine by absorbing or emitting phonons (lattice vibrations), and thus no photons are emitted. This process is called non-radiative recombination. Let’s discuss the excitation of electrons of E1 in the valence band into the conduction band E2 by incident photon and light emission by recombination as shown in Fig. 10.2. The rate of photon emission in the energy space dE per unit time and unit solid angle Ω is given by the following relation according to Lasher and Stern [8] r (E)dE(dΩ/4π) = rspon (E) + n photon rstim (E) dE(dΩ/4π) ,

(10.12)

where n photon is the photon numbers per mode given for thermal equilibrium by n0 =

1 , exp(E/kB T ) − 1

(10.13)

kB is Boltzmann’s constant and T is the absolute temperature. In (10.12) the term rspon (E) represents the spontaneous transition of electrons from the upper level to the lower level and, n photon rstim is the difference between the upward transition (absorption) and stimulated downward transition. For band–to–band transition the spontaneous and stimulated emission rates are given by [6, 8] (see also Appendix G for the derivation)

n r e2 E |M|2 f 2 (1 − f 1 )dE , π0 m 2 2 c3 n r e2 E rstim (E)dE = |M|2 ( f 2 − f 1 )dE , π0 m 2 2 c3

rspon (E)dE =

(10.14) (10.15)

where the factor ( f 2 − f 1 ) of (10.15) is derived from the net rate of stimulated transition between the downward factor f 2 (1 − f 1 ) and the upward factor f 1 (1 − f 2 ); f 2 (1 − f 1 ) − f 1 (1 − f 2 ) = ( f 2 − f 1 ). Here f 2 and f 1 are the electron occupation probabilities of the upper and lower levels, respectively, and n r is the refractive index. The summation is taken over all pairs of states in the conduction and valence bands per unit volume whose energy difference is dE and E + dE. The squared momentum matrix element |M|2 is defined in Chap. 4 and for the purpose of simplicity we assume the value averaged over the all polarizations of the incident light as 1 |Mx |2 + |M y |2 + |Mz |2 , 3 ∂

Mx = −i ψ2 exp(ik · r) ψ1 , ∂x

|M|2 =

(10.16a) (10.16b)

580

10 Light Emission and Laser

where |ψ1 and |ψ2 are the lower and higher bands wave functions, respectively. As stated in Chap. 4, for band–to–band transition the electron wave vectors k2 and k1 , and photon wave vector k are governed by the conservation rule δ(k2 − k1 ± k). Since photon wave vector k is negligibly small, we can use the relation k2 = k1 .2 When the upper and lower energy bands E2 and E1 are expressed by the functions of k = |k2 | = |k1 |, the density of states for the band–to–band transition (reduced density of states) ρred is easily evaluated. Then the transition rates for photon energy E are given by n r e2 E |M|2 ρred (E) f 2 (1 − f 1 ) , π0 m 2 2 c3 n r e2 E rstim (E) = |M|2 ρred (E)( f 2 − f 1 ) , π0 m 2 2 c3

rspon (E) =

(10.17) (10.18)

where the reduced density of states for the band–to–band transition is given by for one direction of spin d(E2 − E1 ) 1 k2 . (10.19) ρred (E) = 2 (2π ) dk From the energy conservation we have E2 − E1 = E, and thus we can define the following relation, Rspon =

rspon (E)dE .

(10.20)

The above equation is evaluated in the three extreme cases by Lasher and Stern [8]. (1) In the case of degenerate valence band, we can put f 1 = 0 for all transitions. Rspon

2n r e2 E = |Mb |2 av π0 m 2 2 c3

me 1+ m hh

−3/2

me + 1+ m lh

−3/2

n(10.21) ,

where n is the electron density, and |Mb |2 av is the average matrix element connecting states near the band edges. (2) In the case of non-degenerate conduction and valence bands Rspon

n r e2 E = π0 m 2 2 c3 ×

2π2 mkB T

3/2 |Mb |2 av

[m lh /(m e + m lh )]3/2 + [m hh /(m e + m hh )]3/2 (m lh /m)3/2 + (m hh /m)3/2

(10.22)

(3) In the case where the matrix elements are all the same for all the transitions (no–selection rule case), the following general equation is derived from (10.14) and (10.15). 2

As described later this assumption is not valid for the transition including the band tail sates.

10.2 Spontaneous Emission and Stimulated Emission

rspon (E) = B

rstim (E) = B E = ω,

581

ρc (E )ρv (E − E) f c (E ) 1 − f v (E − E) dE ,

(10.23)

ρc (E )ρv (E − E) f c (E ) − f v (E − E) dE ,

(10.24)

E = E2 = E1 + E = E1 + ω ,

(10.25)

where ρc and ρv are the density of states of the conduction and valence bands with two spin directions, respectively. For the valence bands the heavy hole and light hole bands should be taken into account. These relations are valid for large amounts of electron and hole injection and the conservation of energies is assumed but the conservation of wave vectors is not included. As mentioned later, the conservation of wave vectors is not required for the transitions including the band tail states, and thus the above equations may be used. For the transitions with the wave vector conservation we have to use the following relations. mr (ω − EG ) , mh mr E2 = Ec + (ω − EG ) , me 1 1 1 = + . mr me mh

E1 = Ev −

(10.26) (10.27) (10.28)

The coefficient B is given by B=

n r e2 E |M|2 av V , π0 m 2 2 c3

(10.29)

where |M|2 av is the average value of the squared matrix element over spins in the upper and lower bands, and V is the crystal volume. Total rate of spontaneous emission is easily evaluated if the selection rule is disregarded and then we obtain the following relation by carrying integration over the conduction and valence bands.. Rspon = Bnp ,

(10.30)

where n and p are the injected electron and hole densities. The total rate Rspon is the spontaneous emission rate per unit volume and the dimension is m3 /s. Distribution functions of the upper E2 (conduction band) and the lower E1 (valence band) states are given by the following relations by using quasi–Fermi level EFn in the conduction band and quasi–Fermi level EFp in the valence band,

582

10 Light Emission and Laser

1 , 1 + exp[(E2 − EFn )/kB T ] 1 . f1 = 1 + exp[(E1 − EFp )/kB T ]

f2 =

(10.31) (10.32)

Using these equations in (10.14) and (10.15), we obtain the following relation, rstim (E) = rspon (E) {1 − exp[(E − ΔEF )/kB T ]} ,

(10.33)

where ΔEF = EFn − EFp is the difference of the quasi–Fermi energies and becomes 0 in the thermal equilibrium. Stimulated emission rstim is related to the absorption coefficient α(E) defined in Chap. 4 and given by π 2 c 2 3 (10.34) α(E) = − 2 2 rstim (E) , nr E where—sign is used to express that the stimulated emission rstim (E) has an opposite sign compared to the absorption coefficient α(E). Equation (10.34) is easily derived from (G.14)and (10.18). When we put g(ω) = −α(ω) for the semiconductor laser gain, g(ω) = −α(ω) = =

π 2 c 2 3 rstim (ω) n 2r (ω)2

πe2 |M|2 ( f 2 − f 1 )ρred (ω) . n r c0 m 2 ω

(10.35)

Here we find that the gain is positive (g > 0) when f 2 − f 1 > 0, which means that the population in the upper level f 2 is higher than the lower level f 1 . This condition is called population inversion. We show in Figs. 10.3 and 10.4 the calculated results of inversion factor f 2 − f 1 and gain factor ( f 2 − f 1 )ρred , respectively, as a function of the emitted photon energy ω, where we used (10.26)–(10.28), (10.31), and (10.32), with m e = 0.068 m, m h = 0.59 m, EG = 1.43 eV, and T = 300 K. The injected electrons and holes are estimated by choosing proper values of the quasi–Fermi levels. The curves of the inversion factors in Fig. 10.3 correspond to the quasi–Fermi levels, EFn − Ec = Ev − EFp = −20, −10, 0, +5, +10, +15, +20 meV from the bottom to the upper curves. The gain factors ( f 2 − f 1 )ρred in Fig. 10.4 are estimated by assuming EFn − Ec = Ev − EFp = −20, −15, −10, −5, 0, 5, 10, 15, 20 meV from the bottom to the upper curves. We see in Figs. 10.3 and 10.4 that the inversion factor and the gain factor become positive near the band edge for higher injection levels. From the results we may write rspon (E) =

40 n 2r E 2 1 . α(E) πc2 3 exp[(E − ΔEF )/kB T ] − 1

(10.36)

10.2 Spontaneous Emission and Stimulated Emission

583

Fig. 10.3 Inversion factor f 2 − f 1 of pn junction is plotted as a function of emitted photon energy, where the curves are obtained by putting EFn − Ec = Ev − EFp = 20, 15, −10, 5 0, −5, −10, −15, −20 meV from the upper to bottom curves. m e = 0.068 m, m h = 0.59 m, EG = 1.43 eV, and T = 300 K

Fig. 10.4 The gain factor ( f 2 − f 1 )ρred is plotted as a function of emitted photon energy, where the curves are obtained by putting EFn − Ec = Ev − EFp = 20, 15, 10, 5, 0, −5, −10, −15, −20 √ meV from the top to bottom curves, where ρred is approximated by ω − EG . m e = 0.068 m, m h = 0.59 m, EG = 1.43 eV, and T = 300 K

Summarizing these results the laser gain due to the stimulated emission is equivalent to the negative absorption coefficient and given by πc2 3 rstim (ω) 40 n 2r (ω)2 ω − ΔEF πc2 3 . r (ω) 1 − exp = spon 40 n 2r (ω)2 kB T

g(ω) =

(10.37)

The above equation expresses the laser action. The gain g is positive (g > 0) for ω > ΔEF = (EFn − EFp ). On the other hand, for ω < ΔEF the gain is negative and light absorption occurs. Spontaneous and stimulated emission rates of GaAs calculated for no–selection rule case from (10.23) and (10.24) are shown in Fig. 10.5, where the parabolic energy bands are assumed and temperature is T = 80 K. In the calculations quasi–Fermi levels are assumed to be 11.8 meV for holes, and 5 and 15 meV for electrons. The

584

10 Light Emission and Laser

Fig. 10.5 Spontaneous emission rate rspon and stimulated emission rate rstim are calculated from (10.23) and (10.24) for GaAs assuming parabolic energy bands at 80 K, where the quasi–Fermi levels are 11.8 meV for holes, and 5 and 15 meV for electrons. Coefficient C is for GaAs and defined by (10.38) and (10.40) [8]

coefficient C for GaAs is estimated from (10.38) and (10.40) [8], which is given by 1/2

C=

3/2

128 mc mv m EG + Δ n r EEG κ3 . · · 3 2 4 3 ∗3 3π me c m EG + (2/3)Δ

(10.38)

Using the values EG = 1.521 eV, m c = 0.072 m,E = 1.47 eV, Δ = 0.33 eV, n r = 3.6, and κ = 12.5, we obtain B = 0.75 × 10−9 cm2 /s, C = 2.6 × 1023 cm−3 s−1 meV−3 .

(10.39) (10.40)

10.3 Band Tail Effect In the previous section we are concerned with the emission rates in semiconductors with parabolic bands, and assumed that no electronic states in the band gap. In such a case distributions of electrons and holes are schematically shown as in Fig. 10.6. However, Kane [10] pointed out that the electronic states are deformed by the potential due to impurities (cluster of impurities). Taking account of the Thomas–Fermi screening (see Sect. 6.3.10) by electrons and assuming Gaussian distribution for the potential fluctuations, the density of states is approximated as 3/2

mc ρc (E ) = 2 3 (2ηc )1/2 y π

E − Ec ηc

,

(10.41)

where m c is the electron effective mass and Ec is the conduction band bottom energy obtained without the impurity potentials. Putting E − Ec = E and x = E/ηc the function y(x) is written as

10.3 Band Tail Effect

585

Fig. 10.6 Electron and hole distribution in parabolic bands, a thermal equilibrium, b population inversion at T = 0 K, and c population inversion at T > 0 K

y(x) =

1 π 1/2

x

−∞

(x − z)1/2 exp(−z 2 )dz .

(10.42)

Here ηc represents the extension of the band tail, and e2 (4π ND L scr )1/2 , 4πκ

ηc =

(10.43)

where κ0 is the dielectric constant, ND is the donor density and L scr is the screening length, defined by 1/qs in Sect. 6.3.10 (see (6.277) or (6.279)). The fluctuation of the potentials results in a Gaussian type modification of the band edge and gives rise to extended electronic states in the band gap. This band states are called band tail states and the effect is referred to as band tail effect. The same effect is expected in the valence band. When both of the conduction and valence bands are affected by such potential fluctuations, the donor density ND+ in (10.43) is replaced as ND → ND+ + NA− , where ND+ is the ionized donor density and NA+ is the ionized acceptor density. Figure 10.7 shows a comparison between the density of states with √ the band tail effect, (10.42), and the density of states for the parabolic band y(x) = x without the band tail effect. It is clear from (10.42) that ρ ∝ E 1/2 at higher energies and ρ ∝ exp(−E 2 /ηc2 ) at lower energies. Here we will summarize the theory of band tail effect proposed by Kane [10]. Hamiltonian of an electron is written as H = H0 + HI , 2 H0 = − ∗ ∇ 2 , 2m HI = v(r − r i ) , i

(10.44) (10.45) (10.46)

586

10 Light Emission and Laser

Fig. 10.7 Band edge states with the band tail effect y(x) of (10.42) is compared with √ the parabolic band states given by y(x) = x

r e2 , exp − v(r ) = − 4πκ0 r L scr

(10.47)

where H0 is the unperturbed Hamiltonian of a perfect single crystal with the effective mass m ∗ and the dielectric constant κ0 , and perturbation HI arises from randomly distributed impurities over lattice sites r i . The potential energy of an impurity v(r ) is screened by electrons with the density n, and the screening length L scr = (1/qs ) is given by (6.273) as shown in Sect. 6.3.10, 1 = L scr

e2 ∂n . κ0 ∂EF

(10.48)

As described in Sect. 6.3.10, the screening length in a degenerate semiconductors is given by Thomas–Fermi screening length, (6.277), 3e2 n ≡ qTF , 2κ0 EF

1 = L scr

(10.49)

or in a non-degenerate semiconductor the screening length is given by Debye–Huckel screening length, (6.279), 1 = L scr

e2 n ≡ qDH . κ0 kB T

(10.50)

We define the potential distribution function, F(V), by Δp = F(V)ΔV ,

(10.51)

where Δp is the probability of finding the potential between V and V + ΔV. The total density of states is given by

10.3 Band Tail Effect

587

Fig. 10.8 Electron and hole distribution in the conduction band and valence band, where the band tail effect is included

Fig. 10.9 The calculated spontaneous emission spectra in GaAs with ND = 3 × 1018 cm−3 and NA = 6 × 1018 cm−3 at several temperatures. The arrows show the peak positions of −α(E ) (from Stern [9])

ρ(E) =

√ ∗3/2 E 2m V (E − V)1/2 F(V)dV . π 2 3 −∞

(10.52)

Assuming Gaussian distribution of the impurities, Kane [10] derived

1 V2 F(V) = √ exp − 2 , η πη 2 e η= (4πn L scr )1/2 , 4πκ0

(10.53a) (10.53b)

where η has been defined by (10.43), and v 2 (r )d3 r =

2πe4 L scr (4πκ0 )2

(10.54)

588

10 Light Emission and Laser

Fig. 10.10 The gain g is plotted as a function of injected current density in GaAs with donor density ND = 1 × 1018 and acceptor density NA = 4 × 1018 cm−3 . The solid and dashed curves are calculated with and without the band tail effect, respectively (from Stern [9])

Fig. 10.11 Injected current density required to get gain g = 100 cm−1 is plotted as a function of temperature for GaAs with the impurity density NA − ND = 3 × 1018 cm−3 (from Stern [9])

for the screened Coulomb potential. Substituting (10.53a) into (10.52), Kane derived (10.41) for the density of states with the band tail effect. Distributions of the electron and hole densities with the band tail effect are shown in Fig. 10.8. Spontaneous emission spectra rspon calculated by Stern [9] with the band tail effect are shown as a function of photon energy in Fig. 10.9, where the arrows are the peak positions of −α(E). The spectra are calculated for the gain g = 100cm−1 . The gain g vs. current density in GaAs is shown in Fig. 10.10, where curves are plotted for several temperatures, and the donor and acceptor densities are ND = 1 × 1018 and NA = 4 × 1018 cm−3 , respectively. The solid and dashed curves are the gains with and without the band tail effect, respectively. In Fig. 10.11, current density required to get the gain g = 100 cm−1 is plotted as a function of temperature for different impurity densities, where NA − ND = 3 × 1018 cm−3 and donor densities ND = 3 × 1017 , 3 × 1018 , 1.0 × 1019 , 3 × 1019 cm−3 . Semiconductor laser diodes consist of highly doped pn junctions and thus the band tail effect plays an important role in the laser action. In such a case the momentum (wave vector) conservation rule is not fulfilled, and thus the laser gain is calculated by taking account of the density of states with the band tail effect and the energy conservation rule. We will discuss laser oscillations in Sects. 10.4 in connection with luminescence and detailed mechanisms in Sect. 10.5. The difference between LDs

10.4 Luminescence

589

(Laser Diodes) and LEDs (Light Emitting Diodes) is the line width of the emission spectra. The spectral line shapes of LDs are very narrow with high output but LEDs exhibit wide line width. In the next section we deal with the emission of LDs and LEDs in various materials and discuss the mechanisms of the luminescence.

10.4 Luminescence Excited electrons and holes in semiconductors recombine to emit photons. This process is called luminescence. The excitations (pumping) by light (photons), cathode ray (electron beams) and electron–hole injection by forward current in pn junction are called, respectively, photoluminescence, cathode luminescence, and electro– luminescence. Luminescence in semiconductors is based on the light emission due to the recombination of excited electrons and holes. Various mechanisms are involved in the recombination processes, in which the direct recombination of electrons and holes in direct gap semiconductors play the most important role. In indirect semiconductors the recombination involves phonon emission or absorption and thus the intensity is very weak. Luminescence is also induced by other mechanisms such as (1) recombination of excited electrons in the conduction band with the holes trapped in acceptors, (2) recombination of trapped electrons in donors with holes in the valence band, (3) recombination of the pair states of donor and acceptor, and so on. At low temperatures an electron bound to a donor attracts an hole and forms an electron– hole pair (exciton) bound at a donor (DX pair) which dissociates to emit light. In addition isoelectronic traps in GaP such as GaP:N results in strong light emission in indirect semiconductors. In this section we will concern with the mechanisms of luminescence in semiconductors. See the review articles of Bebb and Williams [3], Williams and Bebb [4], and Holonyak and Lee [5] for the details of the theories and experiments on luminescence.

10.4.1 Luminescence Due to Band to Band Transition In semiconductors without the band tail effect luminescence is governed by band to band transition, and the luminescence intensity I is proportional to the spontaneous emission rate rspon , which is given by the following relation with the emitted photon energy ω from (10.17), I (ω) ∝ rspon ∝

ω − EG , ω − EG exp − kB T

(10.55)

where the excited electron density is approximated by Boltzmann distribution f 2 ∼ = exp (−ω/kB T ) and the hole distribution function is assumed to be f 1 ∼ = 1. Using this relation calculated luminescence spectra are shown in Fig. 10.12, where the

590

10 Light Emission and Laser

Fig. 10.12 Calculated luminescence spectra for the band to band transition in GaAs in GaAs, where the distribution function of the excited electrons is assumed to be given by Boltzmann distribution function and the temperature dependence of the band gap is taken account. EG (300 K) = 1.43 eV at T = 300 K and EG (77 K) = 1.50 eV at T = 77 K

normalized intensities at T = 300 and T = 77 K are compared in GaAs. In Fig. 10.12 the temperature dependence of the band gap is taken into account; EG (300 K) = 1.43 eV at T = 300 K and EG (77K) = 1.50 eV at T = 77 K. We see in the figure that the band width of the luminescence becomes narrower at lower temperatures.

10.4.2 Luminescence Due to Excitons We discussed in Sect. 4.5 excitons in an direct band gap semiconductor and in indirect band gap semiconductor. Luminescence is the reverse process of the absorption. 10.4.2.1

(1) Luminescence Due to Free Excitons

In Sect. 4.5 we discussed Coulomb interaction of an electron–hole pair (exciton) by solving Hamiltonian, and the exciton state is described by the bound state with the dissociation energy Ex /n 2 , n = 1, 2, 3, . . .) and the continuum state with the center of mass motion. These excitons are possible to move freely in the crystal (called free excitons) and are distinguished from the excitons bound to donors or acceptors, bound excitons, which will be discussed later. From the analogy to hydrogen atom model, using the Bohr radius of an exciton ax = (m/μ)(/0 )aB and the exciton reduced mass 1/μ = 1/m e + 1/m h , we obtain Ex = (μ/m)(0 /)2 EH = (μe4 )/[2(4π)2 2 ], and the absorption coefficient of the exciton is given by (see Sect. 4.5). 1 α(ω) ∝ , (10.56) (ω − EG + Ex )2 + Γ 2 where the dielectric function of the exciton is approximated by Lorentzian. Therefore the luminescence intensity has a peak around the energy Ex below the band edge. The luminescence near the band edge is modified by the factor exp(−ω/kB T ) and the peak position is shifted to the lower energy side by kB T . Therefore it is very

10.4 Luminescence

591

difficult to determine the energy gap exactly from the luminescence spectrum. The luminescence spectrum of the free exciton is given by I (ω) ∝

1 exp [−(ω − EG + Ex )/kB T ] , (ω − EG + Ex )2 + Γ 2

(10.57)

where Γ is the broadening energy.

10.4.2.2

(2) Luminescence Due to Indirect Excitons

The locations of the conduction band bottom and valence band top in a indirect gap semiconductor are different in the k space, such as in GaP. As described in Sec. 4.5 light absorption occurs accompanying absorption or emission of a phonon. Since various types of phonons are involved in the absorption, complicated structures of the absorption spectra are observed. The absorption coefficient due to indirect excitons is expressed as follows (see Sect. 4.5.2) 1/2 α(ω) ∝ ω − EG ∓ ωqα + Ex /n 2 ,

(10.58)

where ωqα is the phonon energy involved in the absorption and ∓ corresponds to absorption and emission of a phonon. Therefore luminescence involving phonon emission appears below the band gap energy and is well resolved. Thus the luminescence spectrum is given by 1/2 I (ω) ∝ ω − EG + ωqα + Ex /n 2 × exp −(ω − EG + ωqα + Ex /n 2 )/kB T . (10.59) Comparing with (10.59) with (10.55) we find the line shape of the photoluminescence due to the indirect exciton is similar to the line shape of the direct band to band transition. From these considerations the luminescence spectrum due to indirect exciton accompanies well resolved phonon peaks.

10.4.2.3

(3) Luminescence Due to Excitons Bound to Impurities

The state in which an electron and a hole are bound to an impurity is called bound exciton and the energy state depends on the mass ratio of an electron and a hole, σ = m e /m h . See the references for the detailed analysis of the bound excitons. Here we summarize the luminescence due to the bound excitons. The bound state of the exciton–ionized donor (an exciton bound to an ionized donor) is expressed as (D+ , x),

⊕ − +,

or

D+ e h .

(10.60)

592

10 Light Emission and Laser

The exciton bound to ionized acceptor is expressed by (A− , x),

+ −,

or

A− e h ,

(10.61)

where other symbols are also used in papers reported so far. The exciton bound to a neutral donor consists of a neutral donor D0 , two electrons − − and a hole +, and expressed as (10.62) (D0 , x), ⊕ − − + or D+ e e h . The exciton bound to a neutral acceptor is shown by (A0 , x),

++−

or

A− h h e .

(10.63)

The emitted photon energy due to the dissociation of the exciton complex in GaAs is written as [11]

10.4.2.4

ω(D0 , x) = EG − Ex − 0.13ED , ω(D+ , x) = EG − ED − 0.06ED ,

(10.64a) (10.64b)

ω(A0 , x) = EG − Ex − 0.0.07EA , ω(A− , x) = EG − EA − 0.4EA .

(10.64c) (10.64d)

(4) Luminescence Due to Donor–Acceptor Pairs

A donor and an acceptor occupy different sites of the lattices. In the case where the wave functions of the donor and the acceptor overlap, the donor ion D+ , the acceptor ion A− , an electron − and a hole + compose a complex state, and luminescence due to the dissociation of the complex is observed. Such a complex is written as (D0 , A0 ),

(D+ A− , x),

⊕−+

D+ A− e h .

(10.65)

This type of a complex is called an exciton bound to donor–acceptor pair D+ A− and the bound energy depends on the distance between the donor D+ and the acceptor A− .

10.4.2.5

(5) Exciton Molecules

Another important example of complexes is exciton molecules (exciton–exciton complex) which is expressed as (x x),

+ + − −,

The excitation energy of an exciton is given by

or

hhee.

(10.66)

10.4 Luminescence

593

E(x) = EG − Ex .

(10.67)

Letting the interaction energy of two excitons D0 , the excitation energy of two excitons is approximated as 2E(x) − D0 . Therefore we obtain the following relation for the excitation energy of an exciton molecule, E(x1 x2 ) = E(x1 ) + E(x2 ) − D0 .

(10.68)

When an exciton molecule dissociates, one of the exciton of the molecule dissociates and leaves a free exciton of the energy E(x2 ) and a photon ω. Since the final state of the energy ω + E(x2 ) is equivalent to the initial state E(x x), the following relation is obtained, (10.69) ω = E(x1 ) − D0 ≡ EG − Ex − D0 , where the crystal still has the energy E(x2 ) and thus emits the second photon of energy ω = EG − Ex .

10.4.3 Luminescence via Impurities The luminescence via impurities plays an important role in the recombination in semiconductors. Here we will deal with the basic mechanisms of luminescence associated with impurities. See the papers by Dumke [12] and Eagles [13] for the theoretical treatments. These two papers are based on different expressions of the wave functions of the impurity states, but the obtained results are the same. We will describe the method of Dumke in detail and briefly refer the result of Eagles. For simplicity, we calculate the recombination rate between a hole bound to the ground state of an acceptor and an electron in the conduction band. It is apparent that the recombination rate between an electron bound to a donor and a hole in the valence band as seen from the following treatment. The wave function (envelop function) F(r) of a particle bound to an impurity ion is given by the effective mass approximation, e2 2 − E F(r) = 0 . (10.70) − ∗ ∇2 − 2m 4πκ0 r Since a hole near the valence band edge k ∼ = 0 is captured by an acceptor, the wave function may be expressed by the envelop function given by the above equation. Therefore the wave function of a hole captured by an acceptor is given by the product of the Bloch function Ψv,k (r) = eik·r u v,k (r) and the envelop function F(r). In other words, (10.71) ΨA (r) = u v,k (r)eik·r F(r) ∼ = u v,0 (r)F(r) The eigenvalue of the resulting effective mass equation is given by

594

10 Light Emission and Laser

En = −

m ∗ e4 1 · , 2(4πκ0 )2 2 n 2

n = 1, 2, . . . ,

(10.72)

and the eigenfunction of the ground state (n = 1) is written as F1 (r) =

1 −r/aA e πaA3

aA =

(10.73)

4π2 κ0 . m ∗ e2

(10.74)

Using these results the momentum matrix element for the transition of the electron in the conduction band to the acceptor is obtained as follows. Here we will present the calculations of the momentum matrix element proposed by Dumke [3, 12]. The momentum matrix element is written as (e · p)cA = c, k|e · p|A =

e−ik·r u c,k (e · p)ΨA (r)d3 r ,

(10.75)

where e is the unit vector of the light polarization and p is the momentum operator. The calculation of the above momentum matrix element is carried out by operating p = −i∇ to ΨA (r) and the following two terms appear. (e · p)cA =

e−ik·r F(r) u c,k (r)(e · p)u v,0 (r) d3 r + e−ikr (e · p)F(r) u c,k (r)u v,0 (r)d3 r .

(10.76)

The above integration is not easy, but may be carried out under the following assumption. When the functions F(r) and e−ik·r are assumed to change slowly compared to the period of the Bloch function u(r + Rm) = u(r), the integral is replaced by the summation of the unit cells Ω; → Rm ω . The slowly varying function F(r) may be assumed to be constant within a unit cell and approximated by the value at the center of the unit cell F(Rm ). Thus we obtain 1 Ω e−ik·Rm F(Rm ) u c,k (r)(e · p)u v,0 (r)d3 r Ω Ω Rm 1 +Ω e−ik·Rm [(e · p)F(r)] Rm u c,k (r)u v,0 (r)d3 r . (10.77) Ω Ω R m

The second term of the above equation vanishes due the orthogonality of the Bloch functions. The summation of the first term may be transformed into an integral form by using an approximation Ωe−ik·Rm F(Rm ) =

Ω

e−ik·Rm F(Rm )d3 r

Ω

e−ik·r F(r)d3 r ,

(10.78)

10.4 Luminescence

595

and therefore the summation over the unit cells is rewritten by the integral over the crystal volume V

Ωe−ik·Rm F(Rm )

e−ik·r F(r)d3 r .

(10.79)

V

Rm

The momentum matrix element of (10.76) is thus given by (e · p)c,A = c, k|e · p|A = where

1 pcv (k) = Ω

e−ik·r F(r)d3 r · pcv ≡ a(k) · pcv ,

(10.80a)

u c,k (r)(e · p)u v,0 (r)d3 r .

(10.80b)

Ω

Since the matrix element pcv (k) varies very slowly with the k value, we use the value at the band edge pcv (0) pcv (0) =

1 Ω

Ω

u c,0 (r)(e · p)vv,0 (r)d3 r .

(10.80c)

The integral of a(k) is evaluated to obtain

e−ik·r F(r)d3 r 1 = e−ikr cos θ e−r/aA r 2 sin θdθdφdr (πaA3 )1/2 1/2 8 πaA3 = 2 . 1 + (kaA )2

a(k) =

(10.81)

Eagles expressed the wave function of the impurity by a linear combination of Bloch functions [13] and the shallow impurity state by using the valence band wave functions, and obtained the same results of Dumke described above. Using the momentum matrix element for a bulk crystal Mcv (≡ pcv ), the squared matrix element of an electron transition between the conduction band and the acceptor level is given by 1 64 πaA3 2 2 (10.82) |M| av = |Mb | av , V 1 + (kaA )2 4 where V is the volume of the crystal. |Mcv |2 av is the average matrix element connecting bulk states near the band edges and given by the following relation using the interband matrix element P defined in Chap. 2 |Mcv |2 av =

m2 P 2 m 2 EG (EG + Δ0 ) , 62 12m ∗e EG + 2Δ0 /3

(10.83)

596

10 Light Emission and Laser

where m ∗e is the band edge effective mass of the conduction band and given by (2.158). The above relation is easily deduced from the wave functions of the heavy and light hole bands given by (2.63a), (2.63b), (2.63e), (2.63f) and P = (/m)S| pz |Z = (/m)P0 , and the conduction band wave function |S.3 When the overlapping of the acceptor wave functions is negligible, then the spontaneous emission rate is obtained from (G.28) of Appendix G 64 πaA3 n r e2 ω 2 NA |Mb | av rspon (ω) = 4 π0 m 2 2 c3 1 + (kaA )2 k ×δ Ec (k) − (Ev,0 + EA ) − ω f (E2 )[1 − f (E1 )] , (10.84) where NA is the density of the acceptors, and f (E2 ) and f (E1 ) are the occupation functions of the electrons in the conduction band and the acceptor level, respectively. Similar expression is obtained for the transition of electron from the donor state to the valence band. From the above considerations the luminescence intensity due to the transition of the electrons in the conduction band to the acceptor level is given by the following relation

ω − EG + EA , (10.85) I (ω) ∝ rspon ∝ ω − EG + EA exp − kB T The term m 2 P 2 /62 of (10.83) should be replaced by 4m 2 P 2 /32 , when we take the heavy and light hole bands into account and neglect the spin–orbit split–off band. For spin orientation | ↑, we obtain 2 2 1 m2 2 3 3 3 3 S px , = S py , = P , 2 2 2 2 2 2 2 2 1 m2 2 1 1 3 3 S px , − = S py , − = P , 2 2 2 2 6 2 2 4 m2 2 3 1 S pz , = P . 2 2 6 2

3

Then we find the momentum matrix element for spin orientation | ↑ 2

1 1 2 1 m2 2 3 3 3 + S px , − = P . |Mx |2 = S px , + 2 2 2 2 2 6 2 Summing up all the components and multiplying by 2 of spin degeneracy, we obtain |Mb |2 av =

4m 2 P 2 2 , |Mx |2 + |M y |2 + |Mz |2 = 3 32

where we used the following definitions, S| px |X 2 = S| p y |Y 2 = S| pz |Z 2 = .

m2 2 P . 2

10.4 Luminescence

597

Fig. 10.13 Experimental data of photoluminescence from Cd doped GaAs (GaAs:Cd) at T = 20 and 80 K are compared with (10.85). ◦ and • are for the sample 1 at T = 20 and T = 80 K, respectively, and are for the sample 2 at T = 20 K (after Williams and Webb [14])

which is quite similar to the band to band transition of (10.55), and the luminescence peak shifts to the lower energy site by EA compared to the band to band transition. The luminescence line shape is expected to be similar to Fig. 10.12. Photoluminescence spectra of GaAs:Cd (Cd doped GaAs) are compared with (10.85) at T = 20 and 80 K in Fig. 10.13, where we find the luminescence peak appears at EG − EA but strong tails are observed at the lower energy side. Since the acceptor density is NA = 4 × 1016 cm−3 , the band tail effect of the conduction band is negligible and thus the tails of the luminescence is ascribed to the excitons bound to acceptors (an electron is bound to an acceptor capturing a hole). Assuming the band gap EG = 1.521 eV at T = 20 K, the binding energy of the acceptor is EA = 34.5 meV. The band gap at T = 80 K is estimated as EG (T = 80) = 1.512 eV.

10.4.4 Luminescence in GaP and GaAsP via N Traps It is well known that the bottoms of the conduction bands of GaP and GaAsx P1−x (x ≥ 0.47) are located near the X point in the Brillouin zone, and therefore optical transition is indirect with emission or absorption of phonons. However, strong luminescence is observed in nitrogen (N) doped samples. Here we explain the mechanisms of the luminescence due to N levels. For more detailed treatments see the review paper by Holonyak and Lee [5] and references cited in the text. LED (Light–Emitting Diode) based on GaAsx P1−x crystals are now commercially popular devices. Success of such LEDs are due to the following two factors. One is the unique mechanisms of the luminescence and the other is the crystal growth technologies of GaAsx P1−x on large GaP or GaAs substrates utilizing open–tube vapor–phase–epitaxy (VPE) by transport of AsH3 -PH3 . The luminescence of GaAsx P1−x in the direct transition region x ≤ 0.46 (T = 77 K); x ≤ 0.49 (300 K) is quite similar to GaAs and in the region of direct–indirect transition the luminescence is ruled by the emission via the

598

10 Light Emission and Laser

Fig. 10.14 Band structure of GaP:N, where the shaded region represents the amplitude of the electron wave function ψN (k) bound to the isoelectronic N trap and has large amplitudes near the X and Γ points reflecting the respective conduction band minima. The binding energy of the N trap is about 10 meV and the potential is localized near the N atom (broadened in the k space), the wave function ψN (k) has a large amplitude near the region k = 0, resulting in a strong quasi–direct transition. (Figure after Holonyak and Lee [5])

X conduction band with the large effective mass and the donor level associated with the X conduction band. In the indirect transition region of GaAsx P1−x (x ≥ 0.46) the luminescence is dominated by the isoelectronic N level. Nitrogen (N) atoms doped in GaP and GaAsx P1−x substitute phosphorous (P) atoms. The N atoms are electronically equivalent to P atoms and thus called isoelectronic traps. The electronegativity of N is larger than P. Lattices surrounding doped N atoms relax and the negativity of N atom is reduced but electrons are localized around the N atoms. It is known that the potential on N atom is different from the Coulomb potential of usual donors screened up to several atomic distance and that the potential attracts an electron toward the central part (central cell potential). The dissociation energy of a trapped electron at N atom in GaP is quite small and is estimated to be about 10 meV. Since the electron is captured by the N trap, the wave function ψ is expected to be spread in k space as shown in Fig. 10.14 from the uncertainty principle and strong luminescence similar to the direct transition is observed although GaP is an indirect transition semiconductor. Experimental data indicate that the wave function at k = 0 of the electron trapped at N is about 100 times of the wave function of the electron bound to a regular donor. In addition the wave function of an electron captured by the N trap overlaps with a hole wave function at k = 0 (Γ point), resulting in a formation of an exciton, and luminescence due to the exciton is observed. When we increase doping of N atoms in GaP, NN pairs are formed. The nearest neighbor pair is expressed by NN1 (NN2 , NN3 , . . . are the second, the third, . . . nearest pairs). As shown in Fig. 10.15, luminescence of NN1 and NN3 pairs are observed and such a pair luminescence is distinguished from the luminescence due to the isolated N atoms (NX and A–B line). The series of

10.4 Luminescence

599

Fig. 10.15 The energy levels of the Γ conduction band, X conduction band, and N and NN pairs in N–doped GaAsx P1−x at 77 K. NΓ is the donor level (x ≤ 0.55) associated with the Γ conduction band. NN1 and NN3 pairs are experimentally resolved for x ≥ 0.90, but in the other region observed as a broad NX level. Such a broad luminescence in GaP:N is called A–line. (Figure after Holonyak and Lee [5])

Fig. 10.16 Photoluminescence of excitons trapped at N isoelectronic traps in GaP. The peaks A and B are no–phonon lines. T = 4.2 K and N = 5 × 1016 cm−3 . The energy gap of GaP EG (T = 0K) = E (X ) − E (Γ ) = 2.339 eV. (Dean [17])

N pairs NN1 , NN2 , . . ., NN10 are resolved by the fluorescence (photoluminescence) spectroscopy [15, 16]. In GaAsx P1−x (x ∼ = 0.28) overlapped luminescence of NX and of the EΓ band is observed. A typical example of the experimental results of luminescence of excitons trapped at N isoelectronic traps is shown in Fig. 10.16. The energy gap of GaP is EG (T = 0K) = E(X ) − E(Γ ) = 2.339 eV. The peaks of A and B are the no–phonon lines of the excitons bound to N atoms (N and NN pairs) and phonon lines are well resolved. Figure 10.17 shows photoluminescence spectra of GaAsx P1−x (x = 0.34):N+ , ND = 1.8 × 1017 cm−3 , where N+ means heavy doping of N atoms (1019 cm−3 ). In the region of weak excitation (500 W/cm2 ), luminescence from the Γ conduction band and from NX is well resolved. Increasing the excitation power luminescence from the Γ conduction band dominates the luminescence from NX level. For excitation power 7 × 104 W/cm2 , laser oscillations from NX level are observed. The shaded region consists of well resolved 10 lines of laser oscillations. Luminescence of p–type GaAsx P1−x (x = 0.34):N+ :Zn is shown in Fig. 10.18, where luminescence from N doped GaAsP substrate is shown by the dashed curve.

600

10 Light Emission and Laser

Fig. 10.17 Photoluminescence spectra of GaAsx P1−x (x = 0.34):N+ , ND = 1.8 × 1017 cm−3 . In a low excitation (500 W/cm2 ), the band to band transition associated with the Γ conduction band and emission from the NX level are well resolved. Increasing the excitation power the emission of the band to band dominates the emission of NX level. For excitation power of 7 × 104 W/cm2 laser oscillations of NX level are observed, where the shaded region consists of 10 lines of laser oscillations. (After Holonyak and Lee [5])

Luminescence from a p–type substrate with additional doping by Zn exhibit an emission peak from NX at 29 meV lower than the emission peak of NX in n–type GaAsP:N+ . This emission peak is ascribed to the recombination of the electrons captured by NX with the holes captured at Zn acceptors. In GaAs doped with Zn and O, oxygen O behaves as a donor and Zn as a shallow acceptor. When these two dopant occupy the nearest lattice sites, a pair of Zn·O is formed. Electrons far from the pair see an electronically neutral complex, but for an electron close to the pair the electronegativity of O is larger than Zn. Therefore O atom forms electron trap of binding energy about 0.3 eV. When an electron is captured by the Zn·O complex, the complex is negatively charged and the resulting Coulomb potential attracts a hole, forming an exciton. The photoluminescence due to the recombination of the electron–hole pair exhibits a peak at about 1.8 eV, emitting red light.

10.4 Luminescence

601

Fig. 10.18 Luminescence spectra of p–type GaAsx P1−x (x = 0.34):N+ :Zn, ND = 1.8 × 1017 cm−3 . For low excitation (500 W/cm2 ), the band to band transition associated with the Γ conduction band and emission from the NX level are well resolved. Increasing the excitation power the emission of the band to band dominates the emission o